#------------------------------------------------------------------------------
#$Date: 2025-07-01 14:21:59 +0300 (Tue, 01 Jul 2025) $
#$Revision: 1234 $
#$URL: svn://crystallography.net/testcod/cif/1/00/00/1000022.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1000022
loop_
_publ_author_name
'Hunger, Jens'
'Beta, Ilir A.'
'Böhlig, Heinz'
'Ling, Chris'
'Jobic, Herve'
'Hunger, Bernd'
_publ_section_title
;
 Adsorption Structures of Water in NaX Studied by DRIFT Spectroscopy and
 Neutron Powder Diffraction
;
_journal_issue                   1
_journal_name_full               'The Journal of Physical Chemistry B'
_journal_page_first              342
_journal_page_last               353
_journal_paper_doi               10.1021/jp054636u
_journal_volume                  110
_journal_year                    2006
_chemical_formula_analytical     'Na88.1[Al88.1Si103.9O384] *43H2O'
_chemical_formula_sum            'Al0.92 D0.89 Na0.84 O4.45 Si1.08'
_chemical_formula_weight         147.49
_chemical_name_common            NaX
_space_group_IT_number           203
_space_group_name_Hall           '-F 2uv 2vw 3'
_space_group_name_H-M_alt        'F d -3 :2'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-F 2uv 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 :2'
_audit_creation_date             2005-08-01T20:13
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
' 2005-08-01T20:13  Initial CIF as created by GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            96
_cell_length_a                   25.10442(14)
_cell_length_b                   25.10442
_cell_length_c                   25.10442
_cell_measurement_temperature    5
_cell_volume                     15821.61(9)
_computing_molecular_graphics    'Diamond 3'
_computing_publication_material  EXPGUI
_computing_structure_refinement  GSAS
_diffrn_radiation_probe          neutron
_diffrn_radiation_wavelength     2.4
_exptl_absorpt_correction_T_max  0.98183
_exptl_absorpt_correction_T_min  0.98177
_exptl_absorpt_process_details
;   GSAS Absorption/surface roughness correction: function number 0
 Debye-Scherrer absorption correction
Term (= MU.r/wave) =     0.45173E-02
Correction is not refined.
;
_pd_block_id                     2005-08-01T20:13|NAX48
_pd_calc_method                  'Rietveld Refinement'
_pd_instr_location               ' ?'
_pd_meas_2theta_range_inc        0.05
_pd_meas_2theta_range_max        151.2
_pd_meas_2theta_range_min        0.05
_pd_meas_number_of_points        3024
_pd_phase_name                   NaX-48
_pd_proc_2theta_range_inc        0.05
_pd_proc_2theta_range_max        151.1267
_pd_proc_2theta_range_min        -0.0233
_pd_proc_info_datetime           2005-08-01T20:13:45
_pd_proc_info_excluded_regions   ' ?'
_pd_proc_ls_background_function
;   GSAS Background function number 1 with 20 terms.
 Shifted Chebyshev function of 1st kind
      1:    182.346     2:   -30.6779     3:    29.7169     4:   -4.50833    
      5:    3.10634     6:   -3.18890     7:    2.44189     8:   -1.72787    
      9:  -0.781007    10:  -0.474458    11:   0.804027    12:    2.86164    
     13:   -2.07429    14:   -1.54306    15:    2.91886    16:  -0.107104    
     17:   0.885740    18:    1.19362    19:  -0.696129    20:   0.400034    
;
_pd_proc_ls_peak_cutoff          0.00000
_pd_proc_ls_profile_function
;
 CW Profile function number 2 with  18 terms
 Profile coefficients for Simpson's rule integration of pseudovoigt function
 C.J. Howard (1982). J. Appl. Cryst.,15,615-620.
 P. Thompson, D.E. Cox & J.B. Hastings (1987). J. Appl. Cryst.,20,79-83.
 #1(GU)   =  141.178 #2(GV)   = -157.250 #3(GW)   =  152.287
 #4(LX)   =    8.212 #5(LY)   =    9.468 #6(trns) =    0.000
 #7(asym) =   7.6704 #8(shft) =   0.0000 #9(GP)   =    0.000
 #10(stec)=     0.00 #11(ptec)=     0.00 #12(sfec)=     0.00
 #13(L11) =    0.000 #14(L22) =    0.000 #15(L33) =    0.000
 #16(L12) =    0.000 #17(L13) =    0.000 #18(L23) =    0.000
 Peak tails are ignored  where the intensity is below 0.0000 times the peak
   Aniso. broadening axis   0.0   0.0   1.0
;
_pd_proc_ls_prof_R_factor        0.0239
_pd_proc_ls_prof_wR_expected     0.0211
_pd_proc_ls_prof_wR_factor       0.0312
_pd_proc_number_of_points        3024
_pd_spec_mounting                ' ?'
_refine_ls_goodness_of_fit_all   1.50
_refine_ls_matrix_type           full
_refine_ls_number_parameters     98
_refine_ls_number_restraints     28
_refine_ls_R_Fsqd_factor         0.01630
_refine_ls_shift/su_max          0.04
_refine_ls_shift/su_mean         0.00
_reflns_d_resolution_high        1.243
_reflns_d_resolution_low         8.876
_reflns_limit_h_max              20
_reflns_limit_h_min              1
_reflns_limit_k_max              14
_reflns_limit_k_min              0
_reflns_limit_l_max              13
_reflns_limit_l_min              0
_reflns_number_total             369
_cod_data_source_file            jp054636usi20050825_095708.cif
_cod_data_source_block           NAX48_publ
_cod_original_cell_volume        15821.61(26)
_cod_original_sg_symbol_Hall     'F d -3'
_cod_original_sg_symbol_H-M      'F d -3'
_cod_database_code               1000022
_gsas_exptl_extinct_corr_t_min   1.00000
_gsas_exptl_extinct_corr_t_max   1.00000
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 +z,+x,+y
3 +y,+z,+x
4 +x+1/4,+y+1/4,-z
5 -z,+x+1/4,+y+1/4
6 +y+1/4,-z,+x+1/4
7 -z+1/4,+x+1/2,-y+3/4
8 -y+3/4,-z+1/4,+x+1/2
9 +y+1/2,-z+1/4,-x+3/4
10 -x+3/4,+y+1/2,-z+1/4
11 -z+1/4,-x+3/4,+y+1/2
12 +x+1/2,-y+3/4,-z+1/4
-1 -x,-y,-z
-2 -z,-x,-y
-3 -y,-z,-x
-4 -x+3/4,-y+3/4,+z
-5 +z,-x+3/4,-y+3/4
-6 -y+3/4,+z,-x+3/4
-7 +z+3/4,-x+1/2,+y+1/4
-8 +y+1/4,+z+3/4,-x+1/2
-9 -y+1/2,+z+3/4,+x+1/4
-10 +x+1/4,-y+1/2,+z+3/4
-11 +z+3/4,+x+1/4,-y+1/2
-12 -x+1/2,+y+1/4,+z+3/4
101 +x,+y+1/2,+z+1/2
102 +z,+x+1/2,+y+1/2
103 +y,+z+1/2,+x+1/2
104 +x+1/4,+y+3/4,-z+1/2
105 -z,+x+3/4,+y+3/4
106 +y+1/4,-z+1/2,+x+3/4
107 -z+1/4,+x,-y+1/4
108 -y+3/4,-z+3/4,+x
109 +y+1/2,-z+3/4,-x+1/4
110 -x+3/4,+y,-z+3/4
111 -z+1/4,-x+1/4,+y
112 +x+1/2,-y+1/4,-z+3/4
-101 -x,-y+1/2,-z+1/2
-102 -z,-x+1/2,-y+1/2
-103 -y,-z+1/2,-x+1/2
-104 -x+3/4,-y+1/4,+z+1/2
-105 +z,-x+1/4,-y+1/4
-106 -y+3/4,+z+1/2,-x+1/4
-107 +z+3/4,-x,+y+3/4
-108 +y+1/4,+z+1/4,-x
-109 -y+1/2,+z+1/4,+x+3/4
-110 +x+1/4,-y,+z+1/4
-111 +z+3/4,+x+3/4,-y
-112 -x+1/2,+y+3/4,+z+1/4
201 +x+1/2,+y,+z+1/2
202 +z+1/2,+x,+y+1/2
203 +y+1/2,+z,+x+1/2
204 +x+3/4,+y+1/4,-z+1/2
205 -z+1/2,+x+1/4,+y+3/4
206 +y+3/4,-z,+x+3/4
207 -z+3/4,+x+1/2,-y+1/4
208 -y+1/4,-z+1/4,+x
209 +y,-z+1/4,-x+1/4
210 -x+1/4,+y+1/2,-z+3/4
211 -z+3/4,-x+3/4,+y
212 +x,-y+3/4,-z+3/4
-201 -x+1/2,-y,-z+1/2
-202 -z+1/2,-x,-y+1/2
-203 -y+1/2,-z,-x+1/2
-204 -x+1/4,-y+3/4,+z+1/2
-205 +z+1/2,-x+3/4,-y+1/4
-206 -y+1/4,+z,-x+1/4
-207 +z+1/4,-x+1/2,+y+3/4
-208 +y+3/4,+z+3/4,-x
-209 -y,+z+3/4,+x+3/4
-210 +x+3/4,-y+1/2,+z+1/4
-211 +z+1/4,+x+1/4,-y
-212 -x,+y+1/4,+z+1/4
301 +x+1/2,+y+1/2,+z
302 +z+1/2,+x+1/2,+y
303 +y+1/2,+z+1/2,+x
304 +x+3/4,+y+3/4,-z
305 -z+1/2,+x+3/4,+y+1/4
306 +y+3/4,-z+1/2,+x+1/4
307 -z+3/4,+x,-y+3/4
308 -y+1/4,-z+3/4,+x+1/2
309 +y,-z+3/4,-x+3/4
310 -x+1/4,+y,-z+1/4
311 -z+3/4,-x+1/4,+y+1/2
312 +x,-y+1/4,-z+1/4
-301 -x+1/2,-y+1/2,-z
-302 -z+1/2,-x+1/2,-y
-303 -y+1/2,-z+1/2,-x
-304 -x+1/4,-y+1/4,+z
-305 +z+1/2,-x+1/4,-y+3/4
-306 -y+1/4,+z+1/2,-x+3/4
-307 +z+1/4,-x,+y+1/4
-308 +y+3/4,+z+1/4,-x+1/2
-309 -y,+z+1/4,+x+1/4
-310 +x+3/4,-y,+z+3/4
-311 +z+1/4,+x+3/4,-y+1/2
-312 -x,+y+3/4,+z+3/4
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
Si Si1 0.12214(23) -0.05384(22) 0.03803(20) 1.0 Uiso 0.0061(5) 96
Si Si2 -0.05452(24) 0.12641(23) 0.03309(23) 0.0826 Uiso 0.0061(5) 96
Al Al1 -0.05452(24) 0.12641(23) 0.03309(23) 0.9174 Uiso 0.0061(5) 96
O O1 0.10771(15) -0.10417(15) -0.00014(34) 1.0 Uiso 0.02207(24) 96
O O2 0.17697(15) 0.17348(17) -0.03397(11) 1.0 Uiso 0.02207(24) 96
O O3 -0.00073(16) -0.00281(16) 0.14308(10) 1.0 Uiso 0.02207(24) 96
O O4 0.18229(14) 0.17597(15) 0.31919(12) 1.0 Uiso 0.02207(24) 96
Na SI 0.0 0.0 0.0 0.223(17) Uiso 0.0241 16
Na SI' 0.05105(20) 0.05105(20) 0.05105(20) 0.825(12) Uiso 0.0241 32
Na SII 0.23158(19) 0.23158(19) 0.23158(19) 0.937(12) Uiso 0.0241 32
Na SJ 0.1973(13) 0.0383(12) -0.1365(11) 0.176(9) Uiso 0.0241 96
O Oc 0.1878(5) -0.0155(7) -0.1693(4) 0.2110(23) Uiso 0.07453 96
D Dc1 0.2079(7) 0.0131(8) -0.1849(8) 0.2110(23) Uiso 0.07453 96
D Dc2 0.1565(5) 0.0014(9) -0.1551(7) 0.2110(23) Uiso 0.07453 96
O Od 0.2140(21) 0.0303(22) -0.1440(19) 0.0454(23) Uiso 0.07453 96
D Dd1 0.2371(30) -0.0002(27) -0.1445(33) 0.0454(23) Uiso 0.07453 96
D Dd2 0.211(4) 0.040(4) -0.1070(23) 0.0454(23) Uiso 0.07453 96
O OII' 0.1605(11) 0.1605(11) 0.1605(11) 0.0834(20) Uiso 0.07453 32
D DII'1 0.1342(23) 0.156(4) 0.1878(20) 0.0279(7) Uiso 0.07453 96
D DII'2 0.1452(25) 0.1442(32) 0.1295(20) 0.0279(7) Uiso 0.07453 96
O OII* 0.2923(19) 0.2923(19) 0.2923(19) 0.068(4) Uiso 0.07453 32
D DII*1 0.2613(32) 0.295(7) 0.314(5) 0.0227(12) Uiso 0.07453 96
D DII*2 0.319(4) 0.314(6) 0.310(7) 0.0227(12) Uiso 0.07453 96
O Of 0.1333(13) 0.1624(11) -0.1805(14) 0.0640(19) Uiso 0.07453 96
D Df1 0.1140(19) 0.1692(23) -0.2128(15) 0.0640(19) Uiso 0.07453 96
D Df2 0.1318(22) 0.1955(17) -0.1613(20) 0.0640(19) Uiso 0.07453 96
O Oe 0.2936(13) 0.0872(10) -0.2170(13) 0.0752(23) Uiso 0.07453 96
D De1 0.3248(16) 0.0689(21) -0.2293(21) 0.0752(23) Uiso 0.07453 96
D De2 0.2971(20) 0.0875(25) -0.1789(13) 0.0752(23) Uiso 0.07453 96
Na SIII 0.375 0.375 0.1281(27) 0.086(8) Uiso 0.0241 48
loop_
_atom_type_symbol
_atom_type_number_in_cell
_atom_type_scat_length_neutron
_atom_type_scat_source
Si 103.93 0.4149 International_Tables_Vol_C
Al 88.07 0.3449 International_Tables_Vol_C
O 426.82 0.5803 International_Tables_Vol_C
Na 81.031 0.3630 International_Tables_Vol_C
D 85.674 0.6671 International_Tables_Vol_C
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Si2 Si1 Si2 122.74(29) 2_555 . 3_555 N
Si2 Si1 Si2 90.81(22) 2_555 . -1_555 N
Si2 Si1 Si2 93.14(22) 2_555 . 107_533 N
Si2 Si1 Al1 0.0 2_555 . 2_555 N
Si2 Si1 Al1 122.74(29) 2_555 . 3_555 N
Si2 Si1 Al1 90.81(22) 2_555 . -1_555 N
Si2 Si1 Al1 93.14(22) 2_555 . 107_443 N
Si2 Si1 O1 104.6(4) 2_555 . 1_555 N
Si2 Si1 O1 26.28(14) 2_555 . -2_555 N
Si2 Si1 O1 125.21(22) 2_555 . -3_555 N
Si2 Si1 O2 65.77(17) 2_555 . 3_555 N
Si2 Si1 O2 97.09(21) 2_555 . 105_544 N
Si2 Si1 O2 20.66(17) 2_555 . -206_444 N
Si2 Si1 O2 96.07(20) 2_555 . -304_444 N
Si2 Si1 O3 128.74(32) 2_555 . 2_555 N
Si2 Si1 O3 67.45(18) 2_555 . -3_555 N
Si2 Si1 O3 106.16(20) 2_555 . 310_334 N
Si2 Si1 O4 27.27(13) 2_555 . 208_343 N
Si2 Si1 O4 105.76(29) 2_555 . 209_343 N
Si2 Si1 SI 64.57(16) 2_555 . 1_555 N
Si2 Si1 SI' 62.38(17) 2_555 . 1_555 N
Si2 Si1 SII 133.86(27) 2_555 . -105_566 N
Si2 Si1 SJ 115.4(6) 2_555 . -206_556 N
Si2 Si1 Oc 109.76(31) 2_555 . -2_555 N
Si2 Si1 Si2 90.06(21) 3_555 . -1_555 N
Si2 Si1 Si2 117.83(30) 3_555 . 107_533 N
Si2 Si1 Al1 122.74(29) 3_555 . 2_555 N
Si2 Si1 Al1 0.0 3_555 . 3_555 N
Si2 Si1 Al1 90.06(21) 3_555 . -1_555 N
Si2 Si1 Al1 117.83(30) 3_555 . 107_443 N
Si2 Si1 O1 96.3(4) 3_555 . 1_555 N
Si2 Si1 O1 126.79(24) 3_555 . -2_555 N
Si2 Si1 O1 24.38(16) 3_555 . -3_555 N
Si2 Si1 O2 125.08(23) 3_555 . 3_555 N
Si2 Si1 O2 62.49(17) 3_555 . 105_544 N
Si2 Si1 O2 102.76(31) 3_555 . -206_444 N
Si2 Si1 O2 26.78(13) 3_555 . -304_444 N
Si2 Si1 O3 17.90(16) 3_555 . 2_555 N
Si2 Si1 O3 104.29(20) 3_555 . -3_555 N
Si2 Si1 O3 94.06(20) 3_555 . 310_334 N
Si2 Si1 O4 140.07(23) 3_555 . 208_343 N
Si2 Si1 O4 118.58(33) 3_555 . 209_343 N
Si2 Si1 SI 64.19(15) 3_555 . 1_555 N
Si2 Si1 SI' 61.95(16) 3_555 . 1_555 N
Si2 Si1 SII 59.45(16) 3_555 . -105_566 N
Si2 Si1 SJ 121.6(6) 3_555 . -206_556 N
Si2 Si1 Oc 120.81(33) 3_555 . -2_555 N
Si2 Si1 Si2 142.99(31) -1_555 . 107_533 N
Si2 Si1 Al1 90.81(22) -1_555 . 2_555 N
Si2 Si1 Al1 90.06(21) -1_555 . 3_555 N
Si2 Si1 Al1 0.0 -1_555 . -1_555 N
Si2 Si1 Al1 142.99(31) -1_555 . 107_443 N
Si2 Si1 O1 21.80(19) -1_555 . 1_555 N
Si2 Si1 O1 65.78(16) -1_555 . -2_555 N
Si2 Si1 O1 66.34(17) -1_555 . -3_555 N
Si2 Si1 O2 144.21(19) -1_555 . 3_555 N
Si2 Si1 O2 29.43(13) -1_555 . 105_544 N
Si2 Si1 O2 96.55(29) -1_555 . -206_444 N
Si2 Si1 O2 93.06(18) -1_555 . -304_444 N
Si2 Si1 O3 106.03(25) -1_555 . 2_555 N
Si2 Si1 O3 23.46(13) -1_555 . -3_555 N
Si2 Si1 O3 156.49(24) -1_555 . 310_334 N
Si2 Si1 O4 108.41(18) -1_555 . 208_343 N
Si2 Si1 O4 126.85(34) -1_555 . 209_343 N
Si2 Si1 SI 65.39(16) -1_555 . 1_555 N
Si2 Si1 SI' 103.89(26) -1_555 . 1_555 N
Si2 Si1 SII 134.03(21) -1_555 . -105_566 N
Si2 Si1 SJ 94.2(6) -1_555 . -206_556 N
Si2 Si1 Oc 62.37(27) -1_555 . -2_555 N
Si2 Si1 Al1 93.14(22) 107_443 . 2_555 N
Si2 Si1 Al1 117.83(30) 107_443 . 3_555 N
Si2 Si1 Al1 142.99(31) 107_443 . -1_555 N
Si2 Si1 Al1 0.0 107_443 . 107_443 N
Si2 Si1 O1 123.77(34) 107_433 . 1_555 N
Si2 Si1 O1 107.98(21) 107_433 . -2_555 N
Si2 Si1 O1 135.34(24) 107_433 . -3_555 N
Si2 Si1 O2 28.69(13) 107_433 . 3_555 N
Si2 Si1 O2 167.03(24) 107_433 . 105_544 N
Si2 Si1 O2 99.95(30) 107_433 . -206_444 N
Si2 Si1 O2 122.99(23) 107_433 . -304_444 N
Si2 Si1 O3 99.93(29) 107_433 . 2_555 N
Si2 Si1 O3 137.41(23) 107_433 . -3_555 N
Si2 Si1 O3 23.86(14) 107_433 . 310_334 N
Si2 Si1 O4 66.46(17) 107_433 . 208_343 N
Si2 Si1 O4 18.94(18) 107_433 . 209_343 N
Si2 Si1 SI 147.02(23) 107_433 . 1_555 N
Si2 Si1 SI' 110.50(27) 107_433 . 1_555 N
Si2 Si1 SII 59.30(16) 107_555 . -105_566 N
Si2 Si1 SJ 51.3(6) 107_545 . -206_556 N
Si2 Si1 Oc 81.77(29) 107_545 . -2_555 N
Al1 Si1 Al1 122.74(29) 2_555 . 3_555 N
Al1 Si1 Al1 90.81(22) 2_555 . -1_555 N
Al1 Si1 Al1 93.14(22) 2_555 . 107_443 N
Al1 Si1 O1 104.6(4) 2_555 . 1_555 N
Al1 Si1 O1 26.28(14) 2_555 . -2_555 N
Al1 Si1 O1 125.21(22) 2_555 . -3_555 N
Al1 Si1 O2 65.77(17) 2_555 . 3_555 N
Al1 Si1 O2 97.09(21) 2_555 . 105_544 N
Al1 Si1 O2 20.66(17) 2_555 . -206_444 N
Al1 Si1 O2 96.07(20) 2_555 . -304_444 N
Al1 Si1 O3 128.74(32) 2_555 . 2_555 N
Al1 Si1 O3 67.45(18) 2_555 . -3_555 N
Al1 Si1 O3 106.16(20) 2_555 . 310_334 N
Al1 Si1 O4 27.27(13) 2_555 . 208_343 N
Al1 Si1 O4 105.76(29) 2_555 . 209_343 N
Al1 Si1 SI 64.57(16) 2_555 . 1_555 N
Al1 Si1 SI' 62.38(17) 2_555 . 1_555 N
Al1 Si1 SII 133.86(27) 2_555 . -105_566 N
Al1 Si1 SJ 115.4(6) 2_555 . -206_556 N
Al1 Si1 Oc 109.76(31) 2_555 . -2_555 N
Al1 Si1 Al1 90.06(21) 3_555 . -1_555 N
Al1 Si1 Al1 117.83(30) 3_555 . 107_443 N
Al1 Si1 O1 96.3(4) 3_555 . 1_555 N
Al1 Si1 O1 126.79(24) 3_555 . -2_555 N
Al1 Si1 O1 24.38(16) 3_555 . -3_555 N
Al1 Si1 O2 125.08(23) 3_555 . 3_555 N
Al1 Si1 O2 62.49(17) 3_555 . 105_544 N
Al1 Si1 O2 102.76(31) 3_555 . -206_444 N
Al1 Si1 O2 26.78(13) 3_555 . -304_444 N
Al1 Si1 O3 17.90(16) 3_555 . 2_555 N
Al1 Si1 O3 104.29(20) 3_555 . -3_555 N
Al1 Si1 O3 94.06(20) 3_555 . 310_334 N
Al1 Si1 O4 140.07(23) 3_555 . 208_343 N
Al1 Si1 O4 118.58(33) 3_555 . 209_343 N
Al1 Si1 SI 64.19(15) 3_555 . 1_555 N
Al1 Si1 SI' 61.95(16) 3_555 . 1_555 N
Al1 Si1 SII 59.45(16) 3_555 . -105_566 N
Al1 Si1 SJ 121.6(6) 3_555 . -206_556 N
Al1 Si1 Oc 120.81(33) 3_555 . -2_555 N
Al1 Si1 Al1 142.99(31) -1_555 . 107_443 N
Al1 Si1 O1 21.80(19) -1_555 . 1_555 N
Al1 Si1 O1 65.78(16) -1_555 . -2_555 N
Al1 Si1 O1 66.34(17) -1_555 . -3_555 N
Al1 Si1 O2 144.21(19) -1_555 . 3_555 N
Al1 Si1 O2 29.43(13) -1_555 . 105_544 N
Al1 Si1 O2 96.55(29) -1_555 . -206_444 N
Al1 Si1 O2 93.06(18) -1_555 . -304_444 N
Al1 Si1 O3 106.03(25) -1_555 . 2_555 N
Al1 Si1 O3 23.46(13) -1_555 . -3_555 N
Al1 Si1 O3 156.49(24) -1_555 . 310_334 N
Al1 Si1 O4 108.41(18) -1_555 . 208_343 N
Al1 Si1 O4 126.85(34) -1_555 . 209_343 N
Al1 Si1 SI 65.39(16) -1_555 . 1_555 N
Al1 Si1 SI' 103.89(26) -1_555 . 1_555 N
Al1 Si1 SII 134.03(21) -1_555 . -105_566 N
Al1 Si1 SJ 94.2(6) -1_555 . -206_556 N
Al1 Si1 Oc 62.37(27) -1_555 . -2_555 N
Al1 Si1 O1 123.77(34) 107_433 . 1_555 N
Al1 Si1 O1 107.98(21) 107_433 . -2_555 N
Al1 Si1 O1 135.34(24) 107_433 . -3_555 N
Al1 Si1 O2 28.69(13) 107_433 . 3_555 N
Al1 Si1 O2 167.03(24) 107_433 . 105_544 N
Al1 Si1 O2 99.95(30) 107_433 . -206_444 N
Al1 Si1 O2 122.99(23) 107_433 . -304_444 N
Al1 Si1 O3 99.93(29) 107_433 . 2_555 N
Al1 Si1 O3 137.41(23) 107_433 . -3_555 N
Al1 Si1 O3 23.86(14) 107_433 . 310_334 N
Al1 Si1 O4 66.46(17) 107_433 . 208_343 N
Al1 Si1 O4 18.94(18) 107_433 . 209_343 N
Al1 Si1 SI 147.02(23) 107_433 . 1_555 N
Al1 Si1 SI' 110.50(27) 107_433 . 1_555 N
Al1 Si1 SII 59.30(16) 107_555 . -105_566 N
Al1 Si1 SJ 51.3(6) 107_545 . -206_556 N
Al1 Si1 Oc 81.77(29) 107_545 . -2_555 N
O1 Si1 O1 78.36(29) 1_555 . -2_555 N
O1 Si1 O1 72.16(24) 1_555 . -3_555 N
O1 Si1 O2 136.68(34) 1_555 . 3_555 N
O1 Si1 O2 45.60(23) 1_555 . 105_544 N
O1 Si1 O2 115.2(4) 1_555 . -206_444 N
O1 Si1 O2 107.79(32) 1_555 . -304_444 N
O1 Si1 O3 108.1(4) 1_555 . 2_555 N
O1 Si1 O3 39.89(23) 1_555 . -3_555 N
O1 Si1 O3 134.77(29) 1_555 . 310_334 N
O1 Si1 O4 114.1(4) 1_555 . 208_343 N
O1 Si1 O4 106.1(4) 1_555 . 209_343 N
O1 Si1 SI 86.79(24) 1_555 . 1_555 N
O1 Si1 SI' 125.14(32) 1_555 . 1_555 N
O1 Si1 SII 121.3(4) 1_555 . -105_566 N
O1 Si1 SJ 73.1(6) 1_555 . -206_556 N
O1 Si1 Oc 42.00(31) 1_555 . -2_555 N
O1 Si1 O1 116.40(20) -2_555 . -3_555 N
O1 Si1 O2 85.22(16) -2_555 . 3_555 N
O1 Si1 O2 78.80(15) -2_555 . 105_544 N
O1 Si1 O2 41.24(20) -2_555 . -206_444 N
O1 Si1 O2 104.37(17) -2_555 . -304_444 N
O1 Si1 O3 140.97(29) -2_555 . 2_555 N
O1 Si1 O3 42.35(11) -2_555 . -3_555 N
O1 Si1 O3 127.11(16) -2_555 . 310_334 N
O1 Si1 O4 44.47(11) -2_555 . 208_343 N
O1 Si1 O4 113.61(27) -2_555 . 209_343 N
O1 Si1 SI 62.67(13) -2_555 . 1_555 N
O1 Si1 SI' 78.18(16) -2_555 . 1_555 N
O1 Si1 SII 159.94(22) -2_555 . -105_566 N
O1 Si1 SJ 107.5(6) -2_555 . -206_556 N
O1 Si1 Oc 90.07(24) -2_555 . -2_555 N
O1 Si1 O2 149.27(20) -3_555 . 3_555 N
O1 Si1 O2 40.91(12) -3_555 . 105_544 N
O1 Si1 O2 109.70(28) -3_555 . -206_444 N
O1 Si1 O2 41.37(13) -3_555 . -304_444 N
O1 Si1 O3 39.75(19) -3_555 . 2_555 N
O1 Si1 O3 83.40(16) -3_555 . -3_555 N
O1 Si1 O3 113.38(17) -3_555 . 310_334 N
O1 Si1 O4 151.37(18) -3_555 . 208_343 N
O1 Si1 O4 128.14(28) -3_555 . 209_343 N
O1 Si1 SI 60.65(10) -3_555 . 1_555 N
O1 Si1 SI' 75.35(16) -3_555 . 1_555 N
O1 Si1 SII 76.65(13) -3_555 . -105_566 N
O1 Si1 SJ 115.3(6) -3_555 . -206_556 N
O1 Si1 Oc 102.30(31) -3_555 . -2_555 N
O2 Si1 O2 162.85(18) 3_555 . 105_544 N
O2 Si1 O2 71.29(25) 3_555 . -206_444 N
O2 Si1 O2 115.08(16) 3_555 . -304_444 N
O2 Si1 O3 109.74(26) 3_555 . 2_555 N
O2 Si1 O3 124.74(17) 3_555 . -3_555 N
O2 Si1 O3 41.91(10) 3_555 . 310_334 N
O2 Si1 O4 40.89(11) 3_555 . 208_343 N
O2 Si1 O4 45.96(20) 3_555 . 209_343 N
O2 Si1 SI 120.36(17) 3_555 . 1_555 N
O2 Si1 SI' 89.26(19) 3_555 . 1_555 N
O2 Si1 SII 77.38(15) 3_555 . -105_566 N
O2 Si1 SJ 74.2(6) 3_555 . -206_556 N
O2 Si1 Oc 99.04(29) 3_555 . -2_555 N
O2 Si1 O2 92.38(28) 105_544 . -206_444 N
O2 Si1 O2 63.86(12) 105_544 . -304_444 N
O2 Si1 O3 79.80(21) 105_544 . 2_555 N
O2 Si1 O3 42.53(11) 105_544 . -3_555 N
O2 Si1 O3 153.73(18) 105_544 . 310_334 N
O2 Si1 O4 122.54(18) 105_544 . 208_343 N
O2 Si1 O4 148.20(30) 105_544 . 209_343 N
O2 Si1 SI 45.87(8) 105_544 . 1_555 N
O2 Si1 SI' 81.45(19) 105_544 . 1_555 N
O2 Si1 SII 117.04(16) 105_544 . -105_566 N
O2 Si1 SJ 116.5(6) 105_544 . -206_556 N
O2 Si1 Oc 87.27(27) 105_544 . -2_555 N
O2 Si1 O2 75.98(26) -206_444 . -304_444 N
O2 Si1 O3 108.14(35) -206_444 . 2_555 N
O2 Si1 O3 75.34(25) -206_444 . -3_555 N
O2 Si1 O3 105.05(28) -206_444 . 310_334 N
O2 Si1 O4 41.73(19) -206_444 . 208_343 N
O2 Si1 O4 116.5(4) -206_444 . 209_343 N
O2 Si1 SI 51.03(21) -206_444 . 1_555 N
O2 Si1 SI' 41.73(18) -206_444 . 1_555 N
O2 Si1 SII 121.73(32) -206_566 . -105_566 N
O2 Si1 SJ 134.3(7) -206_556 . -206_556 N
O2 Si1 Oc 129.8(4) -206_556 . -2_555 N
O2 Si1 O3 36.61(16) -304_444 . 2_555 N
O2 Si1 O3 97.37(14) -304_444 . -3_555 N
O2 Si1 O3 101.00(15) -304_444 . 310_334 N
O2 Si1 O4 114.72(15) -304_444 . 208_343 N
O2 Si1 O4 133.04(29) -304_444 . 209_343 N
O2 Si1 SI 43.62(8) -304_444 . 1_555 N
O2 Si1 SI' 35.67(8) -304_444 . 1_555 N
O2 Si1 SII 74.78(14) -304_566 . -105_566 N
O2 Si1 SJ 147.5(6) -304_556 . -206_556 N
O2 Si1 Oc 143.62(31) -304_556 . -2_555 N
O3 Si1 O3 122.01(26) 2_555 . -3_555 N
O3 Si1 O3 76.19(24) 2_555 . 310_334 N
O3 Si1 O4 135.98(27) 2_555 . 208_343 N
O3 Si1 O4 101.67(35) 2_555 . 209_343 N
O3 Si1 SI 79.02(20) 2_555 . 1_555 N
O3 Si1 SI' 66.60(20) 2_555 . 1_555 N
O3 Si1 SII 41.88(16) 2_555 . -105_566 N
O3 Si1 SJ 111.2(6) 2_555 . -206_556 N
O3 Si1 Oc 121.1(4) 2_555 . -2_555 N
O3 Si1 O3 161.16(17) -3_555 . 310_334 N
O3 Si1 O4 85.77(14) -3_555 . 208_343 N
O3 Si1 O4 129.28(28) -3_555 . 209_343 N
O3 Si1 SI 58.34(10) -3_555 . 1_555 N
O3 Si1 SI' 94.00(20) -3_555 . 1_555 N
O3 Si1 SII 157.20(19) -3_555 . -105_566 N
O3 Si1 SJ 101.8(5) -3_555 . -206_556 N
O3 Si1 Oc 71.05(22) -3_555 . -2_555 N
O3 Si1 O4 82.78(13) 310_334 . 208_343 N
O3 Si1 O4 33.30(19) 310_334 . 209_343 N
O3 Si1 SI 136.57(17) 310_334 . 1_555 N
O3 Si1 SI' 98.45(22) 310_334 . 1_555 N
O3 Si1 SII 36.80(8) 310_456 . -105_566 N
O3 Si1 SJ 64.0(5) 310_446 . -206_556 N
O3 Si1 Oc 96.02(24) 310_446 . -2_555 N
O4 Si1 O4 78.52(23) 208_343 . 209_343 N
O4 Si1 SI 91.18(14) 208_343 . 1_555 N
O4 Si1 SI' 79.08(13) 208_343 . 1_555 N
O4 Si1 SII 117.01(18) 208_465 . -105_566 N
O4 Si1 SJ 92.8(6) 208_455 . -206_556 N
O4 Si1 Oc 99.07(29) 208_455 . -2_555 N
O4 Si1 SI 165.93(31) 209_343 . 1_555 N
O4 Si1 SI' 128.73(34) 209_343 . 1_555 N
O4 Si1 SII 60.00(22) 209_465 . -105_566 N
O4 Si1 SJ 33.0(6) 209_455 . -206_556 N
O4 Si1 Oc 64.49(30) 209_455 . -2_555 N
SI Si1 SI' 38.51(16) 1_555 . 1_555 N
SI Si1 SII 118.32(17) 1_555 . -105_566 N
SI Si1 SJ 159.4(6) 1_555 . -206_556 N
SI Si1 Oc 127.36(26) 1_555 . -2_555 N
SI' Si1 SII 91.55(22) 1_555 . -105_566 N
SI' Si1 SJ 161.7(6) 1_555 . -206_556 N
SI' Si1 Oc 165.05(31) 1_555 . -2_555 N
SII Si1 SJ 77.4(5) -105_556 . -206_556 N
SII Si1 Oc 102.35(26) -105_556 . -2_555 N
SJ Si1 Oc 32.0(6) -206_556 . -2_555 N
Si1 Si2 Si1 117.26(29) 2_555 . 3_555 N
Si1 Si2 Si1 89.13(22) 2_555 . -1_555 N
Si1 Si2 Si1 121.77(30) 2_555 . 209_344 N
Si1 Si2 O1 25.64(16) 2_555 . 2_555 N
Si1 Si2 O1 122.34(23) 2_555 . 3_555 N
Si1 Si2 O1 103.5(4) 2_555 . -1_555 N
Si1 Si2 O2 123.34(24) 2_555 . 2_555 N
Si1 Si2 O2 100.38(29) 2_555 . -105_444 N
Si1 Si2 O2 65.22(17) 2_555 . 206_454 N
Si1 Si2 O2 22.90(13) 2_555 . -304_444 N
Si1 Si2 O3 19.70(17) 2_555 . 3_555 N
Si1 Si2 O3 104.63(21) 2_555 . -2_555 N
Si1 Si2 O3 95.73(21) 2_555 . 312_334 N
Si1 Si2 O4 124.96(33) 2_555 . 107_433 N
Si1 Si2 O4 133.33(23) 2_555 . 111_433 N
Si1 Si2 SI 61.94(16) 2_555 . 1_555 N
Si1 Si2 SI' 59.15(16) 2_555 . 1_555 N
Si1 Si2 SII 62.42(17) 2_555 . 107_555 N
Si1 Si2 SJ 127.3(7) 2_555 . 2_555 N
Si1 Si2 Oc 112.18(33) 2_555 . 2_555 N
Si1 Si2 Dc1 122.8(4) 2_555 . 2_555 N
Si1 Si2 Dc2 118.6(6) 2_555 . 2_555 N
Si1 Si2 Od 121.9(10) 2_555 . 2_555 N
Si1 Si2 Dd1 108.5(12) 2_555 . 2_555 N
Si1 Si2 Si1 89.87(22) 3_555 . -1_555 N
Si1 Si2 Si1 86.86(22) 3_555 . 209_344 N
Si1 Si2 O1 124.34(23) 3_555 . 2_555 N
Si1 Si2 O1 23.84(14) 3_555 . 3_555 N
Si1 Si2 O1 96.9(4) 3_555 . -1_555 N
Si1 Si2 O2 64.80(17) 3_555 . 2_555 N
Si1 Si2 O2 17.39(15) 3_555 . -105_444 N
Si1 Si2 O2 94.15(20) 3_555 . 206_454 N
Si1 Si2 O2 94.42(20) 3_555 . -304_444 N
Si1 Si2 O3 123.65(34) 3_555 . 3_555 N
Si1 Si2 O3 64.86(17) 3_555 . -2_555 N
Si1 Si2 O3 103.48(21) 3_555 . 312_334 N
Si1 Si2 O4 98.44(29) 3_555 . 107_433 N
Si1 Si2 O4 23.14(12) 3_555 . 111_433 N
Si1 Si2 SI 62.28(15) 3_555 . 1_555 N
Si1 Si2 SI' 59.53(16) 3_555 . 1_555 N
Si1 Si2 SII 130.76(28) 3_555 . 107_555 N
Si1 Si2 SJ 115.5(7) 3_555 . 2_555 N
Si1 Si2 Oc 124.33(33) 3_555 . 2_555 N
Si1 Si2 Dc1 117.8(4) 3_555 . 2_555 N
Si1 Si2 Dc2 113.8(5) 3_555 . 2_555 N
Si1 Si2 Od 120.8(10) 3_555 . 2_555 N
Si1 Si2 Dd1 134.2(12) 3_555 . 2_555 N
Si1 Si2 Si1 146.50(30) -1_555 . 209_344 N
Si1 Si2 O1 65.81(18) -1_555 . 2_555 N
Si1 Si2 O1 67.53(16) -1_555 . 3_555 N
Si1 Si2 O1 21.24(19) -1_555 . -1_555 N
Si1 Si2 O2 144.91(20) -1_555 . 2_555 N
Si1 Si2 O2 93.96(27) -1_555 . -105_444 N
Si1 Si2 O2 25.11(13) -1_555 . 206_454 N
Si1 Si2 O2 90.72(20) -1_555 . -304_444 N
Si1 Si2 O3 107.13(30) -1_555 . 3_555 N
Si1 Si2 O3 25.50(12) -1_555 . -2_555 N
Si1 Si2 O3 161.60(24) -1_555 . 312_334 N
Si1 Si2 O4 133.74(34) -1_555 . 107_433 N
Si1 Si2 O4 105.03(18) -1_555 . 111_433 N
Si1 Si2 SI 63.02(16) -1_555 . 1_555 N
Si1 Si2 SI' 100.62(26) -1_555 . 1_555 N
Si1 Si2 SII 137.11(22) -1_555 . 107_555 N
Si1 Si2 SJ 89.9(8) -1_555 . 2_555 N
Si1 Si2 Oc 66.52(29) -1_555 . 2_555 N
Si1 Si2 Dc1 76.80(32) -1_555 . 2_555 N
Si1 Si2 Dc2 59.1(4) -1_555 . 2_555 N
Si1 Si2 Od 90.4(10) -1_555 . 2_555 N
Si1 Si2 Dd1 88.7(13) -1_555 . 2_555 N
Si1 Si2 O1 140.07(25) 209_343 . 2_555 N
Si1 Si2 O1 101.03(21) 209_343 . 3_555 N
Si1 Si2 O1 126.7(4) 209_343 . -1_555 N
Si1 Si2 O2 23.44(13) 209_343 . 2_555 N
Si1 Si2 O2 92.73(28) 209_343 . -105_444 N
Si1 Si2 O2 171.37(27) 209_343 . 206_454 N
Si1 Si2 O2 122.76(24) 209_343 . -304_444 N
Si1 Si2 O3 102.32(31) 209_343 . 3_555 N
Si1 Si2 O3 133.15(24) 209_343 . -2_555 N
Si1 Si2 O3 26.32(13) 209_343 . 312_334 N
Si1 Si2 O4 16.89(15) 209_343 . 107_433 N
Si1 Si2 O4 64.56(17) 209_343 . 111_433 N
Si1 Si2 SI 140.32(24) 209_343 . 1_555 N
Si1 Si2 SI' 106.23(26) 209_343 . 1_555 N
Si1 Si2 SII 62.26(16) 209_465 . 107_555 N
Si1 Si2 SJ 62.0(7) 209_455 . 2_555 N
Si1 Si2 Oc 88.14(31) 209_455 . 2_555 N
Si1 Si2 Dc1 75.40(31) 209_464 . 2_555 N
Si1 Si2 Dc2 92.0(5) 209_465 . 2_555 N
Si1 Si2 Od 63.4(11) 209_464 . 2_555 N
Si1 Si2 Dd1 70.5(12) 209_443 . 2_555 N
O1 Si2 O1 117.28(20) 2_555 . 3_555 N
O1 Si2 O1 78.05(26) 2_555 . -1_555 N
O1 Si2 O2 148.42(23) 2_555 . 2_555 N
O1 Si2 O2 111.08(27) 2_555 . -105_444 N
O1 Si2 O2 44.58(13) 2_555 . 206_454 N
O1 Si2 O2 41.21(14) 2_555 . -304_444 N
O1 Si2 O3 41.41(21) 2_555 . 3_555 N
O1 Si2 O3 85.84(16) 2_555 . -2_555 N
O1 Si2 O3 114.36(19) 2_555 . 312_334 N
O1 Si2 O4 135.08(29) 2_555 . 107_433 N
O1 Si2 O4 146.75(19) 2_555 . 111_433 N
O1 Si2 SI 62.07(12) 2_555 . 1_555 N
O1 Si2 SI' 76.09(18) 2_555 . 1_555 N
O1 Si2 SII 77.91(15) 2_555 . 107_555 N
O1 Si2 SJ 113.7(7) 2_555 . 2_555 N
O1 Si2 Oc 92.01(31) 2_555 . 2_555 N
O1 Si2 Dc1 104.75(34) 2_555 . 2_555 N
O1 Si2 Dc2 95.9(5) 2_555 . 2_555 N
O1 Si2 Od 109.2(10) 2_555 . 2_555 N
O1 Si2 Dd1 96.3(12) 2_555 . 2_555 N
O1 Si2 O1 73.08(29) 3_555 . -1_555 N
O1 Si2 O2 82.48(16) 3_555 . 2_555 N
O1 Si2 O2 36.30(18) 3_555 . -105_444 N
O1 Si2 O2 77.26(15) 3_555 . 206_454 N
O1 Si2 O2 102.26(16) 3_555 . -304_444 N
O1 Si2 O3 136.51(30) 3_555 . 3_555 N
O1 Si2 O3 42.06(11) 3_555 . -2_555 N
O1 Si2 O3 122.96(18) 3_555 . 312_334 N
O1 Si2 O4 107.43(28) 3_555 . 107_433 N
O1 Si2 O4 38.55(11) 3_555 . 111_433 N
O1 Si2 SI 60.47(12) 3_555 . 1_555 N
O1 Si2 SI' 73.89(15) 3_555 . 1_555 N
O1 Si2 SII 154.46(23) 3_555 . 107_555 N
O1 Si2 SJ 105.5(7) 3_555 . 2_555 N
O1 Si2 Oc 105.34(27) 3_555 . 2_555 N
O1 Si2 Dc1 102.8(4) 3_555 . 2_555 N
O1 Si2 Dc2 94.0(4) 3_555 . 2_555 N
O1 Si2 Od 110.7(9) 3_555 . 2_555 N
O1 Si2 Dd1 122.0(12) 3_555 . 2_555 N
O1 Si2 O2 133.2(4) -1_555 . 2_555 N
O1 Si2 O2 106.3(4) -1_555 . -105_444 N
O1 Si2 O2 44.71(25) -1_555 . 206_454 N
O1 Si2 O2 110.01(33) -1_555 . -304_444 N
O1 Si2 O3 118.2(4) -1_555 . 3_555 N
O1 Si2 O3 35.19(23) -1_555 . -2_555 N
O1 Si2 O3 141.51(31) -1_555 . 312_334 N
O1 Si2 O4 112.7(4) -1_555 . 107_433 N
O1 Si2 O4 104.7(4) -1_555 . 111_433 N
O1 Si2 SI 83.88(24) -1_555 . 1_555 N
O1 Si2 SI' 121.40(33) -1_555 . 1_555 N
O1 Si2 SII 132.1(4) -1_555 . 107_555 N
O1 Si2 SJ 68.7(8) -1_555 . 2_555 N
O1 Si2 Oc 46.61(29) -1_555 . 2_555 N
O1 Si2 Dc1 55.85(35) -1_555 . 2_555 N
O1 Si2 Dc2 38.2(4) -1_555 . 2_555 N
O1 Si2 Od 69.6(10) -1_555 . 2_555 N
O1 Si2 Dd1 69.4(13) -1_555 . 2_555 N
O2 Si2 O2 69.32(23) 2_555 . -105_444 N
O2 Si2 O2 158.95(18) 2_555 . 206_454 N
O2 Si2 O2 113.92(18) 2_555 . -304_444 N
O2 Si2 O3 107.15(29) 2_555 . 3_555 N
O2 Si2 O3 121.76(18) 2_555 . -2_555 N
O2 Si2 O3 40.51(10) 2_555 . 312_334 N
O2 Si2 O4 39.15(18) 2_555 . 107_433 N
O2 Si2 O4 44.08(11) 2_555 . 111_433 N
O2 Si2 SI 117.70(17) 2_555 . 1_555 N
O2 Si2 SI' 87.44(18) 2_555 . 1_555 N
O2 Si2 SII 75.81(15) 2_555 . 107_555 N
O2 Si2 SJ 80.7(7) 2_555 . 2_555 N
O2 Si2 Oc 106.87(30) 2_555 . 2_555 N
O2 Si2 Dc1 93.35(29) 2_555 . 2_555 N
O2 Si2 Dc2 107.6(5) 2_555 . 2_555 N
O2 Si2 Od 83.3(11) 2_555 . 2_555 N
O2 Si2 Dd1 92.4(12) 2_555 . 2_555 N
O2 Si2 O2 90.71(25) -105_444 . 206_454 N
O2 Si2 O2 77.48(24) -105_444 . -304_444 N
O2 Si2 O3 106.4(4) -105_444 . 3_555 N
O2 Si2 O3 71.49(22) -105_444 . -2_555 N
O2 Si2 O3 102.56(26) -105_444 . 312_334 N
O2 Si2 O4 107.23(34) -105_444 . 107_433 N
O2 Si2 O4 35.81(17) -105_444 . 111_433 N
O2 Si2 SI 50.77(18) -105_444 . 1_555 N
O2 Si2 SI' 42.14(16) -105_444 . 1_555 N
O2 Si2 SII 120.90(31) -105_566 . 107_555 N
O2 Si2 SJ 132.3(7) -105_556 . 2_555 N
O2 Si2 Oc 140.9(4) -105_556 . 2_555 N
O2 Si2 Dc1 135.2(4) -105_565 . 2_555 N
O2 Si2 Dc2 129.9(5) -105_566 . 2_555 N
O2 Si2 Od 137.5(10) -105_565 . 2_555 N
O2 Si2 Dd1 151.0(12) -105_544 . 2_555 N
O2 Si2 O2 65.75(14) 206_454 . -304_444 N
O2 Si2 O3 84.26(26) 206_454 . 3_555 N
O2 Si2 O3 41.26(11) 206_454 . -2_555 N
O2 Si2 O3 158.74(19) 206_454 . 312_334 N
O2 Si2 O4 155.63(30) 206_454 . 107_433 N
O2 Si2 O4 115.21(17) 206_454 . 111_433 N
O2 Si2 SI 46.05(9) 206_454 . 1_555 N
O2 Si2 SI' 81.56(20) 206_454 . 1_555 N
O2 Si2 SII 122.16(19) 206_454 . 107_555 N
O2 Si2 SJ 110.1(7) 206_454 . 2_555 N
O2 Si2 Oc 84.20(29) 206_454 . 2_555 N
O2 Si2 Dc1 96.62(31) 206_454 . 2_555 N
O2 Si2 Dc2 79.7(4) 206_454 . 2_555 N
O2 Si2 Od 109.1(11) 206_454 . 2_555 N
O2 Si2 Dd1 103.1(12) 206_454 . 2_555 N
O2 Si2 O3 34.61(18) -304_444 . 3_555 N
O2 Si2 O3 97.20(15) -304_444 . -2_555 N
O2 Si2 O3 100.65(16) -304_444 . 312_334 N
O2 Si2 O4 133.29(29) -304_444 . 107_433 N
O2 Si2 O4 111.11(15) -304_444 . 111_433 N
O2 Si2 SI 44.20(9) -304_444 . 1_555 N
O2 Si2 SI' 36.65(9) -304_444 . 1_555 N
O2 Si2 SII 75.13(15) -304_566 . 107_555 N
O2 Si2 SJ 150.1(6) -304_556 . 2_555 N
O2 Si2 Oc 132.99(31) -304_556 . 2_555 N
O2 Si2 Dc1 144.96(34) -304_565 . 2_555 N
O2 Si2 Dc2 136.9(5) -304_566 . 2_555 N
O2 Si2 Od 144.7(9) -304_565 . 2_555 N
O2 Si2 Dd1 131.4(12) -304_544 . 2_555 N
O3 Si2 O3 124.29(29) 3_555 . -2_555 N
O3 Si2 O3 76.14(26) 3_555 . 312_334 N
O3 Si2 O4 105.5(4) 3_555 . 107_433 N
O3 Si2 O4 131.42(30) 3_555 . 111_433 N
O3 Si2 SI 78.34(23) 3_555 . 1_555 N
O3 Si2 SI' 64.59(22) 3_555 . 1_555 N
O3 Si2 SII 43.09(18) 3_555 . 107_555 N
O3 Si2 SJ 117.8(7) 3_555 . 2_555 N
O3 Si2 Oc 111.6(4) 3_555 . 2_555 N
O3 Si2 Dc1 118.3(4) 3_555 . 2_555 N
O3 Si2 Dc2 121.1(6) 3_555 . 2_555 N
O3 Si2 Od 112.5(9) 3_555 . 2_555 N
O3 Si2 Dd1 100.3(12) 3_555 . 2_555 N
O3 Si2 O3 159.47(18) -2_555 . 312_334 N
O3 Si2 O4 128.88(28) -2_555 . 107_433 N
O3 Si2 O4 79.69(14) -2_555 . 111_433 N
O3 Si2 SI 57.07(10) -2_555 . 1_555 N
O3 Si2 SI' 91.18(20) -2_555 . 1_555 N
O3 Si2 SII 162.31(21) -2_555 . 107_555 N
O3 Si2 SJ 96.1(7) -2_555 . 2_555 N
O3 Si2 Oc 79.64(25) -2_555 . 2_555 N
O3 Si2 Dc1 85.49(32) -2_555 . 2_555 N
O3 Si2 Dc2 69.3(4) -2_555 . 2_555 N
O3 Si2 Od 98.8(10) -2_555 . 2_555 N
O3 Si2 Dd1 102.4(12) -2_555 . 2_555 N
O3 Si2 O4 32.66(17) 312_334 . 107_433 N
O3 Si2 O4 84.45(14) 312_334 . 111_433 N
O3 Si2 SI 134.54(18) 312_334 . 1_555 N
O3 Si2 SI' 97.09(21) 312_334 . 1_555 N
O3 Si2 SII 36.58(9) 312_456 . 107_555 N
O3 Si2 SJ 73.0(7) 312_446 . 2_555 N
O3 Si2 Oc 95.28(27) 312_446 . 2_555 N
O3 Si2 Dc1 85.70(30) 312_455 . 2_555 N
O3 Si2 Dc2 103.3(4) 312_456 . 2_555 N
O3 Si2 Od 71.9(10) 312_455 . 2_555 N
O3 Si2 Dd1 73.0(13) 312_434 . 2_555 N
O4 Si2 O4 75.32(23) 107_433 . 111_433 N
O4 Si2 SI 156.85(30) 107_433 . 1_555 N
O4 Si2 SI' 122.81(32) 107_433 . 1_555 N
O4 Si2 SII 62.54(20) 107_555 . 107_555 N
O4 Si2 SJ 45.6(7) 107_545 . 2_555 N
O4 Si2 Oc 71.46(32) 107_545 . 2_555 N
O4 Si2 Dc1 59.04(32) 107_554 . 2_555 N
O4 Si2 Dc2 76.2(4) 107_555 . 2_555 N
O4 Si2 Od 46.6(11) 107_554 . 2_555 N
O4 Si2 Dd1 53.7(12) 107_533 . 2_555 N
O4 Si2 SI 85.06(13) 111_433 . 1_555 N
O4 Si2 SI' 74.46(12) 111_433 . 1_555 N
O4 Si2 SII 117.85(20) 111_555 . 107_555 N
O4 Si2 SJ 97.5(6) 111_545 . 2_555 N
O4 Si2 Oc 114.27(29) 111_545 . 2_555 N
O4 Si2 Dc1 103.76(33) 111_554 . 2_555 N
O4 Si2 Dc2 106.5(5) 111_555 . 2_555 N
O4 Si2 Od 102.6(10) 111_554 . 2_555 N
O4 Si2 Dd1 115.9(12) 111_533 . 2_555 N
SI Si2 SI' 37.61(16) 1_555 . 1_555 N
SI Si2 SII 118.96(20) 1_555 . 107_555 N
SI Si2 SJ 152.3(7) 1_555 . 2_555 N
SI Si2 Oc 129.13(30) 1_555 . 2_555 N
SI Si2 Dc1 139.73(32) 1_555 . 2_555 N
SI Si2 Dc2 122.0(4) 1_555 . 2_555 N
SI Si2 Od 153.4(10) 1_555 . 2_555 N
SI Si2 Dd1 149.1(12) 1_555 . 2_555 N
SI' Si2 SII 91.66(24) 1_555 . 107_555 N
SI' Si2 SJ 168.1(7) 1_555 . 2_555 N
SI' Si2 Oc 165.55(35) 1_555 . 2_555 N
SI' Si2 Dc1 176.5(4) 1_555 . 2_555 N
SI' Si2 Dc2 159.6(4) 1_555 . 2_555 N
SI' Si2 Od 169.0(11) 1_555 . 2_555 N
SI' Si2 Dd1 164.0(12) 1_555 . 2_555 N
SII Si2 SJ 84.3(7) 107_545 . 2_555 N
SII Si2 Oc 93.84(29) 107_545 . 2_555 N
SII Si2 Dc1 91.9(4) 107_554 . 2_555 N
SII Si2 Dc2 105.2(4) 107_555 . 2_555 N
SII Si2 Od 80.3(9) 107_554 . 2_555 N
SII Si2 Dd1 72.8(12) 107_533 . 2_555 N
SJ Si2 Oc 26.3(7) 2_555 . 2_555 N
SJ Si2 Dc1 13.5(8) 2_555 . 2_555 N
SJ Si2 Dc2 30.9(8) 2_555 . 2_555 N
SJ Si2 Od 5.4(12) 2_555 . 2_555 N
SJ Si2 Dd1 18.8(13) 2_555 . 2_555 N
Oc Si2 Dc1 13.58(15) 2_555 . 2_555 N
Oc Si2 Dc2 11.48(26) 2_555 . 2_555 N
Oc Si2 Od 24.9(11) 2_555 . 2_555 N
Oc Si2 Dd1 22.9(12) 2_555 . 2_555 N
Dc1 Si2 Dc2 17.7(4) 2_555 . 2_555 N
Dc1 Si2 Od 13.8(10) 2_555 . 2_555 N
Dc1 Si2 Dd1 19.4(12) 2_555 . 2_555 N
Dc2 Si2 Od 31.4(10) 2_555 . 2_555 N
Dc2 Si2 Dd1 33.2(12) 2_555 . 2_555 N
Od Si2 Dd1 13.5(8) 2_555 . 2_555 N
Si1 Al1 Si1 117.26(29) 2_555 . 3_555 N
Si1 Al1 Si1 89.13(22) 2_555 . -1_555 N
Si1 Al1 Si1 121.77(30) 2_555 . 209_344 N
Si1 Al1 O1 25.64(16) 2_555 . 2_555 N
Si1 Al1 O1 122.34(23) 2_555 . 3_555 N
Si1 Al1 O1 103.5(4) 2_555 . -1_555 N
Si1 Al1 O2 123.34(24) 2_555 . 2_555 N
Si1 Al1 O2 100.38(29) 2_555 . -105_444 N
Si1 Al1 O2 65.22(17) 2_555 . 206_454 N
Si1 Al1 O2 22.90(13) 2_555 . -304_444 N
Si1 Al1 O3 19.70(17) 2_555 . 3_555 N
Si1 Al1 O3 104.63(21) 2_555 . -2_555 N
Si1 Al1 O3 95.73(21) 2_555 . 312_334 N
Si1 Al1 O4 124.96(33) 2_555 . 107_433 N
Si1 Al1 O4 133.33(23) 2_555 . 111_433 N
Si1 Al1 SI 61.94(16) 2_555 . 1_555 N
Si1 Al1 SI' 59.15(16) 2_555 . 1_555 N
Si1 Al1 SII 62.42(17) 2_555 . 107_555 N
Si1 Al1 SJ 127.3(7) 2_555 . 2_555 N
Si1 Al1 Oc 112.18(33) 2_555 . 2_555 N
Si1 Al1 Dc1 122.8(4) 2_555 . 2_555 N
Si1 Al1 Dc2 118.6(6) 2_555 . 2_555 N
Si1 Al1 Od 121.9(10) 2_555 . 2_555 N
Si1 Al1 Dd1 108.5(12) 2_555 . 2_555 N
Si1 Al1 Si1 89.87(22) 3_555 . -1_555 N
Si1 Al1 Si1 86.86(22) 3_555 . 209_344 N
Si1 Al1 O1 124.34(23) 3_555 . 2_555 N
Si1 Al1 O1 23.84(14) 3_555 . 3_555 N
Si1 Al1 O1 96.9(4) 3_555 . -1_555 N
Si1 Al1 O2 64.80(17) 3_555 . 2_555 N
Si1 Al1 O2 17.39(15) 3_555 . -105_444 N
Si1 Al1 O2 94.15(20) 3_555 . 206_454 N
Si1 Al1 O2 94.42(20) 3_555 . -304_444 N
Si1 Al1 O3 123.65(34) 3_555 . 3_555 N
Si1 Al1 O3 64.86(17) 3_555 . -2_555 N
Si1 Al1 O3 103.48(21) 3_555 . 312_334 N
Si1 Al1 O4 98.44(29) 3_555 . 107_433 N
Si1 Al1 O4 23.14(12) 3_555 . 111_433 N
Si1 Al1 SI 62.28(15) 3_555 . 1_555 N
Si1 Al1 SI' 59.53(16) 3_555 . 1_555 N
Si1 Al1 SII 130.76(28) 3_555 . 107_555 N
Si1 Al1 SJ 115.5(7) 3_555 . 2_555 N
Si1 Al1 Oc 124.33(33) 3_555 . 2_555 N
Si1 Al1 Dc1 117.8(4) 3_555 . 2_555 N
Si1 Al1 Dc2 113.8(5) 3_555 . 2_555 N
Si1 Al1 Od 120.8(10) 3_555 . 2_555 N
Si1 Al1 Dd1 134.2(12) 3_555 . 2_555 N
Si1 Al1 Si1 146.50(30) -1_555 . 209_344 N
Si1 Al1 O1 65.81(18) -1_555 . 2_555 N
Si1 Al1 O1 67.53(16) -1_555 . 3_555 N
Si1 Al1 O1 21.24(19) -1_555 . -1_555 N
Si1 Al1 O2 144.91(20) -1_555 . 2_555 N
Si1 Al1 O2 93.96(27) -1_555 . -105_444 N
Si1 Al1 O2 25.11(13) -1_555 . 206_454 N
Si1 Al1 O2 90.72(20) -1_555 . -304_444 N
Si1 Al1 O3 107.13(30) -1_555 . 3_555 N
Si1 Al1 O3 25.50(12) -1_555 . -2_555 N
Si1 Al1 O3 161.60(24) -1_555 . 312_334 N
Si1 Al1 O4 133.74(34) -1_555 . 107_433 N
Si1 Al1 O4 105.03(18) -1_555 . 111_433 N
Si1 Al1 SI 63.02(16) -1_555 . 1_555 N
Si1 Al1 SI' 100.62(26) -1_555 . 1_555 N
Si1 Al1 SII 137.11(22) -1_555 . 107_555 N
Si1 Al1 SJ 89.9(8) -1_555 . 2_555 N
Si1 Al1 Oc 66.52(29) -1_555 . 2_555 N
Si1 Al1 Dc1 76.80(32) -1_555 . 2_555 N
Si1 Al1 Dc2 59.1(4) -1_555 . 2_555 N
Si1 Al1 Od 90.4(10) -1_555 . 2_555 N
Si1 Al1 Dd1 88.7(13) -1_555 . 2_555 N
Si1 Al1 O1 140.07(25) 209_343 . 2_555 N
Si1 Al1 O1 101.03(21) 209_343 . 3_555 N
Si1 Al1 O1 126.7(4) 209_343 . -1_555 N
Si1 Al1 O2 23.44(13) 209_343 . 2_555 N
Si1 Al1 O2 92.73(28) 209_343 . -105_444 N
Si1 Al1 O2 171.37(27) 209_343 . 206_454 N
Si1 Al1 O2 122.76(24) 209_343 . -304_444 N
Si1 Al1 O3 102.32(31) 209_343 . 3_555 N
Si1 Al1 O3 133.15(24) 209_343 . -2_555 N
Si1 Al1 O3 26.32(13) 209_343 . 312_334 N
Si1 Al1 O4 16.89(15) 209_343 . 107_433 N
Si1 Al1 O4 64.56(17) 209_343 . 111_433 N
Si1 Al1 SI 140.32(24) 209_343 . 1_555 N
Si1 Al1 SI' 106.23(26) 209_343 . 1_555 N
Si1 Al1 SII 62.26(16) 209_465 . 107_555 N
Si1 Al1 SJ 62.0(7) 209_455 . 2_555 N
Si1 Al1 Oc 88.14(31) 209_455 . 2_555 N
Si1 Al1 Dc1 75.40(31) 209_464 . 2_555 N
Si1 Al1 Dc2 92.0(5) 209_465 . 2_555 N
Si1 Al1 Od 63.4(11) 209_464 . 2_555 N
Si1 Al1 Dd1 70.5(12) 209_443 . 2_555 N
O1 Al1 O1 117.28(20) 2_555 . 3_555 N
O1 Al1 O1 78.05(26) 2_555 . -1_555 N
O1 Al1 O2 148.42(23) 2_555 . 2_555 N
O1 Al1 O2 111.08(27) 2_555 . -105_444 N
O1 Al1 O2 44.58(13) 2_555 . 206_454 N
O1 Al1 O2 41.21(14) 2_555 . -304_444 N
O1 Al1 O3 41.41(21) 2_555 . 3_555 N
O1 Al1 O3 85.84(16) 2_555 . -2_555 N
O1 Al1 O3 114.36(19) 2_555 . 312_334 N
O1 Al1 O4 135.08(29) 2_555 . 107_433 N
O1 Al1 O4 146.75(19) 2_555 . 111_433 N
O1 Al1 SI 62.07(12) 2_555 . 1_555 N
O1 Al1 SI' 76.09(18) 2_555 . 1_555 N
O1 Al1 SII 77.91(15) 2_555 . 107_555 N
O1 Al1 SJ 113.7(7) 2_555 . 2_555 N
O1 Al1 Oc 92.01(31) 2_555 . 2_555 N
O1 Al1 Dc1 104.75(34) 2_555 . 2_555 N
O1 Al1 Dc2 95.9(5) 2_555 . 2_555 N
O1 Al1 Od 109.2(10) 2_555 . 2_555 N
O1 Al1 Dd1 96.3(12) 2_555 . 2_555 N
O1 Al1 O1 73.08(29) 3_555 . -1_555 N
O1 Al1 O2 82.48(16) 3_555 . 2_555 N
O1 Al1 O2 36.30(18) 3_555 . -105_444 N
O1 Al1 O2 77.26(15) 3_555 . 206_454 N
O1 Al1 O2 102.26(16) 3_555 . -304_444 N
O1 Al1 O3 136.51(30) 3_555 . 3_555 N
O1 Al1 O3 42.06(11) 3_555 . -2_555 N
O1 Al1 O3 122.96(18) 3_555 . 312_334 N
O1 Al1 O4 107.43(28) 3_555 . 107_433 N
O1 Al1 O4 38.55(11) 3_555 . 111_433 N
O1 Al1 SI 60.47(12) 3_555 . 1_555 N
O1 Al1 SI' 73.89(15) 3_555 . 1_555 N
O1 Al1 SII 154.46(23) 3_555 . 107_555 N
O1 Al1 SJ 105.5(7) 3_555 . 2_555 N
O1 Al1 Oc 105.34(27) 3_555 . 2_555 N
O1 Al1 Dc1 102.8(4) 3_555 . 2_555 N
O1 Al1 Dc2 94.0(4) 3_555 . 2_555 N
O1 Al1 Od 110.7(9) 3_555 . 2_555 N
O1 Al1 Dd1 122.0(12) 3_555 . 2_555 N
O1 Al1 O2 133.2(4) -1_555 . 2_555 N
O1 Al1 O2 106.3(4) -1_555 . -105_444 N
O1 Al1 O2 44.71(25) -1_555 . 206_454 N
O1 Al1 O2 110.01(33) -1_555 . -304_444 N
O1 Al1 O3 118.2(4) -1_555 . 3_555 N
O1 Al1 O3 35.19(23) -1_555 . -2_555 N
O1 Al1 O3 141.51(31) -1_555 . 312_334 N
O1 Al1 O4 112.7(4) -1_555 . 107_433 N
O1 Al1 O4 104.7(4) -1_555 . 111_433 N
O1 Al1 SI 83.88(24) -1_555 . 1_555 N
O1 Al1 SI' 121.40(33) -1_555 . 1_555 N
O1 Al1 SII 132.1(4) -1_555 . 107_555 N
O1 Al1 SJ 68.7(8) -1_555 . 2_555 N
O1 Al1 Oc 46.61(29) -1_555 . 2_555 N
O1 Al1 Dc1 55.85(35) -1_555 . 2_555 N
O1 Al1 Dc2 38.2(4) -1_555 . 2_555 N
O1 Al1 Od 69.6(10) -1_555 . 2_555 N
O1 Al1 Dd1 69.4(13) -1_555 . 2_555 N
O2 Al1 O2 69.32(23) 2_555 . -105_444 N
O2 Al1 O2 158.95(18) 2_555 . 206_454 N
O2 Al1 O2 113.92(18) 2_555 . -304_444 N
O2 Al1 O3 107.15(29) 2_555 . 3_555 N
O2 Al1 O3 121.76(18) 2_555 . -2_555 N
O2 Al1 O3 40.51(10) 2_555 . 312_334 N
O2 Al1 O4 39.15(18) 2_555 . 107_433 N
O2 Al1 O4 44.08(11) 2_555 . 111_433 N
O2 Al1 SI 117.70(17) 2_555 . 1_555 N
O2 Al1 SI' 87.44(18) 2_555 . 1_555 N
O2 Al1 SII 75.81(15) 2_555 . 107_555 N
O2 Al1 SJ 80.7(7) 2_555 . 2_555 N
O2 Al1 Oc 106.87(30) 2_555 . 2_555 N
O2 Al1 Dc1 93.35(29) 2_555 . 2_555 N
O2 Al1 Dc2 107.6(5) 2_555 . 2_555 N
O2 Al1 Od 83.3(11) 2_555 . 2_555 N
O2 Al1 Dd1 92.4(12) 2_555 . 2_555 N
O2 Al1 O2 90.71(25) -105_444 . 206_454 N
O2 Al1 O2 77.48(24) -105_444 . -304_444 N
O2 Al1 O3 106.4(4) -105_444 . 3_555 N
O2 Al1 O3 71.49(22) -105_444 . -2_555 N
O2 Al1 O3 102.56(26) -105_444 . 312_334 N
O2 Al1 O4 107.23(34) -105_444 . 107_433 N
O2 Al1 O4 35.81(17) -105_444 . 111_433 N
O2 Al1 SI 50.77(18) -105_444 . 1_555 N
O2 Al1 SI' 42.14(16) -105_444 . 1_555 N
O2 Al1 SII 120.90(31) -105_566 . 107_555 N
O2 Al1 SJ 132.3(7) -105_556 . 2_555 N
O2 Al1 Oc 140.9(4) -105_556 . 2_555 N
O2 Al1 Dc1 135.2(4) -105_565 . 2_555 N
O2 Al1 Dc2 129.9(5) -105_566 . 2_555 N
O2 Al1 Od 137.5(10) -105_565 . 2_555 N
O2 Al1 Dd1 151.0(12) -105_544 . 2_555 N
O2 Al1 O2 65.75(14) 206_454 . -304_444 N
O2 Al1 O3 84.26(26) 206_454 . 3_555 N
O2 Al1 O3 41.26(11) 206_454 . -2_555 N
O2 Al1 O3 158.74(19) 206_454 . 312_334 N
O2 Al1 O4 155.63(30) 206_454 . 107_433 N
O2 Al1 O4 115.21(17) 206_454 . 111_433 N
O2 Al1 SI 46.05(9) 206_454 . 1_555 N
O2 Al1 SI' 81.56(20) 206_454 . 1_555 N
O2 Al1 SII 122.16(19) 206_454 . 107_555 N
O2 Al1 SJ 110.1(7) 206_454 . 2_555 N
O2 Al1 Oc 84.20(29) 206_454 . 2_555 N
O2 Al1 Dc1 96.62(31) 206_454 . 2_555 N
O2 Al1 Dc2 79.7(4) 206_454 . 2_555 N
O2 Al1 Od 109.1(11) 206_454 . 2_555 N
O2 Al1 Dd1 103.1(12) 206_454 . 2_555 N
O2 Al1 O3 34.61(18) -304_444 . 3_555 N
O2 Al1 O3 97.20(15) -304_444 . -2_555 N
O2 Al1 O3 100.65(16) -304_444 . 312_334 N
O2 Al1 O4 133.29(29) -304_444 . 107_433 N
O2 Al1 O4 111.11(15) -304_444 . 111_433 N
O2 Al1 SI 44.20(9) -304_444 . 1_555 N
O2 Al1 SI' 36.65(9) -304_444 . 1_555 N
O2 Al1 SII 75.13(15) -304_566 . 107_555 N
O2 Al1 SJ 150.1(6) -304_556 . 2_555 N
O2 Al1 Oc 132.99(31) -304_556 . 2_555 N
O2 Al1 Dc1 144.96(34) -304_565 . 2_555 N
O2 Al1 Dc2 136.9(5) -304_566 . 2_555 N
O2 Al1 Od 144.7(9) -304_565 . 2_555 N
O2 Al1 Dd1 131.4(12) -304_544 . 2_555 N
O3 Al1 O3 124.29(29) 3_555 . -2_555 N
O3 Al1 O3 76.14(26) 3_555 . 312_334 N
O3 Al1 O4 105.5(4) 3_555 . 107_433 N
O3 Al1 O4 131.42(30) 3_555 . 111_433 N
O3 Al1 SI 78.34(23) 3_555 . 1_555 N
O3 Al1 SI' 64.59(22) 3_555 . 1_555 N
O3 Al1 SII 43.09(18) 3_555 . 107_555 N
O3 Al1 SJ 117.8(7) 3_555 . 2_555 N
O3 Al1 Oc 111.6(4) 3_555 . 2_555 N
O3 Al1 Dc1 118.3(4) 3_555 . 2_555 N
O3 Al1 Dc2 121.1(6) 3_555 . 2_555 N
O3 Al1 Od 112.5(9) 3_555 . 2_555 N
O3 Al1 Dd1 100.3(12) 3_555 . 2_555 N
O3 Al1 O3 159.47(18) -2_555 . 312_334 N
O3 Al1 O4 128.88(28) -2_555 . 107_433 N
O3 Al1 O4 79.69(14) -2_555 . 111_433 N
O3 Al1 SI 57.07(10) -2_555 . 1_555 N
O3 Al1 SI' 91.18(20) -2_555 . 1_555 N
O3 Al1 SII 162.31(21) -2_555 . 107_555 N
O3 Al1 SJ 96.1(7) -2_555 . 2_555 N
O3 Al1 Oc 79.64(25) -2_555 . 2_555 N
O3 Al1 Dc1 85.49(32) -2_555 . 2_555 N
O3 Al1 Dc2 69.3(4) -2_555 . 2_555 N
O3 Al1 Od 98.8(10) -2_555 . 2_555 N
O3 Al1 Dd1 102.4(12) -2_555 . 2_555 N
O3 Al1 O4 32.66(17) 312_334 . 107_433 N
O3 Al1 O4 84.45(14) 312_334 . 111_433 N
O3 Al1 SI 134.54(18) 312_334 . 1_555 N
O3 Al1 SI' 97.09(21) 312_334 . 1_555 N
O3 Al1 SII 36.58(9) 312_456 . 107_555 N
O3 Al1 SJ 73.0(7) 312_446 . 2_555 N
O3 Al1 Oc 95.28(27) 312_446 . 2_555 N
O3 Al1 Dc1 85.70(30) 312_455 . 2_555 N
O3 Al1 Dc2 103.3(4) 312_456 . 2_555 N
O3 Al1 Od 71.9(10) 312_455 . 2_555 N
O3 Al1 Dd1 73.0(13) 312_434 . 2_555 N
O4 Al1 O4 75.32(23) 107_433 . 111_433 N
O4 Al1 SI 156.85(30) 107_433 . 1_555 N
O4 Al1 SI' 122.81(32) 107_433 . 1_555 N
O4 Al1 SII 62.54(20) 107_555 . 107_555 N
O4 Al1 SJ 45.6(7) 107_545 . 2_555 N
O4 Al1 Oc 71.46(32) 107_545 . 2_555 N
O4 Al1 Dc1 59.04(32) 107_554 . 2_555 N
O4 Al1 Dc2 76.2(4) 107_555 . 2_555 N
O4 Al1 Od 46.6(11) 107_554 . 2_555 N
O4 Al1 Dd1 53.7(12) 107_533 . 2_555 N
O4 Al1 SI 85.06(13) 111_433 . 1_555 N
O4 Al1 SI' 74.46(12) 111_433 . 1_555 N
O4 Al1 SII 117.85(20) 111_555 . 107_555 N
O4 Al1 SJ 97.5(6) 111_545 . 2_555 N
O4 Al1 Oc 114.27(29) 111_545 . 2_555 N
O4 Al1 Dc1 103.76(33) 111_554 . 2_555 N
O4 Al1 Dc2 106.5(5) 111_555 . 2_555 N
O4 Al1 Od 102.6(10) 111_554 . 2_555 N
O4 Al1 Dd1 115.9(12) 111_533 . 2_555 N
SI Al1 SI' 37.61(16) 1_555 . 1_555 N
SI Al1 SII 118.96(20) 1_555 . 107_555 N
SI Al1 SJ 152.3(7) 1_555 . 2_555 N
SI Al1 Oc 129.13(30) 1_555 . 2_555 N
SI Al1 Dc1 139.73(32) 1_555 . 2_555 N
SI Al1 Dc2 122.0(4) 1_555 . 2_555 N
SI Al1 Od 153.4(10) 1_555 . 2_555 N
SI Al1 Dd1 149.1(12) 1_555 . 2_555 N
SI' Al1 SII 91.66(24) 1_555 . 107_555 N
SI' Al1 SJ 168.1(7) 1_555 . 2_555 N
SI' Al1 Oc 165.55(35) 1_555 . 2_555 N
SI' Al1 Dc1 176.5(4) 1_555 . 2_555 N
SI' Al1 Dc2 159.6(4) 1_555 . 2_555 N
SI' Al1 Od 169.0(11) 1_555 . 2_555 N
SI' Al1 Dd1 164.0(12) 1_555 . 2_555 N
SII Al1 SJ 84.3(7) 107_545 . 2_555 N
SII Al1 Oc 93.84(29) 107_545 . 2_555 N
SII Al1 Dc1 91.9(4) 107_554 . 2_555 N
SII Al1 Dc2 105.2(4) 107_555 . 2_555 N
SII Al1 Od 80.3(9) 107_554 . 2_555 N
SII Al1 Dd1 72.8(12) 107_533 . 2_555 N
SJ Al1 Oc 26.3(7) 2_555 . 2_555 N
SJ Al1 Dc1 13.5(8) 2_555 . 2_555 N
SJ Al1 Dc2 30.9(8) 2_555 . 2_555 N
SJ Al1 Od 5.4(12) 2_555 . 2_555 N
SJ Al1 Dd1 18.8(13) 2_555 . 2_555 N
Oc Al1 Dc1 13.58(15) 2_555 . 2_555 N
Oc Al1 Dc2 11.48(26) 2_555 . 2_555 N
Oc Al1 Od 24.9(11) 2_555 . 2_555 N
Oc Al1 Dd1 22.9(12) 2_555 . 2_555 N
Dc1 Al1 Dc2 17.7(4) 2_555 . 2_555 N
Dc1 Al1 Od 13.8(10) 2_555 . 2_555 N
Dc1 Al1 Dd1 19.4(12) 2_555 . 2_555 N
Dc2 Al1 Od 31.4(10) 2_555 . 2_555 N
Dc2 Al1 Dd1 33.2(12) 2_555 . 2_555 N
Od Al1 Dd1 13.5(8) 2_555 . 2_555 N
Si1 O1 Si1 95.4(4) 1_555 . -2_555 N
Si1 O1 Si1 102.61(32) 1_555 . -3_555 N
Si1 O1 Si2 51.52(30) 1_555 . 2_555 N
Si1 O1 Si2 58.06(26) 1_555 . 3_555 N
Si1 O1 Si2 136.96(32) 1_555 . -1_555 N
Si1 O1 Al1 51.52(30) 1_555 . 2_555 N
Si1 O1 Al1 58.06(26) 1_555 . 3_555 N
Si1 O1 Al1 136.96(32) 1_555 . -1_555 N
Si1 O1 O1 76.6(4) 1_555 . -2_555 N
Si1 O1 O1 83.54(26) 1_555 . -3_555 N
Si1 O1 O2 109.66(26) 1_555 . 105_544 N
Si1 O1 O2 31.26(25) 1_555 . -206_444 N
Si1 O1 O3 37.59(24) 1_555 . 2_555 N
Si1 O1 O3 118.31(34) 1_555 . -3_555 N
Si1 O1 O4 170.91(31) 1_555 . -107_444 N
Si1 O1 O4 36.48(23) 1_555 . 209_343 N
Si1 O1 SI 67.64(22) 1_555 . 1_555 N
Si1 O1 SJ 147.6(7) 1_555 . -2_555 N
Si1 O1 SJ 76.0(6) 1_555 . -206_556 N
Si1 O1 Oc 113.6(5) 1_555 . -2_555 N
Si1 O1 Dc1 123.1(5) 1_555 . -2_555 N
Si1 O1 Dc1 93.27(34) 1_555 . -206_565 N
Si1 O1 Dc2 115.9(7) 1_555 . -2_555 N
Si1 O1 Od 142.6(11) 1_555 . -2_555 N
Si1 O1 Si1 89.81(18) -2_555 . -3_555 N
Si1 O1 Si2 46.13(12) -2_555 . 2_555 N
Si1 O1 Si2 110.43(13) -2_555 . 3_555 N
Si1 O1 Si2 52.16(27) -2_555 . -1_555 N
Si1 O1 Al1 46.13(12) -2_555 . 2_555 N
Si1 O1 Al1 110.43(13) -2_555 . 3_555 N
Si1 O1 Al1 52.16(27) -2_555 . -1_555 N
Si1 O1 O1 24.30(12) -2_555 . -2_555 N
Si1 O1 O1 107.79(12) -2_555 . -3_555 N
Si1 O1 O2 69.49(14) -2_555 . 105_544 N
Si1 O1 O2 64.16(16) -2_555 . -206_444 N
Si1 O1 O3 114.73(15) -2_555 . 2_555 N
Si1 O1 O3 23.65(13) -2_555 . -3_555 N
Si1 O1 O4 80.24(14) -2_555 . -107_444 N
Si1 O1 O4 115.57(28) -2_555 . 209_343 N
Si1 O1 SI 53.84(10) -2_555 . 1_555 N
Si1 O1 SJ 106.2(7) -2_555 . -2_555 N
Si1 O1 SJ 128.2(6) -2_555 . -206_556 N
Si1 O1 Oc 113.78(34) -2_555 . -2_555 N
Si1 O1 Dc1 119.7(4) -2_555 . -2_555 N
Si1 O1 Dc1 127.6(4) -2_555 . -206_565 N
Si1 O1 Dc2 123.1(7) -2_555 . -2_555 N
Si1 O1 Od 105.3(9) -2_555 . -2_555 N
Si1 O1 Si2 110.64(13) -3_555 . 2_555 N
Si1 O1 Si2 48.41(13) -3_555 . 3_555 N
Si1 O1 Si2 56.79(29) -3_555 . -1_555 N
Si1 O1 Al1 110.64(13) -3_555 . 2_555 N
Si1 O1 Al1 48.41(13) -3_555 . 3_555 N
Si1 O1 Al1 56.79(29) -3_555 . -1_555 N
Si1 O1 O1 108.73(14) -3_555 . -2_555 N
Si1 O1 O1 25.05(14) -3_555 . -3_555 N
Si1 O1 O2 21.26(13) -3_555 . 105_544 N
Si1 O1 O2 99.49(15) -3_555 . -206_444 N
Si1 O1 O3 71.14(18) -3_555 . 2_555 N
Si1 O1 O3 79.72(18) -3_555 . -3_555 N
Si1 O1 O4 69.61(19) -3_555 . -107_444 N
Si1 O1 O4 129.23(19) -3_555 . 209_343 N
Si1 O1 SI 55.37(10) -3_555 . 1_555 N
Si1 O1 SJ 101.3(7) -3_555 . -2_555 N
Si1 O1 SJ 142.0(6) -3_555 . -206_556 N
Si1 O1 Oc 133.5(5) -3_555 . -2_555 N
Si1 O1 Dc1 119.2(4) -3_555 . -2_555 N
Si1 O1 Dc1 137.9(4) -3_555 . -206_565 N
Si1 O1 Dc2 123.9(8) -3_555 . -2_555 N
Si1 O1 Od 108.1(11) -3_555 . -2_555 N
Si2 O1 Si2 93.64(21) 2_555 . 3_555 N
Si2 O1 Si2 97.28(34) 2_555 . -1_555 N
Si2 O1 Al1 0.0 2_555 . 2_555 N
Si2 O1 Al1 93.64(21) 2_555 . 3_555 N
Si2 O1 Al1 97.28(34) 2_555 . -1_555 N
Si2 O1 O1 25.08(13) 2_555 . -2_555 N
Si2 O1 O1 110.58(15) 2_555 . -3_555 N
Si2 O1 O2 98.77(15) 2_555 . 105_544 N
Si2 O1 O2 23.63(14) 2_555 . -206_444 N
Si2 O1 O3 82.69(18) 2_555 . 2_555 N
Si2 O1 O3 69.74(18) 2_555 . -3_555 N
Si2 O1 O4 125.77(18) 2_555 . -107_444 N
Si2 O1 O4 70.77(21) 2_555 . 209_343 N
Si2 O1 SI 55.30(11) 2_555 . 1_555 N
Si2 O1 SJ 135.6(7) 2_555 . -2_555 N
Si2 O1 SJ 98.2(6) 2_555 . -206_556 N
Si2 O1 Oc 114.6(4) 2_555 . -2_555 N
Si2 O1 Dc1 128.5(4) 2_555 . -2_555 N
Si2 O1 Dc1 109.78(34) 2_555 . -206_565 N
Si2 O1 Dc2 125.1(8) 2_555 . -2_555 N
Si2 O1 Od 130.2(10) 2_555 . -2_555 N
Si2 O1 Si2 103.2(4) 3_555 . -1_555 N
Si2 O1 Al1 93.64(21) 3_555 . 2_555 N
Si2 O1 Al1 0.0 3_555 . 3_555 N
Si2 O1 Al1 103.2(4) 3_555 . -1_555 N
Si2 O1 O1 111.49(13) 3_555 . -2_555 N
Si2 O1 O1 25.69(12) 3_555 . -3_555 N
Si2 O1 O2 64.66(16) 3_555 . 105_544 N
Si2 O1 O2 71.26(15) 3_555 . -206_444 N
Si2 O1 O3 22.78(14) 3_555 . 2_555 N
Si2 O1 O3 116.19(17) 3_555 . -3_555 N
Si2 O1 O4 115.90(28) 3_555 . -107_444 N
Si2 O1 O4 80.99(16) 3_555 . 209_343 N
Si2 O1 SI 56.60(10) 3_555 . 1_555 N
Si2 O1 SJ 130.7(7) 3_555 . -2_555 N
Si2 O1 SJ 107.3(6) 3_555 . -206_556 N
Si2 O1 Oc 135.66(33) 3_555 . -2_555 N
Si2 O1 Dc1 128.7(4) 3_555 . -2_555 N
Si2 O1 Dc1 117.77(33) 3_555 . -206_565 N
Si2 O1 Dc2 126.4(8) 3_555 . -2_555 N
Si2 O1 Od 135.8(10) 3_555 . -2_555 N
Si2 O1 Al1 97.28(34) -1_555 . 2_555 N
Si2 O1 Al1 103.2(4) -1_555 . 3_555 N
Si2 O1 Al1 0.0 -1_555 . -1_555 N
Si2 O1 O1 76.26(27) -1_555 . -2_555 N
Si2 O1 O1 81.8(4) -1_555 . -3_555 N
Si2 O1 O2 38.54(26) -1_555 . 105_544 N
Si2 O1 O2 109.17(29) -1_555 . -206_444 N
Si2 O1 O3 124.32(34) -1_555 . 2_555 N
Si2 O1 O3 30.28(24) -1_555 . -3_555 N
Si2 O1 O4 34.89(25) -1_555 . -107_444 N
Si2 O1 O4 167.7(5) -1_555 . 209_343 N
Si2 O1 SI 69.98(23) -1_555 . 1_555 N
Si2 O1 SJ 75.0(7) -1_555 . -2_555 N
Si2 O1 SJ 144.6(6) -1_555 . -206_556 N
Si2 O1 Oc 106.0(4) -1_555 . -2_555 N
Si2 O1 Dc1 99.1(5) -1_555 . -2_555 N
Si2 O1 Dc1 128.04(33) -1_555 . -206_565 N
Si2 O1 Dc2 106.3(7) -1_555 . -2_555 N
Si2 O1 Od 79.0(10) -1_555 . -2_555 N
Al1 O1 Al1 93.64(21) 2_555 . 3_555 N
Al1 O1 Al1 97.28(34) 2_555 . -1_555 N
Al1 O1 O1 25.08(13) 2_555 . -2_555 N
Al1 O1 O1 110.58(15) 2_555 . -3_555 N
Al1 O1 O2 98.77(15) 2_555 . 105_544 N
Al1 O1 O2 23.63(14) 2_555 . -206_444 N
Al1 O1 O3 82.69(18) 2_555 . 2_555 N
Al1 O1 O3 69.74(18) 2_555 . -3_555 N
Al1 O1 O4 125.77(18) 2_555 . -107_444 N
Al1 O1 O4 70.77(21) 2_555 . 209_343 N
Al1 O1 SI 55.30(11) 2_555 . 1_555 N
Al1 O1 SJ 135.6(7) 2_555 . -2_555 N
Al1 O1 SJ 98.2(6) 2_555 . -206_556 N
Al1 O1 Oc 114.6(4) 2_555 . -2_555 N
Al1 O1 Dc1 128.5(4) 2_555 . -2_555 N
Al1 O1 Dc1 109.78(34) 2_555 . -206_565 N
Al1 O1 Dc2 125.1(8) 2_555 . -2_555 N
Al1 O1 Od 130.2(10) 2_555 . -2_555 N
Al1 O1 Al1 103.2(4) 3_555 . -1_555 N
Al1 O1 O1 111.49(13) 3_555 . -2_555 N
Al1 O1 O1 25.69(12) 3_555 . -3_555 N
Al1 O1 O2 64.66(16) 3_555 . 105_544 N
Al1 O1 O2 71.26(15) 3_555 . -206_444 N
Al1 O1 O3 22.78(14) 3_555 . 2_555 N
Al1 O1 O3 116.19(17) 3_555 . -3_555 N
Al1 O1 O4 115.90(28) 3_555 . -107_444 N
Al1 O1 O4 80.99(16) 3_555 . 209_343 N
Al1 O1 SI 56.60(10) 3_555 . 1_555 N
Al1 O1 SJ 130.7(7) 3_555 . -2_555 N
Al1 O1 SJ 107.3(6) 3_555 . -206_556 N
Al1 O1 Oc 135.66(33) 3_555 . -2_555 N
Al1 O1 Dc1 128.7(4) 3_555 . -2_555 N
Al1 O1 Dc1 117.77(33) 3_555 . -206_565 N
Al1 O1 Dc2 126.4(8) 3_555 . -2_555 N
Al1 O1 Od 135.8(10) 3_555 . -2_555 N
Al1 O1 O1 76.26(27) -1_555 . -2_555 N
Al1 O1 O1 81.8(4) -1_555 . -3_555 N
Al1 O1 O2 38.54(26) -1_555 . 105_544 N
Al1 O1 O2 109.17(29) -1_555 . -206_444 N
Al1 O1 O3 124.32(34) -1_555 . 2_555 N
Al1 O1 O3 30.28(24) -1_555 . -3_555 N
Al1 O1 O4 34.89(25) -1_555 . -107_444 N
Al1 O1 O4 167.7(5) -1_555 . 209_343 N
Al1 O1 SI 69.98(23) -1_555 . 1_555 N
Al1 O1 SJ 75.0(7) -1_555 . -2_555 N
Al1 O1 SJ 144.6(6) -1_555 . -206_556 N
Al1 O1 Oc 106.0(4) -1_555 . -2_555 N
Al1 O1 Dc1 99.1(5) -1_555 . -2_555 N
Al1 O1 Dc1 128.04(33) -1_555 . -206_565 N
Al1 O1 Dc2 106.3(7) -1_555 . -2_555 N
Al1 O1 Od 79.0(10) -1_555 . -2_555 N
O1 O1 O1 119.932(17) -2_555 . -3_555 N
O1 O1 O2 90.50(14) -2_555 . 105_544 N
O1 O1 O2 47.52(15) -2_555 . -206_444 N
O1 O1 O3 105.75(19) -2_555 . 2_555 N
O1 O1 O3 46.64(12) -2_555 . -3_555 N
O1 O1 O4 101.06(19) -2_555 . -107_444 N
O1 O1 O4 91.45(32) -2_555 . 209_343 N
O1 O1 SI 59.9915(21) -2_555 . 1_555 N
O1 O1 SJ 115.5(7) -2_555 . -2_555 N
O1 O1 SJ 107.8(7) -2_555 . -206_556 N
O1 O1 Oc 107.4(4) -2_555 . -2_555 N
O1 O1 Dc1 118.5(4) -2_555 . -2_555 N
O1 O1 Dc1 112.8(4) -2_555 . -206_565 N
O1 O1 Dc2 118.4(8) -2_555 . -2_555 N
O1 O1 Od 111.8(10) -2_555 . -2_555 N
O1 O1 O2 45.00(15) -3_555 . 105_544 N
O1 O1 O2 91.58(12) -3_555 . -206_444 N
O1 O1 O3 48.07(12) -3_555 . 2_555 N
O1 O1 O3 103.03(22) -3_555 . -3_555 N
O1 O1 O4 90.21(31) -3_555 . -107_444 N
O1 O1 O4 104.69(20) -3_555 . 209_343 N
O1 O1 SI 59.9915(21) -3_555 . 1_555 N
O1 O1 SJ 111.3(7) -3_555 . -2_555 N
O1 O1 SJ 121.3(6) -3_555 . -206_556 N
O1 O1 Oc 132.4(4) -3_555 . -2_555 N
O1 O1 Dc1 119.9(5) -3_555 . -2_555 N
O1 O1 Dc1 124.5(4) -3_555 . -206_565 N
O1 O1 Dc2 121.3(9) -3_555 . -2_555 N
O1 O1 Od 117.7(11) -3_555 . -2_555 N
O2 O1 O2 95.39(17) 105_544 . -206_444 N
O2 O1 O3 86.13(18) 105_544 . 2_555 N
O2 O1 O3 58.56(15) 105_544 . -3_555 N
O2 O1 O4 61.39(17) 105_544 . -107_444 N
O2 O1 O4 143.67(18) 105_544 . 209_343 N
O2 O1 SI 47.61(8) 105_544 . 1_555 N
O2 O1 SJ 100.5(7) 105_544 . -2_555 N
O2 O1 SJ 161.7(6) 105_544 . -206_556 N
O2 O1 Oc 135.8(4) 105_544 . -2_555 N
O2 O1 Dc1 123.5(5) 105_544 . -2_555 N
O2 O1 Dc1 150.81(33) 105_544 . -206_565 N
O2 O1 Dc2 130.1(8) 105_544 . -2_555 N
O2 O1 Od 106.6(11) 105_544 . -2_555 N
O2 O1 O3 59.07(15) -206_444 . 2_555 N
O2 O1 O3 87.08(19) -206_444 . -3_555 N
O2 O1 O4 143.09(19) -206_444 . -107_444 N
O2 O1 O4 60.86(20) -206_444 . 209_343 N
O2 O1 SI 47.78(9) -206_444 . 1_555 N
O2 O1 SJ 157.1(7) -206_556 . -2_555 N
O2 O1 SJ 97.3(6) -206_556 . -206_556 N
O2 O1 Oc 126.6(5) -206_556 . -2_555 N
O2 O1 Dc1 140.5(5) -206_565 . -2_555 N
O2 O1 Dc1 113.18(31) -206_565 . -206_565 N
O2 O1 Dc2 134.4(8) -206_566 . -2_555 N
O2 O1 Od 150.6(11) -206_565 . -2_555 N
O3 O1 O3 129.23(15) 2_555 . -3_555 N
O3 O1 O4 137.75(33) 2_555 . -107_444 N
O3 O1 O4 58.50(15) 2_555 . 209_343 N
O3 O1 SI 64.84(8) 2_555 . 1_555 N
O3 O1 SJ 138.0(7) 2_555 . -2_555 N
O3 O1 SJ 89.2(6) 2_555 . -206_556 N
O3 O1 Oc 124.58(31) 2_555 . -2_555 N
O3 O1 Dc1 124.1(4) 2_555 . -2_555 N
O3 O1 Dc1 103.02(30) 2_555 . -206_565 N
O3 O1 Dc2 118.9(7) 2_555 . -2_555 N
O3 O1 Od 139.9(9) 2_555 . -2_555 N
O3 O1 O4 56.70(15) -3_555 . -107_444 N
O3 O1 O4 137.6(4) -3_555 . 209_343 N
O3 O1 SI 64.39(8) -3_555 . 1_555 N
O3 O1 SJ 87.2(7) -3_555 . -2_555 N
O3 O1 SJ 135.2(6) -3_555 . -206_556 N
O3 O1 Oc 105.74(31) -3_555 . -2_555 N
O3 O1 Dc1 106.3(4) -3_555 . -2_555 N
O3 O1 Dc1 125.91(34) -3_555 . -206_565 N
O3 O1 Dc2 111.8(7) -3_555 . -2_555 N
O3 O1 Od 88.1(9) -3_555 . -2_555 N
O4 O1 O4 152.51(18) -107_444 . 209_343 N
O4 O1 SI 103.51(16) -107_444 . 1_555 N
O4 O1 SJ 41.3(7) -107_556 . -2_555 N
O4 O1 SJ 112.9(5) -107_556 . -206_556 N
O4 O1 Oc 75.47(35) -107_556 . -2_555 N
O4 O1 Dc1 65.8(4) -107_565 . -2_555 N
O4 O1 Dc1 95.71(23) -107_565 . -206_565 N
O4 O1 Dc2 73.0(6) -107_566 . -2_555 N
O4 O1 Od 46.4(10) -107_565 . -2_555 N
O4 O1 SI 103.95(17) 209_343 . 1_555 N
O4 O1 SJ 111.2(7) 209_455 . -2_555 N
O4 O1 SJ 39.6(5) 209_455 . -206_556 N
O4 O1 Oc 77.46(35) 209_455 . -2_555 N
O4 O1 Dc1 86.7(4) 209_464 . -2_555 N
O4 O1 Dc1 56.80(23) 209_464 . -206_565 N
O4 O1 Dc2 79.5(6) 209_465 . -2_555 N
O4 O1 Od 106.2(11) 209_464 . -2_555 N
SI O1 SJ 144.7(7) 1_555 . -2_555 N
SI O1 SJ 143.4(6) 1_555 . -206_556 N
SI O1 Oc 167.1(4) 1_555 . -2_555 N
SI O1 Dc1 169.1(4) 1_555 . -2_555 N
SI O1 Dc1 160.41(28) 1_555 . -206_565 N
SI O1 Dc2 176.1(6) 1_555 . -2_555 N
SI O1 Od 149.0(10) 1_555 . -2_555 N
SJ O1 SJ 71.7(11) -2_555 . -206_556 N
SJ O1 Oc 35.4(7) -2_555 . -2_555 N
SJ O1 Dc1 24.5(8) -2_555 . -2_555 N
SJ O1 Dc1 54.5(7) -2_555 . -206_565 N
SJ O1 Dc2 31.8(9) -2_555 . -2_555 N
SJ O1 Od 6.9(13) -2_555 . -2_555 N
SJ O1 Oc 38.6(6) -206_556 . -2_555 N
SJ O1 Dc1 47.2(6) -206_565 . -2_555 N
SJ O1 Dc1 17.2(6) -206_565 . -206_565 N
SJ O1 Dc2 39.9(8) -206_566 . -2_555 N
SJ O1 Od 66.7(12) -206_565 . -2_555 N
Oc O1 Dc1 14.29(25) -2_555 . -2_555 N
Oc O1 Dc1 22.28(33) -2_555 . -206_565 N
Oc O1 Dc2 11.2(6) -2_555 . -2_555 N
Oc O1 Od 29.3(11) -2_555 . -2_555 N
Dc1 O1 Dc1 30.0(5) -2_555 . -206_565 N
Dc1 O1 Dc2 7.3(7) -2_555 . -2_555 N
Dc1 O1 Od 20.1(10) -2_555 . -2_555 N
Dc1 O1 Dc2 22.8(6) -206_566 . -2_555 N
Dc1 O1 Od 49.5(11) -206_565 . -2_555 N
Dc2 O1 Od 27.3(11) -2_555 . -2_555 N
Si1 O2 Si1 103.52(26) 2_555 . 111_434 N
Si1 O2 Si1 108.17(19) 2_555 . -108_545 N
Si1 O2 Si1 93.18(19) 2_555 . -304_445 N
Si1 O2 Si2 49.43(12) 2_555 . 3_555 N
Si1 O2 Si2 58.58(22) 2_555 . 208_443 N
Si1 O2 Si2 131.25(14) 2_555 . -211_554 N
Si1 O2 Si2 136.36(18) 2_555 . -304_544 N
Si1 O2 Al1 49.43(12) 2_555 . 3_555 N
Si1 O2 Al1 58.58(22) 2_555 . 208_353 N
Si1 O2 Al1 131.25(14) 2_555 . -211_464 N
Si1 O2 Al1 136.36(18) 2_555 . -304_454 N
Si1 O2 O1 116.88(20) 2_555 . 111_433 N
Si1 O2 O1 83.51(16) 2_555 . -108_544 N
Si1 O2 O2 138.58(9) 2_555 . 107_433 N
Si1 O2 O2 108.55(17) 2_555 . 209_343 N
Si1 O2 O2 23.92(12) 2_555 . -304_444 N
Si1 O2 O3 121.29(13) 2_555 . 4_555 N
Si1 O2 O3 71.55(14) 2_555 . 111_433 N
Si1 O2 O3 119.34(17) 2_555 . 208_343 N
Si1 O2 O4 23.37(11) 2_555 . 310_334 N
Si1 O2 O4 71.28(14) 2_555 . 312_334 N
Si1 O2 SI 152.68(18) 2_555 . 4_555 N
Si1 O2 SI' 116.29(23) 2_555 . 111_433 N
Si1 O2 Dd2 81.3(14) 2_555 . 1_555 N
Si1 O2 Si1 108.41(21) 111_434 . -108_545 N
Si1 O2 Si1 162.47(28) 111_434 . -304_445 N
Si1 O2 Si2 56.61(25) 111_533 . 3_555 N
Si1 O2 Si2 141.95(29) 111_533 . 208_443 N
Si1 O2 Si2 58.34(23) 111_533 . -211_554 N
Si1 O2 Si2 54.34(24) 111_533 . -304_544 N
Si1 O2 Al1 56.61(25) 111_443 . 3_555 N
Si1 O2 Al1 141.95(29) 111_443 . 208_353 N
Si1 O2 Al1 58.34(23) 111_443 . -211_464 N
Si1 O2 Al1 54.34(24) 111_443 . -304_454 N
Si1 O2 O1 33.54(24) 111_433 . 111_433 N
Si1 O2 O1 117.50(28) 111_433 . -108_544 N
Si1 O2 O2 81.45(28) 111_433 . 107_433 N
Si1 O2 O2 141.14(28) 111_433 . 209_343 N
Si1 O2 O2 84.79(28) 111_433 . -304_444 N
Si1 O2 O3 81.59(25) 111_433 . 4_555 N
Si1 O2 O3 174.91(29) 111_433 . 111_433 N
Si1 O2 O3 38.89(24) 111_433 . 208_343 N
Si1 O2 O4 117.62(26) 111_433 . 310_334 N
Si1 O2 O4 32.45(23) 111_433 . 312_334 N
Si1 O2 SI 103.77(26) 111_433 . 4_555 N
Si1 O2 SI' 111.98(28) 111_433 . 111_433 N
Si1 O2 Dd2 22.9(14) 111_533 . 1_555 N
Si1 O2 Si1 70.48(14) -108_545 . -304_445 N
Si1 O2 Si2 133.93(15) -108_644 . 3_555 N
Si1 O2 Si2 56.62(22) -108_644 . 208_443 N
Si1 O2 Si2 52.28(12) -108_644 . -211_554 N
Si1 O2 Si2 114.38(16) -108_644 . -304_544 N
Si1 O2 Al1 133.93(15) -108_554 . 3_555 N
Si1 O2 Al1 56.62(22) -108_554 . 208_353 N
Si1 O2 Al1 52.28(12) -108_554 . -211_464 N
Si1 O2 Al1 114.38(16) -108_554 . -304_454 N
Si1 O2 O1 74.94(15) -108_544 . 111_433 N
Si1 O2 O1 24.73(13) -108_544 . -108_544 N
Si1 O2 O2 108.96(10) -108_544 . 107_433 N
Si1 O2 O2 81.92(13) -108_544 . 209_343 N
Si1 O2 O2 129.21(15) -108_544 . -304_444 N
Si1 O2 O3 27.38(11) -108_544 . 4_555 N
Si1 O2 O3 72.56(14) -108_544 . 111_433 N
Si1 O2 O3 125.97(15) -108_544 . 208_343 N
Si1 O2 O4 85.57(15) -108_544 . 310_334 N
Si1 O2 O4 122.09(15) -108_544 . 312_334 N
Si1 O2 SI 63.72(11) -108_544 . 4_555 N
Si1 O2 SI' 108.17(24) -108_544 . 111_433 N
Si1 O2 Dd2 111.2(13) -108_644 . 1_555 N
Si1 O2 Si2 137.09(15) -304_544 . 3_555 N
Si1 O2 Si2 52.84(23) -304_544 . 208_443 N
Si1 O2 Si2 113.76(17) -304_544 . -211_554 N
Si1 O2 Si2 109.39(12) -304_544 . -304_544 N
Si1 O2 Al1 137.09(15) -304_454 . 3_555 N
Si1 O2 Al1 52.84(23) -304_454 . 208_353 N
Si1 O2 Al1 113.76(17) -304_454 . -211_464 N
Si1 O2 Al1 109.39(12) -304_454 . -304_454 N
Si1 O2 O1 139.84(18) -304_444 . 111_433 N
Si1 O2 O1 69.15(18) -304_444 . -108_544 N
Si1 O2 O2 82.49(12) -304_444 . 107_433 N
Si1 O2 O2 22.56(11) -304_444 . 209_343 N
Si1 O2 O2 109.76(18) -304_444 . -304_444 N
Si1 O2 O3 94.38(14) -304_444 . 4_555 N
Si1 O2 O3 22.62(12) -304_444 . 111_433 N
Si1 O2 O3 126.93(14) -304_444 . 208_343 N
Si1 O2 O4 79.91(15) -304_444 . 310_334 N
Si1 O2 O4 162.08(17) -304_444 . 312_334 N
Si1 O2 SI 59.53(11) -304_444 . 4_555 N
Si1 O2 SI' 54.33(12) -304_444 . 111_433 N
Si1 O2 Dd2 174.5(14) -304_544 . 1_555 N
Si2 O2 Si2 105.97(24) 3_555 . 208_443 N
Si2 O2 Si2 107.78(20) 3_555 . -211_554 N
Si2 O2 Si2 92.05(21) 3_555 . -304_544 N
Si2 O2 Al1 0.0 3_555 . 3_555 N
Si2 O2 Al1 105.97(24) 3_555 . 208_353 N
Si2 O2 Al1 107.78(20) 3_555 . -211_464 N
Si2 O2 Al1 92.05(21) 3_555 . -304_454 N
Si2 O2 O1 82.36(18) 3_555 . 111_433 N
Si2 O2 O1 117.26(18) 3_555 . -108_544 N
Si2 O2 O2 110.64(17) 3_555 . 107_433 N
Si2 O2 O2 139.17(10) 3_555 . 209_343 N
Si2 O2 O2 28.21(12) 3_555 . -304_444 N
Si2 O2 O3 121.31(13) 3_555 . 4_555 N
Si2 O2 O3 118.99(15) 3_555 . 111_433 N
Si2 O2 O3 72.44(15) 3_555 . 208_343 N
Si2 O2 O4 70.06(14) 3_555 . 310_334 N
Si2 O2 O4 25.03(13) 3_555 . 312_334 N
Si2 O2 SI 154.73(18) 3_555 . 4_555 N
Si2 O2 SI' 117.85(24) 3_555 . 111_433 N
Si2 O2 Dd2 38.0(15) 3_555 . 1_555 N
Si2 O2 Si2 105.94(20) 208_443 . -211_554 N
Si2 O2 Si2 160.98(26) 208_443 . -304_544 N
Si2 O2 Al1 105.97(24) 208_353 . 3_555 N
Si2 O2 Al1 0.0 208_353 . 208_353 N
Si2 O2 Al1 105.94(20) 208_353 . -211_464 N
Si2 O2 Al1 160.98(26) 208_353 . -304_454 N
Si2 O2 O1 120.07(27) 208_343 . 111_433 N
Si2 O2 O1 35.18(23) 208_343 . -108_544 N
Si2 O2 O2 135.14(27) 208_343 . 107_433 N
Si2 O2 O2 75.41(27) 208_343 . 209_343 N
Si2 O2 O2 82.48(25) 208_343 . -304_444 N
Si2 O2 O3 81.55(24) 208_343 . 4_555 N
Si2 O2 O3 34.35(23) 208_343 . 111_433 N
Si2 O2 O3 177.41(26) 208_343 . 208_343 N
Si2 O2 O4 36.08(21) 208_343 . 310_334 N
Si2 O2 O4 120.75(24) 208_343 . 312_334 N
Si2 O2 SI 99.19(25) 208_343 . 4_555 N
Si2 O2 SI' 106.05(27) 208_343 . 111_433 N
Si2 O2 Dd2 123.2(12) 208_443 . 1_555 N
Si2 O2 Si2 73.31(14) -211_554 . -304_544 N
Si2 O2 Al1 107.78(20) -211_464 . 3_555 N
Si2 O2 Al1 105.94(20) -211_464 . 208_353 N
Si2 O2 Al1 0.0 -211_464 . -211_464 N
Si2 O2 Al1 73.31(14) -211_464 . -304_454 N
Si2 O2 O1 26.12(14) -211_454 . 111_433 N
Si2 O2 O1 70.76(15) -211_454 . -108_544 N
Si2 O2 O2 86.81(13) -211_454 . 107_433 N
Si2 O2 O2 110.94(10) -211_454 . 209_343 N
Si2 O2 O2 130.54(15) -211_454 . -304_444 N
Si2 O2 O3 25.08(12) -211_454 . 4_555 N
Si2 O2 O3 123.76(17) -211_454 . 111_433 N
Si2 O2 O3 76.58(15) -211_454 . 208_343 N
Si2 O2 O4 120.43(14) -211_454 . 310_334 N
Si2 O2 O4 83.77(16) -211_454 . 312_334 N
Si2 O2 SI 66.57(11) -211_454 . 4_555 N
Si2 O2 SI' 112.42(24) -211_454 . 111_433 N
Si2 O2 Dd2 70.4(15) -211_554 . 1_555 N
Si2 O2 Al1 92.05(21) -304_454 . 3_555 N
Si2 O2 Al1 160.98(26) -304_454 . 208_353 N
Si2 O2 Al1 73.31(14) -304_454 . -211_464 N
Si2 O2 Al1 0.0 -304_454 . -304_454 N
Si2 O2 O1 67.53(18) -304_444 . 111_433 N
Si2 O2 O1 138.96(17) -304_444 . -108_544 N
Si2 O2 O2 27.11(12) -304_444 . 107_433 N
Si2 O2 O2 87.02(12) -304_444 . 209_343 N
Si2 O2 O2 112.85(19) -304_444 . -304_444 N
Si2 O2 O3 94.44(14) -304_444 . 4_555 N
Si2 O2 O3 130.14(15) -304_444 . 111_433 N
Si2 O2 O3 20.01(12) -304_444 . 208_343 N
Si2 O2 O4 159.70(18) -304_444 . 310_334 N
Si2 O2 O4 78.26(15) -304_444 . 312_334 N
Si2 O2 SI 62.68(11) -304_444 . 4_555 N
Si2 O2 SI' 58.75(12) -304_444 . 111_433 N
Si2 O2 Dd2 75.0(12) -304_544 . 1_555 N
Al1 O2 Al1 105.97(24) 3_555 . 208_353 N
Al1 O2 Al1 107.78(20) 3_555 . -211_464 N
Al1 O2 Al1 92.05(21) 3_555 . -304_454 N
Al1 O2 O1 82.36(18) 3_555 . 111_433 N
Al1 O2 O1 117.26(18) 3_555 . -108_544 N
Al1 O2 O2 110.64(17) 3_555 . 107_433 N
Al1 O2 O2 139.17(10) 3_555 . 209_343 N
Al1 O2 O2 28.21(12) 3_555 . -304_444 N
Al1 O2 O3 121.31(13) 3_555 . 4_555 N
Al1 O2 O3 118.99(15) 3_555 . 111_433 N
Al1 O2 O3 72.44(15) 3_555 . 208_343 N
Al1 O2 O4 70.06(14) 3_555 . 310_334 N
Al1 O2 O4 25.03(13) 3_555 . 312_334 N
Al1 O2 SI 154.73(18) 3_555 . 4_555 N
Al1 O2 SI' 117.85(24) 3_555 . 111_433 N
Al1 O2 Dd2 38.0(15) 3_555 . 1_555 N
Al1 O2 Al1 105.94(20) 208_353 . -211_464 N
Al1 O2 Al1 160.98(26) 208_353 . -304_454 N
Al1 O2 O1 120.07(27) 208_343 . 111_433 N
Al1 O2 O1 35.18(23) 208_343 . -108_544 N
Al1 O2 O2 135.14(27) 208_343 . 107_433 N
Al1 O2 O2 75.41(27) 208_343 . 209_343 N
Al1 O2 O2 82.48(25) 208_343 . -304_444 N
Al1 O2 O3 81.55(24) 208_343 . 4_555 N
Al1 O2 O3 34.35(23) 208_343 . 111_433 N
Al1 O2 O3 177.41(26) 208_343 . 208_343 N
Al1 O2 O4 36.08(21) 208_343 . 310_334 N
Al1 O2 O4 120.75(24) 208_343 . 312_334 N
Al1 O2 SI 99.19(25) 208_343 . 4_555 N
Al1 O2 SI' 106.05(27) 208_343 . 111_433 N
Al1 O2 Dd2 123.2(12) 208_443 . 1_555 N
Al1 O2 Al1 73.31(14) -211_464 . -304_454 N
Al1 O2 O1 26.12(14) -211_454 . 111_433 N
Al1 O2 O1 70.76(15) -211_454 . -108_544 N
Al1 O2 O2 86.81(13) -211_454 . 107_433 N
Al1 O2 O2 110.94(10) -211_454 . 209_343 N
Al1 O2 O2 130.54(15) -211_454 . -304_444 N
Al1 O2 O3 25.08(12) -211_454 . 4_555 N
Al1 O2 O3 123.76(17) -211_454 . 111_433 N
Al1 O2 O3 76.58(15) -211_454 . 208_343 N
Al1 O2 O4 120.43(14) -211_454 . 310_334 N
Al1 O2 O4 83.77(16) -211_454 . 312_334 N
Al1 O2 SI 66.57(11) -211_454 . 4_555 N
Al1 O2 SI' 112.42(24) -211_454 . 111_433 N
Al1 O2 Dd2 70.4(15) -211_554 . 1_555 N
Al1 O2 O1 67.53(18) -304_444 . 111_433 N
Al1 O2 O1 138.96(17) -304_444 . -108_544 N
Al1 O2 O2 27.11(12) -304_444 . 107_433 N
Al1 O2 O2 87.02(12) -304_444 . 209_343 N
Al1 O2 O2 112.85(19) -304_444 . -304_444 N
Al1 O2 O3 94.44(14) -304_444 . 4_555 N
Al1 O2 O3 130.14(15) -304_444 . 111_433 N
Al1 O2 O3 20.01(12) -304_444 . 208_343 N
Al1 O2 O4 159.70(18) -304_444 . 310_334 N
Al1 O2 O4 78.26(15) -304_444 . 312_334 N
Al1 O2 SI 62.68(11) -304_444 . 4_555 N
Al1 O2 SI' 58.75(12) -304_444 . 111_433 N
Al1 O2 Dd2 75.0(12) -304_544 . 1_555 N
O1 O2 O1 87.48(8) 111_433 . -108_544 N
O1 O2 O2 90.12(20) 111_433 . 107_433 N
O1 O2 O2 133.39(15) 111_433 . 209_343 N
O1 O2 O2 107.68(20) 111_433 . -304_444 N
O1 O2 O3 48.06(12) 111_433 . 4_555 N
O1 O2 O3 147.36(19) 111_433 . 111_433 N
O1 O2 O3 61.99(17) 111_433 . 208_343 N
O1 O2 O4 117.37(19) 111_433 . 310_334 N
O1 O2 O4 57.85(16) 111_433 . 312_334 N
O1 O2 SI 87.21(16) 111_433 . 4_555 N
O1 O2 SI' 122.10(24) 111_433 . 111_433 N
O1 O2 Dd2 44.5(15) 111_533 . 1_555 N
O1 O2 O2 131.21(15) -108_544 . 107_433 N
O1 O2 O2 87.79(20) -108_544 . 209_343 N
O1 O2 O2 105.38(18) -108_544 . -304_444 N
O1 O2 O3 46.57(12) -108_544 . 4_555 N
O1 O2 O3 61.30(16) -108_544 . 111_433 N
O1 O2 O3 147.34(17) -108_544 . 208_343 N
O1 O2 O4 60.84(15) -108_544 . 310_334 N
O1 O2 O4 116.22(18) -108_544 . 312_334 N
O1 O2 SI 85.03(16) -108_544 . 4_555 N
O1 O2 SI' 119.68(25) -108_544 . 111_433 N
O1 O2 Dd2 110.0(11) -108_644 . 1_555 N
O2 O2 O2 60.00000(30) 107_433 . 209_343 N
O2 O2 O2 121.60(12) 107_433 . -304_444 N
O2 O2 O3 100.12(8) 107_433 . 4_555 N
O2 O2 O3 103.06(14) 107_433 . 111_433 N
O2 O2 O3 45.01(13) 107_433 . 208_343 N
O2 O2 O4 151.84(13) 107_433 . 310_334 N
O2 O2 O4 103.04(19) 107_433 . 312_334 N
O2 O2 SI 46.18(4) 107_433 . 4_555 N
O2 O2 SI' 32.72(9) 107_433 . 111_433 N
O2 O2 Dd2 101.6(12) 107_533 . 1_555 N
O2 O2 O2 118.25(14) 209_343 . -304_444 N
O2 O2 O3 99.42(9) 209_343 . 4_555 N
O2 O2 O3 43.66(14) 209_343 . 111_433 N
O2 O2 O3 104.39(13) 209_343 . 208_343 N
O2 O2 O4 100.15(19) 209_343 . 310_334 N
O2 O2 O4 155.38(14) 209_343 . 312_334 N
O2 O2 SI 46.18(4) 209_343 . 4_555 N
O2 O2 SI' 32.72(9) 209_343 . 111_433 N
O2 O2 Dd2 160.9(11) 209_443 . 1_555 N
O2 O2 O3 133.36(6) -304_444 . 4_555 N
O2 O2 O3 90.78(17) -304_444 . 111_433 N
O2 O2 O3 95.43(19) -304_444 . 208_343 N
O2 O2 O4 47.08(12) -304_444 . 310_334 N
O2 O2 O4 52.74(13) -304_444 . 312_334 N
O2 O2 SI 161.90(7) -304_444 . 4_555 N
O2 O2 SI' 111.46(23) -304_444 . 111_433 N
O2 O2 Dd2 65.0(15) -304_544 . 1_555 N
O3 O2 O3 99.75(14) 4_555 . 111_433 N
O3 O2 O3 101.01(13) 4_555 . 208_343 N
O3 O2 O4 102.97(13) 4_555 . 310_334 N
O3 O2 O4 101.27(13) 4_555 . 312_334 N
O3 O2 SI 64.39(8) 4_555 . 4_555 N
O3 O2 SI' 115.03(25) 4_555 . 111_433 N
O3 O2 Dd2 88.6(14) 4_555 . 1_555 N
O3 O2 O3 144.55(15) 111_433 . 208_343 N
O3 O2 O4 57.32(14) 111_433 . 310_334 N
O3 O2 O4 142.76(17) 111_433 . 312_334 N
O3 O2 SI 81.18(13) 111_433 . 4_555 N
O3 O2 SI' 71.99(13) 111_433 . 111_433 N
O3 O2 Dd2 152.0(14) 111_533 . 1_555 N
O3 O2 O4 142.08(18) 208_343 . 310_334 N
O3 O2 O4 58.57(15) 208_343 . 312_334 N
O3 O2 SI 82.33(12) 208_343 . 4_555 N
O3 O2 SI' 73.26(13) 208_343 . 111_433 N
O3 O2 Dd2 56.8(12) 208_443 . 1_555 N
O4 O2 O4 88.06(14) 310_334 . 312_334 N
O4 O2 SI 134.78(19) 310_334 . 4_555 N
O4 O2 SI' 120.53(21) 310_334 . 111_433 N
O4 O2 Dd2 94.9(13) 310_434 . 1_555 N
O4 O2 SI 135.83(18) 312_334 . 4_555 N
O4 O2 SI' 124.06(21) 312_334 . 111_433 N
O4 O2 Dd2 13.3(14) 312_434 . 1_555 N
SI O2 SI' 50.64(22) 4_555 . 111_433 N
SI O2 Dd2 126.0(15) 4_555 . 1_555 N
SI' O2 Dd2 128.3(11) 111_533 . 1_555 N
Si1 O3 Si1 95.45(20) 3_555 . -2_555 N
Si1 O3 Si1 162.67(25) 3_555 . 310_335 N
Si1 O3 Si2 142.40(29) 3_555 . 2_555 N
Si1 O3 Si2 48.47(20) 3_555 . -3_555 N
Si1 O3 Si2 53.75(23) 3_555 . 312_434 N
Si1 O3 Al1 142.40(29) 3_555 . 2_555 N
Si1 O3 Al1 48.47(20) 3_555 . -3_555 N
Si1 O3 Al1 53.75(23) 3_555 . 312_344 N
Si1 O3 O1 34.27(27) 3_555 . 3_555 N
Si1 O3 O1 116.59(28) 3_555 . -2_555 N
Si1 O3 O2 32.97(20) 3_555 . -105_444 N
Si1 O3 O2 120.77(23) 3_555 . -206_444 N
Si1 O3 O2 72.82(21) 3_555 . 304_445 N
Si1 O3 O3 137.30(26) 3_555 . 107_433 N
Si1 O3 O3 77.49(26) 3_555 . 209_343 N
Si1 O3 O4 36.78(22) 3_555 . 111_433 N
Si1 O3 O4 174.43(25) 3_555 . 208_343 N
Si1 O3 SI 72.19(20) 3_555 . 1_555 N
Si1 O3 SI' 80.48(22) 3_555 . 1_555 N
Si1 O3 SII 107.87(26) 3_555 . 111_555 N
Si1 O3 SJ 145.7(5) 3_555 . 3_555 N
Si1 O3 Dc2 128.0(4) 3_555 . 3_555 N
Si1 O3 Dc2 42.5(4) 3_555 . -1_555 N
Si1 O3 Dd2 148.4(15) 3_555 . 3_555 N
Si1 O3 Si1 101.80(15) -2_555 . 310_335 N
Si1 O3 Si2 49.41(23) -2_555 . 2_555 N
Si1 O3 Si2 47.69(10) -2_555 . -3_555 N
Si1 O3 Si2 145.18(16) -2_555 . 312_434 N
Si1 O3 Al1 49.41(23) -2_555 . 2_555 N
Si1 O3 Al1 47.69(10) -2_555 . -3_555 N
Si1 O3 Al1 145.18(16) -2_555 . 312_344 N
Si1 O3 O1 66.51(18) -2_555 . 3_555 N
Si1 O3 O1 21.80(16) -2_555 . -2_555 N
Si1 O3 O2 96.58(13) -2_555 . -105_444 N
Si1 O3 O2 64.92(12) -2_555 . -206_444 N
Si1 O3 O2 23.07(10) -2_555 . 304_445 N
Si1 O3 O3 126.53(19) -2_555 . 107_433 N
Si1 O3 O3 163.34(13) -2_555 . 209_343 N
Si1 O3 O4 123.55(16) -2_555 . 111_433 N
Si1 O3 O4 84.32(15) -2_555 . 208_343 N
Si1 O3 SI 55.64(9) -2_555 . 1_555 N
Si1 O3 SI' 90.46(18) -2_555 . 1_555 N
Si1 O3 SII 141.27(23) -2_555 . 111_555 N
Si1 O3 SJ 65.1(5) -2_555 . 3_555 N
Si1 O3 Dc2 44.00(25) -2_555 . 3_555 N
Si1 O3 Dc2 79.04(29) -2_555 . -1_555 N
Si1 O3 Dd2 76.1(15) -2_555 . 3_555 N
Si1 O3 Si2 53.81(25) 310_434 . 2_555 N
Si1 O3 Si2 148.81(16) 310_434 . -3_555 N
Si1 O3 Si2 110.09(12) 310_434 . 312_434 N
Si1 O3 Al1 53.81(25) 310_344 . 2_555 N
Si1 O3 Al1 148.81(16) 310_344 . -3_555 N
Si1 O3 Al1 110.09(12) 310_344 . 312_344 N
Si1 O3 O1 159.93(21) 310_334 . 3_555 N
Si1 O3 O1 80.73(21) 310_334 . -2_555 N
Si1 O3 O2 140.83(15) 310_334 . -105_444 N
Si1 O3 O2 66.53(13) 310_334 . -206_444 N
Si1 O3 O2 124.21(15) 310_334 . 304_445 N
Si1 O3 O3 26.32(12) 310_334 . 107_433 N
Si1 O3 O3 86.26(12) 310_334 . 209_343 N
Si1 O3 O4 129.25(14) 310_334 . 111_433 N
Si1 O3 O4 18.90(11) 310_334 . 208_343 N
Si1 O3 SI 116.61(13) 310_334 . 1_555 N
Si1 O3 SI' 97.62(16) 310_334 . 1_555 N
Si1 O3 SII 58.66(12) 310_456 . 111_555 N
Si1 O3 SJ 47.6(5) 310_446 . 3_555 N
Si1 O3 Dc2 67.70(34) 310_456 . 3_555 N
Si1 O3 Dc2 142.96(35) 310_456 . -1_555 N
Si1 O3 Dd2 41.2(15) 310_434 . 3_555 N
Si2 O3 Si2 96.93(22) 2_555 . -3_555 N
Si2 O3 Si2 163.83(26) 2_555 . 312_434 N
Si2 O3 Al1 0.0 2_555 . 2_555 N
Si2 O3 Al1 96.93(22) 2_555 . -3_555 N
Si2 O3 Al1 163.83(26) 2_555 . 312_344 N
Si2 O3 O1 115.81(29) 2_555 . 3_555 N
Si2 O3 O1 31.54(27) 2_555 . -2_555 N
Si2 O3 O2 125.38(25) 2_555 . -105_444 N
Si2 O3 O2 39.28(22) 2_555 . -206_444 N
Si2 O3 O2 70.66(24) 2_555 . 304_445 N
Si2 O3 O3 80.02(29) 2_555 . 107_433 N
Si2 O3 O3 140.02(29) 2_555 . 209_343 N
Si2 O3 O4 168.97(29) 2_555 . 111_433 N
Si2 O3 O4 39.44(24) 2_555 . 208_343 N
Si2 O3 SI 75.69(22) 2_555 . 1_555 N
Si2 O3 SI' 86.22(24) 2_555 . 1_555 N
Si2 O3 SII 108.87(28) 2_555 . 111_555 N
Si2 O3 SJ 40.0(5) 2_555 . 3_555 N
Si2 O3 Dc2 37.9(4) 2_555 . 3_555 N
Si2 O3 Dc2 123.7(4) 2_555 . -1_555 N
Si2 O3 Dd2 47.9(15) 2_555 . 3_555 N
Si2 O3 Si2 98.48(15) -3_555 . 312_434 N
Si2 O3 Al1 96.93(22) -3_555 . 2_555 N
Si2 O3 Al1 0.0 -3_555 . -3_555 N
Si2 O3 Al1 98.48(15) -3_555 . 312_344 N
Si2 O3 O1 20.49(15) -3_555 . 3_555 N
Si2 O3 O1 68.20(19) -3_555 . -2_555 N
Si2 O3 O2 62.16(12) -3_555 . -105_444 N
Si2 O3 O2 98.64(13) -3_555 . -206_444 N
Si2 O3 O2 26.96(11) -3_555 . 304_445 N
Si2 O3 O3 165.38(11) -3_555 . 107_433 N
Si2 O3 O3 121.52(19) -3_555 . 209_343 N
Si2 O3 O4 77.36(15) -3_555 . 111_433 N
Si2 O3 O4 130.19(16) -3_555 . 208_343 N
Si2 O3 SI 56.14(10) -3_555 . 1_555 N
Si2 O3 SI' 89.97(19) -3_555 . 1_555 N
Si2 O3 SII 138.33(22) -3_555 . 111_555 N
Si2 O3 SJ 104.0(5) -3_555 . 3_555 N
Si2 O3 Dc2 82.43(33) -3_555 . 3_555 N
Si2 O3 Dc2 41.03(27) -3_555 . -1_555 N
Si2 O3 Dd2 112.9(15) -3_555 . 3_555 N
Si2 O3 Al1 163.83(26) 312_344 . 2_555 N
Si2 O3 Al1 98.48(15) 312_344 . -3_555 N
Si2 O3 Al1 0.0 312_344 . 312_344 N
Si2 O3 O1 78.87(21) 312_334 . 3_555 N
Si2 O3 O1 158.00(24) 312_334 . -2_555 N
Si2 O3 O2 67.05(14) 312_334 . -105_444 N
Si2 O3 O2 141.40(16) 312_334 . -206_444 N
Si2 O3 O2 125.14(16) 312_334 . 304_445 N
Si2 O3 O3 83.84(12) 312_334 . 107_433 N
Si2 O3 O3 23.84(12) 312_334 . 209_343 N
Si2 O3 O4 21.63(12) 312_334 . 111_433 N
Si2 O3 O4 124.63(13) 312_334 . 208_343 N
Si2 O3 SI 117.33(14) 312_334 . 1_555 N
Si2 O3 SI' 98.62(16) 312_334 . 1_555 N
Si2 O3 SII 55.63(12) 312_456 . 111_555 N
Si2 O3 SJ 130.1(5) 312_446 . 3_555 N
Si2 O3 Dc2 140.39(28) 312_456 . 3_555 N
Si2 O3 Dc2 67.18(31) 312_456 . -1_555 N
Si2 O3 Dd2 120.3(15) 312_434 . 3_555 N
Al1 O3 Al1 96.93(22) 2_555 . -3_555 N
Al1 O3 Al1 163.83(26) 2_555 . 312_344 N
Al1 O3 O1 115.81(29) 2_555 . 3_555 N
Al1 O3 O1 31.54(27) 2_555 . -2_555 N
Al1 O3 O2 125.38(25) 2_555 . -105_444 N
Al1 O3 O2 39.28(22) 2_555 . -206_444 N
Al1 O3 O2 70.66(24) 2_555 . 304_445 N
Al1 O3 O3 80.02(29) 2_555 . 107_433 N
Al1 O3 O3 140.02(29) 2_555 . 209_343 N
Al1 O3 O4 168.97(29) 2_555 . 111_433 N
Al1 O3 O4 39.44(24) 2_555 . 208_343 N
Al1 O3 SI 75.69(22) 2_555 . 1_555 N
Al1 O3 SI' 86.22(24) 2_555 . 1_555 N
Al1 O3 SII 108.87(28) 2_555 . 111_555 N
Al1 O3 SJ 40.0(5) 2_555 . 3_555 N
Al1 O3 Dc2 37.9(4) 2_555 . 3_555 N
Al1 O3 Dc2 123.7(4) 2_555 . -1_555 N
Al1 O3 Dd2 47.9(15) 2_555 . 3_555 N
Al1 O3 Al1 98.48(15) -3_555 . 312_344 N
Al1 O3 O1 20.49(15) -3_555 . 3_555 N
Al1 O3 O1 68.20(19) -3_555 . -2_555 N
Al1 O3 O2 62.16(12) -3_555 . -105_444 N
Al1 O3 O2 98.64(13) -3_555 . -206_444 N
Al1 O3 O2 26.96(11) -3_555 . 304_445 N
Al1 O3 O3 165.38(11) -3_555 . 107_433 N
Al1 O3 O3 121.52(19) -3_555 . 209_343 N
Al1 O3 O4 77.36(15) -3_555 . 111_433 N
Al1 O3 O4 130.19(16) -3_555 . 208_343 N
Al1 O3 SI 56.14(10) -3_555 . 1_555 N
Al1 O3 SI' 89.97(19) -3_555 . 1_555 N
Al1 O3 SII 138.33(22) -3_555 . 111_555 N
Al1 O3 SJ 104.0(5) -3_555 . 3_555 N
Al1 O3 Dc2 82.43(33) -3_555 . 3_555 N
Al1 O3 Dc2 41.03(27) -3_555 . -1_555 N
Al1 O3 Dd2 112.9(15) -3_555 . 3_555 N
Al1 O3 O1 78.87(21) 312_334 . 3_555 N
Al1 O3 O1 158.00(24) 312_334 . -2_555 N
Al1 O3 O2 67.05(14) 312_334 . -105_444 N
Al1 O3 O2 141.40(16) 312_334 . -206_444 N
Al1 O3 O2 125.14(16) 312_334 . 304_445 N
Al1 O3 O3 83.84(12) 312_334 . 107_433 N
Al1 O3 O3 23.84(12) 312_334 . 209_343 N
Al1 O3 O4 21.63(12) 312_334 . 111_433 N
Al1 O3 O4 124.63(13) 312_334 . 208_343 N
Al1 O3 SI 117.33(14) 312_334 . 1_555 N
Al1 O3 SI' 98.62(16) 312_334 . 1_555 N
Al1 O3 SII 55.63(12) 312_456 . 111_555 N
Al1 O3 SJ 130.1(5) 312_446 . 3_555 N
Al1 O3 Dc2 140.39(28) 312_456 . 3_555 N
Al1 O3 Dc2 67.18(31) 312_456 . -1_555 N
Al1 O3 Dd2 120.3(15) 312_434 . 3_555 N
O1 O3 O1 85.29(9) 3_555 . -2_555 N
O1 O3 O2 58.94(19) 3_555 . -105_444 N
O1 O3 O2 118.05(14) 3_555 . -206_444 N
O1 O3 O2 47.29(15) 3_555 . 304_445 N
O1 O3 O3 153.24(13) 3_555 . 107_433 N
O1 O3 O3 101.32(23) 3_555 . 209_343 N
O1 O3 O4 57.40(20) 3_555 . 111_433 N
O1 O3 O4 142.35(22) 3_555 . 208_343 N
O1 O3 SI 71.40(9) 3_555 . 1_555 N
O1 O3 SI' 98.69(19) 3_555 . 1_555 N
O1 O3 SII 119.80(21) 3_555 . 111_555 N
O1 O3 SJ 112.7(5) 3_555 . 3_555 N
O1 O3 Dc2 93.8(4) 3_555 . 3_555 N
O1 O3 Dc2 23.31(29) 3_555 . -1_555 N
O1 O3 Dd2 118.7(15) 3_555 . 3_555 N
O1 O3 O2 116.99(15) -2_555 . -105_444 N
O1 O3 O2 60.15(19) -2_555 . -206_444 N
O1 O3 O2 44.86(15) -2_555 . 304_445 N
O1 O3 O3 104.80(24) -2_555 . 107_433 N
O1 O3 O3 155.90(12) -2_555 . 209_343 N
O1 O3 O4 138.89(26) -2_555 . 111_433 N
O1 O3 O4 62.74(19) -2_555 . 208_343 N
O1 O3 SI 70.77(9) -2_555 . 1_555 N
O1 O3 SI' 98.78(17) -2_555 . 1_555 N
O1 O3 SII 122.91(21) -2_555 . 111_555 N
O1 O3 SJ 44.4(5) -2_555 . 3_555 N
O1 O3 Dc2 25.40(23) -2_555 . 3_555 N
O1 O3 Dc2 92.5(4) -2_555 . -1_555 N
O1 O3 Dd2 55.5(15) -2_555 . 3_555 N
O2 O3 O2 91.33(15) -105_444 . -206_444 N
O2 O3 O2 75.21(12) -105_444 . 304_445 N
O2 O3 O3 131.04(11) -105_444 . 107_433 N
O2 O3 O3 85.69(16) -105_444 . 209_343 N
O2 O3 O4 60.43(14) -105_444 . 111_433 N
O2 O3 O4 152.59(17) -105_444 . 208_343 N
O2 O3 SI 50.30(8) -105_444 . 1_555 N
O2 O3 SI' 47.61(9) -105_444 . 1_555 N
O2 O3 SII 119.84(20) -105_566 . 111_555 N
O2 O3 SJ 161.4(5) -105_556 . 3_555 N
O2 O3 Dc2 140.39(28) -105_566 . 3_555 N
O2 O3 Dc2 74.3(4) -105_566 . -1_555 N
O2 O3 Dd2 172.4(15) -105_544 . 3_555 N
O2 O3 O2 74.56(11) -206_444 . 304_445 N
O2 O3 O3 88.06(16) -206_444 . 107_433 N
O2 O3 O3 131.65(11) -206_444 . 209_343 N
O2 O3 O4 150.21(16) -206_444 . 111_433 N
O2 O3 O4 64.15(14) -206_444 . 208_343 N
O2 O3 SI 50.10(8) -206_444 . 1_555 N
O2 O3 SI' 47.18(8) -206_444 . 1_555 N
O2 O3 SII 122.12(20) -206_566 . 111_555 N
O2 O3 SJ 78.0(5) -206_556 . 3_555 N
O2 O3 Dc2 76.21(31) -206_566 . 3_555 N
O2 O3 Dc2 139.45(27) -206_566 . -1_555 N
O2 O3 Dd2 83.6(15) -206_544 . 3_555 N
O2 O3 O3 149.56(19) 304_445 . 107_433 N
O2 O3 O3 148.47(19) 304_445 . 209_343 N
O2 O3 O4 104.27(16) 304_445 . 111_433 N
O2 O3 O4 107.28(15) 304_445 . 208_343 N
O2 O3 SI 44.43(5) 304_445 . 1_555 N
O2 O3 SI' 82.49(17) 304_445 . 1_555 N
O2 O3 SII 154.46(24) 304_445 . 111_555 N
O2 O3 SJ 87.1(5) 304_445 . 3_555 N
O2 O3 Dc2 65.28(28) 304_445 . 3_555 N
O2 O3 Dc2 65.20(26) 304_445 . -1_555 N
O2 O3 Dd2 97.9(15) 304_445 . 3_555 N
O3 O3 O3 60.00000(30) 107_433 . 209_343 N
O3 O3 O4 103.11(13) 107_433 . 111_433 N
O3 O3 O4 42.29(12) 107_433 . 208_343 N
O3 O3 SI 135.22(12) 107_433 . 1_555 N
O3 O3 SI' 104.01(16) 107_433 . 1_555 N
O3 O3 SII 34.26(10) 107_555 . 111_555 N
O3 O3 SJ 64.6(5) 107_545 . 3_555 N
O3 O3 Dc2 86.62(32) 107_555 . 3_555 N
O3 O3 Dc2 130.02(28) 107_555 . -1_555 N
O3 O3 Dd2 54.7(15) 107_533 . 3_555 N
O3 O3 O4 44.20(13) 209_343 . 111_433 N
O3 O3 O4 101.24(12) 209_343 . 208_343 N
O3 O3 SI 133.33(13) 209_343 . 1_555 N
O3 O3 SI' 103.01(16) 209_343 . 1_555 N
O3 O3 SII 34.26(10) 209_465 . 111_555 N
O3 O3 SJ 112.8(5) 209_455 . 3_555 N
O3 O3 Dc2 130.51(23) 209_465 . 3_555 N
O3 O3 Dc2 85.76(29) 209_465 . -1_555 N
O3 O3 Dd2 101.9(15) 209_443 . 3_555 N
O4 O3 O4 139.86(14) 111_433 . 208_343 N
O4 O3 SI 107.90(14) 111_433 . 1_555 N
O4 O3 SI' 103.05(15) 111_433 . 1_555 N
O4 O3 SII 71.26(12) 111_555 . 111_555 N
O4 O3 SJ 131.8(5) 111_545 . 3_555 N
O4 O3 Dc2 131.2(4) 111_555 . 3_555 N
O4 O3 Dc2 46.43(33) 111_555 . -1_555 N
O4 O3 Dd2 125.4(15) 111_533 . 3_555 N
O4 O3 SI 111.94(14) 208_343 . 1_555 N
O4 O3 SI' 105.08(16) 208_343 . 1_555 N
O4 O3 SII 69.53(11) 208_465 . 111_555 N
O4 O3 SJ 29.9(5) 208_455 . 3_555 N
O4 O3 Dc2 48.90(33) 208_465 . 3_555 N
O4 O3 Dc2 132.2(4) 208_465 . -1_555 N
O4 O3 Dd2 26.2(15) 208_443 . 3_555 N
SI O3 SI' 38.06(17) 1_555 . 1_555 N
SI O3 SII 161.06(24) 1_555 . 111_555 N
SI O3 SJ 112.3(5) 1_555 . 3_555 N
SI O3 Dc2 96.16(23) 1_555 . 3_555 N
SI O3 Dc2 94.70(29) 1_555 . -1_555 N
SI O3 Dd2 122.4(15) 1_555 . 3_555 N
SI' O3 SII 123.03(30) 1_555 . 111_555 N
SI' O3 SJ 125.0(5) 1_555 . 3_555 N
SI' O3 Dc2 120.99(29) 1_555 . 3_555 N
SI' O3 Dc2 119.4(4) 1_555 . -1_555 N
SI' O3 Dd2 129.2(15) 1_555 . 3_555 N
SII O3 SJ 78.8(5) 111_545 . 3_555 N
SII O3 Dc2 98.10(28) 111_555 . 3_555 N
SII O3 Dc2 97.46(31) 111_555 . -1_555 N
SII O3 Dd2 67.8(15) 111_533 . 3_555 N
SJ O3 Dc2 22.1(6) 3_555 . 3_555 N
SJ O3 Dc2 103.9(6) 3_555 . -1_555 N
SJ O3 Dd2 11.1(16) 3_555 . 3_555 N
Dc2 O3 Dc2 90.92(7) 3_555 . -1_555 N
Dc2 O3 Dd2 32.6(15) 3_555 . 3_555 N
Dc2 O3 Dd2 106.0(15) -1_555 . 3_555 N
Si1 O4 Si1 98.65(24) 107_434 . -105_445 N
Si1 O4 Si2 144.17(31) 107_533 . 209_443 N
Si1 O4 Si2 51.09(23) 107_533 . -206_544 N
Si1 O4 Al1 144.17(31) 107_443 . 209_353 N
Si1 O4 Al1 51.09(23) 107_443 . -206_454 N
Si1 O4 O1 37.44(23) 107_433 . 107_433 N
Si1 O4 O1 162.12(30) 107_433 . -309_445 N
Si1 O4 O2 110.67(26) 107_433 . 310_334 N
Si1 O4 O2 31.02(22) 107_433 . 312_334 N
Si1 O4 O3 127.79(27) 107_433 . -105_444 N
Si1 O4 O3 41.55(23) 107_433 . -206_444 N
Si1 O4 O4 77.60(24) 107_433 . -304_444 N
Si1 O4 SII 91.46(24) 107_555 . 1_555 N
Si1 O4 SJ 120.7(10) 107_545 . 312_446 N
Si1 O4 Oc 89.37(33) 107_545 . 6_555 N
Si1 O4 Oc 136.6(4) 107_545 . 312_446 N
Si1 O4 Dc1 120.6(4) 107_554 . 312_455 N
Si1 O4 Dc2 75.2(4) 107_555 . 6_555 N
Si1 O4 Dc2 145.0(5) 107_555 . 312_456 N
Si1 O4 Od 116.0(14) 107_554 . 312_455 N
Si1 O4 Dd1 117.8(17) 107_533 . 312_434 N
Si1 O4 Dd2 115(4) 107_533 . 312_434 N
Si1 O4 DII'1 79.2(16) 107_433 . 1_555 N
Si1 O4 DII*1 116.2(15) 107_432 . 1_555 N
Si1 O4 Si2 54.29(22) -105_544 . 209_443 N
Si1 O4 Si2 48.97(11) -105_544 . -206_544 N
Si1 O4 Al1 54.29(22) -105_454 . 209_353 N
Si1 O4 Al1 48.97(11) -105_454 . -206_454 N
Si1 O4 O1 116.73(21) -105_444 . 107_433 N
Si1 O4 O1 65.92(17) -105_444 . -309_445 N
Si1 O4 O2 20.65(12) -105_444 . 310_334 N
Si1 O4 O2 67.83(14) -105_444 . 312_334 N
Si1 O4 O3 79.19(14) -105_444 . -105_444 N
Si1 O4 O3 118.43(15) -105_444 . -206_444 N
Si1 O4 O4 23.88(10) -105_444 . -304_444 N
Si1 O4 SII 118.74(20) -105_566 . 1_555 N
Si1 O4 SJ 114.4(10) -105_556 . 312_446 N
Si1 O4 Oc 117.09(29) -105_556 . 6_555 N
Si1 O4 Oc 108.87(25) -105_556 . 312_446 N
Si1 O4 Dc1 114.4(4) -105_565 . 312_455 N
Si1 O4 Dc2 126.5(5) -105_566 . 6_555 N
Si1 O4 Dc2 93.57(30) -105_566 . 312_456 N
Si1 O4 Od 123.7(13) -105_565 . 312_455 N
Si1 O4 Dd1 133.9(15) -105_544 . 312_434 N
Si1 O4 Dd2 135.7(34) -105_544 . 312_434 N
Si1 O4 DII'1 62.6(5) -105_444 . 1_555 N
Si1 O4 DII*1 141.2(23) -105_443 . 1_555 N
Si2 O4 Si2 102.37(24) 209_443 . -206_544 N
Si2 O4 Al1 0.0 209_353 . 209_353 N
Si2 O4 Al1 102.37(24) 209_353 . -206_454 N
Si2 O4 O1 168.25(30) 209_343 . 107_433 N
Si2 O4 O1 32.44(22) 209_343 . -309_445 N
Si2 O4 O2 36.69(22) 209_343 . 310_334 N
Si2 O4 O2 115.82(26) 209_343 . 312_334 N
Si2 O4 O3 35.05(22) 209_343 . -105_444 N
Si2 O4 O3 125.71(26) 209_343 . -206_444 N
Si2 O4 O4 78.16(24) 209_343 . -304_444 N
Si2 O4 SII 84.31(23) 209_465 . 1_555 N
Si2 O4 SJ 93.8(10) 209_455 . 312_446 N
Si2 O4 Oc 122.46(35) 209_455 . 6_555 N
Si2 O4 Oc 78.57(31) 209_455 . 312_446 N
Si2 O4 Dc1 93.85(33) 209_464 . 312_455 N
Si2 O4 Dc2 138.4(4) 209_465 . 6_555 N
Si2 O4 Dc2 67.3(4) 209_465 . 312_456 N
Si2 O4 Od 99.5(14) 209_464 . 312_455 N
Si2 O4 Dd1 97.7(17) 209_443 . 312_434 N
Si2 O4 Dd2 101(4) 209_443 . 312_434 N
Si2 O4 DII'1 67.8(15) 209_343 . 1_555 N
Si2 O4 DII*1 86.9(23) 209_342 . 1_555 N
Si2 O4 Al1 102.37(24) -206_454 . 209_353 N
Si2 O4 Al1 0.0 -206_454 . -206_454 N
Si2 O4 O1 70.68(19) -206_444 . 107_433 N
Si2 O4 O1 111.64(19) -206_444 . -309_445 N
Si2 O4 O2 65.86(14) -206_444 . 310_334 N
Si2 O4 O2 23.44(12) -206_444 . 312_334 N
Si2 O4 O3 116.39(15) -206_444 . -105_444 N
Si2 O4 O3 84.42(14) -206_444 . -206_444 N
Si2 O4 O4 26.52(11) -206_444 . -304_444 N
Si2 O4 SII 122.41(20) -206_566 . 1_555 N
Si2 O4 SJ 125.3(9) -206_556 . 312_446 N
Si2 O4 Oc 101.02(23) -206_556 . 6_555 N
Si2 O4 Oc 134.37(27) -206_556 . 312_446 N
Si2 O4 Dc1 125.1(4) -206_565 . 312_455 N
Si2 O4 Dc2 97.7(4) -206_566 . 6_555 N
Si2 O4 Dc2 124.4(5) -206_566 . 312_456 N
Si2 O4 Od 130.0(13) -206_565 . 312_455 N
Si2 O4 Dd1 143.9(16) -206_544 . 312_434 N
Si2 O4 Dd2 142(4) -206_544 . 312_434 N
Si2 O4 DII'1 69.6(15) -206_444 . 1_555 N
Si2 O4 DII*1 166.7(11) -206_443 . 1_555 N
Al1 O4 Al1 102.37(24) 209_353 . -206_454 N
Al1 O4 O1 168.25(30) 209_343 . 107_433 N
Al1 O4 O1 32.44(22) 209_343 . -309_445 N
Al1 O4 O2 36.69(22) 209_343 . 310_334 N
Al1 O4 O2 115.82(26) 209_343 . 312_334 N
Al1 O4 O3 35.05(22) 209_343 . -105_444 N
Al1 O4 O3 125.71(26) 209_343 . -206_444 N
Al1 O4 O4 78.16(24) 209_343 . -304_444 N
Al1 O4 SII 84.31(23) 209_465 . 1_555 N
Al1 O4 SJ 93.8(10) 209_455 . 312_446 N
Al1 O4 Oc 122.46(35) 209_455 . 6_555 N
Al1 O4 Oc 78.57(31) 209_455 . 312_446 N
Al1 O4 Dc1 93.85(33) 209_464 . 312_455 N
Al1 O4 Dc2 138.4(4) 209_465 . 6_555 N
Al1 O4 Dc2 67.3(4) 209_465 . 312_456 N
Al1 O4 Od 99.5(14) 209_464 . 312_455 N
Al1 O4 Dd1 97.7(17) 209_443 . 312_434 N
Al1 O4 Dd2 101(4) 209_443 . 312_434 N
Al1 O4 DII'1 67.8(15) 209_343 . 1_555 N
Al1 O4 DII*1 86.9(23) 209_342 . 1_555 N
Al1 O4 O1 70.68(19) -206_444 . 107_433 N
Al1 O4 O1 111.64(19) -206_444 . -309_445 N
Al1 O4 O2 65.86(14) -206_444 . 310_334 N
Al1 O4 O2 23.44(12) -206_444 . 312_334 N
Al1 O4 O3 116.39(15) -206_444 . -105_444 N
Al1 O4 O3 84.42(14) -206_444 . -206_444 N
Al1 O4 O4 26.52(11) -206_444 . -304_444 N
Al1 O4 SII 122.41(20) -206_566 . 1_555 N
Al1 O4 SJ 125.3(9) -206_556 . 312_446 N
Al1 O4 Oc 101.02(23) -206_556 . 6_555 N
Al1 O4 Oc 134.37(27) -206_556 . 312_446 N
Al1 O4 Dc1 125.1(4) -206_565 . 312_455 N
Al1 O4 Dc2 97.7(4) -206_566 . 6_555 N
Al1 O4 Dc2 124.4(5) -206_566 . 312_456 N
Al1 O4 Od 130.0(13) -206_565 . 312_455 N
Al1 O4 Dd1 143.9(16) -206_544 . 312_434 N
Al1 O4 Dd2 142(4) -206_544 . 312_434 N
Al1 O4 DII'1 69.6(15) -206_444 . 1_555 N
Al1 O4 DII*1 166.7(11) -206_443 . 1_555 N
O1 O4 O1 140.28(15) 107_433 . -309_445 N
O1 O4 O2 136.12(22) 107_433 . 310_334 N
O1 O4 O2 61.30(15) 107_433 . 312_334 N
O1 O4 O3 156.50(20) 107_433 . -105_444 N
O1 O4 O3 64.10(17) 107_433 . -206_444 N
O1 O4 O4 92.97(21) 107_433 . -304_444 N
O1 O4 SII 107.39(19) 107_555 . 1_555 N
O1 O4 SJ 83.3(9) 107_545 . 312_446 N
O1 O4 Oc 52.18(24) 107_545 . 6_555 N
O1 O4 Oc 99.33(27) 107_545 . 312_446 N
O1 O4 Dc1 83.16(28) 107_554 . 312_455 N
O1 O4 Dc2 37.81(29) 107_555 . 6_555 N
O1 O4 Dc2 108.3(4) 107_555 . 312_456 N
O1 O4 Od 79.1(14) 107_554 . 312_455 N
O1 O4 Dd1 83.9(17) 107_533 . 312_434 N
O1 O4 Dd2 81(4) 107_533 . 312_434 N
O1 O4 DII'1 116.6(16) 107_433 . 1_555 N
O1 O4 DII*1 101.7(24) 107_432 . 1_555 N
O1 O4 O2 57.77(14) -309_445 . 310_334 N
O1 O4 O2 133.39(20) -309_445 . 312_334 N
O1 O4 O3 60.56(14) -309_445 . -105_444 N
O1 O4 O3 153.32(19) -309_445 . -206_444 N
O1 O4 O4 85.36(19) -309_445 . -304_444 N
O1 O4 SII 103.74(18) -309_567 . 1_555 N
O1 O4 SJ 62.7(10) -309_557 . 312_446 N
O1 O4 Oc 90.02(27) -309_557 . 6_555 N
O1 O4 Oc 49.17(24) -309_557 . 312_446 N
O1 O4 Dc1 62.79(27) -309_566 . 312_455 N
O1 O4 Dc2 106.03(30) -309_567 . 6_555 N
O1 O4 Dc2 35.82(29) -309_567 . 312_456 N
O1 O4 Od 69.8(14) -309_566 . 312_455 N
O1 O4 Dd1 72.4(16) -309_545 . 312_434 N
O1 O4 Dd2 75(4) -309_545 . 312_434 N
O1 O4 DII'1 100.0(14) -309_445 . 1_555 N
O1 O4 DII*1 81.3(14) -309_444 . 1_555 N
O2 O4 O2 80.18(14) 310_334 . 312_334 N
O2 O4 O3 58.54(13) 310_334 . -105_444 N
O2 O4 O3 115.98(15) 310_334 . -206_444 N
O2 O4 O4 43.51(11) 310_334 . -304_444 N
O2 O4 SII 100.66(17) 310_456 . 1_555 N
O2 O4 SJ 117.3(10) 310_446 . 312_446 N
O2 O4 Oc 131.47(30) 310_446 . 6_555 N
O2 O4 Oc 106.39(25) 310_446 . 312_446 N
O2 O4 Dc1 117.32(31) 310_455 . 312_455 N
O2 O4 Dc2 144.4(5) 310_456 . 6_555 N
O2 O4 Dc2 91.70(27) 310_456 . 312_456 N
O2 O4 Od 125.9(14) 310_455 . 312_455 N
O2 O4 Dd1 130.2(16) 310_434 . 312_434 N
O2 O4 Dd2 133(4) 310_434 . 312_434 N
O2 O4 DII'1 52.3(7) 310_334 . 1_555 N
O2 O4 DII*1 122.2(25) 310_333 . 1_555 N
O2 O4 O3 115.53(16) 312_334 . -105_444 N
O2 O4 O3 61.00(13) 312_334 . -206_444 N
O2 O4 O4 48.44(11) 312_334 . -304_444 N
O2 O4 SII 102.89(17) 312_456 . 1_555 N
O2 O4 SJ 137.0(9) 312_446 . 312_446 N
O2 O4 Oc 106.05(24) 312_446 . 6_555 N
O2 O4 Oc 151.33(29) 312_446 . 312_446 N
O2 O4 Dc1 136.8(4) 312_455 . 312_455 N
O2 O4 Dc2 96.6(4) 312_456 . 6_555 N
O2 O4 Dc2 146.0(5) 312_456 . 312_456 N
O2 O4 Od 137.2(14) 312_455 . 312_455 N
O2 O4 Dd1 145.1(17) 312_434 . 312_434 N
O2 O4 Dd2 142(4) 312_434 . 312_434 N
O2 O4 DII'1 62.5(17) 312_334 . 1_555 N
O2 O4 DII*1 143.3(10) 312_333 . 1_555 N
O3 O4 O3 93.51(15) -105_444 . -206_444 N
O3 O4 O4 100.95(14) -105_444 . -304_444 N
O3 O4 SII 49.33(9) -105_566 . 1_555 N
O3 O4 SJ 106.6(9) -105_556 . 312_446 N
O3 O4 Oc 138.40(25) -105_556 . 6_555 N
O3 O4 Oc 90.68(27) -105_556 . 312_446 N
O3 O4 Dc1 106.78(31) -105_565 . 312_455 N
O3 O4 Dc2 145.8(4) -105_566 . 6_555 N
O3 O4 Dc2 86.6(4) -105_566 . 312_456 N
O3 O4 Od 107.3(14) -105_565 . 312_455 N
O3 O4 Dd1 97.2(17) -105_544 . 312_434 N
O3 O4 Dd2 100(4) -105_544 . 312_434 N
O3 O4 DII'1 53.2(17) -105_444 . 1_555 N
O3 O4 DII*1 66.4(26) -105_443 . 1_555 N
O3 O4 O4 107.30(14) -206_444 . -304_444 N
O3 O4 SII 50.06(9) -206_566 . 1_555 N
O3 O4 SJ 126.0(10) -206_556 . 312_446 N
O3 O4 Oc 108.27(31) -206_556 . 6_555 N
O3 O4 Oc 132.47(25) -206_556 . 312_446 N
O3 O4 Dc1 126.02(35) -206_565 . 312_455 N
O3 O4 Dc2 92.0(4) -206_566 . 6_555 N
O3 O4 Dc2 147.49(34) -206_566 . 312_456 N
O3 O4 Od 116.9(13) -206_565 . 312_455 N
O3 O4 Dd1 107.6(15) -206_544 . 312_434 N
O3 O4 Dd2 105.9(34) -206_544 . 312_434 N
O3 O4 DII'1 64.7(10) -206_444 . 1_555 N
O3 O4 DII*1 82.4(10) -206_443 . 1_555 N
O4 O4 SII 129.97(18) -304_566 . 1_555 N
O4 O4 SJ 116.7(9) -304_556 . 312_446 N
O4 O4 Oc 105.45(25) -304_556 . 6_555 N
O4 O4 Oc 118.26(24) -304_556 . 312_446 N
O4 O4 Dc1 116.6(4) -304_565 . 312_455 N
O4 O4 Dc2 109.5(5) -304_566 . 6_555 N
O4 O4 Dc2 104.6(4) -304_566 . 312_456 N
O4 O4 Od 124.9(12) -304_565 . 312_455 N
O4 O4 Dd1 139.3(14) -304_544 . 312_434 N
O4 O4 Dd2 139.3(30) -304_544 . 312_434 N
O4 O4 DII'1 69.5(9) -304_444 . 1_555 N
O4 O4 DII*1 165.0(22) -304_443 . 1_555 N
SII O4 SJ 110.8(9) 1_555 . 312_446 N
SII O4 Oc 123.31(32) 1_555 . 6_555 N
SII O4 Oc 103.18(30) 1_555 . 312_446 N
SII O4 Dc1 111.0(4) 1_555 . 312_455 N
SII O4 Dc2 114.5(5) 1_555 . 6_555 N
SII O4 Dc2 111.0(5) 1_555 . 312_456 N
SII O4 Od 104.0(12) 1_555 . 312_455 N
SII O4 Dd1 89.0(15) 1_555 . 312_434 N
SII O4 Dd2 89.7(31) 1_555 . 312_434 N
SII O4 DII'1 60.4(9) 1_555 . 1_555 N
SII O4 DII*1 48.3(17) 1_555 . 1_555 N
SJ O4 Oc 32.2(9) 312_446 . 6_555 N
SJ O4 Oc 16.3(9) 312_446 . 312_446 N
SJ O4 Dc1 0.1877(31) 312_455 . 312_455 N
SJ O4 Dc2 45.5(10) 312_456 . 6_555 N
SJ O4 Dc2 26.9(10) 312_456 . 312_456 N
SJ O4 Od 9.3(17) 312_455 . 312_455 N
SJ O4 Dd1 22.6(17) 312_434 . 312_434 N
SJ O4 Dd2 22.9(33) 312_434 . 312_434 N
SJ O4 DII'1 159.6(19) 312_334 . 1_555 N
SJ O4 DII*1 62.6(19) 312_333 . 1_555 N
Oc O4 Oc 48.47(34) 6_555 . 312_446 N
Oc O4 Dc1 32.07(34) 6_555 . 312_455 N
Oc O4 Dc2 16.37(11) 6_555 . 6_555 N
Oc O4 Dc2 56.1(4) 6_555 . 312_456 N
Oc O4 Od 31.3(13) 6_555 . 312_455 N
Oc O4 Dd1 43.0(16) 6_555 . 312_434 N
Oc O4 Dd2 41(4) 6_555 . 312_434 N
Oc O4 DII'1 168.2(17) 6_555 . 1_555 N
Oc O4 DII*1 81.5(24) 6_555 . 1_555 N
Oc O4 Dc1 16.42(7) 312_455 . 312_455 N
Oc O4 Dc2 61.5(4) 312_456 . 6_555 N
Oc O4 Dc2 15.34(11) 312_456 . 312_456 N
Oc O4 Od 21.0(14) 312_455 . 312_455 N
Oc O4 Dd1 25.2(15) 312_434 . 312_434 N
Oc O4 Dd2 27(4) 312_434 . 312_434 N
Oc O4 DII'1 143.3(17) 312_334 . 1_555 N
Oc O4 DII*1 56.4(12) 312_333 . 1_555 N
Dc1 O4 Dc2 45.4(4) 312_456 . 6_555 N
Dc1 O4 Dc2 26.97(20) 312_456 . 312_456 N
Dc1 O4 Od 9.4(13) 312_455 . 312_455 N
Dc1 O4 Dd1 22.7(14) 312_434 . 312_434 N
Dc1 O4 Dd2 23.0(31) 312_434 . 312_434 N
Dc1 O4 DII'1 159.7(17) 312_334 . 1_555 N
Dc1 O4 DII*1 62.7(18) 312_333 . 1_555 N
Dc2 O4 Dc2 71.2(5) 6_555 . 312_456 N
Dc2 O4 Od 41.6(14) 6_555 . 312_455 N
Dc2 O4 Dd1 49.2(17) 6_555 . 312_434 N
Dc2 O4 Dd2 46(4) 6_555 . 312_434 N
Dc2 O4 DII'1 153.8(15) 6_555 . 1_555 N
Dc2 O4 DII*1 81.0(26) 6_555 . 1_555 N
Dc2 O4 Od 34.4(14) 312_455 . 312_455 N
Dc2 O4 Dd1 40.5(15) 312_434 . 312_434 N
Dc2 O4 Dd2 43(4) 312_434 . 312_434 N
Dc2 O4 DII'1 134.9(16) 312_334 . 1_555 N
Dc2 O4 DII*1 67.9(11) 312_333 . 1_555 N
Od O4 Dd1 14.9(12) 312_434 . 312_434 N
Od O4 Dd2 14.4(26) 312_434 . 312_434 N
Od O4 DII'1 159.8(21) 312_334 . 1_555 N
Od O4 DII*1 56.1(23) 312_333 . 1_555 N
Dd1 O4 Dd2 3(5) 312_434 . 312_434 N
Dd1 O4 DII'1 146.5(21) 312_334 . 1_555 N
Dd1 O4 DII*1 41.2(24) 312_333 . 1_555 N
Dd2 O4 DII'1 148(4) 312_334 . 1_555 N
Dd2 O4 DII*1 42(4) 312_333 . 1_555 N
DII'1 O4 DII*1 106.0(26) 1_555 . 1_555 N
Si1 SI Si1 101.92(11) 1_555 . 2_555 N
Si1 SI Si1 101.92(11) 1_555 . 3_555 N
Si1 SI Si1 179.972 1_555 . -1_555 N
Si1 SI Si1 78.08(11) 1_555 . -2_555 N
Si1 SI Si1 78.08(11) 1_555 . -3_555 N
Si1 SI Si2 128.40(10) 1_555 . 1_555 N
Si1 SI Si2 53.15(11) 1_555 . 2_555 N
Si1 SI Si2 53.88(11) 1_555 . 3_555 N
Si1 SI Si2 51.60(10) 1_555 . -1_555 N
Si1 SI Si2 126.85(11) 1_555 . -2_555 N
Si1 SI Si2 126.12(11) 1_555 . -3_555 N
Si1 SI Al1 128.40(10) 1_555 . 1_555 N
Si1 SI Al1 53.15(11) 1_555 . 2_555 N
Si1 SI Al1 53.88(11) 1_555 . 3_555 N
Si1 SI Al1 51.60(10) 1_555 . -1_555 N
Si1 SI Al1 126.85(11) 1_555 . -2_555 N
Si1 SI Al1 126.12(11) 1_555 . -3_555 N
Si1 SI O1 25.58(13) 1_555 . 1_555 N
Si1 SI O1 118.04(16) 1_555 . 2_555 N
Si1 SI O1 114.48(12) 1_555 . 3_555 N
Si1 SI O1 154.42(13) 1_555 . -1_555 N
Si1 SI O1 61.95(16) 1_555 . -2_555 N
Si1 SI O1 65.52(12) 1_555 . -3_555 N
Si1 SI O2 70.41(11) 1_555 . 105_544 N
Si1 SI Si1 101.92(11) 2_555 . 3_555 N
Si1 SI Si1 78.08(11) 2_555 . -1_555 N
Si1 SI Si1 179.972 2_555 . -2_555 N
Si1 SI Si1 78.08(11) 2_555 . -3_555 N
Si1 SI Si2 53.88(11) 2_555 . 1_555 N
Si1 SI Si2 128.40(10) 2_555 . 2_555 N
Si1 SI Si2 53.15(11) 2_555 . 3_555 N
Si1 SI Si2 126.12(11) 2_555 . -1_555 N
Si1 SI Si2 51.60(10) 2_555 . -2_555 N
Si1 SI Si2 126.85(11) 2_555 . -3_555 N
Si1 SI Al1 53.88(11) 2_555 . 1_555 N
Si1 SI Al1 128.40(10) 2_555 . 2_555 N
Si1 SI Al1 53.15(11) 2_555 . 3_555 N
Si1 SI Al1 126.12(11) 2_555 . -1_555 N
Si1 SI Al1 51.60(10) 2_555 . -2_555 N
Si1 SI Al1 126.85(11) 2_555 . -3_555 N
Si1 SI O1 114.48(12) 2_555 . 1_555 N
Si1 SI O1 25.58(13) 2_555 . 2_555 N
Si1 SI O1 118.04(16) 2_555 . 3_555 N
Si1 SI O1 65.52(12) 2_555 . -1_555 N
Si1 SI O1 154.42(13) 2_555 . -2_555 N
Si1 SI O1 61.95(16) 2_555 . -3_555 N
Si1 SI O2 103.15(13) 2_555 . 105_544 N
Si1 SI Si1 78.08(11) 3_555 . -1_555 N
Si1 SI Si1 78.08(11) 3_555 . -2_555 N
Si1 SI Si1 179.972 3_555 . -3_555 N
Si1 SI Si2 53.15(11) 3_555 . 1_555 N
Si1 SI Si2 53.88(11) 3_555 . 2_555 N
Si1 SI Si2 128.40(10) 3_555 . 3_555 N
Si1 SI Si2 126.85(11) 3_555 . -1_555 N
Si1 SI Si2 126.12(11) 3_555 . -2_555 N
Si1 SI Si2 51.60(10) 3_555 . -3_555 N
Si1 SI Al1 53.15(11) 3_555 . 1_555 N
Si1 SI Al1 53.88(11) 3_555 . 2_555 N
Si1 SI Al1 128.40(10) 3_555 . 3_555 N
Si1 SI Al1 126.85(11) 3_555 . -1_555 N
Si1 SI Al1 126.12(11) 3_555 . -2_555 N
Si1 SI Al1 51.60(10) 3_555 . -3_555 N
Si1 SI O1 118.04(16) 3_555 . 1_555 N
Si1 SI O1 114.48(12) 3_555 . 2_555 N
Si1 SI O1 25.58(13) 3_555 . 3_555 N
Si1 SI O1 61.95(16) 3_555 . -1_555 N
Si1 SI O1 65.52(12) 3_555 . -2_555 N
Si1 SI O1 154.42(13) 3_555 . -3_555 N
Si1 SI O2 154.80(12) 3_555 . 105_544 N
Si1 SI Si1 101.92(11) -1_555 . -2_555 N
Si1 SI Si1 101.92(11) -1_555 . -3_555 N
Si1 SI Si2 51.60(10) -1_555 . 1_555 N
Si1 SI Si2 126.85(11) -1_555 . 2_555 N
Si1 SI Si2 126.12(11) -1_555 . 3_555 N
Si1 SI Si2 128.40(10) -1_555 . -1_555 N
Si1 SI Si2 53.15(11) -1_555 . -2_555 N
Si1 SI Si2 53.88(11) -1_555 . -3_555 N
Si1 SI Al1 51.60(10) -1_555 . 1_555 N
Si1 SI Al1 126.85(11) -1_555 . 2_555 N
Si1 SI Al1 126.12(11) -1_555 . 3_555 N
Si1 SI Al1 128.40(10) -1_555 . -1_555 N
Si1 SI Al1 53.15(11) -1_555 . -2_555 N
Si1 SI Al1 53.88(11) -1_555 . -3_555 N
Si1 SI O1 154.42(13) -1_555 . 1_555 N
Si1 SI O1 61.95(16) -1_555 . 2_555 N
Si1 SI O1 65.52(12) -1_555 . 3_555 N
Si1 SI O1 25.58(13) -1_555 . -1_555 N
Si1 SI O1 118.04(16) -1_555 . -2_555 N
Si1 SI O1 114.48(12) -1_555 . -3_555 N
Si1 SI O2 109.59(11) -1_555 . 105_544 N
Si1 SI Si1 101.92(11) -2_555 . -3_555 N
Si1 SI Si2 126.12(11) -2_555 . 1_555 N
Si1 SI Si2 51.60(10) -2_555 . 2_555 N
Si1 SI Si2 126.85(11) -2_555 . 3_555 N
Si1 SI Si2 53.88(11) -2_555 . -1_555 N
Si1 SI Si2 128.40(10) -2_555 . -2_555 N
Si1 SI Si2 53.15(11) -2_555 . -3_555 N
Si1 SI Al1 126.12(11) -2_555 . 1_555 N
Si1 SI Al1 51.60(10) -2_555 . 2_555 N
Si1 SI Al1 126.85(11) -2_555 . 3_555 N
Si1 SI Al1 53.88(11) -2_555 . -1_555 N
Si1 SI Al1 128.40(10) -2_555 . -2_555 N
Si1 SI Al1 53.15(11) -2_555 . -3_555 N
Si1 SI O1 65.52(12) -2_555 . 1_555 N
Si1 SI O1 154.42(13) -2_555 . 2_555 N
Si1 SI O1 61.95(16) -2_555 . 3_555 N
Si1 SI O1 114.48(12) -2_555 . -1_555 N
Si1 SI O1 25.58(13) -2_555 . -2_555 N
Si1 SI O1 118.04(16) -2_555 . -3_555 N
Si1 SI O2 76.85(13) -2_555 . 105_544 N
Si1 SI Si2 126.85(11) -3_555 . 1_555 N
Si1 SI Si2 126.12(11) -3_555 . 2_555 N
Si1 SI Si2 51.60(10) -3_555 . 3_555 N
Si1 SI Si2 53.15(11) -3_555 . -1_555 N
Si1 SI Si2 53.88(11) -3_555 . -2_555 N
Si1 SI Si2 128.40(10) -3_555 . -3_555 N
Si1 SI Al1 126.85(11) -3_555 . 1_555 N
Si1 SI Al1 126.12(11) -3_555 . 2_555 N
Si1 SI Al1 51.60(10) -3_555 . 3_555 N
Si1 SI Al1 53.15(11) -3_555 . -1_555 N
Si1 SI Al1 53.88(11) -3_555 . -2_555 N
Si1 SI Al1 128.40(10) -3_555 . -3_555 N
Si1 SI O1 61.95(16) -3_555 . 1_555 N
Si1 SI O1 65.52(12) -3_555 . 2_555 N
Si1 SI O1 154.42(13) -3_555 . 3_555 N
Si1 SI O1 118.04(16) -3_555 . -1_555 N
Si1 SI O1 114.48(12) -3_555 . -2_555 N
Si1 SI O1 25.58(13) -3_555 . -3_555 N
Si1 SI O2 25.20(12) -3_555 . 105_544 N
Si2 SI Si2 103.01(12) 1_555 . 2_555 N
Si2 SI Si2 103.01(12) 1_555 . 3_555 N
Si2 SI Si2 180.0 1_555 . -1_555 N
Si2 SI Si2 76.99(12) 1_555 . -2_555 N
Si2 SI Si2 76.99(12) 1_555 . -3_555 N
Si2 SI Al1 0.0 1_555 . 1_555 N
Si2 SI Al1 103.01(12) 1_555 . 2_555 N
Si2 SI Al1 103.01(12) 1_555 . 3_555 N
Si2 SI Al1 180.0 1_555 . -1_555 N
Si2 SI Al1 76.99(12) 1_555 . -2_555 N
Si2 SI Al1 76.99(12) 1_555 . -3_555 N
Si2 SI O1 153.86(13) 1_555 . 1_555 N
Si2 SI O1 61.34(13) 1_555 . 2_555 N
Si2 SI O1 64.22(16) 1_555 . 3_555 N
Si2 SI O1 26.14(13) 1_555 . -1_555 N
Si2 SI O1 118.66(13) 1_555 . -2_555 N
Si2 SI O1 115.78(16) 1_555 . -3_555 N
Si2 SI O2 149.95(13) 1_555 . 105_544 N
Si2 SI Si2 103.01(12) 2_555 . 3_555 N
Si2 SI Si2 76.99(12) 2_555 . -1_555 N
Si2 SI Si2 180.0 2_555 . -2_555 N
Si2 SI Si2 76.99(12) 2_555 . -3_555 N
Si2 SI Al1 103.01(12) 2_555 . 1_555 N
Si2 SI Al1 0.0 2_555 . 2_555 N
Si2 SI Al1 103.01(12) 2_555 . 3_555 N
Si2 SI Al1 76.99(12) 2_555 . -1_555 N
Si2 SI Al1 180.0 2_555 . -2_555 N
Si2 SI Al1 76.99(12) 2_555 . -3_555 N
Si2 SI O1 64.22(16) 2_555 . 1_555 N
Si2 SI O1 153.86(13) 2_555 . 2_555 N
Si2 SI O1 61.34(13) 2_555 . 3_555 N
Si2 SI O1 115.78(16) 2_555 . -1_555 N
Si2 SI O1 26.14(13) 2_555 . -2_555 N
Si2 SI O1 118.66(13) 2_555 . -3_555 N
Si2 SI O2 106.88(13) 2_555 . 105_544 N
Si2 SI Si2 76.99(12) 3_555 . -1_555 N
Si2 SI Si2 76.99(12) 3_555 . -2_555 N
Si2 SI Si2 180.0 3_555 . -3_555 N
Si2 SI Al1 103.01(12) 3_555 . 1_555 N
Si2 SI Al1 103.01(12) 3_555 . 2_555 N
Si2 SI Al1 0.0 3_555 . 3_555 N
Si2 SI Al1 76.99(12) 3_555 . -1_555 N
Si2 SI Al1 76.99(12) 3_555 . -2_555 N
Si2 SI Al1 180.0 3_555 . -3_555 N
Si2 SI O1 61.34(13) 3_555 . 1_555 N
Si2 SI O1 64.22(16) 3_555 . 2_555 N
Si2 SI O1 153.86(13) 3_555 . 3_555 N
Si2 SI O1 118.66(13) 3_555 . -1_555 N
Si2 SI O1 115.78(16) 3_555 . -2_555 N
Si2 SI O1 26.14(13) 3_555 . -3_555 N
Si2 SI O2 67.38(11) 3_555 . 105_544 N
Si2 SI Si2 103.01(12) -1_555 . -2_555 N
Si2 SI Si2 103.01(12) -1_555 . -3_555 N
Si2 SI Al1 180.0 -1_555 . 1_555 N
Si2 SI Al1 76.99(12) -1_555 . 2_555 N
Si2 SI Al1 76.99(12) -1_555 . 3_555 N
Si2 SI Al1 0.0 -1_555 . -1_555 N
Si2 SI Al1 103.01(12) -1_555 . -2_555 N
Si2 SI Al1 103.01(12) -1_555 . -3_555 N
Si2 SI O1 26.14(13) -1_555 . 1_555 N
Si2 SI O1 118.66(13) -1_555 . 2_555 N
Si2 SI O1 115.78(16) -1_555 . 3_555 N
Si2 SI O1 153.86(13) -1_555 . -1_555 N
Si2 SI O1 61.34(13) -1_555 . -2_555 N
Si2 SI O1 64.22(16) -1_555 . -3_555 N
Si2 SI O2 30.05(13) -1_555 . 105_544 N
Si2 SI Si2 103.01(12) -2_555 . -3_555 N
Si2 SI Al1 76.99(12) -2_555 . 1_555 N
Si2 SI Al1 180.0 -2_555 . 2_555 N
Si2 SI Al1 76.99(12) -2_555 . 3_555 N
Si2 SI Al1 103.01(12) -2_555 . -1_555 N
Si2 SI Al1 0.0 -2_555 . -2_555 N
Si2 SI Al1 103.01(12) -2_555 . -3_555 N
Si2 SI O1 115.78(16) -2_555 . 1_555 N
Si2 SI O1 26.14(13) -2_555 . 2_555 N
Si2 SI O1 118.66(13) -2_555 . 3_555 N
Si2 SI O1 64.22(16) -2_555 . -1_555 N
Si2 SI O1 153.86(13) -2_555 . -2_555 N
Si2 SI O1 61.34(13) -2_555 . -3_555 N
Si2 SI O2 73.12(13) -2_555 . 105_544 N
Si2 SI Al1 76.99(12) -3_555 . 1_555 N
Si2 SI Al1 76.99(12) -3_555 . 2_555 N
Si2 SI Al1 180.0 -3_555 . 3_555 N
Si2 SI Al1 103.01(12) -3_555 . -1_555 N
Si2 SI Al1 103.01(12) -3_555 . -2_555 N
Si2 SI Al1 0.0 -3_555 . -3_555 N
Si2 SI O1 118.66(13) -3_555 . 1_555 N
Si2 SI O1 115.78(16) -3_555 . 2_555 N
Si2 SI O1 26.14(13) -3_555 . 3_555 N
Si2 SI O1 61.34(13) -3_555 . -1_555 N
Si2 SI O1 64.22(16) -3_555 . -2_555 N
Si2 SI O1 153.86(13) -3_555 . -3_555 N
Si2 SI O2 112.62(11) -3_555 . 105_544 N
Al1 SI Al1 103.01(12) 1_555 . 2_555 N
Al1 SI Al1 103.01(12) 1_555 . 3_555 N
Al1 SI Al1 180.0 1_555 . -1_555 N
Al1 SI Al1 76.99(12) 1_555 . -2_555 N
Al1 SI Al1 76.99(12) 1_555 . -3_555 N
Al1 SI O1 153.86(13) 1_555 . 1_555 N
Al1 SI O1 61.34(13) 1_555 . 2_555 N
Al1 SI O1 64.22(16) 1_555 . 3_555 N
Al1 SI O1 26.14(13) 1_555 . -1_555 N
Al1 SI O1 118.66(13) 1_555 . -2_555 N
Al1 SI O1 115.78(16) 1_555 . -3_555 N
Al1 SI O2 149.95(13) 1_555 . 105_544 N
Al1 SI Al1 103.01(12) 2_555 . 3_555 N
Al1 SI Al1 76.99(12) 2_555 . -1_555 N
Al1 SI Al1 180.0 2_555 . -2_555 N
Al1 SI Al1 76.99(12) 2_555 . -3_555 N
Al1 SI O1 64.22(16) 2_555 . 1_555 N
Al1 SI O1 153.86(13) 2_555 . 2_555 N
Al1 SI O1 61.34(13) 2_555 . 3_555 N
Al1 SI O1 115.78(16) 2_555 . -1_555 N
Al1 SI O1 26.14(13) 2_555 . -2_555 N
Al1 SI O1 118.66(13) 2_555 . -3_555 N
Al1 SI O2 106.88(13) 2_555 . 105_544 N
Al1 SI Al1 76.99(12) 3_555 . -1_555 N
Al1 SI Al1 76.99(12) 3_555 . -2_555 N
Al1 SI Al1 180.0 3_555 . -3_555 N
Al1 SI O1 61.34(13) 3_555 . 1_555 N
Al1 SI O1 64.22(16) 3_555 . 2_555 N
Al1 SI O1 153.86(13) 3_555 . 3_555 N
Al1 SI O1 118.66(13) 3_555 . -1_555 N
Al1 SI O1 115.78(16) 3_555 . -2_555 N
Al1 SI O1 26.14(13) 3_555 . -3_555 N
Al1 SI O2 67.38(11) 3_555 . 105_544 N
Al1 SI Al1 103.01(12) -1_555 . -2_555 N
Al1 SI Al1 103.01(12) -1_555 . -3_555 N
Al1 SI O1 26.14(13) -1_555 . 1_555 N
Al1 SI O1 118.66(13) -1_555 . 2_555 N
Al1 SI O1 115.78(16) -1_555 . 3_555 N
Al1 SI O1 153.86(13) -1_555 . -1_555 N
Al1 SI O1 61.34(13) -1_555 . -2_555 N
Al1 SI O1 64.22(16) -1_555 . -3_555 N
Al1 SI O2 30.05(13) -1_555 . 105_544 N
Al1 SI Al1 103.01(12) -2_555 . -3_555 N
Al1 SI O1 115.78(16) -2_555 . 1_555 N
Al1 SI O1 26.14(13) -2_555 . 2_555 N
Al1 SI O1 118.66(13) -2_555 . 3_555 N
Al1 SI O1 64.22(16) -2_555 . -1_555 N
Al1 SI O1 153.86(13) -2_555 . -2_555 N
Al1 SI O1 61.34(13) -2_555 . -3_555 N
Al1 SI O2 73.12(13) -2_555 . 105_544 N
Al1 SI O1 118.66(13) -3_555 . 1_555 N
Al1 SI O1 115.78(16) -3_555 . 2_555 N
Al1 SI O1 26.14(13) -3_555 . 3_555 N
Al1 SI O1 61.34(13) -3_555 . -1_555 N
Al1 SI O1 64.22(16) -3_555 . -2_555 N
Al1 SI O1 153.86(13) -3_555 . -3_555 N
Al1 SI O2 112.62(11) -3_555 . 105_544 N
O1 SI O1 119.983(4) 1_555 . 2_555 N
O1 SI O1 119.983(4) 1_555 . 3_555 N
O1 SI O1 180.0 1_555 . -1_555 N
O1 SI O1 60.017(4) 1_555 . -2_555 N
O1 SI O1 60.017(4) 1_555 . -3_555 N
O1 SI O2 47.36(14) 1_555 . 105_544 N
O1 SI O1 119.983(4) 2_555 . 3_555 N
O1 SI O1 60.017(4) 2_555 . -1_555 N
O1 SI O1 180.0 2_555 . -2_555 N
O1 SI O1 60.017(4) 2_555 . -3_555 N
O1 SI O2 89.66(12) 2_555 . 105_544 N
O1 SI O1 60.017(4) 3_555 . -1_555 N
O1 SI O1 60.017(4) 3_555 . -2_555 N
O1 SI O1 180.0 3_555 . -3_555 N
O1 SI O2 134.99(14) 3_555 . 105_544 N
O1 SI O1 119.983(4) -1_555 . -2_555 N
O1 SI O1 119.983(4) -1_555 . -3_555 N
O1 SI O2 132.64(14) -1_555 . 105_544 N
O1 SI O1 119.983(4) -2_555 . -3_555 N
O1 SI O2 90.34(12) -2_555 . 105_544 N
O1 SI O2 45.01(14) -3_555 . 105_544 N
Si1 SI' Si1 115.62(13) 1_555 . 2_555 N
Si1 SI' Si1 115.62(13) 1_555 . 3_555 N
Si1 SI' Si2 155.48(32) 1_555 . 1_555 N
Si1 SI' Si2 58.09(13) 1_555 . 2_555 N
Si1 SI' Si2 58.90(12) 1_555 . 3_555 N
Si1 SI' Al1 155.48(32) 1_555 . 1_555 N
Si1 SI' Al1 58.09(13) 1_555 . 2_555 N
Si1 SI' Al1 58.90(12) 1_555 . 3_555 N
Si1 SI' O2 138.19(26) 1_555 . -105_444 N
Si1 SI' O2 26.29(15) 1_555 . -206_444 N
Si1 SI' O2 90.01(16) 1_555 . -304_444 N
Si1 SI' O3 87.08(13) 1_555 . 1_555 N
Si1 SI' O3 32.92(13) 1_555 . 2_555 N
Si1 SI' O3 148.02(20) 1_555 . 3_555 N
Si1 SI' SI 77.75(18) 1_555 . 1_555 N
Si1 SI' OII' 126.5(8) 1_555 . 107_533 N
Si1 SI' OII' 100.08(19) 1_555 . 111_533 N
Si1 SI' OII' 77.9(8) 1_555 . -105_544 N
Si1 SI' DII'1 135.0(16) 1_555 . 107_433 N
Si1 SI' DII'1 117.9(5) 1_555 . 111_433 N
Si1 SI' DII'1 83.2(10) 1_555 . -105_444 N
Si1 SI' DII'1 86.1(15) 1_555 . 208_343 N
Si1 SI' DII'1 69.8(12) 1_555 . 209_343 N
Si1 SI' DII'1 127.2(13) 1_555 . -206_444 N
Si1 SI' Si1 115.62(13) 2_555 . 3_555 N
Si1 SI' Si2 58.90(12) 2_555 . 1_555 N
Si1 SI' Si2 155.48(32) 2_555 . 2_555 N
Si1 SI' Si2 58.09(13) 2_555 . 3_555 N
Si1 SI' Al1 58.90(12) 2_555 . 1_555 N
Si1 SI' Al1 155.48(32) 2_555 . 2_555 N
Si1 SI' Al1 58.09(13) 2_555 . 3_555 N
Si1 SI' O2 90.01(16) 2_555 . -105_444 N
Si1 SI' O2 138.19(26) 2_555 . -206_444 N
Si1 SI' O2 26.29(15) 2_555 . -304_444 N
Si1 SI' O3 148.02(20) 2_555 . 1_555 N
Si1 SI' O3 87.08(13) 2_555 . 2_555 N
Si1 SI' O3 32.92(13) 2_555 . 3_555 N
Si1 SI' SI 77.75(18) 2_555 . 1_555 N
Si1 SI' OII' 77.9(8) 2_555 . 107_533 N
Si1 SI' OII' 126.5(8) 2_555 . 111_533 N
Si1 SI' OII' 100.08(19) 2_555 . -105_544 N
Si1 SI' DII'1 84.1(21) 2_555 . 107_433 N
Si1 SI' DII'1 114.5(10) 2_555 . 111_433 N
Si1 SI' DII'1 94.9(15) 2_555 . -105_444 N
Si1 SI' DII'1 135.0(16) 2_555 . 208_343 N
Si1 SI' DII'1 117.9(5) 2_555 . 209_343 N
Si1 SI' DII'1 83.2(10) 2_555 . -206_444 N
Si1 SI' Si2 58.09(13) 3_555 . 1_555 N
Si1 SI' Si2 58.90(12) 3_555 . 2_555 N
Si1 SI' Si2 155.48(32) 3_555 . 3_555 N
Si1 SI' Al1 58.09(13) 3_555 . 1_555 N
Si1 SI' Al1 58.90(12) 3_555 . 2_555 N
Si1 SI' Al1 155.48(32) 3_555 . 3_555 N
Si1 SI' O2 26.29(15) 3_555 . -105_444 N
Si1 SI' O2 90.01(16) 3_555 . -206_444 N
Si1 SI' O2 138.19(26) 3_555 . -304_444 N
Si1 SI' O3 32.92(13) 3_555 . 1_555 N
Si1 SI' O3 148.02(20) 3_555 . 2_555 N
Si1 SI' O3 87.08(13) 3_555 . 3_555 N
Si1 SI' SI 77.75(18) 3_555 . 1_555 N
Si1 SI' OII' 100.08(19) 3_555 . 107_533 N
Si1 SI' OII' 77.9(8) 3_555 . 111_533 N
Si1 SI' OII' 126.5(8) 3_555 . -105_544 N
Si1 SI' DII'1 86.1(15) 3_555 . 107_433 N
Si1 SI' DII'1 69.8(12) 3_555 . 111_433 N
Si1 SI' DII'1 127.2(13) 3_555 . -105_444 N
Si1 SI' DII'1 84.1(21) 3_555 . 208_343 N
Si1 SI' DII'1 114.5(10) 3_555 . 209_343 N
Si1 SI' DII'1 94.9(15) 3_555 . -206_444 N
Si2 SI' Si2 115.62(12) 1_555 . 2_555 N
Si2 SI' Si2 115.62(12) 1_555 . 3_555 N
Si2 SI' Al1 0.0 1_555 . 1_555 N
Si2 SI' Al1 115.62(12) 1_555 . 2_555 N
Si2 SI' Al1 115.62(12) 1_555 . 3_555 N
Si2 SI' O2 31.81(15) 1_555 . -105_444 N
Si2 SI' O2 142.43(29) 1_555 . -206_444 N
Si2 SI' O2 84.61(17) 1_555 . -304_444 N
Si2 SI' O3 90.90(15) 1_555 . 1_555 N
Si2 SI' O3 144.58(18) 1_555 . 2_555 N
Si2 SI' O3 29.19(13) 1_555 . 3_555 N
Si2 SI' SI 77.74(18) 1_555 . 1_555 N
Si2 SI' OII' 77.4(8) 1_555 . 107_533 N
Si2 SI' OII' 101.27(18) 1_555 . 111_533 N
Si2 SI' OII' 125.8(7) 1_555 . -105_544 N
Si2 SI' DII'1 69.5(16) 1_555 . 107_433 N
Si2 SI' DII'1 83.5(4) 1_555 . 111_433 N
Si2 SI' DII'1 120.1(11) 1_555 . -105_444 N
Si2 SI' DII'1 115.0(17) 1_555 . 208_343 N
Si2 SI' DII'1 134.7(12) 1_555 . 209_343 N
Si2 SI' DII'1 77.2(13) 1_555 . -206_444 N
Si2 SI' Si2 115.62(12) 2_555 . 3_555 N
Si2 SI' Al1 115.62(12) 2_555 . 1_555 N
Si2 SI' Al1 0.0 2_555 . 2_555 N
Si2 SI' Al1 115.62(12) 2_555 . 3_555 N
Si2 SI' O2 84.61(17) 2_555 . -105_444 N
Si2 SI' O2 31.81(15) 2_555 . -206_444 N
Si2 SI' O2 142.43(29) 2_555 . -304_444 N
Si2 SI' O3 29.19(13) 2_555 . 1_555 N
Si2 SI' O3 90.90(15) 2_555 . 2_555 N
Si2 SI' O3 144.58(18) 2_555 . 3_555 N
Si2 SI' SI 77.74(18) 2_555 . 1_555 N
Si2 SI' OII' 125.8(7) 2_555 . 107_533 N
Si2 SI' OII' 77.4(8) 2_555 . 111_533 N
Si2 SI' OII' 101.27(18) 2_555 . -105_544 N
Si2 SI' DII'1 117.6(20) 2_555 . 107_433 N
Si2 SI' DII'1 87.0(12) 2_555 . 111_433 N
Si2 SI' DII'1 107.0(14) 2_555 . -105_444 N
Si2 SI' DII'1 69.5(16) 2_555 . 208_343 N
Si2 SI' DII'1 83.5(4) 2_555 . 209_343 N
Si2 SI' DII'1 120.1(11) 2_555 . -206_444 N
Si2 SI' Al1 115.62(12) 3_555 . 1_555 N
Si2 SI' Al1 115.62(12) 3_555 . 2_555 N
Si2 SI' Al1 0.0 3_555 . 3_555 N
Si2 SI' O2 142.43(29) 3_555 . -105_444 N
Si2 SI' O2 84.61(17) 3_555 . -206_444 N
Si2 SI' O2 31.81(15) 3_555 . -304_444 N
Si2 SI' O3 144.58(18) 3_555 . 1_555 N
Si2 SI' O3 29.19(13) 3_555 . 2_555 N
Si2 SI' O3 90.90(15) 3_555 . 3_555 N
Si2 SI' SI 77.74(18) 3_555 . 1_555 N
Si2 SI' OII' 101.27(18) 3_555 . 107_533 N
Si2 SI' OII' 125.8(7) 3_555 . 111_533 N
Si2 SI' OII' 77.4(8) 3_555 . -105_544 N
Si2 SI' DII'1 115.0(17) 3_555 . 107_433 N
Si2 SI' DII'1 134.7(12) 3_555 . 111_433 N
Si2 SI' DII'1 77.2(13) 3_555 . -105_444 N
Si2 SI' DII'1 117.6(20) 3_555 . 208_343 N
Si2 SI' DII'1 87.0(12) 3_555 . 209_343 N
Si2 SI' DII'1 107.0(14) 3_555 . -206_444 N
Al1 SI' Al1 115.62(12) 1_555 . 2_555 N
Al1 SI' Al1 115.62(12) 1_555 . 3_555 N
Al1 SI' O2 31.81(15) 1_555 . -105_444 N
Al1 SI' O2 142.43(29) 1_555 . -206_444 N
Al1 SI' O2 84.61(17) 1_555 . -304_444 N
Al1 SI' O3 90.90(15) 1_555 . 1_555 N
Al1 SI' O3 144.58(18) 1_555 . 2_555 N
Al1 SI' O3 29.19(13) 1_555 . 3_555 N
Al1 SI' SI 77.74(18) 1_555 . 1_555 N
Al1 SI' OII' 77.4(8) 1_555 . 107_533 N
Al1 SI' OII' 101.27(18) 1_555 . 111_533 N
Al1 SI' OII' 125.8(7) 1_555 . -105_544 N
Al1 SI' DII'1 69.5(16) 1_555 . 107_433 N
Al1 SI' DII'1 83.5(4) 1_555 . 111_433 N
Al1 SI' DII'1 120.1(11) 1_555 . -105_444 N
Al1 SI' DII'1 115.0(17) 1_555 . 208_343 N
Al1 SI' DII'1 134.7(12) 1_555 . 209_343 N
Al1 SI' DII'1 77.2(13) 1_555 . -206_444 N
Al1 SI' Al1 115.62(12) 2_555 . 3_555 N
Al1 SI' O2 84.61(17) 2_555 . -105_444 N
Al1 SI' O2 31.81(15) 2_555 . -206_444 N
Al1 SI' O2 142.43(29) 2_555 . -304_444 N
Al1 SI' O3 29.19(13) 2_555 . 1_555 N
Al1 SI' O3 90.90(15) 2_555 . 2_555 N
Al1 SI' O3 144.58(18) 2_555 . 3_555 N
Al1 SI' SI 77.74(18) 2_555 . 1_555 N
Al1 SI' OII' 125.8(7) 2_555 . 107_533 N
Al1 SI' OII' 77.4(8) 2_555 . 111_533 N
Al1 SI' OII' 101.27(18) 2_555 . -105_544 N
Al1 SI' DII'1 117.6(20) 2_555 . 107_433 N
Al1 SI' DII'1 87.0(12) 2_555 . 111_433 N
Al1 SI' DII'1 107.0(14) 2_555 . -105_444 N
Al1 SI' DII'1 69.5(16) 2_555 . 208_343 N
Al1 SI' DII'1 83.5(4) 2_555 . 209_343 N
Al1 SI' DII'1 120.1(11) 2_555 . -206_444 N
Al1 SI' O2 142.43(29) 3_555 . -105_444 N
Al1 SI' O2 84.61(17) 3_555 . -206_444 N
Al1 SI' O2 31.81(15) 3_555 . -304_444 N
Al1 SI' O3 144.58(18) 3_555 . 1_555 N
Al1 SI' O3 29.19(13) 3_555 . 2_555 N
Al1 SI' O3 90.90(15) 3_555 . 3_555 N
Al1 SI' SI 77.74(18) 3_555 . 1_555 N
Al1 SI' OII' 101.27(18) 3_555 . 107_533 N
Al1 SI' OII' 125.8(7) 3_555 . 111_533 N
Al1 SI' OII' 77.4(8) 3_555 . -105_544 N
Al1 SI' DII'1 115.0(17) 3_555 . 107_433 N
Al1 SI' DII'1 134.7(12) 3_555 . 111_433 N
Al1 SI' DII'1 77.2(13) 3_555 . -105_444 N
Al1 SI' DII'1 117.6(20) 3_555 . 208_343 N
Al1 SI' DII'1 87.0(12) 3_555 . 209_343 N
Al1 SI' DII'1 107.0(14) 3_555 . -206_444 N
O2 SI' O2 114.56(17) -105_444 . -206_444 N
O2 SI' O2 114.56(17) -105_444 . -304_444 N
O2 SI' O3 59.12(15) -105_444 . 1_555 N
O2 SI' O3 162.5(4) -105_444 . 2_555 N
O2 SI' O3 60.82(14) -105_444 . 3_555 N
O2 SI' SI 76.28(23) -105_444 . 1_555 N
O2 SI' OII' 89.4(5) -105_544 . 107_533 N
O2 SI' OII' 88.1(5) -105_544 . 111_533 N
O2 SI' OII' 132.1(9) -105_544 . -105_544 N
O2 SI' DII'1 76.7(14) -105_444 . 107_433 N
O2 SI' DII'1 73.8(9) -105_444 . 111_433 N
O2 SI' DII'1 129.3(11) -105_444 . -105_444 N
O2 SI' DII'1 98.8(20) -105_444 . 208_343 N
O2 SI' DII'1 128.3(13) -105_444 . 209_343 N
O2 SI' DII'1 86.1(15) -105_444 . -206_444 N
O2 SI' O2 114.56(17) -206_444 . -304_444 N
O2 SI' O3 60.82(14) -206_444 . 1_555 N
O2 SI' O3 59.12(15) -206_444 . 2_555 N
O2 SI' O3 162.5(4) -206_444 . 3_555 N
O2 SI' SI 76.28(23) -206_444 . 1_555 N
O2 SI' OII' 132.1(9) -206_544 . 107_533 N
O2 SI' OII' 89.4(5) -206_544 . 111_533 N
O2 SI' OII' 88.1(5) -206_544 . -105_544 N
O2 SI' DII'1 132.6(20) -206_444 . 107_433 N
O2 SI' DII'1 105.0(8) -206_444 . 111_433 N
O2 SI' DII'1 94.3(12) -206_444 . -105_444 N
O2 SI' DII'1 76.7(14) -206_444 . 208_343 N
O2 SI' DII'1 73.8(9) -206_444 . 209_343 N
O2 SI' DII'1 129.3(11) -206_444 . -206_444 N
O2 SI' O3 162.5(4) -304_444 . 1_555 N
O2 SI' O3 60.82(14) -304_444 . 2_555 N
O2 SI' O3 59.12(15) -304_444 . 3_555 N
O2 SI' SI 76.28(23) -304_444 . 1_555 N
O2 SI' OII' 88.1(5) -304_544 . 107_533 N
O2 SI' OII' 132.1(9) -304_544 . 111_533 N
O2 SI' OII' 89.4(5) -304_544 . -105_544 N
O2 SI' DII'1 98.8(20) -304_444 . 107_433 N
O2 SI' DII'1 128.3(13) -304_444 . 111_433 N
O2 SI' DII'1 86.1(15) -304_444 . -105_444 N
O2 SI' DII'1 132.6(20) -304_444 . 208_343 N
O2 SI' DII'1 105.0(8) -304_444 . 209_343 N
O2 SI' DII'1 94.3(12) -304_444 . -206_444 N
O3 SI' O3 119.56(4) 1_555 . 2_555 N
O3 SI' O3 119.56(4) 1_555 . 3_555 N
O3 SI' SI 86.20(17) 1_555 . 1_555 N
O3 SI' OII' 107.5(4) 1_555 . 107_533 N
O3 SI' OII' 65.5(9) 1_555 . 111_533 N
O3 SI' OII' 106.9(4) 1_555 . -105_544 N
O3 SI' DII'1 95.5(19) 1_555 . 107_433 N
O3 SI' DII'1 67.7(13) 1_555 . 111_433 N
O3 SI' DII'1 110.7(15) 1_555 . -105_444 N
O3 SI' DII'1 64.5(19) 1_555 . 208_343 N
O3 SI' DII'1 90.2(6) 1_555 . 209_343 N
O3 SI' DII'1 101.3(13) 1_555 . -206_444 N
O3 SI' O3 119.56(4) 2_555 . 3_555 N
O3 SI' SI 86.20(17) 2_555 . 1_555 N
O3 SI' OII' 106.9(4) 2_555 . 107_533 N
O3 SI' OII' 107.5(4) 2_555 . 111_533 N
O3 SI' OII' 65.5(9) 2_555 . -105_544 N
O3 SI' DII'1 120.1(14) 2_555 . 107_433 N
O3 SI' DII'1 123.0(8) 2_555 . 111_433 N
O3 SI' DII'1 68.3(11) 2_555 . -105_444 N
O3 SI' DII'1 95.5(19) 2_555 . 208_343 N
O3 SI' DII'1 67.7(13) 2_555 . 209_343 N
O3 SI' DII'1 110.7(15) 2_555 . -206_444 N
O3 SI' SI 86.20(17) 3_555 . 1_555 N
O3 SI' OII' 65.5(9) 3_555 . 107_533 N
O3 SI' OII' 106.9(4) 3_555 . 111_533 N
O3 SI' OII' 107.5(4) 3_555 . -105_544 N
O3 SI' DII'1 64.5(19) 3_555 . 107_433 N
O3 SI' DII'1 90.2(6) 3_555 . 111_433 N
O3 SI' DII'1 101.3(13) 3_555 . -105_444 N
O3 SI' DII'1 120.1(14) 3_555 . 208_343 N
O3 SI' DII'1 123.0(8) 3_555 . 209_343 N
O3 SI' DII'1 68.3(11) 3_555 . -206_444 N
SI SI' OII' 151.7(9) 1_555 . 107_533 N
SI SI' OII' 151.7(9) 1_555 . 111_533 N
SI SI' OII' 151.7(9) 1_555 . -105_544 N
SI SI' DII'1 147.3(16) 1_555 . 107_433 N
SI SI' DII'1 147.5(12) 1_555 . 111_433 N
SI SI' DII'1 153.9(12) 1_555 . -105_444 N
SI SI' DII'1 147.3(16) 1_555 . 208_343 N
SI SI' DII'1 147.5(12) 1_555 . 209_343 N
SI SI' DII'1 153.9(12) 1_555 . -206_444 N
OII' SI' OII' 48.6(15) 107_533 . 111_533 N
OII' SI' OII' 48.6(15) 107_533 . -105_544 N
OII' SI' DII'1 14.0(15) 107_433 . 107_433 N
OII' SI' DII'1 40.2(15) 107_433 . 111_433 N
OII' SI' DII'1 43.3(13) 107_433 . -105_444 N
OII' SI' DII'1 58.2(18) 107_433 . 208_343 N
OII' SI' DII'1 59.2(14) 107_433 . 209_343 N
OII' SI' DII'1 6.2(13) 107_433 . -206_444 N
OII' SI' OII' 48.6(15) 111_533 . -105_544 N
OII' SI' DII'1 43.6(22) 111_433 . 107_433 N
OII' SI' DII'1 17.9(4) 111_433 . 111_433 N
OII' SI' DII'1 49.6(17) 111_433 . -105_444 N
OII' SI' DII'1 14.0(15) 111_433 . 208_343 N
OII' SI' DII'1 40.2(15) 111_433 . 209_343 N
OII' SI' DII'1 43.3(13) 111_433 . -206_444 N
OII' SI' DII'1 58.2(18) -105_444 . 107_433 N
OII' SI' DII'1 59.2(14) -105_444 . 111_433 N
OII' SI' DII'1 6.2(13) -105_444 . -105_444 N
OII' SI' DII'1 43.6(22) -105_444 . 208_343 N
OII' SI' DII'1 17.9(4) -105_444 . 209_343 N
OII' SI' DII'1 49.6(17) -105_444 . -206_444 N
DII'1 SI' DII'1 30.7(30) 107_433 . 111_433 N
DII'1 SI' DII'1 53.8(24) 107_433 . -105_444 N
DII'1 SI' DII'1 55.9(27) 107_433 . 208_343 N
DII'1 SI' DII'1 65.2(28) 107_433 . 209_343 N
DII'1 SI' DII'1 9.4(26) 107_433 . -206_444 N
DII'1 SI' DII'1 58.2(21) 111_433 . -105_444 N
DII'1 SI' DII'1 31.9(19) 111_433 . 208_343 N
DII'1 SI' DII'1 55.5(19) 111_433 . 209_343 N
DII'1 SI' DII'1 34.1(21) 111_433 . -206_444 N
DII'1 SI' DII'1 46.5(33) -105_444 . 208_343 N
DII'1 SI' DII'1 23.5(10) -105_444 . 209_343 N
DII'1 SI' DII'1 44.8(20) -105_444 . -206_444 N
DII'1 SI' DII'1 30.7(30) 208_343 . 209_343 N
DII'1 SI' DII'1 53.8(24) 208_343 . -206_444 N
DII'1 SI' DII'1 58.2(21) 209_343 . -206_444 N
Si1 SII Si1 114.10(13) 107_434 . 208_344 N
Si1 SII Si1 114.10(13) 107_434 . 312_335 N
Si1 SII Si2 153.55(30) 107_533 . 111_533 N
Si1 SII Si2 58.45(12) 107_533 . 209_443 N
Si1 SII Si2 58.13(13) 107_533 . 310_434 N
Si1 SII Al1 153.55(30) 107_443 . 111_443 N
Si1 SII Al1 58.45(12) 107_443 . 209_353 N
Si1 SII Al1 58.13(13) 107_443 . 310_344 N
Si1 SII O3 84.54(17) 107_433 . -105_444 N
Si1 SII O3 30.25(15) 107_433 . -206_444 N
Si1 SII O3 137.51(28) 107_433 . -304_444 N
Si1 SII O4 28.53(12) 107_433 . 1_555 N
Si1 SII O4 91.28(13) 107_433 . 2_555 N
Si1 SII O4 142.34(19) 107_433 . 3_555 N
Si1 SII Dd2 96.0(19) 107_533 . 107_533 N
Si1 SII Dd2 149.8(19) 107_533 . 208_443 N
Si1 SII Dd2 46.4(16) 107_533 . 312_434 N
Si1 SII OII' 75.68(16) 107_533 . 1_555 N
Si1 SII DII'1 66.0(15) 107_433 . 1_555 N
Si1 SII DII'1 69.7(18) 107_433 . 2_555 N
Si1 SII DII'1 92.5(6) 107_433 . 3_555 N
Si1 SII OII* 104.32(16) 107_433 . 1_555 N
Si1 SII DII*1 96(4) 107_432 . 1_555 N
Si1 SII DII*1 91.0(29) 107_432 . 2_555 N
Si1 SII Si1 114.10(13) 208_344 . 312_335 N
Si1 SII Si2 58.13(13) 208_443 . 111_533 N
Si1 SII Si2 153.55(30) 208_443 . 209_443 N
Si1 SII Si2 58.45(12) 208_443 . 310_434 N
Si1 SII Al1 58.13(13) 208_353 . 111_443 N
Si1 SII Al1 153.55(30) 208_353 . 209_353 N
Si1 SII Al1 58.45(12) 208_353 . 310_344 N
Si1 SII O3 137.51(28) 208_343 . -105_444 N
Si1 SII O3 84.54(17) 208_343 . -206_444 N
Si1 SII O3 30.25(15) 208_343 . -304_444 N
Si1 SII O4 142.34(19) 208_343 . 1_555 N
Si1 SII O4 28.53(12) 208_343 . 2_555 N
Si1 SII O4 91.28(13) 208_343 . 3_555 N
Si1 SII Dd2 46.4(16) 208_443 . 107_533 N
Si1 SII Dd2 96.0(19) 208_443 . 208_443 N
Si1 SII Dd2 149.8(19) 208_443 . 312_434 N
Si1 SII OII' 75.68(16) 208_443 . 1_555 N
Si1 SII DII'1 92.5(6) 208_343 . 1_555 N
Si1 SII DII'1 66.0(15) 208_343 . 2_555 N
Si1 SII DII'1 69.7(18) 208_343 . 3_555 N
Si1 SII OII* 104.32(16) 208_343 . 1_555 N
Si1 SII DII*1 124.5(11) 208_342 . 1_555 N
Si1 SII DII*1 96(4) 208_342 . 2_555 N
Si1 SII Si2 58.45(12) 312_434 . 111_533 N
Si1 SII Si2 58.13(13) 312_434 . 209_443 N
Si1 SII Si2 153.55(30) 312_434 . 310_434 N
Si1 SII Al1 58.45(12) 312_344 . 111_443 N
Si1 SII Al1 58.13(13) 312_344 . 209_353 N
Si1 SII Al1 153.55(30) 312_344 . 310_344 N
Si1 SII O3 30.25(15) 312_334 . -105_444 N
Si1 SII O3 137.51(28) 312_334 . -206_444 N
Si1 SII O3 84.54(17) 312_334 . -304_444 N
Si1 SII O4 91.28(13) 312_334 . 1_555 N
Si1 SII O4 142.34(19) 312_334 . 2_555 N
Si1 SII O4 28.53(12) 312_334 . 3_555 N
Si1 SII Dd2 149.8(19) 312_434 . 107_533 N
Si1 SII Dd2 46.4(16) 312_434 . 208_443 N
Si1 SII Dd2 96.0(19) 312_434 . 312_434 N
Si1 SII OII' 75.68(16) 312_434 . 1_555 N
Si1 SII DII'1 69.7(18) 312_334 . 1_555 N
Si1 SII DII'1 92.5(6) 312_334 . 2_555 N
Si1 SII DII'1 66.0(15) 312_334 . 3_555 N
Si1 SII OII* 104.32(16) 312_334 . 1_555 N
Si1 SII DII*1 91.0(29) 312_333 . 1_555 N
Si1 SII DII*1 124.5(11) 312_333 . 2_555 N
Si2 SII Si2 115.70(12) 111_533 . 209_443 N
Si2 SII Si2 115.70(12) 111_533 . 310_434 N
Si2 SII Al1 0.0 111_443 . 111_443 N
Si2 SII Al1 115.70(12) 111_443 . 209_353 N
Si2 SII Al1 115.70(12) 111_443 . 310_344 N
Si2 SII O3 87.79(17) 111_433 . -105_444 N
Si2 SII O3 137.13(27) 111_433 . -206_444 N
Si2 SII O3 28.04(16) 111_433 . -304_444 N
Si2 SII O4 147.97(20) 111_433 . 1_555 N
Si2 SII O4 86.25(14) 111_433 . 2_555 N
Si2 SII O4 33.15(13) 111_433 . 3_555 N
Si2 SII Dd2 93.7(19) 111_533 . 107_533 N
Si2 SII Dd2 45.7(16) 111_533 . 208_443 N
Si2 SII Dd2 150.5(19) 111_533 . 312_434 N
Si2 SII OII' 77.87(18) 111_533 . 1_555 N
Si2 SII DII'1 88.3(14) 111_433 . 1_555 N
Si2 SII DII'1 84.8(17) 111_433 . 2_555 N
Si2 SII DII'1 61.1(6) 111_433 . 3_555 N
Si2 SII OII* 102.13(18) 111_433 . 1_555 N
Si2 SII DII*1 109(4) 111_432 . 1_555 N
Si2 SII DII*1 114.3(32) 111_432 . 2_555 N
Si2 SII Si2 115.70(12) 209_443 . 310_434 N
Si2 SII Al1 115.70(12) 209_353 . 111_443 N
Si2 SII Al1 0.0 209_353 . 209_353 N
Si2 SII Al1 115.70(12) 209_353 . 310_344 N
Si2 SII O3 28.04(16) 209_343 . -105_444 N
Si2 SII O3 87.79(17) 209_343 . -206_444 N
Si2 SII O3 137.13(27) 209_343 . -304_444 N
Si2 SII O4 33.15(13) 209_343 . 1_555 N
Si2 SII O4 147.97(20) 209_343 . 2_555 N
Si2 SII O4 86.25(14) 209_343 . 3_555 N
Si2 SII Dd2 150.5(19) 209_443 . 107_533 N
Si2 SII Dd2 93.7(19) 209_443 . 208_443 N
Si2 SII Dd2 45.7(16) 209_443 . 312_434 N
Si2 SII OII' 77.87(18) 209_443 . 1_555 N
Si2 SII DII'1 61.1(6) 209_343 . 1_555 N
Si2 SII DII'1 88.3(14) 209_343 . 2_555 N
Si2 SII DII'1 84.8(17) 209_343 . 3_555 N
Si2 SII OII* 102.13(18) 209_343 . 1_555 N
Si2 SII DII*1 81.9(10) 209_342 . 1_555 N
Si2 SII DII*1 109(4) 209_342 . 2_555 N
Si2 SII Al1 115.70(12) 310_344 . 111_443 N
Si2 SII Al1 115.70(12) 310_344 . 209_353 N
Si2 SII Al1 0.0 310_344 . 310_344 N
Si2 SII O3 137.13(27) 310_334 . -105_444 N
Si2 SII O3 28.04(16) 310_334 . -206_444 N
Si2 SII O3 87.79(17) 310_334 . -304_444 N
Si2 SII O4 86.25(14) 310_334 . 1_555 N
Si2 SII O4 33.15(13) 310_334 . 2_555 N
Si2 SII O4 147.97(20) 310_334 . 3_555 N
Si2 SII Dd2 45.7(16) 310_434 . 107_533 N
Si2 SII Dd2 150.5(19) 310_434 . 208_443 N
Si2 SII Dd2 93.7(19) 310_434 . 312_434 N
Si2 SII OII' 77.87(18) 310_434 . 1_555 N
Si2 SII DII'1 84.8(17) 310_334 . 1_555 N
Si2 SII DII'1 61.1(6) 310_334 . 2_555 N
Si2 SII DII'1 88.3(14) 310_334 . 3_555 N
Si2 SII OII* 102.13(18) 310_334 . 1_555 N
Si2 SII DII*1 114.3(32) 310_333 . 1_555 N
Si2 SII DII*1 81.9(10) 310_333 . 2_555 N
Al1 SII Al1 115.70(12) 111_443 . 209_353 N
Al1 SII Al1 115.70(12) 111_443 . 310_344 N
Al1 SII O3 87.79(17) 111_433 . -105_444 N
Al1 SII O3 137.13(27) 111_433 . -206_444 N
Al1 SII O3 28.04(16) 111_433 . -304_444 N
Al1 SII O4 147.97(20) 111_433 . 1_555 N
Al1 SII O4 86.25(14) 111_433 . 2_555 N
Al1 SII O4 33.15(13) 111_433 . 3_555 N
Al1 SII Dd2 93.7(19) 111_533 . 107_533 N
Al1 SII Dd2 45.7(16) 111_533 . 208_443 N
Al1 SII Dd2 150.5(19) 111_533 . 312_434 N
Al1 SII OII' 77.87(18) 111_533 . 1_555 N
Al1 SII DII'1 88.3(14) 111_433 . 1_555 N
Al1 SII DII'1 84.8(17) 111_433 . 2_555 N
Al1 SII DII'1 61.1(6) 111_433 . 3_555 N
Al1 SII OII* 102.13(18) 111_433 . 1_555 N
Al1 SII DII*1 109(4) 111_432 . 1_555 N
Al1 SII DII*1 114.3(32) 111_432 . 2_555 N
Al1 SII Al1 115.70(12) 209_353 . 310_344 N
Al1 SII O3 28.04(16) 209_343 . -105_444 N
Al1 SII O3 87.79(17) 209_343 . -206_444 N
Al1 SII O3 137.13(27) 209_343 . -304_444 N
Al1 SII O4 33.15(13) 209_343 . 1_555 N
Al1 SII O4 147.97(20) 209_343 . 2_555 N
Al1 SII O4 86.25(14) 209_343 . 3_555 N
Al1 SII Dd2 150.5(19) 209_443 . 107_533 N
Al1 SII Dd2 93.7(19) 209_443 . 208_443 N
Al1 SII Dd2 45.7(16) 209_443 . 312_434 N
Al1 SII OII' 77.87(18) 209_443 . 1_555 N
Al1 SII DII'1 61.1(6) 209_343 . 1_555 N
Al1 SII DII'1 88.3(14) 209_343 . 2_555 N
Al1 SII DII'1 84.8(17) 209_343 . 3_555 N
Al1 SII OII* 102.13(18) 209_343 . 1_555 N
Al1 SII DII*1 81.9(10) 209_342 . 1_555 N
Al1 SII DII*1 109(4) 209_342 . 2_555 N
Al1 SII O3 137.13(27) 310_334 . -105_444 N
Al1 SII O3 28.04(16) 310_334 . -206_444 N
Al1 SII O3 87.79(17) 310_334 . -304_444 N
Al1 SII O4 86.25(14) 310_334 . 1_555 N
Al1 SII O4 33.15(13) 310_334 . 2_555 N
Al1 SII O4 147.97(20) 310_334 . 3_555 N
Al1 SII Dd2 45.7(16) 310_434 . 107_533 N
Al1 SII Dd2 150.5(19) 310_434 . 208_443 N
Al1 SII Dd2 93.7(19) 310_434 . 312_434 N
Al1 SII OII' 77.87(18) 310_434 . 1_555 N
Al1 SII DII'1 84.8(17) 310_334 . 1_555 N
Al1 SII DII'1 61.1(6) 310_334 . 2_555 N
Al1 SII DII'1 88.3(14) 310_334 . 3_555 N
Al1 SII OII* 102.13(18) 310_334 . 1_555 N
Al1 SII DII*1 114.3(32) 310_333 . 1_555 N
Al1 SII DII*1 81.9(10) 310_333 . 2_555 N
O3 SII O3 111.48(20) -105_444 . -206_444 N
O3 SII O3 111.48(20) -105_444 . -304_444 N
O3 SII O4 61.14(14) -105_444 . 1_555 N
O3 SII O4 157.6(4) -105_444 . 2_555 N
O3 SII O4 58.69(14) -105_444 . 3_555 N
O3 SII Dd2 175.3(15) -105_544 . 107_533 N
O3 SII Dd2 71.2(18) -105_544 . 208_443 N
O3 SII Dd2 70.3(18) -105_544 . 312_434 N
O3 SII OII' 72.62(21) -105_544 . 1_555 N
O3 SII DII'1 59.2(13) -105_444 . 1_555 N
O3 SII DII'1 88.1(8) -105_444 . 2_555 N
O3 SII DII'1 71.8(18) -105_444 . 3_555 N
O3 SII OII* 107.38(21) -105_444 . 1_555 N
O3 SII DII*1 88.0(14) -105_443 . 1_555 N
O3 SII DII*1 122.3(29) -105_443 . 2_555 N
O3 SII O3 111.48(20) -206_444 . -304_444 N
O3 SII O4 58.69(14) -206_444 . 1_555 N
O3 SII O4 61.14(14) -206_444 . 2_555 N
O3 SII O4 157.6(4) -206_444 . 3_555 N
O3 SII Dd2 70.3(18) -206_544 . 107_533 N
O3 SII Dd2 175.3(15) -206_544 . 208_443 N
O3 SII Dd2 71.2(18) -206_544 . 312_434 N
O3 SII OII' 72.62(21) -206_544 . 1_555 N
O3 SII DII'1 71.8(18) -206_444 . 1_555 N
O3 SII DII'1 59.2(13) -206_444 . 2_555 N
O3 SII DII'1 88.1(8) -206_444 . 3_555 N
O3 SII OII* 107.38(21) -206_444 . 1_555 N
O3 SII DII*1 110(4) -206_443 . 1_555 N
O3 SII DII*1 88.0(14) -206_443 . 2_555 N
O3 SII O4 157.6(4) -304_444 . 1_555 N
O3 SII O4 58.69(14) -304_444 . 2_555 N
O3 SII O4 61.14(14) -304_444 . 3_555 N
O3 SII Dd2 71.2(18) -304_544 . 107_533 N
O3 SII Dd2 70.3(18) -304_544 . 208_443 N
O3 SII Dd2 175.3(15) -304_544 . 312_434 N
O3 SII OII' 72.62(21) -304_544 . 1_555 N
O3 SII DII'1 88.1(8) -304_444 . 1_555 N
O3 SII DII'1 71.8(18) -304_444 . 2_555 N
O3 SII DII'1 59.2(13) -304_444 . 3_555 N
O3 SII OII* 107.38(21) -304_444 . 1_555 N
O3 SII DII*1 122.3(29) -304_443 . 1_555 N
O3 SII DII*1 110(4) -304_443 . 2_555 N
O4 SII O4 119.25(5) 1_555 . 2_555 N
O4 SII O4 119.25(5) 1_555 . 3_555 N
O4 SII Dd2 117.9(19) 1_555 . 107_533 N
O4 SII Dd2 121.3(19) 1_555 . 208_443 N
O4 SII Dd2 27.1(14) 1_555 . 312_434 N
O4 SII OII' 85.01(18) 1_555 . 1_555 N
O4 SII DII'1 69.8(9) 1_555 . 1_555 N
O4 SII DII'1 86.5(18) 1_555 . 2_555 N
O4 SII DII'1 99.0(12) 1_555 . 3_555 N
O4 SII OII* 94.99(18) 1_555 . 1_555 N
O4 SII DII*1 79.7(27) 1_555 . 1_555 N
O4 SII DII*1 91(4) 1_555 . 2_555 N
O4 SII O4 119.25(5) 2_555 . 3_555 N
O4 SII Dd2 27.1(14) 2_555 . 107_533 N
O4 SII Dd2 117.9(19) 2_555 . 208_443 N
O4 SII Dd2 121.3(19) 2_555 . 312_434 N
O4 SII OII' 85.01(18) 2_555 . 1_555 N
O4 SII DII'1 99.0(12) 2_555 . 1_555 N
O4 SII DII'1 69.8(9) 2_555 . 2_555 N
O4 SII DII'1 86.5(18) 2_555 . 3_555 N
O4 SII OII* 94.99(18) 2_555 . 1_555 N
O4 SII DII*1 114.4(15) 2_555 . 1_555 N
O4 SII DII*1 79.7(27) 2_555 . 2_555 N
O4 SII Dd2 121.3(19) 3_555 . 107_533 N
O4 SII Dd2 27.1(14) 3_555 . 208_443 N
O4 SII Dd2 117.9(19) 3_555 . 312_434 N
O4 SII OII' 85.01(18) 3_555 . 1_555 N
O4 SII DII'1 86.5(18) 3_555 . 1_555 N
O4 SII DII'1 99.0(12) 3_555 . 2_555 N
O4 SII DII'1 69.8(9) 3_555 . 3_555 N
O4 SII OII* 94.99(18) 3_555 . 1_555 N
O4 SII DII*1 91(4) 3_555 . 1_555 N
O4 SII DII*1 114.4(15) 3_555 . 2_555 N
Dd2 SII Dd2 106.7(15) 107_533 . 208_443 N
Dd2 SII Dd2 106.7(15) 107_533 . 312_434 N
Dd2 SII OII' 112.1(14) 107_533 . 1_555 N
Dd2 SII DII'1 125.3(20) 107_433 . 1_555 N
Dd2 SII DII'1 96.5(16) 107_433 . 2_555 N
Dd2 SII DII'1 112.9(23) 107_433 . 3_555 N
Dd2 SII OII* 67.9(14) 107_433 . 1_555 N
Dd2 SII DII*1 87.3(20) 107_432 . 1_555 N
Dd2 SII DII*1 53.0(33) 107_432 . 2_555 N
Dd2 SII Dd2 106.7(15) 208_443 . 312_434 N
Dd2 SII OII' 112.1(14) 208_443 . 1_555 N
Dd2 SII DII'1 112.9(23) 208_343 . 1_555 N
Dd2 SII DII'1 125.3(20) 208_343 . 2_555 N
Dd2 SII DII'1 96.5(16) 208_343 . 3_555 N
Dd2 SII OII* 67.9(14) 208_343 . 1_555 N
Dd2 SII DII*1 66(4) 208_342 . 1_555 N
Dd2 SII DII*1 87.3(20) 208_342 . 2_555 N
Dd2 SII OII' 112.1(14) 312_434 . 1_555 N
Dd2 SII DII'1 96.5(16) 312_334 . 1_555 N
Dd2 SII DII'1 112.9(23) 312_334 . 2_555 N
Dd2 SII DII'1 125.3(20) 312_334 . 3_555 N
Dd2 SII OII* 67.9(14) 312_334 . 1_555 N
Dd2 SII DII*1 53.0(33) 312_333 . 1_555 N
Dd2 SII DII*1 66(4) 312_333 . 2_555 N
OII' SII DII'1 16.9(5) 1_555 . 1_555 N
OII' SII DII'1 16.9(5) 1_555 . 2_555 N
OII' SII DII'1 16.9(5) 1_555 . 3_555 N
OII' SII OII* 180.0 1_555 . 1_555 N
OII' SII DII*1 159.5(7) 1_555 . 1_555 N
OII' SII DII*1 159.5(7) 1_555 . 2_555 N
DII'1 SII DII'1 29.2(8) 1_555 . 2_555 N
DII'1 SII DII'1 29.2(8) 1_555 . 3_555 N
DII'1 SII OII* 163.1(5) 1_555 . 1_555 N
DII'1 SII DII*1 142.9(11) 1_555 . 1_555 N
DII'1 SII DII*1 157.0(32) 1_555 . 2_555 N
DII'1 SII DII'1 29.2(8) 2_555 . 3_555 N
DII'1 SII OII* 163.1(5) 2_555 . 1_555 N
DII'1 SII DII*1 166(4) 2_555 . 1_555 N
DII'1 SII DII*1 142.9(11) 2_555 . 2_555 N
DII'1 SII OII* 163.1(5) 3_555 . 1_555 N
DII'1 SII DII*1 157.0(32) 3_555 . 1_555 N
DII'1 SII DII*1 166(4) 3_555 . 2_555 N
OII* SII DII*1 20.5(7) 1_555 . 1_555 N
OII* SII DII*1 20.5(7) 1_555 . 2_555 N
DII*1 SII DII*1 35.3(12) 1_555 . 2_555 N
Si1 SJ Si2 66.7(6) 111_533 . 3_555 N
Si1 SJ Al1 66.7(6) 111_443 . 3_555 N
Si1 SJ O1 100.8(9) 111_433 . -3_555 N
Si1 SJ O1 30.82(35) 111_433 . 111_433 N
Si1 SJ O3 68.4(6) 111_433 . 2_555 N
Si1 SJ O4 26.4(5) 111_433 . 312_334 N
Si1 SJ SJ 159.4(13) 111_545 . 105_544 N
Si1 SJ SJ 79.2(11) 111_545 . -108_656 N
Si1 SJ Oc 168.6(16) 111_545 . 1_555 N
Si1 SJ Oc 89.4(12) 111_545 . -108_656 N
Si1 SJ Dc1 153.4(19) 111_554 . 1_555 N
Si1 SJ Dc1 171.4(11) 111_554 . 105_544 N
Si1 SJ Dc1 101.8(11) 111_554 . -108_665 N
Si1 SJ Dc2 139.8(17) 111_555 . 1_555 N
Si1 SJ Dc2 64.9(9) 111_555 . -108_666 N
Si1 SJ Od 116(8) 111_554 . 1_555 N
Si1 SJ Od 160.6(14) 111_554 . 105_544 N
Si1 SJ Od 86.9(12) 111_554 . -108_665 N
Si1 SJ Dd1 121(4) 111_533 . 1_555 N
Si1 SJ Dd1 152.6(16) 111_533 . 105_544 N
Si1 SJ Dd1 95.4(16) 111_533 . -108_644 N
Si1 SJ Dd2 46(7) 111_533 . 1_555 N
Si1 SJ Dd2 146.6(15) 111_533 . 105_544 N
Si1 SJ Dd2 76.5(14) 111_533 . -108_644 N
Si2 SJ Al1 0.0 3_555 . 3_555 N
Si2 SJ O1 36.3(4) 3_555 . -3_555 N
Si2 SJ O1 97.2(9) 3_555 . 111_433 N
Si2 SJ O3 22.27(28) 3_555 . 2_555 N
Si2 SJ O4 40.6(6) 3_555 . 312_334 N
Si2 SJ SJ 95.5(12) 3_555 . 105_544 N
Si2 SJ SJ 145.2(12) 3_555 . -108_656 N
Si2 SJ Oc 104.6(15) 3_555 . 1_555 N
Si2 SJ Oc 148.7(15) 3_555 . -108_656 N
Si2 SJ Dc1 139.5(20) 3_555 . 1_555 N
Si2 SJ Dc1 119.6(12) 3_555 . 105_544 N
Si2 SJ Dc1 167.2(14) 3_555 . -108_665 N
Si2 SJ Dc2 75.7(13) 3_555 . 1_555 N
Si2 SJ Dc2 131.2(15) 3_555 . -108_666 N
Si2 SJ Od 144(7) 3_555 . 1_555 N
Si2 SJ Od 101.4(14) 3_555 . 105_544 N
Si2 SJ Od 151.4(14) 3_555 . -108_665 N
Si2 SJ Dd1 123(4) 3_555 . 1_555 N
Si2 SJ Dd1 111.2(16) 3_555 . 105_544 N
Si2 SJ Dd1 149.5(19) 3_555 . -108_644 N
Si2 SJ Dd2 67(7) 3_555 . 1_555 N
Si2 SJ Dd2 87.2(14) 3_555 . 105_544 N
Si2 SJ Dd2 140.3(16) 3_555 . -108_644 N
Al1 SJ O1 36.3(4) 3_555 . -3_555 N
Al1 SJ O1 97.2(9) 3_555 . 111_433 N
Al1 SJ O3 22.27(28) 3_555 . 2_555 N
Al1 SJ O4 40.6(6) 3_555 . 312_334 N
Al1 SJ SJ 95.5(12) 3_555 . 105_544 N
Al1 SJ SJ 145.2(12) 3_555 . -108_656 N
Al1 SJ Oc 104.6(15) 3_555 . 1_555 N
Al1 SJ Oc 148.7(15) 3_555 . -108_656 N
Al1 SJ Dc1 139.5(20) 3_555 . 1_555 N
Al1 SJ Dc1 119.6(12) 3_555 . 105_544 N
Al1 SJ Dc1 167.2(14) 3_555 . -108_665 N
Al1 SJ Dc2 75.7(13) 3_555 . 1_555 N
Al1 SJ Dc2 131.2(15) 3_555 . -108_666 N
Al1 SJ Od 144(7) 3_555 . 1_555 N
Al1 SJ Od 101.4(14) 3_555 . 105_544 N
Al1 SJ Od 151.4(14) 3_555 . -108_665 N
Al1 SJ Dd1 123(4) 3_555 . 1_555 N
Al1 SJ Dd1 111.2(16) 3_555 . 105_544 N
Al1 SJ Dd1 149.5(19) 3_555 . -108_644 N
Al1 SJ Dd2 67(7) 3_555 . 1_555 N
Al1 SJ Dd2 87.2(14) 3_555 . 105_544 N
Al1 SJ Dd2 140.3(16) 3_555 . -108_644 N
O1 SJ O1 128.9(11) -3_555 . 111_433 N
O1 SJ O3 48.4(5) -3_555 . 2_555 N
O1 SJ O4 76.0(9) -3_555 . 312_334 N
O1 SJ SJ 59.9(11) -3_555 . 105_544 N
O1 SJ SJ 160.4(16) -3_555 . -108_656 N
O1 SJ Oc 72.7(13) -3_555 . 1_555 N
O1 SJ Oc 145.3(16) -3_555 . -108_656 N
O1 SJ Dc1 104.1(18) -3_555 . 1_555 N
O1 SJ Dc1 84.3(10) -3_555 . 105_544 N
O1 SJ Dc1 150.9(14) -3_555 . -108_665 N
O1 SJ Dc2 39.8(10) -3_555 . 1_555 N
O1 SJ Dc2 156.8(16) -3_555 . -108_666 N
O1 SJ Od 135(8) -3_555 . 1_555 N
O1 SJ Od 65.3(12) -3_555 . 105_544 N
O1 SJ Od 155.0(14) -3_555 . -108_665 N
O1 SJ Dd1 115(4) -3_555 . 1_555 N
O1 SJ Dd1 75.3(14) -3_555 . 105_544 N
O1 SJ Dd1 138.6(15) -3_555 . -108_644 N
O1 SJ Dd2 99(7) -3_555 . 1_555 N
O1 SJ Dd2 50.9(12) -3_555 . 105_544 N
O1 SJ Dd2 152.8(16) -3_555 . -108_644 N
O1 SJ O3 98.3(8) 111_433 . 2_555 N
O1 SJ O4 57.2(8) 111_433 . 312_334 N
O1 SJ SJ 160.1(13) 111_545 . 105_544 N
O1 SJ SJ 48.4(9) 111_545 . -108_656 N
O1 SJ Oc 158.0(16) 111_545 . 1_555 N
O1 SJ Oc 59.3(9) 111_545 . -108_656 N
O1 SJ Dc1 122.6(17) 111_554 . 1_555 N
O1 SJ Dc1 141.6(10) 111_554 . 105_544 N
O1 SJ Dc1 71.0(9) 111_554 . -108_665 N
O1 SJ Dc2 159.8(19) 111_555 . 1_555 N
O1 SJ Dc2 34.1(7) 111_555 . -108_666 N
O1 SJ Od 94(8) 111_554 . 1_555 N
O1 SJ Od 152.2(13) 111_554 . 105_544 N
O1 SJ Od 56.1(11) 111_554 . -108_665 N
O1 SJ Dd1 109(4) 111_533 . 1_555 N
O1 SJ Dd1 136.0(13) 111_533 . 105_544 N
O1 SJ Dd1 65.9(14) 111_533 . -108_644 N
O1 SJ Dd2 62(8) 111_533 . 1_555 N
O1 SJ Dd2 153.7(16) 111_533 . 105_544 N
O1 SJ Dd2 45.9(13) 111_533 . -108_644 N
O3 SJ O4 43.5(6) 2_555 . 312_334 N
O3 SJ SJ 99.3(10) 2_555 . 105_544 N
O3 SJ SJ 143.7(12) 2_555 . -108_656 N
O3 SJ Oc 100.7(13) 2_555 . 1_555 N
O3 SJ Oc 157.5(15) 2_555 . -108_656 N
O3 SJ Dc1 136.9(18) 2_555 . 1_555 N
O3 SJ Dc1 119.8(10) 2_555 . 105_544 N
O3 SJ Dc1 160.1(13) 2_555 . -108_665 N
O3 SJ Dc2 82.3(13) 2_555 . 1_555 N
O3 SJ Dc2 130.4(13) 2_555 . -108_666 N
O3 SJ Od 122(7) 2_555 . 1_555 N
O3 SJ Od 106.8(13) 2_555 . 105_544 N
O3 SJ Od 152.4(14) 2_555 . -108_665 N
O3 SJ Dd1 102(4) 2_555 . 1_555 N
O3 SJ Dd1 120.7(14) 2_555 . 105_544 N
O3 SJ Dd1 163.7(18) 2_555 . -108_644 N
O3 SJ Dd2 50(7) 2_555 . 1_555 N
O3 SJ Dd2 95.4(14) 2_555 . 105_544 N
O3 SJ Dd2 143.8(15) 2_555 . -108_644 N
O4 SJ SJ 135.9(15) 312_446 . 105_544 N
O4 SJ SJ 105.6(15) 312_446 . -108_656 N
O4 SJ Oc 143.7(19) 312_446 . 1_555 N
O4 SJ Oc 115.0(16) 312_446 . -108_656 N
O4 SJ Dc1 179.548(18) 312_455 . 1_555 N
O4 SJ Dc1 160.2(15) 312_455 . 105_544 N
O4 SJ Dc1 128.1(16) 312_455 . -108_665 N
O4 SJ Dc2 115.8(18) 312_456 . 1_555 N
O4 SJ Dc2 91.3(14) 312_456 . -108_666 N
O4 SJ Od 132(7) 312_455 . 1_555 N
O4 SJ Od 141.0(17) 312_455 . 105_544 N
O4 SJ Od 113.2(16) 312_455 . -108_665 N
O4 SJ Dd1 125(4) 312_434 . 1_555 N
O4 SJ Dd1 145.8(20) 312_434 . 105_544 N
O4 SJ Dd1 120.2(20) 312_434 . -108_644 N
O4 SJ Dd2 44(6) 312_434 . 1_555 N
O4 SJ Dd2 125.9(17) 312_434 . 105_544 N
O4 SJ Dd2 102.6(17) 312_434 . -108_644 N
SJ SJ SJ 116.3(6) 105_544 . -108_656 N
SJ SJ Oc 20.3(6) 105_544 . 1_555 N
SJ SJ Oc 102.9(10) 105_544 . -108_656 N
SJ SJ Dc1 44.2(10) 105_544 . 1_555 N
SJ SJ Dc1 24.4(5) 105_544 . 105_544 N
SJ SJ Dc1 94.6(6) 105_544 . -108_665 N
SJ SJ Dc2 20.1(13) 105_544 . 1_555 N
SJ SJ Dc2 130.2(10) 105_544 . -108_666 N
SJ SJ Od 84(7) 105_544 . 1_555 N
SJ SJ Od 8.0(12) 105_544 . 105_544 N
SJ SJ Od 107.9(11) 105_544 . -108_665 N
SJ SJ Dd1 77(4) 105_544 . 1_555 N
SJ SJ Dd1 24.1(12) 105_544 . 105_544 N
SJ SJ Dd1 95.7(13) 105_544 . -108_644 N
SJ SJ Dd2 137(8) 105_544 . 1_555 N
SJ SJ Dd2 13.5(14) 105_544 . 105_544 N
SJ SJ Dd2 116.9(13) 105_544 . -108_644 N
SJ SJ Oc 110.1(9) -108_656 . 1_555 N
SJ SJ Oc 16.8(7) -108_656 . -108_656 N
SJ SJ Dc1 74.2(10) -108_665 . 1_555 N
SJ SJ Dc1 93.6(5) -108_665 . 105_544 N
SJ SJ Dc1 22.6(6) -108_665 . -108_665 N
SJ SJ Dc2 134.0(15) -108_666 . 1_555 N
SJ SJ Dc2 14.3(9) -108_666 . -108_666 N
SJ SJ Od 59(7) -108_665 . 1_555 N
SJ SJ Od 109.1(12) -108_665 . 105_544 N
SJ SJ Od 8.7(11) -108_665 . -108_665 N
SJ SJ Dd1 81(4) -108_644 . 1_555 N
SJ SJ Dd1 95.6(12) -108_644 . 105_544 N
SJ SJ Dd1 24.4(11) -108_644 . -108_644 N
SJ SJ Dd2 95(8) -108_644 . 1_555 N
SJ SJ Dd2 120.9(15) -108_644 . 105_544 N
SJ SJ Dd2 8.0(15) -108_644 . -108_644 N
Oc SJ Oc 101.2(16) 1_555 . -108_656 N
Oc SJ Dc1 36.6(9) 1_555 . 1_555 N
Oc SJ Dc1 20.0(9) 1_555 . 105_544 N
Oc SJ Dc1 87.5(13) 1_555 . -108_665 N
Oc SJ Dc2 36.3(8) 1_555 . 1_555 N
Oc SJ Dc2 124.2(17) 1_555 . -108_666 N
Oc SJ Od 66(8) 1_555 . 1_555 N
Oc SJ Od 23.4(13) 1_555 . 105_544 N
Oc SJ Od 102.9(16) 1_555 . -108_665 N
Oc SJ Dd1 57(4) 1_555 . 1_555 N
Oc SJ Dd1 36.0(15) 1_555 . 105_544 N
Oc SJ Dd1 95.5(18) 1_555 . -108_644 N
Oc SJ Dd2 124(8) 1_555 . 1_555 N
Oc SJ Dd2 33.6(17) 1_555 . 105_544 N
Oc SJ Dd2 113.6(18) 1_555 . -108_644 N
Oc SJ Dc1 64.7(14) -108_665 . 1_555 N
Oc SJ Dc1 82.5(11) -108_665 . 105_544 N
Oc SJ Dc1 19.3(5) -108_665 . -108_665 N
Oc SJ Dc2 118.7(19) -108_666 . 1_555 N
Oc SJ Dc2 28.0(5) -108_666 . -108_666 N
Oc SJ Od 64(7) -108_665 . 1_555 N
Oc SJ Od 95.3(15) -108_665 . 105_544 N
Oc SJ Od 9.7(11) -108_665 . -108_665 N
Oc SJ Dd1 86(4) -108_644 . 1_555 N
Oc SJ Dd1 80.5(15) -108_644 . 105_544 N
Oc SJ Dd1 7.8(11) -108_644 . -108_644 N
Oc SJ Dd2 112(8) -108_644 . 1_555 N
Oc SJ Dd2 105.4(18) -108_644 . 105_544 N
Oc SJ Dd2 14.1(13) -108_644 . -108_644 N
Dc1 SJ Dc1 19.9(11) 1_555 . 105_544 N
Dc1 SJ Dc1 51.6(12) 1_555 . -108_665 N
Dc1 SJ Dc2 64.3(15) 1_555 . 1_555 N
Dc1 SJ Dc2 88.5(16) 1_555 . -108_666 N
Dc1 SJ Od 48(6) 1_555 . 1_555 N
Dc1 SJ Od 39.1(16) 1_555 . 105_544 N
Dc1 SJ Od 66.5(15) 1_555 . -108_665 N
Dc1 SJ Dd1 55(4) 1_555 . 1_555 N
Dc1 SJ Dd1 34.1(19) 1_555 . 105_544 N
Dc1 SJ Dd1 59.4(19) 1_555 . -108_644 N
Dc1 SJ Dd2 136(7) 1_555 . 1_555 N
Dc1 SJ Dd2 54.1(18) 1_555 . 105_544 N
Dc1 SJ Dd2 77.1(18) 1_555 . -108_644 N
Dc1 SJ Dc1 71.2(10) 105_544 . -108_665 N
Dc1 SJ Dc2 44.6(10) 105_544 . 1_555 N
Dc1 SJ Dc2 107.9(12) 105_544 . -108_666 N
Dc1 SJ Od 63(7) 105_544 . 1_555 N
Dc1 SJ Od 20.2(10) 105_544 . 105_544 N
Dc1 SJ Od 85.6(12) 105_544 . -108_665 N
Dc1 SJ Dd1 62(4) 105_544 . 1_555 N
Dc1 SJ Dd1 22.3(13) 105_544 . 105_544 N
Dc1 SJ Dd1 76.3(15) 105_544 . -108_644 N
Dc1 SJ Dd2 140(7) 105_544 . 1_555 N
Dc1 SJ Dd2 35.4(13) 105_544 . 105_544 N
Dc1 SJ Dd2 95.8(14) 105_544 . -108_644 N
Dc1 SJ Dc2 113.6(18) -108_666 . 1_555 N
Dc1 SJ Dc2 36.9(6) -108_666 . -108_666 N
Dc1 SJ Od 45(7) -108_665 . 1_555 N
Dc1 SJ Od 88.0(14) -108_665 . 105_544 N
Dc1 SJ Od 15.8(10) -108_665 . -108_665 N
Dc1 SJ Dd1 67(4) -108_644 . 1_555 N
Dc1 SJ Dd1 76.2(15) -108_644 . 105_544 N
Dc1 SJ Dd1 20.6(15) -108_644 . -108_644 N
Dc1 SJ Dd2 110(7) -108_644 . 1_555 N
Dc1 SJ Dd2 101.2(16) -108_644 . 105_544 N
Dc1 SJ Dd2 26.9(13) -108_644 . -108_644 N
Dc2 SJ Dc2 146.7(19) 1_555 . -108_666 N
Dc2 SJ Od 102(8) 1_555 . 1_555 N
Dc2 SJ Od 25.7(13) 1_555 . 105_544 N
Dc2 SJ Od 125.3(18) 1_555 . -108_665 N
Dc2 SJ Dd1 91(4) 1_555 . 1_555 N
Dc2 SJ Dd1 38.4(15) 1_555 . 105_544 N
Dc2 SJ Dd1 111.0(19) 1_555 . -108_644 N
Dc2 SJ Dd2 128(8) 1_555 . 1_555 N
Dc2 SJ Dd2 13.3(16) 1_555 . 105_544 N
Dc2 SJ Dd2 132.7(20) 1_555 . -108_644 N
Dc2 SJ Od 68(8) -108_665 . 1_555 N
Dc2 SJ Od 122.9(16) -108_665 . 105_544 N
Dc2 SJ Od 22.4(10) -108_665 . -108_665 N
Dc2 SJ Dd1 88(4) -108_644 . 1_555 N
Dc2 SJ Dd1 108.5(15) -108_644 . 105_544 N
Dc2 SJ Dd1 35.7(12) -108_644 . -108_644 N
Dc2 SJ Dd2 85(8) -108_644 . 1_555 N
Dc2 SJ Dd2 133.4(18) -108_644 . 105_544 N
Dc2 SJ Dd2 14.0(13) -108_644 . -108_644 N
Od SJ Od 82(8) 1_555 . 105_544 N
Od SJ Od 57(8) 1_555 . -108_665 N
Od SJ Dd1 22(6) 1_555 . 1_555 N
Od SJ Dd1 82(8) 1_555 . 105_544 N
Od SJ Dd1 66(8) 1_555 . -108_644 N
Od SJ Dd2 90(9) 1_555 . 1_555 N
Od SJ Dd2 97(8) 1_555 . 105_544 N
Od SJ Dd2 66(8) 1_555 . -108_644 N
Od SJ Od 100.6(20) 105_544 . -108_665 N
Od SJ Dd1 78(4) 105_544 . 1_555 N
Od SJ Dd1 16.2(7) 105_544 . 105_544 N
Od SJ Dd1 88.0(20) 105_544 . -108_644 N
Od SJ Dd2 145(8) 105_544 . 1_555 N
Od SJ Dd2 15.2(9) 105_544 . 105_544 N
Od SJ Dd2 109.3(19) 105_544 . -108_644 N
Od SJ Dd1 80(4) -108_644 . 1_555 N
Od SJ Dd1 86.9(19) -108_644 . 105_544 N
Od SJ Dd1 16.65(34) -108_644 . -108_644 N
Od SJ Dd2 104(8) -108_644 . 1_555 N
Od SJ Dd2 112.2(20) -108_644 . 105_544 N
Od SJ Dd2 11.0(10) -108_644 . -108_644 N
Dd1 SJ Dd1 84(5) 1_555 . 105_544 N
Dd1 SJ Dd1 88(5) 1_555 . -108_644 N
Dd1 SJ Dd2 81(5) 1_555 . 1_555 N
Dd1 SJ Dd2 90(4) 1_555 . 105_544 N
Dd1 SJ Dd2 88(4) 1_555 . -108_644 N
Dd1 SJ Dd1 73.0(22) 105_544 . -108_644 N
Dd1 SJ Dd2 160(7) 105_544 . 1_555 N
Dd1 SJ Dd2 25.3(6) 105_544 . 105_544 N
Dd1 SJ Dd2 94.6(21) 105_544 . -108_644 N
Dd1 SJ Dd2 120(8) -108_644 . 1_555 N
Dd1 SJ Dd2 97.8(24) -108_644 . 105_544 N
Dd1 SJ Dd2 21.7(9) -108_644 . -108_644 N
Dd2 SJ Dd2 141(8) 1_555 . 105_544 N
Dd2 SJ Dd2 98(8) 1_555 . -108_644 N
Dd2 SJ Dd2 119.4(23) 105_544 . -108_644 N
Si1 Oc Si2 51.11(21) -3_555 . 3_555 N
Si1 Oc Al1 51.11(21) -3_555 . 3_555 N
Si1 Oc O1 24.38(21) -3_555 . -3_555 N
Si1 Oc O4 26.14(14) -3_555 . -111_444 N
Si1 Oc O4 79.74(28) -3_555 . 312_334 N
Si1 Oc SJ 95.8(13) -3_555 . 1_555 N
Si1 Oc SJ 58.6(10) -3_555 . 105_544 N
Si1 Oc Oc 93.7(5) -3_555 . 105_544 N
Si1 Oc Oc 126.6(7) -3_555 . -108_656 N
Si1 Oc Dc1 137.6(12) -3_555 . 1_555 N
Si1 Oc Dc1 102.1(8) -3_555 . 105_544 N
Si1 Oc Dc1 144.8(8) -3_555 . -108_665 N
Si1 Oc Dc1 123.6(6) -3_555 . 308_454 N
Si1 Oc Dc2 35.5(10) -3_555 . 1_555 N
Si1 Oc Dc2 81.7(6) -3_555 . 105_544 N
Si1 Oc Dc2 124.4(7) -3_555 . -108_666 N
Si1 Oc Od 113.4(21) -3_555 . 1_555 N
Si1 Oc Od 66.8(18) -3_555 . 105_544 N
Si1 Oc Od 138.9(9) -3_555 . -108_665 N
Si1 Oc Od 110.8(10) -3_555 . 308_454 N
Si1 Oc Dd1 134.6(34) -3_555 . 1_555 N
Si1 Oc Dd1 81.6(19) -3_555 . 105_544 N
Si1 Oc Dd1 130.7(13) -3_555 . -108_644 N
Si1 Oc Dd1 121.2(12) -3_555 . 308_433 N
Si2 Oc Al1 0.0 3_555 . 3_555 N
Si2 Oc O1 27.35(21) 3_555 . -3_555 N
Si2 Oc O4 77.24(30) 3_555 . -111_444 N
Si2 Oc O4 29.97(15) 3_555 . 312_334 N
Si2 Oc SJ 49.1(11) 3_555 . 1_555 N
Si2 Oc SJ 109.4(11) 3_555 . 105_544 N
Si2 Oc Oc 143.8(5) 3_555 . 105_544 N
Si2 Oc Oc 91.2(6) 3_555 . -108_656 N
Si2 Oc Dc1 107.9(13) 3_555 . 1_555 N
Si2 Oc Dc1 151.4(9) 3_555 . 105_544 N
Si2 Oc Dc1 108.5(6) 3_555 . -108_665 N
Si2 Oc Dc1 174.0(5) 3_555 . 308_454 N
Si2 Oc Dc2 34.8(10) 3_555 . 1_555 N
Si2 Oc Dc2 132.5(6) 3_555 . 105_544 N
Si2 Oc Dc2 80.5(6) 3_555 . -108_666 N
Si2 Oc Od 64.3(21) 3_555 . 1_555 N
Si2 Oc Od 114.9(19) 3_555 . 105_544 N
Si2 Oc Od 102.8(9) 3_555 . -108_665 N
Si2 Oc Od 160.2(10) 3_555 . 308_454 N
Si2 Oc Dd1 85.9(30) 3_555 . 1_555 N
Si2 Oc Dd1 120.6(21) 3_555 . 105_544 N
Si2 Oc Dd1 105.7(14) 3_555 . -108_644 N
Si2 Oc Dd1 161.2(13) 3_555 . 308_433 N
Al1 Oc O1 27.35(21) 3_555 . -3_555 N
Al1 Oc O4 77.24(30) 3_555 . -111_444 N
Al1 Oc O4 29.97(15) 3_555 . 312_334 N
Al1 Oc SJ 49.1(11) 3_555 . 1_555 N
Al1 Oc SJ 109.4(11) 3_555 . 105_544 N
Al1 Oc Oc 143.8(5) 3_555 . 105_544 N
Al1 Oc Oc 91.2(6) 3_555 . -108_656 N
Al1 Oc Dc1 107.9(13) 3_555 . 1_555 N
Al1 Oc Dc1 151.4(9) 3_555 . 105_544 N
Al1 Oc Dc1 108.5(6) 3_555 . -108_665 N
Al1 Oc Dc1 174.0(5) 3_555 . 308_454 N
Al1 Oc Dc2 34.8(10) 3_555 . 1_555 N
Al1 Oc Dc2 132.5(6) 3_555 . 105_544 N
Al1 Oc Dc2 80.5(6) 3_555 . -108_666 N
Al1 Oc Od 64.3(21) 3_555 . 1_555 N
Al1 Oc Od 114.9(19) 3_555 . 105_544 N
Al1 Oc Od 102.8(9) 3_555 . -108_665 N
Al1 Oc Od 160.2(10) 3_555 . 308_454 N
Al1 Oc Dd1 85.9(30) 3_555 . 1_555 N
Al1 Oc Dd1 120.6(21) 3_555 . 105_544 N
Al1 Oc Dd1 105.7(14) 3_555 . -108_644 N
Al1 Oc Dd1 161.2(13) 3_555 . 308_433 N
O1 Oc O4 50.36(27) -3_555 . -111_444 N
O1 Oc O4 55.36(30) -3_555 . 312_334 N
O1 Oc SJ 72.0(12) -3_555 . 1_555 N
O1 Oc SJ 82.1(11) -3_555 . 105_544 N
O1 Oc Oc 116.6(6) -3_555 . 105_544 N
O1 Oc Oc 108.1(8) -3_555 . -108_656 N
O1 Oc Dc1 123.0(12) -3_555 . 1_555 N
O1 Oc Dc1 124.5(9) -3_555 . 105_544 N
O1 Oc Dc1 127.2(8) -3_555 . -108_665 N
O1 Oc Dc1 147.0(7) -3_555 . 308_454 N
O1 Oc Dc2 20.9(13) -3_555 . 1_555 N
O1 Oc Dc2 106.0(7) -3_555 . 105_544 N
O1 Oc Dc2 102.1(8) -3_555 . -108_666 N
O1 Oc Od 89.2(21) -3_555 . 1_555 N
O1 Oc Od 88.1(19) -3_555 . 105_544 N
O1 Oc Od 120.9(9) -3_555 . -108_665 N
O1 Oc Od 135.2(10) -3_555 . 308_454 N
O1 Oc Dd1 113.1(31) -3_555 . 1_555 N
O1 Oc Dd1 97.8(20) -3_555 . 105_544 N
O1 Oc Dd1 117.9(14) -3_555 . -108_644 N
O1 Oc Dd1 144.9(13) -3_555 . 308_433 N
O4 Oc O4 105.59(34) -111_444 . 312_334 N
O4 Oc SJ 120.1(13) -111_556 . 1_555 N
O4 Oc SJ 32.8(9) -111_556 . 105_544 N
O4 Oc Oc 68.0(5) -111_556 . 105_544 N
O4 Oc Oc 137.8(8) -111_556 . -108_656 N
O4 Oc Dc1 139.4(13) -111_565 . 1_555 N
O4 Oc Dc1 76.5(7) -111_565 . 105_544 N
O4 Oc Dc1 148.2(8) -111_565 . -108_665 N
O4 Oc Dc1 97.5(6) -111_565 . 308_454 N
O4 Oc Dc2 56.5(8) -111_566 . 1_555 N
O4 Oc Dc2 55.7(5) -111_566 . 105_544 N
O4 Oc Dc2 143.7(8) -111_566 . -108_666 N
O4 Oc Od 138.3(22) -111_565 . 1_555 N
O4 Oc Od 43.2(18) -111_565 . 105_544 N
O4 Oc Od 145.5(8) -111_565 . -108_665 N
O4 Oc Od 84.9(9) -111_565 . 308_454 N
O4 Oc Dd1 156(4) -111_544 . 1_555 N
O4 Oc Dd1 62.2(18) -111_544 . 105_544 N
O4 Oc Dd1 132.1(10) -111_544 . -108_644 N
O4 Oc Dd1 96.3(11) -111_544 . 308_433 N
O4 Oc SJ 20.0(10) 312_446 . 1_555 N
O4 Oc SJ 135.3(11) 312_446 . 105_544 N
O4 Oc Oc 160.0(8) 312_446 . 105_544 N
O4 Oc Oc 63.6(5) 312_446 . -108_656 N
O4 Oc Dc1 80.0(13) 312_455 . 1_555 N
O4 Oc Dc1 159.2(12) 312_455 . 105_544 N
O4 Oc Dc1 79.2(5) 312_455 . -108_665 N
O4 Oc Dc1 153.6(7) 312_455 . 308_454 N
O4 Oc Dc2 53.0(7) 312_456 . 1_555 N
O4 Oc Dc2 161.1(6) 312_456 . 105_544 N
O4 Oc Dc2 51.1(5) 312_456 . -108_666 N
O4 Oc Od 34.4(21) 312_455 . 1_555 N
O4 Oc Od 135.0(19) 312_455 . 105_544 N
O4 Oc Od 74.0(8) 312_455 . -108_665 N
O4 Oc Od 169.4(10) 312_455 . 308_454 N
O4 Oc Dd1 62.3(25) 312_434 . 1_555 N
O4 Oc Dd1 128.2(21) 312_434 . 105_544 N
O4 Oc Dd1 79.6(13) 312_434 . -108_644 N
O4 Oc Dd1 156.6(10) 312_434 . 308_433 N
SJ Oc SJ 142.9(11) 1_555 . 105_544 N
SJ Oc Oc 147.7(14) 1_555 . 105_544 N
SJ Oc Oc 43.6(12) 1_555 . -108_656 N
SJ Oc Dc1 60.0(16) 1_555 . 1_555 N
SJ Oc Dc1 142.6(16) 1_555 . 105_544 N
SJ Oc Dc1 59.5(12) 1_555 . -108_665 N
SJ Oc Dc1 133.9(13) 1_555 . 308_454 N
SJ Oc Dc2 63.8(13) 1_555 . 1_555 N
SJ Oc Dc2 164.1(15) 1_555 . 105_544 N
SJ Oc Dc2 31.5(12) 1_555 . -108_666 N
SJ Oc Od 18.2(24) 1_555 . 1_555 N
SJ Oc Od 135.4(24) 1_555 . 105_544 N
SJ Oc Od 54.1(14) 1_555 . -108_665 N
SJ Oc Od 150.7(16) 1_555 . 308_454 N
SJ Oc Dd1 54.8(25) 1_555 . 1_555 N
SJ Oc Dd1 120.0(24) 1_555 . 105_544 N
SJ Oc Dd1 59.8(16) 1_555 . -108_644 N
SJ Oc Dd1 143.0(17) 1_555 . 308_433 N
SJ Oc Oc 35.1(10) 105_544 . 105_544 N
SJ Oc Oc 128.9(11) 105_544 . -108_656 N
SJ Oc Dc1 119.4(16) 105_544 . 1_555 N
SJ Oc Dc1 43.7(12) 105_544 . 105_544 N
SJ Oc Dc1 125.9(11) 105_544 . -108_665 N
SJ Oc Dc1 65.1(11) 105_544 . 308_454 N
SJ Oc Dc2 82.5(12) 105_544 . 1_555 N
SJ Oc Dc2 26.0(11) 105_544 . 105_544 N
SJ Oc Dc2 144.2(12) 105_544 . -108_666 N
SJ Oc Od 157.5(24) 105_544 . 1_555 N
SJ Oc Od 14.9(21) 105_544 . 105_544 N
SJ Oc Od 127.4(12) 105_544 . -108_665 N
SJ Oc Od 54.6(14) 105_544 . 308_454 N
SJ Oc Dd1 161.9(26) 105_544 . 1_555 N
SJ Oc Dd1 37.5(21) 105_544 . 105_544 N
SJ Oc Dd1 114.6(12) 105_544 . -108_644 N
SJ Oc Dd1 68.0(15) 105_544 . 308_433 N
Oc Oc Oc 107.7(6) 105_544 . -108_656 N
Oc Oc Dc1 92.9(13) 105_544 . 1_555 N
Oc Oc Dc1 8.7(6) 105_544 . 105_544 N
Oc Oc Dc1 96.6(5) 105_544 . -108_665 N
Oc Oc Dc1 30.4(4) 105_544 . 308_454 N
Oc Oc Dc2 112.2(8) 105_544 . 1_555 N
Oc Oc Dc2 19.26(12) 105_544 . 105_544 N
Oc Oc Dc2 123.0(5) 105_544 . -108_666 N
Oc Oc Od 142.8(21) 105_544 . 1_555 N
Oc Oc Od 29.2(18) 105_544 . 105_544 N
Oc Oc Od 100.3(9) 105_544 . -108_665 N
Oc Oc Od 25.0(8) 105_544 . 308_454 N
Oc Oc Dd1 130.2(30) 105_544 . 1_555 N
Oc Oc Dd1 31.8(20) 105_544 . 105_544 N
Oc Oc Dd1 91.0(12) 105_544 . -108_644 N
Oc Oc Dd1 39.6(9) 105_544 . 308_433 N
Oc Oc Dc1 16.6(12) -108_665 . 1_555 N
Oc Oc Dc1 100.6(8) -108_665 . 105_544 N
Oc Oc Dc1 19.07(16) -108_665 . -108_665 N
Oc Oc Dc1 90.8(4) -108_665 . 308_454 N
Oc Oc Dc2 91.5(11) -108_666 . 1_555 N
Oc Oc Dc2 126.9(6) -108_666 . 105_544 N
Oc Oc Dc2 16.08(14) -108_666 . -108_666 N
Oc Oc Od 35.7(20) -108_665 . 1_555 N
Oc Oc Od 114.0(19) -108_665 . 105_544 N
Oc Oc Od 12.8(8) -108_665 . -108_665 N
Oc Oc Od 108.0(8) -108_665 . 308_454 N
Oc Oc Dd1 57.8(31) -108_644 . 1_555 N
Oc Oc Dd1 91.6(19) -108_644 . 105_544 N
Oc Oc Dd1 16.7(11) -108_644 . -108_644 N
Oc Oc Dd1 104.9(12) -108_644 . 308_433 N
Dc1 Oc Dc1 85.2(17) 1_555 . 105_544 N
Dc1 Oc Dc1 8.9(16) 1_555 . -108_665 N
Dc1 Oc Dc1 74.2(15) 1_555 . 308_454 N
Dc1 Oc Dc2 104.4953 1_555 . 1_555 N
Dc1 Oc Dc2 111.9(13) 1_555 . 105_544 N
Dc1 Oc Dc2 30.2(12) 1_555 . -108_666 N
Dc1 Oc Od 49.9(22) 1_555 . 1_555 N
Dc1 Oc Od 104.7(22) 1_555 . 105_544 N
Dc1 Oc Od 8.0(15) 1_555 . -108_665 N
Dc1 Oc Od 91.3(15) 1_555 . 308_454 N
Dc1 Oc Dd1 62(4) 1_555 . 1_555 N
Dc1 Oc Dd1 82.4(22) 1_555 . 105_544 N
Dc1 Oc Dd1 7.5(16) 1_555 . -108_644 N
Dc1 Oc Dd1 88.6(18) 1_555 . 308_433 N
Dc1 Oc Dc1 88.4(9) 105_544 . -108_665 N
Dc1 Oc Dc1 22.7(7) 105_544 . 308_454 N
Dc1 Oc Dc2 118.2(13) 105_544 . 1_555 N
Dc1 Oc Dc2 26.6(6) 105_544 . 105_544 N
Dc1 Oc Dc2 115.4(8) 105_544 . -108_666 N
Dc1 Oc Od 135.0(22) 105_544 . 1_555 N
Dc1 Oc Od 36.5(18) 105_544 . 105_544 N
Dc1 Oc Od 92.4(11) 105_544 . -108_665 N
Dc1 Oc Od 21.7(11) 105_544 . 308_454 N
Dc1 Oc Dd1 122.4(32) 105_544 . 1_555 N
Dc1 Oc Dd1 34.1(20) 105_544 . 105_544 N
Dc1 Oc Dd1 83.9(14) 105_544 . -108_644 N
Dc1 Oc Dd1 35.4(13) 105_544 . 308_433 N
Dc1 Oc Dc1 74.4(5) -108_665 . 308_454 N
Dc1 Oc Dc2 110.2(12) -108_666 . 1_555 N
Dc1 Oc Dc2 114.8(4) -108_666 . 105_544 N
Dc1 Oc Dc2 28.14(13) -108_666 . -108_666 N
Dc1 Oc Od 46.7(21) -108_665 . 1_555 N
Dc1 Oc Od 111.6(19) -108_665 . 105_544 N
Dc1 Oc Od 6.2(8) -108_665 . -108_665 N
Dc1 Oc Od 91.3(9) -108_665 . 308_454 N
Dc1 Oc Dd1 53(4) -108_644 . 1_555 N
Dc1 Oc Dd1 89.7(19) -108_644 . 105_544 N
Dc1 Oc Dd1 16.3(11) -108_644 . -108_644 N
Dc1 Oc Dd1 86.4(12) -108_644 . 308_433 N
Dc1 Oc Dc2 139.5(7) 308_455 . 1_555 N
Dc1 Oc Dc2 42.8(4) 308_455 . 105_544 N
Dc1 Oc Dc2 102.6(5) 308_455 . -108_666 N
Dc1 Oc Od 119.7(22) 308_454 . 1_555 N
Dc1 Oc Od 59.2(18) 308_454 . 105_544 N
Dc1 Oc Od 79.8(9) 308_454 . -108_665 N
Dc1 Oc Od 17.2(9) 308_454 . 308_454 N
Dc1 Oc Dd1 99.9(30) 308_433 . 1_555 N
Dc1 Oc Dd1 53.7(20) 308_433 . 105_544 N
Dc1 Oc Dd1 75.5(14) 308_433 . -108_644 N
Dc1 Oc Dd1 20.8(12) 308_433 . 308_433 N
Dc2 Oc Dc2 108.6(6) 1_555 . 105_544 N
Dc2 Oc Dc2 89.4(6) 1_555 . -108_666 N
Dc2 Oc Od 82.0(22) 1_555 . 1_555 N
Dc2 Oc Od 83.3(19) 1_555 . 105_544 N
Dc2 Oc Od 104.1(13) 1_555 . -108_665 N
Dc2 Oc Od 136.2(10) 1_555 . 308_454 N
Dc2 Oc Dd1 115.2(26) 1_555 . 1_555 N
Dc2 Oc Dd1 85.9(22) 1_555 . 105_544 N
Dc2 Oc Dd1 98.6(18) 1_555 . -108_644 N
Dc2 Oc Dd1 150.4(11) 1_555 . 308_433 N
Dc2 Oc Dc2 142.0(5) 105_544 . -108_666 N
Dc2 Oc Od 161.6(21) 105_544 . 1_555 N
Dc2 Oc Od 29.8(18) 105_544 . 105_544 N
Dc2 Oc Od 119.0(9) 105_544 . -108_665 N
Dc2 Oc Od 29.3(9) 105_544 . 308_454 N
Dc2 Oc Dd1 136.0(25) 105_544 . 1_555 N
Dc2 Oc Dd1 44.2(19) 105_544 . 105_544 N
Dc2 Oc Dd1 110.2(12) 105_544 . -108_644 N
Dc2 Oc Dd1 42.0(10) 105_544 . 308_433 N
Dc2 Oc Od 19.9(20) -108_665 . 1_555 N
Dc2 Oc Od 129.5(19) -108_665 . 105_544 N
Dc2 Oc Od 23.2(8) -108_665 . -108_665 N
Dc2 Oc Od 119.3(9) -108_665 . 308_454 N
Dc2 Oc Dd1 45.5(28) -108_644 . 1_555 N
Dc2 Oc Dd1 107.4(19) -108_644 . 105_544 N
Dc2 Oc Dd1 32.3(10) -108_644 . -108_644 N
Dc2 Oc Dd1 112.9(12) -108_644 . 308_433 N
Od Oc Od 145.4(18) 1_555 . 105_544 N
Od Oc Od 42.6(16) 1_555 . -108_665 N
Od Oc Od 135.1(25) 1_555 . 308_454 N
Od Oc Dd1 38.6(16) 1_555 . 1_555 N
Od Oc Dd1 124.8(26) 1_555 . 105_544 N
Od Oc Dd1 52.2(21) 1_555 . -108_644 N
Od Oc Dd1 125.2(27) 1_555 . 308_433 N
Od Oc Od 112.7(25) 105_544 . -108_665 N
Od Oc Od 53.1(17) 105_544 . 308_454 N
Od Oc Dd1 159(4) 105_544 . 1_555 N
Od Oc Dd1 22.6(17) 105_544 . 105_544 N
Od Oc Dd1 99.7(26) 105_544 . -108_644 N
Od Oc Dd1 67.6(18) 105_544 . 308_433 N
Od Oc Od 96.8(10) -108_665 . 308_454 N
Od Oc Dd1 54(4) -108_644 . 1_555 N
Od Oc Dd1 90.3(23) -108_644 . 105_544 N
Od Oc Dd1 13.88(23) -108_644 . -108_644 N
Od Oc Dd1 92.5(14) -108_644 . 308_433 N
Od Oc Dd1 108.3(31) 308_433 . 1_555 N
Od Oc Dd1 55.6(23) 308_433 . 105_544 N
Od Oc Dd1 92.7(14) 308_433 . -108_644 N
Od Oc Dd1 14.63(25) 308_433 . 308_433 N
Dd1 Oc Dd1 141(5) 1_555 . 105_544 N
Dd1 Oc Dd1 68(4) 1_555 . -108_644 N
Dd1 Oc Dd1 94.4(32) 1_555 . 308_433 N
Dd1 Oc Dd1 77.1(25) 105_544 . -108_644 N
Dd1 Oc Dd1 69.5(26) 105_544 . 308_433 N
Dd1 Oc Dd1 91.8(18) -108_644 . 308_433 N
Si2 Dc1 Al1 0.0 3_555 . 3_555 N
Si2 Dc1 O1 25.03(20) 3_555 . -3_555 N
Si2 Dc1 O1 66.80(34) 3_555 . 111_433 N
Si2 Dc1 O4 27.12(16) 3_555 . 312_334 N
Si2 Dc1 SJ 27.0(14) 3_555 . 1_555 N
Si2 Dc1 SJ 86.3(8) 3_555 . 105_544 N
Si2 Dc1 SJ 107.9(8) 3_555 . -108_656 N
Si2 Dc1 Oc 58.6(11) 3_555 . 1_555 N
Si2 Dc1 Oc 119.3(5) 3_555 . 105_544 N
Si2 Dc1 Oc 96.2(9) 3_555 . -108_656 N
Si2 Dc1 Oc 135.1(7) 3_555 . -305_556 N
Si2 Dc1 Dc1 119.3(8) 3_555 . 105_544 N
Si2 Dc1 Dc1 121.7(8) 3_555 . -108_665 N
Si2 Dc1 Dc1 177.6(9) 3_555 . -201_564 N
Si2 Dc1 Dc1 148.2(8) 3_555 . 308_454 N
Si2 Dc1 Dc1 150.6(8) 3_555 . -305_565 N
Si2 Dc1 Dc2 33.4(9) 3_555 . 1_555 N
Si2 Dc1 Dc2 107.1(5) 3_555 . 105_544 N
Si2 Dc1 Dc2 83.2(6) 3_555 . -108_666 N
Si2 Dc1 Od 41.8(28) 3_555 . 1_555 N
Si2 Dc1 Od 91.3(15) 3_555 . 105_544 N
Si2 Dc1 Od 114.7(12) 3_555 . -108_665 N
Si2 Dc1 Od 132.9(9) 3_555 . 308_454 N
Si2 Dc1 Dd1 70.9(33) 3_555 . 1_555 N
Al1 Dc1 O1 25.03(20) 3_555 . -3_555 N
Al1 Dc1 O1 66.80(34) 3_555 . 111_433 N
Al1 Dc1 O4 27.12(16) 3_555 . 312_334 N
Al1 Dc1 SJ 27.0(14) 3_555 . 1_555 N
Al1 Dc1 SJ 86.3(8) 3_555 . 105_544 N
Al1 Dc1 SJ 107.9(8) 3_555 . -108_656 N
Al1 Dc1 Oc 58.6(11) 3_555 . 1_555 N
Al1 Dc1 Oc 119.3(5) 3_555 . 105_544 N
Al1 Dc1 Oc 96.2(9) 3_555 . -108_656 N
Al1 Dc1 Oc 135.1(7) 3_555 . -305_556 N
Al1 Dc1 Dc1 119.3(8) 3_555 . 105_544 N
Al1 Dc1 Dc1 121.7(8) 3_555 . -108_665 N
Al1 Dc1 Dc1 177.6(9) 3_555 . -201_564 N
Al1 Dc1 Dc1 148.2(8) 3_555 . 308_454 N
Al1 Dc1 Dc1 150.6(8) 3_555 . -305_565 N
Al1 Dc1 Dc2 33.4(9) 3_555 . 1_555 N
Al1 Dc1 Dc2 107.1(5) 3_555 . 105_544 N
Al1 Dc1 Dc2 83.2(6) 3_555 . -108_666 N
Al1 Dc1 Od 41.8(28) 3_555 . 1_555 N
Al1 Dc1 Od 91.3(15) 3_555 . 105_544 N
Al1 Dc1 Od 114.7(12) 3_555 . -108_665 N
Al1 Dc1 Od 132.9(9) 3_555 . 308_454 N
Al1 Dc1 Dd1 70.9(33) 3_555 . 1_555 N
O1 Dc1 O1 89.5(5) -3_555 . 111_433 N
O1 Dc1 O4 51.44(30) -3_555 . 312_334 N
O1 Dc1 SJ 51.4(14) -3_555 . 1_555 N
O1 Dc1 SJ 61.8(8) -3_555 . 105_544 N
O1 Dc1 SJ 129.2(9) -3_555 . -108_656 N
O1 Dc1 Oc 42.7(10) -3_555 . 1_555 N
O1 Dc1 Oc 94.7(6) -3_555 . 105_544 N
O1 Dc1 Oc 114.2(11) -3_555 . -108_656 N
O1 Dc1 Oc 159.7(8) -3_555 . -305_556 N
O1 Dc1 Dc1 95.1(9) -3_555 . 105_544 N
O1 Dc1 Dc1 142.6(10) -3_555 . -108_665 N
O1 Dc1 Dc1 154.5(9) -3_555 . -201_564 N
O1 Dc1 Dc1 125.5(9) -3_555 . 308_454 N
O1 Dc1 Dc1 173.4(8) -3_555 . -305_565 N
O1 Dc1 Dc2 8.5(8) -3_555 . 1_555 N
O1 Dc1 Dc2 83.7(5) -3_555 . 105_544 N
O1 Dc1 Dc2 105.6(7) -3_555 . -108_666 N
O1 Dc1 Od 66.8(28) -3_555 . 1_555 N
O1 Dc1 Od 66.3(15) -3_555 . 105_544 N
O1 Dc1 Od 134.1(12) -3_555 . -108_665 N
O1 Dc1 Od 111.6(10) -3_555 . 308_454 N
O1 Dc1 Dd1 88(4) -3_555 . 1_555 N
O1 Dc1 O4 40.04(25) 111_433 . 312_334 N
O1 Dc1 SJ 40.2(14) 111_545 . 1_555 N
O1 Dc1 SJ 149.3(10) 111_545 . 105_544 N
O1 Dc1 SJ 41.2(6) 111_545 . -108_656 N
O1 Dc1 Oc 122.9(14) 111_545 . 1_555 N
O1 Dc1 Oc 165.3(9) 111_545 . 105_544 N
O1 Dc1 Oc 33.2(6) 111_545 . -108_656 N
O1 Dc1 Oc 70.3(5) 111_545 . -305_556 N
O1 Dc1 Dc1 169.1(14) 111_554 . 105_544 N
O1 Dc1 Dc1 55.0(6) 111_554 . -108_665 N
O1 Dc1 Dc1 114.6(6) 111_554 . -201_564 N
O1 Dc1 Dc1 144.7(6) 111_554 . 308_454 N
O1 Dc1 Dc1 84.8(6) 111_554 . -305_565 N
O1 Dc1 Dc2 97.8(11) 111_555 . 1_555 N
O1 Dc1 Dc2 172.4(5) 111_555 . 105_544 N
O1 Dc1 Dc2 16.4(4) 111_555 . -108_666 N
O1 Dc1 Od 35.3(29) 111_554 . 1_555 N
O1 Dc1 Od 148.7(16) 111_554 . 105_544 N
O1 Dc1 Od 48.5(11) 111_554 . -108_665 N
O1 Dc1 Od 158.5(9) 111_554 . 308_454 N
O1 Dc1 Dd1 70.1(31) 111_533 . 1_555 N
O4 Dc1 SJ 0.264(6) 312_446 . 1_555 N
O4 Dc1 SJ 113.2(9) 312_446 . 105_544 N
O4 Dc1 SJ 81.2(7) 312_446 . -108_656 N
O4 Dc1 Oc 83.5(12) 312_446 . 1_555 N
O4 Dc1 Oc 146.1(6) 312_446 . 105_544 N
O4 Dc1 Oc 71.4(8) 312_446 . -108_656 N
O4 Dc1 Oc 108.3(7) 312_446 . -305_556 N
O4 Dc1 Dc1 146.3(7) 312_455 . 105_544 N
O4 Dc1 Dc1 94.9(8) 312_455 . -108_665 N
O4 Dc1 Dc1 153.9(8) 312_455 . -201_564 N
O4 Dc1 Dc1 171.7(5) 312_455 . 308_454 N
O4 Dc1 Dc1 123.7(7) 312_455 . -305_565 N
O4 Dc1 Dc2 59.9(10) 312_456 . 1_555 N
O4 Dc1 Dc2 134.1(6) 312_456 . 105_544 N
O4 Dc1 Dc2 56.4(5) 312_456 . -108_666 N
O4 Dc1 Od 19.6(27) 312_455 . 1_555 N
O4 Dc1 Od 117.4(16) 312_455 . 105_544 N
O4 Dc1 Od 88.5(11) 312_455 . -108_665 N
O4 Dc1 Od 157.3(9) 312_455 . 308_454 N
O4 Dc1 Dd1 63.1(28) 312_434 . 1_555 N
SJ Dc1 SJ 113.1(12) 1_555 . 105_544 N
SJ Dc1 SJ 81.4(11) 1_555 . -108_656 N
SJ Dc1 Oc 83.4(18) 1_555 . 1_555 N
SJ Dc1 Oc 146.1(16) 1_555 . 105_544 N
SJ Dc1 Oc 71.6(17) 1_555 . -108_656 N
SJ Dc1 Oc 108.3(17) 1_555 . -305_556 N
SJ Dc1 Dc1 146.3(17) 1_555 . 105_544 N
SJ Dc1 Dc1 95.1(17) 1_555 . -108_665 N
SJ Dc1 Dc1 154.0(17) 1_555 . -201_564 N
SJ Dc1 Dc1 171.5(16) 1_555 . 308_454 N
SJ Dc1 Dc1 123.7(17) 1_555 . -305_565 N
SJ Dc1 Dc2 59.9(16) 1_555 . 1_555 N
SJ Dc1 Dc2 134.0(15) 1_555 . 105_544 N
SJ Dc1 Dc2 56.5(15) 1_555 . -108_666 N
SJ Dc1 Od 19.5(31) 1_555 . 1_555 N
SJ Dc1 Od 117.4(23) 1_555 . 105_544 N
SJ Dc1 Od 88.6(19) 1_555 . -108_665 N
SJ Dc1 Od 157.0(18) 1_555 . 308_454 N
SJ Dc1 Dd1 62.9(32) 1_555 . 1_555 N
SJ Dc1 SJ 157.4(13) 105_544 . -108_656 N
SJ Dc1 Oc 41.3(12) 105_544 . 1_555 N
SJ Dc1 Oc 33.0(8) 105_544 . 105_544 N
SJ Dc1 Oc 148.9(15) 105_544 . -108_656 N
SJ Dc1 Oc 138.5(11) 105_544 . -305_556 N
SJ Dc1 Dc1 33.3(11) 105_544 . 105_544 N
SJ Dc1 Dc1 147.7(13) 105_544 . -108_665 N
SJ Dc1 Dc1 92.9(11) 105_544 . -201_564 N
SJ Dc1 Dc1 64.2(11) 105_544 . 308_454 N
SJ Dc1 Dc1 123.0(11) 105_544 . -305_565 N
SJ Dc1 Dc2 53.3(10) 105_544 . 1_555 N
SJ Dc1 Dc2 23.2(8) 105_544 . 105_544 N
SJ Dc1 Dc2 161.4(12) 105_544 . -108_666 N
SJ Dc1 Od 126.2(31) 105_544 . 1_555 N
SJ Dc1 Od 9.3(16) 105_544 . 105_544 N
SJ Dc1 Od 149.2(14) 105_544 . -108_665 N
SJ Dc1 Od 52.0(13) 105_544 . 308_454 N
SJ Dc1 Dd1 116(4) 105_544 . 1_555 N
SJ Dc1 Oc 161.1(17) -108_656 . 1_555 N
SJ Dc1 Oc 129.8(8) -108_656 . 105_544 N
SJ Dc1 Oc 17.4(8) -108_656 . -108_656 N
SJ Dc1 Oc 32.4(6) -108_656 . -305_556 N
SJ Dc1 Dc1 131.2(8) -108_665 . 105_544 N
SJ Dc1 Dc1 13.8(7) -108_665 . -108_665 N
SJ Dc1 Dc1 73.6(7) -108_665 . -201_564 N
SJ Dc1 Dc1 103.8(7) -108_665 . 308_454 N
SJ Dc1 Dc1 44.6(7) -108_665 . -305_565 N
SJ Dc1 Dc2 136.6(14) -108_666 . 1_555 N
SJ Dc1 Dc2 144.2(9) -108_666 . 105_544 N
SJ Dc1 Dc2 24.9(6) -108_666 . -108_666 N
SJ Dc1 Od 72.8(30) -108_665 . 1_555 N
SJ Dc1 Od 148.2(17) -108_665 . 105_544 N
SJ Dc1 Od 8.4(12) -108_665 . -108_665 N
SJ Dc1 Od 118.8(11) -108_665 . 308_454 N
SJ Dc1 Dd1 86(4) -108_644 . 1_555 N
Oc Dc1 Oc 68.0(12) 1_555 . 105_544 N
Oc Dc1 Oc 154.7(18) 1_555 . -108_656 N
Oc Dc1 Oc 149.1(14) 1_555 . -305_556 N
Oc Dc1 Dc1 66.0(15) 1_555 . 105_544 N
Oc Dc1 Dc1 166.9(23) 1_555 . -108_665 N
Oc Dc1 Dc1 119.5(15) 1_555 . -201_564 N
Oc Dc1 Dc1 90.1(15) 1_555 . 308_454 N
Oc Dc1 Dc1 143.9(13) 1_555 . -305_565 N
Oc Dc1 Dc2 37.7702 1_555 . 1_555 N
Oc Dc1 Dc2 52.9(10) 1_555 . 105_544 N
Oc Dc1 Dc2 138.4(15) 1_555 . -108_666 N
Oc Dc1 Od 89.2(31) 1_555 . 1_555 N
Oc Dc1 Od 50.3(17) 1_555 . 105_544 N
Oc Dc1 Od 169.5(19) 1_555 . -108_665 N
Oc Dc1 Od 74.6(15) 1_555 . 308_454 N
Oc Dc1 Dd1 78(4) 1_555 . 1_555 N
Oc Dc1 Oc 133.8(11) 105_544 . -108_656 N
Oc Dc1 Oc 105.6(5) 105_544 . -305_556 N
Oc Dc1 Dc1 4.3(8) 105_544 . 105_544 N
Oc Dc1 Dc1 116.9(7) 105_544 . -108_665 N
Oc Dc1 Dc1 59.9(5) 105_544 . -201_564 N
Oc Dc1 Dc1 32.3(5) 105_544 . 308_454 N
Oc Dc1 Dc1 90.0(5) 105_544 . -305_565 N
Oc Dc1 Dc2 86.2(9) 105_544 . 1_555 N
Oc Dc1 Dc2 15.43(21) 105_544 . 105_544 N
Oc Dc1 Dc2 153.4(8) 105_544 . -108_666 N
Oc Dc1 Od 157.3(30) 105_544 . 1_555 N
Oc Dc1 Od 29.0(15) 105_544 . 105_544 N
Oc Dc1 Od 121.6(12) 105_544 . -108_665 N
Oc Dc1 Od 24.5(8) 105_544 . 308_454 N
Oc Dc1 Dd1 124.1(32) 105_544 . 1_555 N
Oc Dc1 Oc 49.0(5) -108_656 . -305_556 N
Oc Dc1 Dc1 136.7(13) -108_665 . 105_544 N
Oc Dc1 Dc1 28.72(23) -108_665 . -108_665 N
Oc Dc1 Dc1 85.70(30) -108_665 . -201_564 N
Oc Dc1 Dc1 115.13(33) -108_665 . 308_454 N
Oc Dc1 Dc1 59.3(5) -108_665 . -305_565 N
Oc Dc1 Dc2 120.8(16) -108_666 . 1_555 N
Oc Dc1 Dc2 149.1(12) -108_666 . 105_544 N
Oc Dc1 Dc2 20.4(4) -108_666 . -108_666 N
Oc Dc1 Od 68.3(30) -108_665 . 1_555 N
Oc Dc1 Od 140.4(20) -108_665 . 105_544 N
Oc Dc1 Od 19.9(11) -108_665 . -108_665 N
Oc Dc1 Od 130.7(10) -108_665 . 308_454 N
Oc Dc1 Dd1 94(4) -108_644 . 1_555 N
Oc Dc1 Dc1 105.28(19) -305_565 . 105_544 N
Oc Dc1 Dc1 20.7(6) -305_565 . -108_665 N
Oc Dc1 Dc1 45.68(22) -305_565 . -201_564 N
Oc Dc1 Dc1 74.75(15) -305_565 . 308_454 N
Oc Dc1 Dc1 15.70(9) -305_565 . -305_565 N
Oc Dc1 Dc2 168.1(13) -305_566 . 1_555 N
Oc Dc1 Dc2 116.6(6) -305_566 . 105_544 N
Oc Dc1 Dc2 54.51(35) -305_566 . -108_666 N
Oc Dc1 Od 93.9(30) -305_565 . 1_555 N
Oc Dc1 Od 133.4(16) -305_565 . 105_544 N
Oc Dc1 Od 29.6(10) -305_565 . -108_665 N
Oc Dc1 Od 88.4(9) -305_565 . 308_454 N
Oc Dc1 Dd1 83(4) -305_544 . 1_555 N
Dc1 Dc1 Dc1 118.0(6) 105_544 . -108_665 N
Dc1 Dc1 Dc1 59.74(8) 105_544 . -201_564 N
Dc1 Dc1 Dc1 31.01(30) 105_544 . 308_454 N
Dc1 Dc1 Dc1 90.00000(30) 105_544 . -305_565 N
Dc1 Dc1 Dc2 86.6(14) 105_544 . 1_555 N
Dc1 Dc1 Dc2 13.1(7) 105_544 . 105_544 N
Dc1 Dc1 Dc2 155.6(8) 105_544 . -108_666 N
Dc1 Dc1 Od 155.0(32) 105_544 . 1_555 N
Dc1 Dc1 Od 30.5(16) 105_544 . 105_544 N
Dc1 Dc1 Od 123.3(12) 105_544 . -108_665 N
Dc1 Dc1 Od 21.4(11) 105_544 . 308_454 N
Dc1 Dc1 Dd1 119.8(35) 105_544 . 1_555 N
Dc1 Dc1 Dc1 59.74(8) -108_665 . -201_564 N
Dc1 Dc1 Dc1 90.00000(30) -108_665 . 308_454 N
Dc1 Dc1 Dc1 31.01(30) -108_665 . -305_565 N
Dc1 Dc1 Dc2 149.5(15) -108_666 . 1_555 N
Dc1 Dc1 Dc2 130.8(7) -108_666 . 105_544 N
Dc1 Dc1 Dc2 38.58(35) -108_666 . -108_666 N
Dc1 Dc1 Od 85.3(30) -108_665 . 1_555 N
Dc1 Dc1 Od 139.4(19) -108_665 . 105_544 N
Dc1 Dc1 Od 9.0(11) -108_665 . -108_665 N
Dc1 Dc1 Od 105.0(9) -108_665 . 308_454 N
Dc1 Dc1 Dd1 90(4) -108_644 . 1_555 N
Dc1 Dc1 Dc1 30.26(8) -201_564 . 308_454 N
Dc1 Dc1 Dc1 30.26(8) -201_564 . -305_565 N
Dc1 Dc1 Dc2 146.0(14) -201_565 . 1_555 N
Dc1 Dc1 Dc2 71.7(6) -201_565 . 105_544 N
Dc1 Dc1 Dc2 98.20(34) -201_565 . -108_666 N
Dc1 Dc1 Od 138.3(30) -201_564 . 1_555 N
Dc1 Dc1 Od 88.2(16) -201_564 . 105_544 N
Dc1 Dc1 Od 67.0(11) -201_564 . -108_665 N
Dc1 Dc1 Od 45.5(9) -201_564 . 308_454 N
Dc1 Dc1 Dd1 107.5(34) -201_543 . 1_555 N
Dc1 Dc1 Dc1 60.00000(20) 308_454 . -305_565 N
Dc1 Dc1 Dc2 117.2(13) 308_455 . 1_555 N
Dc1 Dc1 Dc2 41.9(6) 308_455 . 105_544 N
Dc1 Dc1 Dc2 128.41(34) 308_455 . -108_666 N
Dc1 Dc1 Od 155.8(28) 308_454 . 1_555 N
Dc1 Dc1 Od 61.3(16) 308_454 . 105_544 N
Dc1 Dc1 Od 97.1(11) 308_454 . -108_665 N
Dc1 Dc1 Od 15.6(9) 308_454 . 308_454 N
Dc1 Dc1 Dd1 110.4(28) 308_433 . 1_555 N
Dc1 Dc1 Dc2 174.0(13) -305_566 . 1_555 N
Dc1 Dc1 Dc2 101.8(6) -305_566 . 105_544 N
Dc1 Dc1 Dc2 68.5(4) -305_566 . -108_666 N
Dc1 Dc1 Od 109.6(30) -305_565 . 1_555 N
Dc1 Dc1 Od 117.7(16) -305_565 . 105_544 N
Dc1 Dc1 Od 39.4(11) -305_565 . -108_665 N
Dc1 Dc1 Od 74.4(9) -305_565 . 308_454 N
Dc1 Dc1 Dd1 93(4) -305_544 . 1_555 N
Dc2 Dc1 Dc2 75.3(7) 1_555 . 105_544 N
Dc2 Dc1 Dc2 113.7(10) 1_555 . -108_666 N
Dc2 Dc1 Od 75.0(30) 1_555 . 1_555 N
Dc2 Dc1 Od 57.9(17) 1_555 . 105_544 N
Dc2 Dc1 Od 140.7(17) 1_555 . -108_665 N
Dc2 Dc1 Od 103.5(13) 1_555 . 308_454 N
Dc2 Dc1 Dd1 93(4) 1_555 . 1_555 N
Dc2 Dc1 Dc2 168.7(7) 105_544 . -108_666 N
Dc2 Dc1 Od 142.0(30) 105_544 . 1_555 N
Dc2 Dc1 Od 24.0(14) 105_544 . 105_544 N
Dc2 Dc1 Od 136.4(12) 105_544 . -108_665 N
Dc2 Dc1 Od 28.8(9) 105_544 . 308_454 N
Dc2 Dc1 Dd1 112.8(34) 105_544 . 1_555 N
Dc2 Dc1 Od 49.3(29) -108_665 . 1_555 N
Dc2 Dc1 Od 156.3(18) -108_665 . 105_544 N
Dc2 Dc1 Od 32.4(10) -108_665 . -108_665 N
Dc2 Dc1 Od 142.8(9) -108_665 . 308_454 N
Dc2 Dc1 Dd1 74.6(34) -108_644 . 1_555 N
Od Dc1 Od 132.6(29) 1_555 . 105_544 N
Od Dc1 Od 81.0(25) 1_555 . -108_665 N
Od Dc1 Od 150.5(35) 1_555 . 308_454 N
Od Dc1 Dd1 46.1(24) 1_555 . 1_555 N
Od Dc1 Od 140.1(24) 105_544 . -108_665 N
Od Dc1 Od 51.2(11) 105_544 . 308_454 N
Od Dc1 Dd1 125(4) 105_544 . 1_555 N
Od Dc1 Od 112.5(10) -108_665 . 308_454 N
Od Dc1 Dd1 93(4) -108_644 . 1_555 N
Od Dc1 Dd1 105.4(32) 308_433 . 1_555 N
Si1 Dc2 Si2 65.82(35) -3_555 . 3_555 N
Si1 Dc2 Al1 65.82(35) -3_555 . 3_555 N
Si1 Dc2 O1 30.5(4) -3_555 . -3_555 N
Si1 Dc2 O3 68.3(4) -3_555 . 2_555 N
Si1 Dc2 O3 24.42(19) -3_555 . -1_555 N
Si1 Dc2 O4 32.25(22) -3_555 . -111_444 N
Si1 Dc2 O4 101.6(4) -3_555 . 312_334 N
Si1 Dc2 SJ 138.9(14) -3_555 . 1_555 N
Si1 Dc2 SJ 75.5(10) -3_555 . 105_544 N
Si1 Dc2 Oc 133.4(13) -3_555 . 1_555 N
Si1 Dc2 Oc 99.6(6) -3_555 . 105_544 N
Si1 Dc2 Oc 156.5(10) -3_555 . -108_656 N
Si1 Dc2 Dc1 165.2(12) -3_555 . 1_555 N
Si1 Dc2 Dc1 110.5(6) -3_555 . 105_544 N
Si1 Dc2 Dc1 168.8(9) -3_555 . -108_665 N
Si1 Dc2 Dc2 87.0(7) -3_555 . 105_544 N
Si1 Dc2 Dc2 151.7(8) -3_555 . -108_666 N
Si1 Dc2 Od 152.9(20) -3_555 . 1_555 N
Si1 Dc2 Od 85.8(17) -3_555 . 105_544 N
Si1 Dc2 Dd1 147.4(27) -3_555 . 1_555 N
Si1 Dc2 Dd1 96.9(20) -3_555 . 105_544 N
Si1 Dc2 Dd2 125.9(22) -3_555 . 1_555 N
Si1 Dc2 Dd2 60.0(18) -3_555 . 105_544 N
Si1 Dc2 DII*1 110.6(27) -3_555 . 312_333 N
Si2 Dc2 Al1 0.0 3_555 . 3_555 N
Si2 Dc2 O1 35.5(4) 3_555 . -3_555 N
Si2 Dc2 O3 21.00(24) 3_555 . 2_555 N
Si2 Dc2 O3 69.70(29) 3_555 . -1_555 N
Si2 Dc2 O4 97.7(5) 3_555 . -111_444 N
Si2 Dc2 O4 36.55(25) 3_555 . 312_334 N
Si2 Dc2 SJ 73.4(13) 3_555 . 1_555 N
Si2 Dc2 SJ 140.1(12) 3_555 . 105_544 N
Si2 Dc2 Oc 133.7(12) 3_555 . 1_555 N
Si2 Dc2 Oc 164.1(9) 3_555 . 105_544 N
Si2 Dc2 Oc 104.2(7) 3_555 . -108_656 N
Si2 Dc2 Dc1 128.9(13) 3_555 . 1_555 N
Si2 Dc2 Dc1 169.9(11) 3_555 . 105_544 N
Si2 Dc2 Dc1 116.0(8) 3_555 . -108_665 N
Si2 Dc2 Dc2 147.9(9) 3_555 . 105_544 N
Si2 Dc2 Dc2 90.1(7) 3_555 . -108_666 N
Si2 Dc2 Od 87.5(19) 3_555 . 1_555 N
Si2 Dc2 Od 151.7(18) 3_555 . 105_544 N
Si2 Dc2 Dd1 99.1(23) 3_555 . 1_555 N
Si2 Dc2 Dd1 155.3(21) 3_555 . 105_544 N
Si2 Dc2 Dd2 60.8(21) 3_555 . 1_555 N
Si2 Dc2 Dd2 125.2(18) 3_555 . 105_544 N
Si2 Dc2 DII*1 73.8(21) 3_555 . 312_333 N
Al1 Dc2 O1 35.5(4) 3_555 . -3_555 N
Al1 Dc2 O3 21.00(24) 3_555 . 2_555 N
Al1 Dc2 O3 69.70(29) 3_555 . -1_555 N
Al1 Dc2 O4 97.7(5) 3_555 . -111_444 N
Al1 Dc2 O4 36.55(25) 3_555 . 312_334 N
Al1 Dc2 SJ 73.4(13) 3_555 . 1_555 N
Al1 Dc2 SJ 140.1(12) 3_555 . 105_544 N
Al1 Dc2 Oc 133.7(12) 3_555 . 1_555 N
Al1 Dc2 Oc 164.1(9) 3_555 . 105_544 N
Al1 Dc2 Oc 104.2(7) 3_555 . -108_656 N
Al1 Dc2 Dc1 128.9(13) 3_555 . 1_555 N
Al1 Dc2 Dc1 169.9(11) 3_555 . 105_544 N
Al1 Dc2 Dc1 116.0(8) 3_555 . -108_665 N
Al1 Dc2 Dc2 147.9(9) 3_555 . 105_544 N
Al1 Dc2 Dc2 90.1(7) 3_555 . -108_666 N
Al1 Dc2 Od 87.5(19) 3_555 . 1_555 N
Al1 Dc2 Od 151.7(18) 3_555 . 105_544 N
Al1 Dc2 Dd1 99.1(23) 3_555 . 1_555 N
Al1 Dc2 Dd1 155.3(21) 3_555 . 105_544 N
Al1 Dc2 Dd2 60.8(21) 3_555 . 1_555 N
Al1 Dc2 Dd2 125.2(18) 3_555 . 105_544 N
Al1 Dc2 DII*1 73.8(21) 3_555 . 312_333 N
O1 Dc2 O3 42.8(5) -3_555 . 2_555 N
O1 Dc2 O3 37.8(4) -3_555 . -1_555 N
O1 Dc2 O4 62.7(5) -3_555 . -111_444 N
O1 Dc2 O4 71.1(6) -3_555 . 312_334 N
O1 Dc2 SJ 108.4(15) -3_555 . 1_555 N
O1 Dc2 SJ 105.9(12) -3_555 . 105_544 N
O1 Dc2 Oc 147.9(19) -3_555 . 1_555 N
O1 Dc2 Oc 130.1(9) -3_555 . 105_544 N
O1 Dc2 Oc 134.4(10) -3_555 . -108_656 N
O1 Dc2 Dc1 164.2(15) -3_555 . 1_555 N
O1 Dc2 Dc1 140.9(9) -3_555 . 105_544 N
O1 Dc2 Dc1 148.9(11) -3_555 . -108_665 N
O1 Dc2 Dc2 116.8(10) -3_555 . 105_544 N
O1 Dc2 Dc2 123.2(10) -3_555 . -108_666 N
O1 Dc2 Od 123.1(21) -3_555 . 1_555 N
O1 Dc2 Od 116.2(18) -3_555 . 105_544 N
O1 Dc2 Dd1 130.3(27) -3_555 . 1_555 N
O1 Dc2 Dd1 124.3(21) -3_555 . 105_544 N
O1 Dc2 Dd2 96.3(22) -3_555 . 1_555 N
O1 Dc2 Dd2 89.7(19) -3_555 . 105_544 N
O1 Dc2 DII*1 96.3(24) -3_555 . 312_333 N
O3 Dc2 O3 80.55(26) 2_555 . -1_555 N
O3 Dc2 O4 96.2(5) 2_555 . -111_444 N
O3 Dc2 O4 44.51(26) 2_555 . 312_334 N
O3 Dc2 SJ 75.6(13) 2_555 . 1_555 N
O3 Dc2 SJ 131.8(12) 2_555 . 105_544 N
O3 Dc2 Oc 115.8(12) 2_555 . 1_555 N
O3 Dc2 Oc 149.4(9) 2_555 . 105_544 N
O3 Dc2 Oc 110.5(6) 2_555 . -108_656 N
O3 Dc2 Dc1 124.5(13) 2_555 . 1_555 N
O3 Dc2 Dc1 149.4(10) 2_555 . 105_544 N
O3 Dc2 Dc1 117.7(6) 2_555 . -108_665 N
O3 Dc2 Dc2 133.5(10) 2_555 . 105_544 N
O3 Dc2 Dc2 94.7(6) 2_555 . -108_666 N
O3 Dc2 Od 85.0(19) 2_555 . 1_555 N
O3 Dc2 Od 146.0(19) 2_555 . 105_544 N
O3 Dc2 Dd1 87.5(25) 2_555 . 1_555 N
O3 Dc2 Dd1 164.7(20) 2_555 . 105_544 N
O3 Dc2 Dd2 58.9(23) 2_555 . 1_555 N
O3 Dc2 Dd2 126.4(20) 2_555 . 105_544 N
O3 Dc2 DII*1 56.0(21) 2_555 . 312_333 N
O3 Dc2 O4 41.52(20) -1_555 . -111_444 N
O3 Dc2 O4 99.17(35) -1_555 . 312_334 N
O3 Dc2 SJ 132.0(15) -1_555 . 1_555 N
O3 Dc2 SJ 79.2(10) -1_555 . 105_544 N
O3 Dc2 Oc 148.0(8) -1_555 . 1_555 N
O3 Dc2 Oc 99.8(5) -1_555 . 105_544 N
O3 Dc2 Oc 133.3(9) -1_555 . -108_656 N
O3 Dc2 Dc1 151.9(15) -1_555 . 1_555 N
O3 Dc2 Dc1 111.2(6) -1_555 . 105_544 N
O3 Dc2 Dc1 144.4(8) -1_555 . -108_665 N
O3 Dc2 Dc2 92.9(6) -1_555 . 105_544 N
O3 Dc2 Dc2 134.8(10) -1_555 . -108_666 N
O3 Dc2 Od 149.3(21) -1_555 . 1_555 N
O3 Dc2 Od 84.5(16) -1_555 . 105_544 N
O3 Dc2 Dd1 168.1(26) -1_555 . 1_555 N
O3 Dc2 Dd1 87.3(20) -1_555 . 105_544 N
O3 Dc2 Dd2 127.9(20) -1_555 . 1_555 N
O3 Dc2 Dd2 57.9(18) -1_555 . 105_544 N
O3 Dc2 DII*1 132.0(25) -1_555 . 312_333 N
O4 Dc2 O4 133.9(5) -111_444 . 312_334 N
O4 Dc2 SJ 171.1(14) -111_556 . 1_555 N
O4 Dc2 SJ 43.2(9) -111_556 . 105_544 N
O4 Dc2 Oc 107.1(9) -111_556 . 1_555 N
O4 Dc2 Oc 67.4(5) -111_556 . 105_544 N
O4 Dc2 Oc 152.1(9) -111_556 . -108_656 N
O4 Dc2 Dc1 133.0(11) -111_565 . 1_555 N
O4 Dc2 Dc1 78.2(5) -111_565 . 105_544 N
O4 Dc2 Dc1 145.6(5) -111_565 . -108_665 N
O4 Dc2 Dc2 55.1(5) -111_566 . 105_544 N
O4 Dc2 Dc2 167.2(11) -111_566 . -108_666 N
O4 Dc2 Od 168.5(22) -111_565 . 1_555 N
O4 Dc2 Od 54.1(16) -111_565 . 105_544 N
O4 Dc2 Dd1 141.0(22) -111_544 . 1_555 N
O4 Dc2 Dd1 68.5(19) -111_544 . 105_544 N
O4 Dc2 Dd2 154.7(26) -111_544 . 1_555 N
O4 Dc2 Dd2 30.3(19) -111_544 . 105_544 N
O4 Dc2 DII*1 118.1(28) -111_443 . 312_333 N
O4 Dc2 SJ 37.3(12) 312_446 . 1_555 N
O4 Dc2 SJ 176.3(13) 312_446 . 105_544 N
O4 Dc2 Oc 111.7(7) 312_446 . 1_555 N
O4 Dc2 Oc 158.8(6) 312_446 . 105_544 N
O4 Dc2 Oc 68.2(5) 312_446 . -108_656 N
O4 Dc2 Dc1 93.1(11) 312_455 . 1_555 N
O4 Dc2 Dc1 147.8(5) 312_455 . 105_544 N
O4 Dc2 Dc1 79.5(6) 312_455 . -108_665 N
O4 Dc2 Dc2 166.7(9) 312_456 . 105_544 N
O4 Dc2 Dc2 53.6(5) 312_456 . -108_666 N
O4 Dc2 Od 53.0(19) 312_455 . 1_555 N
O4 Dc2 Od 169.5(20) 312_455 . 105_544 N
O4 Dc2 Dd1 72.1(20) 312_434 . 1_555 N
O4 Dc2 Dd1 148.3(20) 312_434 . 105_544 N
O4 Dc2 Dd2 28.9(20) 312_434 . 1_555 N
O4 Dc2 Dd2 156.6(21) 312_434 . 105_544 N
O4 Dc2 DII*1 65.2(22) 312_333 . 312_333 N
SJ Dc2 SJ 145.5(20) 1_555 . 105_544 N
SJ Dc2 Oc 79.9(14) 1_555 . 1_555 N
SJ Dc2 Oc 121.5(12) 1_555 . 105_544 N
SJ Dc2 Oc 35.2(12) 1_555 . -108_656 N
SJ Dc2 Dc1 55.8(15) 1_555 . 1_555 N
SJ Dc2 Dc1 110.6(12) 1_555 . 105_544 N
SJ Dc2 Dc1 43.2(13) 1_555 . -108_665 N
SJ Dc2 Dc2 133.3(13) 1_555 . 105_544 N
SJ Dc2 Dc2 19.5(12) 1_555 . -108_666 N
SJ Dc2 Od 17.4(23) 1_555 . 1_555 N
SJ Dc2 Od 134.8(21) 1_555 . 105_544 N
SJ Dc2 Dd1 43.5(23) 1_555 . 1_555 N
SJ Dc2 Dd1 119.7(24) 1_555 . 105_544 N
SJ Dc2 Dd2 18.2(28) 1_555 . 1_555 N
SJ Dc2 Dd2 157.6(26) 1_555 . 105_544 N
SJ Dc2 DII*1 60.2(29) 1_555 . 312_333 N
SJ Dc2 Oc 69.5(10) 105_544 . 1_555 N
SJ Dc2 Oc 24.3(9) 105_544 . 105_544 N
SJ Dc2 Oc 115.3(10) 105_544 . -108_656 N
SJ Dc2 Dc1 89.8(12) 105_544 . 1_555 N
SJ Dc2 Dc1 35.0(10) 105_544 . 105_544 N
SJ Dc2 Dc1 103.8(9) 105_544 . -108_665 N
SJ Dc2 Dc2 13.8(9) 105_544 . 105_544 N
SJ Dc2 Dc2 129.7(9) 105_544 . -108_666 N
SJ Dc2 Od 129.4(21) 105_544 . 1_555 N
SJ Dc2 Od 14.2(19) 105_544 . 105_544 N
SJ Dc2 Dd1 108.9(22) 105_544 . 1_555 N
SJ Dc2 Dd1 35.3(20) 105_544 . 105_544 N
SJ Dc2 Dd2 152.3(23) 105_544 . 1_555 N
SJ Dc2 Dd2 22.8(22) 105_544 . 105_544 N
SJ Dc2 DII*1 113.4(25) 105_544 . 312_333 N
Oc Dc2 Oc 51.7(7) 1_555 . 105_544 N
Oc Dc2 Oc 69.3(10) 1_555 . -108_656 N
Oc Dc2 Dc1 37.73450(10) 1_555 . 1_555 N
Oc Dc2 Dc1 41.4(9) 1_555 . 105_544 N
Oc Dc2 Dc1 54.3(10) 1_555 . -108_665 N
Oc Dc2 Dc2 55.6(6) 1_555 . 105_544 N
Oc Dc2 Dc2 73.9(6) 1_555 . -108_666 N
Oc Dc2 Od 62.5(20) 1_555 . 1_555 N
Oc Dc2 Od 66.6(16) 1_555 . 105_544 N
Oc Dc2 Dd1 39.6(20) 1_555 . 1_555 N
Oc Dc2 Dd1 70.9(21) 1_555 . 105_544 N
Oc Dc2 Dd2 82.9(21) 1_555 . 1_555 N
Oc Dc2 Dd2 91.7(20) 1_555 . 105_544 N
Oc Dc2 DII*1 60.2(22) 1_555 . 312_333 N
Oc Dc2 Oc 91.7(5) 105_544 . -108_656 N
Oc Dc2 Dc1 65.7(9) 105_544 . 1_555 N
Oc Dc2 Dc1 11.45(33) 105_544 . 105_544 N
Oc Dc2 Dc1 79.56(22) 105_544 . -108_665 N
Oc Dc2 Dc2 16.70(7) 105_544 . 105_544 N
Oc Dc2 Dc2 105.57(27) 105_544 . -108_666 N
Oc Dc2 Od 106.2(19) 105_544 . 1_555 N
Oc Dc2 Od 15.3(15) 105_544 . 105_544 N
Oc Dc2 Dd1 90.3(21) 105_544 . 1_555 N
Oc Dc2 Dd1 24.9(17) 105_544 . 105_544 N
Oc Dc2 Dd2 131.9(20) 105_544 . 1_555 N
Oc Dc2 Dd2 42.1(18) 105_544 . 105_544 N
Oc Dc2 DII*1 107.7(21) 105_544 . 312_333 N
Oc Dc2 Dc1 32.6(10) -108_665 . 1_555 N
Oc Dc2 Dc1 82.67(30) -108_665 . 105_544 N
Oc Dc2 Dc1 15.25(24) -108_665 . -108_665 N
Oc Dc2 Dc2 107.23(35) -108_666 . 105_544 N
Oc Dc2 Dc2 15.80(9) -108_666 . -108_666 N
Oc Dc2 Od 32.1(18) -108_665 . 1_555 N
Oc Dc2 Od 102.0(17) -108_665 . 105_544 N
Oc Dc2 Dd1 51.9(23) -108_644 . 1_555 N
Oc Dc2 Dd1 84.7(19) -108_644 . 105_544 N
Oc Dc2 Dd2 53.1(25) -108_644 . 1_555 N
Oc Dc2 Dd2 122.4(21) -108_644 . 105_544 N
Oc Dc2 DII*1 85.0(27) -108_543 . 312_333 N
Dc1 Dc2 Dc1 54.8(11) 1_555 . 105_544 N
Dc1 Dc2 Dc1 17.3(8) 1_555 . -108_665 N
Dc1 Dc2 Dc2 78.6(8) 1_555 . 105_544 N
Dc1 Dc2 Dc2 41.7(8) 1_555 . -108_666 N
Dc1 Dc2 Od 41.5(19) 1_555 . 1_555 N
Dc1 Dc2 Od 79.5(19) 1_555 . 105_544 N
Dc1 Dc2 Dd1 39.3(26) 1_555 . 1_555 N
Dc1 Dc2 Dd1 69.6(23) 1_555 . 105_544 N
Dc1 Dc2 Dd2 68.4(22) 1_555 . 1_555 N
Dc1 Dc2 Dd2 105.6(21) 1_555 . 105_544 N
Dc1 Dc2 DII*1 76.1(26) 1_555 . 312_333 N
Dc1 Dc2 Dc1 69.6(4) 105_544 . -108_665 N
Dc1 Dc2 Dc2 24.58(25) 105_544 . 105_544 N
Dc1 Dc2 Dc2 95.63(25) 105_544 . -108_666 N
Dc1 Dc2 Od 94.9(19) 105_544 . 1_555 N
Dc1 Dc2 Od 26.6(15) 105_544 . 105_544 N
Dc1 Dc2 Dd1 79.1(22) 105_544 . 1_555 N
Dc1 Dc2 Dd1 30.9(19) 105_544 . 105_544 N
Dc1 Dc2 Dd2 120.5(20) 105_544 . 1_555 N
Dc1 Dc2 Dd2 53.6(18) 105_544 . 105_544 N
Dc1 Dc2 DII*1 99.8(21) 105_544 . 312_333 N
Dc1 Dc2 Dc2 94.04(13) -108_666 . 105_544 N
Dc1 Dc2 Dc2 26.06(14) -108_666 . -108_666 N
Dc1 Dc2 Od 33.1(19) -108_665 . 1_555 N
Dc1 Dc2 Od 91.8(16) -108_665 . 105_544 N
Dc1 Dc2 Dd1 43.7(25) -108_644 . 1_555 N
Dc1 Dc2 Dd1 77.5(19) -108_644 . 105_544 N
Dc1 Dc2 Dd2 58.9(23) -108_644 . 1_555 N
Dc1 Dc2 Dd2 115.6(18) -108_644 . 105_544 N
Dc1 Dc2 DII*1 80.1(26) -108_543 . 312_333 N
Dc2 Dc2 Dc2 120.0000(8) 105_544 . -108_666 N
Dc2 Dc2 Od 116.4(19) 105_544 . 1_555 N
Dc2 Dc2 Od 17.7(15) 105_544 . 105_544 N
Dc2 Dc2 Dd1 95.1(20) 105_544 . 1_555 N
Dc2 Dc2 Dd1 37.3(17) 105_544 . 105_544 N
Dc2 Dc2 Dd2 138.4(21) 105_544 . 1_555 N
Dc2 Dc2 Dd2 36.5(20) 105_544 . 105_544 N
Dc2 Dc2 DII*1 102.4(23) 105_544 . 312_333 N
Dc2 Dc2 Od 20.6(18) -108_665 . 1_555 N
Dc2 Dc2 Od 117.1(17) -108_665 . 105_544 N
Dc2 Dc2 Dd1 46.3(20) -108_644 . 1_555 N
Dc2 Dc2 Dd1 100.5(19) -108_644 . 105_544 N
Dc2 Dc2 Dd2 37.4(25) -108_644 . 1_555 N
Dc2 Dc2 Dd2 138.2(22) -108_644 . 105_544 N
Dc2 Dc2 DII*1 73.8(27) -108_543 . 312_333 N
Od Dc2 Od 120.7(34) 1_555 . 105_544 N
Od Dc2 Dd1 27.6(15) 1_555 . 1_555 N
Od Dc2 Dd1 110.0(32) 1_555 . 105_544 N
Od Dc2 Dd2 27.0(17) 1_555 . 1_555 N
Od Dc2 Dd2 147.1(32) 1_555 . 105_544 N
Od Dc2 DII*1 53.6(32) 1_555 . 312_333 N
Od Dc2 Dd1 105.5(31) 105_544 . 1_555 N
Od Dc2 Dd1 21.4(14) 105_544 . 105_544 N
Od Dc2 Dd2 147.0(31) 105_544 . 1_555 N
Od Dc2 Dd2 27.0(14) 105_544 . 105_544 N
Od Dc2 DII*1 119.3(26) 105_544 . 312_333 N
Dd1 Dc2 Dd1 104(4) 1_555 . 105_544 N
Dd1 Dc2 Dd2 43.4(12) 1_555 . 1_555 N
Dd1 Dc2 Dd2 131.3(31) 1_555 . 105_544 N
Dd1 Dc2 DII*1 37.2(35) 1_555 . 312_333 N
Dd1 Dc2 Dd2 136.4(30) 105_544 . 1_555 N
Dd1 Dc2 Dd2 38.2(11) 105_544 . 105_544 N
Dd1 Dc2 DII*1 130.6(28) 105_544 . 312_333 N
Dd2 Dc2 Dd2 174.0(27) 1_555 . 105_544 N
Dd2 Dc2 DII*1 46(4) 1_555 . 312_333 N
Dd2 Dc2 DII*1 132.5(35) 105_544 . 312_333 N
Si1 Od Si2 59.2(9) 111_533 . 3_555 N
Si1 Od Al1 59.2(9) 111_443 . 3_555 N
Si1 Od O1 88.0(14) 111_433 . -3_555 N
Si1 Od O1 29.0(5) 111_433 . 111_433 N
Si1 Od O4 25.4(7) 111_433 . 312_334 N
Si1 Od SJ 56(7) 111_545 . 1_555 N
Si1 Od SJ 143.1(18) 111_545 . 105_544 N
Si1 Od SJ 78.9(14) 111_545 . -108_656 N
Si1 Od Oc 149.5(29) 111_545 . 1_555 N
Si1 Od Oc 160.2(16) 111_545 . 105_544 N
Si1 Od Oc 84.3(21) 111_545 . -108_656 N
Si1 Od Oc 105.3(15) 111_545 . -305_556 N
Si1 Od Dc1 154(4) 111_554 . 1_555 N
Si1 Od Dc1 162.6(19) 111_554 . 105_544 N
Si1 Od Dc1 102.2(20) 111_554 . -108_665 N
Si1 Od Dc1 118.1(16) 111_554 . -305_565 N
Si1 Od Dc2 115.3(25) 111_555 . 1_555 N
Si1 Od Dc2 59.6(15) 111_555 . -108_666 N
Si1 Od Od 143.8(23) 111_554 . 105_544 N
Si1 Od Od 86.7(19) 111_554 . -108_665 N
Si1 Od Dd1 127(4) 111_533 . 1_555 N
Si1 Od Dd1 140.0(26) 111_533 . 105_544 N
Si1 Od Dd1 93.9(22) 111_533 . -108_644 N
Si1 Od Dd2 33(5) 111_533 . 1_555 N
Si2 Od Al1 0.0 3_555 . 3_555 N
Si2 Od O1 31.4(6) 3_555 . -3_555 N
Si2 Od O1 87.4(14) 3_555 . 111_433 N
Si2 Od O4 33.9(7) 3_555 . 312_334 N
Si2 Od SJ 31(6) 3_555 . 1_555 N
Si2 Od SJ 88.3(15) 3_555 . 105_544 N
Si2 Od SJ 135.5(19) 3_555 . -108_656 N
Si2 Od Oc 90.8(24) 3_555 . 1_555 N
Si2 Od Oc 111.2(15) 3_555 . 105_544 N
Si2 Od Oc 129.6(26) 3_555 . -108_656 N
Si2 Od Oc 164.5(19) 3_555 . -305_556 N
Si2 Od Dc1 124(4) 3_555 . 1_555 N
Si2 Od Dc1 113.1(18) 3_555 . 105_544 N
Si2 Od Dc1 154.5(24) 3_555 . -108_665 N
Si2 Od Dc1 173.1(17) 3_555 . -305_565 N
Si2 Od Dc2 61.1(17) 3_555 . 1_555 N
Si2 Od Dc2 116.4(24) 3_555 . -108_666 N
Si2 Od Od 93.1(20) 3_555 . 105_544 N
Si2 Od Od 140.6(23) 3_555 . -108_665 N
Si2 Od Dd1 117(5) 3_555 . 1_555 N
Si2 Od Dd1 102.1(21) 3_555 . 105_544 N
Si2 Od Dd1 136.0(28) 3_555 . -108_644 N
Si2 Od Dd2 42(5) 3_555 . 1_555 N
Al1 Od O1 31.4(6) 3_555 . -3_555 N
Al1 Od O1 87.4(14) 3_555 . 111_433 N
Al1 Od O4 33.9(7) 3_555 . 312_334 N
Al1 Od SJ 31(6) 3_555 . 1_555 N
Al1 Od SJ 88.3(15) 3_555 . 105_544 N
Al1 Od SJ 135.5(19) 3_555 . -108_656 N
Al1 Od Oc 90.8(24) 3_555 . 1_555 N
Al1 Od Oc 111.2(15) 3_555 . 105_544 N
Al1 Od Oc 129.6(26) 3_555 . -108_656 N
Al1 Od Oc 164.5(19) 3_555 . -305_556 N
Al1 Od Dc1 124(4) 3_555 . 1_555 N
Al1 Od Dc1 113.1(18) 3_555 . 105_544 N
Al1 Od Dc1 154.5(24) 3_555 . -108_665 N
Al1 Od Dc1 173.1(17) 3_555 . -305_565 N
Al1 Od Dc2 61.1(17) 3_555 . 1_555 N
Al1 Od Dc2 116.4(24) 3_555 . -108_666 N
Al1 Od Od 93.1(20) 3_555 . 105_544 N
Al1 Od Od 140.6(23) 3_555 . -108_665 N
Al1 Od Dd1 117(5) 3_555 . 1_555 N
Al1 Od Dd1 102.1(21) 3_555 . 105_544 N
Al1 Od Dd1 136.0(28) 3_555 . -108_644 N
Al1 Od Dd2 42(5) 3_555 . 1_555 N
O1 Od O1 113.4(17) -3_555 . 111_433 N
O1 Od O4 63.8(13) -3_555 . 312_334 N
O1 Od SJ 39(7) -3_555 . 1_555 N
O1 Od SJ 57.2(11) -3_555 . 105_544 N
O1 Od SJ 148.5(19) -3_555 . -108_656 N
O1 Od Oc 61.5(19) -3_555 . 1_555 N
O1 Od Oc 80.0(12) -3_555 . 105_544 N
O1 Od Oc 130.0(25) -3_555 . -108_656 N
O1 Od Oc 160.8(17) -3_555 . -305_556 N
O1 Od Dc1 93.1(31) -3_555 . 1_555 N
O1 Od Dc1 82.0(15) -3_555 . 105_544 N
O1 Od Dc1 146.6(22) -3_555 . -108_665 N
O1 Od Dc1 147.4(17) -3_555 . -305_565 N
O1 Od Dc2 29.7(12) -3_555 . 1_555 N
O1 Od Dc2 136.0(26) -3_555 . -108_666 N
O1 Od Od 61.7(18) -3_555 . 105_544 N
O1 Od Od 145.7(27) -3_555 . -108_665 N
O1 Od Dd1 111(5) -3_555 . 1_555 N
O1 Od Dd1 71.5(18) -3_555 . 105_544 N
O1 Od Dd1 129.9(25) -3_555 . -108_644 N
O1 Od Dd2 73(5) -3_555 . 1_555 N
O1 Od O4 54.1(12) 111_433 . 312_334 N
O1 Od SJ 76(8) 111_545 . 1_555 N
O1 Od SJ 154.2(18) 111_545 . 105_544 N
O1 Od SJ 50.0(10) 111_545 . -108_656 N
O1 Od Oc 167.0(29) 111_545 . 1_555 N
O1 Od Oc 148.3(15) 111_545 . 105_544 N
O1 Od Oc 57.7(16) 111_545 . -108_656 N
O1 Od Oc 77.1(12) 111_545 . -305_556 N
O1 Od Dc1 133(4) 111_554 . 1_555 N
O1 Od Dc1 148.6(18) 111_554 . 105_544 N
O1 Od Dc1 73.3(16) 111_554 . -108_665 N
O1 Od Dc1 89.3(13) 111_554 . -305_565 N
O1 Od Dc2 135.2(27) 111_555 . 1_555 N
O1 Od Dc2 30.7(11) 111_555 . -108_666 N
O1 Od Od 148.4(26) 111_554 . 105_544 N
O1 Od Od 57.9(17) 111_554 . -108_665 N
O1 Od Dd1 123(4) 111_533 . 1_555 N
O1 Od Dd1 134.0(24) 111_533 . 105_544 N
O1 Od Dd1 67.2(19) 111_533 . -108_644 N
O1 Od Dd2 59(6) 111_533 . 1_555 N
O4 Od SJ 39(6) 312_446 . 1_555 N
O4 Od SJ 120.7(21) 312_446 . 105_544 N
O4 Od SJ 103.7(20) 312_446 . -108_656 N
O4 Od Oc 124.6(31) 312_446 . 1_555 N
O4 Od Oc 142.9(21) 312_446 . 105_544 N
O4 Od Oc 105.5(26) 312_446 . -108_656 N
O4 Od Oc 130.6(21) 312_446 . -305_556 N
O4 Od Dc1 151(4) 312_455 . 1_555 N
O4 Od Dc1 145.2(23) 312_455 . 105_544 N
O4 Od Dc1 126.5(26) 312_455 . -108_665 N
O4 Od Dc1 143.4(22) 312_455 . -305_565 N
O4 Od Dc2 92.6(24) 312_456 . 1_555 N
O4 Od Dc2 84.2(22) 312_456 . -108_666 N
O4 Od Od 124.1(25) 312_455 . 105_544 N
O4 Od Od 110.9(25) 312_455 . -108_665 N
O4 Od Dd1 127(5) 312_434 . 1_555 N
O4 Od Dd1 128.1(27) 312_434 . 105_544 N
O4 Od Dd1 114.7(28) 312_434 . -108_644 N
O4 Od Dd2 23(5) 312_434 . 1_555 N
SJ Od SJ 87(7) 1_555 . 105_544 N
SJ Od SJ 113(8) 1_555 . -108_656 N
SJ Od Oc 96(8) 1_555 . 1_555 N
SJ Od Oc 106(8) 1_555 . 105_544 N
SJ Od Oc 101(8) 1_555 . -108_656 N
SJ Od Oc 142(8) 1_555 . -305_556 N
SJ Od Dc1 112(8) 1_555 . 1_555 N
SJ Od Dc1 109(8) 1_555 . 105_544 N
SJ Od Dc1 126(8) 1_555 . -108_665 N
SJ Od Dc1 143(7) 1_555 . -305_565 N
SJ Od Dc2 60(7) 1_555 . 1_555 N
SJ Od Dc2 98(8) 1_555 . -108_666 N
SJ Od Od 88(8) 1_555 . 105_544 N
SJ Od Od 115(9) 1_555 . -108_665 N
SJ Od Dd1 146(9) 1_555 . 1_555 N
SJ Od Dd1 90(8) 1_555 . 105_544 N
SJ Od Dd1 106(8) 1_555 . -108_644 N
SJ Od Dd2 59(8) 1_555 . 1_555 N
SJ Od SJ 123.7(18) 105_544 . -108_656 N
SJ Od Oc 12.8(13) 105_544 . 1_555 N
SJ Od Oc 23.0(7) 105_544 . 105_544 N
SJ Od Oc 107.7(21) 105_544 . -108_656 N
SJ Od Oc 106.2(15) 105_544 . -305_556 N
SJ Od Dc1 37.9(24) 105_544 . 1_555 N
SJ Od Dc1 24.8(8) 105_544 . 105_544 N
SJ Od Dc1 101.8(19) 105_544 . -108_665 N
SJ Od Dc1 92.1(13) 105_544 . -305_565 N
SJ Od Dc2 28.2(13) 105_544 . 1_555 N
SJ Od Dc2 137.8(22) 105_544 . -108_666 N
SJ Od Od 7.9(12) 105_544 . 105_544 N
SJ Od Od 114.4(14) 105_544 . -108_665 N
SJ Od Dd1 81(4) 105_544 . 1_555 N
SJ Od Dd1 24.2(12) 105_544 . 105_544 N
SJ Od Dd1 99.5(15) 105_544 . -108_644 N
SJ Od Dd2 128(5) 105_544 . 1_555 N
SJ Od Oc 127.5(27) -108_656 . 1_555 N
SJ Od Oc 103.4(14) -108_656 . 105_544 N
SJ Od Oc 21.2(13) -108_656 . -108_656 N
SJ Od Oc 30.2(8) -108_656 . -305_556 N
SJ Od Dc1 87.0(30) -108_665 . 1_555 N
SJ Od Dc1 102.5(16) -108_665 . 105_544 N
SJ Od Dc1 23.5(10) -108_665 . -108_665 N
SJ Od Dc1 40.0(8) -108_665 . -305_565 N
SJ Od Dc2 138.9(26) -108_666 . 1_555 N
SJ Od Dc2 19.5(10) -108_666 . -108_666 N
SJ Od Od 116.2(16) -108_665 . 105_544 N
SJ Od Od 9.3(12) -108_665 . -108_665 N
SJ Od Dd1 100(5) -108_644 . 1_555 N
SJ Od Dd1 100.8(15) -108_644 . 105_544 N
SJ Od Dd1 26.0(12) -108_644 . -108_644 N
SJ Od Dd2 107(5) -108_644 . 1_555 N
Oc Od Oc 24.3(14) 1_555 . 105_544 N
Oc Od Oc 115.1(30) 1_555 . -108_656 N
Oc Od Oc 104.6(24) 1_555 . -305_556 N
Oc Od Dc1 40.8(19) 1_555 . 1_555 N
Oc Od Dc1 25.1(13) 1_555 . 105_544 N
Oc Od Dc1 104.2(27) 1_555 . -108_665 N
Oc Od Dc1 91.1(22) 1_555 . -305_565 N
Oc Od Dc2 35.5(13) 1_555 . 1_555 N
Oc Od Dc2 144.8(33) 1_555 . -108_666 N
Oc Od Od 18.9(8) 1_555 . 105_544 N
Oc Od Od 118.6(20) 1_555 . -108_665 N
Oc Od Dd1 69(5) 1_555 . 1_555 N
Oc Od Dd1 34.2(14) 1_555 . 105_544 N
Oc Od Dd1 106.1(23) 1_555 . -108_644 N
Oc Od Dd2 125(5) 1_555 . 1_555 N
Oc Od Oc 91.3(19) 105_544 . -108_656 N
Oc Od Oc 83.2(10) 105_544 . -305_556 N
Oc Od Dc1 16.5(23) 105_544 . 1_555 N
Oc Od Dc1 2.5(5) 105_544 . 105_544 N
Oc Od Dc1 80.3(15) 105_544 . -108_665 N
Oc Od Dc1 69.2(9) 105_544 . -305_565 N
Oc Od Dc2 50.6(15) 105_544 . 1_555 N
Oc Od Dc2 120.5(20) 105_544 . -108_666 N
Oc Od Od 18.8(7) 105_544 . 105_544 N
Oc Od Od 94.3(9) 105_544 . -108_665 N
Oc Od Dd1 72(4) 105_544 . 1_555 N
Oc Od Dd1 20.3(13) 105_544 . 105_544 N
Oc Od Dd1 82.0(14) 105_544 . -108_644 N
Oc Od Dd2 150(5) 105_544 . 1_555 N
Oc Od Oc 41.0(14) -108_656 . -305_556 N
Oc Od Dc1 75.2(28) -108_665 . 1_555 N
Oc Od Dc1 91.2(20) -108_665 . 105_544 N
Oc Od Dc1 24.9(9) -108_665 . -108_665 N
Oc Od Dc1 43.9(14) -108_665 . -305_565 N
Oc Od Dc2 118.1(29) -108_666 . 1_555 N
Oc Od Dc2 30.2(9) -108_666 . -108_666 N
Oc Od Od 99.8(22) -108_665 . 105_544 N
Oc Od Od 15.7(13) -108_665 . -108_665 N
Oc Od Dd1 113(6) -108_644 . 1_555 N
Oc Od Dd1 83.6(20) -108_644 . 105_544 N
Oc Od Dd1 9.6(19) -108_644 . -108_644 N
Oc Od Dd2 117(6) -108_644 . 1_555 N
Oc Od Dc1 68.9(27) -305_565 . 1_555 N
Oc Od Dc1 81.5(12) -305_565 . 105_544 N
Oc Od Dc1 17.9(10) -305_565 . -108_665 N
Oc Od Dc1 14.12(21) -305_565 . -305_565 N
Oc Od Dc2 132.1(24) -305_566 . 1_555 N
Oc Od Dc2 48.6(13) -305_566 . -108_666 N
Oc Od Od 100.7(8) -305_565 . 105_544 N
Oc Od Od 27.1(8) -305_565 . -108_665 N
Oc Od Dd1 72(5) -305_544 . 1_555 N
Oc Od Dd1 89.6(12) -305_544 . 105_544 N
Oc Od Dd1 37.3(14) -305_544 . -108_644 N
Oc Od Dd2 125(5) -305_544 . 1_555 N
Dc1 Od Dc1 16.1(22) 1_555 . 105_544 N
Dc1 Od Dc1 64.2(25) 1_555 . -108_665 N
Dc1 Od Dc1 54.8(25) 1_555 . -305_565 N
Dc1 Od Dc2 63.5(26) 1_555 . 1_555 N
Dc1 Od Dc2 104.1(35) 1_555 . -108_666 N
Dc1 Od Od 31.8(21) 1_555 . 105_544 N
Dc1 Od Od 77.8(23) 1_555 . -108_665 N
Dc1 Od Dd1 76(6) 1_555 . 1_555 N
Dc1 Od Dd1 23.3(23) 1_555 . 105_544 N
Dc1 Od Dd1 65.8(26) 1_555 . -108_644 N
Dc1 Od Dd2 165(6) 1_555 . 1_555 N
Dc1 Od Dc1 79.3(17) 105_544 . -108_665 N
Dc1 Od Dc1 67.5(10) 105_544 . -305_565 N
Dc1 Od Dc2 52.7(16) 105_544 . 1_555 N
Dc1 Od Dc2 120.1(22) 105_544 . -108_666 N
Dc1 Od Od 21.1(7) 105_544 . 105_544 N
Dc1 Od Od 93.5(10) 105_544 . -108_665 N
Dc1 Od Dd1 70(4) 105_544 . 1_555 N
Dc1 Od Dd1 22.6(12) 105_544 . 105_544 N
Dc1 Od Dd1 81.8(15) 105_544 . -108_644 N
Dc1 Od Dd2 150(5) 105_544 . 1_555 N
Dc1 Od Dc1 19.2(9) -108_665 . -305_565 N
Dc1 Od Dc2 123.0(29) -108_666 . 1_555 N
Dc1 Od Dc2 42.6(12) -108_666 . -108_666 N
Dc1 Od Od 94.9(14) -108_665 . 105_544 N
Dc1 Od Od 15.6(10) -108_665 . -108_665 N
Dc1 Od Dd1 88(5) -108_644 . 1_555 N
Dc1 Od Dd1 80.9(15) -108_644 . 105_544 N
Dc1 Od Dd1 19.7(14) -108_644 . -108_644 N
Dc1 Od Dd2 130(6) -108_644 . 1_555 N
Dc1 Od Dc2 118.1(23) -305_566 . 1_555 N
Dc1 Od Dc2 59.4(14) -305_566 . -108_666 N
Dc1 Od Od 86.6(6) -305_565 . 105_544 N
Dc1 Od Od 33.9(6) -305_565 . -108_665 N
Dc1 Od Dd1 70(5) -305_544 . 1_555 N
Dc1 Od Dd1 75.9(11) -305_544 . 105_544 N
Dc1 Od Dd1 37.2(16) -305_544 . -108_644 N
Dc1 Od Dd2 140(5) -305_544 . 1_555 N
Dc2 Od Dc2 141.7(31) 1_555 . -108_666 N
Dc2 Od Od 32.0(22) 1_555 . 105_544 N
Dc2 Od Od 130.7(29) 1_555 . -108_665 N
Dc2 Od Dd1 100(5) 1_555 . 1_555 N
Dc2 Od Dd1 42.8(21) 1_555 . 105_544 N
Dc2 Od Dd1 113.1(27) 1_555 . -108_644 N
Dc2 Od Dd2 102(5) 1_555 . 1_555 N
Dc2 Od Od 129.9(25) -108_665 . 105_544 N
Dc2 Od Od 27.3(18) -108_665 . -108_665 N
Dc2 Od Dd1 112(5) -108_644 . 1_555 N
Dc2 Od Dd1 113.6(23) -108_644 . 105_544 N
Dc2 Od Dd1 38.8(18) -108_644 . -108_644 N
Dc2 Od Dd2 89(6) -108_644 . 1_555 N
Od Od Od 106.9(19) 105_544 . -108_665 N
Od Od Dd1 85(4) 105_544 . 1_555 N
Od Od Dd1 16.4(7) 105_544 . 105_544 N
Od Od Dd1 91.7(21) 105_544 . -108_644 N
Od Od Dd2 134(5) 105_544 . 1_555 N
Od Od Dd1 99(5) -108_644 . 1_555 N
Od Od Dd1 91.5(19) -108_644 . 105_544 N
Od Od Dd1 17.7(5) -108_644 . -108_644 N
Od Od Dd2 116(5) -108_644 . 1_555 N
Dd1 Od Dd1 93(5) 1_555 . 105_544 N
Dd1 Od Dd1 107(7) 1_555 . -108_644 N
Dd1 Od Dd2 104.4932(7) 1_555 . 1_555 N
Dd1 Od Dd1 75.7(22) 105_544 . -108_644 N
Dd1 Od Dd2 144(5) 105_544 . 1_555 N
Dd1 Od Dd2 126(6) -108_644 . 1_555 N
Si1 Dd1 Si2 49.2(8) 111_533 . 3_555 N
Si1 Dd1 Al1 49.2(8) 111_443 . 3_555 N
Si1 Dd1 O1 72.2(11) 111_433 . -3_555 N
Si1 Dd1 O1 24.0(4) 111_433 . 111_433 N
Si1 Dd1 O4 20.7(6) 111_433 . 312_334 N
Si1 Dd1 SJ 41.5(29) 111_545 . 1_555 N
Si1 Dd1 SJ 119.4(17) 111_545 . 105_544 N
Si1 Dd1 SJ 66.8(12) 111_545 . -108_656 N
Si1 Dd1 Oc 109.1(26) 111_545 . 1_555 N
Si1 Dd1 Oc 135.5(17) 111_545 . 105_544 N
Si1 Dd1 Oc 63.6(14) 111_545 . -108_656 N
Si1 Dd1 Oc 96.3(18) 111_545 . -305_556 N
Si1 Dd1 Dc1 98.6(28) 111_554 . 1_555 N
Si1 Dd1 Dc1 133.3(20) 111_554 . 105_544 N
Si1 Dd1 Dc1 82.5(17) 111_554 . -108_665 N
Si1 Dd1 Dc1 108.1(19) 111_554 . -305_565 N
Si1 Dd1 Dc2 84.4(18) 111_555 . 1_555 N
Si1 Dd1 Dc2 45.8(12) 111_555 . -108_666 N
Si1 Dd1 Od 42(4) 111_554 . 1_555 N
Si1 Dd1 Od 117.2(21) 111_554 . 105_544 N
Si1 Dd1 Od 73.0(16) 111_554 . -108_665 N
Si1 Dd1 Dd1 113.4(24) 111_533 . 105_544 N
Si1 Dd1 Dd1 77.6(23) 111_533 . -108_644 N
Si1 Dd1 Dd1 166.3(14) 111_533 . 308_433 N
Si2 Dd1 Al1 0.0 3_555 . 3_555 N
Si2 Dd1 O1 26.8(6) 3_555 . -3_555 N
Si2 Dd1 O1 71.5(11) 3_555 . 111_433 N
Si2 Dd1 O4 28.6(7) 3_555 . 312_334 N
Si2 Dd1 SJ 38.6(29) 3_555 . 1_555 N
Si2 Dd1 SJ 80.0(17) 3_555 . 105_544 N
Si2 Dd1 SJ 109.5(15) 3_555 . -108_656 N
Si2 Dd1 Oc 71.1(28) 3_555 . 1_555 N
Si2 Dd1 Oc 104.2(19) 3_555 . 105_544 N
Si2 Dd1 Oc 93.9(17) 3_555 . -108_656 N
Si2 Dd1 Oc 141.0(19) 3_555 . -305_556 N
Si2 Dd1 Dc1 89.7(32) 3_555 . 1_555 N
Si2 Dd1 Dc1 103.6(22) 3_555 . 105_544 N
Si2 Dd1 Dc1 117.5(19) 3_555 . -108_665 N
Si2 Dd1 Dc1 145.6(19) 3_555 . -305_565 N
Si2 Dd1 Dc2 47.7(17) 3_555 . 1_555 N
Si2 Dd1 Dc2 88.0(17) 3_555 . -108_666 N
Si2 Dd1 Od 50(4) 3_555 . 1_555 N
Si2 Dd1 Od 82.6(21) 3_555 . 105_544 N
Si2 Dd1 Od 112.5(20) 3_555 . -108_665 N
Si2 Dd1 Dd1 89.1(24) 3_555 . 105_544 N
Si2 Dd1 Dd1 107.5(23) 3_555 . -108_644 N
Si2 Dd1 Dd1 132.1(32) 3_555 . 308_433 N
Al1 Dd1 O1 26.8(6) 3_555 . -3_555 N
Al1 Dd1 O1 71.5(11) 3_555 . 111_433 N
Al1 Dd1 O4 28.6(7) 3_555 . 312_334 N
Al1 Dd1 SJ 38.6(29) 3_555 . 1_555 N
Al1 Dd1 SJ 80.0(17) 3_555 . 105_544 N
Al1 Dd1 SJ 109.5(15) 3_555 . -108_656 N
Al1 Dd1 Oc 71.1(28) 3_555 . 1_555 N
Al1 Dd1 Oc 104.2(19) 3_555 . 105_544 N
Al1 Dd1 Oc 93.9(17) 3_555 . -108_656 N
Al1 Dd1 Oc 141.0(19) 3_555 . -305_556 N
Al1 Dd1 Dc1 89.7(32) 3_555 . 1_555 N
Al1 Dd1 Dc1 103.6(22) 3_555 . 105_544 N
Al1 Dd1 Dc1 117.5(19) 3_555 . -108_665 N
Al1 Dd1 Dc1 145.6(19) 3_555 . -305_565 N
Al1 Dd1 Dc2 47.7(17) 3_555 . 1_555 N
Al1 Dd1 Dc2 88.0(17) 3_555 . -108_666 N
Al1 Dd1 Od 50(4) 3_555 . 1_555 N
Al1 Dd1 Od 82.6(21) 3_555 . 105_544 N
Al1 Dd1 Od 112.5(20) 3_555 . -108_665 N
Al1 Dd1 Dd1 89.1(24) 3_555 . 105_544 N
Al1 Dd1 Dd1 107.5(23) 3_555 . -108_644 N
Al1 Dd1 Dd1 132.1(32) 3_555 . 308_433 N
O1 Dd1 O1 90.6(13) -3_555 . 111_433 N
O1 Dd1 O4 52.1(11) -3_555 . 312_334 N
O1 Dd1 SJ 43.5(31) -3_555 . 1_555 N
O1 Dd1 SJ 53.3(13) -3_555 . 105_544 N
O1 Dd1 SJ 117.8(16) -3_555 . -108_656 N
O1 Dd1 Oc 44.5(23) -3_555 . 1_555 N
O1 Dd1 Oc 77.5(16) -3_555 . 105_544 N
O1 Dd1 Oc 95.6(19) -3_555 . -108_656 N
O1 Dd1 Oc 142.4(21) -3_555 . -305_556 N
O1 Dd1 Dc1 70.3(32) -3_555 . 1_555 N
O1 Dd1 Dc1 77.0(19) -3_555 . 105_544 N
O1 Dd1 Dc1 116.2(22) -3_555 . -108_665 N
O1 Dd1 Dc1 136.1(22) -3_555 . -305_565 N
O1 Dd1 Dc2 23.0(13) -3_555 . 1_555 N
O1 Dd1 Dc2 100.0(18) -3_555 . -108_666 N
O1 Dd1 Od 54(4) -3_555 . 1_555 N
O1 Dd1 Od 56.1(18) -3_555 . 105_544 N
O1 Dd1 Od 116.6(24) -3_555 . -108_665 N
O1 Dd1 Dd1 64.4(22) -3_555 . 105_544 N
O1 Dd1 Dd1 105.1(24) -3_555 . -108_644 N
O1 Dd1 Dd1 106.2(28) -3_555 . 308_433 N
O1 Dd1 O4 43.2(9) 111_433 . 312_334 N
O1 Dd1 SJ 50.5(31) 111_545 . 1_555 N
O1 Dd1 SJ 126.0(18) 111_545 . 105_544 N
O1 Dd1 SJ 42.9(10) 111_545 . -108_656 N
O1 Dd1 Oc 116.7(27) 111_545 . 1_555 N
O1 Dd1 Oc 130.3(20) 111_545 . 105_544 N
O1 Dd1 Oc 44.4(13) 111_545 . -108_656 N
O1 Dd1 Oc 72.4(16) 111_545 . -305_556 N
O1 Dd1 Dc1 90.8(31) 111_554 . 1_555 N
O1 Dd1 Dc1 127.8(23) 111_554 . 105_544 N
O1 Dd1 Dc1 59.7(15) 111_554 . -108_665 N
O1 Dd1 Dc1 84.1(18) 111_554 . -305_565 N
O1 Dd1 Dc2 96.0(19) 111_555 . 1_555 N
O1 Dd1 Dc2 23.1(9) 111_555 . -108_666 N
O1 Dd1 Od 44(4) 111_554 . 1_555 N
O1 Dd1 Od 120.2(24) 111_554 . 105_544 N
O1 Dd1 Od 49.7(14) 111_554 . -108_665 N
O1 Dd1 Dd1 110.3(23) 111_533 . 105_544 N
O1 Dd1 Dd1 56.8(21) 111_533 . -108_644 N
O1 Dd1 Dd1 146.1(25) 111_533 . 308_433 N
O4 Dd1 SJ 32.2(24) 312_446 . 1_555 N
O4 Dd1 SJ 102.7(21) 312_446 . 105_544 N
O4 Dd1 SJ 84.1(16) 312_446 . -108_656 N
O4 Dd1 Oc 92.5(28) 312_446 . 1_555 N
O4 Dd1 Oc 123.5(21) 312_446 . 105_544 N
O4 Dd1 Oc 74.7(15) 312_446 . -108_656 N
O4 Dd1 Oc 115.1(22) 312_446 . -305_556 N
O4 Dd1 Dc1 94.2(28) 312_455 . 1_555 N
O4 Dd1 Dc1 122.0(23) 312_455 . 105_544 N
O4 Dd1 Dc1 96.9(20) 312_455 . -108_665 N
O4 Dd1 Dc1 124.8(23) 312_455 . -305_565 N
O4 Dd1 Dc2 67.3(17) 312_456 . 1_555 N
O4 Dd1 Dc2 62.3(14) 312_456 . -108_666 N
O4 Dd1 Od 38(4) 312_455 . 1_555 N
O4 Dd1 Od 102.5(24) 312_455 . 105_544 N
O4 Dd1 Od 89.0(21) 312_455 . -108_665 N
O4 Dd1 Dd1 103.2(28) 312_434 . 105_544 N
O4 Dd1 Dd1 89.4(27) 312_434 . -108_644 N
O4 Dd1 Dd1 157.1(29) 312_434 . 308_433 N
SJ Dd1 SJ 78.7(34) 1_555 . 105_544 N
SJ Dd1 SJ 75.4(34) 1_555 . -108_656 N
SJ Dd1 Oc 68.5(34) 1_555 . 1_555 N
SJ Dd1 Oc 94(4) 1_555 . 105_544 N
SJ Dd1 Oc 56.1(29) 1_555 . -108_656 N
SJ Dd1 Oc 105(4) 1_555 . -305_556 N
SJ Dd1 Dc1 62.0(30) 1_555 . 1_555 N
SJ Dd1 Dc1 92(4) 1_555 . 105_544 N
SJ Dd1 Dc1 79(4) 1_555 . -108_665 N
SJ Dd1 Dc1 107(4) 1_555 . -305_565 N
SJ Dd1 Dc2 45.6(27) 1_555 . 1_555 N
SJ Dd1 Dc2 56.5(30) 1_555 . -108_666 N
SJ Dd1 Od 11.5(32) 1_555 . 1_555 N
SJ Dd1 Od 76(4) 1_555 . 105_544 N
SJ Dd1 Od 76(4) 1_555 . -108_665 N
SJ Dd1 Dd1 73(5) 1_555 . 105_544 N
SJ Dd1 Dd1 69(5) 1_555 . -108_644 N
SJ Dd1 Dd1 128(4) 1_555 . 308_433 N
SJ Dd1 SJ 115.1(26) 105_544 . -108_656 N
SJ Dd1 Oc 10.4(15) 105_544 . 1_555 N
SJ Dd1 Oc 24.7(9) 105_544 . 105_544 N
SJ Dd1 Oc 95.1(25) 105_544 . -108_656 N
SJ Dd1 Oc 110.5(24) 105_544 . -305_556 N
SJ Dd1 Dc1 43.3(29) 105_544 . 1_555 N
SJ Dd1 Dc1 24.8(10) 105_544 . 105_544 N
SJ Dd1 Dc1 98.3(27) 105_544 . -108_665 N
SJ Dd1 Dc1 96.2(22) 105_544 . -305_565 N
SJ Dd1 Dc2 35.4(15) 105_544 . 1_555 N
SJ Dd1 Dc2 116.1(25) 105_544 . -108_666 N
SJ Dd1 Od 82(4) 105_544 . 1_555 N
SJ Dd1 Od 8.4(12) 105_544 . 105_544 N
SJ Dd1 Od 107.3(27) 105_544 . -108_665 N
SJ Dd1 Dd1 23.3(13) 105_544 . 105_544 N
SJ Dd1 Dd1 91.9(21) 105_544 . -108_644 N
SJ Dd1 Dd1 54.5(19) 105_544 . 308_433 N
SJ Dd1 Oc 112(4) -108_656 . 1_555 N
SJ Dd1 Oc 101.6(22) -108_656 . 105_544 N
SJ Dd1 Oc 24.0(12) -108_656 . -108_656 N
SJ Dd1 Oc 31.5(10) -108_656 . -305_556 N
SJ Dd1 Dc1 72(4) -108_665 . 1_555 N
SJ Dd1 Dc1 99.6(26) -108_665 . 105_544 N
SJ Dd1 Dc1 19.2(11) -108_665 . -108_665 N
SJ Dd1 Dc1 41.3(12) -108_665 . -305_565 N
SJ Dd1 Dc2 108.0(27) -108_666 . 1_555 N
SJ Dd1 Dc2 21.9(11) -108_666 . -108_666 N
SJ Dd1 Od 64(5) -108_665 . 1_555 N
SJ Dd1 Od 106.7(28) -108_665 . 105_544 N
SJ Dd1 Od 8.5(11) -108_665 . -108_665 N
SJ Dd1 Dd1 91.8(20) -108_644 . 105_544 N
SJ Dd1 Dd1 23.2(12) -108_644 . -108_644 N
SJ Dd1 Dd1 103.6(21) -108_644 . 308_433 N
Oc Dd1 Oc 33.0(22) 1_555 . 105_544 N
Oc Dd1 Oc 90.4(34) 1_555 . -108_656 N
Oc Dd1 Oc 114(4) 1_555 . -305_556 N
Oc Dd1 Dc1 40.7(23) 1_555 . 1_555 N
Oc Dd1 Dc1 32.5(21) 1_555 . 105_544 N
Oc Dd1 Dc1 98(4) 1_555 . -108_665 N
Oc Dd1 Dc1 101(4) 1_555 . -305_565 N
Oc Dd1 Dc2 25.2(13) 1_555 . 1_555 N
Oc Dd1 Dc2 109.6(35) 1_555 . -108_666 N
Oc Dd1 Od 73(4) 1_555 . 1_555 N
Oc Dd1 Od 11.8(23) 1_555 . 105_544 N
Oc Dd1 Od 105(4) 1_555 . -108_665 N
Oc Dd1 Dd1 24.0(31) 1_555 . 105_544 N
Oc Dd1 Dd1 90(4) 1_555 . -108_644 N
Oc Dd1 Dd1 64.6(30) 1_555 . 308_433 N
Oc Dd1 Oc 88.4(24) 105_544 . -108_656 N
Oc Dd1 Oc 88.2(18) 105_544 . -305_556 N
Oc Dd1 Dc1 39.6(26) 105_544 . 1_555 N
Oc Dd1 Dc1 2.5(5) 105_544 . 105_544 N
Oc Dd1 Dc1 82.6(23) 105_544 . -108_665 N
Oc Dd1 Dc1 73.4(15) 105_544 . -305_565 N
Oc Dd1 Dc2 57.4(19) 105_544 . 1_555 N
Oc Dd1 Dc2 111.6(27) 105_544 . -108_666 N
Oc Dd1 Od 94(4) 105_544 . 1_555 N
Oc Dd1 Od 21.7(9) 105_544 . 105_544 N
Oc Dd1 Od 93.1(23) 105_544 . -108_665 N
Oc Dd1 Dd1 22.1(9) 105_544 . 105_544 N
Oc Dd1 Dd1 79.8(15) 105_544 . -108_644 N
Oc Dd1 Dd1 34.2(11) 105_544 . 308_433 N
Oc Dd1 Oc 48.8(17) -108_656 . -305_556 N
Oc Dd1 Dc1 52.2(28) -108_665 . 1_555 N
Oc Dd1 Dc1 85.9(26) -108_665 . 105_544 N
Oc Dd1 Dc1 23.6(9) -108_665 . -108_665 N
Oc Dd1 Dc1 52.1(18) -108_665 . -305_565 N
Oc Dd1 Dc2 83.9(24) -108_666 . 1_555 N
Oc Dd1 Dc2 23.2(7) -108_666 . -108_666 N
Oc Dd1 Od 45(4) -108_665 . 1_555 N
Oc Dd1 Od 87.0(29) -108_665 . 105_544 N
Oc Dd1 Od 21.0(16) -108_665 . -108_665 N
Oc Dd1 Dd1 73.0(25) -108_644 . 105_544 N
Oc Dd1 Dd1 14.7(23) -108_644 . -108_644 N
Oc Dd1 Dd1 103.6(20) -108_644 . 308_433 N
Oc Dd1 Dc1 77(4) -305_565 . 1_555 N
Oc Dd1 Dc1 87.2(22) -305_565 . 105_544 N
Oc Dd1 Dc1 26.4(11) -305_565 . -108_665 N
Oc Dd1 Dc1 14.9(4) -305_565 . -305_565 N
Oc Dd1 Dc2 123.7(33) -305_566 . 1_555 N
Oc Dd1 Dc2 53.3(18) -305_566 . -108_666 N
Oc Dd1 Od 93(5) -305_565 . 1_555 N
Oc Dd1 Od 103.4(25) -305_565 . 105_544 N
Oc Dd1 Od 28.8(9) -305_565 . -108_665 N
Oc Dd1 Dd1 89.9(15) -305_544 . 105_544 N
Oc Dd1 Dd1 37.5(6) -305_544 . -108_644 N
Oc Dd1 Dd1 76.6(15) -305_544 . 308_433 N
Dc1 Dd1 Dc1 37.1(25) 1_555 . 105_544 N
Dc1 Dd1 Dc1 56.9(34) 1_555 . -108_665 N
Dc1 Dd1 Dc1 66(4) 1_555 . -305_565 N
Dc1 Dd1 Dc2 48.0(25) 1_555 . 1_555 N
Dc1 Dd1 Dc2 74.5(33) 1_555 . -108_666 N
Dc1 Dd1 Od 58(4) 1_555 . 1_555 N
Dc1 Dd1 Od 35.0(29) 1_555 . 105_544 N
Dc1 Dd1 Od 65(4) 1_555 . -108_665 N
Dc1 Dd1 Dd1 20.8(32) 1_555 . 105_544 N
Dc1 Dd1 Dd1 49.0(35) 1_555 . -108_644 N
Dc1 Dd1 Dd1 68.6(28) 1_555 . 308_433 N
Dc1 Dd1 Dc1 80.7(26) 105_544 . -108_665 N
Dc1 Dd1 Dc1 72.4(19) 105_544 . -305_565 N
Dc1 Dd1 Dc2 56.5(20) 105_544 . 1_555 N
Dc1 Dd1 Dc2 109.1(30) 105_544 . -108_666 N
Dc1 Dd1 Od 92(5) 105_544 . 1_555 N
Dc1 Dd1 Od 21.0(10) 105_544 . 105_544 N
Dc1 Dd1 Od 91.1(26) 105_544 . -108_665 N
Dc1 Dd1 Dd1 20.0(9) 105_544 . 105_544 N
Dc1 Dd1 Dd1 77.6(17) 105_544 . -108_644 N
Dc1 Dd1 Dd1 36.0(13) 105_544 . 308_433 N
Dc1 Dd1 Dc1 28.6(11) -108_665 . -305_565 N
Dc1 Dd1 Dc2 99.9(31) -108_666 . 1_555 N
Dc1 Dd1 Dc2 36.8(12) -108_666 . -108_666 N
Dc1 Dd1 Od 68(5) -108_665 . 1_555 N
Dc1 Dd1 Od 90.0(30) -108_665 . 105_544 N
Dc1 Dd1 Od 10.8(12) -108_665 . -108_665 N
Dc1 Dd1 Dd1 75.0(21) -108_644 . 105_544 N
Dc1 Dd1 Dd1 11.2(13) -108_644 . -108_644 N
Dc1 Dd1 Dd1 86.3(17) -108_644 . 308_433 N
Dc1 Dd1 Dc2 114.3(32) -305_566 . 1_555 N
Dc1 Dd1 Dc2 62.8(20) -305_566 . -108_666 N
Dc1 Dd1 Od 96(5) -305_565 . 1_555 N
Dc1 Dd1 Od 89.6(22) -305_565 . 105_544 N
Dc1 Dd1 Od 35.8(10) -305_565 . -108_665 N
Dc1 Dd1 Dd1 76.8(12) -305_544 . 105_544 N
Dc1 Dd1 Dd1 38.1(7) -305_544 . -108_644 N
Dc1 Dd1 Dd1 63.2(12) -305_544 . 308_433 N
Dc2 Dd1 Dc2 96.4(22) 1_555 . -108_666 N
Dc2 Dd1 Od 52(4) 1_555 . 1_555 N
Dc2 Dd1 Od 35.7(21) 1_555 . 105_544 N
Dc2 Dd1 Od 103.7(34) 1_555 . -108_665 N
Dc2 Dd1 Dd1 41.7(27) 1_555 . 105_544 N
Dc2 Dd1 Dd1 89.4(32) 1_555 . -108_644 N
Dc2 Dd1 Dd1 89.8(30) 1_555 . 308_433 N
Dc2 Dd1 Od 46(4) -108_665 . 1_555 N
Dc2 Dd1 Od 108.5(31) -108_665 . 105_544 N
Dc2 Dd1 Od 27.2(16) -108_665 . -108_665 N
Dc2 Dd1 Dd1 95.3(27) -108_644 . 105_544 N
Dc2 Dd1 Dd1 33.9(23) -108_644 . -108_644 N
Dc2 Dd1 Dd1 123.0(26) -108_644 . 308_433 N
Od Dd1 Od 78(4) 1_555 . 105_544 N
Od Dd1 Od 65(5) 1_555 . -108_665 N
Od Dd1 Dd1 72(5) 1_555 . 105_544 N
Od Dd1 Dd1 58(6) 1_555 . -108_644 N
Od Dd1 Dd1 126(4) 1_555 . 308_433 N
Od Dd1 Od 98.9(34) 105_544 . -108_665 N
Od Dd1 Dd1 15.0(10) 105_544 . 105_544 N
Od Dd1 Dd1 83.5(27) 105_544 . -108_644 N
Od Dd1 Dd1 54.8(14) 105_544 . 308_433 N
Od Dd1 Dd1 84.0(26) -108_644 . 105_544 N
Od Dd1 Dd1 15.7(7) -108_644 . -108_644 N
Od Dd1 Dd1 96.4(16) -108_644 . 308_433 N
Dd1 Dd1 Dd1 68.6(22) 105_544 . -108_644 N
Dd1 Dd1 Dd1 55.7(11) 105_544 . 308_433 N
Dd1 Dd1 Dd1 90.0000(4) -108_644 . 308_433 N
Si1 Dd2 Si2 77.9(17) 111_533 . 3_555 N
Si1 Dd2 Al1 77.9(17) 111_443 . 3_555 N
Si1 Dd2 O1 107.8(26) 111_433 . -3_555 N
Si1 Dd2 O1 35.3(13) 111_433 . 111_433 N
Si1 Dd2 O2 13.3(7) 111_433 . 1_555 N
Si1 Dd2 O3 81.8(14) 111_433 . 2_555 N
Si1 Dd2 O3 31.7(8) 111_433 . 208_343 N
Si1 Dd2 O4 34.0(23) 111_433 . 312_334 N
Si1 Dd2 SII 68.8(12) 111_555 . -105_566 N
Si1 Dd2 SJ 120(8) 111_545 . 1_555 N
Si1 Dd2 SJ 147.5(30) 111_545 . 105_544 N
Si1 Dd2 SJ 83.0(28) 111_545 . -108_656 N
Si1 Dd2 Oc 157(4) 111_545 . 1_555 N
Si1 Dd2 Oc 94(4) 111_545 . -108_656 N
Si1 Dd2 Dc1 140(4) 111_554 . 1_555 N
Si1 Dd2 Dc1 151.8(31) 111_554 . 105_544 N
Si1 Dd2 Dc1 105(4) 111_554 . -108_665 N
Si1 Dd2 Dc2 135(4) 111_555 . 1_555 N
Si1 Dd2 Dc2 74.9(31) 111_555 . -108_666 N
Si1 Dd2 Od 135(7) 111_554 . 1_555 N
Si1 Dd2 Od 144.5(35) 111_554 . 105_544 N
Si1 Dd2 Od 89.2(32) 111_554 . -108_665 N
Si1 Dd2 Dd1 152(7) 111_533 . 1_555 N
Si1 Dd2 Dd1 94.0(26) 111_533 . -108_644 N
Si2 Dd2 Al1 0.0 3_555 . 3_555 N
Si2 Dd2 O1 35.3(13) 3_555 . -3_555 N
Si2 Dd2 O1 110.4(25) 3_555 . 111_433 N
Si2 Dd2 O2 68.0(14) 3_555 . 1_555 N
Si2 Dd2 O3 28.3(9) 3_555 . 2_555 N
Si2 Dd2 O3 83.0(13) 3_555 . 208_343 N
Si2 Dd2 O4 44.0(26) 3_555 . 312_334 N
Si2 Dd2 SII 67.2(15) 3_555 . -105_566 N
Si2 Dd2 SJ 96(8) 3_555 . 1_555 N
Si2 Dd2 SJ 84.6(26) 3_555 . 105_544 N
Si2 Dd2 SJ 147.3(33) 3_555 . -108_656 N
Si2 Dd2 Oc 96(4) 3_555 . 1_555 N
Si2 Dd2 Oc 134(4) 3_555 . -108_656 N
Si2 Dd2 Dc1 116(4) 3_555 . 1_555 N
Si2 Dd2 Dc1 104.9(29) 3_555 . 105_544 N
Si2 Dd2 Dc1 148.0(33) 3_555 . -108_665 N
Si2 Dd2 Dc2 73.2(31) 3_555 . 1_555 N
Si2 Dd2 Dc2 139(4) 3_555 . -108_666 N
Si2 Dd2 Od 123(6) 3_555 . 1_555 N
Si2 Dd2 Od 88.8(30) 3_555 . 105_544 N
Si2 Dd2 Od 146(4) 3_555 . -108_665 N
Si2 Dd2 Dd1 130(7) 3_555 . 1_555 N
Si2 Dd2 Dd1 134.2(31) 3_555 . -108_644 N
Al1 Dd2 O1 35.3(13) 3_555 . -3_555 N
Al1 Dd2 O1 110.4(25) 3_555 . 111_433 N
Al1 Dd2 O2 68.0(14) 3_555 . 1_555 N
Al1 Dd2 O3 28.3(9) 3_555 . 2_555 N
Al1 Dd2 O3 83.0(13) 3_555 . 208_343 N
Al1 Dd2 O4 44.0(26) 3_555 . 312_334 N
Al1 Dd2 SII 67.2(15) 3_555 . -105_566 N
Al1 Dd2 SJ 96(8) 3_555 . 1_555 N
Al1 Dd2 SJ 84.6(26) 3_555 . 105_544 N
Al1 Dd2 SJ 147.3(33) 3_555 . -108_656 N
Al1 Dd2 Oc 96(4) 3_555 . 1_555 N
Al1 Dd2 Oc 134(4) 3_555 . -108_656 N
Al1 Dd2 Dc1 116(4) 3_555 . 1_555 N
Al1 Dd2 Dc1 104.9(29) 3_555 . 105_544 N
Al1 Dd2 Dc1 148.0(33) 3_555 . -108_665 N
Al1 Dd2 Dc2 73.2(31) 3_555 . 1_555 N
Al1 Dd2 Dc2 139(4) 3_555 . -108_666 N
Al1 Dd2 Od 123(6) 3_555 . 1_555 N
Al1 Dd2 Od 88.8(30) 3_555 . 105_544 N
Al1 Dd2 Od 146(4) 3_555 . -108_665 N
Al1 Dd2 Dd1 130(7) 3_555 . 1_555 N
Al1 Dd2 Dd1 134.2(31) 3_555 . -108_644 N
O1 Dd2 O1 130.9(30) -3_555 . 111_433 N
O1 Dd2 O2 95.3(19) -3_555 . 1_555 N
O1 Dd2 O3 53.8(16) -3_555 . 2_555 N
O1 Dd2 O3 118.3(20) -3_555 . 208_343 N
O1 Dd2 O4 75(4) -3_555 . 312_334 N
O1 Dd2 SII 95.5(24) -3_555 . -105_566 N
O1 Dd2 SJ 65(7) -3_555 . 1_555 N
O1 Dd2 SJ 49.5(14) -3_555 . 105_544 N
O1 Dd2 SJ 134.0(24) -3_555 . -108_656 N
O1 Dd2 Oc 61.3(24) -3_555 . 1_555 N
O1 Dd2 Oc 112.2(29) -3_555 . -108_656 N
O1 Dd2 Dc1 80.9(29) -3_555 . 1_555 N
O1 Dd2 Dc1 69.7(17) -3_555 . 105_544 N
O1 Dd2 Dc1 119.2(24) -3_555 . -108_665 N
O1 Dd2 Dc2 37.9(18) -3_555 . 1_555 N
O1 Dd2 Dc2 131.9(35) -3_555 . -108_666 N
O1 Dd2 Od 88(5) -3_555 . 1_555 N
O1 Dd2 Od 53.5(19) -3_555 . 105_544 N
O1 Dd2 Od 127.3(25) -3_555 . -108_665 N
O1 Dd2 Dd1 100(6) -3_555 . 1_555 N
O1 Dd2 Dd1 112.6(24) -3_555 . -108_644 N
O1 Dd2 O2 42.7(10) 111_433 . 1_555 N
O1 Dd2 O3 116.9(18) 111_433 . 2_555 N
O1 Dd2 O3 52.7(14) 111_433 . 208_343 N
O1 Dd2 O4 67(4) 111_433 . 312_334 N
O1 Dd2 SII 94.3(20) 111_555 . -105_566 N
O1 Dd2 SJ 102(8) 111_545 . 1_555 N
O1 Dd2 SJ 136.8(25) 111_545 . 105_544 N
O1 Dd2 SJ 47.8(16) 111_545 . -108_656 N
O1 Dd2 Oc 135.3(35) 111_545 . 1_555 N
O1 Dd2 Oc 61.6(25) 111_545 . -108_656 N
O1 Dd2 Dc1 110(4) 111_554 . 1_555 N
O1 Dd2 Dc1 124.9(24) 111_554 . 105_544 N
O1 Dd2 Dc1 70.1(24) 111_554 . -108_665 N
O1 Dd2 Dc2 133(4) 111_555 . 1_555 N
O1 Dd2 Dc2 40.1(18) 111_555 . -108_666 N
O1 Dd2 Od 103(6) 111_554 . 1_555 N
O1 Dd2 Od 130.0(27) 111_554 . 105_544 N
O1 Dd2 Od 54.4(22) 111_554 . -108_665 N
O1 Dd2 Dd1 119(6) 111_533 . 1_555 N
O1 Dd2 Dd1 61.6(18) 111_533 . -108_644 N
O2 Dd2 O3 77.2(11) 1_555 . 2_555 N
O2 Dd2 O3 42.2(8) 1_555 . 208_343 N
O2 Dd2 O4 24.5(28) 1_555 . 312_334 N
O2 Dd2 SII 73.8(11) 1_555 . -105_566 N
O2 Dd2 SJ 111(7) 1_555 . 1_555 N
O2 Dd2 SJ 134.8(24) 1_555 . 105_544 N
O2 Dd2 SJ 88.3(23) 1_555 . -108_656 N
O2 Dd2 Oc 145.4(34) 1_555 . 1_555 N
O2 Dd2 Oc 94.8(29) 1_555 . -108_656 N
O2 Dd2 Dc1 135(4) 1_555 . 1_555 N
O2 Dd2 Dc1 143.3(23) 1_555 . 105_544 N
O2 Dd2 Dc1 108.4(29) 1_555 . -108_665 N
O2 Dd2 Dc2 121.6(32) 1_555 . 1_555 N
O2 Dd2 Dc2 79.5(26) 1_555 . -108_666 N
O2 Dd2 Od 133(6) 1_555 . 1_555 N
O2 Dd2 Od 132.6(28) 1_555 . 105_544 N
O2 Dd2 Od 93.4(27) 1_555 . -108_665 N
O2 Dd2 Dd1 161(7) 1_555 . 1_555 N
O2 Dd2 Dd1 94.9(19) 1_555 . -108_644 N
O3 Dd2 O3 71.4(11) 2_555 . 208_343 N
O3 Dd2 O4 53.9(29) 2_555 . 312_334 N
O3 Dd2 SII 42.0(9) 2_555 . -105_566 N
O3 Dd2 SJ 119(8) 2_555 . 1_555 N
O3 Dd2 SJ 95.7(25) 2_555 . 105_544 N
O3 Dd2 SJ 164.7(26) 2_555 . -108_656 N
O3 Dd2 Oc 104(4) 2_555 . 1_555 N
O3 Dd2 Oc 162(4) 2_555 . -108_656 N
O3 Dd2 Dc1 129(4) 2_555 . 1_555 N
O3 Dd2 Dc1 114.3(28) 2_555 . 105_544 N
O3 Dd2 Dc1 172.1(33) 2_555 . -108_665 N
O3 Dd2 Dc2 88.5(34) 2_555 . 1_555 N
O3 Dd2 Dc2 156.6(32) 2_555 . -108_666 N
O3 Dd2 Od 137(6) 2_555 . 1_555 N
O3 Dd2 Od 101.8(29) 2_555 . 105_544 N
O3 Dd2 Od 170.5(29) 2_555 . -108_665 N
O3 Dd2 Dd1 121(7) 2_555 . 1_555 N
O3 Dd2 Dd1 162.6(29) 2_555 . -108_644 N
O3 Dd2 O4 48.9(23) 208_343 . 312_334 N
O3 Dd2 SII 41.7(7) 208_465 . -105_566 N
O3 Dd2 SJ 152(9) 208_455 . 1_555 N
O3 Dd2 SJ 167.0(29) 208_455 . 105_544 N
O3 Dd2 SJ 94.5(26) 208_455 . -108_656 N
O3 Dd2 Oc 171(4) 208_455 . 1_555 N
O3 Dd2 Oc 113(4) 208_455 . -108_656 N
O3 Dd2 Dc1 159(5) 208_464 . 1_555 N
O3 Dd2 Dc1 171.6(28) 208_464 . 105_544 N
O3 Dd2 Dc1 116.5(34) 208_464 . -108_665 N
O3 Dd2 Dc2 155.9(35) 208_465 . 1_555 N
O3 Dd2 Dc2 89.5(31) 208_465 . -108_666 N
O3 Dd2 Od 152(7) 208_464 . 1_555 N
O3 Dd2 Od 171.7(28) 208_464 . 105_544 N
O3 Dd2 Od 102.3(29) 208_464 . -108_665 N
O3 Dd2 Dd1 134(6) 208_443 . 1_555 N
O3 Dd2 Dd1 113.0(27) 208_443 . -108_644 N
O4 Dd2 SII 63.1(22) 312_456 . -105_566 N
O4 Dd2 SJ 113(8) 312_446 . 1_555 N
O4 Dd2 SJ 122(5) 312_446 . 105_544 N
O4 Dd2 SJ 112(5) 312_446 . -108_656 N
O4 Dd2 Oc 135(6) 312_446 . 1_555 N
O4 Dd2 Oc 115(5) 312_446 . -108_656 N
O4 Dd2 Dc1 141(5) 312_455 . 1_555 N
O4 Dd2 Dc1 139(5) 312_455 . 105_544 N
O4 Dd2 Dc1 131(5) 312_455 . -108_665 N
O4 Dd2 Dc2 109(5) 312_456 . 1_555 N
O4 Dd2 Dc2 103(5) 312_456 . -108_666 N
O4 Dd2 Od 143(7) 312_455 . 1_555 N
O4 Dd2 Od 123(5) 312_455 . 105_544 N
O4 Dd2 Od 117(5) 312_455 . -108_665 N
O4 Dd2 Dd1 174(9) 312_434 . 1_555 N
O4 Dd2 Dd1 115(4) 312_434 . -108_644 N
SII Dd2 SJ 160(9) -105_556 . 1_555 N
SII Dd2 SJ 128.4(31) -105_556 . 105_544 N
SII Dd2 SJ 129.1(30) -105_556 . -108_656 N
SII Dd2 Oc 130(4) -105_556 . 1_555 N
SII Dd2 Oc 151(4) -105_556 . -108_656 N
SII Dd2 Dc1 151(4) -105_565 . 1_555 N
SII Dd2 Dc1 138.7(30) -105_565 . 105_544 N
SII Dd2 Dc1 144.3(34) -105_565 . -108_665 N
SII Dd2 Dc2 127(4) -105_566 . 1_555 N
SII Dd2 Dc2 127(4) -105_566 . -108_666 N
SII Dd2 Od 153(6) -105_565 . 1_555 N
SII Dd2 Od 135.3(34) -105_565 . 105_544 N
SII Dd2 Od 136.6(32) -105_565 . -108_665 N
SII Dd2 Dd1 115(6) -105_544 . 1_555 N
SII Dd2 Dd1 150.7(33) -105_544 . -108_644 N
SJ Dd2 SJ 35(7) 1_555 . 105_544 N
SJ Dd2 SJ 71(7) 1_555 . -108_656 N
SJ Dd2 Oc 37(5) 1_555 . 1_555 N
SJ Dd2 Oc 49(6) 1_555 . -108_656 N
SJ Dd2 Dc1 28(4) 1_555 . 1_555 N
SJ Dd2 Dc1 32(6) 1_555 . 105_544 N
SJ Dd2 Dc1 54(6) 1_555 . -108_665 N
SJ Dd2 Dc2 34(6) 1_555 . 1_555 N
SJ Dd2 Dc2 73(7) 1_555 . -108_666 N
SJ Dd2 Od 32(4) 1_555 . 1_555 N
SJ Dd2 Od 28(6) 1_555 . 105_544 N
SJ Dd2 Od 64(7) 1_555 . -108_665 N
SJ Dd2 Dd1 66(5) 1_555 . 1_555 N
SJ Dd2 Dd1 50(7) 1_555 . -108_644 N
SJ Dd2 SJ 98.1(15) 105_544 . -108_656 N
SJ Dd2 Oc 12.4(13) 105_544 . 1_555 N
SJ Dd2 Oc 78.6(16) 105_544 . -108_656 N
SJ Dd2 Dc1 33.6(19) 105_544 . 1_555 N
SJ Dd2 Dc1 20.3(7) 105_544 . 105_544 N
SJ Dd2 Dc1 76.4(13) 105_544 . -108_665 N
SJ Dd2 Dc2 13.7(11) 105_544 . 1_555 N
SJ Dd2 Dc2 102.6(19) 105_544 . -108_666 N
SJ Dd2 Od 41(4) 105_544 . 1_555 N
SJ Dd2 Od 6.9(10) 105_544 . 105_544 N
SJ Dd2 Od 90.2(9) 105_544 . -108_665 N
SJ Dd2 Dd1 54(4) 105_544 . 1_555 N
SJ Dd2 Dd1 78.7(13) 105_544 . -108_644 N
SJ Dd2 Oc 91.2(21) -108_656 . 1_555 N
SJ Dd2 Oc 22.1(13) -108_656 . -108_656 N
SJ Dd2 Dc1 65.3(23) -108_665 . 1_555 N
SJ Dd2 Dc1 80.4(12) -108_665 . 105_544 N
SJ Dd2 Dc1 22.8(10) -108_665 . -108_665 N
SJ Dd2 Dc2 103.6(24) -108_666 . 1_555 N
SJ Dd2 Dc2 9.1(10) -108_666 . -108_666 N
SJ Dd2 Od 58(5) -108_665 . 1_555 N
SJ Dd2 Od 91.6(11) -108_665 . 105_544 N
SJ Dd2 Od 8.0(11) -108_665 . -108_665 N
SJ Dd2 Dd1 73(5) -108_644 . 1_555 N
SJ Dd2 Dd1 21.8(11) -108_644 . -108_644 N
Oc Dd2 Oc 74.0(17) 1_555 . -108_656 N
Oc Dd2 Dc1 26.0(8) 1_555 . 1_555 N
Oc Dd2 Dc1 10.9(12) 1_555 . 105_544 N
Oc Dd2 Dc1 68.6(15) 1_555 . -108_665 N
Oc Dd2 Dc2 26.0(9) 1_555 . 1_555 N
Oc Dd2 Dc2 97.1(24) 1_555 . -108_666 N
Oc Dd2 Od 33(4) 1_555 . 1_555 N
Oc Dd2 Od 12.8(10) 1_555 . 105_544 N
Oc Dd2 Od 83.6(15) 1_555 . -108_665 N
Oc Dd2 Dd1 41.3(35) 1_555 . 1_555 N
Oc Dd2 Dd1 74.1(21) 1_555 . -108_644 N
Oc Dd2 Dc1 48.3(16) -108_665 . 1_555 N
Oc Dd2 Dc1 63.4(13) -108_665 . 105_544 N
Oc Dd2 Dc1 17.0(6) -108_665 . -108_665 N
Oc Dd2 Dc2 82.2(22) -108_666 . 1_555 N
Oc Dd2 Dc2 24.1(9) -108_666 . -108_666 N
Oc Dd2 Od 42(4) -108_665 . 1_555 N
Oc Dd2 Od 71.7(14) -108_665 . 105_544 N
Oc Dd2 Od 15.1(14) -108_665 . -108_665 N
Oc Dd2 Dd1 69(4) -108_644 . 1_555 N
Oc Dd2 Dd1 0.451(11) -108_644 . -108_644 N
Dc1 Dd2 Dc1 15.2(16) 1_555 . 105_544 N
Dc1 Dd2 Dc1 43.0(15) 1_555 . -108_665 N
Dc1 Dd2 Dc2 43.1(14) 1_555 . 1_555 N
Dc1 Dd2 Dc2 71.1(23) 1_555 . -108_666 N
Dc1 Dd2 Od 7.9(31) 1_555 . 1_555 N
Dc1 Dd2 Od 28.0(17) 1_555 . 105_544 N
Dc1 Dd2 Od 57.6(19) 1_555 . -108_665 N
Dc1 Dd2 Dd1 38.6(30) 1_555 . 1_555 N
Dc1 Dd2 Dd1 48.4(25) 1_555 . -108_644 N
Dc1 Dd2 Dc1 57.8(11) 105_544 . -108_665 N
Dc1 Dd2 Dc2 32.4(10) 105_544 . 1_555 N
Dc1 Dd2 Dc2 86.2(17) 105_544 . -108_666 N
Dc1 Dd2 Od 23(4) 105_544 . 1_555 N
Dc1 Dd2 Od 16.7(6) 105_544 . 105_544 N
Dc1 Dd2 Od 72.7(7) 105_544 . -108_665 N
Dc1 Dd2 Dd1 38(4) 105_544 . 1_555 N
Dc1 Dd2 Dd1 63.5(13) 105_544 . -108_644 N
Dc1 Dd2 Dc2 83.7(19) -108_666 . 1_555 N
Dc1 Dd2 Dc2 30.1(10) -108_666 . -108_666 N
Dc1 Dd2 Od 35(4) -108_665 . 1_555 N
Dc1 Dd2 Od 70.2(9) -108_665 . 105_544 N
Dc1 Dd2 Od 15.8(9) -108_665 . -108_665 N
Dc1 Dd2 Dd1 54(4) -108_644 . 1_555 N
Dc1 Dd2 Dd1 16.6(17) -108_644 . -108_644 N
Dc2 Dd2 Dc2 106.1(29) 1_555 . -108_666 N
Dc2 Dd2 Od 51(4) 1_555 . 1_555 N
Dc2 Dd2 Od 15.8(15) 1_555 . 105_544 N
Dc2 Dd2 Od 95.7(20) 1_555 . -108_665 N
Dc2 Dd2 Dd1 67(4) 1_555 . 1_555 N
Dc2 Dd2 Dd1 82.4(23) 1_555 . -108_644 N
Dc2 Dd2 Od 64(5) -108_665 . 1_555 N
Dc2 Dd2 Od 95.8(16) -108_665 . 105_544 N
Dc2 Dd2 Od 14.3(14) -108_665 . -108_665 N
Dc2 Dd2 Dd1 82(5) -108_644 . 1_555 N
Dc2 Dd2 Dd1 23.9(14) -108_644 . -108_644 N
Od Dd2 Od 36(4) 1_555 . 105_544 N
Od Dd2 Od 50(4) 1_555 . -108_665 N
Od Dd2 Dd1 37.7361(5) 1_555 . 1_555 N
Od Dd2 Dd1 42(5) 1_555 . -108_644 N
Od Dd2 Od 83.7(13) 105_544 . -108_665 N
Od Dd2 Dd1 53(4) 105_544 . 1_555 N
Od Dd2 Dd1 71.9(16) 105_544 . -108_644 N
Od Dd2 Dd1 69(5) -108_644 . 1_555 N
Od Dd2 Dd1 14.7(5) -108_644 . -108_644 N
Dd1 Dd2 Dd1 69(6) 1_555 . -108_644 N
Si1 OII' Si1 90.2(8) 107_434 . 208_344 N
Si1 OII' Si1 90.2(8) 107_434 . 312_335 N
Si1 OII' Si2 107.6(12) 107_533 . 111_533 N
Si1 OII' Si2 47.8(4) 107_533 . 209_443 N
Si1 OII' Si2 47.5(4) 107_533 . 310_434 N
Si1 OII' Al1 107.6(12) 107_443 . 111_443 N
Si1 OII' Al1 47.8(4) 107_443 . 209_353 N
Si1 OII' Al1 47.5(4) 107_443 . 310_344 N
Si1 OII' O2 105.5(8) 107_433 . 107_433 N
Si1 OII' O2 60.99(35) 107_433 . 111_433 N
Si1 OII' O2 106.5(8) 107_433 . 208_343 N
Si1 OII' O2 134.2(13) 107_433 . 209_343 N
Si1 OII' O2 57.84(34) 107_433 . 310_334 N
Si1 OII' O2 22.70(18) 107_433 . 312_334 N
Si1 OII' O3 64.3(6) 107_433 . -105_444 N
Si1 OII' O3 26.22(22) 107_433 . -206_444 N
Si1 OII' O3 93.9(11) 107_433 . -304_444 N
Si1 OII' SI' 52.49(33) 107_433 . 107_433 N
Si1 OII' SI' 142.3(10) 107_433 . 111_433 N
Si1 OII' SI' 94.8(5) 107_433 . -105_444 N
Si1 OII' SII 54.9(6) 107_555 . 1_555 N
Si1 OII' OII' 151.3(5) 107_533 . 107_533 N
Si1 OII' OII' 93.4(6) 107_533 . 111_533 N
Si1 OII' OII' 118.2(5) 107_533 . -105_544 N
Si1 OII' Si1 90.2(8) 208_344 . 312_335 N
Si1 OII' Si2 47.5(4) 208_443 . 111_533 N
Si1 OII' Si2 107.6(12) 208_443 . 209_443 N
Si1 OII' Si2 47.8(4) 208_443 . 310_434 N
Si1 OII' Al1 47.5(4) 208_353 . 111_443 N
Si1 OII' Al1 107.6(12) 208_353 . 209_353 N
Si1 OII' Al1 47.8(4) 208_353 . 310_344 N
Si1 OII' O2 22.70(18) 208_343 . 107_433 N
Si1 OII' O2 57.84(34) 208_343 . 111_433 N
Si1 OII' O2 105.5(8) 208_343 . 208_343 N
Si1 OII' O2 60.99(35) 208_343 . 209_343 N
Si1 OII' O2 134.2(13) 208_343 . 310_334 N
Si1 OII' O2 106.5(8) 208_343 . 312_334 N
Si1 OII' O3 93.9(11) 208_343 . -105_444 N
Si1 OII' O3 64.3(6) 208_343 . -206_444 N
Si1 OII' O3 26.22(22) 208_343 . -304_444 N
Si1 OII' SI' 94.8(5) 208_343 . 107_433 N
Si1 OII' SI' 52.49(33) 208_343 . 111_433 N
Si1 OII' SI' 142.3(10) 208_343 . -105_444 N
Si1 OII' SII 54.9(6) 208_465 . 1_555 N
Si1 OII' OII' 118.2(5) 208_443 . 107_533 N
Si1 OII' OII' 151.3(5) 208_443 . 111_533 N
Si1 OII' OII' 93.4(6) 208_443 . -105_544 N
Si1 OII' Si2 47.8(4) 312_434 . 111_533 N
Si1 OII' Si2 47.5(4) 312_434 . 209_443 N
Si1 OII' Si2 107.6(12) 312_434 . 310_434 N
Si1 OII' Al1 47.8(4) 312_344 . 111_443 N
Si1 OII' Al1 47.5(4) 312_344 . 209_353 N
Si1 OII' Al1 107.6(12) 312_344 . 310_344 N
Si1 OII' O2 106.5(8) 312_334 . 107_433 N
Si1 OII' O2 134.2(13) 312_334 . 111_433 N
Si1 OII' O2 22.70(18) 312_334 . 208_343 N
Si1 OII' O2 57.84(34) 312_334 . 209_343 N
Si1 OII' O2 60.99(35) 312_334 . 310_334 N
Si1 OII' O2 105.5(8) 312_334 . 312_334 N
Si1 OII' O3 26.22(22) 312_334 . -105_444 N
Si1 OII' O3 93.9(11) 312_334 . -206_444 N
Si1 OII' O3 64.3(6) 312_334 . -304_444 N
Si1 OII' SI' 142.3(10) 312_334 . 107_433 N
Si1 OII' SI' 94.8(5) 312_334 . 111_433 N
Si1 OII' SI' 52.49(33) 312_334 . -105_444 N
Si1 OII' SII 54.9(6) 312_456 . 1_555 N
Si1 OII' OII' 93.4(6) 312_434 . 107_533 N
Si1 OII' OII' 118.2(5) 312_434 . 111_533 N
Si1 OII' OII' 151.3(5) 312_434 . -105_544 N
Si2 OII' Si2 87.1(8) 111_533 . 209_443 N
Si2 OII' Si2 87.1(8) 111_533 . 310_434 N
Si2 OII' Al1 0.0 111_443 . 111_443 N
Si2 OII' Al1 87.1(8) 111_443 . 209_353 N
Si2 OII' Al1 87.1(8) 111_443 . 310_344 N
Si2 OII' O2 59.2(4) 111_433 . 107_433 N
Si2 OII' O2 104.6(8) 111_433 . 111_433 N
Si2 OII' O2 58.4(4) 111_433 . 208_343 N
Si2 OII' O2 26.67(20) 111_433 . 209_343 N
Si2 OII' O2 107.6(8) 111_433 . 310_334 N
Si2 OII' O2 130.3(13) 111_433 . 312_334 N
Si2 OII' O3 64.6(7) 111_433 . -105_444 N
Si2 OII' O3 91.1(11) 111_433 . -206_444 N
Si2 OII' O3 23.09(21) 111_433 . -304_444 N
Si2 OII' SI' 140.4(11) 111_433 . 107_433 N
Si2 OII' SI' 53.8(4) 111_433 . 111_433 N
Si2 OII' SI' 95.8(5) 111_433 . -105_444 N
Si2 OII' SII 52.7(6) 111_555 . 1_555 N
Si2 OII' OII' 95.7(5) 111_533 . 107_533 N
Si2 OII' OII' 153.5(4) 111_533 . 111_533 N
Si2 OII' OII' 119.4(4) 111_533 . -105_544 N
Si2 OII' Si2 87.1(8) 209_443 . 310_434 N
Si2 OII' Al1 87.1(8) 209_353 . 111_443 N
Si2 OII' Al1 0.0 209_353 . 209_353 N
Si2 OII' Al1 87.1(8) 209_353 . 310_344 N
Si2 OII' O2 130.3(13) 209_343 . 107_433 N
Si2 OII' O2 107.6(8) 209_343 . 111_433 N
Si2 OII' O2 59.2(4) 209_343 . 208_343 N
Si2 OII' O2 104.6(8) 209_343 . 209_343 N
Si2 OII' O2 26.67(20) 209_343 . 310_334 N
Si2 OII' O2 58.4(4) 209_343 . 312_334 N
Si2 OII' O3 23.09(21) 209_343 . -105_444 N
Si2 OII' O3 64.6(7) 209_343 . -206_444 N
Si2 OII' O3 91.1(11) 209_343 . -304_444 N
Si2 OII' SI' 95.8(5) 209_343 . 107_433 N
Si2 OII' SI' 140.4(11) 209_343 . 111_433 N
Si2 OII' SI' 53.8(4) 209_343 . -105_444 N
Si2 OII' SII 52.7(6) 209_465 . 1_555 N
Si2 OII' OII' 119.4(4) 209_443 . 107_533 N
Si2 OII' OII' 95.7(5) 209_443 . 111_533 N
Si2 OII' OII' 153.5(4) 209_443 . -105_544 N
Si2 OII' Al1 87.1(8) 310_344 . 111_443 N
Si2 OII' Al1 87.1(8) 310_344 . 209_353 N
Si2 OII' Al1 0.0 310_344 . 310_344 N
Si2 OII' O2 58.4(4) 310_334 . 107_433 N
Si2 OII' O2 26.67(20) 310_334 . 111_433 N
Si2 OII' O2 130.3(13) 310_334 . 208_343 N
Si2 OII' O2 107.6(8) 310_334 . 209_343 N
Si2 OII' O2 104.6(8) 310_334 . 310_334 N
Si2 OII' O2 59.2(4) 310_334 . 312_334 N
Si2 OII' O3 91.1(11) 310_334 . -105_444 N
Si2 OII' O3 23.09(21) 310_334 . -206_444 N
Si2 OII' O3 64.6(7) 310_334 . -304_444 N
Si2 OII' SI' 53.8(4) 310_334 . 107_433 N
Si2 OII' SI' 95.8(5) 310_334 . 111_433 N
Si2 OII' SI' 140.4(11) 310_334 . -105_444 N
Si2 OII' SII 52.7(6) 310_456 . 1_555 N
Si2 OII' OII' 153.5(4) 310_434 . 107_533 N
Si2 OII' OII' 119.4(4) 310_434 . 111_533 N
Si2 OII' OII' 95.7(5) 310_434 . -105_544 N
Al1 OII' Al1 87.1(8) 111_443 . 209_353 N
Al1 OII' Al1 87.1(8) 111_443 . 310_344 N
Al1 OII' O2 59.2(4) 111_433 . 107_433 N
Al1 OII' O2 104.6(8) 111_433 . 111_433 N
Al1 OII' O2 58.4(4) 111_433 . 208_343 N
Al1 OII' O2 26.67(20) 111_433 . 209_343 N
Al1 OII' O2 107.6(8) 111_433 . 310_334 N
Al1 OII' O2 130.3(13) 111_433 . 312_334 N
Al1 OII' O3 64.6(7) 111_433 . -105_444 N
Al1 OII' O3 91.1(11) 111_433 . -206_444 N
Al1 OII' O3 23.09(21) 111_433 . -304_444 N
Al1 OII' SI' 140.4(11) 111_433 . 107_433 N
Al1 OII' SI' 53.8(4) 111_433 . 111_433 N
Al1 OII' SI' 95.8(5) 111_433 . -105_444 N
Al1 OII' SII 52.7(6) 111_555 . 1_555 N
Al1 OII' OII' 95.7(5) 111_533 . 107_533 N
Al1 OII' OII' 153.5(4) 111_533 . 111_533 N
Al1 OII' OII' 119.4(4) 111_533 . -105_544 N
Al1 OII' Al1 87.1(8) 209_353 . 310_344 N
Al1 OII' O2 130.3(13) 209_343 . 107_433 N
Al1 OII' O2 107.6(8) 209_343 . 111_433 N
Al1 OII' O2 59.2(4) 209_343 . 208_343 N
Al1 OII' O2 104.6(8) 209_343 . 209_343 N
Al1 OII' O2 26.67(20) 209_343 . 310_334 N
Al1 OII' O2 58.4(4) 209_343 . 312_334 N
Al1 OII' O3 23.09(21) 209_343 . -105_444 N
Al1 OII' O3 64.6(7) 209_343 . -206_444 N
Al1 OII' O3 91.1(11) 209_343 . -304_444 N
Al1 OII' SI' 95.8(5) 209_343 . 107_433 N
Al1 OII' SI' 140.4(11) 209_343 . 111_433 N
Al1 OII' SI' 53.8(4) 209_343 . -105_444 N
Al1 OII' SII 52.7(6) 209_465 . 1_555 N
Al1 OII' OII' 119.4(4) 209_443 . 107_533 N
Al1 OII' OII' 95.7(5) 209_443 . 111_533 N
Al1 OII' OII' 153.5(4) 209_443 . -105_544 N
Al1 OII' O2 58.4(4) 310_334 . 107_433 N
Al1 OII' O2 26.67(20) 310_334 . 111_433 N
Al1 OII' O2 130.3(13) 310_334 . 208_343 N
Al1 OII' O2 107.6(8) 310_334 . 209_343 N
Al1 OII' O2 104.6(8) 310_334 . 310_334 N
Al1 OII' O2 59.2(4) 310_334 . 312_334 N
Al1 OII' O3 91.1(11) 310_334 . -105_444 N
Al1 OII' O3 23.09(21) 310_334 . -206_444 N
Al1 OII' O3 64.6(7) 310_334 . -304_444 N
Al1 OII' SI' 53.8(4) 310_334 . 107_433 N
Al1 OII' SI' 95.8(5) 310_334 . 111_433 N
Al1 OII' SI' 140.4(11) 310_334 . -105_444 N
Al1 OII' SII 52.7(6) 310_456 . 1_555 N
Al1 OII' OII' 153.5(4) 310_434 . 107_533 N
Al1 OII' OII' 119.4(4) 310_434 . 111_533 N
Al1 OII' OII' 95.7(5) 310_434 . -105_544 N
O2 OII' O2 56.14(19) 107_433 . 111_433 N
O2 OII' O2 115.5(5) 107_433 . 208_343 N
O2 OII' O2 61.23(19) 107_433 . 209_343 N
O2 OII' O2 156.7(15) 107_433 . 310_334 N
O2 OII' O2 115.5(5) 107_433 . 312_334 N
O2 OII' O3 115.5(12) 107_433 . -105_444 N
O2 OII' O3 79.6(6) 107_433 . -206_444 N
O2 OII' O3 43.81(25) 107_433 . -304_444 N
O2 OII' SI' 90.89(10) 107_433 . 107_433 N
O2 OII' SI' 37.47(13) 107_433 . 111_433 N
O2 OII' SI' 151.34(21) 107_433 . -105_444 N
O2 OII' SII 77.6(7) 107_555 . 1_555 N
O2 OII' OII' 100.7(6) 107_533 . 107_533 N
O2 OII' OII' 131.2(7) 107_533 . 111_533 N
O2 OII' OII' 71.5(7) 107_533 . -105_544 N
O2 OII' O2 156.7(15) 111_433 . 208_343 N
O2 OII' O2 116.6(5) 111_433 . 209_343 N
O2 OII' O2 116.6(5) 111_433 . 310_334 N
O2 OII' O2 61.23(19) 111_433 . 312_334 N
O2 OII' O3 116.6(12) 111_433 . -105_444 N
O2 OII' O3 44.57(24) 111_433 . -206_444 N
O2 OII' O3 81.8(6) 111_433 . -304_444 N
O2 OII' SI' 37.02(11) 111_433 . 107_433 N
O2 OII' SI' 90.12(8) 111_433 . 111_433 N
O2 OII' SI' 151.94(12) 111_433 . -105_444 N
O2 OII' SII 79.3(7) 111_555 . 1_555 N
O2 OII' OII' 129.4(7) 111_533 . 107_533 N
O2 OII' OII' 99.6(6) 111_533 . 111_533 N
O2 OII' OII' 69.7(7) 111_533 . -105_544 N
O2 OII' O2 56.14(19) 208_343 . 209_343 N
O2 OII' O2 61.23(19) 208_343 . 310_334 N
O2 OII' O2 115.5(5) 208_343 . 312_334 N
O2 OII' O3 43.81(25) 208_343 . -105_444 N
O2 OII' O3 115.5(12) 208_343 . -206_444 N
O2 OII' O3 79.6(6) 208_343 . -304_444 N
O2 OII' SI' 151.34(21) 208_343 . 107_433 N
O2 OII' SI' 90.89(10) 208_343 . 111_433 N
O2 OII' SI' 37.47(13) 208_343 . -105_444 N
O2 OII' SII 77.6(7) 208_465 . 1_555 N
O2 OII' OII' 71.5(7) 208_443 . 107_533 N
O2 OII' OII' 100.7(6) 208_443 . 111_533 N
O2 OII' OII' 131.2(7) 208_443 . -105_544 N
O2 OII' O2 116.6(5) 209_343 . 310_334 N
O2 OII' O2 156.7(15) 209_343 . 312_334 N
O2 OII' O3 81.8(6) 209_343 . -105_444 N
O2 OII' O3 116.6(12) 209_343 . -206_444 N
O2 OII' O3 44.57(24) 209_343 . -304_444 N
O2 OII' SI' 151.94(12) 209_343 . 107_433 N
O2 OII' SI' 37.02(11) 209_343 . 111_433 N
O2 OII' SI' 90.12(8) 209_343 . -105_444 N
O2 OII' SII 79.3(7) 209_465 . 1_555 N
O2 OII' OII' 69.7(7) 209_443 . 107_533 N
O2 OII' OII' 129.4(7) 209_443 . 111_533 N
O2 OII' OII' 99.6(6) 209_443 . -105_544 N
O2 OII' O2 56.14(19) 310_334 . 312_334 N
O2 OII' O3 44.57(24) 310_334 . -105_444 N
O2 OII' O3 81.8(6) 310_334 . -206_444 N
O2 OII' O3 116.6(12) 310_334 . -304_444 N
O2 OII' SI' 90.12(8) 310_334 . 107_433 N
O2 OII' SI' 151.94(12) 310_334 . 111_433 N
O2 OII' SI' 37.02(11) 310_334 . -105_444 N
O2 OII' SII 79.3(7) 310_456 . 1_555 N
O2 OII' OII' 99.6(6) 310_434 . 107_533 N
O2 OII' OII' 69.7(7) 310_434 . 111_533 N
O2 OII' OII' 129.4(7) 310_434 . -105_544 N
O2 OII' O3 79.6(6) 312_334 . -105_444 N
O2 OII' O3 43.81(25) 312_334 . -206_444 N
O2 OII' O3 115.5(12) 312_334 . -304_444 N
O2 OII' SI' 37.47(13) 312_334 . 107_433 N
O2 OII' SI' 151.34(21) 312_334 . 111_433 N
O2 OII' SI' 90.89(10) 312_334 . -105_444 N
O2 OII' SII 77.6(7) 312_456 . 1_555 N
O2 OII' OII' 131.2(7) 312_434 . 107_533 N
O2 OII' OII' 71.5(7) 312_434 . 111_533 N
O2 OII' OII' 100.7(6) 312_434 . -105_544 N
O3 OII' O3 72.4(9) -105_444 . -206_444 N
O3 OII' O3 72.4(9) -105_444 . -304_444 N
O3 OII' SI' 116.1(8) -105_444 . 107_433 N
O3 OII' SI' 117.3(9) -105_444 . 111_433 N
O3 OII' SI' 55.91(33) -105_444 . -105_444 N
O3 OII' SII 43.0(6) -105_566 . 1_555 N
O3 OII' OII' 114.0(5) -105_544 . 107_533 N
O3 OII' OII' 113.3(5) -105_544 . 111_533 N
O3 OII' OII' 172.3(6) -105_544 . -105_544 N
O3 OII' O3 72.4(9) -206_444 . -304_444 N
O3 OII' SI' 55.91(33) -206_444 . 107_433 N
O3 OII' SI' 116.1(8) -206_444 . 111_433 N
O3 OII' SI' 117.3(9) -206_444 . -105_444 N
O3 OII' SII 43.0(6) -206_566 . 1_555 N
O3 OII' OII' 172.3(6) -206_544 . 107_533 N
O3 OII' OII' 114.0(5) -206_544 . 111_533 N
O3 OII' OII' 113.3(5) -206_544 . -105_544 N
O3 OII' SI' 117.3(9) -304_444 . 107_433 N
O3 OII' SI' 55.91(33) -304_444 . 111_433 N
O3 OII' SI' 116.1(8) -304_444 . -105_444 N
O3 OII' SII 43.0(6) -304_566 . 1_555 N
O3 OII' OII' 113.3(5) -304_544 . 107_533 N
O3 OII' OII' 172.3(6) -304_544 . 111_533 N
O3 OII' OII' 114.0(5) -304_544 . -105_544 N
SI' OII' SI' 117.7(5) 107_433 . 111_433 N
SI' OII' SI' 117.7(5) 107_433 . -105_444 N
SI' OII' SII 98.9(9) 107_555 . 1_555 N
SI' OII' OII' 116.4(9) 107_533 . 107_533 N
SI' OII' OII' 65.7(8) 107_533 . 111_533 N
SI' OII' OII' 65.7(8) 107_533 . -105_544 N
SI' OII' SI' 117.7(5) 111_433 . -105_444 N
SI' OII' SII 98.9(9) 111_555 . 1_555 N
SI' OII' OII' 65.7(8) 111_533 . 107_533 N
SI' OII' OII' 116.4(9) 111_533 . 111_533 N
SI' OII' OII' 65.7(8) 111_533 . -105_544 N
SI' OII' SII 98.9(9) -105_566 . 1_555 N
SI' OII' OII' 65.7(8) -105_544 . 107_533 N
SI' OII' OII' 65.7(8) -105_544 . 111_533 N
SI' OII' OII' 116.4(9) -105_544 . -105_544 N
SII OII' OII' 144.7356 1_555 . 107_533 N
SII OII' OII' 144.7356 1_555 . 111_533 N
SII OII' OII' 144.7356 1_555 . -105_544 N
OII' OII' OII' 60.00010(20) 107_533 . 111_533 N
OII' OII' OII' 60.00000(20) 107_533 . -105_544 N
OII' OII' OII' 60.00000(20) 111_533 . -105_544 N
Si1 DII'1 Si1 71.7(9) 107_434 . -105_445 N
Si1 DII'1 Si1 98.3(18) 107_434 . 312_335 N
Si1 DII'1 Si2 55.0(10) 107_533 . 209_443 N
Si1 DII'1 Al1 55.0(10) 107_443 . 209_353 N
Si1 DII'1 O2 119.8(22) 107_433 . 208_343 N
Si1 DII'1 O2 69.5(13) 107_433 . 310_334 N
Si1 DII'1 O2 25.1(6) 107_433 . 312_334 N
Si1 DII'1 O3 72.3(15) 107_433 . -105_444 N
Si1 DII'1 O3 94.3(11) 107_433 . 209_343 N
Si1 DII'1 O3 29.0(7) 107_433 . -206_444 N
Si1 DII'1 O3 88.5(14) 107_433 . -304_444 N
Si1 DII'1 O4 25.7(5) 107_433 . 1_555 N
Si1 DII'1 SI' 56.3(15) 107_433 . 107_433 N
Si1 DII'1 SI' 122.9(14) 107_433 . 111_433 N
Si1 DII'1 SI' 119.3(14) 107_433 . -105_444 N
Si1 DII'1 SII 57.5(12) 107_555 . 1_555 N
Si1 DII'1 OII' 104(6) 107_533 . 1_555 N
Si1 DII'1 OII' 165.6(32) 107_533 . 107_533 N
Si1 DII'1 OII' 111(4) 107_533 . 111_533 N
Si1 DII'1 OII' 114.2(29) 107_533 . -105_544 N
Si1 DII'1 DII'1 83(5) 107_433 . 2_555 N
Si1 DII'1 DII'1 126.4(35) 107_433 . 3_555 N
Si1 DII'1 DII'1 155.9(34) 107_433 . 107_433 N
Si1 DII'1 DII'1 129(5) 107_433 . 111_433 N
Si1 DII'1 Si1 90.4(14) -105_445 . 312_335 N
Si1 DII'1 Si2 51.54(34) -105_544 . 209_443 N
Si1 DII'1 Al1 51.54(34) -105_454 . 209_353 N
Si1 DII'1 O2 88.1(14) -105_444 . 208_343 N
Si1 DII'1 O2 20.6(4) -105_444 . 310_334 N
Si1 DII'1 O2 62.7(8) -105_444 . 312_334 N
Si1 DII'1 O3 76.8(9) -105_444 . -105_444 N
Si1 DII'1 O3 25.96(16) -105_444 . 209_343 N
Si1 DII'1 O3 100.5(16) -105_444 . -206_444 N
Si1 DII'1 O3 142.0(22) -105_444 . -304_444 N
Si1 DII'1 O4 62.4(6) -105_444 . 1_555 N
Si1 DII'1 SI' 96.1(19) -105_444 . 107_433 N
Si1 DII'1 SI' 165.0(25) -105_444 . 111_433 N
Si1 DII'1 SI' 56.03(11) -105_444 . -105_444 N
Si1 DII'1 SII 108.6(15) -105_566 . 1_555 N
Si1 DII'1 OII' 175(7) -105_544 . 1_555 N
Si1 DII'1 OII' 115.9(17) -105_544 . 107_533 N
Si1 DII'1 OII' 76.7(15) -105_544 . 111_533 N
Si1 DII'1 OII' 130.5(25) -105_544 . -105_544 N
Si1 DII'1 DII'1 145(8) -105_444 . 2_555 N
Si1 DII'1 DII'1 155(8) -105_444 . 3_555 N
Si1 DII'1 DII'1 100.4(20) -105_444 . 107_433 N
Si1 DII'1 DII'1 71.4(29) -105_444 . 111_433 N
Si1 DII'1 Si2 52.9(14) 312_434 . 209_443 N
Si1 DII'1 Al1 52.9(14) 312_344 . 209_353 N
Si1 DII'1 O2 23.8(7) 312_334 . 208_343 N
Si1 DII'1 O2 70.9(18) 312_334 . 310_334 N
Si1 DII'1 O2 120.1(19) 312_334 . 312_334 N
Si1 DII'1 O3 26.6(10) 312_334 . -105_444 N
Si1 DII'1 O3 99.8(16) 312_334 . 209_343 N
Si1 DII'1 O3 95.0(19) 312_334 . -206_444 N
Si1 DII'1 O3 60.0(13) 312_334 . -304_444 N
Si1 DII'1 O4 74.8(16) 312_334 . 1_555 N
Si1 DII'1 SI' 149.4(23) 312_334 . 107_433 N
Si1 DII'1 SI' 84.4(17) 312_334 . 111_433 N
Si1 DII'1 SI' 57.3(21) 312_334 . -105_444 N
Si1 DII'1 SII 55.7(14) 312_456 . 1_555 N
Si1 DII'1 OII' 93(6) 312_434 . 1_555 N
Si1 DII'1 OII' 93.9(28) 312_434 . 107_533 N
Si1 DII'1 OII' 141.3(34) 312_434 . 111_533 N
Si1 DII'1 OII' 133.1(21) 312_434 . -105_544 N
Si1 DII'1 DII'1 118(4) 312_334 . 2_555 N
Si1 DII'1 DII'1 71(5) 312_334 . 3_555 N
Si1 DII'1 DII'1 105(4) 312_334 . 107_433 N
Si1 DII'1 DII'1 115.9(27) 312_334 . 111_433 N
Si2 DII'1 Al1 0.0 209_353 . 209_353 N
Si2 DII'1 O2 67.8(17) 209_343 . 208_343 N
Si2 DII'1 O2 32.9(7) 209_343 . 310_334 N
Si2 DII'1 O2 69.7(12) 209_343 . 312_334 N
Si2 DII'1 O3 29.0(6) 209_343 . -105_444 N
Si2 DII'1 O3 74.98(31) 209_343 . 209_343 N
Si2 DII'1 O3 71.5(14) 209_343 . -206_444 N
Si2 DII'1 O3 90.5(18) 209_343 . -304_444 N
Si2 DII'1 O4 29.8(6) 209_343 . 1_555 N
Si2 DII'1 SI' 110.1(23) 209_343 . 107_433 N
Si2 DII'1 SI' 131.7(25) 209_343 . 111_433 N
Si2 DII'1 SI' 68.4(15) 209_343 . -105_444 N
Si2 DII'1 SII 58.7(13) 209_465 . 1_555 N
Si2 DII'1 OII' 128(6) 209_443 . 1_555 N
Si2 DII'1 OII' 139(4) 209_443 . 107_533 N
Si2 DII'1 OII' 128.2(14) 209_443 . 111_533 N
Si2 DII'1 OII' 169.0(32) 209_443 . -105_544 N
Si2 DII'1 DII'1 128.9(27) 209_343 . 2_555 N
Si2 DII'1 DII'1 121(4) 209_343 . 3_555 N
Si2 DII'1 DII'1 137(4) 209_343 . 107_433 N
Si2 DII'1 DII'1 118.8(16) 209_343 . 111_433 N
Al1 DII'1 O2 67.8(17) 209_343 . 208_343 N
Al1 DII'1 O2 32.9(7) 209_343 . 310_334 N
Al1 DII'1 O2 69.7(12) 209_343 . 312_334 N
Al1 DII'1 O3 29.0(6) 209_343 . -105_444 N
Al1 DII'1 O3 74.98(31) 209_343 . 209_343 N
Al1 DII'1 O3 71.5(14) 209_343 . -206_444 N
Al1 DII'1 O3 90.5(18) 209_343 . -304_444 N
Al1 DII'1 O4 29.8(6) 209_343 . 1_555 N
Al1 DII'1 SI' 110.1(23) 209_343 . 107_433 N
Al1 DII'1 SI' 131.7(25) 209_343 . 111_433 N
Al1 DII'1 SI' 68.4(15) 209_343 . -105_444 N
Al1 DII'1 SII 58.7(13) 209_465 . 1_555 N
Al1 DII'1 OII' 128(6) 209_443 . 1_555 N
Al1 DII'1 OII' 139(4) 209_443 . 107_533 N
Al1 DII'1 OII' 128.2(14) 209_443 . 111_533 N
Al1 DII'1 OII' 169.0(32) 209_443 . -105_544 N
Al1 DII'1 DII'1 128.9(27) 209_343 . 2_555 N
Al1 DII'1 DII'1 121(4) 209_343 . 3_555 N
Al1 DII'1 DII'1 137(4) 209_343 . 107_433 N
Al1 DII'1 DII'1 118.8(16) 209_343 . 111_433 N
O2 DII'1 O2 73.0(19) 208_343 . 310_334 N
O2 DII'1 O2 137.4(19) 208_343 . 312_334 N
O2 DII'1 O3 47.7(16) 208_343 . -105_444 N
O2 DII'1 O3 87.5(14) 208_343 . 209_343 N
O2 DII'1 O3 118.7(24) 208_343 . -206_444 N
O2 DII'1 O3 73.8(17) 208_343 . -304_444 N
O2 DII'1 O4 94.6(20) 208_343 . 1_555 N
O2 DII'1 SI' 172.5(21) 208_343 . 107_433 N
O2 DII'1 SI' 81.5(17) 208_343 . 111_433 N
O2 DII'1 SI' 39.8(17) 208_343 . -105_444 N
O2 DII'1 SII 78.6(21) 208_465 . 1_555 N
O2 DII'1 OII' 96(7) 208_443 . 1_555 N
O2 DII'1 OII' 73.7(23) 208_443 . 107_533 N
O2 DII'1 OII' 118.1(31) 208_443 . 111_533 N
O2 DII'1 OII' 121.5(23) 208_443 . -105_544 N
O2 DII'1 DII'1 126(6) 208_343 . 2_555 N
O2 DII'1 DII'1 68(6) 208_343 . 3_555 N
O2 DII'1 DII'1 81.8(34) 208_343 . 107_433 N
O2 DII'1 DII'1 92.8(23) 208_343 . 111_433 N
O2 DII'1 O2 69.9(12) 310_334 . 312_334 N
O2 DII'1 O3 56.3(12) 310_334 . -105_444 N
O2 DII'1 O3 42.1(4) 310_334 . 209_343 N
O2 DII'1 O3 95.3(18) 310_334 . -206_444 N
O2 DII'1 O3 122.2(26) 310_334 . -304_444 N
O2 DII'1 O4 52.0(9) 310_334 . 1_555 N
O2 DII'1 SI' 109.5(24) 310_334 . 107_433 N
O2 DII'1 SI' 154(4) 310_334 . 111_433 N
O2 DII'1 SI' 50.5(7) 310_334 . -105_444 N
O2 DII'1 SII 91.5(19) 310_456 . 1_555 N
O2 DII'1 OII' 160(7) 310_434 . 1_555 N
O2 DII'1 OII' 122.1(25) 310_434 . 107_533 N
O2 DII'1 OII' 96.3(16) 310_434 . 111_533 N
O2 DII'1 OII' 150.9(27) 310_434 . -105_544 N
O2 DII'1 DII'1 152(7) 310_334 . 2_555 N
O2 DII'1 DII'1 141(8) 310_334 . 3_555 N
O2 DII'1 DII'1 111.0(31) 310_334 . 107_433 N
O2 DII'1 DII'1 86.6(25) 310_334 . 111_433 N
O2 DII'1 O3 93.4(17) 312_334 . -105_444 N
O2 DII'1 O3 78.8(10) 312_334 . 209_343 N
O2 DII'1 O3 47.0(12) 312_334 . -206_444 N
O2 DII'1 O3 109.7(18) 312_334 . -304_444 N
O2 DII'1 O4 45.4(9) 312_334 . 1_555 N
O2 DII'1 SI' 41.8(13) 312_334 . 107_433 N
O2 DII'1 SI' 131.8(20) 312_334 . 111_433 N
O2 DII'1 SI' 118.4(8) 312_334 . -105_444 N
O2 DII'1 SII 82.1(17) 312_456 . 1_555 N
O2 DII'1 OII' 112(6) 312_434 . 1_555 N
O2 DII'1 OII' 145.6(35) 312_434 . 107_533 N
O2 DII'1 OII' 86.4(31) 312_434 . 111_533 N
O2 DII'1 OII' 101.1(29) 312_434 . -105_544 N
O2 DII'1 DII'1 84(7) 312_334 . 2_555 N
O2 DII'1 DII'1 141(6) 312_334 . 3_555 N
O2 DII'1 DII'1 131.0(28) 312_334 . 107_433 N
O2 DII'1 DII'1 105(4) 312_334 . 111_433 N
O3 DII'1 O3 95.5(10) -105_444 . 209_343 N
O3 DII'1 O3 75.4(16) -105_444 . -206_444 N
O3 DII'1 O3 66.3(14) -105_444 . -304_444 N
O3 DII'1 O4 48.2(10) -105_444 . 1_555 N
O3 DII'1 SI' 127.3(26) -105_444 . 107_433 N
O3 DII'1 SI' 103.4(21) -105_444 . 111_433 N
O3 DII'1 SI' 67.9(22) -105_444 . -105_444 N
O3 DII'1 SII 43.8(11) -105_566 . 1_555 N
O3 DII'1 OII' 104(6) -105_544 . 1_555 N
O3 DII'1 OII' 120(4) -105_544 . 107_533 N
O3 DII'1 OII' 150.2(18) -105_544 . 111_533 N
O3 DII'1 OII' 152.6(18) -105_544 . -105_544 N
O3 DII'1 DII'1 118.6(13) -105_444 . 2_555 N
O3 DII'1 DII'1 92(4) -105_444 . 3_555 N
O3 DII'1 DII'1 129(5) -105_444 . 107_433 N
O3 DII'1 DII'1 129.7(17) -105_444 . 111_433 N
O3 DII'1 O3 123.1(18) 209_343 . -206_444 N
O3 DII'1 O3 159.8(27) 209_343 . -304_444 N
O3 DII'1 O4 88.3(5) 209_343 . 1_555 N
O3 DII'1 SI' 99.0(20) 209_343 . 107_433 N
O3 DII'1 SI' 141.7(20) 209_343 . 111_433 N
O3 DII'1 SI' 48.1(6) 209_343 . -105_444 N
O3 DII'1 SII 133.5(15) 209_465 . 1_555 N
O3 DII'1 OII' 157(6) 209_443 . 1_555 N
O3 DII'1 OII' 91.0(16) 209_443 . 107_533 N
O3 DII'1 OII' 55.2(12) 209_443 . 111_533 N
O3 DII'1 OII' 109.9(21) 209_443 . -105_544 N
O3 DII'1 DII'1 143(6) 209_343 . 2_555 N
O3 DII'1 DII'1 139(6) 209_343 . 3_555 N
O3 DII'1 DII'1 74.6(18) 209_343 . 107_433 N
O3 DII'1 DII'1 45.6(27) 209_343 . 111_433 N
O3 DII'1 O3 62.7(9) -206_444 . -304_444 N
O3 DII'1 O4 44.0(9) -206_444 . 1_555 N
O3 DII'1 SI' 54.4(15) -206_444 . 107_433 N
O3 DII'1 SI' 94.0(7) -206_444 . 111_433 N
O3 DII'1 SI' 139.7(26) -206_444 . -105_444 N
O3 DII'1 SII 40.9(8) -206_566 . 1_555 N
O3 DII'1 OII' 75(5) -206_544 . 1_555 N
O3 DII'1 OII' 142.4(9) -206_544 . 107_533 N
O3 DII'1 OII' 123(4) -206_544 . 111_533 N
O3 DII'1 OII' 97.8(21) -206_544 . -105_544 N
O3 DII'1 DII'1 59(4) -206_444 . 2_555 N
O3 DII'1 DII'1 97.9(35) -206_444 . 3_555 N
O3 DII'1 DII'1 151(4) -206_444 . 107_433 N
O3 DII'1 DII'1 148(5) -206_444 . 111_433 N
O3 DII'1 O4 85.7(15) -304_444 . 1_555 N
O3 DII'1 SI' 99.2(13) -304_444 . 107_433 N
O3 DII'1 SI' 44.1(4) -304_444 . 111_433 N
O3 DII'1 SI' 113.6(33) -304_444 . -105_444 N
O3 DII'1 SII 36.0(6) -304_566 . 1_555 N
O3 DII'1 OII' 38(5) -304_544 . 1_555 N
O3 DII'1 OII' 91.1(14) -304_544 . 107_533 N
O3 DII'1 OII' 141.3(16) -304_544 . 111_533 N
O3 DII'1 OII' 86.90(17) -304_544 . -105_544 N
O3 DII'1 DII'1 57.6(31) -304_444 . 2_555 N
O3 DII'1 DII'1 39.9(14) -304_444 . 3_555 N
O3 DII'1 DII'1 109.4(10) -304_444 . 107_433 N
O3 DII'1 DII'1 141(4) -304_444 . 111_433 N
O4 DII'1 SI' 81.9(20) 1_555 . 107_433 N
O4 DII'1 SI' 128.9(16) 1_555 . 111_433 N
O4 DII'1 SI' 97.2(17) 1_555 . -105_444 N
O4 DII'1 SII 49.7(10) 1_555 . 1_555 N
O4 DII'1 OII' 114(5) 1_555 . 1_555 N
O4 DII'1 OII' 168(4) 1_555 . 107_533 N
O4 DII'1 OII' 126.4(30) 1_555 . 111_533 N
O4 DII'1 OII' 139.2(31) 1_555 . -105_544 N
O4 DII'1 DII'1 103(4) 1_555 . 2_555 N
O4 DII'1 DII'1 125.0(7) 1_555 . 3_555 N
O4 DII'1 DII'1 162.6(19) 1_555 . 107_433 N
O4 DII'1 DII'1 132.8(34) 1_555 . 111_433 N
SI' DII'1 SI' 95.5(12) 107_433 . 111_433 N
SI' DII'1 SI' 147.0(26) 107_433 . -105_444 N
SI' DII'1 SII 94.1(20) 107_555 . 1_555 N
SI' DII'1 OII' 79(6) 107_533 . 1_555 N
SI' DII'1 OII' 109.6(26) 107_533 . 107_533 N
SI' DII'1 OII' 69.0(28) 107_533 . 111_533 N
SI' DII'1 OII' 59.8(17) 107_533 . -105_544 N
SI' DII'1 DII'1 49(6) 107_433 . 2_555 N
SI' DII'1 DII'1 108(6) 107_433 . 3_555 N
SI' DII'1 DII'1 103.5(30) 107_433 . 107_433 N
SI' DII'1 DII'1 94.4(31) 107_433 . 111_433 N
SI' DII'1 SI' 109.8(28) 111_433 . -105_444 N
SI' DII'1 SII 79.9(9) 111_555 . 1_555 N
SI' DII'1 OII' 20(4) 111_533 . 1_555 N
SI' DII'1 OII' 50.8(6) 111_533 . 107_533 N
SI' DII'1 OII' 98.8(18) 111_533 . 111_533 N
SI' DII'1 OII' 50.0(4) 111_533 . -105_544 N
SI' DII'1 DII'1 48(5) 111_433 . 2_555 N
SI' DII'1 DII'1 14(4) 111_433 . 3_555 N
SI' DII'1 DII'1 67.6(10) 111_433 . 107_433 N
SI' DII'1 DII'1 98.2(27) 111_433 . 111_433 N
SI' DII'1 SII 110.5(33) -105_566 . 1_555 N
SI' DII'1 OII' 129(8) -105_544 . 1_555 N
SI' DII'1 OII' 73.9(24) -105_544 . 107_533 N
SI' DII'1 OII' 86.0(21) -105_544 . 111_533 N
SI' DII'1 OII' 122.4(27) -105_544 . -105_544 N
SI' DII'1 DII'1 157(7) -105_444 . 2_555 N
SI' DII'1 DII'1 99(8) -105_444 . 3_555 N
SI' DII'1 DII'1 69(4) -105_444 . 107_433 N
SI' DII'1 DII'1 62.1(13) -105_444 . 111_433 N
SII DII'1 OII' 70(5) 1_555 . 1_555 N
SII DII'1 OII' 125.8(22) 1_555 . 107_533 N
SII DII'1 OII' 163(4) 1_555 . 111_533 N
SII DII'1 OII' 115.2(9) 1_555 . -105_544 N
SII DII'1 DII'1 75.4(4) 1_555 . 2_555 N
SII DII'1 DII'1 75.4(4) 1_555 . 3_555 N
SII DII'1 DII'1 144.1(19) 1_555 . 107_433 N
SII DII'1 DII'1 171(4) 1_555 . 111_433 N
OII' DII'1 OII' 68(5) 1_555 . 107_533 N
OII' DII'1 OII' 103(6) 1_555 . 111_533 N
OII' DII'1 OII' 49(5) 1_555 . -105_544 N
OII' DII'1 DII'1 30.2(5) 1_555 . 2_555 N
OII' DII'1 DII'1 30.2(5) 1_555 . 3_555 N
OII' DII'1 DII'1 83(4) 1_555 . 107_433 N
OII' DII'1 DII'1 111(5) 1_555 . 111_433 N
OII' DII'1 OII' 61.4(21) 107_533 . 111_533 N
OII' DII'1 OII' 51.5(13) 107_533 . -105_544 N
OII' DII'1 DII'1 84.7(30) 107_433 . 2_555 N
OII' DII'1 DII'1 51.3(28) 107_433 . 3_555 N
OII' DII'1 DII'1 18.4(11) 107_433 . 107_433 N
OII' DII'1 DII'1 49.6(23) 107_433 . 111_433 N
OII' DII'1 OII' 54.9(19) 111_533 . -105_544 N
OII' DII'1 DII'1 91(4) 111_433 . 2_555 N
OII' DII'1 DII'1 106.9(12) 111_433 . 3_555 N
OII' DII'1 DII'1 44.7(10) 111_433 . 107_433 N
OII' DII'1 DII'1 25.4(13) 111_433 . 111_433 N
OII' DII'1 DII'1 41.7(10) -105_444 . 2_555 N
OII' DII'1 DII'1 62.5(27) -105_444 . 3_555 N
OII' DII'1 DII'1 53.2(17) -105_444 . 107_433 N
OII' DII'1 DII'1 68.7(13) -105_444 . 111_433 N
DII'1 DII'1 DII'1 60.0000(6) 2_555 . 3_555 N
DII'1 DII'1 DII'1 92.9(4) 2_555 . 107_433 N
DII'1 DII'1 DII'1 109.73(20) 2_555 . 111_433 N
DII'1 DII'1 DII'1 69.5(18) 3_555 . 107_433 N
DII'1 DII'1 DII'1 101(5) 3_555 . 111_433 N
DII'1 DII'1 DII'1 31.4(32) 107_433 . 111_433 N
O2 DII'2 O2 60.5(12) 107_433 . 209_343 N
O2 DII'2 O3 40.9(7) 107_433 . -304_444 N
O2 DII'2 SI' 120.7(11) 107_433 . 1_555 N
O2 DII'2 SI' 87.9(15) 107_433 . 107_433 N
O2 DII'2 SI' 36.6(8) 107_433 . 111_433 N
O2 DII'2 SI' 139.5(20) 107_433 . -105_444 N
O2 DII'2 OII' 80(4) 107_533 . 1_555 N
O2 DII'2 OII' 118.2(33) 107_533 . 107_533 N
O2 DII'2 OII' 151.0(32) 107_533 . 111_533 N
O2 DII'2 OII' 76.6(22) 107_533 . -105_544 N
O2 DII'2 DII'1 117(4) 107_433 . 1_555 N
O2 DII'2 DII'1 57(5) 107_433 . 2_555 N
O2 DII'2 DII'1 67(6) 107_433 . 3_555 N
O2 DII'2 DII'1 136(4) 107_433 . 107_433 N
O2 DII'2 DII'1 174(4) 107_433 . 111_433 N
O2 DII'2 DII'1 43.6(18) 107_433 . -105_444 N
O2 DII'2 DII'1 132.9(33) 107_433 . 208_343 N
O2 DII'2 DII'1 92.3(32) 107_433 . 209_343 N
O2 DII'2 DII'1 118(4) 107_433 . -206_444 N
O2 DII'2 DII'1 90.7(29) 107_433 . 310_334 N
O2 DII'2 DII'1 88(4) 107_433 . 312_334 N
O2 DII'2 DII'1 134.8(23) 107_433 . -304_444 N
O2 DII'2 DII'2 153.25(32) 107_533 . 2_555 N
O2 DII'2 DII'2 117(13) 107_533 . 3_555 N
O2 DII'2 O3 41.7(9) 209_343 . -304_444 N
O2 DII'2 SI' 118.4(16) 209_343 . 1_555 N
O2 DII'2 SI' 141.8(16) 209_343 . 107_433 N
O2 DII'2 SI' 36.1(11) 209_343 . 111_433 N
O2 DII'2 SI' 86.9(18) 209_343 . -105_444 N
O2 DII'2 OII' 81(5) 209_443 . 1_555 N
O2 DII'2 OII' 74.1(29) 209_443 . 107_533 N
O2 DII'2 OII' 148.3(29) 209_443 . 111_533 N
O2 DII'2 OII' 117.7(32) 209_443 . -105_544 N
O2 DII'2 DII'1 102(6) 209_343 . 1_555 N
O2 DII'2 DII'1 102(6) 209_343 . 2_555 N
O2 DII'2 DII'1 27.7(30) 209_343 . 3_555 N
O2 DII'2 DII'1 97.2(34) 209_343 . 107_433 N
O2 DII'2 DII'1 123.7(29) 209_343 . 111_433 N
O2 DII'2 DII'1 95(5) 209_343 . -105_444 N
O2 DII'2 DII'1 153(4) 209_343 . 208_343 N
O2 DII'2 DII'1 144(4) 209_343 . 209_343 N
O2 DII'2 DII'1 58.8(34) 209_343 . -206_444 N
O2 DII'2 DII'1 66(5) 209_343 . 310_334 N
O2 DII'2 DII'1 105.6(29) 209_343 . 312_334 N
O2 DII'2 DII'1 151.6(25) 209_343 . -304_444 N
O2 DII'2 DII'2 110(13) 209_443 . 2_555 N
O2 DII'2 DII'2 154(4) 209_443 . 3_555 N
O3 DII'2 SI' 154.5(20) -304_444 . 1_555 N
O3 DII'2 SI' 100.4(12) -304_444 . 107_433 N
O3 DII'2 SI' 50.8(11) -304_444 . 111_433 N
O3 DII'2 SI' 98.9(14) -304_444 . -105_444 N
O3 DII'2 OII' 49(4) -304_544 . 1_555 N
O3 DII'2 OII' 116(4) -304_544 . 107_533 N
O3 DII'2 OII' 153.2(14) -304_544 . 111_533 N
O3 DII'2 OII' 117.5(28) -304_544 . -105_544 N
O3 DII'2 DII'1 84(4) -304_444 . 1_555 N
O3 DII'2 DII'1 61(5) -304_444 . 2_555 N
O3 DII'2 DII'1 31(5) -304_444 . 3_555 N
O3 DII'2 DII'1 138(4) -304_444 . 107_433 N
O3 DII'2 DII'1 146(4) -304_444 . 111_433 N
O3 DII'2 DII'1 84.3(24) -304_444 . -105_444 N
O3 DII'2 DII'1 165(5) -304_444 . 208_343 N
O3 DII'2 DII'1 128.8(35) -304_444 . 209_343 N
O3 DII'2 DII'1 94.5(30) -304_444 . -206_444 N
O3 DII'2 DII'1 104(5) -304_444 . 310_334 N
O3 DII'2 DII'1 126(4) -304_444 . 312_334 N
O3 DII'2 DII'1 128.2(17) -304_444 . -304_444 N
O3 DII'2 DII'2 114(5) -304_544 . 2_555 N
O3 DII'2 DII'2 117(4) -304_544 . 3_555 N
SI' DII'2 SI' 95.3(19) 1_555 . 107_433 N
SI' DII'2 SI' 103.7(9) 1_555 . 111_433 N
SI' DII'2 SI' 94.8(14) 1_555 . -105_444 N
SI' DII'2 OII' 156(6) 1_555 . 1_555 N
SI' DII'2 OII' 50.8(12) 1_555 . 107_533 N
SI' DII'2 OII' 52.3(6) 1_555 . 111_533 N
SI' DII'2 OII' 50.6(10) 1_555 . -105_544 N
SI' DII'2 DII'1 120(6) 1_555 . 1_555 N
SI' DII'2 DII'1 131(5) 1_555 . 2_555 N
SI' DII'2 DII'1 141(4) 1_555 . 3_555 N
SI' DII'2 DII'1 34.5(20) 1_555 . 107_433 N
SI' DII'2 DII'1 53.4(29) 1_555 . 111_433 N
SI' DII'2 DII'1 81.6(13) 1_555 . -105_444 N
SI' DII'2 DII'1 35.8(20) 1_555 . 208_343 N
SI' DII'2 DII'1 53.2(31) 1_555 . 209_343 N
SI' DII'2 DII'1 80.1(19) 1_555 . -206_444 N
SI' DII'2 DII'1 52(4) 1_555 . 310_334 N
SI' DII'2 DII'1 32.6(27) 1_555 . 312_334 N
SI' DII'2 DII'1 77.0(15) 1_555 . -304_444 N
SI' DII'2 DII'2 86.0(10) 1_555 . 2_555 N
SI' DII'2 DII'2 86.0(10) 1_555 . 3_555 N
SI' DII'2 SI' 123.1(22) 107_433 . 111_433 N
SI' DII'2 SI' 108.8(20) 107_433 . -105_444 N
SI' DII'2 OII' 73(5) 107_533 . 1_555 N
SI' DII'2 OII' 143.9(35) 107_533 . 107_533 N
SI' DII'2 OII' 66.7(23) 107_533 . 111_533 N
SI' DII'2 OII' 69.4(27) 107_533 . -105_544 N
SI' DII'2 DII'1 72(6) 107_433 . 1_555 N
SI' DII'2 DII'1 40(4) 107_433 . 2_555 N
SI' DII'2 DII'1 123.4(32) 107_433 . 3_555 N
SI' DII'2 DII'1 121(4) 107_433 . 107_433 N
SI' DII'2 DII'1 90.0(20) 107_433 . 111_433 N
SI' DII'2 DII'1 72(6) 107_433 . -105_444 N
SI' DII'2 DII'1 65(4) 107_433 . 208_343 N
SI' DII'2 DII'1 47.5(20) 107_433 . 209_343 N
SI' DII'2 DII'1 152(5) 107_433 . -206_444 N
SI' DII'2 DII'1 140(5) 107_433 . 310_334 N
SI' DII'2 DII'1 93.3(21) 107_433 . 312_334 N
SI' DII'2 DII'1 47.5(20) 107_433 . -304_444 N
SI' DII'2 DII'2 88(14) 107_533 . 2_555 N
SI' DII'2 DII'2 29(13) 107_533 . 3_555 N
SI' DII'2 SI' 122.0(29) 111_433 . -105_444 N
SI' DII'2 OII' 100(5) 111_533 . 1_555 N
SI' DII'2 OII' 82.3(30) 111_533 . 107_533 N
SI' DII'2 OII' 156.0(6) 111_533 . 111_533 N
SI' DII'2 OII' 82.7(24) 111_533 . -105_544 N
SI' DII'2 DII'1 133(6) 111_433 . 1_555 N
SI' DII'2 DII'1 93(6) 111_433 . 2_555 N
SI' DII'2 DII'1 59(5) 111_433 . 3_555 N
SI' DII'2 DII'1 103(4) 111_433 . 107_433 N
SI' DII'2 DII'1 143.4(22) 111_433 . 111_433 N
SI' DII'2 DII'1 59(4) 111_433 . -105_444 N
SI' DII'2 DII'1 135.8(6) 111_433 . 208_343 N
SI' DII'2 DII'1 108.1(33) 111_433 . 209_343 N
SI' DII'2 DII'1 84(4) 111_433 . -206_444 N
SI' DII'2 DII'1 58(4) 111_433 . 310_334 N
SI' DII'2 DII'1 77.8(32) 111_433 . 312_334 N
SI' DII'2 DII'1 170.3(29) 111_433 . -304_444 N
SI' DII'2 DII'2 145(15) 111_533 . 2_555 N
SI' DII'2 DII'2 152(15) 111_533 . 3_555 N
SI' DII'2 OII' 71.0(35) -105_544 . 1_555 N
SI' DII'2 OII' 68.3(20) -105_544 . 107_533 N
SI' DII'2 OII' 66.0(17) -105_544 . 111_533 N
SI' DII'2 OII' 143.5(30) -105_544 . -105_544 N
SI' DII'2 DII'1 43(5) -105_444 . 1_555 N
SI' DII'2 DII'1 114.6(34) -105_444 . 2_555 N
SI' DII'2 DII'1 73(5) -105_444 . 3_555 N
SI' DII'2 DII'1 65.7(24) -105_444 . 107_433 N
SI' DII'2 DII'1 46.9(26) -105_444 . 111_433 N
SI' DII'2 DII'1 176.5(23) -105_444 . -105_444 N
SI' DII'2 DII'1 87.1(20) -105_444 . 208_343 N
SI' DII'2 DII'1 126(5) -105_444 . 209_343 N
SI' DII'2 DII'1 45.2(34) -105_444 . -206_444 N
SI' DII'2 DII'1 97.6(28) -105_444 . 310_334 N
SI' DII'2 DII'1 126(4) -105_444 . 312_334 N
SI' DII'2 DII'1 67.3(29) -105_444 . -304_444 N
SI' DII'2 DII'2 23(12) -105_544 . 2_555 N
SI' DII'2 DII'2 82(13) -105_544 . 3_555 N
OII' DII'2 OII' 133(6) 1_555 . 107_533 N
OII' DII'2 OII' 104(6) 1_555 . 111_533 N
OII' DII'2 OII' 136(6) 1_555 . -105_544 N
OII' DII'2 DII'1 37.7(6) 1_555 . 1_555 N
OII' DII'2 DII'1 48.2(31) 1_555 . 2_555 N
OII' DII'2 DII'1 54(4) 1_555 . 3_555 N
OII' DII'2 DII'1 137(5) 1_555 . 107_433 N
OII' DII'2 DII'1 105(5) 1_555 . 111_433 N
OII' DII'2 DII'1 112(6) 1_555 . -105_444 N
OII' DII'2 DII'1 122(6) 1_555 . 208_343 N
OII' DII'2 DII'1 120(6) 1_555 . 209_343 N
OII' DII'2 DII'1 101(5) 1_555 . -206_444 N
OII' DII'2 DII'1 146(10) 1_555 . 310_334 N
OII' DII'2 DII'1 162(6) 1_555 . 312_334 N
OII' DII'2 DII'1 80(6) 1_555 . -304_444 N
OII' DII'2 DII'2 74(4) 1_555 . 2_555 N
OII' DII'2 DII'2 74(4) 1_555 . 3_555 N
OII' DII'2 OII' 80.6(22) 107_533 . 111_533 N
OII' DII'2 OII' 91.70(16) 107_533 . -105_544 N
OII' DII'2 DII'1 111(6) 107_433 . 1_555 N
OII' DII'2 DII'1 175(7) 107_433 . 2_555 N
OII' DII'2 DII'1 91(4) 107_433 . 3_555 N
OII' DII'2 DII'1 23.4(7) 107_433 . 107_433 N
OII' DII'2 DII'1 61.1(29) 107_433 . 111_433 N
OII' DII'2 DII'1 109(4) 107_433 . -105_444 N
OII' DII'2 DII'1 78.9(30) 107_433 . 208_343 N
OII' DII'2 DII'1 103(4) 107_433 . 209_343 N
OII' DII'2 DII'1 31.9(17) 107_433 . -206_444 N
OII' DII'2 DII'1 30.4(13) 107_433 . 310_334 N
OII' DII'2 DII'1 65.3(12) 107_433 . 312_334 N
OII' DII'2 DII'1 105.1(29) 107_433 . -304_444 N
OII' DII'2 DII'2 78(11) 107_533 . 2_555 N
OII' DII'2 DII'2 122(8) 107_533 . 3_555 N
OII' DII'2 OII' 81.2(29) 111_533 . -105_544 N
OII' DII'2 DII'1 69(6) 111_433 . 1_555 N
OII' DII'2 DII'1 104(6) 111_433 . 2_555 N
OII' DII'2 DII'1 138(6) 111_433 . 3_555 N
OII' DII'2 DII'1 57.6(28) 111_433 . 107_433 N
OII' DII'2 DII'1 24.66(27) 111_433 . 111_433 N
OII' DII'2 DII'1 112(5) 111_433 . -105_444 N
OII' DII'2 DII'1 23.1(5) 111_433 . 208_343 N
OII' DII'2 DII'1 60(4) 111_433 . 209_343 N
OII' DII'2 DII'1 90(5) 111_433 . -206_444 N
OII' DII'2 DII'1 99.9(32) 111_433 . 310_334 N
OII' DII'2 DII'1 79.8(30) 111_433 . 312_334 N
OII' DII'2 DII'1 26.6(9) 111_433 . -304_444 N
OII' DII'2 DII'2 45(8) 111_533 . 2_555 N
OII' DII'2 DII'2 42(6) 111_533 . 3_555 N
OII' DII'2 DII'1 138(9) -105_444 . 1_555 N
OII' DII'2 DII'1 88(5) -105_444 . 2_555 N
OII' DII'2 DII'1 140(7) -105_444 . 3_555 N
OII' DII'2 DII'1 83.8(26) -105_444 . 107_433 N
OII' DII'2 DII'1 97(4) -105_444 . 111_433 N
OII' DII'2 DII'1 33.2(14) -105_444 . -105_444 N
OII' DII'2 DII'1 58.4(30) -105_444 . 208_343 N
OII' DII'2 DII'1 26.9(15) -105_444 . 209_343 N
OII' DII'2 DII'1 123.4(18) -105_444 . -206_444 N
OII' DII'2 DII'1 71.8(23) -105_444 . 310_334 N
OII' DII'2 DII'1 26.5(14) -105_444 . 312_334 N
OII' DII'2 DII'1 90.6(34) -105_444 . -304_444 N
OII' DII'2 DII'2 126(9) -105_544 . 2_555 N
OII' DII'2 DII'2 84(13) -105_544 . 3_555 N
DII'1 DII'2 DII'1 72.2(16) 1_555 . 2_555 N
DII'1 DII'2 DII'1 75.9(26) 1_555 . 3_555 N
DII'1 DII'2 DII'1 103(5) 1_555 . 107_433 N
DII'1 DII'2 DII'1 68(5) 1_555 . 111_433 N
DII'1 DII'2 DII'1 139(10) 1_555 . -105_444 N
DII'1 DII'2 DII'1 91(6) 1_555 . 208_343 N
DII'1 DII'2 DII'1 112(8) 1_555 . 209_343 N
DII'1 DII'2 DII'1 86(8) 1_555 . -206_444 N
DII'1 DII'2 DII'1 140(7) 1_555 . 310_334 N
DII'1 DII'2 DII'1 149(7) 1_555 . 312_334 N
DII'1 DII'2 DII'1 51(7) 1_555 . -304_444 N
DII'1 DII'2 DII'2 37(5) 1_555 . 2_555 N
DII'1 DII'2 DII'2 54(7) 1_555 . 3_555 N
DII'1 DII'2 DII'1 87(7) 2_555 . 3_555 N
DII'1 DII'2 DII'1 160(8) 2_555 . 107_433 N
DII'1 DII'2 DII'1 123(6) 2_555 . 111_433 N
DII'1 DII'2 DII'1 68(8) 2_555 . -105_444 N
DII'1 DII'2 DII'1 104(6) 2_555 . 208_343 N
DII'1 DII'2 DII'1 78(4) 2_555 . 209_343 N
DII'1 DII'2 DII'1 148(4) 2_555 . -206_444 N
DII'1 DII'2 DII'1 146(5) 2_555 . 310_334 N
DII'1 DII'2 DII'1 114(5) 2_555 . 312_334 N
DII'1 DII'2 DII'1 79(6) 2_555 . -304_444 N
DII'1 DII'2 DII'2 106(9) 2_555 . 2_555 N
DII'1 DII'2 DII'2 62(10) 2_555 . 3_555 N
DII'1 DII'2 DII'1 111(5) 3_555 . 107_433 N
DII'1 DII'2 DII'1 119(5) 3_555 . 111_433 N
DII'1 DII'2 DII'1 110(9) 3_555 . -105_444 N
DII'1 DII'2 DII'1 160(5) 3_555 . 208_343 N
DII'1 DII'2 DII'1 159(9) 3_555 . 209_343 N
DII'1 DII'2 DII'1 65(5) 3_555 . -206_444 N
DII'1 DII'2 DII'1 92(7) 3_555 . 310_334 N
DII'1 DII'2 DII'1 133(4) 3_555 . 312_334 N
DII'1 DII'2 DII'1 127(6) 3_555 . -304_444 N
DII'1 DII'2 DII'2 93(9) 3_555 . 2_555 N
DII'1 DII'2 DII'2 126.4(28) 3_555 . 3_555 N
DII'1 DII'2 DII'1 41(5) 107_433 . 111_433 N
DII'1 DII'2 DII'1 111(5) 107_433 . -105_444 N
DII'1 DII'2 DII'1 56(4) 107_433 . 208_343 N
DII'1 DII'2 DII'1 87(4) 107_433 . 209_343 N
DII'1 DII'2 DII'1 46.5(15) 107_433 . -206_444 N
DII'1 DII'2 DII'1 45.9(13) 107_433 . 310_334 N
DII'1 DII'2 DII'1 60(4) 107_433 . 312_334 N
DII'1 DII'2 DII'1 83(4) 107_433 . -304_444 N
DII'1 DII'2 DII'2 66(6) 107_533 . 2_555 N
DII'1 DII'2 DII'2 99(7) 107_533 . 3_555 N
DII'1 DII'2 DII'1 130(5) 111_433 . -105_444 N
DII'1 DII'2 DII'1 41.0(6) 111_433 . 208_343 N
DII'1 DII'2 DII'1 82(5) 111_433 . 209_343 N
DII'1 DII'2 DII'1 65(5) 111_433 . -206_444 N
DII'1 DII'2 DII'1 87(4) 111_433 . 310_334 N
DII'1 DII'2 DII'1 85.8(31) 111_433 . 312_334 N
DII'1 DII'2 DII'1 44.3(6) 111_433 . -304_444 N
DII'1 DII'2 DII'2 32.7(22) 111_533 . 2_555 N
DII'1 DII'2 DII'2 62(10) 111_533 . 3_555 N
DII'1 DII'2 DII'1 90(5) -105_444 . 208_343 N
DII'1 DII'2 DII'1 51.3(26) -105_444 . 209_343 N
DII'1 DII'2 DII'1 133(6) -105_444 . -206_444 N
DII'1 DII'2 DII'1 80.2(33) -105_444 . 310_334 N
DII'1 DII'2 DII'1 50.8(22) -105_444 . 312_334 N
DII'1 DII'2 DII'1 112(5) -105_444 . -304_444 N
DII'1 DII'2 DII'2 155(16) -105_544 . 2_555 N
DII'1 DII'2 DII'2 98(19) -105_544 . 3_555 N
DII'1 DII'2 DII'1 41(5) 208_343 . 209_343 N
DII'1 DII'2 DII'1 99(6) 208_343 . -206_444 N
DII'1 DII'2 DII'1 88.1(29) 208_343 . 310_334 N
DII'1 DII'2 DII'1 58(4) 208_343 . 312_334 N
DII'1 DII'2 DII'1 42.4(9) 208_343 . -304_444 N
DII'1 DII'2 DII'2 68(7) 208_443 . 2_555 N
DII'1 DII'2 DII'2 50.2(18) 208_443 . 3_555 N
DII'1 DII'2 DII'1 133.2(28) 209_343 . -206_444 N
DII'1 DII'2 DII'1 93(5) 209_343 . 310_334 N
DII'1 DII'2 DII'1 46.3(14) 209_343 . 312_334 N
DII'1 DII'2 DII'1 64(4) 209_343 . -304_444 N
DII'1 DII'2 DII'2 105(12) 209_443 . 2_555 N
DII'1 DII'2 DII'2 57(11) 209_443 . 3_555 N
DII'1 DII'2 DII'1 54.9(31) -206_444 . 310_334 N
DII'1 DII'2 DII'1 96.9(15) -206_444 . 312_334 N
DII'1 DII'2 DII'1 105(4) -206_444 . -304_444 N
DII'1 DII'2 DII'2 64(15) -206_544 . 2_555 N
DII'1 DII'2 DII'2 123(15) -206_544 . 3_555 N
DII'1 DII'2 DII'1 47(5) 310_334 . 312_334 N
DII'1 DII'2 DII'1 126(4) 310_334 . -304_444 N
DII'1 DII'2 DII'2 109(11) 310_434 . 2_555 N
DII'1 DII'2 DII'2 138(4) 310_434 . 3_555 N
DII'1 DII'2 DII'1 99(4) 312_334 . -304_444 N
DII'1 DII'2 DII'2 118.5(33) 312_434 . 2_555 N
DII'1 DII'2 DII'2 100(7) 312_434 . 3_555 N
DII'1 DII'2 DII'2 44(14) -304_544 . 2_555 N
DII'1 DII'2 DII'2 18(12) -304_544 . 3_555 N
DII'2 DII'2 DII'2 60.0000(7) 2_555 . 3_555 N
SII OII* SJ 72.5(12) 1_555 . 107_545 N
SII OII* SJ 72.5(12) 1_555 . 208_455 N
SII OII* SJ 72.5(12) 1_555 . 312_446 N
SII OII* Od 78.9(15) 1_555 . 107_554 N
SII OII* Od 78.9(15) 1_555 . 208_464 N
SII OII* Od 78.9(15) 1_555 . 312_455 N
SII OII* Dd1 91.3(19) 1_555 . 107_533 N
SII OII* Dd1 91.3(19) 1_555 . 208_443 N
SII OII* Dd1 91.3(19) 1_555 . 312_434 N
SII OII* Dd2 64.6(16) 1_555 . 107_533 N
SII OII* Dd2 64.6(16) 1_555 . 208_443 N
SII OII* Dd2 64.6(16) 1_555 . 312_434 N
SII OII* DII*1 85(9) 1_555 . 1_555 N
SII OII* DII*1 85(9) 1_555 . 2_555 N
SII OII* DII*1 85(9) 1_555 . 3_555 N
SII OII* DII*2 170(8) 1_555 . 1_555 N
SII OII* DII*2 170(8) 1_555 . 2_555 N
SII OII* DII*2 170(8) 1_555 . 3_555 N
SII OII* Of 91.8(15) 1_555 . -102_443 N
SII OII* Of 91.8(15) 1_555 . -203_443 N
SII OII* Of 91.8(15) 1_555 . -301_443 N
SII OII* Df1 103.7(16) 1_555 . -102_444 N
SII OII* Df1 103.7(16) 1_555 . -203_444 N
SII OII* Df1 103.7(16) 1_555 . -301_444 N
SJ OII* SJ 111.3(12) 107_545 . 208_455 N
SJ OII* SJ 111.3(12) 107_545 . 312_446 N
SJ OII* Od 6.8(9) 107_554 . 107_554 N
SJ OII* Od 116.2(14) 107_554 . 208_464 N
SJ OII* Od 112.1(14) 107_554 . 312_455 N
SJ OII* Dd1 18.8(13) 107_533 . 107_533 N
SJ OII* Dd1 118.6(18) 107_533 . 208_443 N
SJ OII* Dd1 119.3(18) 107_533 . 312_434 N
SJ OII* Dd2 8.9(12) 107_533 . 107_533 N
SJ OII* Dd2 110.8(23) 107_533 . 208_443 N
SJ OII* Dd2 104.1(21) 107_533 . 312_434 N
SJ OII* DII*1 147(11) 107_432 . 1_555 N
SJ OII* DII*1 37(11) 107_432 . 2_555 N
SJ OII* DII*1 83(11) 107_432 . 3_555 N
SJ OII* DII*2 99(7) 107_433 . 1_555 N
SJ OII* DII*2 116(11) 107_433 . 2_555 N
SJ OII* DII*2 107(12) 107_433 . 3_555 N
SJ OII* Of 163.7(25) 107_432 . -102_443 N
SJ OII* Of 66.3(7) 107_432 . -203_443 N
SJ OII* Of 58.0(7) 107_432 . -301_443 N
SJ OII* Df1 165.7(13) 107_433 . -102_444 N
SJ OII* Df1 79.6(9) 107_433 . -203_444 N
SJ OII* Df1 54.9(11) 107_433 . -301_444 N
SJ OII* SJ 111.3(12) 208_455 . 312_446 N
SJ OII* Od 112.1(14) 208_464 . 107_554 N
SJ OII* Od 6.8(9) 208_464 . 208_464 N
SJ OII* Od 116.2(14) 208_464 . 312_455 N
SJ OII* Dd1 119.3(18) 208_443 . 107_533 N
SJ OII* Dd1 18.8(13) 208_443 . 208_443 N
SJ OII* Dd1 118.6(18) 208_443 . 312_434 N
SJ OII* Dd2 104.1(21) 208_443 . 107_533 N
SJ OII* Dd2 8.9(12) 208_443 . 208_443 N
SJ OII* Dd2 110.8(23) 208_443 . 312_434 N
SJ OII* DII*1 83(11) 208_342 . 1_555 N
SJ OII* DII*1 147(11) 208_342 . 2_555 N
SJ OII* DII*1 37(11) 208_342 . 3_555 N
SJ OII* DII*2 107(12) 208_343 . 1_555 N
SJ OII* DII*2 99(7) 208_343 . 2_555 N
SJ OII* DII*2 116(11) 208_343 . 3_555 N
SJ OII* Of 58.0(7) 208_342 . -102_443 N
SJ OII* Of 163.7(25) 208_342 . -203_443 N
SJ OII* Of 66.3(7) 208_342 . -301_443 N
SJ OII* Df1 54.9(11) 208_343 . -102_444 N
SJ OII* Df1 165.7(13) 208_343 . -203_444 N
SJ OII* Df1 79.6(9) 208_343 . -301_444 N
SJ OII* Od 116.2(14) 312_455 . 107_554 N
SJ OII* Od 112.1(14) 312_455 . 208_464 N
SJ OII* Od 6.8(9) 312_455 . 312_455 N
SJ OII* Dd1 118.6(18) 312_434 . 107_533 N
SJ OII* Dd1 119.3(18) 312_434 . 208_443 N
SJ OII* Dd1 18.8(13) 312_434 . 312_434 N
SJ OII* Dd2 110.8(23) 312_434 . 107_533 N
SJ OII* Dd2 104.1(21) 312_434 . 208_443 N
SJ OII* Dd2 8.9(12) 312_434 . 312_434 N
SJ OII* DII*1 37(11) 312_333 . 1_555 N
SJ OII* DII*1 83(11) 312_333 . 2_555 N
SJ OII* DII*1 147(11) 312_333 . 3_555 N
SJ OII* DII*2 116(11) 312_334 . 1_555 N
SJ OII* DII*2 107(12) 312_334 . 2_555 N
SJ OII* DII*2 99(7) 312_334 . 3_555 N
SJ OII* Of 66.3(7) 312_333 . -102_443 N
SJ OII* Of 58.0(7) 312_333 . -203_443 N
SJ OII* Of 163.7(25) 312_333 . -301_443 N
SJ OII* Df1 79.6(9) 312_334 . -102_444 N
SJ OII* Df1 54.9(11) 312_334 . -203_444 N
SJ OII* Df1 165.7(13) 312_334 . -301_444 N
Od OII* Od 116.4(10) 107_554 . 208_464 N
Od OII* Od 116.4(10) 107_554 . 312_455 N
Od OII* Dd1 12.7(8) 107_533 . 107_533 N
Od OII* Dd1 117.0(15) 107_533 . 208_443 N
Od OII* Dd1 122.3(14) 107_533 . 312_434 N
Od OII* Dd2 14.4(4) 107_533 . 107_533 N
Od OII* Dd2 112.7(21) 107_533 . 208_443 N
Od OII* Dd2 109.5(19) 107_533 . 312_434 N
Od OII* DII*1 153(11) 107_432 . 1_555 N
Od OII* DII*1 38(11) 107_432 . 2_555 N
Od OII* DII*1 81(11) 107_432 . 3_555 N
Od OII* DII*2 93(7) 107_433 . 1_555 N
Od OII* DII*2 109(11) 107_433 . 2_555 N
Od OII* DII*2 101(12) 107_433 . 3_555 N
Od OII* Of 168.5(24) 107_432 . -102_443 N
Od OII* Of 67.6(10) 107_432 . -203_443 N
Od OII* Of 54.5(10) 107_432 . -301_443 N
Od OII* Df1 163.6(13) 107_433 . -102_444 N
Od OII* Df1 79.9(12) 107_433 . -203_444 N
Od OII* Df1 49.7(13) 107_433 . -301_444 N
Od OII* Od 116.4(10) 208_464 . 312_455 N
Od OII* Dd1 122.3(14) 208_443 . 107_533 N
Od OII* Dd1 12.7(8) 208_443 . 208_443 N
Od OII* Dd1 117.0(15) 208_443 . 312_434 N
Od OII* Dd2 109.5(19) 208_443 . 107_533 N
Od OII* Dd2 14.4(4) 208_443 . 208_443 N
Od OII* Dd2 112.7(21) 208_443 . 312_434 N
Od OII* DII*1 81(11) 208_342 . 1_555 N
Od OII* DII*1 153(11) 208_342 . 2_555 N
Od OII* DII*1 38(11) 208_342 . 3_555 N
Od OII* DII*2 101(12) 208_343 . 1_555 N
Od OII* DII*2 93(7) 208_343 . 2_555 N
Od OII* DII*2 109(11) 208_343 . 3_555 N
Od OII* Of 54.5(10) 208_342 . -102_443 N
Od OII* Of 168.5(24) 208_342 . -203_443 N
Od OII* Of 67.6(10) 208_342 . -301_443 N
Od OII* Df1 49.7(13) 208_343 . -102_444 N
Od OII* Df1 163.6(13) 208_343 . -203_444 N
Od OII* Df1 79.9(12) 208_343 . -301_444 N
Od OII* Dd1 117.0(15) 312_434 . 107_533 N
Od OII* Dd1 122.3(14) 312_434 . 208_443 N
Od OII* Dd1 12.7(8) 312_434 . 312_434 N
Od OII* Dd2 112.7(21) 312_434 . 107_533 N
Od OII* Dd2 109.5(19) 312_434 . 208_443 N
Od OII* Dd2 14.4(4) 312_434 . 312_434 N
Od OII* DII*1 38(11) 312_333 . 1_555 N
Od OII* DII*1 81(11) 312_333 . 2_555 N
Od OII* DII*1 153(11) 312_333 . 3_555 N
Od OII* DII*2 109(11) 312_334 . 1_555 N
Od OII* DII*2 101(12) 312_334 . 2_555 N
Od OII* DII*2 93(7) 312_334 . 3_555 N
Od OII* Of 67.6(10) 312_333 . -102_443 N
Od OII* Of 54.5(10) 312_333 . -203_443 N
Od OII* Of 168.5(24) 312_333 . -301_443 N
Od OII* Df1 79.9(12) 312_334 . -102_444 N
Od OII* Df1 49.7(13) 312_334 . -203_444 N
Od OII* Df1 163.6(13) 312_334 . -301_444 N
Dd1 OII* Dd1 119.95(14) 107_533 . 208_443 N
Dd1 OII* Dd1 119.95(14) 107_533 . 312_434 N
Dd1 OII* Dd2 27.1(6) 107_533 . 107_533 N
Dd1 OII* Dd2 121.5(27) 107_533 . 208_443 N
Dd1 OII* Dd2 113.3(28) 107_533 . 312_434 N
Dd1 OII* DII*1 155(11) 107_432 . 1_555 N
Dd1 OII* DII*1 36(11) 107_432 . 2_555 N
Dd1 OII* DII*1 85(11) 107_432 . 3_555 N
Dd1 OII* DII*2 81(8) 107_433 . 1_555 N
Dd1 OII* DII*2 97(11) 107_433 . 2_555 N
Dd1 OII* DII*2 88(12) 107_433 . 3_555 N
Dd1 OII* Of 174.9(23) 107_432 . -102_443 N
Dd1 OII* Of 64.0(16) 107_432 . -203_443 N
Dd1 OII* Of 55.9(16) 107_432 . -301_443 N
Dd1 OII* Df1 159.7(26) 107_433 . -102_444 N
Dd1 OII* Df1 74.0(18) 107_433 . -203_444 N
Dd1 OII* Df1 47.3(19) 107_433 . -301_444 N
Dd1 OII* Dd1 119.95(14) 208_443 . 312_434 N
Dd1 OII* Dd2 113.3(28) 208_443 . 107_533 N
Dd1 OII* Dd2 27.1(6) 208_443 . 208_443 N
Dd1 OII* Dd2 121.5(27) 208_443 . 312_434 N
Dd1 OII* DII*1 85(11) 208_342 . 1_555 N
Dd1 OII* DII*1 155(11) 208_342 . 2_555 N
Dd1 OII* DII*1 36(11) 208_342 . 3_555 N
Dd1 OII* DII*2 88(12) 208_343 . 1_555 N
Dd1 OII* DII*2 81(8) 208_343 . 2_555 N
Dd1 OII* DII*2 97(11) 208_343 . 3_555 N
Dd1 OII* Of 55.9(16) 208_342 . -102_443 N
Dd1 OII* Of 174.9(23) 208_342 . -203_443 N
Dd1 OII* Of 64.0(16) 208_342 . -301_443 N
Dd1 OII* Df1 47.3(19) 208_343 . -102_444 N
Dd1 OII* Df1 159.7(26) 208_343 . -203_444 N
Dd1 OII* Df1 74.0(18) 208_343 . -301_444 N
Dd1 OII* Dd2 121.5(27) 312_434 . 107_533 N
Dd1 OII* Dd2 113.3(28) 312_434 . 208_443 N
Dd1 OII* Dd2 27.1(6) 312_434 . 312_434 N
Dd1 OII* DII*1 36(11) 312_333 . 1_555 N
Dd1 OII* DII*1 85(11) 312_333 . 2_555 N
Dd1 OII* DII*1 155(11) 312_333 . 3_555 N
Dd1 OII* DII*2 97(11) 312_334 . 1_555 N
Dd1 OII* DII*2 88(12) 312_334 . 2_555 N
Dd1 OII* DII*2 81(8) 312_334 . 3_555 N
Dd1 OII* Of 64.0(16) 312_333 . -102_443 N
Dd1 OII* Of 55.9(16) 312_333 . -203_443 N
Dd1 OII* Of 174.9(23) 312_333 . -301_443 N
Dd1 OII* Df1 74.0(18) 312_334 . -102_444 N
Dd1 OII* Df1 47.3(19) 312_334 . -203_444 N
Dd1 OII* Df1 159.7(26) 312_334 . -301_444 N
Dd2 OII* Dd2 102.9(19) 107_533 . 208_443 N
Dd2 OII* Dd2 102.9(19) 107_533 . 312_434 N
Dd2 OII* DII*1 144(10) 107_432 . 1_555 N
Dd2 OII* DII*1 43(11) 107_432 . 2_555 N
Dd2 OII* DII*1 79(11) 107_432 . 3_555 N
Dd2 OII* DII*2 107(7) 107_433 . 1_555 N
Dd2 OII* DII*2 123(12) 107_433 . 2_555 N
Dd2 OII* DII*2 115(12) 107_433 . 3_555 N
Dd2 OII* Of 154.9(27) 107_432 . -102_443 N
Dd2 OII* Of 71.7(19) 107_432 . -203_443 N
Dd2 OII* Of 56.6(19) 107_432 . -301_443 N
Dd2 OII* Df1 159.0(23) 107_433 . -102_444 N
Dd2 OII* Df1 85.8(19) 107_433 . -203_444 N
Dd2 OII* Df1 56.2(19) 107_433 . -301_444 N
Dd2 OII* Dd2 102.9(19) 208_443 . 312_434 N
Dd2 OII* DII*1 79(11) 208_342 . 1_555 N
Dd2 OII* DII*1 144(10) 208_342 . 2_555 N
Dd2 OII* DII*1 43(11) 208_342 . 3_555 N
Dd2 OII* DII*2 115(12) 208_343 . 1_555 N
Dd2 OII* DII*2 107(7) 208_343 . 2_555 N
Dd2 OII* DII*2 123(12) 208_343 . 3_555 N
Dd2 OII* Of 56.6(19) 208_342 . -102_443 N
Dd2 OII* Of 154.9(27) 208_342 . -203_443 N
Dd2 OII* Of 71.7(19) 208_342 . -301_443 N
Dd2 OII* Df1 56.2(19) 208_343 . -102_444 N
Dd2 OII* Df1 159.0(23) 208_343 . -203_444 N
Dd2 OII* Df1 85.8(19) 208_343 . -301_444 N
Dd2 OII* DII*1 43(11) 312_333 . 1_555 N
Dd2 OII* DII*1 79(11) 312_333 . 2_555 N
Dd2 OII* DII*1 144(10) 312_333 . 3_555 N
Dd2 OII* DII*2 123(12) 312_334 . 1_555 N
Dd2 OII* DII*2 115(12) 312_334 . 2_555 N
Dd2 OII* DII*2 107(7) 312_334 . 3_555 N
Dd2 OII* Of 71.7(19) 312_333 . -102_443 N
Dd2 OII* Of 56.6(19) 312_333 . -203_443 N
Dd2 OII* Of 154.9(27) 312_333 . -301_443 N
Dd2 OII* Df1 85.8(19) 312_334 . -102_444 N
Dd2 OII* Df1 56.2(19) 312_334 . -203_444 N
Dd2 OII* Df1 159.0(23) 312_334 . -301_444 N
DII*1 OII* DII*1 119.2(27) 1_555 . 2_555 N
DII*1 OII* DII*1 119.2(27) 1_555 . 3_555 N
DII*1 OII* DII*2 104(4) 1_555 . 1_555 N
DII*1 OII* DII*2 89(19) 1_555 . 2_555 N
DII*1 OII* DII*2 91(14) 1_555 . 3_555 N
DII*1 OII* Of 30(11) 1_555 . -102_443 N
DII*1 OII* Of 91(11) 1_555 . -203_443 N
DII*1 OII* Of 149(11) 1_555 . -301_443 N
DII*1 OII* Df1 43(11) 1_555 . -102_444 N
DII*1 OII* Df1 83(11) 1_555 . -203_444 N
DII*1 OII* Df1 157(11) 1_555 . -301_444 N
DII*1 OII* DII*1 119.2(27) 2_555 . 3_555 N
DII*1 OII* DII*2 91(14) 2_555 . 1_555 N
DII*1 OII* DII*2 104(4) 2_555 . 2_555 N
DII*1 OII* DII*2 89(19) 2_555 . 3_555 N
DII*1 OII* Of 149(11) 2_555 . -102_443 N
DII*1 OII* Of 30(11) 2_555 . -203_443 N
DII*1 OII* Of 91(11) 2_555 . -301_443 N
DII*1 OII* Df1 157(11) 2_555 . -102_444 N
DII*1 OII* Df1 43(11) 2_555 . -203_444 N
DII*1 OII* Df1 83(11) 2_555 . -301_444 N
DII*1 OII* DII*2 89(19) 3_555 . 1_555 N
DII*1 OII* DII*2 91(14) 3_555 . 2_555 N
DII*1 OII* DII*2 104(4) 3_555 . 3_555 N
DII*1 OII* Of 91(11) 3_555 . -102_443 N
DII*1 OII* Of 149(11) 3_555 . -203_443 N
DII*1 OII* Of 30(11) 3_555 . -301_443 N
DII*1 OII* Df1 83(11) 3_555 . -102_444 N
DII*1 OII* Df1 157(11) 3_555 . -203_444 N
DII*1 OII* Df1 43(11) 3_555 . -301_444 N
DII*2 OII* DII*2 17(14) 1_555 . 2_555 N
DII*2 OII* DII*2 17(14) 1_555 . 3_555 N
DII*2 OII* Of 96(8) 1_555 . -102_443 N
DII*2 OII* Of 89(12) 1_555 . -203_443 N
DII*2 OII* Of 79(11) 1_555 . -301_443 N
DII*2 OII* Df1 83(8) 1_555 . -102_444 N
DII*2 OII* Df1 79(13) 1_555 . -203_444 N
DII*2 OII* Df1 67(10) 1_555 . -301_444 N
DII*2 OII* DII*2 17(14) 2_555 . 3_555 N
DII*2 OII* Of 79(11) 2_555 . -102_443 N
DII*2 OII* Of 96(8) 2_555 . -203_443 N
DII*2 OII* Of 89(12) 2_555 . -301_443 N
DII*2 OII* Df1 67(10) 2_555 . -102_444 N
DII*2 OII* Df1 83(8) 2_555 . -203_444 N
DII*2 OII* Df1 79(13) 2_555 . -301_444 N
DII*2 OII* Of 89(12) 3_555 . -102_443 N
DII*2 OII* Of 79(11) 3_555 . -203_443 N
DII*2 OII* Of 96(8) 3_555 . -301_443 N
DII*2 OII* Df1 79(13) 3_555 . -102_444 N
DII*2 OII* Df1 67(10) 3_555 . -203_444 N
DII*2 OII* Df1 83(8) 3_555 . -301_444 N
Of OII* Of 119.90(16) -102_443 . -203_443 N
Of OII* Of 119.90(16) -102_443 . -301_443 N
Of OII* Df1 15.30(24) -102_444 . -102_444 N
Of OII* Df1 109.1(10) -102_444 . -203_444 N
Of OII* Df1 127.9(11) -102_444 . -301_444 N
Of OII* Of 119.90(16) -203_443 . -301_443 N
Of OII* Df1 127.9(11) -203_444 . -102_444 N
Of OII* Df1 15.30(24) -203_444 . -203_444 N
Of OII* Df1 109.1(10) -203_444 . -301_444 N
Of OII* Df1 109.1(10) -301_444 . -102_444 N
Of OII* Df1 127.9(11) -301_444 . -203_444 N
Of OII* Df1 15.30(24) -301_444 . -301_444 N
Df1 OII* Df1 114.6(12) -102_444 . -203_444 N
Df1 OII* Df1 114.6(12) -102_444 . -301_444 N
Df1 OII* Df1 114.6(12) -203_444 . -301_444 N
Si2 DII*1 Al1 0.0 209_353 . 209_353 N
Si2 DII*1 O3 24.1(7) 209_343 . -105_444 N
Si2 DII*1 O4 26.9(8) 209_343 . 1_555 N
Si2 DII*1 O4 63.9(19) 209_343 . 3_555 N
Si2 DII*1 SII 54.6(20) 209_465 . 1_555 N
Si2 DII*1 SJ 88.4(28) 209_455 . 208_455 N
Si2 DII*1 SJ 43.4(14) 209_455 . 312_446 N
Si2 DII*1 Oc 56.9(14) 209_455 . 312_446 N
Si2 DII*1 Dc1 61.9(16) 209_464 . 312_455 N
Si2 DII*1 Dc2 42.3(10) 209_465 . 312_456 N
Si2 DII*1 Od 92.8(31) 209_464 . 208_464 N
Si2 DII*1 Od 51.9(20) 209_464 . 312_455 N
Si2 DII*1 Dd1 121(4) 209_443 . 107_533 N
Si2 DII*1 Dd1 106(4) 209_443 . 208_443 N
Si2 DII*1 Dd1 66.1(29) 209_443 . 312_434 N
Si2 DII*1 Dd2 81.4(29) 209_443 . 208_443 N
Si2 DII*1 Dd2 39.3(24) 209_443 . 312_434 N
Si2 DII*1 OII* 128(10) 209_343 . 1_555 N
Si2 DII*1 DII*1 115(6) 209_342 . 2_555 N
Si2 DII*1 DII*1 123(4) 209_342 . 3_555 N
Si2 DII*1 DII*2 165(9) 209_343 . 1_555 N
Si2 DII*1 DII*2 174(5) 209_343 . 2_555 N
Si2 DII*1 DII*2 165(15) 209_343 . 3_555 N
Si2 DII*1 Of 82.8(8) 209_342 . 5_555 N
Al1 DII*1 O3 24.1(7) 209_343 . -105_444 N
Al1 DII*1 O4 26.9(8) 209_343 . 1_555 N
Al1 DII*1 O4 63.9(19) 209_343 . 3_555 N
Al1 DII*1 SII 54.6(20) 209_465 . 1_555 N
Al1 DII*1 SJ 88.4(28) 209_455 . 208_455 N
Al1 DII*1 SJ 43.4(14) 209_455 . 312_446 N
Al1 DII*1 Oc 56.9(14) 209_455 . 312_446 N
Al1 DII*1 Dc1 61.9(16) 209_464 . 312_455 N
Al1 DII*1 Dc2 42.3(10) 209_465 . 312_456 N
Al1 DII*1 Od 92.8(31) 209_464 . 208_464 N
Al1 DII*1 Od 51.9(20) 209_464 . 312_455 N
Al1 DII*1 Dd1 121(4) 209_443 . 107_533 N
Al1 DII*1 Dd1 106(4) 209_443 . 208_443 N
Al1 DII*1 Dd1 66.1(29) 209_443 . 312_434 N
Al1 DII*1 Dd2 81.4(29) 209_443 . 208_443 N
Al1 DII*1 Dd2 39.3(24) 209_443 . 312_434 N
Al1 DII*1 OII* 128(10) 209_343 . 1_555 N
Al1 DII*1 DII*1 115(6) 209_342 . 2_555 N
Al1 DII*1 DII*1 123(4) 209_342 . 3_555 N
Al1 DII*1 DII*2 165(9) 209_343 . 1_555 N
Al1 DII*1 DII*2 174(5) 209_343 . 2_555 N
Al1 DII*1 DII*2 165(15) 209_343 . 3_555 N
Al1 DII*1 Of 82.8(8) 209_342 . 5_555 N
O3 DII*1 O4 44.4(15) -105_444 . 1_555 N
O3 DII*1 O4 39.9(15) -105_444 . 3_555 N
O3 DII*1 SII 41.4(17) -105_566 . 1_555 N
O3 DII*1 SJ 65.8(26) -105_556 . 208_455 N
O3 DII*1 SJ 67.5(21) -105_556 . 312_446 N
O3 DII*1 Oc 78.9(17) -105_556 . 312_446 N
O3 DII*1 Dc1 85.7(20) -105_565 . 312_455 N
O3 DII*1 Dc2 64.4(14) -105_566 . 312_456 N
O3 DII*1 Od 71.1(29) -105_565 . 208_464 N
O3 DII*1 Od 76.0(26) -105_565 . 312_455 N
O3 DII*1 Dd1 114.2(30) -105_544 . 107_533 N
O3 DII*1 Dd1 85(4) -105_544 . 208_443 N
O3 DII*1 Dd1 90.2(34) -105_544 . 312_434 N
O3 DII*1 Dd2 58.3(25) -105_544 . 208_443 N
O3 DII*1 Dd2 62.0(29) -105_544 . 312_434 N
O3 DII*1 OII* 114(10) -105_444 . 1_555 N
O3 DII*1 DII*1 112.7(15) -105_443 . 2_555 N
O3 DII*1 DII*1 100(5) -105_443 . 3_555 N
O3 DII*1 DII*2 149(9) -105_444 . 1_555 N
O3 DII*1 DII*2 153(11) -105_444 . 2_555 N
O3 DII*1 DII*2 158(5) -105_444 . 3_555 N
O3 DII*1 Of 91.1(16) -105_443 . 5_555 N
O4 DII*1 O4 81.7(25) 1_555 . 3_555 N
O4 DII*1 SII 52.0(24) 1_555 . 1_555 N
O4 DII*1 SJ 109.6(33) 1_555 . 208_455 N
O4 DII*1 SJ 32.6(15) 1_555 . 312_446 N
O4 DII*1 Oc 58.4(20) 1_555 . 312_446 N
O4 DII*1 Dc1 55.2(20) 1_555 . 312_455 N
O4 DII*1 Dc2 47.0(15) 1_555 . 312_456 N
O4 DII*1 Od 115(4) 1_555 . 208_464 N
O4 DII*1 Od 39.8(21) 1_555 . 312_455 N
O4 DII*1 Dd1 100(4) 1_555 . 107_533 N
O4 DII*1 Dd1 129(4) 1_555 . 208_443 N
O4 DII*1 Dd1 55.6(33) 1_555 . 312_434 N
O4 DII*1 Dd2 101.8(34) 1_555 . 208_443 N
O4 DII*1 Dd2 21.6(17) 1_555 . 312_434 N
O4 DII*1 OII* 113(11) 1_555 . 1_555 N
O4 DII*1 DII*1 91(8) 1_555 . 2_555 N
O4 DII*1 DII*1 123(4) 1_555 . 3_555 N
O4 DII*1 DII*2 141(9) 1_555 . 1_555 N
O4 DII*1 DII*2 149(9) 1_555 . 2_555 N
O4 DII*1 DII*2 138(14) 1_555 . 3_555 N
O4 DII*1 Of 99.5(11) 1_555 . 5_555 N
O4 DII*1 SII 46.2(23) 3_555 . 1_555 N
O4 DII*1 SJ 28.5(13) 3_555 . 208_455 N
O4 DII*1 SJ 107.3(29) 3_555 . 312_446 N
O4 DII*1 Oc 113.4(23) 3_555 . 312_446 N
O4 DII*1 Dc1 123.8(23) 3_555 . 312_455 N
O4 DII*1 Dc2 100.3(23) 3_555 . 312_456 N
O4 DII*1 Od 34.8(17) 3_555 . 208_464 N
O4 DII*1 Od 115.8(33) 3_555 . 312_455 N
O4 DII*1 Dd1 99.7(21) 3_555 . 107_533 N
O4 DII*1 Dd1 47.7(24) 3_555 . 208_443 N
O4 DII*1 Dd1 129(4) 3_555 . 312_434 N
O4 DII*1 Dd2 20.5(13) 3_555 . 208_443 N
O4 DII*1 Dd2 101(4) 3_555 . 312_434 N
O4 DII*1 OII* 88(10) 3_555 . 1_555 N
O4 DII*1 DII*1 106(7) 3_555 . 2_555 N
O4 DII*1 DII*1 64(8) 3_555 . 3_555 N
O4 DII*1 DII*2 114(9) 3_555 . 1_555 N
O4 DII*1 DII*2 114(11) 3_555 . 2_555 N
O4 DII*1 DII*2 123(8) 3_555 . 3_555 N
O4 DII*1 Of 99.3(31) 3_555 . 5_555 N
SII DII*1 SJ 71.6(33) 1_555 . 208_455 N
SII DII*1 SJ 85(4) 1_555 . 312_446 N
SII DII*1 Oc 109(4) 1_555 . 312_446 N
SII DII*1 Dc1 107(4) 1_555 . 312_455 N
SII DII*1 Dc2 95.1(32) 1_555 . 312_456 N
SII DII*1 Od 78(4) 1_555 . 208_464 N
SII DII*1 Od 92(4) 1_555 . 312_455 N
SII DII*1 Dd1 72.9(19) 1_555 . 107_533 N
SII DII*1 Dd1 88(4) 1_555 . 208_443 N
SII DII*1 Dd1 107(6) 1_555 . 312_434 N
SII DII*1 Dd2 64.4(32) 1_555 . 208_443 N
SII DII*1 Dd2 73(4) 1_555 . 312_434 N
SII DII*1 OII* 75(8) 1_555 . 1_555 N
SII DII*1 DII*1 72.3(6) 1_555 . 2_555 N
SII DII*1 DII*1 72.3(6) 1_555 . 3_555 N
SII DII*1 DII*2 112(7) 1_555 . 1_555 N
SII DII*1 DII*2 120(6) 1_555 . 2_555 N
SII DII*1 DII*2 118(7) 1_555 . 3_555 N
SII DII*1 Of 132.4(31) 1_555 . 5_555 N
SJ DII*1 SJ 130.2(32) 208_455 . 312_446 N
SJ DII*1 Oc 123.6(31) 208_455 . 312_446 N
SJ DII*1 Dc1 138.1(24) 208_464 . 312_455 N
SJ DII*1 Dc2 115.1(29) 208_465 . 312_456 N
SJ DII*1 Od 6.6(10) 208_464 . 208_464 N
SJ DII*1 Od 137.9(33) 208_464 . 312_455 N
SJ DII*1 Dd1 100.2(23) 208_443 . 107_533 N
SJ DII*1 Dd1 19.3(15) 208_443 . 208_443 N
SJ DII*1 Dd1 146(4) 208_443 . 312_434 N
SJ DII*1 Dd2 8.0(13) 208_443 . 208_443 N
SJ DII*1 Dd2 128(4) 208_443 . 312_434 N
SJ DII*1 OII* 83(10) 208_343 . 1_555 N
SJ DII*1 DII*1 110(10) 208_342 . 2_555 N
SJ DII*1 DII*1 53(10) 208_342 . 3_555 N
SJ DII*1 DII*2 94(9) 208_343 . 1_555 N
SJ DII*1 DII*2 92(10) 208_343 . 2_555 N
SJ DII*1 DII*2 102(11) 208_343 . 3_555 N
SJ DII*1 Of 88.8(34) 208_342 . 5_555 N
SJ DII*1 Oc 28.4(11) 312_446 . 312_446 N
SJ DII*1 Dc1 22.5(10) 312_455 . 312_455 N
SJ DII*1 Dc2 23.2(8) 312_456 . 312_456 N
SJ DII*1 Od 133.2(32) 312_455 . 208_464 N
SJ DII*1 Od 8.5(12) 312_455 . 312_455 N
SJ DII*1 Dd1 114(5) 312_434 . 107_533 N
SJ DII*1 Dd1 145(4) 312_434 . 208_443 N
SJ DII*1 Dd1 23.8(21) 312_434 . 312_434 N
SJ DII*1 Dd2 124.0(35) 312_434 . 208_443 N
SJ DII*1 Dd2 12.6(15) 312_434 . 312_434 N
SJ DII*1 OII* 133(13) 312_334 . 1_555 N
SJ DII*1 DII*1 103(13) 312_333 . 2_555 N
SJ DII*1 DII*1 154(8) 312_333 . 3_555 N
SJ DII*1 DII*2 136(11) 312_334 . 1_555 N
SJ DII*1 DII*2 138(13) 312_334 . 2_555 N
SJ DII*1 DII*2 127(11) 312_334 . 3_555 N
SJ DII*1 Of 75.7(10) 312_333 . 5_555 N
Oc DII*1 Dc1 15.0(7) 312_455 . 312_455 N
Oc DII*1 Dc2 14.6(4) 312_456 . 312_456 N
Oc DII*1 Od 122.8(32) 312_455 . 208_464 N
Oc DII*1 Od 26.4(13) 312_455 . 312_455 N
Oc DII*1 Dd1 135(5) 312_434 . 107_533 N
Oc DII*1 Dd1 128(4) 312_434 . 208_443 N
Oc DII*1 Dd1 22.8(20) 312_434 . 312_434 N
Oc DII*1 Dd2 121.3(33) 312_434 . 208_443 N
Oc DII*1 Dd2 40.9(19) 312_434 . 312_434 N
Oc DII*1 OII* 154(14) 312_334 . 1_555 N
Oc DII*1 DII*1 124(14) 312_333 . 2_555 N
Oc DII*1 DII*1 176(14) 312_333 . 3_555 N
Oc DII*1 DII*2 131(11) 312_334 . 1_555 N
Oc DII*1 DII*2 128(10) 312_334 . 2_555 N
Oc DII*1 DII*2 122(6) 312_334 . 3_555 N
Oc DII*1 Of 48.0(9) 312_333 . 5_555 N
Dc1 DII*1 Dc2 24.0(6) 312_456 . 312_456 N
Dc1 DII*1 Od 137.7(26) 312_455 . 208_464 N
Dc1 DII*1 Od 16.4(12) 312_455 . 312_455 N
Dc1 DII*1 Dd1 120(5) 312_434 . 107_533 N
Dc1 DII*1 Dd1 143(4) 312_434 . 208_443 N
Dc1 DII*1 Dd1 7.8(22) 312_434 . 312_434 N
Dc1 DII*1 Dd2 135.0(28) 312_434 . 208_443 N
Dc1 DII*1 Dd2 34.4(17) 312_434 . 312_434 N
Dc1 DII*1 OII* 139(13) 312_334 . 1_555 N
Dc1 DII*1 DII*1 109(13) 312_333 . 2_555 N
Dc1 DII*1 DII*1 169(13) 312_333 . 3_555 N
Dc1 DII*1 DII*2 123(11) 312_334 . 1_555 N
Dc1 DII*1 DII*2 121(11) 312_334 . 2_555 N
Dc1 DII*1 DII*2 113(7) 312_334 . 3_555 N
Dc1 DII*1 Of 60.5(9) 312_333 . 5_555 N
Dc2 DII*1 Od 115.9(30) 312_455 . 208_464 N
Dc2 DII*1 Od 26.1(12) 312_455 . 312_455 N
Dc2 DII*1 Dd1 137(5) 312_434 . 107_533 N
Dc2 DII*1 Dd1 125(4) 312_434 . 208_443 N
Dc2 DII*1 Dd1 31.1(21) 312_434 . 312_434 N
Dc2 DII*1 Dd2 111.2(31) 312_434 . 208_443 N
Dc2 DII*1 Dd2 33.7(20) 312_434 . 312_434 N
Dc2 DII*1 OII* 156(14) 312_334 . 1_555 N
Dc2 DII*1 DII*1 126(13) 312_333 . 2_555 N
Dc2 DII*1 DII*1 164(7) 312_333 . 3_555 N
Dc2 DII*1 DII*2 146(11) 312_334 . 1_555 N
Dc2 DII*1 DII*2 142(10) 312_334 . 2_555 N
Dc2 DII*1 DII*2 136(7) 312_334 . 3_555 N
Dc2 DII*1 Of 54.1(7) 312_333 . 5_555 N
Od DII*1 Od 140.3(31) 208_464 . 312_455 N
Od DII*1 Dd1 102.0(23) 208_443 . 107_533 N
Od DII*1 Dd1 13.6(10) 208_443 . 208_443 N
Od DII*1 Dd1 145(4) 208_443 . 312_434 N
Od DII*1 Dd2 14.4(10) 208_443 . 208_443 N
Od DII*1 Dd2 132(5) 208_443 . 312_434 N
Od DII*1 OII* 84(11) 208_343 . 1_555 N
Od DII*1 DII*1 112(10) 208_342 . 2_555 N
Od DII*1 DII*1 53(11) 208_342 . 3_555 N
Od DII*1 DII*2 91(9) 208_343 . 1_555 N
Od DII*1 DII*2 88(10) 208_343 . 2_555 N
Od DII*1 DII*2 99(11) 208_343 . 3_555 N
Od DII*1 Of 84.5(34) 208_342 . 5_555 N
Od DII*1 Dd1 112(5) 312_434 . 107_533 N
Od DII*1 Dd1 150.5(35) 312_434 . 208_443 N
Od DII*1 Dd1 15.8(15) 312_434 . 312_434 N
Od DII*1 Dd2 132(4) 312_434 . 208_443 N
Od DII*1 Dd2 18.4(10) 312_434 . 312_434 N
Od DII*1 OII* 131(13) 312_334 . 1_555 N
Od DII*1 DII*1 100(13) 312_333 . 2_555 N
Od DII*1 DII*1 157(11) 312_333 . 3_555 N
Od DII*1 DII*2 128(11) 312_334 . 1_555 N
Od DII*1 DII*2 129(12) 312_334 . 2_555 N
Od DII*1 DII*2 120(10) 312_334 . 3_555 N
Od DII*1 Of 74.4(14) 312_333 . 5_555 N
Dd1 DII*1 Dd1 96.6(18) 107_533 . 208_443 N
Dd1 DII*1 Dd1 112(5) 107_533 . 312_434 N
Dd1 DII*1 Dd2 100.5(30) 107_533 . 208_443 N
Dd1 DII*1 Dd2 105(5) 107_533 . 312_434 N
Dd1 DII*1 OII* 19(9) 107_433 . 1_555 N
Dd1 DII*1 DII*1 11(8) 107_432 . 2_555 N
Dd1 DII*1 DII*1 49(9) 107_432 . 3_555 N
Dd1 DII*1 DII*2 44(6) 107_433 . 1_555 N
Dd1 DII*1 DII*2 53(5) 107_433 . 2_555 N
Dd1 DII*1 DII*2 47(9) 107_433 . 3_555 N
Dd1 DII*1 Of 155(4) 107_432 . 5_555 N
Dd1 DII*1 Dd1 150(4) 208_443 . 312_434 N
Dd1 DII*1 Dd2 27.2(16) 208_443 . 208_443 N
Dd1 DII*1 Dd2 145(5) 208_443 . 312_434 N
Dd1 DII*1 OII* 77(10) 208_343 . 1_555 N
Dd1 DII*1 DII*1 108(10) 208_342 . 2_555 N
Dd1 DII*1 DII*1 48(10) 208_342 . 3_555 N
Dd1 DII*1 DII*2 78(9) 208_343 . 1_555 N
Dd1 DII*1 DII*2 75(9) 208_343 . 2_555 N
Dd1 DII*1 DII*2 86(12) 208_343 . 3_555 N
Dd1 DII*1 Of 84(4) 208_342 . 5_555 N
Dd1 DII*1 Dd2 142(4) 312_434 . 208_443 N
Dd1 DII*1 Dd2 34.0(22) 312_434 . 312_434 N
Dd1 DII*1 OII* 131(14) 312_334 . 1_555 N
Dd1 DII*1 DII*1 101(14) 312_333 . 2_555 N
Dd1 DII*1 DII*1 161(14) 312_333 . 3_555 N
Dd1 DII*1 DII*2 117(12) 312_334 . 1_555 N
Dd1 DII*1 DII*2 116(12) 312_334 . 2_555 N
Dd1 DII*1 DII*2 108(8) 312_334 . 3_555 N
Dd1 DII*1 Of 66.6(23) 312_333 . 5_555 N
Dd2 DII*1 Dd2 120(4) 208_443 . 312_434 N
Dd2 DII*1 OII* 84(10) 208_343 . 1_555 N
Dd2 DII*1 DII*1 109(9) 208_342 . 2_555 N
Dd2 DII*1 DII*1 55(10) 208_342 . 3_555 N
Dd2 DII*1 DII*2 100(9) 208_343 . 1_555 N
Dd2 DII*1 DII*2 98(11) 208_343 . 2_555 N
Dd2 DII*1 DII*2 108(10) 208_343 . 3_555 N
Dd2 DII*1 Of 92(4) 208_342 . 5_555 N
Dd2 DII*1 OII* 123(13) 312_334 . 1_555 N
Dd2 DII*1 DII*1 94(12) 312_333 . 2_555 N
Dd2 DII*1 DII*1 142(8) 312_333 . 3_555 N
Dd2 DII*1 DII*2 135(11) 312_334 . 1_555 N
Dd2 DII*1 DII*2 140(13) 312_334 . 2_555 N
Dd2 DII*1 DII*2 128(13) 312_334 . 3_555 N
Dd2 DII*1 Of 87.5(19) 312_333 . 5_555 N
OII* DII*1 DII*1 30.4(13) 1_555 . 2_555 N
OII* DII*1 DII*1 30.4(13) 1_555 . 3_555 N
OII* DII*1 DII*2 37.8(34) 1_555 . 1_555 N
OII* DII*1 DII*2 45(10) 1_555 . 2_555 N
OII* DII*1 DII*2 44(8) 1_555 . 3_555 N
OII* DII*1 Of 147(12) 1_555 . 5_555 N
DII*1 DII*1 DII*1 60.0 2_555 . 3_555 N
DII*1 DII*1 DII*2 51(7) 2_555 . 1_555 N
DII*1 DII*1 DII*2 59.7(29) 2_555 . 2_555 N
DII*1 DII*1 DII*2 52(10) 2_555 . 3_555 N
DII*1 DII*1 Of 154(7) 2_555 . 5_555 N
DII*1 DII*1 DII*2 50(9) 3_555 . 1_555 N
DII*1 DII*1 DII*2 53(7) 3_555 . 2_555 N
DII*1 DII*1 DII*2 59.3(21) 3_555 . 3_555 N
DII*1 DII*1 Of 128(12) 3_555 . 5_555 N
DII*2 DII*1 DII*2 9(7) 1_555 . 2_555 N
DII*2 DII*1 DII*2 9(10) 1_555 . 3_555 N
DII*2 DII*1 Of 112(9) 1_555 . 5_555 N
DII*2 DII*1 DII*2 12(11) 2_555 . 3_555 N
DII*2 DII*1 Of 103(5) 2_555 . 5_555 N
DII*2 DII*1 Of 108(10) 3_555 . 5_555 N
SII DII*2 Od 66.8(17) 1_555 . 107_554 N
SII DII*2 Od 65.3(22) 1_555 . 208_464 N
SII DII*2 Dd1 75.6(21) 1_555 . 107_533 N
SII DII*2 Dd1 74.2(27) 1_555 . 208_443 N
SII DII*2 Dd1 72.6(21) 1_555 . 312_434 N
SII DII*2 Dd2 52.5(13) 1_555 . 107_533 N
SII DII*2 Dd2 51.5(16) 1_555 . 208_443 N
SII DII*2 Dd2 50.7(14) 1_555 . 312_434 N
SII DII*2 OII* 7(6) 1_555 . 1_555 N
SII DII*2 DII*1 45(6) 1_555 . 1_555 N
SII DII*2 DII*1 42(5) 1_555 . 2_555 N
SII DII*2 DII*1 41(4) 1_555 . 3_555 N
SII DII*2 DII*2 87.8(19) 1_555 . 2_555 N
SII DII*2 DII*2 87.8(19) 1_555 . 3_555 N
SII DII*2 Of 75.2(15) 1_555 . -102_443 N
SII DII*2 Of 76.5(25) 1_555 . -203_443 N
SII DII*2 Of 78.6(26) 1_555 . -301_443 N
SII DII*2 Df1 104(4) 1_555 . 4_555 N
SII DII*2 Df1 102(4) 1_555 . 6_555 N
SII DII*2 Df1 84.9(21) 1_555 . -102_444 N
SII DII*2 Df1 85.9(31) 1_555 . -203_444 N
SII DII*2 Df1 88.9(30) 1_555 . -301_444 N
SII DII*2 Df2 68.9(21) 1_555 . -301_434 N
Od DII*2 Od 106(4) 107_554 . 208_464 N
Od DII*2 Dd1 9.4(11) 107_533 . 107_533 N
Od DII*2 Dd1 110(4) 107_533 . 208_443 N
Od DII*2 Dd1 111(4) 107_533 . 312_434 N
Od DII*2 Dd2 14.4(5) 107_533 . 107_533 N
Od DII*2 Dd2 98.8(32) 107_533 . 208_443 N
Od DII*2 Dd2 94.7(29) 107_533 . 312_434 N
Od DII*2 OII* 73(7) 107_433 . 1_555 N
Od DII*2 DII*1 108(7) 107_432 . 1_555 N
Od DII*2 DII*1 42(8) 107_432 . 2_555 N
Od DII*2 DII*1 72(10) 107_432 . 3_555 N
Od DII*2 DII*2 154.5(23) 107_433 . 2_555 N
Od DII*2 DII*2 116(65) 107_433 . 3_555 N
Od DII*2 Of 141.6(16) 107_432 . -102_443 N
Od DII*2 Of 64.7(26) 107_432 . -203_443 N
Od DII*2 Of 53.3(21) 107_432 . -301_443 N
Od DII*2 Df1 86.0(35) 107_433 . 4_555 N
Od DII*2 Df1 57.1(24) 107_433 . 6_555 N
Od DII*2 Df1 148.6(35) 107_433 . -102_444 N
Od DII*2 Df1 77.8(34) 107_433 . -203_444 N
Od DII*2 Df1 48.8(22) 107_433 . -301_444 N
Od DII*2 Df2 41.7(18) 107_423 . -301_434 N
Od DII*2 Dd1 114(5) 208_443 . 107_533 N
Od DII*2 Dd1 9.0(10) 208_443 . 208_443 N
Od DII*2 Dd1 103.9(27) 208_443 . 312_434 N
Od DII*2 Dd2 96.1(34) 208_443 . 107_533 N
Od DII*2 Dd2 13.9(7) 208_443 . 208_443 N
Od DII*2 Dd2 95.1(22) 208_443 . 312_434 N
Od DII*2 OII* 65(11) 208_343 . 1_555 N
Od DII*2 DII*1 67(8) 208_342 . 1_555 N
Od DII*2 DII*1 106(9) 208_342 . 2_555 N
Od DII*2 DII*1 35(10) 208_342 . 3_555 N
Od DII*2 DII*2 60(62) 208_343 . 2_555 N
Od DII*2 DII*2 114(62) 208_343 . 3_555 N
Od DII*2 Of 50.5(21) 208_342 . -102_443 N
Od DII*2 Of 140.6(14) 208_342 . -203_443 N
Od DII*2 Of 64.7(34) 208_342 . -301_443 N
Od DII*2 Df1 56.4(31) 208_343 . 4_555 N
Od DII*2 Df1 163.0(33) 208_343 . 6_555 N
Od DII*2 Df1 46.5(26) 208_343 . -102_444 N
Od DII*2 Df1 145.0(26) 208_343 . -203_444 N
Od DII*2 Df1 78(4) 208_343 . -301_444 N
Od DII*2 Df2 70.0(33) 208_333 . -301_434 N
Dd1 DII*2 Dd1 117(5) 107_533 . 208_443 N
Dd1 DII*2 Dd1 113(5) 107_533 . 312_434 N
Dd1 DII*2 Dd2 23.6(12) 107_533 . 107_533 N
Dd1 DII*2 Dd2 108(4) 107_533 . 208_443 N
Dd1 DII*2 Dd2 99(4) 107_533 . 312_434 N
Dd1 DII*2 OII* 82(7) 107_433 . 1_555 N
Dd1 DII*2 DII*1 116(7) 107_432 . 1_555 N
Dd1 DII*2 DII*1 47(7) 107_432 . 2_555 N
Dd1 DII*2 DII*1 81(10) 107_432 . 3_555 N
Dd1 DII*2 DII*2 163(17) 107_433 . 2_555 N
Dd1 DII*2 DII*2 115(71) 107_433 . 3_555 N
Dd1 DII*2 Of 150.8(18) 107_432 . -102_443 N
Dd1 DII*2 Of 62.6(35) 107_432 . -203_443 N
Dd1 DII*2 Of 56.5(29) 107_432 . -301_443 N
Dd1 DII*2 Df1 87(4) 107_433 . 4_555 N
Dd1 DII*2 Df1 49.7(29) 107_433 . 6_555 N
Dd1 DII*2 Df1 158(4) 107_433 . -102_444 N
Dd1 DII*2 Df1 75(4) 107_433 . -203_444 N
Dd1 DII*2 Df1 49.3(28) 107_433 . -301_444 N
Dd1 DII*2 Df2 46.4(27) 107_423 . -301_434 N
Dd1 DII*2 Dd1 109.4(30) 208_443 . 312_434 N
Dd1 DII*2 Dd2 101(4) 208_443 . 107_533 N
Dd1 DII*2 Dd2 22.8(13) 208_443 . 208_443 N
Dd1 DII*2 Dd2 102.7(28) 208_443 . 312_434 N
Dd1 DII*2 OII* 74(11) 208_343 . 1_555 N
Dd1 DII*2 DII*1 74(8) 208_342 . 1_555 N
Dd1 DII*2 DII*1 115(10) 208_342 . 2_555 N
Dd1 DII*2 DII*1 42(9) 208_342 . 3_555 N
Dd1 DII*2 DII*2 61(67) 208_343 . 2_555 N
Dd1 DII*2 DII*2 118(67) 208_343 . 3_555 N
Dd1 DII*2 Of 52.7(26) 208_342 . -102_443 N
Dd1 DII*2 Of 149.6(16) 208_342 . -203_443 N
Dd1 DII*2 Of 64(4) 208_342 . -301_443 N
Dd1 DII*2 Df1 49.8(33) 208_343 . 4_555 N
Dd1 DII*2 Df1 166(5) 208_343 . 6_555 N
Dd1 DII*2 Df1 46.2(29) 208_343 . -102_444 N
Dd1 DII*2 Df1 152.8(33) 208_343 . -203_444 N
Dd1 DII*2 Df1 76(5) 208_343 . -301_444 N
Dd1 DII*2 Df2 71(4) 208_333 . -301_434 N
Dd1 DII*2 Dd2 105(4) 312_434 . 107_533 N
Dd1 DII*2 Dd2 96.3(29) 312_434 . 208_443 N
Dd1 DII*2 Dd2 22.3(12) 312_434 . 312_434 N
Dd1 DII*2 OII* 66(10) 312_334 . 1_555 N
Dd1 DII*2 DII*1 39(8) 312_333 . 1_555 N
Dd1 DII*2 DII*1 70(11) 312_333 . 2_555 N
Dd1 DII*2 DII*1 108(4) 312_333 . 3_555 N
Dd1 DII*2 DII*2 58(65) 312_334 . 2_555 N
Dd1 DII*2 DII*2 16(15) 312_334 . 3_555 N
Dd1 DII*2 Of 59.3(24) 312_333 . -102_443 N
Dd1 DII*2 Of 53.0(32) 312_333 . -203_443 N
Dd1 DII*2 Of 151.1(18) 312_333 . -301_443 N
Dd1 DII*2 Df1 158(5) 312_334 . 4_555 N
Dd1 DII*2 Df1 82(5) 312_334 . 6_555 N
Dd1 DII*2 Df1 70.4(29) 312_334 . -102_444 N
Dd1 DII*2 Df1 45.5(32) 312_334 . -203_444 N
Dd1 DII*2 Df1 158(4) 312_334 . -301_444 N
Dd1 DII*2 Df2 139.8(21) 312_324 . -301_434 N
Dd2 DII*2 Dd2 86.9(27) 107_533 . 208_443 N
Dd2 DII*2 Dd2 85.5(24) 107_533 . 312_434 N
Dd2 DII*2 OII* 59(6) 107_433 . 1_555 N
Dd2 DII*2 DII*1 95(7) 107_432 . 1_555 N
Dd2 DII*2 DII*1 35(10) 107_432 . 2_555 N
Dd2 DII*2 DII*1 61(9) 107_432 . 3_555 N
Dd2 DII*2 DII*2 140.3(22) 107_433 . 2_555 N
Dd2 DII*2 DII*2 113(54) 107_433 . 3_555 N
Dd2 DII*2 Of 127.3(16) 107_432 . -102_443 N
Dd2 DII*2 Of 66.2(30) 107_432 . -203_443 N
Dd2 DII*2 Of 53.7(26) 107_432 . -301_443 N
Dd2 DII*2 Df1 89(4) 107_433 . 4_555 N
Dd2 DII*2 Df1 67.0(29) 107_433 . 6_555 N
Dd2 DII*2 Df1 134.9(30) 107_433 . -102_444 N
Dd2 DII*2 Df1 80(4) 107_433 . -203_444 N
Dd2 DII*2 Df1 53.5(27) 107_433 . -301_444 N
Dd2 DII*2 Df2 40.5(24) 107_423 . -301_434 N
Dd2 DII*2 Dd2 83.9(16) 208_443 . 312_434 N
Dd2 DII*2 OII* 51(10) 208_343 . 1_555 N
Dd2 DII*2 DII*1 57(8) 208_342 . 1_555 N
Dd2 DII*2 DII*1 93(8) 208_342 . 2_555 N
Dd2 DII*2 DII*1 27(9) 208_342 . 3_555 N
Dd2 DII*2 DII*2 63(51) 208_343 . 2_555 N
Dd2 DII*2 DII*2 109(52) 208_343 . 3_555 N
Dd2 DII*2 Of 50.8(24) 208_342 . -102_443 N
Dd2 DII*2 Of 126.9(17) 208_342 . -203_443 N
Dd2 DII*2 Of 66(4) 208_342 . -301_443 N
Dd2 DII*2 Df1 66(4) 208_343 . 4_555 N
Dd2 DII*2 Df1 152.2(27) 208_343 . 6_555 N
Dd2 DII*2 Df1 50.8(28) 208_343 . -102_444 N
Dd2 DII*2 Df1 132.7(26) 208_343 . -203_444 N
Dd2 DII*2 Df1 81(5) 208_343 . -301_444 N
Dd2 DII*2 Df2 68.4(33) 208_333 . -301_434 N
Dd2 DII*2 OII* 45(10) 312_334 . 1_555 N
Dd2 DII*2 DII*1 29(8) 312_333 . 1_555 N
Dd2 DII*2 DII*1 52(9) 312_333 . 2_555 N
Dd2 DII*2 DII*1 89.0(31) 312_333 . 3_555 N
Dd2 DII*2 DII*2 67(52) 312_334 . 2_555 N
Dd2 DII*2 DII*2 37.2(30) 312_334 . 3_555 N
Dd2 DII*2 Of 63.0(23) 312_333 . -102_443 N
Dd2 DII*2 Of 50.7(27) 312_333 . -203_443 N
Dd2 DII*2 Of 128.8(19) 312_333 . -301_443 N
Dd2 DII*2 Df1 150(4) 312_334 . 4_555 N
Dd2 DII*2 Df1 85(4) 312_334 . 6_555 N
Dd2 DII*2 Df1 76.1(27) 312_334 . -102_444 N
Dd2 DII*2 Df1 50.1(29) 312_334 . -203_444 N
Dd2 DII*2 Df1 136.6(25) 312_334 . -301_444 N
Dd2 DII*2 Df2 117.6(17) 312_324 . -301_434 N
OII* DII*2 DII*1 37.7(6) 1_555 . 1_555 N
OII* DII*2 DII*1 44(7) 1_555 . 2_555 N
OII* DII*2 DII*1 45(9) 1_555 . 3_555 N
OII* DII*2 DII*2 82(7) 1_555 . 2_555 N
OII* DII*2 DII*2 82(7) 1_555 . 3_555 N
OII* DII*2 Of 69(7) 1_555 . -102_443 N
OII* DII*2 Of 76(11) 1_555 . -203_443 N
OII* DII*2 Of 85(10) 1_555 . -301_443 N
OII* DII*2 Df1 108(13) 1_555 . 4_555 N
OII* DII*2 Df1 104(12) 1_555 . 6_555 N
OII* DII*2 Df1 80(8) 1_555 . -102_444 N
OII* DII*2 Df1 84(12) 1_555 . -203_444 N
OII* DII*2 Df1 96(10) 1_555 . -301_444 N
OII* DII*2 Df2 76(9) 1_555 . -301_434 N
DII*1 DII*2 DII*1 70(5) 1_555 . 2_555 N
DII*1 DII*2 DII*1 70(6) 1_555 . 3_555 N
DII*1 DII*2 DII*2 48(28) 1_555 . 2_555 N
DII*1 DII*2 DII*2 54(33) 1_555 . 3_555 N
DII*1 DII*2 Of 39(7) 1_555 . -102_443 N
DII*1 DII*2 Of 79(9) 1_555 . -203_443 N
DII*1 DII*2 Of 117(9) 1_555 . -301_443 N
DII*1 DII*2 Df1 123(10) 1_555 . 4_555 N
DII*1 DII*2 Df1 113(10) 1_555 . 6_555 N
DII*1 DII*2 Df1 52(8) 1_555 . -102_444 N
DII*1 DII*2 Df1 79(9) 1_555 . -203_444 N
DII*1 DII*2 Df1 130(10) 1_555 . -301_444 N
DII*1 DII*2 Df2 111(8) 1_555 . -301_434 N
DII*1 DII*2 DII*1 75(10) 2_555 . 3_555 N
DII*1 DII*2 DII*2 117(40) 2_555 . 2_555 N
DII*1 DII*2 DII*2 79(54) 2_555 . 3_555 N
DII*1 DII*2 Of 108(5) 2_555 . -102_443 N
DII*1 DII*2 Of 40(11) 2_555 . -203_443 N
DII*1 DII*2 Of 87(12) 2_555 . -301_443 N
DII*1 DII*2 Df1 122(13) 2_555 . 4_555 N
DII*1 DII*2 Df1 60(8) 2_555 . 6_555 N
DII*1 DII*2 Df1 121(4) 2_555 . -102_444 N
DII*1 DII*2 Df1 53(12) 2_555 . -203_444 N
DII*1 DII*2 Df1 88(11) 2_555 . -301_444 N
DII*1 DII*2 Df2 74(11) 2_555 . -301_434 N
DII*1 DII*2 DII*2 89(51) 3_555 . 2_555 N
DII*1 DII*2 DII*2 124(27) 3_555 . 3_555 N
DII*1 DII*2 Of 77(10) 3_555 . -102_443 N
DII*1 DII*2 Of 115(8) 3_555 . -203_443 N
DII*1 DII*2 Of 47(6) 3_555 . -301_443 N
DII*1 DII*2 Df1 63(6) 3_555 . 4_555 N
DII*1 DII*2 Df1 128(11) 3_555 . 6_555 N
DII*1 DII*2 Df1 78(11) 3_555 . -102_444 N
DII*1 DII*2 Df1 126(8) 3_555 . -203_444 N
DII*1 DII*2 Df1 61(6) 3_555 . -301_444 N
DII*1 DII*2 Df2 44(7) 3_555 . -301_434 N
DII*2 DII*2 DII*2 60.0 2_555 . 3_555 N
DII*2 DII*2 Of 14(24) 2_555 . -102_443 N
DII*2 DII*2 Of 110(69) 2_555 . -203_443 N
DII*2 DII*2 Of 124(71) 2_555 . -301_443 N
DII*2 DII*2 Df1 101(71) 2_555 . 4_555 N
DII*2 DII*2 Df1 133(70) 2_555 . 6_555 N
DII*2 DII*2 Df1 15(66) 2_555 . -102_444 N
DII*2 DII*2 Df1 101(71) 2_555 . -203_444 N
DII*2 DII*2 Df1 135(74) 2_555 . -301_444 N
DII*2 DII*2 Df2 130(63) 2_555 . -301_434 N
DII*2 DII*2 Of 66(66) 3_555 . -102_443 N
DII*2 DII*2 Of 52(69) 3_555 . -203_443 N
DII*2 DII*2 Of 165(27) 3_555 . -301_443 N
DII*2 DII*2 Df1 158(60) 3_555 . 4_555 N
DII*2 DII*2 Df1 75(71) 3_555 . 6_555 N
DII*2 DII*2 Df1 74(68) 3_555 . -102_444 N
DII*2 DII*2 Df1 41(71) 3_555 . -203_444 N
DII*2 DII*2 Df1 164(73) 3_555 . -301_444 N
DII*2 DII*2 Df2 152(38) 3_555 . -301_434 N
Of DII*2 Of 111(4) -102_443 . -203_443 N
Of DII*2 Of 115(5) -102_443 . -301_443 N
Of DII*2 Df1 99(5) -102_444 . 4_555 N
Of DII*2 Df1 140(5) -102_444 . 6_555 N
Of DII*2 Df1 13.2(6) -102_444 . -102_444 N
Of DII*2 Df1 105(4) -102_444 . -203_444 N
Of DII*2 Df1 128(6) -102_444 . -301_444 N
Of DII*2 Df2 119(4) -102_434 . -301_434 N
Of DII*2 Of 118.0(33) -203_443 . -301_443 N
Of DII*2 Df1 148(4) -203_444 . 4_555 N
Of DII*2 Df1 34.1(19) -203_444 . 6_555 N
Of DII*2 Df1 123(4) -203_444 . -102_444 N
Of DII*2 Df1 14.0(8) -203_444 . -203_444 N
Of DII*2 Df1 112(4) -203_444 . -301_444 N
Of DII*2 Df2 105.9(30) -203_434 . -301_434 N
Of DII*2 Df1 35.0(21) -301_444 . 4_555 N
Of DII*2 Df1 102.4(31) -301_444 . 6_555 N
Of DII*2 Df1 110(6) -301_444 . -102_444 N
Of DII*2 Df1 131(4) -301_444 . -203_444 N
Of DII*2 Df1 14.3(10) -301_444 . -301_444 N
Of DII*2 Df2 13.3(6) -301_434 . -301_434 N
Df1 DII*2 Df1 119.7(27) 4_555 . 6_555 N
Df1 DII*2 Df1 88(5) 4_555 . -102_444 N
Df1 DII*2 Df1 156(4) 4_555 . -203_444 N
Df1 DII*2 Df1 37.4(30) 4_555 . -301_444 N
Df1 DII*2 Df2 48.3(24) 4_555 . -301_434 N
Df1 DII*2 Df1 148(6) 6_555 . -102_444 N
Df1 DII*2 Df1 36.6(26) 6_555 . -203_444 N
Df1 DII*2 Df1 90.6(33) 6_555 . -301_444 N
Df1 DII*2 Df2 95.1(29) 6_555 . -301_434 N
Df1 DII*2 Df1 115(5) -102_444 . -203_444 N
Df1 DII*2 Df1 121(7) -102_444 . -301_444 N
Df1 DII*2 Df2 116(5) -102_434 . -301_434 N
Df1 DII*2 Df1 123(5) -203_444 . -301_444 N
Df1 DII*2 Df2 119(4) -203_434 . -301_434 N
Df1 DII*2 Df2 20.0(13) -301_434 . -301_434 N
Si1 Of Si1 69.9(6) 111_434 . -108_545 N
Si1 Of Si2 50.8(5) 111_533 . 208_443 N
Si1 Of Al1 50.8(5) 111_443 . 208_353 N
Si1 Of O1 25.03(26) 111_433 . 111_433 N
Si1 Of O1 65.8(7) 111_433 . -108_544 N
Si1 Of O2 22.91(23) 111_433 . 1_555 N
Si1 Of O3 61.2(5) 111_433 . 4_555 N
Si1 Of O4 64.8(6) 111_433 . 310_334 N
Si1 Of O4 24.09(22) 111_433 . 312_334 N
Si1 Of SJ 48.3(6) 111_545 . 1_555 N
Si1 Of SJ 117.8(10) 111_545 . -207_566 N
Si1 Of SJ 98.9(12) 111_545 . -304_556 N
Si1 Of Oc 125.2(10) 111_545 . -3_555 N
Si1 Of Oc 60.4(6) 111_545 . -108_656 N
Si1 Of Oc 113.7(10) 111_545 . -304_556 N
Si1 Of Dc1 133.1(9) 111_554 . -3_555 N
Si1 Of Dc1 135.0(9) 111_554 . -207_575 N
Si1 Of Dc1 124.8(11) 111_554 . -304_565 N
Si1 Of Dc2 110.4(9) 111_555 . -3_555 N
Si1 Of Dc2 46.1(5) 111_555 . -108_666 N
Si1 Of Dc2 101.1(11) 111_555 . -304_566 N
Si1 Of Od 50.3(8) 111_554 . 1_555 N
Si1 Of Od 124.1(13) 111_554 . -207_575 N
Si1 Of Od 106.0(14) 111_554 . -304_565 N
Si1 Of Si2 49.5(5) -108_644 . 208_443 N
Si1 Of Al1 49.5(5) -108_554 . 208_353 N
Si1 Of O1 64.4(6) -108_544 . 111_433 N
Si1 Of O1 23.05(29) -108_544 . -108_544 N
Si1 Of O2 57.0(5) -108_544 . 1_555 N
Si1 Of O3 26.97(25) -108_544 . 4_555 N
Si1 Of O4 78.1(7) -108_544 . 310_334 N
Si1 Of O4 93.8(8) -108_544 . 312_334 N
Si1 Of SJ 113.8(10) -108_656 . 1_555 N
Si1 Of SJ 48.7(6) -108_656 . -207_566 N
Si1 Of SJ 76.5(10) -108_656 . -304_556 N
Si1 Of Oc 112.8(8) -108_656 . -3_555 N
Si1 Of Oc 102.6(9) -108_656 . -108_656 N
Si1 Of Oc 61.5(6) -108_656 . -304_556 N
Si1 Of Dc1 110.4(7) -108_665 . -3_555 N
Si1 Of Dc1 68.6(6) -108_665 . -207_575 N
Si1 Of Dc1 79.2(7) -108_665 . -304_565 N
Si1 Of Dc2 112.5(8) -108_666 . -3_555 N
Si1 Of Dc2 89.1(8) -108_666 . -108_666 N
Si1 Of Dc2 49.0(7) -108_666 . -304_566 N
Si1 Of Od 112.8(11) -108_665 . 1_555 N
Si1 Of Od 55.1(10) -108_665 . -207_575 N
Si1 Of Od 79.8(13) -108_665 . -304_565 N
Si2 Of Al1 0.0 208_353 . 208_353 N
Si2 Of O1 67.6(7) 208_343 . 111_433 N
Si2 Of O1 28.7(4) 208_343 . -108_544 N
Si2 Of O2 27.92(30) 208_343 . 1_555 N
Si2 Of O3 66.3(6) 208_343 . 4_555 N
Si2 Of O4 30.52(33) 208_343 . 310_334 N
Si2 Of O4 65.0(6) 208_343 . 312_334 N
Si2 Of SJ 95.2(9) 208_455 . 1_555 N
Si2 Of SJ 78.7(8) 208_455 . -207_566 N
Si2 Of SJ 51.1(9) 208_455 . -304_556 N
Si2 Of Oc 87.9(8) 208_455 . -3_555 N
Si2 Of Oc 110.8(10) 208_455 . -108_656 N
Si2 Of Oc 63.5(6) 208_455 . -304_556 N
Si2 Of Dc1 92.2(8) 208_464 . -3_555 N
Si2 Of Dc1 88.3(7) 208_464 . -207_575 N
Si2 Of Dc1 74.3(8) 208_464 . -304_565 N
Si2 Of Dc2 78.0(7) 208_465 . -3_555 N
Si2 Of Dc2 95.5(9) 208_465 . -108_666 N
Si2 Of Dc2 52.2(7) 208_465 . -304_566 N
Si2 Of Od 98.9(11) 208_464 . 1_555 N
Si2 Of Od 83.5(12) 208_464 . -207_575 N
Si2 Of Od 57.9(11) 208_464 . -304_565 N
Al1 Of O1 67.6(7) 208_343 . 111_433 N
Al1 Of O1 28.7(4) 208_343 . -108_544 N
Al1 Of O2 27.92(30) 208_343 . 1_555 N
Al1 Of O3 66.3(6) 208_343 . 4_555 N
Al1 Of O4 30.52(33) 208_343 . 310_334 N
Al1 Of O4 65.0(6) 208_343 . 312_334 N
Al1 Of SJ 95.2(9) 208_455 . 1_555 N
Al1 Of SJ 78.7(8) 208_455 . -207_566 N
Al1 Of SJ 51.1(9) 208_455 . -304_556 N
Al1 Of Oc 87.9(8) 208_455 . -3_555 N
Al1 Of Oc 110.8(10) 208_455 . -108_656 N
Al1 Of Oc 63.5(6) 208_455 . -304_556 N
Al1 Of Dc1 92.2(8) 208_464 . -3_555 N
Al1 Of Dc1 88.3(7) 208_464 . -207_575 N
Al1 Of Dc1 74.3(8) 208_464 . -304_565 N
Al1 Of Dc2 78.0(7) 208_465 . -3_555 N
Al1 Of Dc2 95.5(9) 208_465 . -108_666 N
Al1 Of Dc2 52.2(7) 208_465 . -304_566 N
Al1 Of Od 98.9(11) 208_464 . 1_555 N
Al1 Of Od 83.5(12) 208_464 . -207_575 N
Al1 Of Od 57.9(11) 208_464 . -304_565 N
O1 Of O1 71.0(8) 111_433 . -108_544 N
O1 Of O2 42.0(4) 111_433 . 1_555 N
O1 Of O3 45.4(4) 111_433 . 4_555 N
O1 Of O4 88.2(8) 111_433 . 310_334 N
O1 Of O4 41.0(4) 111_433 . 312_334 N
O1 Of SJ 49.8(7) 111_545 . 1_555 N
O1 Of SJ 111.5(10) 111_545 . -207_566 N
O1 Of SJ 118.7(13) 111_545 . -304_556 N
O1 Of Oc 150.2(11) 111_545 . -3_555 N
O1 Of Oc 45.3(5) 111_545 . -108_656 N
O1 Of Oc 122.5(11) 111_545 . -304_556 N
O1 Of Dc1 157.7(11) 111_554 . -3_555 N
O1 Of Dc1 132.2(9) 111_554 . -207_575 N
O1 Of Dc1 138.7(12) 111_554 . -304_565 N
O1 Of Dc2 135.4(10) 111_555 . -3_555 N
O1 Of Dc2 29.29(33) 111_555 . -108_666 N
O1 Of Dc2 108.7(12) 111_555 . -304_566 N
O1 Of Od 48.4(9) 111_554 . 1_555 N
O1 Of Od 117.6(13) 111_554 . -207_575 N
O1 Of Od 125.6(15) 111_554 . -304_565 N
O1 Of O2 46.0(5) -108_544 . 1_555 N
O1 Of O3 47.0(5) -108_544 . 4_555 N
O1 Of O4 55.3(6) -108_544 . 310_334 N
O1 Of O4 86.7(9) -108_544 . 312_334 N
O1 Of SJ 114.1(11) -108_656 . 1_555 N
O1 Of SJ 54.0(6) -108_656 . -207_566 N
O1 Of SJ 57.0(10) -108_656 . -304_556 N
O1 Of Oc 96.0(9) -108_656 . -3_555 N
O1 Of Oc 115.4(11) -108_656 . -108_656 N
O1 Of Oc 51.6(5) -108_656 . -304_556 N
O1 Of Dc1 96.2(8) -108_665 . -3_555 N
O1 Of Dc1 69.2(6) -108_665 . -207_575 N
O1 Of Dc1 68.0(7) -108_665 . -304_565 N
O1 Of Dc2 92.1(9) -108_666 . -3_555 N
O1 Of Dc2 99.7(10) -108_666 . -108_666 N
O1 Of Dc2 37.8(6) -108_666 . -304_566 N
O1 Of Od 115.7(13) -108_665 . 1_555 N
O1 Of Od 59.9(11) -108_665 . -207_575 N
O1 Of Od 61.7(12) -108_665 . -304_565 N
O2 Of O3 59.7(5) 1_555 . 4_555 N
O2 Of O4 46.9(5) 1_555 . 310_334 N
O2 Of O4 40.7(4) 1_555 . 312_334 N
O2 Of SJ 69.5(7) 1_555 . 1_555 N
O2 Of SJ 100.0(9) 1_555 . -207_566 N
O2 Of SJ 77.4(10) 1_555 . -304_556 N
O2 Of Oc 109.8(9) 1_555 . -3_555 N
O2 Of Oc 83.0(7) 1_555 . -108_656 N
O2 Of Oc 91.0(8) 1_555 . -304_556 N
O2 Of Dc1 116.1(9) 1_555 . -3_555 N
O2 Of Dc1 114.0(8) 1_555 . -207_575 N
O2 Of Dc1 102.1(10) 1_555 . -304_565 N
O2 Of Dc2 96.7(8) 1_555 . -3_555 N
O2 Of Dc2 68.0(6) 1_555 . -108_666 N
O2 Of Dc2 78.8(10) 1_555 . -304_566 N
O2 Of Od 72.3(9) 1_555 . 1_555 N
O2 Of Od 105.9(13) 1_555 . -207_575 N
O2 Of Od 84.5(12) 1_555 . -304_565 N
O3 Of O4 96.8(9) 4_555 . 310_334 N
O3 Of O4 83.9(7) 4_555 . 312_334 N
O3 Of SJ 93.8(9) 4_555 . 1_555 N
O3 Of SJ 66.9(7) 4_555 . -207_566 N
O3 Of SJ 103.1(12) 4_555 . -304_556 N
O3 Of Oc 139.5(9) 4_555 . -3_555 N
O3 Of Oc 76.4(7) 4_555 . -108_656 N
O3 Of Oc 87.2(8) 4_555 . -304_556 N
O3 Of Dc1 136.1(8) 4_555 . -3_555 N
O3 Of Dc1 87.6(7) 4_555 . -207_575 N
O3 Of Dc1 104.6(9) 4_555 . -304_565 N
O3 Of Dc2 139.0(10) 4_555 . -3_555 N
O3 Of Dc2 64.4(6) 4_555 . -108_666 N
O3 Of Dc2 75.5(9) 4_555 . -304_566 N
O3 Of Od 91.1(11) 4_555 . 1_555 N
O3 Of Od 72.7(11) 4_555 . -207_575 N
O3 Of Od 106.7(14) 4_555 . -304_565 N
O4 Of O4 65.9(6) 310_334 . 312_334 N
O4 Of SJ 93.0(8) 310_446 . 1_555 N
O4 Of SJ 90.8(8) 310_446 . -207_566 N
O4 Of SJ 36.7(8) 310_446 . -304_556 N
O4 Of Oc 62.9(6) 310_446 . -3_555 N
O4 Of Oc 120.4(10) 310_446 . -108_656 N
O4 Of Oc 63.4(6) 310_446 . -304_556 N
O4 Of Dc1 69.5(6) 310_455 . -3_555 N
O4 Of Dc1 90.1(7) 310_455 . -207_575 N
O4 Of Dc1 64.9(7) 310_455 . -304_565 N
O4 Of Dc2 50.2(5) 310_456 . -3_555 N
O4 Of Dc2 109.5(9) 310_456 . -108_666 N
O4 Of Dc2 58.9(8) 310_456 . -304_566 N
O4 Of Od 98.4(10) 310_455 . 1_555 N
O4 Of Od 93.0(12) 310_455 . -207_575 N
O4 Of Od 43.3(11) 310_455 . -304_565 N
O4 Of SJ 30.3(5) 312_446 . 1_555 N
O4 Of SJ 140.5(11) 312_446 . -207_566 N
O4 Of SJ 102.6(12) 312_446 . -304_556 N
O4 Of Oc 113.9(9) 312_446 . -3_555 N
O4 Of Oc 54.5(5) 312_446 . -108_656 N
O4 Of Oc 126.9(10) 312_446 . -304_556 N
O4 Of Dc1 122.6(8) 312_455 . -3_555 N
O4 Of Dc1 153.3(10) 312_455 . -207_575 N
O4 Of Dc1 130.7(11) 312_455 . -304_565 N
O4 Of Dc2 99.2(8) 312_456 . -3_555 N
O4 Of Dc2 46.0(5) 312_456 . -108_666 N
O4 Of Dc2 117.2(12) 312_456 . -304_566 N
O4 Of Od 34.5(8) 312_455 . 1_555 N
O4 Of Od 146.6(14) 312_455 . -207_575 N
O4 Of Od 108.9(14) 312_455 . -304_565 N
SJ Of SJ 160.7(13) 1_555 . -207_566 N
SJ Of SJ 127.7(14) 1_555 . -304_556 N
SJ Of Oc 120.2(10) 1_555 . -3_555 N
SJ Of Oc 31.3(6) 1_555 . -108_656 N
SJ Of Oc 156.3(12) 1_555 . -304_556 N
SJ Of Dc1 127.3(10) 1_555 . -3_555 N
SJ Of Dc1 176.4(12) 1_555 . -207_575 N
SJ Of Dc1 152.3(12) 1_555 . -304_565 N
SJ Of Dc2 109.4(9) 1_555 . -3_555 N
SJ Of Dc2 32.8(6) 1_555 . -108_666 N
SJ Of Dc2 147.5(14) 1_555 . -304_566 N
SJ Of Od 5.8(9) 1_555 . 1_555 N
SJ Of Od 165.8(15) 1_555 . -207_575 N
SJ Of Od 132.5(15) 1_555 . -304_565 N
SJ Of SJ 61.8(9) -207_566 . -304_556 N
SJ Of Oc 78.2(8) -207_566 . -3_555 N
SJ Of Oc 134.4(11) -207_566 . -108_656 N
SJ Of Oc 31.7(5) -207_566 . -304_556 N
SJ Of Dc1 71.6(7) -207_575 . -3_555 N
SJ Of Dc1 20.7(6) -207_575 . -207_575 N
SJ Of Dc1 43.5(6) -207_575 . -304_565 N
SJ Of Dc2 87.4(8) -207_576 . -3_555 N
SJ Of Dc2 128.8(11) -207_576 . -108_666 N
SJ Of Dc2 32.0(7) -207_576 . -304_566 N
SJ Of Od 157.2(13) -207_575 . 1_555 N
SJ Of Od 6.4(11) -207_575 . -207_575 N
SJ Of Od 59.2(13) -207_575 . -304_565 N
SJ Of Oc 39.5(8) -304_556 . -3_555 N
SJ Of Oc 157.1(14) -304_556 . -108_656 N
SJ Of Oc 30.4(8) -304_556 . -304_556 N
SJ Of Dc1 41.8(8) -304_565 . -3_555 N
SJ Of Dc1 54.9(9) -304_565 . -207_575 N
SJ Of Dc1 28.1(8) -304_565 . -304_565 N
SJ Of Dc2 36.0(8) -304_566 . -3_555 N
SJ Of Dc2 145.0(14) -304_566 . -108_666 N
SJ Of Dc2 33.2(9) -304_566 . -304_566 N
SJ Of Od 133.5(14) -304_565 . 1_555 N
SJ Of Od 61.6(13) -304_565 . -207_575 N
SJ Of Od 7.1(11) -304_565 . -304_565 N
Oc Of Oc 143.8(11) -3_555 . -108_656 N
Oc Of Oc 52.7(6) -3_555 . -304_556 N
Oc Of Dc1 8.73(32) -3_555 . -3_555 N
Oc Of Dc1 59.8(6) -3_555 . -207_575 N
Oc Of Dc1 35.9(5) -3_555 . -304_565 N
Oc Of Dc2 15.07(27) -3_555 . -3_555 N
Oc Of Dc2 153.0(10) -3_555 . -108_666 N
Oc Of Dc2 64.0(8) -3_555 . -304_566 N
Oc Of Od 124.6(12) -3_555 . 1_555 N
Oc Of Od 73.9(11) -3_555 . -207_575 N
Oc Of Od 34.3(11) -3_555 . -304_565 N
Oc Of Oc 163.4(12) -108_656 . -304_556 N
Oc Of Dc1 147.0(11) -108_665 . -3_555 N
Oc Of Dc1 146.6(10) -108_665 . -207_575 N
Oc Of Dc1 174.6(13) -108_665 . -304_565 N
Oc Of Dc2 137.8(9) -108_666 . -3_555 N
Oc Of Dc2 16.05(20) -108_666 . -108_666 N
Oc Of Dc2 151.5(14) -108_666 . -304_566 N
Oc Of Od 25.6(8) -108_665 . 1_555 N
Oc Of Od 136.7(14) -108_665 . -207_575 N
Oc Of Od 163.2(15) -108_665 . -304_565 N
Oc Of Dc1 49.0(6) -304_565 . -3_555 N
Oc Of Dc1 27.0(4) -304_565 . -207_575 N
Oc Of Dc1 17.68(19) -304_565 . -304_565 N
Oc Of Dc2 58.1(6) -304_566 . -3_555 N
Oc Of Dc2 150.3(12) -304_566 . -108_666 N
Oc Of Dc2 13.8(4) -304_566 . -304_566 N
Oc Of Od 161.3(13) -304_565 . 1_555 N
Oc Of Od 31.3(9) -304_565 . -207_575 N
Oc Of Od 27.5(11) -304_565 . -304_565 N
Dc1 Of Dc1 52.4(6) -3_555 . -207_575 N
Dc1 Of Dc1 31.4(5) -3_555 . -304_565 N
Dc1 Of Dc2 23.67(25) -3_555 . -3_555 N
Dc1 Of Dc2 159.3(10) -3_555 . -108_666 N
Dc1 Of Dc2 61.5(8) -3_555 . -304_566 N
Dc1 Of Od 131.2(11) -3_555 . 1_555 N
Dc1 Of Od 66.9(11) -3_555 . -207_575 N
Dc1 Of Od 35.6(11) -3_555 . -304_565 N
Dc1 Of Dc1 29.4(6) -207_575 . -304_565 N
Dc1 Of Dc2 71.3(7) -207_576 . -3_555 N
Dc1 Of Dc2 146.8(10) -207_576 . -108_666 N
Dc1 Of Dc2 36.1(5) -207_576 . -304_566 N
Dc1 Of Od 171.5(12) -207_575 . 1_555 N
Dc1 Of Od 14.9(9) -207_575 . -207_575 N
Dc1 Of Od 49.9(12) -207_575 . -304_565 N
Dc1 Of Dc2 43.9(6) -304_566 . -3_555 N
Dc1 Of Dc2 167.7(13) -304_566 . -108_666 N
Dc1 Of Dc2 30.9(4) -304_566 . -304_566 N
Dc1 Of Od 157.9(13) -304_565 . 1_555 N
Dc1 Of Od 40.5(10) -304_565 . -207_575 N
Dc1 Of Od 21.8(11) -304_565 . -304_565 N
Dc2 Of Dc2 141.6(9) -3_555 . -108_666 N
Dc2 Of Dc2 66.6(8) -3_555 . -304_566 N
Dc2 Of Od 114.5(11) -3_555 . 1_555 N
Dc2 Of Od 84.2(11) -3_555 . -207_575 N
Dc2 Of Od 33.5(12) -3_555 . -304_565 N
Dc2 Of Dc2 136.9(14) -108_666 . -304_566 N
Dc2 Of Od 28.4(9) -108_665 . 1_555 N
Dc2 Of Od 133.1(13) -108_665 . -207_575 N
Dc2 Of Od 152.1(16) -108_665 . -304_565 N
Dc2 Of Od 151.0(15) -304_565 . 1_555 N
Dc2 Of Od 34.4(10) -304_565 . -207_575 N
Dc2 Of Od 33.4(12) -304_565 . -304_565 N
Od Of Od 161.3(13) 1_555 . -207_575 N
Od Of Od 138.3(17) 1_555 . -304_565 N
Od Of Od 58.1(14) -207_575 . -304_565 N
O1 Df1 O4 46.5(5) -108_544 . 310_334 N
O1 Df1 SJ 105.9(13) -108_656 . -3_555 N
O1 Df1 SJ 53.3(10) -108_656 . -207_566 N
O1 Df1 SJ 49.2(10) -108_656 . -304_556 N
O1 Df1 Oc 92.1(14) -108_656 . -3_555 N
O1 Df1 Oc 91.9(9) -108_656 . -108_656 N
O1 Df1 Oc 76.6(11) -108_656 . -207_566 N
O1 Df1 Oc 48.2(8) -108_656 . -304_556 N
O1 Df1 Dc1 97.5(14) -108_665 . -3_555 N
O1 Df1 Dc1 71.4(11) -108_665 . -207_575 N
O1 Df1 Dc1 64.1(11) -108_665 . -304_565 N
O1 Df1 Dc2 86.4(11) -108_666 . -3_555 N
O1 Df1 Dc2 30.1(6) -108_666 . -304_566 N
O1 Df1 Od 109.8(15) -108_665 . -3_555 N
O1 Df1 Od 58.1(15) -108_665 . -207_575 N
O1 Df1 Od 55.9(13) -108_665 . -304_565 N
O1 Df1 Dd1 120.3(21) -108_644 . -3_555 N
O1 Df1 Dd1 99.3(14) -108_644 . -108_644 N
O1 Df1 Dd1 75.9(18) -108_644 . -207_554 N
O1 Df1 Dd1 58.3(16) -108_644 . -304_544 N
O1 Df1 Dd2 49.8(19) -108_644 . -207_554 N
O1 Df1 Dd2 49.6(18) -108_644 . -304_544 N
O1 Df1 OII* 97.4(19) -108_544 . -301_444 N
O1 Df1 DII*1 149.3(24) -108_543 . -208_443 N
O4 Df1 SJ 67.5(10) 310_446 . -3_555 N
O4 Df1 SJ 86.9(12) 310_446 . -207_566 N
O4 Df1 SJ 29.1(8) 310_446 . -304_556 N
O4 Df1 Oc 58.0(9) 310_446 . -3_555 N
O4 Df1 Oc 96.5(9) 310_446 . -108_656 N
O4 Df1 Oc 102.4(12) 310_446 . -207_566 N
O4 Df1 Oc 58.5(8) 310_446 . -304_556 N
O4 Df1 Dc1 69.8(10) 310_455 . -3_555 N
O4 Df1 Dc1 91.0(12) 310_455 . -207_575 N
O4 Df1 Dc1 59.8(10) 310_455 . -304_565 N
O4 Df1 Dc2 46.9(7) 310_456 . -3_555 N
O4 Df1 Dc2 49.8(9) 310_456 . -304_566 N
O4 Df1 Od 73.4(13) 310_455 . -3_555 N
O4 Df1 Od 89.5(16) 310_455 . -207_575 N
O4 Df1 Od 37.6(12) 310_455 . -304_565 N
O4 Df1 Dd1 84.9(18) 310_434 . -3_555 N
O4 Df1 Dd1 116.4(14) 310_434 . -108_644 N
O4 Df1 Dd1 106.5(22) 310_434 . -207_554 N
O4 Df1 Dd1 47.2(13) 310_434 . -304_544 N
O4 Df1 Dd2 90.5(22) 310_434 . -207_554 N
O4 Df1 Dd2 22.9(11) 310_434 . -304_544 N
O4 Df1 OII* 142.8(19) 310_334 . -301_444 N
O4 Df1 DII*1 102.8(22) 310_333 . -208_443 N
SJ Df1 SJ 101.8(15) -3_555 . -207_566 N
SJ Df1 SJ 56.9(11) -3_555 . -304_556 N
SJ Df1 Oc 14.7(7) -3_555 . -3_555 N
SJ Df1 Oc 129.5(16) -3_555 . -108_656 N
SJ Df1 Oc 91.0(10) -3_555 . -207_566 N
SJ Df1 Oc 72.9(11) -3_555 . -304_556 N
SJ Df1 Dc1 19.4(6) -3_555 . -3_555 N
SJ Df1 Dc1 81.7(11) -3_555 . -207_575 N
SJ Df1 Dc1 55.2(11) -3_555 . -304_565 N
SJ Df1 Dc2 20.7(6) -3_555 . -3_555 N
SJ Df1 Dc2 84.8(14) -3_555 . -304_566 N
SJ Df1 Od 6.5(10) -3_555 . -3_555 N
SJ Df1 Od 98.5(16) -3_555 . -207_575 N
SJ Df1 Od 51.4(15) -3_555 . -304_565 N
SJ Df1 Dd1 17.5(15) -3_555 . -3_555 N
SJ Df1 Dd1 142.9(20) -3_555 . -108_644 N
SJ Df1 Dd1 98.5(23) -3_555 . -207_554 N
SJ Df1 Dd1 53.0(16) -3_555 . -304_544 N
SJ Df1 Dd2 115.5(19) -3_555 . -207_554 N
SJ Df1 Dd2 56.5(19) -3_555 . -304_544 N
SJ Df1 OII* 146.3(17) -3_555 . -301_444 N
SJ Df1 DII*1 51.4(28) -3_555 . -208_443 N
SJ Df1 SJ 66.0(13) -207_566 . -304_556 N
SJ Df1 Oc 89.6(15) -207_566 . -3_555 N
SJ Df1 Oc 125.8(15) -207_566 . -108_656 N
SJ Df1 Oc 23.8(7) -207_566 . -207_566 N
SJ Df1 Oc 34.6(8) -207_566 . -304_556 N
SJ Df1 Dc1 82.8(13) -207_575 . -3_555 N
SJ Df1 Dc1 23.9(7) -207_575 . -207_575 N
SJ Df1 Dc1 48.4(11) -207_575 . -304_565 N
SJ Df1 Dc2 95.9(14) -207_576 . -3_555 N
SJ Df1 Dc2 37.1(10) -207_576 . -304_566 N
SJ Df1 Od 99.7(15) -207_575 . -3_555 N
SJ Df1 Od 5.3(12) -207_575 . -207_575 N
SJ Df1 Od 63.6(16) -207_575 . -304_565 N
SJ Df1 Dd1 101.9(22) -207_554 . -3_555 N
SJ Df1 Dd1 115.0(19) -207_554 . -108_644 N
SJ Df1 Dd1 22.7(15) -207_554 . -207_554 N
SJ Df1 Dd1 56.0(15) -207_554 . -304_544 N
SJ Df1 Dd2 13.9(12) -207_554 . -207_554 N
SJ Df1 Dd2 71.9(19) -207_554 . -304_544 N
SJ Df1 OII* 73.1(14) -207_454 . -301_444 N
SJ Df1 DII*1 141.4(33) -207_453 . -208_443 N
SJ Df1 Oc 42.9(11) -304_556 . -3_555 N
SJ Df1 Oc 124.8(13) -304_556 . -108_656 N
SJ Df1 Oc 75.8(14) -304_556 . -207_566 N
SJ Df1 Oc 32.5(9) -304_556 . -304_556 N
SJ Df1 Dc1 49.8(11) -304_565 . -3_555 N
SJ Df1 Dc1 63.6(13) -304_565 . -207_575 N
SJ Df1 Dc1 30.7(10) -304_565 . -304_565 N
SJ Df1 Dc2 38.6(10) -304_566 . -3_555 N
SJ Df1 Dc2 32.4(10) -304_566 . -304_566 N
SJ Df1 Od 60.6(14) -304_565 . -3_555 N
SJ Df1 Od 66.8(18) -304_565 . -207_575 N
SJ Df1 Od 9.2(12) -304_565 . -304_565 N
SJ Df1 Dd1 71.3(19) -304_544 . -3_555 N
SJ Df1 Dd1 142.6(16) -304_544 . -108_644 N
SJ Df1 Dd1 81.2(24) -304_544 . -207_554 N
SJ Df1 Dd1 18.1(14) -304_544 . -304_544 N
SJ Df1 Dd2 74.6(23) -304_544 . -207_554 N
SJ Df1 Dd2 6.7(15) -304_544 . -304_544 N
SJ Df1 OII* 137.8(24) -304_444 . -301_444 N
SJ Df1 DII*1 106.0(29) -304_443 . -208_443 N
Oc Df1 Oc 137.0(19) -3_555 . -108_656 N
Oc Df1 Oc 82.8(13) -3_555 . -207_566 N
Oc Df1 Oc 58.8(11) -3_555 . -304_556 N
Oc Df1 Dc1 13.9(4) -3_555 . -3_555 N
Oc Df1 Dc1 72.0(13) -3_555 . -207_575 N
Oc Df1 Dc1 41.7(9) -3_555 . -304_565 N
Oc Df1 Dc2 13.4(4) -3_555 . -3_555 N
Oc Df1 Dc2 70.1(13) -3_555 . -304_566 N
Oc Df1 Od 17.7(9) -3_555 . -3_555 N
Oc Df1 Od 87.0(18) -3_555 . -207_575 N
Oc Df1 Od 36.8(13) -3_555 . -304_565 N
Oc Df1 Dd1 28.7(14) -3_555 . -3_555 N
Oc Df1 Dd1 155.0(25) -3_555 . -108_644 N
Oc Df1 Dd1 90.5(25) -3_555 . -207_554 N
Oc Df1 Dd1 38.4(15) -3_555 . -304_544 N
Oc Df1 Dd2 102.9(21) -3_555 . -207_554 N
Oc Df1 Dd2 43.4(18) -3_555 . -304_544 N
Oc Df1 OII* 148.9(18) -3_555 . -301_444 N
Oc Df1 DII*1 66.1(29) -3_555 . -208_443 N
Oc Df1 Oc 139.5(15) -108_656 . -207_566 N
Oc Df1 Oc 140.1(13) -108_656 . -304_556 N
Oc Df1 Dc1 148.6(19) -108_665 . -3_555 N
Oc Df1 Dc1 148.4(17) -108_665 . -207_575 N
Oc Df1 Dc1 153.8(14) -108_665 . -304_565 N
Oc Df1 Dc2 125.1(15) -108_666 . -3_555 N
Oc Df1 Dc2 122.0(13) -108_666 . -304_566 N
Oc Df1 Od 133.2(18) -108_665 . -3_555 N
Oc Df1 Od 130.1(19) -108_665 . -207_575 N
Oc Df1 Od 133.9(16) -108_665 . -304_565 N
Oc Df1 Dd1 132.3(25) -108_644 . -3_555 N
Oc Df1 Dd1 21.7(12) -108_644 . -108_644 N
Oc Df1 Dd1 131.9(27) -108_644 . -207_554 N
Oc Df1 Dd1 142.6(16) -108_644 . -304_544 N
Oc Df1 Dd2 112.1(17) -108_644 . -207_554 N
Oc Df1 Dd2 119.2(15) -108_644 . -304_544 N
Oc Df1 OII* 72.4(10) -108_544 . -301_444 N
Oc Df1 DII*1 90.6(34) -108_543 . -208_443 N
Oc Df1 Oc 44.0(8) -207_566 . -304_556 N
Oc Df1 Dc1 71.9(10) -207_575 . -3_555 N
Oc Df1 Dc1 12.54(29) -207_575 . -207_575 N
Oc Df1 Dc1 48.5(10) -207_575 . -304_565 N
Oc Df1 Dc2 93.2(12) -207_576 . -3_555 N
Oc Df1 Dc2 54.9(11) -207_576 . -304_566 N
Oc Df1 Od 86.8(12) -207_575 . -3_555 N
Oc Df1 Od 18.7(12) -207_575 . -207_575 N
Oc Df1 Od 69.9(15) -207_575 . -304_565 N
Oc Df1 Dd1 85.3(20) -207_554 . -3_555 N
Oc Df1 Dd1 121.4(19) -207_554 . -108_644 N
Oc Df1 Dd1 7.7(20) -207_554 . -207_554 N
Oc Df1 Dd1 60.2(14) -207_554 . -304_544 N
Oc Df1 Dd2 33.6(14) -207_554 . -207_554 N
Oc Df1 Dd2 82.4(17) -207_554 . -304_544 N
Oc Df1 OII* 70.9(10) -207_454 . -301_444 N
Oc Df1 DII*1 119.0(30) -207_453 . -208_443 N
Oc Df1 Dc1 56.6(10) -304_565 . -3_555 N
Oc Df1 Dc1 32.7(7) -304_565 . -207_575 N
Oc Df1 Dc1 18.4(4) -304_565 . -304_565 N
Oc Df1 Dc2 62.3(10) -304_566 . -3_555 N
Oc Df1 Dc2 18.1(4) -304_566 . -304_566 N
Oc Df1 Od 73.2(13) -304_565 . -3_555 N
Oc Df1 Od 34.6(12) -304_565 . -207_575 N
Oc Df1 Od 29.0(12) -304_565 . -304_565 N
Oc Df1 Dd1 79.9(20) -304_544 . -3_555 N
Oc Df1 Dd1 142.7(20) -304_544 . -108_644 N
Oc Df1 Dd1 48.9(19) -304_544 . -207_554 N
Oc Df1 Dd1 21.7(13) -304_544 . -304_544 N
Oc Df1 Dd2 45.7(17) -304_544 . -207_554 N
Oc Df1 Dd2 39.0(15) -304_544 . -304_544 N
Oc Df1 OII* 107.7(19) -304_444 . -301_444 N
Oc Df1 DII*1 123.2(33) -304_443 . -208_443 N
Dc1 Df1 Dc1 62.3(11) -3_555 . -207_575 N
Dc1 Df1 Dc1 38.2(8) -3_555 . -304_565 N
Dc1 Df1 Dc2 27.2(4) -3_555 . -3_555 N
Dc1 Df1 Dc2 71.2(13) -3_555 . -304_566 N
Dc1 Df1 Od 17.2(8) -3_555 . -3_555 N
Dc1 Df1 Od 79.2(16) -3_555 . -207_575 N
Dc1 Df1 Od 41.8(13) -3_555 . -304_565 N
Dc1 Df1 Dd1 23.7(15) -3_555 . -3_555 N
Dc1 Df1 Dd1 160.7(21) -3_555 . -108_644 N
Dc1 Df1 Dd1 79.5(23) -3_555 . -207_554 N
Dc1 Df1 Dd1 39.6(15) -3_555 . -304_544 N
Dc1 Df1 Dd2 96.6(19) -3_555 . -207_554 N
Dc1 Df1 Dd2 52.0(17) -3_555 . -304_544 N
Dc1 Df1 OII* 135.1(16) -3_555 . -301_444 N
Dc1 Df1 DII*1 66.6(31) -3_555 . -208_443 N
Dc1 Df1 Dc1 36.0(9) -207_575 . -304_565 N
Dc1 Df1 Dc2 81.6(12) -207_576 . -3_555 N
Dc1 Df1 Dc2 45.9(10) -207_576 . -304_566 N
Dc1 Df1 Od 78.4(13) -207_575 . -3_555 N
Dc1 Df1 Od 18.9(11) -207_575 . -207_575 N
Dc1 Df1 Od 57.5(15) -207_575 . -304_565 N
Dc1 Df1 Dd1 78.8(20) -207_554 . -3_555 N
Dc1 Df1 Dd1 132.8(21) -207_554 . -108_644 N
Dc1 Df1 Dd1 19.5(20) -207_554 . -207_554 N
Dc1 Df1 Dd1 47.7(13) -207_554 . -304_544 N
Dc1 Df1 Dd2 37.0(13) -207_554 . -207_554 N
Dc1 Df1 Dd2 70.3(16) -207_554 . -304_544 N
Dc1 Df1 OII* 83.1(13) -207_454 . -301_444 N
Dc1 Df1 DII*1 117.6(33) -207_453 . -208_443 N
Dc1 Df1 Dc2 47.7(10) -304_566 . -3_555 N
Dc1 Df1 Dc2 34.7(7) -304_566 . -304_566 N
Dc1 Df1 Od 55.0(12) -304_565 . -3_555 N
Dc1 Df1 Od 46.5(14) -304_565 . -207_575 N
Dc1 Df1 Od 22.7(12) -304_565 . -304_565 N
Dc1 Df1 Dd1 61.5(18) -304_544 . -3_555 N
Dc1 Df1 Dd1 161.1(22) -304_544 . -108_644 N
Dc1 Df1 Dd1 55.3(22) -304_544 . -207_554 N
Dc1 Df1 Dd1 12.7(12) -304_544 . -304_544 N
Dc1 Df1 Dd2 61.3(18) -304_544 . -207_554 N
Dc1 Df1 Dd2 37.1(13) -304_544 . -304_544 N
Dc1 Df1 OII* 118.7(20) -304_444 . -301_444 N
Dc1 Df1 DII*1 104.8(33) -304_443 . -208_443 N
Dc2 Df1 Dc2 69.7(12) -3_555 . -304_566 N
Dc2 Df1 Od 26.5(10) -3_555 . -3_555 N
Dc2 Df1 Od 94.2(17) -3_555 . -207_575 N
Dc2 Df1 Od 35.5(13) -3_555 . -304_565 N
Dc2 Df1 Dd1 38.0(15) -3_555 . -3_555 N
Dc2 Df1 Dd1 145.3(21) -3_555 . -108_644 N
Dc2 Df1 Dd1 100.8(25) -3_555 . -207_554 N
Dc2 Df1 Dd1 40.6(14) -3_555 . -304_544 N
Dc2 Df1 Dd2 108.0(21) -3_555 . -207_554 N
Dc2 Df1 Dd2 36.9(19) -3_555 . -304_544 N
Dc2 Df1 OII* 162.1(17) -3_555 . -301_444 N
Dc2 Df1 DII*1 67.5(25) -3_555 . -208_443 N
Dc2 Df1 Od 86.6(16) -304_565 . -3_555 N
Dc2 Df1 Od 39.7(14) -304_565 . -207_575 N
Dc2 Df1 Od 34.3(13) -304_565 . -304_565 N
Dc2 Df1 Dd1 95.0(22) -304_544 . -3_555 N
Dc2 Df1 Dd1 127.3(19) -304_544 . -108_644 N
Dc2 Df1 Dd1 57.5(19) -304_544 . -207_554 N
Dc2 Df1 Dd1 32.1(15) -304_544 . -304_544 N
Dc2 Df1 Dd2 42.9(20) -304_544 . -207_554 N
Dc2 Df1 Dd2 37.0(19) -304_544 . -304_544 N
Dc2 Df1 OII* 105.5(22) -304_444 . -301_444 N
Dc2 Df1 DII*1 136.2(32) -304_443 . -208_443 N
Od Df1 Od 96.0(21) -3_555 . -207_575 N
Od Df1 Od 54.3(14) -3_555 . -304_565 N
Od Df1 Dd1 11.5(10) -3_555 . -3_555 N
Od Df1 Dd1 143.8(20) -3_555 . -108_644 N
Od Df1 Dd1 94.2(26) -3_555 . -207_554 N
Od Df1 Dd1 54.5(16) -3_555 . -304_544 N
Od Df1 Dd2 113.6(23) -3_555 . -207_554 N
Od Df1 Dd2 60.9(18) -3_555 . -304_544 N
Od Df1 OII* 139.7(19) -3_555 . -301_444 N
Od Df1 DII*1 50.2(29) -3_555 . -208_443 N
Od Df1 Od 63.5(15) -207_575 . -304_565 N
Od Df1 Dd1 97.5(25) -207_554 . -3_555 N
Od Df1 Dd1 117.9(24) -207_554 . -108_644 N
Od Df1 Dd1 18.3(7) -207_554 . -207_554 N
Od Df1 Dd1 55.2(17) -207_554 . -304_544 N
Od Df1 Dd2 18.1(6) -207_554 . -207_554 N
Od Df1 Dd2 73.0(17) -207_554 . -304_544 N
Od Df1 OII* 73.5(17) -207_454 . -301_444 N
Od Df1 DII*1 136.2(35) -207_453 . -208_443 N
Od Df1 Dd1 64.3(19) -304_544 . -3_555 N
Od Df1 Dd1 151.8(21) -304_544 . -108_644 N
Od Df1 Dd1 76.1(22) -304_544 . -207_554 N
Od Df1 Dd1 10.0(11) -304_544 . -304_544 N
Od Df1 Dd2 73.9(22) -304_544 . -207_554 N
Od Df1 Dd2 14.8(9) -304_544 . -304_544 N
Od Df1 OII* 136.7(24) -304_444 . -301_444 N
Od Df1 DII*1 102.2(31) -304_443 . -208_443 N
Dd1 Df1 Dd1 137.3(21) -3_555 . -108_644 N
Dd1 Df1 Dd1 92(4) -3_555 . -207_554 N
Dd1 Df1 Dd1 63.2(23) -3_555 . -304_544 N
Dd1 Df1 Dd2 115.6(26) -3_555 . -207_554 N
Dd1 Df1 Dd2 72.1(25) -3_555 . -304_544 N
Dd1 Df1 OII* 129.2(23) -3_555 . -301_444 N
Dd1 Df1 DII*1 43.6(33) -3_555 . -208_443 N
Dd1 Df1 Dd1 113.8(34) -108_644 . -207_554 N
Dd1 Df1 Dd1 157.4(25) -108_644 . -304_544 N
Dd1 Df1 Dd2 101.5(21) -108_644 . -207_554 N
Dd1 Df1 Dd2 138.1(19) -108_644 . -304_544 N
Dd1 Df1 OII* 51.4(14) -108_544 . -301_444 N
Dd1 Df1 DII*1 94.1(33) -108_543 . -208_443 N
Dd1 Df1 Dd1 66.6(25) -207_554 . -304_544 N
Dd1 Df1 Dd2 29.3(14) -207_554 . -207_554 N
Dd1 Df1 Dd2 87.8(27) -207_554 . -304_544 N
Dd1 Df1 OII* 63.7(22) -207_454 . -301_444 N
Dd1 Df1 DII*1 123.1(34) -207_453 . -208_443 N
Dd1 Df1 Dd2 67.4(23) -304_544 . -207_554 N
Dd1 Df1 Dd2 24.4(5) -304_544 . -304_544 N
Dd1 Df1 OII* 128.7(21) -304_444 . -301_444 N
Dd1 Df1 DII*1 104.4(33) -304_443 . -208_443 N
Dd2 Df1 Dd2 79.7(16) -207_554 . -304_544 N
Dd2 Df1 OII* 63.3(21) -207_454 . -301_444 N
Dd2 Df1 DII*1 152.4(34) -207_453 . -208_443 N
Dd2 Df1 OII* 142.3(27) -304_444 . -301_444 N
Dd2 Df1 DII*1 103.5(32) -304_443 . -208_443 N
OII* Df1 DII*1 112.4(28) -301_443 . -208_443 N
Si1 Df2 Si1 80.0(12) 111_434 . -108_545 N
Si1 Df2 Si2 55.2(10) 111_533 . 208_443 N
Si1 Df2 Si2 47.1(7) 111_533 . -211_554 N
Si1 Df2 Al1 55.2(10) 111_443 . 208_353 N
Si1 Df2 Al1 47.1(7) 111_443 . -211_464 N
Si1 Df2 O1 25.4(4) 111_433 . 111_433 N
Si1 Df2 O1 74.0(17) 111_433 . -108_544 N
Si1 Df2 O2 23.9(4) 111_433 . 1_555 N
Si1 Df2 O3 66.1(10) 111_433 . 4_555 N
Si1 Df2 O4 69.2(12) 111_433 . 310_334 N
Si1 Df2 O4 107.3(12) 111_433 . -302_444 N
Si1 Df2 SJ 141.7(14) 111_545 . -207_566 N
Si1 Df2 SJ 112.1(22) 111_545 . -304_556 N
Si1 Df2 Oc 124.6(17) 111_545 . -3_555 N
Si1 Df2 Oc 55.9(8) 111_545 . -108_656 N
Si1 Df2 Oc 138.7(16) 111_545 . -304_556 N
Si1 Df2 Dc1 133.9(16) 111_554 . -3_555 N
Si1 Df2 Dc1 162.5(10) 111_554 . -207_575 N
Si1 Df2 Dc1 145.2(20) 111_554 . -304_565 N
Si1 Df2 Dc2 110.8(15) 111_555 . -3_555 N
Si1 Df2 Dc2 43.9(7) 111_555 . -108_666 N
Si1 Df2 Dc2 127.4(21) 111_555 . -304_566 N
Si1 Df2 Od 150.4(18) 111_554 . -207_575 N
Si1 Df2 Od 119.7(22) 111_554 . -304_565 N
Si1 Df2 Si2 64.4(8) -108_644 . 208_443 N
Si1 Df2 Si2 53.2(8) -108_644 . -211_554 N
Si1 Df2 Al1 64.4(8) -108_554 . 208_353 N
Si1 Df2 Al1 53.2(8) -108_554 . -211_464 N
Si1 Df2 O1 73.1(11) -108_544 . 111_433 N
Si1 Df2 O1 29.9(8) -108_544 . -108_544 N
Si1 Df2 O2 69.0(9) -108_544 . 1_555 N
Si1 Df2 O3 32.4(5) -108_544 . 4_555 N
Si1 Df2 O4 99.8(11) -108_544 . 310_334 N
Si1 Df2 O4 28.5(4) -108_544 . -302_444 N
Si1 Df2 SJ 61.7(10) -108_656 . -207_566 N
Si1 Df2 SJ 105.1(15) -108_656 . -304_556 N
Si1 Df2 Oc 138.7(16) -108_656 . -3_555 N
Si1 Df2 Oc 105.7(15) -108_656 . -108_656 N
Si1 Df2 Oc 81.8(11) -108_656 . -304_556 N
Si1 Df2 Dc1 131.8(15) -108_665 . -3_555 N
Si1 Df2 Dc1 84.2(12) -108_665 . -207_575 N
Si1 Df2 Dc1 103.7(14) -108_665 . -304_565 N
Si1 Df2 Dc2 136.8(14) -108_666 . -3_555 N
Si1 Df2 Dc2 94.4(14) -108_666 . -108_666 N
Si1 Df2 Dc2 69.9(14) -108_666 . -304_566 N
Si1 Df2 Od 70.4(15) -108_665 . -207_575 N
Si1 Df2 Od 105.7(17) -108_665 . -304_565 N
Si2 Df2 Si2 81.6(12) 208_443 . -211_554 N
Si2 Df2 Al1 0.0 208_353 . 208_353 N
Si2 Df2 Al1 81.6(12) 208_353 . -211_464 N
Si2 Df2 O1 75.1(13) 208_343 . 111_433 N
Si2 Df2 O1 37.0(9) 208_343 . -108_544 N
Si2 Df2 O2 31.4(6) 208_343 . 1_555 N
Si2 Df2 O3 81.5(11) 208_343 . 4_555 N
Si2 Df2 O4 36.9(7) 208_343 . 310_334 N
Si2 Df2 O4 87.4(8) 208_343 . -302_444 N
Si2 Df2 SJ 102.9(12) 208_455 . -207_566 N
Si2 Df2 SJ 66.7(15) 208_455 . -304_556 N
Si2 Df2 Oc 100.5(17) 208_455 . -3_555 N
Si2 Df2 Oc 111.1(17) 208_455 . -108_656 N
Si2 Df2 Oc 83.5(12) 208_455 . -304_556 N
Si2 Df2 Dc1 103.9(16) 208_464 . -3_555 N
Si2 Df2 Dc1 110.9(13) 208_464 . -207_575 N
Si2 Df2 Dc1 94.6(15) 208_464 . -304_565 N
Si2 Df2 Dc2 87.2(14) 208_465 . -3_555 N
Si2 Df2 Dc2 98.8(16) 208_465 . -108_666 N
Si2 Df2 Dc2 72.9(15) 208_465 . -304_566 N
Si2 Df2 Od 109.7(16) 208_464 . -207_575 N
Si2 Df2 Od 73.3(16) 208_464 . -304_565 N
Si2 Df2 Al1 81.6(12) -211_464 . 208_353 N
Si2 Df2 Al1 0.0 -211_464 . -211_464 N
Si2 Df2 O1 25.3(4) -211_454 . 111_433 N
Si2 Df2 O1 70.7(15) -211_454 . -108_544 N
Si2 Df2 O2 58.0(8) -211_454 . 1_555 N
Si2 Df2 O3 23.9(4) -211_454 . 4_555 N
Si2 Df2 O4 111.5(16) -211_454 . 310_334 N
Si2 Df2 O4 70.4(9) -211_454 . -302_444 N
Si2 Df2 SJ 104.1(15) -211_566 . -207_566 N
Si2 Df2 SJ 147.8(19) -211_566 . -304_556 N
Si2 Df2 Oc 167.6(14) -211_566 . -3_555 N
Si2 Df2 Oc 53.0(7) -211_566 . -108_656 N
Si2 Df2 Oc 134.7(14) -211_566 . -304_556 N
Si2 Df2 Dc1 173.7(11) -211_575 . -3_555 N
Si2 Df2 Dc1 125.9(15) -211_575 . -207_575 N
Si2 Df2 Dc1 155.9(16) -211_575 . -304_565 N
Si2 Df2 Dc2 157.5(18) -211_576 . -3_555 N
Si2 Df2 Dc2 41.2(6) -211_576 . -108_666 N
Si2 Df2 Dc2 123.1(19) -211_576 . -304_566 N
Si2 Df2 Od 110.2(19) -211_575 . -207_575 N
Si2 Df2 Od 153.1(18) -211_575 . -304_565 N
Al1 Df2 Al1 81.6(12) 208_353 . -211_464 N
Al1 Df2 O1 75.1(13) 208_343 . 111_433 N
Al1 Df2 O1 37.0(9) 208_343 . -108_544 N
Al1 Df2 O2 31.4(6) 208_343 . 1_555 N
Al1 Df2 O3 81.5(11) 208_343 . 4_555 N
Al1 Df2 O4 36.9(7) 208_343 . 310_334 N
Al1 Df2 O4 87.4(8) 208_343 . -302_444 N
Al1 Df2 SJ 102.9(12) 208_455 . -207_566 N
Al1 Df2 SJ 66.7(15) 208_455 . -304_556 N
Al1 Df2 Oc 100.5(17) 208_455 . -3_555 N
Al1 Df2 Oc 111.1(17) 208_455 . -108_656 N
Al1 Df2 Oc 83.5(12) 208_455 . -304_556 N
Al1 Df2 Dc1 103.9(16) 208_464 . -3_555 N
Al1 Df2 Dc1 110.9(13) 208_464 . -207_575 N
Al1 Df2 Dc1 94.6(15) 208_464 . -304_565 N
Al1 Df2 Dc2 87.2(14) 208_465 . -3_555 N
Al1 Df2 Dc2 98.8(16) 208_465 . -108_666 N
Al1 Df2 Dc2 72.9(15) 208_465 . -304_566 N
Al1 Df2 Od 109.7(16) 208_464 . -207_575 N
Al1 Df2 Od 73.3(16) 208_464 . -304_565 N
Al1 Df2 O1 25.3(4) -211_454 . 111_433 N
Al1 Df2 O1 70.7(15) -211_454 . -108_544 N
Al1 Df2 O2 58.0(8) -211_454 . 1_555 N
Al1 Df2 O3 23.9(4) -211_454 . 4_555 N
Al1 Df2 O4 111.5(16) -211_454 . 310_334 N
Al1 Df2 O4 70.4(9) -211_454 . -302_444 N
Al1 Df2 SJ 104.1(15) -211_566 . -207_566 N
Al1 Df2 SJ 147.8(19) -211_566 . -304_556 N
Al1 Df2 Oc 167.6(14) -211_566 . -3_555 N
Al1 Df2 Oc 53.0(7) -211_566 . -108_656 N
Al1 Df2 Oc 134.7(14) -211_566 . -304_556 N
Al1 Df2 Dc1 173.7(11) -211_575 . -3_555 N
Al1 Df2 Dc1 125.9(15) -211_575 . -207_575 N
Al1 Df2 Dc1 155.9(16) -211_575 . -304_565 N
Al1 Df2 Dc2 157.5(18) -211_576 . -3_555 N
Al1 Df2 Dc2 41.2(6) -211_576 . -108_666 N
Al1 Df2 Dc2 123.1(19) -211_576 . -304_566 N
Al1 Df2 Od 110.2(19) -211_575 . -207_575 N
Al1 Df2 Od 153.1(18) -211_575 . -304_565 N
O1 Df2 O1 80.4(17) 111_433 . -108_544 N
O1 Df2 O2 44.7(7) 111_433 . 1_555 N
O1 Df2 O3 48.4(8) 111_433 . 4_555 N
O1 Df2 O4 94.6(15) 111_433 . 310_334 N
O1 Df2 O4 94.7(12) 111_433 . -302_444 N
O1 Df2 SJ 129.2(17) 111_545 . -207_566 N
O1 Df2 SJ 137.3(24) 111_545 . -304_556 N
O1 Df2 Oc 143.3(16) 111_545 . -3_555 N
O1 Df2 Oc 40.9(6) 111_545 . -108_656 N
O1 Df2 Oc 152.2(14) 111_545 . -304_556 N
O1 Df2 Dc1 152.8(14) 111_554 . -3_555 N
O1 Df2 Dc1 151.2(17) 111_554 . -207_575 N
O1 Df2 Dc1 169.6(18) 111_554 . -304_565 N
O1 Df2 Dc2 132.5(17) 111_555 . -3_555 N
O1 Df2 Dc2 26.8(4) 111_555 . -108_666 N
O1 Df2 Dc2 138.7(20) 111_555 . -304_566 N
O1 Df2 Od 135.5(21) 111_554 . -207_575 N
O1 Df2 Od 144.9(24) 111_554 . -304_565 N
O1 Df2 O2 53.9(14) -108_544 . 1_555 N
O1 Df2 O3 57.3(12) -108_544 . 4_555 N
O1 Df2 O4 70.3(15) -108_544 . 310_334 N
O1 Df2 O4 50.5(11) -108_544 . -302_444 N
O1 Df2 SJ 72.0(15) -108_656 . -207_566 N
O1 Df2 SJ 80.3(17) -108_656 . -304_556 N
O1 Df2 Oc 118.2(21) -108_656 . -3_555 N
O1 Df2 Oc 120.8(22) -108_656 . -108_656 N
O1 Df2 Oc 71.8(13) -108_656 . -304_556 N
O1 Df2 Dc1 115.5(20) -108_665 . -3_555 N
O1 Df2 Dc1 88.6(17) -108_665 . -207_575 N
O1 Df2 Dc1 92.0(17) -108_665 . -304_565 N
O1 Df2 Dc2 110.6(20) -108_666 . -3_555 N
O1 Df2 Dc2 106.9(20) -108_666 . -108_666 N
O1 Df2 Dc2 58.3(12) -108_666 . -304_566 N
O1 Df2 Od 80.4(18) -108_665 . -207_575 N
O1 Df2 Od 83.4(19) -108_665 . -304_565 N
O2 Df2 O3 68.5(10) 1_555 . 4_555 N
O2 Df2 O4 53.5(9) 1_555 . 310_334 N
O2 Df2 O4 97.4(10) 1_555 . -302_444 N
O2 Df2 SJ 125.8(11) 1_555 . -207_566 N
O2 Df2 SJ 93.8(19) 1_555 . -304_556 N
O2 Df2 Oc 118.8(17) 1_555 . -3_555 N
O2 Df2 Oc 79.8(11) 1_555 . -108_656 N
O2 Df2 Oc 114.9(14) 1_555 . -304_556 N
O2 Df2 Dc1 125.9(16) 1_555 . -3_555 N
O2 Df2 Dc1 140.5(11) 1_555 . -207_575 N
O2 Df2 Dc1 124.9(17) 1_555 . -304_565 N
O2 Df2 Dc2 103.7(15) 1_555 . -3_555 N
O2 Df2 Dc2 67.4(10) 1_555 . -108_666 N
O2 Df2 Dc2 103.5(19) 1_555 . -304_566 N
O2 Df2 Od 134.3(15) 1_555 . -207_575 N
O2 Df2 Od 101.1(19) 1_555 . -304_565 N
O3 Df2 O4 117.7(15) 4_555 . 310_334 N
O3 Df2 O4 46.6(6) 4_555 . -302_444 N
O3 Df2 SJ 80.8(13) 4_555 . -207_566 N
O3 Df2 SJ 136.9(15) 4_555 . -304_556 N
O3 Df2 Oc 168.2(19) 4_555 . -3_555 N
O3 Df2 Oc 73.8(11) 4_555 . -108_656 N
O3 Df2 Oc 111.5(14) 4_555 . -304_556 N
O3 Df2 Dc1 158.6(17) 4_555 . -3_555 N
O3 Df2 Dc1 103.5(14) 4_555 . -207_575 N
O3 Df2 Dc1 132.1(17) 4_555 . -304_565 N
O3 Df2 Dc2 167.8(13) 4_555 . -3_555 N
O3 Df2 Dc2 63.8(10) 4_555 . -108_666 N
O3 Df2 Dc2 101.1(18) 4_555 . -304_566 N
O3 Df2 Od 87.7(17) 4_555 . -207_575 N
O3 Df2 Od 138.1(17) 4_555 . -304_565 N
O4 Df2 O4 117.1(10) 310_334 . -302_444 N
O4 Df2 SJ 114.0(15) 310_446 . -207_566 N
O4 Df2 SJ 43.0(13) 310_446 . -304_556 N
O4 Df2 Oc 66.6(12) 310_446 . -3_555 N
O4 Df2 Oc 112.4(16) 310_446 . -108_656 N
O4 Df2 Oc 77.9(14) 310_446 . -304_556 N
O4 Df2 Dc1 72.6(12) 310_455 . -3_555 N
O4 Df2 Dc1 106.7(16) 310_455 . -207_575 N
O4 Df2 Dc1 76.1(15) 310_455 . -304_565 N
O4 Df2 Dc2 52.0(9) 310_456 . -3_555 N
O4 Df2 Dc2 107.2(16) 310_456 . -108_666 N
O4 Df2 Dc2 74.6(19) 310_456 . -304_566 N
O4 Df2 Od 115.8(20) 310_455 . -207_575 N
O4 Df2 Od 50.5(15) 310_455 . -304_565 N
O4 Df2 SJ 35.4(8) -302_556 . -207_566 N
O4 Df2 SJ 101.7(17) -302_556 . -304_556 N
O4 Df2 Oc 121.7(17) -302_556 . -3_555 N
O4 Df2 Oc 114.5(15) -302_556 . -108_656 N
O4 Df2 Oc 66.4(11) -302_556 . -304_556 N
O4 Df2 Dc1 112.4(15) -302_565 . -3_555 N
O4 Df2 Dc1 58.5(9) -302_565 . -207_575 N
O4 Df2 Dc1 85.7(14) -302_565 . -304_565 N
O4 Df2 Dc2 128.7(16) -302_566 . -3_555 N
O4 Df2 Dc2 108.3(14) -302_566 . -108_666 N
O4 Df2 Dc2 58.7(15) -302_566 . -304_566 N
O4 Df2 Od 43.4(13) -302_565 . -207_575 N
O4 Df2 Od 98.6(19) -302_565 . -304_565 N
SJ Df2 SJ 79.0(19) -207_566 . -304_556 N
SJ Df2 Oc 87.4(16) -207_566 . -3_555 N
SJ Df2 Oc 133.3(18) -207_566 . -108_656 N
SJ Df2 Oc 39.4(10) -207_566 . -304_556 N
SJ Df2 Dc1 77.8(14) -207_575 . -3_555 N
SJ Df2 Dc1 23.2(8) -207_575 . -207_575 N
SJ Df2 Dc1 53.4(12) -207_575 . -304_565 N
SJ Df2 Dc2 97.4(16) -207_576 . -3_555 N
SJ Df2 Dc2 134.8(18) -207_576 . -108_666 N
SJ Df2 Dc2 39.5(16) -207_576 . -304_566 N
SJ Df2 Od 8.9(13) -207_575 . -207_575 N
SJ Df2 Od 73.2(20) -207_575 . -304_565 N
SJ Df2 Oc 38.1(12) -304_556 . -3_555 N
SJ Df2 Oc 143.7(21) -304_556 . -108_656 N
SJ Df2 Oc 39.6(13) -304_556 . -304_556 N
SJ Df2 Dc1 38.2(12) -304_565 . -3_555 N
SJ Df2 Dc1 65.1(16) -304_565 . -207_575 N
SJ Df2 Dc1 33.2(13) -304_565 . -304_565 N
SJ Df2 Dc2 31.8(12) -304_566 . -3_555 N
SJ Df2 Dc2 146.2(24) -304_566 . -108_666 N
SJ Df2 Dc2 43.3(17) -304_566 . -304_566 N
SJ Df2 Od 77.3(21) -304_565 . -207_575 N
SJ Df2 Od 7.6(14) -304_565 . -304_565 N
Oc Df2 Oc 115.6(10) -3_555 . -108_656 N
Oc Df2 Oc 57.6(13) -3_555 . -304_556 N
Oc Df2 Dc1 9.7(4) -3_555 . -3_555 N
Oc Df2 Dc1 64.9(11) -3_555 . -207_575 N
Oc Df2 Dc1 36.5(9) -3_555 . -304_565 N
Oc Df2 Dc2 15.09(33) -3_555 . -3_555 N
Oc Df2 Dc2 126.7(11) -3_555 . -108_666 N
Oc Df2 Dc2 68.8(20) -3_555 . -304_566 N
Oc Df2 Od 80.8(18) -3_555 . -207_575 N
Oc Df2 Od 34.9(14) -3_555 . -304_565 N
Oc Df2 Oc 165.3(18) -108_656 . -304_556 N
Oc Df2 Dc1 121.4(9) -108_665 . -3_555 N
Oc Df2 Dc1 136.9(15) -108_665 . -207_575 N
Oc Df2 Dc1 147.2(13) -108_665 . -304_565 N
Oc Df2 Dc2 114.9(11) -108_666 . -3_555 N
Oc Df2 Dc2 14.06(18) -108_666 . -108_666 N
Oc Df2 Dc2 172.6(28) -108_666 . -304_566 N
Oc Df2 Od 131.6(21) -108_665 . -207_575 N
Oc Df2 Od 146.5(21) -108_665 . -304_565 N
Oc Df2 Dc1 50.0(11) -304_565 . -3_555 N
Oc Df2 Dc1 29.7(8) -304_565 . -207_575 N
Oc Df2 Dc1 21.9(5) -304_565 . -304_565 N
Oc Df2 Dc2 62.3(13) -304_566 . -3_555 N
Oc Df2 Dc2 174.2(21) -304_566 . -108_666 N
Oc Df2 Dc2 13.5(9) -304_566 . -304_566 N
Oc Df2 Od 38.4(13) -304_565 . -207_575 N
Oc Df2 Od 34.1(15) -304_565 . -304_565 N
Dc1 Df2 Dc1 55.2(10) -3_555 . -207_575 N
Dc1 Df2 Dc1 28.2(8) -3_555 . -304_565 N
Dc1 Df2 Dc2 23.4(4) -3_555 . -3_555 N
Dc1 Df2 Dc2 133.7(10) -3_555 . -108_666 N
Dc1 Df2 Dc2 62.1(18) -3_555 . -304_566 N
Dc1 Df2 Od 71.0(16) -3_555 . -207_575 N
Dc1 Df2 Od 33.1(14) -3_555 . -304_565 N
Dc1 Df2 Dc1 34.0(9) -207_575 . -304_565 N
Dc1 Df2 Dc2 76.3(12) -207_576 . -3_555 N
Dc1 Df2 Dc2 145.8(16) -207_576 . -108_666 N
Dc1 Df2 Dc2 38.2(15) -207_576 . -304_566 N
Dc1 Df2 Od 15.8(11) -207_575 . -207_575 N
Dc1 Df2 Od 58.0(17) -207_575 . -304_565 N
Dc1 Df2 Dc2 44.1(10) -304_566 . -3_555 N
Dc1 Df2 Dc2 160.9(13) -304_566 . -108_666 N
Dc1 Df2 Dc2 34.8(13) -304_566 . -304_566 N
Dc1 Df2 Od 48.6(15) -304_565 . -207_575 N
Dc1 Df2 Od 25.6(14) -304_565 . -304_565 N
Dc2 Df2 Dc2 122.9(12) -3_555 . -108_666 N
Dc2 Df2 Dc2 71.0(20) -3_555 . -304_566 N
Dc2 Df2 Od 91.9(19) -3_555 . -207_575 N
Dc2 Df2 Od 31.9(15) -3_555 . -304_565 N
Dc2 Df2 Dc2 164.2(23) -108_666 . -304_566 N
Dc2 Df2 Od 136.1(22) -108_665 . -207_575 N
Dc2 Df2 Od 151.7(23) -108_665 . -304_565 N
Dc2 Df2 Od 41.8(17) -304_565 . -207_575 N
Dc2 Df2 Od 39.9(19) -304_565 . -304_565 N
Od Df2 Od 70.8(23) -207_575 . -304_565 N
Si1 Oe Si2 54.4(4) -12_654 . -211_554 N
Si1 Oe Al1 54.4(4) -12_564 . -211_464 N
Si1 Oe O1 28.03(28) -12_554 . -12_554 N
Si1 Oe O1 80.9(6) -12_554 . 111_433 N
Si1 Oe O4 25.93(33) -12_554 . -303_444 N
Si1 Oe SJ 134.6(11) -12_666 . 1_555 N
Si1 Oe SJ 56.7(30) -12_666 . -108_656 N
Si1 Oe SJ 83.0(11) -12_666 . -305_556 N
Si1 Oe Oc 158.4(11) -12_666 . 1_555 N
Si1 Oe Oc 127.4(15) -12_666 . -108_656 N
Si1 Oe Oc 111.4(10) -12_666 . -201_555 N
Si1 Oe Oc 87.3(17) -12_666 . -305_556 N
Si1 Oe Dc1 158.8(13) -12_675 . 1_555 N
Si1 Oe Dc1 157.4(27) -12_675 . -108_665 N
Si1 Oe Dc1 126.7(11) -12_675 . -201_564 N
Si1 Oe Dc1 110.8(15) -12_675 . -305_565 N
Si1 Oe Dc2 103.7(12) -12_676 . -108_666 N
Si1 Oe Dc2 55.6(10) -12_676 . -305_566 N
Si1 Oe Od 138.2(15) -12_675 . 1_555 N
Si1 Oe Od 73(6) -12_675 . -108_665 N
Si1 Oe Od 92.6(16) -12_675 . -305_565 N
Si1 Oe Dd1 142.8(18) -12_654 . 1_555 N
Si1 Oe Dd1 105(4) -12_654 . -108_644 N
Si1 Oe Dd1 102.5(22) -12_654 . -305_544 N
Si2 Oe Al1 0.0 -211_464 . -211_464 N
Si2 Oe O1 82.2(6) -211_454 . -12_554 N
Si2 Oe O1 27.77(28) -211_454 . 111_433 N
Si2 Oe O4 28.7(4) -211_454 . -303_444 N
Si2 Oe SJ 80.9(9) -211_566 . 1_555 N
Si2 Oe SJ 5.7(27) -211_566 . -108_656 N
Si2 Oe SJ 137.0(12) -211_566 . -305_556 N
Si2 Oe Oc 105.0(9) -211_566 . 1_555 N
Si2 Oe Oc 74.1(12) -211_566 . -108_656 N
Si2 Oe Oc 161.9(10) -211_566 . -201_555 N
Si2 Oe Oc 133.6(20) -211_566 . -305_556 N
Si2 Oe Dc1 104.6(11) -211_575 . 1_555 N
Si2 Oe Dc1 103.1(24) -211_575 . -108_665 N
Si2 Oe Dc1 173.4(10) -211_575 . -201_564 N
Si2 Oe Dc1 164.8(17) -211_575 . -305_565 N
Si2 Oe Dc2 50.0(9) -211_576 . -108_666 N
Si2 Oe Dc2 109.8(14) -211_576 . -305_566 N
Si2 Oe Od 85.7(14) -211_575 . 1_555 N
Si2 Oe Od 42(6) -211_575 . -108_665 N
Si2 Oe Od 145.3(17) -211_575 . -305_565 N
Si2 Oe Dd1 97.3(15) -211_554 . 1_555 N
Si2 Oe Dd1 85(4) -211_554 . -108_644 N
Si2 Oe Dd1 143.8(23) -211_554 . -305_544 N
Al1 Oe O1 82.2(6) -211_454 . -12_554 N
Al1 Oe O1 27.77(28) -211_454 . 111_433 N
Al1 Oe O4 28.7(4) -211_454 . -303_444 N
Al1 Oe SJ 80.9(9) -211_566 . 1_555 N
Al1 Oe SJ 5.7(27) -211_566 . -108_656 N
Al1 Oe SJ 137.0(12) -211_566 . -305_556 N
Al1 Oe Oc 105.0(9) -211_566 . 1_555 N
Al1 Oe Oc 74.1(12) -211_566 . -108_656 N
Al1 Oe Oc 161.9(10) -211_566 . -201_555 N
Al1 Oe Oc 133.6(20) -211_566 . -305_556 N
Al1 Oe Dc1 104.6(11) -211_575 . 1_555 N
Al1 Oe Dc1 103.1(24) -211_575 . -108_665 N
Al1 Oe Dc1 173.4(10) -211_575 . -201_564 N
Al1 Oe Dc1 164.8(17) -211_575 . -305_565 N
Al1 Oe Dc2 50.0(9) -211_576 . -108_666 N
Al1 Oe Dc2 109.8(14) -211_576 . -305_566 N
Al1 Oe Od 85.7(14) -211_575 . 1_555 N
Al1 Oe Od 42(6) -211_575 . -108_665 N
Al1 Oe Od 145.3(17) -211_575 . -305_565 N
Al1 Oe Dd1 97.3(15) -211_554 . 1_555 N
Al1 Oe Dd1 85(4) -211_554 . -108_644 N
Al1 Oe Dd1 143.8(23) -211_554 . -305_544 N
O1 Oe O1 107.6(8) -12_554 . 111_433 N
O1 Oe O4 54.0(6) -12_554 . -303_444 N
O1 Oe SJ 159.1(12) -12_666 . 1_555 N
O1 Oe SJ 84.8(32) -12_666 . -108_656 N
O1 Oe SJ 55.0(9) -12_666 . -305_556 N
O1 Oe Oc 167.0(10) -12_666 . 1_555 N
O1 Oe Oc 155.1(16) -12_666 . -108_656 N
O1 Oe Oc 85.1(9) -12_666 . -201_555 N
O1 Oe Oc 61.1(15) -12_666 . -305_556 N
O1 Oe Dc1 170.3(12) -12_675 . 1_555 N
O1 Oe Dc1 174.4(26) -12_675 . -108_665 N
O1 Oe Dc1 99.5(10) -12_675 . -201_564 N
O1 Oe Dc1 82.9(14) -12_675 . -305_565 N
O1 Oe Dc2 130.2(14) -12_676 . -108_666 N
O1 Oe Dc2 27.6(9) -12_676 . -305_566 N
O1 Oe Od 158.9(15) -12_675 . 1_555 N
O1 Oe Od 96(6) -12_675 . -108_665 N
O1 Oe Od 64.6(15) -12_675 . -305_565 N
O1 Oe Dd1 149.9(17) -12_654 . 1_555 N
O1 Oe Dd1 115(4) -12_654 . -108_644 N
O1 Oe Dd1 76.6(20) -12_654 . -305_544 N
O1 Oe O4 56.0(6) 111_433 . -303_444 N
O1 Oe SJ 53.8(8) 111_545 . 1_555 N
O1 Oe SJ 28.0(30) 111_545 . -108_656 N
O1 Oe SJ 157.7(13) 111_545 . -305_556 N
O1 Oe Oc 77.9(8) 111_545 . 1_555 N
O1 Oe Oc 51.3(11) 111_545 . -108_656 N
O1 Oe Oc 167.2(11) 111_545 . -201_555 N
O1 Oe Oc 141.1(21) 111_545 . -305_556 N
O1 Oe Dc1 77.9(10) 111_554 . 1_555 N
O1 Oe Dc1 77.2(22) 111_554 . -108_665 N
O1 Oe Dc1 152.4(11) 111_554 . -201_564 N
O1 Oe Dc1 162.6(16) 111_554 . -305_565 N
O1 Oe Dc2 22.8(7) 111_555 . -108_666 N
O1 Oe Dc2 134.3(16) 111_555 . -305_566 N
O1 Oe Od 58.1(12) 111_554 . 1_555 N
O1 Oe Od 51(6) 111_554 . -108_665 N
O1 Oe Od 158.4(17) 111_554 . -305_565 N
O1 Oe Dd1 69.8(14) 111_533 . 1_555 N
O1 Oe Dd1 85(4) 111_533 . -108_644 N
O1 Oe Dd1 140.6(19) 111_533 . -305_544 N
O4 Oe SJ 109.6(12) -303_556 . 1_555 N
O4 Oe SJ 30.8(28) -303_556 . -108_656 N
O4 Oe SJ 108.9(13) -303_556 . -305_556 N
O4 Oe Oc 133.7(13) -303_556 . 1_555 N
O4 Oe Oc 101.6(15) -303_556 . -108_656 N
O4 Oe Oc 135.5(12) -303_556 . -201_555 N
O4 Oe Oc 111.3(19) -303_556 . -305_556 N
O4 Oe Dc1 133.2(14) -303_565 . 1_555 N
O4 Oe Dc1 131.4(28) -303_565 . -108_665 N
O4 Oe Dc1 151.3(13) -303_565 . -201_564 N
O4 Oe Dc1 136.7(18) -303_565 . -305_565 N
O4 Oe Dc2 78.6(12) -303_566 . -108_666 N
O4 Oe Dc2 81.5(13) -303_566 . -305_566 N
O4 Oe Od 114.1(16) -303_565 . 1_555 N
O4 Oe Od 53(6) -303_565 . -108_665 N
O4 Oe Od 118.4(18) -303_565 . -305_565 N
O4 Oe Dd1 123.9(18) -303_544 . 1_555 N
O4 Oe Dd1 93(4) -303_544 . -108_644 N
O4 Oe Dd1 125.7(24) -303_544 . -305_544 N
SJ Oe SJ 79.5(31) 1_555 . -108_656 N
SJ Oe SJ 139.3(13) 1_555 . -305_556 N
SJ Oe Oc 24.1(6) 1_555 . 1_555 N
SJ Oe Oc 20.5(8) 1_555 . -108_656 N
SJ Oe Oc 114.0(10) 1_555 . -201_555 N
SJ Oe Oc 125.5(18) 1_555 . -305_556 N
SJ Oe Dc1 24.2(8) 1_555 . 1_555 N
SJ Oe Dc1 24.4(19) 1_555 . -108_665 N
SJ Oe Dc1 98.7(9) 1_555 . -201_564 N
SJ Oe Dc1 113.0(14) 1_555 . -305_565 N
SJ Oe Dc2 31.0(9) 1_555 . -108_666 N
SJ Oe Dc2 163.5(17) 1_555 . -305_566 N
SJ Oe Od 6.9(12) 1_555 . 1_555 N
SJ Oe Od 79(6) 1_555 . -108_665 N
SJ Oe Od 128.5(16) 1_555 . -305_565 N
SJ Oe Dd1 24.5(12) 1_555 . 1_555 N
SJ Oe Dd1 76(4) 1_555 . -108_644 N
SJ Oe Dd1 111.2(17) 1_555 . -305_544 N
SJ Oe SJ 140(4) -108_656 . -305_556 N
SJ Oe Oc 103.4(35) -108_656 . 1_555 N
SJ Oe Oc 71.0(34) -108_656 . -108_656 N
SJ Oe Oc 159.4(34) -108_656 . -201_555 N
SJ Oe Oc 139(4) -108_656 . -305_556 N
SJ Oe Dc1 103(4) -108_665 . 1_555 N
SJ Oe Dc1 101(4) -108_665 . -108_665 N
SJ Oe Dc1 167.7(33) -108_665 . -201_564 N
SJ Oe Dc1 167(4) -108_665 . -305_565 N
SJ Oe Dc2 49.0(31) -108_666 . -108_666 N
SJ Oe Dc2 112(4) -108_666 . -305_566 N
SJ Oe Od 85(4) -108_665 . 1_555 N
SJ Oe Od 36(6) -108_665 . -108_665 N
SJ Oe Od 149(4) -108_665 . -305_565 N
SJ Oe Dd1 98(4) -108_644 . 1_555 N
SJ Oe Dd1 79(5) -108_644 . -108_644 N
SJ Oe Dd1 149(4) -108_644 . -305_544 N
SJ Oe Oc 116.3(11) -305_556 . 1_555 N
SJ Oe Oc 148.9(17) -305_556 . -108_656 N
SJ Oe Oc 34.1(8) -305_556 . -201_555 N
SJ Oe Oc 22.1(15) -305_556 . -305_556 N
SJ Oe Dc1 117.4(12) -305_565 . 1_555 N
SJ Oe Dc1 119.6(25) -305_565 . -108_665 N
SJ Oe Dc1 45.7(8) -305_565 . -201_564 N
SJ Oe Dc1 27.9(11) -305_565 . -305_565 N
SJ Oe Dc2 164.0(16) -305_566 . -108_666 N
SJ Oe Dc2 27.4(11) -305_566 . -305_566 N
SJ Oe Od 133.1(16) -305_565 . 1_555 N
SJ Oe Od 137(6) -305_565 . -108_665 N
SJ Oe Od 10.9(14) -305_565 . -305_565 N
SJ Oe Dd1 117.1(15) -305_544 . 1_555 N
SJ Oe Dd1 115(4) -305_544 . -108_644 N
SJ Oe Dd1 31.2(15) -305_544 . -305_544 N
Oc Oe Oc 35.9(8) 1_555 . -108_656 N
Oc Oe Oc 90.1(7) 1_555 . -201_555 N
Oc Oe Oc 107.1(17) 1_555 . -305_556 N
Oc Oe Dc1 3.8(4) 1_555 . 1_555 N
Oc Oe Dc1 9.0(18) 1_555 . -108_665 N
Oc Oe Dc1 74.6(6) 1_555 . -201_564 N
Oc Oe Dc1 89.2(12) 1_555 . -305_565 N
Oc Oe Dc2 55.1(8) 1_555 . -108_666 N
Oc Oe Dc2 143.3(16) 1_555 . -305_566 N
Oc Oe Od 20.3(11) 1_555 . 1_555 N
Oc Oe Od 96(6) 1_555 . -108_665 N
Oc Oe Od 105.9(15) 1_555 . -305_565 N
Oc Oe Dd1 20.5(14) 1_555 . 1_555 N
Oc Oe Dd1 77(4) 1_555 . -108_644 N
Oc Oe Dd1 91.8(18) 1_555 . -305_544 N
Oc Oe Oc 116.1(14) -108_656 . -201_555 N
Oc Oe Oc 143.0(23) -108_656 . -305_556 N
Oc Oe Dc1 33.7(9) -108_665 . 1_555 N
Oc Oe Dc1 30.4(14) -108_665 . -108_665 N
Oc Oe Dc1 103.2(13) -108_665 . -201_564 N
Oc Oe Dc1 121.1(18) -108_665 . -305_565 N
Oc Oe Dc2 31.0(7) -108_666 . -108_666 N
Oc Oe Dc2 172.5(23) -108_666 . -305_566 N
Oc Oe Od 27.0(11) -108_665 . 1_555 N
Oc Oe Od 61(6) -108_665 . -108_665 N
Oc Oe Od 140.0(20) -108_665 . -305_565 N
Oc Oe Dd1 44.2(13) -108_644 . 1_555 N
Oc Oe Dd1 56(4) -108_644 . -108_644 N
Oc Oe Dd1 127.7(22) -108_644 . -305_544 N
Oc Oe Oc 46.7(15) -201_555 . -305_556 N
Oc Oe Dc1 89.8(8) -201_564 . 1_555 N
Oc Oe Dc1 90.3(22) -201_564 . -108_665 N
Oc Oe Dc1 15.81(17) -201_564 . -201_564 N
Oc Oe Dc1 15.8(10) -201_564 . -305_565 N
Oc Oe Dc2 144.7(14) -201_565 . -108_666 N
Oc Oe Dc2 58.4(12) -201_565 . -305_566 N
Oc Oe Od 110.1(14) -201_564 . 1_555 N
Oc Oe Od 128(6) -201_564 . -108_665 N
Oc Oe Od 30.2(12) -201_564 . -305_565 N
Oc Oe Dd1 100.1(15) -201_543 . 1_555 N
Oc Oe Dd1 89(4) -201_543 . -108_644 N
Oc Oe Dd1 42.6(18) -201_543 . -305_544 N
Oc Oe Dc1 109.5(17) -305_565 . 1_555 N
Oc Oe Dc1 113.4(28) -305_565 . -108_665 N
Oc Oe Dc1 51.7(14) -305_565 . -201_564 N
Oc Oe Dc1 33.2(11) -305_565 . -305_565 N
Oc Oe Dc2 142.3(22) -305_566 . -108_666 N
Oc Oe Dc2 38.1(12) -305_566 . -305_566 N
Oc Oe Od 118.6(21) -305_565 . 1_555 N
Oc Oe Od 156(7) -305_565 . -108_665 N
Oc Oe Od 17.3(16) -305_565 . -305_565 N
Oc Oe Dd1 101.2(20) -305_544 . 1_555 N
Oc Oe Dd1 134(5) -305_544 . -108_644 N
Oc Oe Dd1 15.4(19) -305_544 . -305_544 N
Dc1 Oe Dc1 5.2(20) 1_555 . -108_665 N
Dc1 Oe Dc1 74.5(8) 1_555 . -201_564 N
Dc1 Oe Dc1 89.9(14) 1_555 . -305_565 N
Dc1 Oe Dc2 55.1(10) 1_555 . -108_666 N
Dc1 Oe Dc2 144.7(17) 1_555 . -305_566 N
Dc1 Oe Od 21.4(11) 1_555 . 1_555 N
Dc1 Oe Od 93(7) 1_555 . -108_665 N
Dc1 Oe Od 107.3(16) 1_555 . -305_565 N
Dc1 Oe Dd1 24.0(14) 1_555 . 1_555 N
Dc1 Oe Dd1 73(4) 1_555 . -108_644 N
Dc1 Oe Dd1 94.1(19) 1_555 . -305_544 N
Dc1 Oe Dc1 75.5(21) -108_665 . -201_564 N
Dc1 Oe Dc1 91.8(24) -108_665 . -305_565 N
Dc1 Oe Dc2 54.4(20) -108_666 . -108_666 N
Dc1 Oe Dc2 147.0(32) -108_666 . -305_566 N
Dc1 Oe Od 23.1(21) -108_665 . 1_555 N
Dc1 Oe Od 89(7) -108_665 . -108_665 N
Dc1 Oe Od 109.9(26) -108_665 . -305_565 N
Dc1 Oe Dd1 28.6(23) -108_644 . 1_555 N
Dc1 Oe Dd1 68(4) -108_644 . -108_644 N
Dc1 Oe Dd1 98.0(27) -108_644 . -305_544 N
Dc1 Oe Dc1 19.1(9) -201_564 . -305_565 N
Dc1 Oe Dc2 129.6(13) -201_565 . -108_666 N
Dc1 Oe Dc2 72.2(12) -201_565 . -305_566 N
Dc1 Oe Od 94.5(13) -201_564 . 1_555 N
Dc1 Oe Od 132(6) -201_564 . -108_665 N
Dc1 Oe Od 38.6(13) -201_564 . -305_565 N
Dc1 Oe Dd1 84.4(15) -201_543 . 1_555 N
Dc1 Oe Dd1 88(4) -201_543 . -108_644 N
Dc1 Oe Dd1 42.4(20) -201_543 . -305_544 N
Dc1 Oe Dc2 143.3(19) -305_566 . -108_666 N
Dc1 Oe Dc2 55.2(13) -305_566 . -305_566 N
Dc1 Oe Od 107.7(17) -305_565 . 1_555 N
Dc1 Oe Od 144(6) -305_565 . -108_665 N
Dc1 Oe Od 19.6(13) -305_565 . -305_565 N
Dc1 Oe Dd1 94.1(17) -305_544 . 1_555 N
Dc1 Oe Dd1 104(4) -305_544 . -108_644 N
Dc1 Oe Dd1 26.9(19) -305_544 . -305_544 N
Dc2 Oe Dc2 155.8(21) -108_666 . -305_566 N
Dc2 Oe Od 35.8(13) -108_665 . 1_555 N
Dc2 Oe Od 59(6) -108_665 . -108_665 N
Dc2 Oe Od 154.3(19) -108_665 . -305_565 N
Dc2 Oe Dd1 49.6(14) -108_644 . 1_555 N
Dc2 Oe Dd1 78(4) -108_644 . -108_644 N
Dc2 Oe Dd1 133.0(19) -108_644 . -305_544 N
Dc2 Oe Od 156.5(20) -305_565 . 1_555 N
Dc2 Oe Od 118(7) -305_565 . -108_665 N
Dc2 Oe Od 37.4(15) -305_565 . -305_565 N
Dc2 Oe Dd1 139.0(20) -305_544 . 1_555 N
Dc2 Oe Dd1 117(4) -305_544 . -108_644 N
Dc2 Oe Dd1 52.8(19) -305_544 . -305_544 N
Od Oe Od 86(6) 1_555 . -108_665 N
Od Oe Od 122.2(23) 1_555 . -305_565 N
Od Oe Dd1 17.5(5) 1_555 . 1_555 N
Od Oe Dd1 81(4) 1_555 . -108_644 N
Od Oe Dd1 104.4(24) 1_555 . -305_544 N
Od Oe Od 146(6) -108_665 . -305_565 N
Od Oe Dd1 103(6) -108_644 . 1_555 N
Od Oe Dd1 44(6) -108_644 . -108_644 N
Od Oe Dd1 168(6) -108_644 . -305_544 N
Od Oe Dd1 106.3(23) -305_544 . 1_555 N
Od Oe Dd1 117(4) -305_544 . -108_644 N
Od Oe Dd1 21.5(6) -305_544 . -305_544 N
Dd1 Oe Dd1 95(5) 1_555 . -108_644 N
Dd1 Oe Dd1 87.3(25) 1_555 . -305_544 N
Dd1 Oe Dd1 130(6) -108_644 . -305_544 N
Si1 De1 Si2 51.3(8) -12_654 . 112_533 N
Si1 De1 Al1 51.3(8) -12_564 . 112_443 N
Si1 De1 O1 26.3(5) -12_554 . -12_554 N
Si1 De1 O4 78.8(11) -12_554 . 311_433 N
Si1 De1 O4 27.1(5) -12_554 . -303_444 N
Si1 De1 SJ 62.0(19) -12_666 . -108_656 N
Si1 De1 SJ 95.9(23) -12_666 . -305_556 N
Si1 De1 Oc 100.6(13) -12_666 . -108_656 N
Si1 De1 Oc 125.2(20) -12_666 . -201_555 N
Si1 De1 Oc 116(13) -12_666 . -305_556 N
Si1 De1 Dc1 131.1(11) -12_675 . 1_555 N
Si1 De1 Dc1 111.8(19) -12_675 . -108_665 N
Si1 De1 Dc1 143.0(20) -12_675 . -201_564 N
Si1 De1 Dc1 137(4) -12_675 . -305_565 N
Si1 De1 Dc2 87.4(11) -12_676 . -108_666 N
Si1 De1 Dc2 121.7(16) -12_676 . -201_565 N
Si1 De1 Dc2 44.8(24) -12_676 . -305_566 N
Si1 De1 Od 117.5(14) -12_675 . 1_555 N
Si1 De1 Od 71.6(29) -12_675 . -108_665 N
Si1 De1 Od 111.1(30) -12_675 . -305_565 N
Si1 De1 Dd1 127.9(16) -12_654 . 1_555 N
Si1 De1 Dd1 87.3(27) -12_654 . -108_644 N
Si1 De1 Dd1 130.8(22) -12_654 . -201_543 N
Si1 De1 Dd1 129(4) -12_654 . -305_544 N
Si2 De1 Al1 0.0 112_443 . 112_443 N
Si2 De1 O1 25.6(5) 112_433 . -12_554 N
Si2 De1 O4 28.8(4) 112_433 . 311_433 N
Si2 De1 O4 78.4(12) 112_433 . -303_444 N
Si2 De1 SJ 113.0(26) 112_545 . -108_656 N
Si2 De1 SJ 47.8(15) 112_545 . -305_556 N
Si2 De1 Oc 150.7(19) 112_545 . -108_656 N
Si2 De1 Oc 86.5(12) 112_545 . -201_555 N
Si2 De1 Oc 65(13) 112_545 . -305_556 N
Si2 De1 Dc1 176.7(15) 112_554 . 1_555 N
Si2 De1 Dc1 160.2(28) 112_554 . -108_665 N
Si2 De1 Dc1 102.5(12) 112_554 . -201_564 N
Si2 De1 Dc1 97.4(29) 112_554 . -305_565 N
Si2 De1 Dc2 138.1(17) 112_555 . -108_666 N
Si2 De1 Dc2 76.3(9) 112_555 . -201_565 N
Si2 De1 Dc2 26.4(24) 112_555 . -305_566 N
Si2 De1 Od 165.3(17) 112_554 . 1_555 N
Si2 De1 Od 119(4) 112_554 . -108_665 N
Si2 De1 Od 61.2(24) 112_554 . -305_565 N
Si2 De1 Dd1 160.7(21) 112_533 . 1_555 N
Si2 De1 Dd1 123.6(33) 112_533 . -108_644 N
Si2 De1 Dd1 101.5(18) 112_533 . -201_543 N
Si2 De1 Dd1 79.5(31) 112_533 . -305_544 N
Al1 De1 O1 25.6(5) 112_433 . -12_554 N
Al1 De1 O4 28.8(4) 112_433 . 311_433 N
Al1 De1 O4 78.4(12) 112_433 . -303_444 N
Al1 De1 SJ 113.0(26) 112_545 . -108_656 N
Al1 De1 SJ 47.8(15) 112_545 . -305_556 N
Al1 De1 Oc 150.7(19) 112_545 . -108_656 N
Al1 De1 Oc 86.5(12) 112_545 . -201_555 N
Al1 De1 Oc 65(13) 112_545 . -305_556 N
Al1 De1 Dc1 176.7(15) 112_554 . 1_555 N
Al1 De1 Dc1 160.2(28) 112_554 . -108_665 N
Al1 De1 Dc1 102.5(12) 112_554 . -201_564 N
Al1 De1 Dc1 97.4(29) 112_554 . -305_565 N
Al1 De1 Dc2 138.1(17) 112_555 . -108_666 N
Al1 De1 Dc2 76.3(9) 112_555 . -201_565 N
Al1 De1 Dc2 26.4(24) 112_555 . -305_566 N
Al1 De1 Od 165.3(17) 112_554 . 1_555 N
Al1 De1 Od 119(4) 112_554 . -108_665 N
Al1 De1 Od 61.2(24) 112_554 . -305_565 N
Al1 De1 Dd1 160.7(21) 112_533 . 1_555 N
Al1 De1 Dd1 123.6(33) 112_533 . -108_644 N
Al1 De1 Dd1 101.5(18) 112_533 . -201_543 N
Al1 De1 Dd1 79.5(31) 112_533 . -305_544 N
O1 De1 O4 52.5(9) -12_554 . 311_433 N
O1 De1 O4 53.3(9) -12_554 . -303_444 N
O1 De1 SJ 87.5(24) -12_666 . -108_656 N
O1 De1 SJ 69.9(19) -12_666 . -305_556 N
O1 De1 Oc 125.3(18) -12_666 . -108_656 N
O1 De1 Oc 103.7(18) -12_666 . -201_555 N
O1 De1 Oc 91(13) -12_666 . -305_556 N
O1 De1 Dc1 156.3(15) -12_675 . 1_555 N
O1 De1 Dc1 135.8(25) -12_675 . -108_665 N
O1 De1 Dc1 121.6(18) -12_675 . -201_564 N
O1 De1 Dc1 116(4) -12_675 . -305_565 N
O1 De1 Dc2 113.7(16) -12_676 . -108_666 N
O1 De1 Dc2 97.0(15) -12_676 . -201_565 N
O1 De1 Dc2 23.4(23) -12_676 . -305_566 N
O1 De1 Od 143.7(17) -12_675 . 1_555 N
O1 De1 Od 94.2(33) -12_675 . -108_665 N
O1 De1 Od 84.9(28) -12_675 . -305_565 N
O1 De1 Dd1 152.6(20) -12_654 . 1_555 N
O1 De1 Dd1 103.7(32) -12_654 . -108_644 N
O1 De1 Dd1 114.7(23) -12_654 . -201_543 N
O1 De1 Dd1 105.0(34) -12_654 . -305_544 N
O4 De1 O4 105.7(16) 311_433 . -303_444 N
O4 De1 SJ 137.9(31) 311_545 . -108_656 N
O4 De1 SJ 19.3(12) 311_545 . -305_556 N
O4 De1 Oc 161.8(21) 311_545 . -108_656 N
O4 De1 Oc 59.5(8) 311_545 . -201_555 N
O4 De1 Oc 40(13) 311_545 . -305_556 N
O4 De1 Dc1 148.2(14) 311_554 . 1_555 N
O4 De1 Dc1 157.1(26) 311_554 . -108_665 N
O4 De1 Dc1 74.2(9) 311_554 . -201_564 N
O4 De1 Dc1 69.4(24) 311_554 . -305_565 N
O4 De1 Dc2 166.0(20) 311_555 . -108_666 N
O4 De1 Dc2 47.9(6) 311_555 . -201_565 N
O4 De1 Dc2 40.4(19) 311_555 . -305_566 N
O4 De1 Od 163.6(18) 311_554 . 1_555 N
O4 De1 Od 137(4) 311_554 . -108_665 N
O4 De1 Od 32.6(22) 311_554 . -305_565 N
O4 De1 Dd1 150.0(18) 311_533 . 1_555 N
O4 De1 Dd1 127.5(32) 311_533 . -108_644 N
O4 De1 Dd1 75.8(15) 311_533 . -201_543 N
O4 De1 Dd1 56.5(26) 311_533 . -305_544 N
O4 De1 SJ 35.4(15) -303_556 . -108_656 N
O4 De1 SJ 121.7(27) -303_556 . -305_556 N
O4 De1 Oc 74.0(10) -303_556 . -108_656 N
O4 De1 Oc 140.1(22) -303_556 . -201_555 N
O4 De1 Oc 143(13) -303_556 . -305_556 N
O4 De1 Dc1 104.1(11) -303_565 . 1_555 N
O4 De1 Dc1 85.4(16) -303_565 . -108_665 N
O4 De1 Dc1 151.9(20) -303_565 . -201_564 N
O4 De1 Dc1 149(4) -303_565 . -305_565 N
O4 De1 Dc2 60.4(8) -303_566 . -108_666 N
O4 De1 Dc2 143.4(21) -303_566 . -201_565 N
O4 De1 Dc2 68.7(26) -303_566 . -305_566 N
O4 De1 Od 90.7(13) -303_565 . 1_555 N
O4 De1 Od 47.5(26) -303_565 . -108_665 N
O4 De1 Od 137.5(34) -303_565 . -305_565 N
O4 De1 Dd1 102.4(15) -303_544 . 1_555 N
O4 De1 Dd1 68.1(24) -303_544 . -108_644 N
O4 De1 Dd1 135.6(20) -303_544 . -201_543 N
O4 De1 Dd1 153(4) -303_544 . -305_544 N
SJ De1 SJ 147(4) -108_656 . -305_556 N
SJ De1 Oc 38.7(15) -108_656 . -108_656 N
SJ De1 Oc 132.8(28) -108_656 . -201_555 N
SJ De1 Oc 178(17) -108_656 . -305_556 N
SJ De1 Dc1 69.2(20) -108_665 . 1_555 N
SJ De1 Dc1 50.0(17) -108_665 . -108_665 N
SJ De1 Dc1 129.9(25) -108_665 . -201_564 N
SJ De1 Dc1 131(4) -108_665 . -305_565 N
SJ De1 Dc2 28.6(16) -108_666 . -108_666 N
SJ De1 Dc2 146.6(29) -108_666 . -201_565 N
SJ De1 Dc2 98(4) -108_666 . -305_566 N
SJ De1 Od 58.1(22) -108_665 . 1_555 N
SJ De1 Od 17.5(24) -108_665 . -108_665 N
SJ De1 Od 160(5) -108_665 . -305_565 N
SJ De1 Dd1 72.1(24) -108_644 . 1_555 N
SJ De1 Dd1 41.8(26) -108_644 . -108_644 N
SJ De1 Dd1 118.0(25) -108_644 . -201_543 N
SJ De1 Dd1 165(5) -108_644 . -305_544 N
SJ De1 Oc 147.8(26) -305_556 . -108_656 N
SJ De1 Oc 40.4(13) -305_556 . -201_555 N
SJ De1 Oc 31(14) -305_556 . -305_556 N
SJ De1 Dc1 129.1(23) -305_565 . 1_555 N
SJ De1 Dc1 139.3(31) -305_565 . -108_665 N
SJ De1 Dc1 54.9(15) -305_565 . -201_564 N
SJ De1 Dc1 50.1(21) -305_565 . -305_565 N
SJ De1 Dc2 168.2(26) -305_566 . -108_666 N
SJ De1 Dc2 28.6(13) -305_566 . -201_565 N
SJ De1 Dc2 53.1(23) -305_566 . -305_566 N
SJ De1 Od 145.9(27) -305_565 . 1_555 N
SJ De1 Od 138(4) -305_565 . -108_665 N
SJ De1 Od 16.0(22) -305_565 . -305_565 N
SJ De1 Dd1 135.9(27) -305_544 . 1_555 N
SJ De1 Dd1 120(4) -305_544 . -108_644 N
SJ De1 Dd1 57.0(19) -305_544 . -201_543 N
SJ De1 Dd1 47.2(23) -305_544 . -305_544 N
Oc De1 Oc 108.7(17) -108_656 . -201_555 N
Oc De1 Oc 143(13) -108_656 . -305_556 N
Oc De1 Dc1 31.0(8) -108_665 . 1_555 N
Oc De1 Dc1 11.5(8) -108_665 . -108_665 N
Oc De1 Dc1 97.4(16) -108_665 . -201_564 N
Oc De1 Dc1 101.0(30) -108_665 . -305_565 N
Oc De1 Dc2 21.0(4) -108_666 . -108_666 N
Oc De1 Dc2 122.3(17) -108_666 . -201_565 N
Oc De1 Dc2 129(4) -108_666 . -305_566 N
Oc De1 Od 25.6(11) -108_665 . 1_555 N
Oc De1 Od 31.9(24) -108_665 . -108_665 N
Oc De1 Od 141.2(32) -108_665 . -305_565 N
Oc De1 Dd1 40.8(13) -108_644 . 1_555 N
Oc De1 Dd1 34.9(22) -108_644 . -108_644 N
Oc De1 Dd1 91.7(18) -108_644 . -201_543 N
Oc De1 Dd1 130(4) -108_644 . -305_544 N
Oc De1 Oc 47(11) -201_555 . -305_556 N
Oc De1 Dc1 90.2(14) -201_564 . 1_555 N
Oc De1 Dc1 99.1(21) -201_564 . -108_665 N
Oc De1 Dc1 18.07(30) -201_564 . -201_564 N
Oc De1 Dc1 12.2(23) -201_564 . -305_565 N
Oc De1 Dc2 129.6(18) -201_565 . -108_666 N
Oc De1 Dc2 14.59(24) -201_565 . -201_565 N
Oc De1 Dc2 81.4(30) -201_565 . -305_566 N
Oc De1 Od 108.1(18) -201_564 . 1_555 N
Oc De1 Od 115.4(32) -201_564 . -108_665 N
Oc De1 Od 33.9(20) -201_564 . -305_565 N
Oc De1 Dd1 103.6(20) -201_543 . 1_555 N
Oc De1 Dd1 91.3(27) -201_543 . -108_644 N
Oc De1 Dd1 17.0(11) -201_543 . -201_543 N
Oc De1 Dd1 52.7(29) -201_543 . -305_544 N
Oc De1 Dc1 113(13) -305_565 . 1_555 N
Oc De1 Dc1 132(14) -305_565 . -108_665 N
Oc De1 Dc1 51(11) -305_565 . -201_564 N
Oc De1 Dc1 49(10) -305_565 . -305_565 N
Oc De1 Dc2 154(16) -305_566 . -108_666 N
Oc De1 Dc2 33(12) -305_566 . -201_565 N
Oc De1 Dc2 80(14) -305_566 . -305_566 N
Oc De1 Od 124(15) -305_565 . 1_555 N
Oc De1 Od 162(14) -305_565 . -108_665 N
Oc De1 Od 18(13) -305_565 . -305_565 N
Oc De1 Dd1 110(15) -305_544 . 1_555 N
Oc De1 Dd1 138(13) -305_544 . -108_644 N
Oc De1 Dd1 62(11) -305_544 . -201_543 N
Oc De1 Dd1 17(13) -305_544 . -305_544 N
Dc1 De1 Dc1 20.8(14) 1_555 . -108_665 N
Dc1 De1 Dc1 74.2(12) 1_555 . -201_564 N
Dc1 De1 Dc1 79.3(29) 1_555 . -305_565 N
Dc1 De1 Dc2 44.7(9) 1_555 . -108_666 N
Dc1 De1 Dc2 100.5(13) 1_555 . -201_565 N
Dc1 De1 Dc2 152(4) 1_555 . -305_566 N
Dc1 De1 Od 18.0(9) 1_555 . 1_555 N
Dc1 De1 Od 62.3(28) 1_555 . -108_665 N
Dc1 De1 Od 115.9(29) 1_555 . -305_565 N
Dc1 De1 Dd1 21.4(13) 1_555 . 1_555 N
Dc1 De1 Dd1 56.2(25) 1_555 . -108_644 N
Dc1 De1 Dd1 75.2(17) 1_555 . -201_543 N
Dc1 De1 Dd1 99(4) 1_555 . -305_544 N
Dc1 De1 Dc1 86.6(20) -108_665 . -201_564 N
Dc1 De1 Dc1 90.5(33) -108_665 . -305_565 N
Dc1 De1 Dc2 30.7(10) -108_666 . -108_666 N
Dc1 De1 Dc2 112.1(22) -108_666 . -201_565 N
Dc1 De1 Dc2 135(5) -108_666 . -305_566 N
Dc1 De1 Od 21.8(17) -108_665 . 1_555 N
Dc1 De1 Od 41.5(23) -108_665 . -108_665 N
Dc1 De1 Od 130(4) -108_665 . -305_565 N
Dc1 De1 Dd1 35.3(20) -108_644 . 1_555 N
Dc1 De1 Dd1 38.0(24) -108_644 . -108_644 N
Dc1 De1 Dd1 82.3(22) -108_644 . -201_543 N
Dc1 De1 Dd1 119(5) -108_644 . -305_544 N
Dc1 De1 Dc1 5.9(23) -201_564 . -305_565 N
Dc1 De1 Dc2 117.1(17) -201_565 . -108_666 N
Dc1 De1 Dc2 26.3(4) -201_565 . -201_565 N
Dc1 De1 Dc2 99.5(32) -201_565 . -305_566 N
Dc1 De1 Od 91.7(16) -201_564 . 1_555 N
Dc1 De1 Od 113.2(31) -201_564 . -108_665 N
Dc1 De1 Od 43.9(21) -201_564 . -305_565 N
Dc1 De1 Dd1 85.8(19) -201_543 . 1_555 N
Dc1 De1 Dd1 89.4(26) -201_543 . -108_644 N
Dc1 De1 Dd1 16.3(10) -201_543 . -201_543 N
Dc1 De1 Dd1 49.6(33) -201_543 . -305_544 N
Dc1 De1 Dc2 121.2(32) -305_566 . -108_666 N
Dc1 De1 Dc2 21.7(18) -305_566 . -201_565 N
Dc1 De1 Dc2 94(4) -305_566 . -305_566 N
Dc1 De1 Od 97.0(32) -305_565 . 1_555 N
Dc1 De1 Od 114(4) -305_565 . -108_665 N
Dc1 De1 Od 40.3(22) -305_565 . -305_565 N
Dc1 De1 Dd1 92(4) -305_544 . 1_555 N
Dc1 De1 Dd1 90(4) -305_544 . -108_644 N
Dc1 De1 Dd1 14.1(23) -305_544 . -201_543 N
Dc1 De1 Dd1 50.3(34) -305_544 . -305_544 N
Dc2 De1 Dc2 142.9(18) -108_666 . -201_565 N
Dc2 De1 Dc2 126.2(32) -108_666 . -305_566 N
Dc2 De1 Od 30.4(11) -108_665 . 1_555 N
Dc2 De1 Od 33.2(24) -108_665 . -108_665 N
Dc2 De1 Od 160.5(34) -108_665 . -305_565 N
Dc2 De1 Dd1 43.6(13) -108_644 . 1_555 N
Dc2 De1 Dd1 48.7(22) -108_644 . -108_644 N
Dc2 De1 Dd1 112.6(19) -108_644 . -201_543 N
Dc2 De1 Dd1 137(4) -108_644 . -305_544 N
Dc2 De1 Dc2 76.9(25) -201_565 . -305_566 N
Dc2 De1 Od 117.7(17) -201_564 . 1_555 N
Dc2 De1 Od 129.5(33) -201_564 . -108_665 N
Dc2 De1 Od 19.4(19) -201_564 . -305_565 N
Dc2 De1 Dd1 110.1(19) -201_543 . 1_555 N
Dc2 De1 Dd1 105.6(27) -201_543 . -108_644 N
Dc2 De1 Dd1 31.3(11) -201_543 . -201_543 N
Dc2 De1 Dd1 41.3(26) -201_543 . -305_544 N
Dc2 De1 Od 154.3(34) -305_565 . 1_555 N
Dc2 De1 Od 98(5) -305_565 . -108_665 N
Dc2 De1 Od 69.1(31) -305_565 . -305_565 N
Dc2 De1 Dd1 169.5(33) -305_544 . 1_555 N
Dc2 De1 Dd1 98(5) -305_544 . -108_644 N
Dc2 De1 Dd1 91(4) -305_544 . -201_543 N
Dc2 De1 Dd1 96.9(35) -305_544 . -305_544 N
Od De1 Od 56.5(27) 1_555 . -108_665 N
Od De1 Od 131.4(34) 1_555 . -305_565 N
Od De1 Dd1 15.28(30) 1_555 . 1_555 N
Od De1 Dd1 59.1(28) 1_555 . -108_644 N
Od De1 Dd1 93.2(19) 1_555 . -201_543 N
Od De1 Dd1 108(4) 1_555 . -305_544 N
Od De1 Od 146(4) -108_665 . -305_565 N
Od De1 Dd1 71.7(29) -108_644 . 1_555 N
Od De1 Dd1 24.3(22) -108_644 . -108_644 N
Od De1 Dd1 101(4) -108_644 . -201_543 N
Od De1 Dd1 159(6) -108_644 . -305_544 N
Od De1 Dd1 120(4) -305_544 . 1_555 N
Od De1 Dd1 123(4) -305_544 . -108_644 N
Od De1 Dd1 50.7(22) -305_544 . -201_543 N
Od De1 Dd1 32.8(13) -305_544 . -305_544 N
Dd1 De1 Dd1 73.2(32) 1_555 . -108_644 N
Dd1 De1 Dd1 91.4(23) 1_555 . -201_543 N
Dd1 De1 Dd1 93(4) 1_555 . -305_544 N
Dd1 De1 Dd1 76.3(30) -108_644 . -201_543 N
Dd1 De1 Dd1 138(6) -108_644 . -305_544 N
Dd1 De1 Dd1 64(4) -201_543 . -305_544 N
Si1 De2 Si1 107.7(14) -12_555 . 111_434 N
Si1 De2 Si2 58.2(10) -12_654 . -211_554 N
Si1 De2 Al1 58.2(10) -12_564 . -211_464 N
Si1 De2 O1 27.4(4) -12_554 . -12_554 N
Si1 De2 O1 91.2(16) -12_554 . 111_433 N
Si1 De2 O4 23.4(5) -12_554 . -303_444 N
Si1 De2 SJ 153.2(22) -12_666 . 1_555 N
Si1 De2 SJ 54(4) -12_666 . -108_656 N
Si1 De2 SJ 73.6(10) -12_666 . -305_556 N
Si1 De2 Oc 165.9(15) -12_666 . 1_555 N
Si1 De2 Oc 128.3(29) -12_666 . -108_656 N
Si1 De2 Oc 79.3(17) -12_666 . -305_556 N
Si1 De2 Dc1 158.6(17) -12_675 . 1_555 N
Si1 De2 Dc1 127.3(27) -12_675 . -108_665 N
Si1 De2 Dc1 92.9(13) -12_675 . -305_565 N
Si1 De2 Dc2 120.4(35) -12_676 . -108_666 N
Si1 De2 Dc2 55.3(12) -12_676 . -305_566 N
Si1 De2 Od 161.2(26) -12_675 . 1_555 N
Si1 De2 Od 72(4) -12_675 . -108_665 N
Si1 De2 Od 81.9(14) -12_675 . -305_565 N
Si1 De2 Dd1 175.3(22) -12_654 . 1_555 N
Si1 De2 Dd1 89.7(28) -12_654 . -108_644 N
Si1 De2 Dd1 93.6(18) -12_654 . -305_544 N
Si1 De2 Dd2 148.7(22) -12_654 . 1_555 N
Si1 De2 Si2 50.2(7) 111_533 . -211_554 N
Si1 De2 Al1 50.2(7) 111_443 . -211_464 N
Si1 De2 O1 135.0(16) 111_433 . -12_554 N
Si1 De2 O1 17.0(4) 111_433 . 111_433 N
Si1 De2 O4 86.0(14) 111_433 . -303_444 N
Si1 De2 SJ 50.7(8) 111_545 . 1_555 N
Si1 De2 SJ 96(4) 111_545 . -108_656 N
Si1 De2 SJ 177.1(15) 111_545 . -305_556 N
Si1 De2 Oc 74.4(8) 111_545 . 1_555 N
Si1 De2 Oc 66.7(14) 111_545 . -108_656 N
Si1 De2 Oc 173.0(26) 111_545 . -305_556 N
Si1 De2 Dc1 77.8(11) 111_554 . 1_555 N
Si1 De2 Dc1 102.1(24) 111_554 . -108_665 N
Si1 De2 Dc1 155.8(18) 111_554 . -305_565 N
Si1 De2 Dc2 29.8(13) 111_555 . -108_666 N
Si1 De2 Dc2 161.1(25) 111_555 . -305_566 N
Si1 De2 Od 56.9(14) 111_554 . 1_555 N
Si1 De2 Od 109(4) 111_554 . -108_665 N
Si1 De2 Od 170.4(20) 111_554 . -305_565 N
Si1 De2 Dd1 70.4(16) 111_533 . 1_555 N
Si1 De2 Dd1 102.1(31) 111_533 . -108_644 N
Si1 De2 Dd1 155.4(22) 111_533 . -305_544 N
Si1 De2 Dd2 41.1(15) 111_533 . 1_555 N
Si2 De2 Al1 0.0 -211_464 . -211_464 N
Si2 De2 O1 85.6(14) -211_454 . -12_554 N
Si2 De2 O1 33.3(7) -211_454 . 111_433 N
Si2 De2 O4 35.9(8) -211_454 . -303_444 N
Si2 De2 SJ 96.7(15) -211_566 . 1_555 N
Si2 De2 SJ 60(4) -211_566 . -108_656 N
Si2 De2 SJ 130.6(18) -211_566 . -305_556 N
Si2 De2 Oc 120.0(14) -211_566 . 1_555 N
Si2 De2 Oc 92.4(25) -211_566 . -108_656 N
Si2 De2 Oc 136.6(26) -211_566 . -305_556 N
Si2 De2 Dc1 120.3(18) -211_575 . 1_555 N
Si2 De2 Dc1 125(4) -211_575 . -108_665 N
Si2 De2 Dc1 144.4(21) -211_575 . -305_565 N
Si2 De2 Dc2 65.2(24) -211_576 . -108_666 N
Si2 De2 Dc2 111.3(22) -211_576 . -305_566 N
Si2 De2 Od 104.3(20) -211_575 . 1_555 N
Si2 De2 Od 86(4) -211_575 . -108_665 N
Si2 De2 Od 139.1(20) -211_575 . -305_565 N
Si2 De2 Dd1 120.4(19) -211_554 . 1_555 N
Si2 De2 Dd1 92.8(33) -211_554 . -108_644 N
Si2 De2 Dd1 151.7(23) -211_554 . -305_544 N
Si2 De2 Dd2 90.7(19) -211_554 . 1_555 N
Al1 De2 O1 85.6(14) -211_454 . -12_554 N
Al1 De2 O1 33.3(7) -211_454 . 111_433 N
Al1 De2 O4 35.9(8) -211_454 . -303_444 N
Al1 De2 SJ 96.7(15) -211_566 . 1_555 N
Al1 De2 SJ 60(4) -211_566 . -108_656 N
Al1 De2 SJ 130.6(18) -211_566 . -305_556 N
Al1 De2 Oc 120.0(14) -211_566 . 1_555 N
Al1 De2 Oc 92.4(25) -211_566 . -108_656 N
Al1 De2 Oc 136.6(26) -211_566 . -305_556 N
Al1 De2 Dc1 120.3(18) -211_575 . 1_555 N
Al1 De2 Dc1 125(4) -211_575 . -108_665 N
Al1 De2 Dc1 144.4(21) -211_575 . -305_565 N
Al1 De2 Dc2 65.2(24) -211_576 . -108_666 N
Al1 De2 Dc2 111.3(22) -211_576 . -305_566 N
Al1 De2 Od 104.3(20) -211_575 . 1_555 N
Al1 De2 Od 86(4) -211_575 . -108_665 N
Al1 De2 Od 139.1(20) -211_575 . -305_565 N
Al1 De2 Dd1 120.4(19) -211_554 . 1_555 N
Al1 De2 Dd1 92.8(33) -211_554 . -108_644 N
Al1 De2 Dd1 151.7(23) -211_554 . -305_544 N
Al1 De2 Dd2 90.7(19) -211_554 . 1_555 N
O1 De2 O1 118.7(19) -12_554 . 111_433 N
O1 De2 O4 50.1(9) -12_554 . -303_444 N
O1 De2 SJ 167.4(16) -12_666 . 1_555 N
O1 De2 SJ 63(4) -12_666 . -108_656 N
O1 De2 SJ 46.5(8) -12_666 . -305_556 N
O1 De2 Oc 149.1(12) -12_666 . 1_555 N
O1 De2 Oc 132.8(22) -12_666 . -108_656 N
O1 De2 Oc 52.0(13) -12_666 . -305_556 N
O1 De2 Dc1 143.7(13) -12_675 . 1_555 N
O1 De2 Dc1 112.0(21) -12_675 . -108_665 N
O1 De2 Dc1 66.8(10) -12_675 . -305_565 N
O1 De2 Dc2 144(4) -12_676 . -108_666 N
O1 De2 Dc2 29.2(8) -12_676 . -305_566 N
O1 De2 Od 166.3(18) -12_675 . 1_555 N
O1 De2 Od 70(4) -12_675 . -108_665 N
O1 De2 Od 54.6(12) -12_675 . -305_565 N
O1 De2 Dd1 153.9(24) -12_654 . 1_555 N
O1 De2 Dd1 86.1(27) -12_654 . -108_644 N
O1 De2 Dd1 66.4(16) -12_654 . -305_544 N
O1 De2 Dd2 175.8(21) -12_654 . 1_555 N
O1 De2 O4 69.1(15) 111_433 . -303_444 N
O1 De2 SJ 65.3(11) 111_545 . 1_555 N
O1 De2 SJ 82(4) 111_545 . -108_656 N
O1 De2 SJ 163.3(24) 111_545 . -305_556 N
O1 De2 Oc 89.2(13) 111_545 . 1_555 N
O1 De2 Oc 73.3(19) 111_545 . -108_656 N
O1 De2 Oc 169.4(31) 111_545 . -305_556 N
O1 De2 Dc1 91.6(15) 111_554 . 1_555 N
O1 De2 Dc1 110.3(30) 111_554 . -108_665 N
O1 De2 Dc1 162.2(23) 111_554 . -305_565 N
O1 De2 Dc2 37.8(15) 111_555 . -108_666 N
O1 De2 Dc2 144.2(28) 111_555 . -305_566 N
O1 De2 Od 72.3(17) 111_554 . 1_555 N
O1 De2 Od 101(4) 111_554 . -108_665 N
O1 De2 Od 171.7(25) 111_554 . -305_565 N
O1 De2 Dd1 87.1(18) 111_533 . 1_555 N
O1 De2 Dd1 98.2(34) 111_533 . -108_644 N
O1 De2 Dd1 170.6(25) 111_533 . -305_544 N
O1 De2 Dd2 57.6(17) 111_533 . 1_555 N
O4 De2 SJ 129.9(22) -303_556 . 1_555 N
O4 De2 SJ 45(4) -303_556 . -108_656 N
O4 De2 SJ 94.8(14) -303_556 . -305_556 N
O4 De2 Oc 149.4(21) -303_556 . 1_555 N
O4 De2 Oc 111.7(31) -303_556 . -108_656 N
O4 De2 Oc 100.8(21) -303_556 . -305_556 N
O4 De2 Dc1 145.6(24) -303_565 . 1_555 N
O4 De2 Dc1 127(4) -303_565 . -108_665 N
O4 De2 Dc1 111.5(17) -303_565 . -305_565 N
O4 De2 Dc2 97.1(33) -303_566 . -108_666 N
O4 De2 Dc2 75.7(16) -303_566 . -305_566 N
O4 De2 Od 137.9(26) -303_565 . 1_555 N
O4 De2 Od 71(4) -303_565 . -108_665 N
O4 De2 Od 103.4(17) -303_565 . -305_565 N
O4 De2 Dd1 156.0(24) -303_544 . 1_555 N
O4 De2 Dd1 85.4(31) -303_544 . -108_644 N
O4 De2 Dd1 116.6(21) -303_544 . -305_544 N
O4 De2 Dd2 126.4(24) -303_544 . 1_555 N
SJ De2 SJ 108(5) 1_555 . -108_656 N
SJ De2 SJ 127.3(19) 1_555 . -305_556 N
SJ De2 Oc 23.9(8) 1_555 . 1_555 N
SJ De2 Oc 35.0(13) 1_555 . -108_656 N
SJ De2 Oc 122.6(25) 1_555 . -305_556 N
SJ De2 Dc1 27.3(9) 1_555 . 1_555 N
SJ De2 Dc1 56.7(20) 1_555 . -108_665 N
SJ De2 Dc1 105.7(19) 1_555 . -305_565 N
SJ De2 Dc2 32.8(19) 1_555 . -108_666 N
SJ De2 Dc2 141.8(20) 1_555 . -305_566 N
SJ De2 Od 8.0(14) 1_555 . 1_555 N
SJ De2 Od 98(4) 1_555 . -108_665 N
SJ De2 Od 120.1(20) 1_555 . -305_565 N
SJ De2 Dd1 27.8(14) 1_555 . 1_555 N
SJ De2 Dd1 81.5(28) 1_555 . -108_644 N
SJ De2 Dd1 111.5(24) 1_555 . -305_544 N
SJ De2 Dd2 15.6(15) 1_555 . 1_555 N
SJ De2 SJ 83.2(34) -108_656 . -305_556 N
SJ De2 Oc 112(4) -108_656 . 1_555 N
SJ De2 Oc 75(4) -108_656 . -108_656 N
SJ De2 Oc 88(4) -108_656 . -305_556 N
SJ De2 Dc1 106(4) -108_665 . 1_555 N
SJ De2 Dc1 81(4) -108_665 . -108_665 N
SJ De2 Dc1 86.3(34) -108_665 . -305_565 N
SJ De2 Dc2 84(5) -108_666 . -108_666 N
SJ De2 Dc2 68.2(35) -108_666 . -305_566 N
SJ De2 Od 113(5) -108_665 . 1_555 N
SJ De2 Od 27(4) -108_665 . -108_665 N
SJ De2 Od 90(4) -108_665 . -305_565 N
SJ De2 Dd1 130(5) -108_644 . 1_555 N
SJ De2 Dd1 40(4) -108_644 . -108_644 N
SJ De2 Dd1 107(4) -108_644 . -305_544 N
SJ De2 Dd2 117(5) -108_644 . 1_555 N
SJ De2 Oc 103.7(14) -305_556 . 1_555 N
SJ De2 Oc 110.4(17) -305_556 . -108_656 N
SJ De2 Oc 6.1(11) -305_556 . -305_556 N
SJ De2 Dc1 100.0(15) -305_565 . 1_555 N
SJ De2 Dc1 75.2(20) -305_565 . -108_665 N
SJ De2 Dc1 21.8(7) -305_565 . -305_565 N
SJ De2 Dc2 147.3(24) -305_566 . -108_666 N
SJ De2 Dc2 19.3(8) -305_566 . -305_566 N
SJ De2 Od 121.3(22) -305_565 . 1_555 N
SJ De2 Od 68.6(35) -305_565 . -108_665 N
SJ De2 Od 8.6(11) -305_565 . -305_565 N
SJ De2 Dd1 108.5(22) -305_544 . 1_555 N
SJ De2 Dd1 75.3(28) -305_544 . -108_644 N
SJ De2 Dd1 24.9(13) -305_544 . -305_544 N
SJ De2 Dd2 137.5(24) -305_544 . 1_555 N
Oc De2 Oc 38.8(17) 1_555 . -108_656 N
Oc De2 Oc 98.8(21) 1_555 . -305_556 N
Oc De2 Dc1 7.5(4) 1_555 . 1_555 N
Oc De2 Dc1 40.2(20) 1_555 . -108_665 N
Oc De2 Dc1 82.6(14) 1_555 . -305_565 N
Oc De2 Dc2 54.9(22) 1_555 . -108_666 N
Oc De2 Dc2 120.0(17) 1_555 . -305_566 N
Oc De2 Od 17.6(12) 1_555 . 1_555 N
Oc De2 Od 94(4) 1_555 . -108_665 N
Oc De2 Od 96.3(16) 1_555 . -305_565 N
Oc De2 Dd1 18.7(16) 1_555 . 1_555 N
Oc De2 Dd1 76.3(26) 1_555 . -108_644 N
Oc De2 Dd1 88.0(20) 1_555 . -305_544 N
Oc De2 Dd2 35.1(14) 1_555 . 1_555 N
Oc De2 Oc 108.9(23) -108_656 . -305_556 N
Oc De2 Dc1 33.8(15) -108_665 . 1_555 N
Oc De2 Dc1 37.0(14) -108_665 . -108_665 N
Oc De2 Dc1 90.6(19) -108_665 . -305_565 N
Oc De2 Dc2 37.0(14) -108_666 . -108_666 N
Oc De2 Dc2 115.5(20) -108_666 . -305_566 N
Oc De2 Od 39.0(16) -108_665 . 1_555 N
Oc De2 Od 63(4) -108_665 . -108_665 N
Oc De2 Od 107.4(20) -108_665 . -305_565 N
Oc De2 Dd1 55.3(21) -108_644 . 1_555 N
Oc De2 Dd1 46.8(26) -108_644 . -108_644 N
Oc De2 Dd1 109.5(27) -108_644 . -305_544 N
Oc De2 Dd2 49.3(20) -108_644 . 1_555 N
Oc De2 Dc1 95.6(21) -305_565 . 1_555 N
Oc De2 Dc1 72.7(22) -305_565 . -108_665 N
Oc De2 Dc1 18.5(7) -305_565 . -305_565 N
Oc De2 Dc2 145.9(32) -305_566 . -108_666 N
Oc De2 Dc2 25.3(7) -305_566 . -305_566 N
Oc De2 Od 116.2(28) -305_565 . 1_555 N
Oc De2 Od 72.2(34) -305_565 . -108_665 N
Oc De2 Od 2.6(13) -305_565 . -305_565 N
Oc De2 Dd1 102.7(28) -305_544 . 1_555 N
Oc De2 Dd1 77.2(29) -305_544 . -108_644 N
Oc De2 Dd1 19.2(14) -305_544 . -305_544 N
Oc De2 Dd2 131.9(30) -305_544 . 1_555 N
Dc1 De2 Dc1 33.1(19) 1_555 . -108_665 N
Dc1 De2 Dc1 78.5(15) 1_555 . -305_565 N
Dc1 De2 Dc2 55.4(20) 1_555 . -108_666 N
Dc1 De2 Dc2 115.0(18) 1_555 . -305_566 N
Dc1 De2 Od 22.6(12) 1_555 . 1_555 N
Dc1 De2 Od 86(4) 1_555 . -108_665 N
Dc1 De2 Od 93.2(17) 1_555 . -305_565 N
Dc1 De2 Dd1 26.1(16) 1_555 . 1_555 N
Dc1 De2 Dd1 68.9(26) 1_555 . -108_644 N
Dc1 De2 Dd1 86.9(21) 1_555 . -305_544 N
Dc1 De2 Dd2 40.4(15) 1_555 . 1_555 N
Dc1 De2 Dc1 54.2(18) -108_665 . -305_565 N
Dc1 De2 Dc2 73.3(27) -108_666 . -108_666 N
Dc1 De2 Dc2 85.5(21) -108_666 . -305_566 N
Dc1 De2 Od 54.6(22) -108_665 . 1_555 N
Dc1 De2 Od 57.0(35) -108_665 . -108_665 N
Dc1 De2 Od 70.9(21) -108_665 . -305_565 N
Dc1 De2 Dd1 57.4(28) -108_644 . 1_555 N
Dc1 De2 Dd1 41.4(29) -108_644 . -108_644 N
Dc1 De2 Dd1 72.9(28) -108_644 . -305_544 N
Dc1 De2 Dd2 71.8(25) -108_644 . 1_555 N
Dc1 De2 Dc2 127.5(27) -305_566 . -108_666 N
Dc1 De2 Dc2 37.8(7) -305_566 . -305_566 N
Dc1 De2 Od 100.2(21) -305_565 . 1_555 N
Dc1 De2 Od 64.4(34) -305_565 . -108_665 N
Dc1 De2 Od 16.8(10) -305_565 . -305_565 N
Dc1 De2 Dd1 90.0(22) -305_544 . 1_555 N
Dc1 De2 Dd1 64.5(28) -305_544 . -108_644 N
Dc1 De2 Dd1 25.4(15) -305_544 . -305_544 N
Dc1 De2 Dd2 117.3(23) -305_544 . 1_555 N
Dc2 De2 Dc2 147.2(32) -108_666 . -305_566 N
Dc2 De2 Od 40.8(22) -108_665 . 1_555 N
Dc2 De2 Od 87(5) -108_665 . -108_665 N
Dc2 De2 Od 144.2(27) -108_665 . -305_565 N
Dc2 De2 Dd1 60.1(25) -108_644 . 1_555 N
Dc2 De2 Dd1 75.5(34) -108_644 . -108_644 N
Dc2 De2 Dd1 142(4) -108_644 . -305_544 N
Dc2 De2 Dd2 34.2(25) -108_644 . 1_555 N
Dc2 De2 Od 137.5(24) -305_565 . 1_555 N
Dc2 De2 Od 60.4(34) -305_565 . -108_665 N
Dc2 De2 Od 27.8(12) -305_565 . -305_565 N
Dc2 De2 Dd1 127.3(26) -305_544 . 1_555 N
Dc2 De2 Dd1 72.1(27) -305_544 . -108_644 N
Dc2 De2 Dd1 43.4(15) -305_544 . -305_544 N
Dc2 De2 Dd2 155.0(26) -305_544 . 1_555 N
Od De2 Od 101(4) 1_555 . -108_665 N
Od De2 Od 113.7(26) 1_555 . -305_565 N
Od De2 Dd1 20.0(7) 1_555 . 1_555 N
Od De2 Dd1 84.0(32) 1_555 . -108_644 N
Od De2 Dd1 104.0(28) 1_555 . -305_544 N
Od De2 Dd2 17.8(10) 1_555 . 1_555 N
Od De2 Od 73(4) -108_665 . -305_565 N
Od De2 Dd1 112(4) -108_644 . 1_555 N
Od De2 Dd1 17.5(30) -108_644 . -108_644 N
Od De2 Dd1 89(4) -108_644 . -305_544 N
Od De2 Dd2 112(5) -108_644 . 1_555 N
Od De2 Dd1 100.1(26) -305_544 . 1_555 N
Od De2 Dd1 77.2(31) -305_544 . -108_644 N
Od De2 Dd1 17.3(4) -305_544 . -305_544 N
Od De2 Dd2 129.4(26) -305_544 . 1_555 N
Dd1 De2 Dd1 95(4) 1_555 . -108_644 N
Dd1 De2 Dd1 87.4(30) 1_555 . -305_544 N
Dd1 De2 Dd2 29.7(9) 1_555 . 1_555 N
Dd1 De2 Dd1 90(4) -108_644 . -305_544 N
Dd1 De2 Dd2 96.1(31) -108_644 . 1_555 N
Dd1 De2 Dd2 117.0(33) -305_544 . 1_555 N
Si1 SIII Si1 99.0(21) -211_455 . -302_445 N
Si1 SIII Si2 65.4(11) -211_554 . -108_644 N
Si1 SIII Si2 66.7(11) -211_554 . -303_544 N
Si1 SIII Al1 65.4(11) -211_464 . -108_554 N
Si1 SIII Al1 66.7(11) -211_464 . -303_454 N
Si1 SIII O1 75.5(8) -211_454 . 208_343 N
Si1 SIII O1 30.22(21) -211_454 . -211_454 N
Si1 SIII O1 92.6(10) -211_454 . 303_555 N
Si1 SIII O1 128.5(22) -211_454 . -302_444 N
Si1 SIII O2 80.0(16) -211_454 . 4_555 N
Si1 SIII O2 30.3(5) -211_454 . -301_444 N
Si1 SIII O4 92.4(19) -211_454 . -10_554 N
Si1 SIII O4 33.6(6) -211_454 . -12_554 N
Si1 SIII SJ 121.0(15) -211_566 . 4_555 N
Si1 SIII SJ 65.3(8) -211_566 . -301_556 N
Si1 SIII Oc 116.5(7) -211_566 . 4_555 N
Si1 SIII Oc 70.87(26) -211_566 . 208_455 N
Si1 SIII Oc 156.0(12) -211_566 . 303_555 N
Si1 SIII Oc 83.68(29) -211_566 . -301_556 N
Si1 SIII Dc1 130.2(7) -211_575 . 4_555 N
Si1 SIII Dc1 81.06(35) -211_575 . -301_565 N
Si1 SIII Dc2 107.1(8) -211_576 . 4_555 N
Si1 SIII Dc2 54.68(28) -211_576 . 208_465 N
Si1 SIII Dc2 148.8(20) -211_576 . 303_555 N
Si1 SIII Si2 66.7(11) -302_544 . -108_644 N
Si1 SIII Si2 65.4(11) -302_544 . -303_544 N
Si1 SIII Al1 66.7(11) -302_454 . -108_554 N
Si1 SIII Al1 65.4(11) -302_454 . -303_454 N
Si1 SIII O1 92.6(10) -302_444 . 208_343 N
Si1 SIII O1 128.5(22) -302_444 . -211_454 N
Si1 SIII O1 75.5(8) -302_444 . 303_555 N
Si1 SIII O1 30.22(21) -302_444 . -302_444 N
Si1 SIII O2 30.3(5) -302_444 . 4_555 N
Si1 SIII O2 80.0(16) -302_444 . -301_444 N
Si1 SIII O4 33.6(6) -302_444 . -10_554 N
Si1 SIII O4 92.4(19) -302_444 . -12_554 N
Si1 SIII SJ 65.3(8) -302_556 . 4_555 N
Si1 SIII SJ 121.0(15) -302_556 . -301_556 N
Si1 SIII Oc 83.68(29) -302_556 . 4_555 N
Si1 SIII Oc 156.0(12) -302_556 . 208_455 N
Si1 SIII Oc 70.87(26) -302_556 . 303_555 N
Si1 SIII Oc 116.5(7) -302_556 . -301_556 N
Si1 SIII Dc1 81.06(35) -302_565 . 4_555 N
Si1 SIII Dc1 130.2(7) -302_565 . -301_565 N
Si1 SIII Dc2 88.5(6) -302_566 . 4_555 N
Si1 SIII Dc2 148.8(20) -302_566 . 208_465 N
Si1 SIII Dc2 54.68(28) -302_566 . 303_555 N
Si2 SIII Si2 102.6(21) -108_644 . -303_544 N
Si2 SIII Al1 0.0 -108_554 . -108_554 N
Si2 SIII Al1 102.6(21) -108_554 . -303_454 N
Si2 SIII O1 30.95(23) -108_544 . 208_343 N
Si2 SIII O1 77.9(8) -108_544 . -211_454 N
Si2 SIII O1 131.2(22) -108_544 . 303_555 N
Si2 SIII O1 88.7(10) -108_544 . -302_444 N
Si2 SIII O2 79.4(16) -108_544 . 4_555 N
Si2 SIII O2 35.5(6) -108_544 . -301_444 N
Si2 SIII O4 36.9(6) -108_544 . -10_554 N
Si2 SIII O4 92.2(19) -108_544 . -12_554 N
Si2 SIII SJ 56.0(7) -108_656 . 4_555 N
Si2 SIII SJ 130.7(17) -108_656 . -301_556 N
Si2 SIII Oc 57.89(21) -108_656 . 4_555 N
Si2 SIII Oc 123.6(4) -108_656 . 208_455 N
Si2 SIII Oc 90.63(28) -108_656 . 303_555 N
Si2 SIII Oc 148.7(14) -108_656 . -301_556 N
Si2 SIII Dc1 69.42(28) -108_665 . 4_555 N
Si2 SIII Dc1 145.4(9) -108_665 . -301_565 N
Si2 SIII Dc2 52.2(4) -108_666 . 4_555 N
Si2 SIII Dc2 108.8(7) -108_666 . 208_465 N
Si2 SIII Dc2 86.9(5) -108_666 . 303_555 N
Si2 SIII Al1 102.6(21) -303_454 . -108_554 N
Si2 SIII Al1 0.0 -303_454 . -303_454 N
Si2 SIII O1 131.2(22) -303_444 . 208_343 N
Si2 SIII O1 88.7(10) -303_444 . -211_454 N
Si2 SIII O1 30.95(23) -303_444 . 303_555 N
Si2 SIII O1 77.9(8) -303_444 . -302_444 N
Si2 SIII O2 35.5(6) -303_444 . 4_555 N
Si2 SIII O2 79.4(16) -303_444 . -301_444 N
Si2 SIII O4 92.2(19) -303_444 . -10_554 N
Si2 SIII O4 36.9(6) -303_444 . -12_554 N
Si2 SIII SJ 130.7(17) -303_556 . 4_555 N
Si2 SIII SJ 56.0(7) -303_556 . -301_556 N
Si2 SIII Oc 148.7(14) -303_556 . 4_555 N
Si2 SIII Oc 90.63(28) -303_556 . 208_455 N
Si2 SIII Oc 123.6(4) -303_556 . 303_555 N
Si2 SIII Oc 57.89(21) -303_556 . -301_556 N
Si2 SIII Dc1 145.4(9) -303_565 . 4_555 N
Si2 SIII Dc1 69.42(28) -303_565 . -301_565 N
Si2 SIII Dc2 150.7(20) -303_566 . 4_555 N
Si2 SIII Dc2 86.9(5) -303_566 . 208_465 N
Si2 SIII Dc2 108.8(7) -303_566 . 303_555 N
Al1 SIII Al1 102.6(21) -108_554 . -303_454 N
Al1 SIII O1 30.95(23) -108_544 . 208_343 N
Al1 SIII O1 77.9(8) -108_544 . -211_454 N
Al1 SIII O1 131.2(22) -108_544 . 303_555 N
Al1 SIII O1 88.7(10) -108_544 . -302_444 N
Al1 SIII O2 79.4(16) -108_544 . 4_555 N
Al1 SIII O2 35.5(6) -108_544 . -301_444 N
Al1 SIII O4 36.9(6) -108_544 . -10_554 N
Al1 SIII O4 92.2(19) -108_544 . -12_554 N
Al1 SIII SJ 56.0(7) -108_656 . 4_555 N
Al1 SIII SJ 130.7(17) -108_656 . -301_556 N
Al1 SIII Oc 57.89(21) -108_656 . 4_555 N
Al1 SIII Oc 123.6(4) -108_656 . 208_455 N
Al1 SIII Oc 90.63(28) -108_656 . 303_555 N
Al1 SIII Oc 148.7(14) -108_656 . -301_556 N
Al1 SIII Dc1 69.42(28) -108_665 . 4_555 N
Al1 SIII Dc1 145.4(9) -108_665 . -301_565 N
Al1 SIII Dc2 52.2(4) -108_666 . 4_555 N
Al1 SIII Dc2 108.8(7) -108_666 . 208_465 N
Al1 SIII Dc2 86.9(5) -108_666 . 303_555 N
Al1 SIII O1 131.2(22) -303_444 . 208_343 N
Al1 SIII O1 88.7(10) -303_444 . -211_454 N
Al1 SIII O1 30.95(23) -303_444 . 303_555 N
Al1 SIII O1 77.9(8) -303_444 . -302_444 N
Al1 SIII O2 35.5(6) -303_444 . 4_555 N
Al1 SIII O2 79.4(16) -303_444 . -301_444 N
Al1 SIII O4 92.2(19) -303_444 . -10_554 N
Al1 SIII O4 36.9(6) -303_444 . -12_554 N
Al1 SIII SJ 130.7(17) -303_556 . 4_555 N
Al1 SIII SJ 56.0(7) -303_556 . -301_556 N
Al1 SIII Oc 148.7(14) -303_556 . 4_555 N
Al1 SIII Oc 90.63(28) -303_556 . 208_455 N
Al1 SIII Oc 123.6(4) -303_556 . 303_555 N
Al1 SIII Oc 57.89(21) -303_556 . -301_556 N
Al1 SIII Dc1 145.4(9) -303_565 . 4_555 N
Al1 SIII Dc1 69.42(28) -303_565 . -301_565 N
Al1 SIII Dc2 150.7(20) -303_566 . 4_555 N
Al1 SIII Dc2 86.9(5) -303_566 . 208_465 N
Al1 SIII Dc2 108.8(7) -303_566 . 303_555 N
O1 SIII O1 71.42(31) 208_343 . -211_454 N
O1 SIII O1 161.7(24) 208_343 . 303_555 N
O1 SIII O1 105.0(5) 208_343 . -302_444 N
O1 SIII O2 110.2(17) 208_343 . 4_555 N
O1 SIII O2 53.2(5) 208_343 . -301_444 N
O1 SIII O4 59.1(5) 208_343 . -10_554 N
O1 SIII O4 108.7(14) 208_343 . -12_554 N
O1 SIII SJ 50.9(7) 208_455 . 4_555 N
O1 SIII SJ 130.8(7) 208_455 . -301_556 N
O1 SIII Oc 41.10(25) 208_455 . 4_555 N
O1 SIII Oc 105.3(5) 208_455 . 208_455 N
O1 SIII Oc 83.1(4) 208_455 . 303_555 N
O1 SIII Oc 146.7(4) 208_455 . -301_556 N
O1 SIII Dc1 54.90(30) 208_464 . 4_555 N
O1 SIII Dc1 134.0(7) 208_464 . -301_565 N
O1 SIII Dc2 31.68(29) 208_465 . 4_555 N
O1 SIII Dc2 95.75(30) 208_465 . 208_465 N
O1 SIII Dc2 88.16(33) 208_465 . 303_555 N
O1 SIII O1 105.0(5) -211_454 . 303_555 N
O1 SIII O1 158.5(24) -211_454 . -302_444 N
O1 SIII O2 109.6(17) -211_454 . 4_555 N
O1 SIII O2 50.8(5) -211_454 . -301_444 N
O1 SIII O4 113.1(16) -211_454 . -10_554 N
O1 SIII O4 51.7(4) -211_454 . -12_554 N
O1 SIII SJ 122.2(7) -211_566 . 4_555 N
O1 SIII SJ 59.7(7) -211_566 . -301_556 N
O1 SIII Oc 108.27(25) -211_566 . 4_555 N
O1 SIII Oc 47.44(29) -211_566 . 208_455 N
O1 SIII Oc 147.6(11) -211_566 . 303_555 N
O1 SIII Oc 77.45(25) -211_566 . -301_556 N
O1 SIII Dc1 120.4(4) -211_575 . 4_555 N
O1 SIII Dc1 68.5(4) -211_575 . -301_565 N
O1 SIII Dc2 98.41(26) -211_576 . 4_555 N
O1 SIII Dc2 31.28(22) -211_576 . 208_465 N
O1 SIII Dc2 159.10(34) -211_576 . 303_555 N
O1 SIII O1 71.42(31) 303_555 . -302_444 N
O1 SIII O2 53.2(5) 303_555 . 4_555 N
O1 SIII O2 110.2(17) 303_555 . -301_444 N
O1 SIII O4 108.7(14) 303_555 . -10_554 N
O1 SIII O4 59.1(5) 303_555 . -12_554 N
O1 SIII SJ 130.8(7) 303_555 . 4_555 N
O1 SIII SJ 50.9(7) 303_555 . -301_556 N
O1 SIII Oc 146.7(4) 303_555 . 4_555 N
O1 SIII Oc 83.1(4) 303_555 . 208_455 N
O1 SIII Oc 105.3(5) 303_555 . 303_555 N
O1 SIII Oc 41.10(25) 303_555 . -301_556 N
O1 SIII Dc1 134.0(7) 303_555 . 4_555 N
O1 SIII Dc1 54.90(30) 303_555 . -301_565 N
O1 SIII Dc2 156.5(4) 303_555 . 4_555 N
O1 SIII Dc2 88.16(33) 303_555 . 208_465 N
O1 SIII Dc2 95.75(30) 303_555 . 303_555 N
O1 SIII O2 50.8(5) -302_444 . 4_555 N
O1 SIII O2 109.6(17) -302_444 . -301_444 N
O1 SIII O4 51.7(4) -302_444 . -10_554 N
O1 SIII O4 113.1(16) -302_444 . -12_554 N
O1 SIII SJ 59.7(7) -302_556 . 4_555 N
O1 SIII SJ 122.2(7) -302_556 . -301_556 N
O1 SIII Oc 77.45(25) -302_556 . 4_555 N
O1 SIII Oc 147.6(11) -302_556 . 208_455 N
O1 SIII Oc 47.44(29) -302_556 . 303_555 N
O1 SIII Oc 108.27(25) -302_556 . -301_556 N
O1 SIII Dc1 68.5(4) -302_565 . 4_555 N
O1 SIII Dc1 120.4(4) -302_565 . -301_565 N
O1 SIII Dc2 86.03(28) -302_566 . 4_555 N
O1 SIII Dc2 159.10(34) -302_566 . 208_465 N
O1 SIII Dc2 31.28(22) -302_566 . 303_555 N
O2 SIII O2 74.1(16) 4_555 . -301_444 N
O2 SIII O4 58.0(12) 4_555 . -10_554 N
O2 SIII O4 63.8(13) 4_555 . -12_554 N
O2 SIII SJ 95.3(13) 4_555 . 4_555 N
O2 SIII SJ 91.5(12) 4_555 . -301_556 N
O2 SIII Oc 113.3(8) 4_555 . 4_555 N
O2 SIII Oc 126.0(8) 4_555 . 208_455 N
O2 SIII Oc 97.6(5) 4_555 . 303_555 N
O2 SIII Oc 91.0(5) 4_555 . -301_556 N
O2 SIII Dc1 111.4(7) 4_555 . 4_555 N
O2 SIII Dc1 103.8(6) 4_555 . -301_565 N
O2 SIII Dc2 116.6(12) 4_555 . 4_555 N
O2 SIII Dc2 119.7(13) 4_555 . 208_465 N
O2 SIII Dc2 81.1(6) 4_555 . 303_555 N
O2 SIII O4 63.8(13) -301_444 . -10_554 N
O2 SIII O4 58.0(12) -301_444 . -12_554 N
O2 SIII SJ 91.5(12) -301_556 . 4_555 N
O2 SIII SJ 95.3(13) -301_556 . -301_556 N
O2 SIII Oc 91.0(5) -301_556 . 4_555 N
O2 SIII Oc 97.6(5) -301_556 . 208_455 N
O2 SIII Oc 126.0(8) -301_556 . 303_555 N
O2 SIII Oc 113.3(8) -301_556 . -301_556 N
O2 SIII Dc1 103.8(6) -301_565 . 4_555 N
O2 SIII Dc1 111.4(7) -301_565 . -301_565 N
O2 SIII Dc2 83.2(7) -301_566 . 4_555 N
O2 SIII Dc2 81.1(6) -301_566 . 208_465 N
O2 SIII Dc2 119.7(13) -301_566 . 303_555 N
O4 SIII O4 104.9(25) -10_554 . -12_554 N
O4 SIII SJ 42.5(6) -10_666 . 4_555 N
O4 SIII SJ 145.8(26) -10_666 . -301_556 N
O4 SIII Oc 57.25(32) -10_666 . 4_555 N
O4 SIII Oc 160.3(12) -10_666 . 208_455 N
O4 SIII Oc 66.95(30) -10_666 . 303_555 N
O4 SIII Oc 148.9(16) -10_666 . -301_556 N
O4 SIII Dc1 60.7(5) -10_675 . 4_555 N
O4 SIII Dc1 161.6(19) -10_675 . -301_565 N
O4 SIII Dc2 58.9(4) -10_676 . 4_555 N
O4 SIII Dc2 144.3(17) -10_676 . 208_465 N
O4 SIII Dc2 56.49(31) -10_676 . 303_555 N
O4 SIII SJ 145.8(26) -12_666 . 4_555 N
O4 SIII SJ 42.5(6) -12_666 . -301_556 N
O4 SIII Oc 148.9(16) -12_666 . 4_555 N
O4 SIII Oc 66.95(30) -12_666 . 208_455 N
O4 SIII Oc 160.3(12) -12_666 . 303_555 N
O4 SIII Oc 57.25(32) -12_666 . -301_556 N
O4 SIII Dc1 161.6(19) -12_675 . 4_555 N
O4 SIII Dc1 60.7(5) -12_675 . -301_565 N
O4 SIII Dc2 140.3(15) -12_676 . 4_555 N
O4 SIII Dc2 56.49(31) -12_676 . 208_465 N
O4 SIII Dc2 144.3(17) -12_676 . 303_555 N
SJ SIII SJ 171.5(29) 4_555 . -301_556 N
SJ SIII Oc 18.8(7) 4_555 . 4_555 N
SJ SIII Oc 138.7(19) 4_555 . 208_455 N
SJ SIII Oc 35.1(7) 4_555 . 303_555 N
SJ SIII Oc 155.3(19) 4_555 . -301_556 N
SJ SIII Dc1 18.2(8) 4_555 . 4_555 N
SJ SIII Dc1 153.4(24) 4_555 . -301_565 N
SJ SIII Dc2 26.4(7) 4_555 . 4_555 N
SJ SIII Dc2 139.9(12) 4_555 . 208_465 N
SJ SIII Dc2 37.2(7) 4_555 . 303_555 N
SJ SIII Oc 155.3(19) -301_556 . 4_555 N
SJ SIII Oc 35.1(7) -301_556 . 208_455 N
SJ SIII Oc 138.7(19) -301_556 . 303_555 N
SJ SIII Oc 18.8(7) -301_556 . -301_556 N
SJ SIII Dc1 153.4(24) -301_565 . 4_555 N
SJ SIII Dc1 18.2(8) -301_565 . -301_565 N
SJ SIII Dc2 149.9(15) -301_566 . 4_555 N
SJ SIII Dc2 37.2(7) -301_566 . 208_465 N
SJ SIII Dc2 139.9(12) -301_566 . 303_555 N
Oc SIII Oc 120.3(13) 4_555 . 208_455 N
Oc SIII Oc 42.4(4) 4_555 . 303_555 N
Oc SIII Oc 150.0(19) 4_555 . -301_556 N
Oc SIII Dc1 13.80(9) 4_555 . 4_555 N
Oc SIII Dc1 140.9(18) 4_555 . -301_565 N
Oc SIII Dc2 10.00(21) 4_555 . 4_555 N
Oc SIII Dc2 121.3(9) 4_555 . 208_465 N
Oc SIII Dc2 51.0(4) 4_555 . 303_555 N
Oc SIII Oc 126.4(21) 208_455 . 303_555 N
Oc SIII Oc 42.4(4) 208_455 . -301_556 N
Oc SIII Dc1 122.3(17) 208_464 . 4_555 N
Oc SIII Dc1 28.9(4) 208_464 . -301_565 N
Oc SIII Dc2 115.1(12) 208_465 . 4_555 N
Oc SIII Dc2 16.58(15) 208_465 . 208_465 N
Oc SIII Dc2 140.0(22) 208_465 . 303_555 N
Oc SIII Oc 120.3(13) 303_555 . -301_556 N
Oc SIII Dc1 28.9(4) 303_555 . 4_555 N
Oc SIII Dc1 122.3(17) 303_555 . -301_565 N
Oc SIII Dc2 52.4(5) 303_555 . 4_555 N
Oc SIII Dc2 140.0(22) 303_555 . 208_465 N
Oc SIII Dc2 16.58(15) 303_555 . 303_555 N
Oc SIII Dc1 140.9(18) -301_565 . 4_555 N
Oc SIII Dc1 13.80(9) -301_565 . -301_565 N
Oc SIII Dc2 151.4(20) -301_566 . 4_555 N
Oc SIII Dc2 51.0(4) -301_566 . 208_465 N
Oc SIII Dc2 121.3(9) -301_566 . 303_555 N
Dc1 SIII Dc1 135.6(20) 4_555 . -301_565 N
Dc1 SIII Dc2 23.54(28) 4_555 . 4_555 N
Dc1 SIII Dc2 127.7(14) 4_555 . 208_465 N
Dc1 SIII Dc2 39.4(5) 4_555 . 303_555 N
Dc1 SIII Dc2 139.5(18) -301_566 . 4_555 N
Dc1 SIII Dc2 39.4(5) -301_566 . 208_465 N
Dc1 SIII Dc2 127.7(14) -301_566 . 303_555 N
Dc2 SIII Dc2 113.6(8) 4_555 . 208_465 N
Dc2 SIII Dc2 60.8(5) 4_555 . 303_555 N
Dc2 SIII Dc2 155.3(23) 208_465 . 303_555 N
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Si1 Si2 3.150(7) . 2_555 N
Si1 Si2 3.190(7) . 3_555 N
Si1 Si2 3.064(7) . -1_555 N
Si1 Si2 3.205(7) . 107_555 N
Si1 Al1 3.150(7) . 2_555 N
Si1 Al1 3.190(7) . 3_555 N
Si1 Al1 3.064(7) . -1_555 N
Si1 Al1 3.205(7) . 107_555 N
Si1 O1 1.627(8) . 1_555 N
Si1 O1 3.737(9) . -2_555 N
Si1 O1 3.928(7) . -3_555 N
Si1 O2 3.752(6) . 3_555 N
Si1 O2 3.661(6) . 105_544 N
Si1 O2 1.527(7) . -206_454 N
Si1 O2 3.937(7) . -304_445 N
Si1 O3 4.256(7) . 1_555 N
Si1 O3 1.762(7) . 2_555 N
Si1 O3 3.856(6) . -3_555 N
Si1 O3 3.880(7) . 310_555 N
Si1 O4 3.837(6) . 208_555 N
Si1 O4 1.591(6) . 209_555 N
Si1 SI 3.484(6) . 1_555 N
Si1 SI' 3.198(6) . 1_555 N
Si1 SII 3.329(6) . -105_544 N
Si1 SJ 3.081(32) . -206_454 N
Si1 Oc 3.611(14) . -2_555 N
Si1 Dc2 2.882(16) . -2_555 N
Si1 Od 3.33(6) . -206_454 N
Si1 Dd1 3.99(6) . -206_454 N
Si1 Dd2 2.58(8) . -206_454 N
Si1 OII' 3.942(29) . -105_544 N
Si1 DII'1 3.847(10) . 208_555 N
Si1 DII'1 3.61(8) . 209_555 N
Si1 DII'1 3.78(10) . 312_555 N
Si1 Of 4.105(32) . 3_555 N
Si1 Of 3.819(32) . 105_544 N
Si1 Of 3.842(34) . -206_454 N
Si1 Df2 3.00(4) . 105_544 N
Si1 Df2 3.77(6) . -206_454 N
Si1 Oe 3.460(28) . -112_534 N
Si1 De1 3.49(5) . -112_534 N
Si1 De2 3.50(5) . -112_534 N
Si1 De2 3.93(4) . -206_454 N
Si1 SIII 2.87(4) . 206_454 N
Si2 Si1 3.190(7) . 2_555 N
Si2 Si1 3.150(7) . 3_555 N
Si2 Si1 3.064(7) . -1_555 N
Si2 Si1 3.205(7) . 209_555 N
Si2 O1 3.736(8) . 2_555 N
Si2 O1 3.893(9) . 3_555 N
Si2 O1 1.667(8) . -1_555 N
Si2 O2 3.781(7) . 2_555 N
Si2 O2 1.803(7) . -105_544 N
Si2 O2 3.576(6) . 206_454 N
Si2 O2 3.829(7) . -304_445 N
Si2 O3 1.607(8) . 3_555 N
Si2 O3 3.934(7) . -2_555 N
Si2 O3 3.915(7) . 312_555 N
Si2 O4 1.777(7) . 107_555 N
Si2 O4 3.895(7) . 111_555 N
Si2 O4 4.215(7) . -209_443 N
Si2 O4 4.190(7) . 310_555 N
Si2 SI 3.555(6) . 1_555 N
Si2 SI' 3.287(6) . 1_555 N
Si2 SII 3.234(6) . 107_555 N
Si2 SJ 2.723(28) . 2_555 N
Si2 Oc 3.488(14) . 2_555 N
Si2 Dc1 3.891(18) . 2_555 N
Si2 Dc2 2.754(16) . 2_555 N
Si2 Od 3.14(5) . 2_555 N
Si2 Dd1 3.68(7) . 2_555 N
Si2 Dd2 2.51(9) . 2_555 N
Si2 OII' 3.975(31) . 107_555 N
Si2 DII'1 3.31(6) . 107_555 N
Si2 DII*1 3.93(10) . 107_555 N
Si2 Of 3.454(35) . -105_544 N
Si2 Of 4.084(34) . 206_454 N
Si2 Df2 2.74(5) . -105_544 N
Si2 Df2 3.90(5) . 206_454 N
Si2 Oe 4.26(4) . 112_454 N
Si2 Oe 3.554(31) . 206_454 N
Si2 De1 3.59(5) . 112_454 N
Si2 De2 3.03(6) . 206_454 N
Si2 SIII 2.96(4) . 105_544 N
Al1 Si1 3.190(7) . 2_555 N
Al1 Si1 3.150(7) . 3_555 N
Al1 Si1 3.064(7) . -1_555 N
Al1 Si1 3.205(7) . 209_555 N
Al1 O1 3.736(8) . 2_555 N
Al1 O1 3.893(9) . 3_555 N
Al1 O1 1.667(8) . -1_555 N
Al1 O1 4.326(9) . 209_555 N
Al1 O2 3.781(7) . 2_555 N
Al1 O2 1.803(7) . -105_544 N
Al1 O2 3.576(6) . 206_454 N
Al1 O2 3.829(7) . -304_445 N
Al1 O3 1.607(8) . 3_555 N
Al1 O3 3.934(7) . -2_555 N
Al1 O3 3.915(7) . 312_555 N
Al1 O4 1.777(7) . 107_555 N
Al1 O4 3.895(7) . 111_555 N
Al1 O4 4.215(7) . -209_443 N
Al1 O4 4.190(7) . 310_555 N
Al1 SI 3.555(6) . 1_555 N
Al1 SI' 3.287(6) . 1_555 N
Al1 SII 3.234(6) . 107_555 N
Al1 SJ 2.723(28) . 2_555 N
Al1 Oc 3.488(14) . 2_555 N
Al1 Dc1 3.891(18) . 2_555 N
Al1 Dc2 2.754(16) . 2_555 N
Al1 Od 3.14(5) . 2_555 N
Al1 Dd1 3.68(7) . 2_555 N
Al1 Dd2 2.51(9) . 2_555 N
Al1 OII' 3.975(31) . 107_555 N
Al1 DII'1 3.31(6) . 107_555 N
Al1 DII*1 3.93(10) . 107_555 N
Al1 Of 3.454(35) . -105_544 N
Al1 Of 4.084(34) . 206_454 N
Al1 Df2 2.74(5) . -105_544 N
Al1 Df2 3.90(5) . 206_454 N
Al1 Oe 4.26(4) . 112_454 N
Al1 Oe 3.554(31) . 206_454 N
Al1 De1 3.59(5) . 112_454 N
Al1 De2 3.03(6) . 206_454 N
Al1 SIII 2.96(4) . 105_544 N
O1 Si1 1.627(8) . 1_555 N
O1 Si1 3.928(7) . -2_555 N
O1 Si1 3.737(9) . -3_555 N
O1 Si2 3.893(9) . 2_555 N
O1 Si2 3.736(8) . 3_555 N
O1 Si2 1.667(8) . -1_555 N
O1 Al1 3.893(9) . 2_555 N
O1 Al1 3.736(8) . 3_555 N
O1 Al1 1.667(8) . -1_555 N
O1 Al1 4.326(9) . 107_555 N
O1 O1 3.7627(31) . -2_555 N
O1 O1 3.7627(31) . -3_555 N
O1 O1 5.1158(31) . -209_443 N
O1 O1 5.1158(31) . -307_445 N
O1 O2 5.060(8) . 3_555 N
O1 O2 5.070(9) . -2_555 N
O1 O2 2.778(7) . 105_544 N
O1 O2 2.663(7) . -206_454 N
O1 O2 4.670(5) . 304_445 N
O1 O2 4.696(6) . -304_445 N
O1 O3 5.178(8) . 1_555 N
O1 O3 2.745(6) . 2_555 N
O1 O3 5.225(8) . -1_555 N
O1 O3 2.809(6) . -3_555 N
O1 O3 5.156(7) . 310_555 N
O1 O3 5.322(7) . -312_434 N
O1 O4 2.867(7) . -107_443 N
O1 O4 4.611(9) . -111_434 N
O1 O4 4.739(9) . 208_555 N
O1 O4 2.571(7) . 209_555 N
O1 O4 5.150(7) . 312_555 N
O1 O4 5.067(6) . -310_344 N
O1 SI 3.7617(31) . 1_555 N
O1 SI' 4.343(6) . 1_555 N
O1 SI' 4.393(6) . -1_555 N
O1 SII 4.400(5) . -105_544 N
O1 SII 4.524(4) . -107_443 N
O1 SJ 2.627(32) . -2_555 N
O1 SJ 3.039(33) . -206_454 N
O1 Oc 5.199(14) . 1_555 N
O1 Oc 5.874(16) . 3_555 N
O1 Oc 2.637(13) . -2_555 N
O1 Oc 4.341(16) . 212_544 N
O1 Oc 4.561(17) . -206_454 N
O1 Dc1 3.261(15) . -2_555 N
O1 Dc1 3.968(21) . -206_454 N
O1 Dc2 1.773(13) . -2_555 N
O1 Od 5.62(5) . 1_555 N
O1 Od 5.80(5) . 3_555 N
O1 Od 3.00(5) . -2_555 N
O1 Od 5.84(6) . 105_544 N
O1 Od 5.96(5) . -112_534 N
O1 Od 5.81(6) . 212_544 N
O1 Od 3.12(6) . -206_454 N
O1 Od 5.88(6) . 304_445 N
O1 Dd1 3.46(8) . -2_555 N
O1 Dd1 3.73(7) . -206_454 N
O1 Dd2 2.87(10) . -2_555 N
O1 Dd2 2.75(10) . -206_454 N
O1 OII' 5.518(30) . -105_544 N
O1 OII' 5.616(30) . -107_443 N
O1 OII* 5.00(4) . -105_544 N
O1 OII* 5.11(4) . -107_443 N
O1 Of 4.096(32) . 3_555 N
O1 Of 4.524(28) . -2_555 N
O1 Of 2.874(33) . 105_544 N
O1 Of 3.540(34) . -206_454 N
O1 Df1 3.42(4) . 105_544 N
O1 Df2 1.949(32) . 105_544 N
O1 Df2 3.56(6) . -206_454 N
O1 Oe 5.910(35) . -2_555 N
O1 Oe 2.999(33) . -112_534 N
O1 Oe 5.982(32) . 207_445 N
O1 Oe 3.34(4) . -206_454 N
O1 Oe 5.55(4) . 302_545 N
O1 Oe 5.872(32) . 304_445 N
O1 Oe 5.649(31) . 308_544 N
O1 De1 2.62(6) . -112_534 N
O1 De2 3.32(5) . -112_534 N
O1 De2 2.61(5) . -206_454 N
O1 SIII 3.219(14) . 102_544 N
O1 SIII 3.228(15) . 206_454 N
O2 Si1 3.752(6) . 2_555 N
O2 Si1 1.527(7) . 111_555 N
O2 Si1 3.661(6) . -108_544 N
O2 Si1 3.937(7) . -304_445 N
O2 Si2 3.781(7) . 3_555 N
O2 Si2 1.803(7) . 208_555 N
O2 Si2 3.576(6) . -211_454 N
O2 Si2 3.829(7) . -304_445 N
O2 Al1 3.781(7) . 3_555 N
O2 Al1 1.803(7) . 208_555 N
O2 Al1 3.576(6) . -211_454 N
O2 Al1 3.829(7) . -304_445 N
O2 O1 5.060(8) . 2_555 N
O2 O1 4.670(5) . 4_555 N
O2 O1 5.070(9) . -3_555 N
O2 O1 2.663(7) . 111_555 N
O2 O1 2.778(7) . -108_544 N
O2 O1 4.696(6) . -304_445 N
O2 O2 3.862(5) . 107_555 N
O2 O2 4.025(6) . -109_543 N
O2 O2 3.862(5) . 209_555 N
O2 O2 4.025(6) . -207_453 N
O2 O2 5.578(7) . -301_445 N
O2 O2 3.568(7) . -304_445 N
O2 O3 4.524(6) . 2_555 N
O2 O3 4.653(6) . 3_555 N
O2 O3 3.771(4) . 4_555 N
O2 O3 2.732(6) . 111_555 N
O2 O3 5.853(5) . -108_544 N
O2 O3 2.667(6) . 208_555 N
O2 O3 5.823(4) . -211_454 N
O2 O3 5.960(5) . 310_555 N
O2 O3 5.211(4) . -304_445 N
O2 O4 5.210(6) . -105_544 N
O2 O4 5.155(5) . -206_454 N
O2 O4 2.882(5) . 310_555 N
O2 O4 2.652(6) . 312_555 N
O2 O4 5.082(5) . -302_445 N
O2 O4 5.247(5) . -303_445 N
O2 SI 2.7890(33) . 4_555 N
O2 SI' 4.898(5) . 1_555 N
O2 SI' 4.488(8) . 4_555 N
O2 SI' 2.295(4) . 111_555 N
O2 SII 4.438(6) . 107_555 N
O2 SII 4.332(6) . -105_544 N
O2 SJ 4.289(30) . 1_555 N
O2 SJ 4.156(29) . -304_445 N
O2 Oc 5.841(16) . 1_555 N
O2 Oc 5.601(15) . -3_555 N
O2 Oc 4.736(13) . -108_544 N
O2 Oc 5.018(14) . -304_445 N
O2 Od 4.63(6) . 1_555 N
O2 Od 5.48(6) . -108_544 N
O2 Od 5.73(6) . -207_453 N
O2 Od 4.64(5) . -304_445 N
O2 Dd2 3.92(7) . 1_555 N
O2 OII' 4.911(24) . 1_555 N
O2 OII' 3.812(10) . 107_555 N
O2 OII' 5.75(5) . 111_555 N
O2 OII' 3.771(11) . -105_544 N
O2 DII'1 3.54(11) . -105_544 N
O2 DII'1 2.895(29) . 310_555 N
O2 DII'1 3.31(9) . 312_555 N
O2 DII'2 3.85(9) . 107_555 N
O2 DII'2 3.82(7) . 209_555 N
O2 Of 3.85(4) . 1_555 N
O2 Of 5.234(33) . -109_543 N
O2 Of 5.712(35) . -207_453 N
O2 Of 4.524(31) . -304_445 N
O2 Df2 3.44(5) . 1_555 N
O2 Oe 5.86(4) . 1_555 N
O2 Oe 5.601(34) . 103_554 N
O2 Oe 4.701(28) . 105_544 N
O2 Oe 4.920(30) . -207_453 N
O2 SIII 2.96(5) . 304_445 N
O3 Si1 4.256(7) . 1_555 N
O3 Si1 1.762(7) . 3_555 N
O3 Si1 3.856(6) . -2_555 N
O3 Si1 3.880(7) . 310_555 N
O3 Si2 1.607(8) . 2_555 N
O3 Si2 3.934(7) . -3_555 N
O3 Si2 3.915(7) . 312_555 N
O3 Al1 1.607(8) . 2_555 N
O3 Al1 3.934(7) . -3_555 N
O3 Al1 3.915(7) . 312_555 N
O3 O1 5.178(8) . 1_555 N
O3 O1 2.745(6) . 3_555 N
O3 O1 5.225(8) . -1_555 N
O3 O1 2.809(6) . -2_555 N
O3 O1 5.322(7) . -212_454 N
O3 O1 5.156(7) . 310_555 N
O3 O2 4.653(6) . 2_555 N
O3 O2 4.524(6) . 3_555 N
O3 O2 5.853(5) . 105_544 N
O3 O2 2.667(6) . -105_544 N
O3 O2 5.823(4) . 206_454 N
O3 O2 2.732(6) . -206_454 N
O3 O2 3.771(4) . 304_445 N
O3 O2 5.960(5) . 310_555 N
O3 O2 5.211(4) . -304_445 N
O3 O3 5.143(5) . 2_555 N
O3 O3 5.143(5) . 3_555 N
O3 O3 5.018(5) . -2_555 N
O3 O3 5.018(5) . -3_555 N
O3 O3 3.859(5) . 107_555 N
O3 O3 3.859(5) . 209_555 N
O3 O4 5.249(6) . 107_555 N
O3 O4 2.602(6) . 111_555 N
O3 O4 2.696(6) . 208_555 N
O3 O4 5.103(5) . 209_555 N
O3 O4 5.120(4) . -304_445 N
O3 O4 5.017(5) . -310_344 N
O3 O4 5.236(5) . -312_434 N
O3 SI 3.5927(24) . 1_555 N
O3 SI' 2.9759(29) . 1_555 N
O3 SII 2.3349(34) . 111_555 N
O3 SJ 3.751(28) . 3_555 N
O3 SJ 4.065(32) . -105_544 N
O3 Oc 4.343(12) . 3_555 N
O3 Oc 4.765(13) . -1_555 N
O3 Oc 5.478(14) . -105_544 N
O3 Oc 5.570(14) . -307_445 N
O3 Dc2 3.839(18) . 3_555 N
O3 Dc2 3.923(14) . -1_555 N
O3 Od 4.04(5) . 3_555 N
O3 Od 5.40(5) . -1_555 N
O3 Od 4.19(5) . -105_544 N
O3 Od 5.52(6) . 304_445 N
O3 Dd2 3.29(8) . 3_555 N
O3 Dd2 3.32(7) . -105_544 N
O3 OII' 5.78(4) . 1_555 N
O3 OII' 4.874(19) . 107_555 N
O3 OII' 3.27(4) . 111_555 N
O3 OII' 4.855(18) . -105_544 N
O3 DII'1 3.978(30) . 107_555 N
O3 DII'1 3.38(8) . 111_555 N
O3 DII'1 2.90(9) . 208_555 N
O3 DII'1 3.97(5) . -304_445 N
O3 DII'2 3.82(7) . -304_445 N
O3 OII* 4.01(7) . 111_555 N
O3 DII*1 3.53(12) . 208_555 N
O3 Of 5.681(32) . 2_555 N
O3 Of 5.292(30) . -1_555 N
O3 Of 5.595(34) . -105_544 N
O3 Of 5.025(34) . -206_454 N
O3 Of 3.727(33) . 304_445 N
O3 Of 5.927(29) . -311_435 N
O3 Df2 3.25(5) . 304_445 N
O3 Oe 5.548(35) . -105_544 N
O3 Oe 5.198(34) . 207_445 N
O3 Oe 4.562(30) . 304_445 N
O3 Oe 4.459(27) . -308_345 N
O3 SIII 4.55(5) . 105_544 N
O3 SIII 4.48(5) . 206_454 N
O3 SIII 4.391(7) . 301_445 N
O4 Si1 1.591(6) . 107_555 N
O4 Si1 3.837(6) . -105_544 N
O4 Si2 1.777(7) . 209_555 N
O4 Si2 3.895(7) . -206_454 N
O4 Si2 4.190(7) . 310_555 N
O4 Si2 4.215(7) . -307_445 N
O4 Al1 1.777(7) . 209_555 N
O4 Al1 3.895(7) . -206_454 N
O4 Al1 4.190(7) . 310_555 N
O4 Al1 4.215(7) . -307_445 N
O4 O1 4.611(9) . 6_555 N
O4 O1 2.571(7) . 107_555 N
O4 O1 4.739(9) . -105_544 N
O4 O1 5.067(6) . -110_544 N
O4 O1 5.150(7) . 312_555 N
O4 O1 2.867(7) . -309_445 N
O4 O2 5.155(5) . 111_555 N
O4 O2 5.247(5) . -102_544 N
O4 O2 5.210(6) . 208_555 N
O4 O2 5.082(5) . -203_454 N
O4 O2 2.882(5) . 310_555 N
O4 O2 2.652(6) . 312_555 N
O4 O3 5.103(5) . 107_555 N
O4 O3 2.696(6) . -105_544 N
O4 O3 5.017(5) . -110_544 N
O4 O3 5.249(6) . 209_555 N
O4 O3 2.602(6) . -206_454 N
O4 O3 5.236(5) . -212_454 N
O4 O3 5.120(4) . -304_445 N
O4 O4 4.976(5) . 2_555 N
O4 O4 4.976(5) . 3_555 N
O4 O4 5.2830(32) . -7_455 N
O4 O4 5.2830(32) . -9_545 N
O4 O4 3.850(6) . -304_445 N
O4 SI' 4.3728(35) . 107_555 N
O4 SI' 4.505(4) . -105_544 N
O4 SII 2.8839(31) . 1_555 N
O4 SJ 4.290(34) . 6_555 N
O4 SJ 1.949(29) . 312_555 N
O4 Oc 3.259(14) . 6_555 N
O4 Oc 5.586(15) . 202_555 N
O4 Oc 3.374(14) . 312_555 N
O4 Oc 5.668(15) . -309_445 N
O4 Dc1 3.344(21) . 312_555 N
O4 Dc2 2.844(18) . 6_555 N
O4 Dc2 2.898(18) . 312_555 N
O4 Od 4.46(6) . 6_555 N
O4 Od 5.95(5) . 107_555 N
O4 Od 4.78(6) . -102_544 N
O4 Od 5.51(5) . 310_555 N
O4 Od 2.32(5) . 312_555 N
O4 Dd1 2.99(6) . 312_555 N
O4 Dd2 1.47(6) . 312_555 N
O4 OII' 4.039(35) . 1_555 N
O4 OII' 5.100(4) . 111_555 N
O4 DII'1 3.55(7) . 1_555 N
O4 OII* 4.08(6) . 1_555 N
O4 DII*1 3.60(14) . 1_555 N
O4 DII*1 3.99(15) . 2_555 N
O4 Of 5.706(33) . 5_555 N
O4 Of 5.998(28) . 6_555 N
O4 Of 4.811(32) . -102_544 N
O4 Of 4.079(29) . -203_454 N
O4 Of 3.261(33) . 310_555 N
O4 Of 3.774(31) . 312_555 N
O4 Df1 3.79(4) . 310_555 N
O4 Df2 3.33(5) . -203_454 N
O4 Df2 2.86(6) . 310_555 N
O4 Oe 2.620(27) . -102_544 N
O4 Oe 4.66(4) . 312_555 N
O4 Oe 4.40(4) . -306_445 N
O4 Oe 5.533(29) . -311_435 N
O4 De1 3.05(4) . -102_544 N
O4 De1 3.57(4) . -306_445 N
O4 De2 2.44(6) . -102_544 N
O4 SIII 2.43(4) . -112_534 N
SI Si1 3.484(6) . 1_555 N
SI Si1 3.484(6) . 2_555 N
SI Si1 3.484(6) . 3_555 N
SI Si1 3.484(6) . -1_555 N
SI Si1 3.484(6) . -2_555 N
SI Si1 3.484(6) . -3_555 N
SI Si2 3.555(6) . 1_555 N
SI Si2 3.555(6) . 2_555 N
SI Si2 3.555(6) . 3_555 N
SI Si2 3.555(6) . -1_555 N
SI Si2 3.555(6) . -2_555 N
SI Si2 3.555(6) . -3_555 N
SI Al1 3.555(6) . 1_555 N
SI Al1 3.555(6) . 2_555 N
SI Al1 3.555(6) . 3_555 N
SI Al1 3.555(6) . -1_555 N
SI Al1 3.555(6) . -2_555 N
SI Al1 3.555(6) . -3_555 N
SI O1 3.7617(31) . 1_555 N
SI O1 3.7617(31) . 2_555 N
SI O1 3.7617(31) . 3_555 N
SI O1 3.7617(31) . -1_555 N
SI O1 3.7617(31) . -2_555 N
SI O1 3.7617(31) . -3_555 N
SI O2 2.7890(33) . 105_544 N
SI O2 2.7890(33) . -105_544 N
SI O2 2.7890(33) . 206_454 N
SI O2 2.7890(33) . -206_454 N
SI O2 2.7890(33) . 304_445 N
SI O2 2.7890(33) . -304_445 N
SI O3 3.5927(24) . 1_555 N
SI O3 3.5927(24) . 2_555 N
SI O3 3.5927(24) . 3_555 N
SI O3 3.5927(24) . -1_555 N
SI O3 3.5927(24) . -2_555 N
SI O3 3.5927(24) . -3_555 N
SI SI' 2.220(9) . 1_555 N
SI SI' 2.220(9) . -1_555 N
SI' Si1 3.198(6) . 1_555 N
SI' Si1 3.198(6) . 2_555 N
SI' Si1 3.198(6) . 3_555 N
SI' Si2 3.287(6) . 1_555 N
SI' Si2 3.287(6) . 2_555 N
SI' Si2 3.287(6) . 3_555 N
SI' Al1 3.287(6) . 1_555 N
SI' Al1 3.287(6) . 2_555 N
SI' Al1 3.287(6) . 3_555 N
SI' O1 4.343(6) . 1_555 N
SI' O1 4.343(6) . 2_555 N
SI' O1 4.343(6) . 3_555 N
SI' O1 4.393(6) . -1_555 N
SI' O1 4.393(6) . -2_555 N
SI' O1 4.393(6) . -3_555 N
SI' O2 4.898(5) . 1_555 N
SI' O2 4.898(5) . 2_555 N
SI' O2 4.898(5) . 3_555 N
SI' O2 4.488(8) . 105_544 N
SI' O2 2.295(4) . -105_544 N
SI' O2 4.488(8) . 206_454 N
SI' O2 2.295(4) . -206_454 N
SI' O2 4.488(8) . 304_445 N
SI' O2 2.295(4) . -304_445 N
SI' O3 2.9759(29) . 1_555 N
SI' O3 2.9759(29) . 2_555 N
SI' O3 2.9759(29) . 3_555 N
SI' O4 4.505(4) . 107_555 N
SI' O4 4.3728(35) . 111_555 N
SI' O4 4.505(4) . 208_555 N
SI' O4 4.3728(35) . 209_555 N
SI' O4 4.3728(35) . 310_555 N
SI' O4 4.505(4) . 312_555 N
SI' SI 2.220(9) . 1_555 N
SI' OII' 4.76(5) . 1_555 N
SI' OII' 3.068(11) . 107_555 N
SI' OII' 3.068(11) . 111_555 N
SI' OII' 3.068(11) . -105_544 N
SI' DII'1 2.37(8) . 107_555 N
SI' DII'1 3.10(10) . 111_555 N
SI' DII'1 3.951(32) . -105_544 N
SI' DII'1 2.37(8) . 208_555 N
SI' DII'1 3.10(10) . 209_555 N
SI' DII'1 3.951(32) . -206_454 N
SI' DII'1 3.10(10) . 310_555 N
SI' DII'1 2.37(8) . 312_555 N
SI' DII'1 3.951(32) . -304_445 N
SI' DII'2 3.86(4) . 1_555 N
SI' DII'2 3.86(4) . 2_555 N
SI' DII'2 3.86(4) . 3_555 N
SI' DII'2 3.24(6) . 107_555 N
SI' DII'2 3.21(8) . 111_555 N
SI' DII'2 2.75(8) . -105_544 N
SI' DII'2 3.24(6) . 208_555 N
SI' DII'2 3.21(8) . 209_555 N
SI' DII'2 2.75(8) . -206_454 N
SI' DII'2 3.21(8) . 310_555 N
SI' DII'2 3.24(6) . 312_555 N
SI' DII'2 2.75(8) . -304_445 N
SII Si1 3.329(6) . 107_555 N
SII Si1 3.329(6) . 208_555 N
SII Si1 3.329(6) . 312_555 N
SII Si2 3.234(6) . 111_555 N
SII Si2 3.234(6) . 209_555 N
SII Si2 3.234(6) . 310_555 N
SII Al1 3.234(6) . 111_555 N
SII Al1 3.234(6) . 209_555 N
SII Al1 3.234(6) . 310_555 N
SII O1 4.400(5) . 107_555 N
SII O1 4.524(4) . -110_544 N
SII O1 4.400(5) . 208_555 N
SII O1 4.524(4) . -211_454 N
SII O1 4.400(5) . 312_555 N
SII O1 4.524(4) . -309_445 N
SII O2 4.332(6) . 107_555 N
SII O2 4.438(6) . 111_555 N
SII O2 4.332(6) . 208_555 N
SII O2 4.438(6) . 209_555 N
SII O2 4.438(6) . 310_555 N
SII O2 4.332(6) . 312_555 N
SII O3 2.3349(34) . -105_544 N
SII O3 2.3349(34) . -206_454 N
SII O3 2.3349(34) . -304_445 N
SII O4 2.8839(31) . 1_555 N
SII O4 2.8839(31) . 2_555 N
SII O4 2.8839(31) . 3_555 N
SII Od 4.11(5) . 107_555 N
SII Od 4.11(5) . 208_555 N
SII Od 4.11(5) . 312_555 N
SII Dd2 3.23(6) . 107_555 N
SII Dd2 3.23(6) . 208_555 N
SII Dd2 3.23(6) . 312_555 N
SII OII' 3.09(5) . 1_555 N
SII DII'1 3.29(7) . 1_555 N
SII DII'1 3.29(7) . 2_555 N
SII DII'1 3.29(7) . 3_555 N
SII OII* 2.64(9) . 1_555 N
SII DII*1 2.73(12) . 1_555 N
SII DII*1 2.73(12) . 2_555 N
SII DII*1 2.73(12) . 3_555 N
SII DII*2 3.59(4) . 1_555 N
SII DII*2 3.59(4) . 2_555 N
SII DII*2 3.59(4) . 3_555 N
SII Of 4.499(31) . -102_544 N
SII Of 4.499(31) . -203_454 N
SII Of 4.499(31) . -301_445 N
SII Oe 4.608(27) . -102_544 N
SII Oe 4.608(27) . -203_454 N
SII Oe 4.608(27) . -301_445 N
SJ Si1 3.081(32) . 111_555 N
SJ Si2 2.723(28) . 3_555 N
SJ Al1 2.723(28) . 3_555 N
SJ O1 2.627(32) . -3_555 N
SJ O1 3.039(33) . 111_555 N
SJ O2 4.289(30) . 1_555 N
SJ O2 4.156(29) . -304_445 N
SJ O3 3.751(28) . 2_555 N
SJ O3 4.065(32) . 208_555 N
SJ O4 4.290(34) . -111_434 N
SJ O4 1.949(29) . 312_555 N
SJ SJ 3.334(29) . 105_544 N
SJ SJ 3.334(29) . -108_544 N
SJ Oc 1.599(35) . 1_555 N
SJ Oc 4.164(35) . 105_544 N
SJ Oc 1.916(31) . -108_544 N
SJ Oc 4.200(31) . -305_444 N
SJ Dc1 1.39(4) . 1_555 N
SJ Dc1 3.244(35) . 105_544 N
SJ Dc1 2.530(33) . -108_544 N
SJ Dc2 1.46(4) . 1_555 N
SJ Dc2 2.03(4) . -108_544 N
SJ Od 0.50(6) . 1_555 N
SJ Od 3.10(7) . 105_544 N
SJ Od 3.32(7) . -108_544 N
SJ Dd1 1.41(6) . 1_555 N
SJ Dd1 3.40(9) . 105_544 N
SJ Dd1 3.31(9) . -108_544 N
SJ Dd2 0.82(7) . 1_555 N
SJ Dd2 3.51(10) . 105_544 N
SJ Dd2 3.98(9) . -108_544 N
SJ OII* 3.92(4) . -105_544 N
SJ DII*1 3.93(18) . -105_544 N
SJ DII*1 3.21(14) . 312_555 N
SJ Of 3.67(4) . 1_555 N
SJ Of 4.38(4) . -2_555 N
SJ Of 4.10(4) . 105_544 N
SJ Of 3.64(4) . -109_543 N
SJ Of 2.62(4) . -304_445 N
SJ Df1 3.93(6) . -2_555 N
SJ Df1 3.35(7) . -109_543 N
SJ Df1 2.68(6) . -304_445 N
SJ Df2 3.01(7) . -109_543 N
SJ Df2 2.12(6) . -304_445 N
SJ Oe 3.38(5) . 1_555 N
SJ Oe 0.84(4) . 105_544 N
SJ Oe 4.85(4) . -201_453 N
SJ Oe 2.65(5) . 308_544 N
SJ De1 1.66(4) . 105_544 N
SJ De1 1.82(5) . 308_544 N
SJ De2 2.99(6) . 1_555 N
SJ De2 0.83(6) . 105_544 N
SJ De2 3.33(5) . 308_544 N
SJ SIII 2.841(30) . 304_445 N
Oc Si1 3.611(14) . -3_555 N
Oc Si2 3.488(14) . 3_555 N
Oc Al1 3.488(14) . 3_555 N
Oc O1 5.199(14) . 1_555 N
Oc O1 5.874(16) . 2_555 N
Oc O1 2.637(13) . -3_555 N
Oc O1 4.561(17) . 111_555 N
Oc O1 4.341(16) . 212_544 N
Oc O2 5.841(16) . 1_555 N
Oc O2 5.601(15) . -2_555 N
Oc O2 4.736(13) . 105_544 N
Oc O2 5.018(14) . -304_445 N
Oc O3 4.343(12) . 2_555 N
Oc O3 4.765(13) . -1_555 N
Oc O3 5.478(14) . 208_555 N
Oc O3 5.570(14) . -209_443 N
Oc O4 5.586(15) . 103_544 N
Oc O4 5.668(15) . -107_443 N
Oc O4 3.259(14) . -111_434 N
Oc O4 3.374(14) . 312_555 N
Oc SJ 1.599(35) . 1_555 N
Oc SJ 1.916(31) . 105_544 N
Oc SJ 4.164(35) . -108_544 N
Oc SJ 4.200(31) . 308_544 N
Oc Oc 2.724(14) . 105_544 N
Oc Oc 2.724(14) . -108_544 N
Oc Oc 5.932(32) . 212_544 N
Oc Oc 5.174(24) . -201_453 N
Oc Oc 4.399(21) . 308_544 N
Oc Oc 4.399(21) . -305_444 N
Oc Dc1 0.960000(10) . 1_555 N
Oc Dc1 1.825(19) . 105_544 N
Oc Dc1 2.934(20) . -108_544 N
Oc Dc1 3.547(20) . 308_544 N
Oc Dc2 0.96077 . 1_555 N
Oc Dc2 2.912(17) . 105_544 N
Oc Dc2 3.213(15) . -108_544 N
Oc Od 1.47(6) . 1_555 N
Oc Od 1.75(5) . 105_544 N
Oc Od 3.99(6) . -108_544 N
Oc Od 5.31(5) . -201_453 N
Oc Od 3.79(5) . 308_544 N
Oc Od 5.22(5) . -305_444 N
Oc Dd1 1.44(8) . 1_555 N
Oc Dd1 2.30(8) . 105_544 N
Oc Dd1 3.81(8) . -108_544 N
Oc Dd1 3.62(9) . 308_544 N
Oc Dd2 2.17(7) . 1_555 N
Oc Dd2 2.35(8) . 105_544 N
Oc OII* 5.576(32) . 101_544 N
Oc OII* 4.183(12) . -105_544 N
Oc OII* 4.999(15) . -111_434 N
Oc DII*1 3.30(8) . 312_555 N
Oc Of 4.679(31) . 1_555 N
Oc Of 2.97(4) . -2_555 N
Oc Of 3.271(32) . 105_544 N
Oc Of 4.520(31) . -109_543 N
Oc Of 5.722(31) . 308_544 N
Oc Of 5.578(35) . 309_544 N
Oc Of 3.156(31) . -304_445 N
Oc Df1 2.55(5) . -2_555 N
Oc Df1 3.81(5) . 105_544 N
Oc Df1 3.92(6) . -109_543 N
Oc Df1 2.95(6) . -304_445 N
Oc Df2 3.07(6) . -2_555 N
Oc Df2 3.92(5) . 105_544 N
Oc Df2 2.49(5) . -304_445 N
Oc Oe 3.890(33) . 1_555 N
Oc Oe 1.66(4) . 105_544 N
Oc Oe 5.029(29) . -108_544 N
Oc Oe 3.41(4) . -201_453 N
Oc Oe 5.996(31) . -206_454 N
Oc Oe 1.21(4) . 308_544 N
Oc Oe 4.897(29) . -305_444 N
Oc De1 2.51(4) . 105_544 N
Oc De1 2.89(5) . -201_453 N
Oc De1 0.26(4) . 308_544 N
Oc De2 3.78(5) . 1_555 N
Oc De2 1.60(5) . 105_544 N
Oc De2 1.75(5) . 308_544 N
Oc SIII 3.32(4) . 102_544 N
Oc SIII 3.999(23) . 304_445 N
Dc1 Si2 3.891(18) . 3_555 N
Dc1 Al1 3.891(18) . 3_555 N
Dc1 O1 3.261(15) . -3_555 N
Dc1 O1 3.968(21) . 111_555 N
Dc1 O4 3.344(21) . 312_555 N
Dc1 SJ 1.39(4) . 1_555 N
Dc1 SJ 2.530(33) . 105_544 N
Dc1 SJ 3.244(35) . -108_544 N
Dc1 Oc 0.96 . 1_555 N
Dc1 Oc 2.934(20) . 105_544 N
Dc1 Oc 1.825(19) . -108_544 N
Dc1 Oc 3.547(20) . -305_444 N
Dc1 Dc1 1.991(18) . 105_544 N
Dc1 Dc1 1.991(18) . -108_544 N
Dc1 Dc1 3.951(34) . -201_453 N
Dc1 Dc1 3.412(30) . 308_544 N
Dc1 Dc1 3.412(30) . -305_444 N
Dc1 Dc2 1.518680(10) . 1_555 N
Dc1 Dc2 3.388(25) . 105_544 N
Dc1 Dc2 2.431(22) . -108_544 N
Dc1 Od 1.12(5) . 1_555 N
Dc1 Od 2.20(6) . 105_544 N
Dc1 Od 3.05(6) . -108_544 N
Dc1 Od 3.94(6) . 308_544 N
Dc1 Dd1 1.29(8) . 1_555 N
Dc1 Dd1 2.38(9) . 105_544 N
Dc1 Dd1 2.86(8) . -108_544 N
Dc1 Dd1 3.72(9) . 308_544 N
Dc1 Dd2 2.07(5) . 1_555 N
Dc1 Dd2 2.92(8) . 105_544 N
Dc1 Dd2 3.91(6) . -108_544 N
Dc1 DII*1 3.62(12) . 312_555 N
Dc1 Of 3.78(4) . -2_555 N
Dc1 Of 3.942(33) . -109_543 N
Dc1 Of 2.96(4) . -304_445 N
Dc1 Df1 3.22(5) . -2_555 N
Dc1 Df1 3.38(6) . -109_543 N
Dc1 Df1 2.57(6) . -304_445 N
Dc1 Df2 3.83(6) . -2_555 N
Dc1 Df2 3.50(6) . -109_543 N
Dc1 Df2 2.55(6) . -304_445 N
Dc1 Oe 2.957(33) . 1_555 N
Dc1 Oe 0.97(4) . 105_544 N
Dc1 Oe 3.52(4) . -201_453 N
Dc1 Oe 1.71(4) . 308_544 N
Dc1 De1 3.44(5) . 1_555 N
Dc1 De1 1.64(5) . 105_544 N
Dc1 De1 3.09(5) . -201_453 N
Dc1 De1 1.11(5) . 308_544 N
Dc1 De2 2.92(5) . 1_555 N
Dc1 De2 1.25(5) . 105_544 N
Dc1 De2 2.44(4) . 308_544 N
Dc1 SIII 3.774(33) . 304_445 N
Dc2 Si1 2.882(16) . -3_555 N
Dc2 Si2 2.754(16) . 3_555 N
Dc2 Al1 2.754(16) . 3_555 N
Dc2 O1 1.773(13) . -3_555 N
Dc2 O3 3.839(18) . 2_555 N
Dc2 O3 3.923(14) . -1_555 N
Dc2 O4 2.844(18) . -111_434 N
Dc2 O4 2.898(18) . 312_555 N
Dc2 SJ 1.46(4) . 1_555 N
Dc2 SJ 2.03(4) . 105_544 N
Dc2 Oc 0.960770(10) . 1_555 N
Dc2 Oc 3.213(15) . 105_544 N
Dc2 Oc 2.912(17) . -108_544 N
Dc2 Dc1 1.518680(10) . 1_555 N
Dc2 Dc1 2.431(22) . 105_544 N
Dc2 Dc1 3.388(25) . -108_544 N
Dc2 Dc2 3.344(13) . 105_544 N
Dc2 Dc2 3.344(13) . -108_544 N
Dc2 Od 1.64(6) . 1_555 N
Dc2 Od 1.90(6) . 105_544 N
Dc2 Dd1 2.04(7) . 1_555 N
Dc2 Dd1 2.43(8) . 105_544 N
Dc2 Dd2 2.07(9) . 1_555 N
Dc2 Dd2 2.12(10) . 105_544 N
Dc2 DII*1 3.67(8) . 312_555 N
Dc2 Of 3.44(4) . -2_555 N
Dc2 Of 3.47(4) . 105_544 N
Dc2 Of 2.47(4) . -304_445 N
Dc2 Df1 3.24(6) . -2_555 N
Dc2 Df1 2.52(6) . -304_445 N
Dc2 Df2 3.50(6) . -2_555 N
Dc2 Df2 3.92(6) . 105_544 N
Dc2 Df2 1.65(5) . -304_445 N
Dc2 Oe 1.86(4) . 105_544 N
Dc2 Oe 1.56(4) . 308_544 N
Dc2 De1 2.68(4) . 105_544 N
Dc2 De1 3.43(4) . -201_453 N
Dc2 De1 0.97(6) . 308_544 N
Dc2 De2 1.29(5) . 105_544 N
Dc2 De2 2.18(4) . 308_544 N
Dc2 SIII 3.338(29) . 102_544 N
Dc2 SIII 3.274(25) . 304_445 N
Od Si1 3.33(6) . 111_555 N
Od Si2 3.14(5) . 3_555 N
Od Al1 3.14(5) . 3_555 N
Od O1 5.62(5) . 1_555 N
Od O1 5.80(5) . 2_555 N
Od O1 5.88(6) . 4_555 N
Od O1 3.00(5) . -3_555 N
Od O1 5.96(5) . -12_554 N
Od O1 3.12(6) . 111_555 N
Od O1 5.84(6) . -108_544 N
Od O1 5.81(6) . 212_544 N
Od O2 4.63(6) . 1_555 N
Od O2 5.48(6) . 105_544 N
Od O2 5.73(6) . -109_543 N
Od O2 4.64(5) . -304_445 N
Od O3 4.04(5) . 2_555 N
Od O3 5.52(6) . 4_555 N
Od O3 5.40(5) . -1_555 N
Od O3 4.19(5) . 208_555 N
Od O4 4.46(6) . -111_434 N
Od O4 5.95(5) . 209_555 N
Od O4 5.51(5) . 310_555 N
Od O4 2.32(5) . 312_555 N
Od O4 4.78(6) . -303_445 N
Od SII 4.11(5) . -105_544 N
Od SJ 0.50(6) . 1_555 N
Od SJ 3.32(7) . 105_544 N
Od SJ 3.10(7) . -108_544 N
Od Oc 1.47(6) . 1_555 N
Od Oc 3.99(6) . 105_544 N
Od Oc 1.75(5) . -108_544 N
Od Oc 5.31(5) . -201_453 N
Od Oc 5.22(5) . 308_544 N
Od Oc 3.79(5) . -305_444 N
Od Dc1 1.12(5) . 1_555 N
Od Dc1 3.05(6) . 105_544 N
Od Dc1 2.20(6) . -108_544 N
Od Dc1 3.94(6) . -305_444 N
Od Dc2 1.64(6) . 1_555 N
Od Dc2 1.90(6) . -108_544 N
Od Od 3.08(6) . 105_544 N
Od Od 3.08(6) . -108_544 N
Od Od 5.82(10) . -201_453 N
Od Od 4.94(9) . 308_544 N
Od Od 4.94(9) . -305_444 N
Od Dd1 0.960000(10) . 1_555 N
Od Dd1 3.37(9) . 105_544 N
Od Dd1 3.14(10) . -108_544 N
Od Dd2 0.960750(20) . 1_555 N
Od Dd2 3.60(10) . 105_544 N
Od Dd2 3.81(7) . -108_544 N
Od OII* 3.70(5) . -105_544 N
Od OII* 5.70(5) . -111_434 N
Od OII* 5.81(5) . -301_445 N
Od DII*1 3.68(19) . -105_544 N
Od DII*1 3.00(15) . 312_555 N
Od DII*2 4.00(19) . -105_544 N
Od DII*2 3.87(13) . 209_555 N
Od Of 3.99(6) . 1_555 N
Od Of 4.22(7) . -2_555 N
Od Of 4.04(6) . 105_544 N
Od Of 5.08(6) . -108_544 N
Od Of 3.33(6) . -109_543 N
Od Of 2.98(6) . -304_445 N
Od Df1 3.68(8) . -2_555 N
Od Df1 2.94(8) . -109_543 N
Od Df1 2.90(7) . -304_445 N
Od Df2 2.78(8) . -109_543 N
Od Df2 2.52(7) . -304_445 N
Od Oe 3.07(6) . 1_555 N
Od Oe 0.58(6) . 105_544 N
Od Oe 4.87(6) . -108_544 N
Od Oe 4.57(6) . -201_453 N
Od Oe 2.58(6) . 308_544 N
Od Oe 5.48(6) . -305_444 N
Od De1 3.64(7) . 1_555 N
Od De1 1.51(6) . 105_544 N
Od De1 1.71(7) . 308_544 N
Od De2 2.68(7) . 1_555 N
Od De2 1.08(6) . 105_544 N
Od De2 3.22(7) . 308_544 N
Od SIII 4.67(6) . 8_554 N
Od SIII 4.48(7) . 102_544 N
Od SIII 3.29(5) . 304_445 N
Dd1 Si1 3.99(6) . 111_555 N
Dd1 Si2 3.68(7) . 3_555 N
Dd1 Al1 3.68(7) . 3_555 N
Dd1 O1 3.46(8) . -3_555 N
Dd1 O1 3.73(7) . 111_555 N
Dd1 O4 2.99(6) . 312_555 N
Dd1 SJ 1.41(6) . 1_555 N
Dd1 SJ 3.31(9) . 105_544 N
Dd1 SJ 3.40(9) . -108_544 N
Dd1 Oc 1.44(8) . 1_555 N
Dd1 Oc 3.81(8) . 105_544 N
Dd1 Oc 2.30(8) . -108_544 N
Dd1 Oc 3.62(9) . -305_444 N
Dd1 Dc1 1.29(8) . 1_555 N
Dd1 Dc1 2.86(8) . 105_544 N
Dd1 Dc1 2.38(9) . -108_544 N
Dd1 Dc1 3.72(9) . -305_444 N
Dd1 Dc2 2.04(7) . 1_555 N
Dd1 Dc2 2.43(8) . -108_544 N
Dd1 Od 0.960000(10) . 1_555 N
Dd1 Od 3.14(10) . 105_544 N
Dd1 Od 3.37(9) . -108_544 N
Dd1 Dd1 3.54(13) . 105_544 N
Dd1 Dd1 3.54(13) . -108_544 N
Dd1 Dd1 3.99(13) . 308_544 N
Dd1 Dd1 3.99(13) . -305_444 N
Dd1 Dd2 1.51864 . 1_555 N
Dd1 Dd2 3.79(12) . 105_544 N
Dd1 OII* 3.10(8) . -105_544 N
Dd1 DII*1 3.17(20) . -105_544 N
Dd1 DII*1 3.99(10) . 209_555 N
Dd1 DII*1 2.39(16) . 312_555 N
Dd1 DII*2 3.22(21) . -105_544 N
Dd1 DII*2 3.09(14) . 209_555 N
Dd1 DII*2 3.36(18) . 312_555 N
Dd1 Of 3.66(9) . -2_555 N
Dd1 Of 3.55(9) . 105_544 N
Dd1 Of 3.15(9) . -109_543 N
Dd1 Of 3.85(6) . -304_445 N
Dd1 Df1 2.99(9) . -2_555 N
Dd1 Df1 3.82(9) . 105_544 N
Dd1 Df1 2.54(10) . -109_543 N
Dd1 Df1 3.68(8) . -304_445 N
Dd1 Df2 2.88(10) . -109_543 N
Dd1 Df2 3.31(8) . -304_445 N
Dd1 Oe 3.18(9) . 1_555 N
Dd1 Oe 1.29(7) . 105_544 N
Dd1 Oe 2.56(9) . 308_544 N
Dd1 De1 3.52(10) . 1_555 N
Dd1 De1 2.11(8) . 105_544 N
Dd1 De1 3.93(9) . -201_453 N
Dd1 De1 1.68(9) . 308_544 N
Dd1 De2 2.80(10) . 1_555 N
Dd1 De2 1.94(7) . 105_544 N
Dd1 De2 2.97(9) . 308_544 N
Dd2 Si1 2.58(8) . 111_555 N
Dd2 Si2 2.51(9) . 3_555 N
Dd2 Al1 2.51(9) . 3_555 N
Dd2 O1 2.87(10) . -3_555 N
Dd2 O1 2.75(10) . 111_555 N
Dd2 O2 3.92(7) . 1_555 N
Dd2 O3 3.29(8) . 2_555 N
Dd2 O3 3.32(7) . 208_555 N
Dd2 O4 1.47(6) . 312_555 N
Dd2 SII 3.23(6) . -105_544 N
Dd2 SJ 0.82(7) . 1_555 N
Dd2 SJ 3.98(9) . 105_544 N
Dd2 SJ 3.51(10) . -108_544 N
Dd2 Oc 2.17(7) . 1_555 N
Dd2 Oc 2.35(8) . -108_544 N
Dd2 Dc1 2.07(5) . 1_555 N
Dd2 Dc1 3.91(6) . 105_544 N
Dd2 Dc1 2.92(8) . -108_544 N
Dd2 Dc2 2.07(9) . 1_555 N
Dd2 Dc2 2.12(10) . -108_544 N
Dd2 Od 0.960750(20) . 1_555 N
Dd2 Od 3.81(7) . 105_544 N
Dd2 Od 3.60(10) . -108_544 N
Dd2 Dd1 1.518640(10) . 1_555 N
Dd2 Dd1 3.79(12) . -108_544 N
Dd2 OII* 3.32(9) . -105_544 N
Dd2 DII*1 3.27(19) . -105_544 N
Dd2 DII*1 2.70(17) . 312_555 N
Dd2 DII*2 3.83(18) . -105_544 N
Dd2 DII*2 3.71(14) . 209_555 N
Dd2 DII*2 3.93(16) . 312_555 N
Dd2 Of 3.27(10) . -109_543 N
Dd2 Of 3.24(9) . -304_445 N
Dd2 Df1 3.09(11) . -109_543 N
Dd2 Df1 3.42(9) . -304_445 N
Dd2 Df2 2.66(12) . -109_543 N
Dd2 Df2 2.73(10) . -304_445 N
Dd2 Oe 3.65(9) . 1_555 N
Dd2 Oe 1.41(7) . 105_544 N
Dd2 Oe 3.32(8) . 308_544 N
Dd2 De1 2.11(9) . 105_544 N
Dd2 De1 2.41(8) . 308_544 N
Dd2 De2 3.05(11) . 1_555 N
Dd2 De2 1.63(9) . 105_544 N
Dd2 De2 3.88(9) . 308_544 N
Dd2 SIII 3.09(9) . 304_445 N
OII' Si1 3.942(29) . 107_555 N
OII' Si1 3.942(29) . 208_555 N
OII' Si1 3.942(29) . 312_555 N
OII' Si2 3.975(31) . 111_555 N
OII' Si2 3.975(31) . 209_555 N
OII' Si2 3.975(31) . 310_555 N
OII' Al1 3.975(31) . 111_555 N
OII' Al1 3.975(31) . 209_555 N
OII' Al1 3.975(31) . 310_555 N
OII' O1 5.518(30) . 107_555 N
OII' O1 5.616(30) . -110_544 N
OII' O1 5.518(30) . 208_555 N
OII' O1 5.616(30) . -211_454 N
OII' O1 5.518(30) . 312_555 N
OII' O1 5.616(30) . -309_445 N
OII' O2 4.911(24) . 1_555 N
OII' O2 4.911(24) . 2_555 N
OII' O2 4.911(24) . 3_555 N
OII' O2 3.771(11) . 107_555 N
OII' O2 3.812(10) . 111_555 N
OII' O2 5.75(5) . -105_544 N
OII' O2 3.771(11) . 208_555 N
OII' O2 3.812(10) . 209_555 N
OII' O2 5.75(5) . -206_454 N
OII' O2 3.812(10) . 310_555 N
OII' O2 3.771(11) . 312_555 N
OII' O2 5.75(5) . -304_445 N
OII' O3 5.78(4) . 1_555 N
OII' O3 5.78(4) . 2_555 N
OII' O3 5.78(4) . 3_555 N
OII' O3 4.855(18) . 107_555 N
OII' O3 4.874(19) . 111_555 N
OII' O3 3.27(4) . -105_544 N
OII' O3 4.855(18) . 208_555 N
OII' O3 4.874(19) . 209_555 N
OII' O3 3.27(4) . -206_454 N
OII' O3 4.874(19) . 310_555 N
OII' O3 4.855(18) . 312_555 N
OII' O3 3.27(4) . -304_445 N
OII' O4 4.039(35) . 1_555 N
OII' O4 4.039(35) . 2_555 N
OII' O4 4.039(35) . 3_555 N
OII' O4 5.100(4) . -105_544 N
OII' O4 5.100(4) . -206_454 N
OII' O4 5.100(4) . -304_445 N
OII' SI' 4.76(5) . 1_555 N
OII' SI' 3.068(11) . 107_555 N
OII' SI' 3.068(11) . 111_555 N
OII' SI' 3.068(11) . -105_544 N
OII' SII 3.09(5) . 1_555 N
OII' OII' 2.52(8) . 107_555 N
OII' OII' 2.52(8) . 111_555 N
OII' OII' 2.52(8) . -105_544 N
OII' DII'1 0.9600(19) . 1_555 N
OII' DII'1 0.9600(19) . 2_555 N
OII' DII'1 0.9600(19) . 3_555 N
OII' DII'1 3.05(8) . 107_555 N
OII' DII'1 2.72(8) . 111_555 N
OII' DII'1 2.12(9) . -105_544 N
OII' DII'1 3.05(8) . 208_555 N
OII' DII'1 2.72(8) . 209_555 N
OII' DII'1 2.12(9) . -206_454 N
OII' DII'1 2.72(8) . 310_555 N
OII' DII'1 3.05(8) . 312_555 N
OII' DII'1 2.12(9) . -304_445 N
OII' DII'2 0.961(31) . 1_555 N
OII' DII'2 0.961(31) . 2_555 N
OII' DII'2 0.961(31) . 3_555 N
OII' DII'2 1.74(7) . 107_555 N
OII' DII'2 1.77(8) . 111_555 N
OII' DII'2 2.11(10) . -105_544 N
OII' DII'2 1.74(7) . 208_555 N
OII' DII'2 1.77(8) . 209_555 N
OII' DII'2 2.11(10) . -206_454 N
OII' DII'2 1.77(8) . 310_555 N
OII' DII'2 1.74(7) . 312_555 N
OII' DII'2 2.11(10) . -304_445 N
OII' OII* 5.73(10) . 1_555 N
DII'1 Si1 3.61(8) . 107_555 N
DII'1 Si1 3.847(10) . -105_544 N
DII'1 Si1 3.78(10) . 312_555 N
DII'1 Si2 3.31(6) . 209_555 N
DII'1 Al1 3.31(6) . 209_555 N
DII'1 O2 3.54(11) . 208_555 N
DII'1 O2 2.895(29) . 310_555 N
DII'1 O2 3.31(9) . 312_555 N
DII'1 O3 2.90(9) . -105_544 N
DII'1 O3 3.978(30) . 209_555 N
DII'1 O3 3.38(8) . -206_454 N
DII'1 O3 3.97(5) . -304_445 N
DII'1 O4 3.55(7) . 1_555 N
DII'1 SI' 3.10(10) . 107_555 N
DII'1 SI' 3.951(32) . 111_555 N
DII'1 SI' 2.37(8) . -105_544 N
DII'1 SII 3.29(7) . 1_555 N
DII'1 OII' 0.9600(19) . 1_555 N
DII'1 OII' 2.72(8) . 107_555 N
DII'1 OII' 2.12(9) . 111_555 N
DII'1 OII' 3.05(8) . -105_544 N
DII'1 DII'1 1.660(7) . 2_555 N
DII'1 DII'1 1.660(7) . 3_555 N
DII'1 DII'1 3.01(13) . 107_555 N
DII'1 DII'1 2.22(13) . 111_555 N
DII'1 DII'1 2.89(13) . -105_544 N
DII'1 DII'1 2.89(13) . 208_555 N
DII'1 DII'1 3.01(13) . 209_555 N
DII'1 DII'1 2.22(13) . -206_454 N
DII'1 DII'1 3.19(12) . 310_555 N
DII'1 DII'1 3.51(13) . 312_555 N
DII'1 DII'1 1.61(19) . -304_445 N
DII'1 DII'2 1.518660(10) . 1_555 N
DII'1 DII'2 1.13(12) . 2_555 N
DII'1 DII'2 1.28(8) . 3_555 N
DII'1 DII'2 2.10(9) . 107_555 N
DII'1 DII'2 1.72(13) . 111_555 N
DII'1 DII'2 2.43(4) . -105_544 N
DII'1 DII'2 1.56(12) . 208_555 N
DII'1 DII'2 2.28(6) . 209_555 N
DII'1 DII'2 2.300(26) . -206_454 N
DII'1 DII'2 1.87(10) . 310_555 N
DII'1 DII'2 2.12(7) . 312_555 N
DII'1 DII'2 2.06(4) . -304_445 N
DII'2 O2 3.82(7) . 107_555 N
DII'2 O2 3.85(9) . 209_555 N
DII'2 O3 3.82(7) . -304_445 N
DII'2 SI' 3.86(4) . 1_555 N
DII'2 SI' 3.21(8) . 107_555 N
DII'2 SI' 2.75(8) . 111_555 N
DII'2 SI' 3.24(6) . -105_544 N
DII'2 OII' 0.961(31) . 1_555 N
DII'2 OII' 1.77(8) . 107_555 N
DII'2 OII' 2.11(10) . 111_555 N
DII'2 OII' 1.74(7) . -105_544 N
DII'2 DII'1 1.51866 . 1_555 N
DII'2 DII'1 1.28(8) . 2_555 N
DII'2 DII'1 1.13(12) . 3_555 N
DII'2 DII'1 2.28(6) . 107_555 N
DII'2 DII'1 2.300(26) . 111_555 N
DII'2 DII'1 1.56(12) . -105_544 N
DII'2 DII'1 2.43(4) . 208_555 N
DII'2 DII'1 2.10(9) . 209_555 N
DII'2 DII'1 1.72(13) . -206_454 N
DII'2 DII'1 1.87(10) . 310_555 N
DII'2 DII'1 2.12(7) . 312_555 N
DII'2 DII'1 2.06(4) . -304_445 N
DII'2 DII'2 0.54(13) . 2_555 N
DII'2 DII'2 0.54(13) . 3_555 N
DII'2 DII'2 0.860(29) . 107_555 N
DII'2 DII'2 1.22(11) . 111_555 N
DII'2 DII'2 1.22(11) . -105_544 N
DII'2 DII'2 1.22(11) . 208_555 N
DII'2 DII'2 0.860(29) . 209_555 N
DII'2 DII'2 1.22(11) . -206_454 N
DII'2 DII'2 1.04(11) . 310_555 N
DII'2 DII'2 0.99(14) . 312_555 N
DII'2 DII'2 1.40(14) . -304_445 N
OII* O1 5.00(4) . 107_555 N
OII* O1 5.11(4) . -110_544 N
OII* O1 5.00(4) . 208_555 N
OII* O1 5.11(4) . -211_454 N
OII* O1 5.00(4) . 312_555 N
OII* O1 5.11(4) . -309_445 N
OII* O3 4.01(7) . -105_544 N
OII* O3 4.01(7) . -206_454 N
OII* O3 4.01(7) . -304_445 N
OII* O4 4.08(6) . 1_555 N
OII* O4 4.08(6) . 2_555 N
OII* O4 4.08(6) . 3_555 N
OII* SII 2.64(9) . 1_555 N
OII* SJ 3.92(4) . 107_555 N
OII* SJ 3.92(4) . 208_555 N
OII* SJ 3.92(4) . 312_555 N
OII* Oc 4.999(15) . 4_555 N
OII* Oc 4.999(15) . 5_555 N
OII* Oc 4.999(15) . 6_555 N
OII* Oc 5.576(32) . 101_555 N
OII* Oc 4.183(12) . 107_555 N
OII* Oc 5.576(32) . 202_555 N
OII* Oc 4.183(12) . 208_555 N
OII* Oc 5.576(32) . 303_555 N
OII* Oc 4.183(12) . 312_555 N
OII* Od 5.70(5) . 4_555 N
OII* Od 5.70(5) . 5_555 N
OII* Od 5.70(5) . 6_555 N
OII* Od 3.70(5) . 107_555 N
OII* Od 5.81(5) . -102_544 N
OII* Od 3.70(5) . 208_555 N
OII* Od 5.81(5) . -203_454 N
OII* Od 3.70(5) . 312_555 N
OII* Od 5.81(5) . -301_445 N
OII* Dd1 3.10(8) . 107_555 N
OII* Dd1 3.10(8) . 208_555 N
OII* Dd1 3.10(8) . 312_555 N
OII* Dd2 3.32(9) . 107_555 N
OII* Dd2 3.32(9) . 208_555 N
OII* Dd2 3.32(9) . 312_555 N
OII* OII' 5.73(10) . 1_555 N
OII* OII* 5.87(14) . -4_555 N
OII* OII* 5.87(14) . -5_555 N
OII* OII* 5.87(14) . -6_555 N
OII* DII*1 0.960(5) . 1_555 N
OII* DII*1 0.960(5) . 2_555 N
OII* DII*1 0.960(5) . 3_555 N
OII* DII*2 0.96(6) . 1_555 N
OII* DII*2 0.96(6) . 2_555 N
OII* DII*2 0.96(6) . 3_555 N
OII* Of 4.71(4) . 4_555 N
OII* Of 4.71(4) . 5_555 N
OII* Of 4.71(4) . 6_555 N
OII* Of 3.558(31) . -102_544 N
OII* Of 3.558(31) . -203_454 N
OII* Of 3.558(31) . -301_445 N
OII* Df1 3.23(5) . -102_544 N
OII* Df1 3.23(5) . -203_454 N
OII* Df1 3.23(5) . -301_445 N
OII* Df2 3.81(6) . -102_544 N
OII* Df2 3.81(6) . -203_454 N
OII* Df2 3.81(6) . -301_445 N
OII* Oe 5.460(31) . 107_555 N
OII* Oe 4.169(30) . -102_544 N
OII* Oe 5.253(32) . -104_544 N
OII* Oe 5.460(31) . 208_555 N
OII* Oe 4.169(30) . -203_454 N
OII* Oe 5.253(32) . -205_454 N
OII* Oe 5.460(31) . 312_555 N
OII* Oe 4.169(30) . -301_445 N
OII* Oe 5.253(32) . -306_445 N
DII*1 Si2 3.93(10) . 209_555 N
DII*1 Al1 3.93(10) . 209_555 N
DII*1 O3 3.53(12) . -105_544 N
DII*1 O4 3.60(14) . 1_555 N
DII*1 O4 3.99(15) . 3_555 N
DII*1 SII 2.73(12) . 1_555 N
DII*1 SJ 3.93(18) . 208_555 N
DII*1 SJ 3.21(14) . 312_555 N
DII*1 Oc 3.30(8) . 312_555 N
DII*1 Dc1 3.62(12) . 312_555 N
DII*1 Dc2 3.67(8) . 312_555 N
DII*1 Od 3.68(19) . 208_555 N
DII*1 Od 3.00(15) . 312_555 N
DII*1 Dd1 3.99(10) . 107_555 N
DII*1 Dd1 3.17(20) . 208_555 N
DII*1 Dd1 2.39(16) . 312_555 N
DII*1 Dd2 3.27(19) . 208_555 N
DII*1 Dd2 2.70(17) . 312_555 N
DII*1 OII* 0.960(5) . 1_555 N
DII*1 DII*1 1.656(20) . 2_555 N
DII*1 DII*1 1.656(20) . 3_555 N
DII*1 DII*2 1.518670(20) . 1_555 N
DII*1 DII*2 1.35(22) . 2_555 N
DII*1 DII*2 1.37(16) . 3_555 N
DII*1 Of 3.88(9) . 5_555 N
DII*1 Of 2.77(12) . -102_544 N
DII*1 Of 3.71(18) . -203_454 N
DII*1 Df1 3.37(9) . 5_555 N
DII*1 Df1 2.61(16) . -102_544 N
DII*1 Df1 3.25(18) . -203_454 N
DII*1 Df2 3.11(15) . -102_544 N
DII*1 Df2 3.79(19) . -203_454 N
DII*1 Oe 3.51(15) . -102_544 N
DII*1 De1 3.49(9) . -306_445 N
DII*1 De2 3.97(14) . -102_544 N
DII*2 SII 3.59(4) . 1_555 N
DII*2 Od 3.87(13) . 107_555 N
DII*2 Od 4.00(19) . 208_555 N
DII*2 Dd1 3.09(14) . 107_555 N
DII*2 Dd1 3.22(21) . 208_555 N
DII*2 Dd1 3.36(18) . 312_555 N
DII*2 Dd2 3.71(14) . 107_555 N
DII*2 Dd2 3.83(18) . 208_555 N
DII*2 Dd2 3.93(16) . 312_555 N
DII*2 OII* 0.96(6) . 1_555 N
DII*2 DII*1 1.518670(20) . 1_555 N
DII*2 DII*1 1.37(16) . 2_555 N
DII*2 DII*1 1.35(22) . 3_555 N
DII*2 DII*2 0.28(24) . 2_555 N
DII*2 DII*2 0.28(24) . 3_555 N
DII*2 Of 3.78(12) . -102_544 N
DII*2 Of 3.67(20) . -203_454 N
DII*2 Of 3.51(18) . -301_445 N
DII*2 Df1 3.77(20) . 4_555 N
DII*2 Df1 3.83(18) . 6_555 N
DII*2 Df1 3.26(14) . -102_544 N
DII*2 Df1 3.20(21) . -203_454 N
DII*2 Df1 2.99(17) . -301_445 N
DII*2 Df2 3.93(16) . -301_445 N
Of Si1 4.105(32) . 2_555 N
Of Si1 3.842(34) . 111_555 N
Of Si1 3.819(32) . -108_544 N
Of Si2 3.454(35) . 208_555 N
Of Si2 4.084(34) . -211_454 N
Of Al1 3.454(35) . 208_555 N
Of Al1 4.084(34) . -211_454 N
Of O1 4.096(32) . 2_555 N
Of O1 4.524(28) . -3_555 N
Of O1 3.540(34) . 111_555 N
Of O1 2.874(33) . -108_544 N
Of O2 3.85(4) . 1_555 N
Of O2 5.712(35) . -109_543 N
Of O2 5.234(33) . -207_453 N
Of O2 4.524(31) . -304_445 N
Of O3 5.681(32) . 3_555 N
Of O3 3.727(33) . 4_555 N
Of O3 5.292(30) . -1_555 N
Of O3 5.927(29) . 106_554 N
Of O3 5.025(34) . 111_555 N
Of O3 5.595(34) . 208_555 N
Of O4 5.998(28) . -111_434 N
Of O4 5.706(33) . -208_344 N
Of O4 3.261(33) . 310_555 N
Of O4 3.774(31) . 312_555 N
Of O4 4.079(29) . -302_445 N
Of O4 4.811(32) . -303_445 N
Of SII 4.499(31) . -301_445 N
Of SJ 3.67(4) . 1_555 N
Of SJ 4.38(4) . -3_555 N
Of SJ 4.10(4) . -108_544 N
Of SJ 3.64(4) . -207_453 N
Of SJ 2.62(4) . -304_445 N
Of Oc 4.679(31) . 1_555 N
Of Oc 2.97(4) . -3_555 N
Of Oc 3.271(32) . -108_544 N
Of Oc 4.520(31) . -207_453 N
Of Oc 5.578(35) . 307_454 N
Of Oc 3.156(31) . -304_445 N
Of Oc 5.722(31) . -305_444 N
Of Dc1 3.78(4) . -3_555 N
Of Dc1 3.942(33) . -207_453 N
Of Dc1 2.96(4) . -304_445 N
Of Dc2 3.44(4) . -3_555 N
Of Dc2 3.47(4) . -108_544 N
Of Dc2 2.47(4) . -304_445 N
Of Od 3.99(6) . 1_555 N
Of Od 4.22(7) . -3_555 N
Of Od 5.08(6) . 105_544 N
Of Od 4.04(6) . -108_544 N
Of Od 3.33(6) . -207_453 N
Of Od 2.98(6) . -304_445 N
Of Dd1 3.66(9) . -3_555 N
Of Dd1 3.55(9) . -108_544 N
Of Dd1 3.15(9) . -207_453 N
Of Dd1 3.85(6) . -304_445 N
Of Dd2 3.27(10) . -207_453 N
Of Dd2 3.24(9) . -304_445 N
Of OII* 4.71(4) . -111_434 N
Of OII* 3.558(31) . -301_445 N
Of DII*1 3.88(9) . -208_344 N
Of DII*1 3.71(18) . -302_445 N
Of DII*1 2.77(12) . -303_445 N
Of DII*2 3.51(18) . -301_445 N
Of DII*2 3.67(20) . -302_445 N
Of DII*2 3.78(12) . -303_445 N
Of Of 5.86(4) . -109_543 N
Of Of 5.79(5) . 206_454 N
Of Of 5.86(4) . -207_453 N
Of Of 5.79(5) . -211_454 N
Of Of 1.92(6) . -304_445 N
Of Df1 0.959990(10) . 1_555 N
Of Df1 2.20(6) . -304_445 N
Of Df2 0.96074 . 1_555 N
Of Df2 2.78(6) . -304_445 N
Of Oe 4.54(4) . 1_555 N
Of Oe 3.31(4) . 103_554 N
Of Oe 3.68(4) . 105_544 N
Of Oe 5.56(4) . 204_454 N
Of Oe 2.78(4) . -207_453 N
Of Oe 5.00(4) . 308_544 N
Of Oe 4.53(5) . -304_445 N
Of De1 3.17(7) . 103_554 N
Of De1 3.26(6) . 105_544 N
Of De1 2.84(6) . -207_453 N
Of De2 3.15(6) . 105_544 N
Of De2 1.92(5) . -207_453 N
Of SIII 1.63(6) . 304_445 N
Df1 O1 3.42(4) . -108_544 N
Df1 O4 3.79(4) . 310_555 N
Df1 SJ 3.93(6) . -3_555 N
Df1 SJ 3.35(7) . -207_453 N
Df1 SJ 2.68(6) . -304_445 N
Df1 Oc 2.55(5) . -3_555 N
Df1 Oc 3.81(5) . -108_544 N
Df1 Oc 3.92(6) . -207_453 N
Df1 Oc 2.95(6) . -304_445 N
Df1 Dc1 3.22(5) . -3_555 N
Df1 Dc1 3.38(6) . -207_453 N
Df1 Dc1 2.57(6) . -304_445 N
Df1 Dc2 3.24(6) . -3_555 N
Df1 Dc2 2.52(6) . -304_445 N
Df1 Od 3.68(8) . -3_555 N
Df1 Od 2.94(8) . -207_453 N
Df1 Od 2.90(7) . -304_445 N
Df1 Dd1 2.99(9) . -3_555 N
Df1 Dd1 3.82(9) . -108_544 N
Df1 Dd1 2.54(10) . -207_453 N
Df1 Dd1 3.68(8) . -304_445 N
Df1 Dd2 3.09(11) . -207_453 N
Df1 Dd2 3.42(9) . -304_445 N
Df1 OII* 3.23(5) . -301_445 N
Df1 DII*1 3.37(9) . -208_344 N
Df1 DII*1 3.25(18) . -302_445 N
Df1 DII*1 2.61(16) . -303_445 N
Df1 DII*2 3.83(18) . -111_434 N
Df1 DII*2 3.77(20) . 304_445 N
Df1 DII*2 2.99(17) . -301_445 N
Df1 DII*2 3.20(21) . -302_445 N
Df1 DII*2 3.26(14) . -303_445 N
Df1 Of 0.95999 . 1_555 N
Df1 Of 2.20(6) . -304_445 N
Df1 Df1 2.29(11) . -304_445 N
Df1 Df2 1.518650(10) . 1_555 N
Df1 Df2 3.16(6) . -304_445 N
Df1 Oe 2.94(7) . 103_554 N
Df1 Oe 2.57(6) . -207_453 N
Df1 Oe 3.96(6) . -304_445 N
Df1 De1 2.94(8) . 103_554 N
Df1 De1 3.82(7) . 105_544 N
Df1 De1 2.48(8) . -207_453 N
Df1 De2 3.88(7) . 103_554 N
Df1 De2 3.69(7) . 105_544 N
Df1 De2 1.86(7) . -207_453 N
Df1 SIII 2.41(7) . 304_445 N
Df2 Si1 3.77(6) . 111_555 N
Df2 Si1 3.00(4) . -108_544 N
Df2 Si2 2.74(5) . 208_555 N
Df2 Si2 3.90(5) . -211_454 N
Df2 Al1 2.74(5) . 208_555 N
Df2 Al1 3.90(5) . -211_454 N
Df2 O1 3.56(6) . 111_555 N
Df2 O1 1.949(32) . -108_544 N
Df2 O2 3.44(5) . 1_555 N
Df2 O3 3.25(5) . 4_555 N
Df2 O4 2.86(6) . 310_555 N
Df2 O4 3.33(5) . -302_445 N
Df2 SJ 3.01(7) . -207_453 N
Df2 SJ 2.12(6) . -304_445 N
Df2 Oc 3.07(6) . -3_555 N
Df2 Oc 3.92(5) . -108_544 N
Df2 Oc 2.49(5) . -304_445 N
Df2 Dc1 3.83(6) . -3_555 N
Df2 Dc1 3.50(6) . -207_453 N
Df2 Dc1 2.55(6) . -304_445 N
Df2 Dc2 3.50(6) . -3_555 N
Df2 Dc2 3.92(6) . -108_544 N
Df2 Dc2 1.65(5) . -304_445 N
Df2 Od 2.78(8) . -207_453 N
Df2 Od 2.52(7) . -304_445 N
Df2 Dd1 2.88(10) . -207_453 N
Df2 Dd1 3.31(8) . -304_445 N
Df2 Dd2 2.66(12) . -207_453 N
Df2 Dd2 2.73(10) . -304_445 N
Df2 OII* 3.81(6) . -301_445 N
Df2 DII*1 3.79(19) . -302_445 N
Df2 DII*1 3.11(15) . -303_445 N
Df2 DII*2 3.93(16) . -301_445 N
Df2 Of 0.960740(10) . 1_555 N
Df2 Of 2.78(6) . -304_445 N
Df2 Df1 1.518650(10) . 1_555 N
Df2 Df1 3.16(6) . -304_445 N
Df2 Df2 3.56(8) . -304_445 N
Df2 Oe 2.71(6) . 103_554 N
Df2 Oe 2.50(6) . -207_453 N
Df2 De1 2.49(8) . 103_554 N
Df2 De1 3.93(7) . 105_544 N
Df2 De1 2.88(7) . -207_453 N
Df2 De2 3.50(6) . 103_554 N
Df2 De2 3.91(7) . 105_544 N
Df2 De2 1.54(6) . -207_453 N
Df2 SIII 1.96(6) . 304_445 N
Oe Si1 3.460(28) . -12_554 N
Oe Si2 4.26(4) . 112_554 N
Oe Si2 3.554(31) . -211_454 N
Oe Al1 4.26(4) . 112_554 N
Oe Al1 3.554(31) . -211_454 N
Oe O1 5.872(32) . 4_555 N
Oe O1 5.982(32) . 9_554 N
Oe O1 5.910(35) . -3_555 N
Oe O1 2.999(33) . -12_554 N
Oe O1 3.34(4) . 111_555 N
Oe O1 5.55(4) . 203_554 N
Oe O1 5.649(31) . -305_444 N
Oe O2 5.86(4) . 1_555 N
Oe O2 4.701(28) . -108_544 N
Oe O2 4.920(30) . -109_543 N
Oe O2 5.601(34) . 202_554 N
Oe O3 4.562(30) . 4_555 N
Oe O3 5.198(34) . 9_554 N
Oe O3 4.459(27) . 205_554 N
Oe O3 5.548(35) . 208_555 N
Oe O4 5.533(29) . 106_554 N
Oe O4 4.40(4) . 311_554 N
Oe O4 4.66(4) . 312_555 N
Oe O4 2.620(27) . -303_445 N
Oe SII 4.608(27) . -301_445 N
Oe SJ 3.38(5) . 1_555 N
Oe SJ 0.84(4) . -108_544 N
Oe SJ 4.85(4) . -201_453 N
Oe SJ 2.65(5) . -305_444 N
Oe Oc 3.890(33) . 1_555 N
Oe Oc 5.029(29) . 105_544 N
Oe Oc 5.996(31) . 111_555 N
Oe Oc 1.66(4) . -108_544 N
Oe Oc 3.41(4) . -201_453 N
Oe Oc 4.897(29) . 308_544 N
Oe Oc 1.21(4) . -305_444 N
Oe Dc1 2.957(33) . 1_555 N
Oe Dc1 0.97(4) . -108_544 N
Oe Dc1 3.52(4) . -201_453 N
Oe Dc1 1.71(4) . -305_444 N
Oe Dc2 1.86(4) . -108_544 N
Oe Dc2 1.56(4) . -305_444 N
Oe Od 3.07(6) . 1_555 N
Oe Od 4.87(6) . 105_544 N
Oe Od 0.58(6) . -108_544 N
Oe Od 4.57(6) . -201_453 N
Oe Od 5.48(6) . 308_544 N
Oe Od 2.58(6) . -305_444 N
Oe Dd1 3.18(9) . 1_555 N
Oe Dd1 1.29(7) . -108_544 N
Oe Dd1 2.56(9) . -305_444 N
Oe Dd2 3.65(9) . 1_555 N
Oe Dd2 1.41(7) . -108_544 N
Oe Dd2 3.32(8) . -305_444 N
Oe OII* 5.253(32) . 8_554 N
Oe OII* 5.460(31) . -105_544 N
Oe OII* 4.169(30) . -301_445 N
Oe DII*1 3.51(15) . -303_445 N
Oe Of 4.54(4) . 1_555 N
Oe Of 5.56(4) . 104_544 N
Oe Of 3.68(4) . -108_544 N
Oe Of 2.78(4) . -109_543 N
Oe Of 3.31(4) . 202_554 N
Oe Of 4.53(5) . -304_445 N
Oe Of 5.00(4) . -305_444 N
Oe Df1 2.57(6) . -109_543 N
Oe Df1 2.94(7) . 202_554 N
Oe Df1 3.96(6) . -304_445 N
Oe Df2 2.50(6) . -109_543 N
Oe Df2 2.71(6) . 202_554 N
Oe Oe 2.598(27) . 105_544 N
Oe Oe 2.598(27) . -108_544 N
Oe Oe 5.17(5) . -201_453 N
Oe Oe 4.47(5) . 308_544 N
Oe Oe 4.47(5) . -305_444 N
Oe De1 0.959990(10) . 1_555 N
Oe De1 1.87(4) . 105_544 N
Oe De1 3.24(5) . -108_544 N
Oe De2 0.960760(10) . 1_555 N
Oe De2 3.34(4) . 105_544 N
Oe De2 2.33(5) . -108_544 N
Oe SIII 3.204(34) . 8_554 N
Oe SIII 4.88(5) . 304_445 N
Oe SIII 4.53(5) . 305_544 N
De1 Si1 3.49(5) . -12_554 N
De1 Si2 3.59(5) . 112_554 N
De1 Al1 3.59(5) . 112_554 N
De1 O1 2.62(6) . -12_554 N
De1 O4 3.57(4) . 311_554 N
De1 O4 3.05(4) . -303_445 N
De1 SJ 1.66(4) . -108_544 N
De1 SJ 1.82(5) . -305_444 N
De1 Oc 2.51(4) . -108_544 N
De1 Oc 2.89(5) . -201_453 N
De1 Oc 0.26(4) . -305_444 N
De1 Dc1 3.44(5) . 1_555 N
De1 Dc1 1.64(5) . -108_544 N
De1 Dc1 3.09(5) . -201_453 N
De1 Dc1 1.11(5) . -305_444 N
De1 Dc2 2.68(4) . -108_544 N
De1 Dc2 3.43(4) . -201_453 N
De1 Dc2 0.97(6) . -305_444 N
De1 Od 3.64(7) . 1_555 N
De1 Od 1.51(6) . -108_544 N
De1 Od 1.71(7) . -305_444 N
De1 Dd1 3.52(10) . 1_555 N
De1 Dd1 2.11(8) . -108_544 N
De1 Dd1 3.93(9) . -201_453 N
De1 Dd1 1.68(9) . -305_444 N
De1 Dd2 2.11(9) . -108_544 N
De1 Dd2 2.41(8) . -305_444 N
De1 DII*1 3.49(9) . 311_554 N
De1 Of 3.26(6) . -108_544 N
De1 Of 2.84(6) . -109_543 N
De1 Of 3.17(7) . 202_554 N
De1 Df1 3.82(7) . -108_544 N
De1 Df1 2.48(8) . -109_543 N
De1 Df1 2.94(8) . 202_554 N
De1 Df2 3.93(7) . -108_544 N
De1 Df2 2.88(7) . -109_543 N
De1 Df2 2.49(8) . 202_554 N
De1 Oe 0.959990(10) . 1_555 N
De1 Oe 3.24(5) . 105_544 N
De1 Oe 1.87(4) . -108_544 N
De1 De1 2.69(5) . 105_544 N
De1 De1 2.69(5) . -108_544 N
De1 De2 1.518660(10) . 1_555 N
De1 De2 1.73(6) . -108_544 N
De1 De2 3.98(6) . -305_444 N
De1 SIII 3.20(5) . 8_554 N
De2 Si1 3.50(5) . -12_554 N
De2 Si1 3.93(4) . 111_555 N
De2 Si2 3.03(6) . -211_454 N
De2 Al1 3.03(6) . -211_454 N
De2 O1 3.32(5) . -12_554 N
De2 O1 2.61(5) . 111_555 N
De2 O4 2.44(6) . -303_445 N
De2 SJ 2.99(6) . 1_555 N
De2 SJ 0.83(6) . -108_544 N
De2 SJ 3.33(5) . -305_444 N
De2 Oc 3.78(5) . 1_555 N
De2 Oc 1.60(5) . -108_544 N
De2 Oc 1.75(5) . -305_444 N
De2 Dc1 2.92(5) . 1_555 N
De2 Dc1 1.25(5) . -108_544 N
De2 Dc1 2.44(4) . -305_444 N
De2 Dc2 1.29(5) . -108_544 N
De2 Dc2 2.18(4) . -305_444 N
De2 Od 2.68(7) . 1_555 N
De2 Od 1.08(6) . -108_544 N
De2 Od 3.22(7) . -305_444 N
De2 Dd1 2.80(10) . 1_555 N
De2 Dd1 1.94(7) . -108_544 N
De2 Dd1 2.97(9) . -305_444 N
De2 Dd2 3.05(11) . 1_555 N
De2 Dd2 1.63(9) . -108_544 N
De2 Dd2 3.88(9) . -305_444 N
De2 DII*1 3.97(14) . -303_445 N
De2 Of 3.15(6) . -108_544 N
De2 Of 1.92(5) . -109_543 N
De2 Df1 3.69(7) . -108_544 N
De2 Df1 1.86(7) . -109_543 N
De2 Df1 3.88(7) . 202_554 N
De2 Df2 3.91(7) . -108_544 N
De2 Df2 1.54(6) . -109_543 N
De2 Df2 3.50(6) . 202_554 N
De2 Oe 0.960760(10) . 1_555 N
De2 Oe 2.33(5) . 105_544 N
De2 Oe 3.34(4) . -108_544 N
De2 De1 1.518660(10) . 1_555 N
De2 De1 1.73(6) . 105_544 N
De2 De1 3.98(6) . 308_544 N
De2 De2 3.16(4) . 105_544 N
De2 De2 3.16(4) . -108_544 N
De2 SIII 2.53(5) . 8_554 N
SIII Si1 2.87(4) . -211_454 N
SIII Si1 2.87(4) . -302_445 N
SIII Si2 2.96(4) . -108_544 N
SIII Si2 2.96(4) . -303_445 N
SIII Al1 2.96(4) . -108_544 N
SIII Al1 2.96(4) . -303_445 N
SIII O1 3.219(14) . 208_555 N
SIII O1 3.228(15) . -211_454 N
SIII O1 3.219(14) . 303_555 N
SIII O1 3.228(15) . -302_445 N
SIII O2 2.96(5) . 4_555 N
SIII O2 2.96(5) . -301_445 N
SIII O3 4.55(5) . -108_544 N
SIII O3 4.48(5) . -211_454 N
SIII O3 4.391(7) . 301_555 N
SIII O3 4.48(5) . -302_445 N
SIII O3 4.55(5) . -303_445 N
SIII O3 4.391(7) . -304_445 N
SIII O4 2.43(4) . -10_554 N
SIII O4 2.43(4) . -12_554 N
SIII SJ 2.841(30) . 4_555 N
SIII SJ 2.841(30) . -301_445 N
SIII Oc 3.999(23) . 4_555 N
SIII Oc 3.32(4) . 208_555 N
SIII Oc 3.32(4) . 303_555 N
SIII Oc 3.999(23) . -301_445 N
SIII Dc1 3.774(33) . 4_555 N
SIII Dc1 3.774(33) . -301_445 N
SIII Dc2 3.274(25) . 4_555 N
SIII Dc2 3.338(29) . 208_555 N
SIII Dc2 3.338(29) . 303_555 N
SIII Dc2 3.274(25) . -301_445 N
SIII Od 3.29(5) . 4_555 N
SIII Od 4.67(6) . 107_555 N
SIII Od 4.48(7) . 208_555 N
SIII Od 4.67(6) . -205_454 N
SIII Od 4.48(7) . 303_555 N
SIII Od 3.29(5) . -301_445 N
SIII Dd2 3.09(9) . 4_555 N
SIII Dd2 3.09(9) . -301_445 N
SIII Of 1.63(6) . 4_555 N
SIII Of 1.63(6) . -301_445 N
SIII Df1 2.41(7) . 4_555 N
SIII Df1 2.41(7) . -301_445 N
SIII Df2 1.96(6) . 4_555 N
SIII Df2 1.96(6) . -301_445 N
SIII Oe 4.88(5) . 4_555 N
SIII Oe 4.53(5) . -8_555 N
SIII Oe 3.204(34) . 107_555 N
SIII Oe 4.53(5) . -203_454 N
SIII Oe 3.204(34) . -205_454 N
SIII Oe 4.88(5) . -301_445 N
SIII De1 3.20(5) . 107_555 N
SIII De1 3.20(5) . -205_454 N
SIII De2 2.53(5) . 107_555 N
SIII De2 2.53(5) . -205_454 N
loop_
_pd_meas_intensity_total
_pd_proc_ls_weight
_pd_proc_intensity_bkg_calc
_pd_calc_intensity_total
0.0(20) . . .
0.0(20) . . .
0.0(20) . . .
0.0(20) . . .
0.0(20) . . .
0.0(20) . . .
0.0(20) . . .
0.0(20) . . .
0.0(20) . . .
0.0(20) . . .
0.0(20) . . .
0.0(20) . . .
0.0(20) . . .
0.0(20) . . .
0.0(20) . . .
0.0(20) . . .
0.0(20) . . .
0.0(20) . . .
0.0(20) . . .
0.0(20) . . .
0.0(20) . . .
1.0(20) . . .
2.0(20) . . .
5.0(20) . . .
7.0(20) . . .
8.0(20) . . .
9.0(20) . . .
11.0(20) . . .
14.0(20) . . .
13.0(20) . . .
22.0(20) . . .
17.0(20) . . .
23.0(20) . . .
23.0(20) . . .
24.0(20) . . .
26.0(20) . . .
32.0(20) . . .
30.0(20) . . .
34.0(20) . . .
35.0(20) . . .
36.0(20) . . .
37.0(20) . . .
37.0(20) . . .
41.0(20) . . .
38.0(20) . . .
41.0(20) . . .
43.0(20) . . .
40.0(20) . . .
42.0(20) . . .
41.0(20) . . .
40.0(20) . . .
37.0(20) . . .
39.0(20) . . .
40.0(20) . . .
43.0(20) . . .
40.0(20) . . .
41.0(20) . . .
46.0(20) . . .
46.0(20) . . .
46.0(30) . . .
53.0(20) . . .
52.0(20) . . .
53.0(30) . . .
52.0(30) . . .
53.0(30) . . .
55.0(30) . . .
59.0(30) . . .
59.0(30) . . .
66.0(30) . . .
67.0(30) . . .
76.0(30) . . .
85(4) . . .
98(4) . . .
111(4) . . .
120(4) . . .
134(4) . . .
140(5) . . .
144(5) . . .
161(5) . . .
173(5) . . .
183(5) . . .
204(5) . . .
213(5) . . .
219(5) . . .
244(6) . . .
241(6) . . .
254(6) . . .
266(6) . . .
277(6) . . .
285(6) . . .
293(6) . . .
308(6) . . .
311(6) . . .
333(6) . . .
328(6) . . .
347(6) . . .
354(6) . . .
359(6) . . .
369(7) . . .
382(7) . . .
376(7) . . .
369(7) . . .
381(7) . . .
383(7) . . .
389(7) . . .
384(6) . . .
381(6) . . .
372(6) . . .
376(6) . . .
378(6) . . .
378(6) 0.0 -3443.8 .
385(6) 0.0 -3338.1 .
372(6) 0.0 -3235.0 .
366(6) 0.0 -3134.4 .
369(6) 0.0 -3036.4 .
375(6) 0.0 -2940.8 .
363(6) 0.0 -2847.7 .
352(6) 0.0 -2756.8 .
359(6) 0.0 -2668.3 .
351(6) 0.0 -2582.0 .
352(6) 0.0 -2498.0 .
357(6) 0.0 -2416.0 .
354(6) 0.0 -2336.2 .
352(6) 0.0 -2258.5 .
353(6) 0.0 -2182.7 .
344(6) 0.0 -2108.9 .
342(6) 0.0 -2037.0 .
341(6) 0.0 -1967.1 .
343(6) 0.0 -1898.9 .
337(6) 0.0 -1832.6 .
331(6) 0.0 -1768.0 .
342(6) 0.0 -1705.1 .
333(6) 0.0 -1643.9 .
335(6) 0.0 -1584.3 .
332(6) 0.0 -1526.3 .
325(6) 0.0 -1469.9 .
324(6) 0.0 -1415.0 .
330(6) 0.0 -1361.6 .
320(6) 0.0 -1309.7 .
310(6) 0.0 -1259.2 .
326(6) 0.0 -1210.0 .
324(6) 0.0 -1162.3 .
328(6) 0.0 -1115.8 .
325(6) 0.0 -1070.7 .
329(6) 0.0 -1026.8 .
331(6) 0.0 -984.1 .
330(6) 0.0 -942.7 .
323(6) 0.0 -902.4 .
318(6) 0.0 -863.3 .
315(6) 0.0 -825.2 .
314(6) 0.0 -788.3 .
311(6) 0.0 -752.5 .
316(6) 0.0 -717.6 .
322(6) 0.0 -683.8 .
324(6) 0.0 -651.0 .
320(6) 0.0 -619.1 .
329(6) 0.0 -588.2 .
331(6) 0.0 -558.2 .
338(6) 0.0 -529.1 .
343(6) 0.0 -500.9 .
335(6) 0.0 -473.5 .
344(6) 0.0 -446.9 .
357(7) 0.0 -421.2 .
376(7) 0.0 -396.2 .
370(7) 0.0 -372.0 .
365(7) 0.0 -348.5 .
384(7) 0.0 -325.8 .
397(7) 0.0 -303.8 .
416(7) 0.0 -282.5 .
452(8) 0.0 -261.8 .
463(8) 0.0 -241.8 .
513(9) 0.0 -222.4 .
564(9) 0.0 -203.7 .
629(10) 0.0 -185.5 .
700(11) 0.0 -168.0 .
803(12) 0.0 -151.0 .
933(12) 0.0 -134.6 .
1071(13) 0.0 -118.7 .
1216(14) 0.0 -103.3 .
1414(15) 0.0 -88.5 .
1672(16) 0.0 -74.1 .
1935(17) 0.0 -60.3 .
2251(18) 0.0 -46.9 .
2646(20) 0.0 -33.9 .
3137(22) 0.0 -21.5 .
3824(24) 0.0 -9.4 .
4512(26) 0.0 2.2 .
5235(27) 0.0 13.5 .
5802(28) 0.0 24.3 .
6087(28) 0.0 34.7 .
5921(26) 0.0 44.8 .
5325(23) 0.0 54.5 .
4379(20) 0.0 63.8 .
3340(16) 0.0 72.9 .
2367(12) 0.0 81.5 .
1635(9) 0.0 89.9 .
1108(8) 0.0 97.9 .
767(8) 0.0 105.6 .
558(7) 0.0 113.1 .
454(7) 0.0 120.2 .
412(7) 0.0 127.1 .
380(7) 0.0 133.7 .
360(7) 0.0 140.0 .
346(6) 0.0 146.1 .
335(6) 0.0 152.0 .
329(7) 0.0 157.6 .
330(6) 0.0 163.0 .
307(7) 0.0 168.1 .
321(6) 0.0 173.1 .
303(7) 0.0 177.8 .
303(6) 0.0 182.3 .
304(6) 0.0 186.7 .
309(6) 0.0 190.8 .
301(6) 0.0 194.8 .
312(6) 0.0 198.5 .
299(6) 0.0 202.2 .
299(6) 0.0 205.6 .
294(6) 0.0 208.9 .
289(6) 0.0 212.0 .
290(6) 0.0 215.0 .
291(6) 0.0 217.8 .
289(6) 0.0 220.5 .
292(6) 0.0 223.1 .
280(6) 0.0 225.6 .
279(6) 0.0 227.9 .
290(6) 0.0 230.1 .
298(6) 0.0 232.1 .
279(6) 0.0 234.1 .
278(6) 0.0 236.0 .
280(6) 0.0 237.7 .
271(6) 0.0 239.4 .
267(6) 0.0 240.9 .
275(6) 0.0 242.4 .
277(6) 0.0 243.8 .
266(5) 0.0 245.1 .
271(6) 0.0 246.3 .
268(6) 0.0 247.4 .
264(6) 0.0 248.4 .
281(6) 0.0 249.4 .
272(6) 0.0 250.3 .
269(6) 0.0 251.2 .
283(6) 0.0 252.0 .
275(6) 0.0 252.7 .
266(6) 0.0 253.3 .
269(5) 0.0 254.0 .
268(6) 0.0 254.5 .
277(5) 0.0 255.0 .
271(6) 0.0 255.4 .
274(6) 0.0 255.9 .
261(5) 0.0 256.2 .
257(5) 0.0 256.5 .
260(5) 0.0 256.8 .
277(6) 0.0 257.0 .
271(5) 0.0 257.2 .
263(5) 0.0 257.4 .
264(5) 0.0 257.5 .
265(6) 0.0 257.6 .
269(6) 0.0 257.7 .
277(6) 0.0 257.7 .
265(5) 0.0 257.7 .
261(6) 0.0 257.7 .
259(5) 0.0 257.7 .
266(5) 0.0 257.6 .
256(6) 0.0 257.5 .
263(5) 0.0 257.4 .
255(5) 0.0 257.3 .
261(5) 0.0 257.2 .
266(5) 0.0 257.0 .
262(5) 0.0 256.8 .
263(5) 0.0 256.6 .
260(5) 0.0400 256.4 264.6
264(5) 0.0400 256.2 264.6
272(5) 0.0400 256.0 264.6
259(5) 0.0400 255.8 264.6
260(5) 0.0400 255.5 264.6
252(6) 0.02778 255.3 264.6
260(5) 0.0400 255.0 264.7
264(5) 0.0400 254.7 264.7
260(5) 0.0400 254.4 264.9
257(5) 0.0400 254.1 265.0
264(5) 0.0400 253.9 265.2
267(5) 0.0400 253.6 265.5
258(5) 0.0400 253.2 265.8
265(5) 0.0400 252.9 266.2
271(6) 0.02778 252.6 266.7
283(6) 0.02778 252.3 267.3
277(6) 0.02778 252.0 268.0
266(5) 0.0400 251.7 268.9
273(5) 0.0400 251.4 270.0
262(6) 0.02778 251.0 271.2
279(6) 0.02778 250.7 272.7
280(6) 0.02778 250.4 274.6
280(6) 0.02778 250.1 276.8
268(6) 0.02778 249.7 279.5
287(6) 0.02778 249.4 282.8
297(6) 0.02778 249.1 287.0
314(6) 0.02778 248.8 292.6
307(6) 0.02778 248.5 300.5
340(6) 0.02778 248.1 312.7
372(7) 0.02041 247.8 333.2
406(7) 0.02041 247.5 368.2
451(8) 0.01563 247.2 426.6
541(9) 0.01235 246.9 518.9
663(9) 0.01235 246.6 655.5
813(10) 0.01000 246.3 844.9
1030(12) 0.00694 246.0 1089.9
1277(13) 0.00592 245.7 1383.9
1614(14) 0.00510 245.4 1714.7
1945(15) 0.00444 245.1 2055.2
2209(16) 0.00391 244.8 2332.1
2339(16) 0.00391 244.5 2430.9
2309(15) 0.00444 244.2 2281.5
2032(14) 0.00510 243.9 1933.2
1647(12) 0.00694 243.6 1504.1
1220(10) 0.01000 243.4 1101.9
843(8) 0.01563 243.1 786.9
606(7) 0.02041 242.8 572.8
453(6) 0.02778 242.6 443.2
370(6) 0.02778 242.3 371.2
339(6) 0.02778 242.0 332.6
316(6) 0.02778 241.8 311.3
301(6) 0.02778 241.5 298.3
287(6) 0.02778 241.3 289.3
278(6) 0.02778 241.0 282.5
273(5) 0.0400 240.8 277.1
270(5) 0.0400 240.6 272.6
264(5) 0.0400 240.3 268.9
258(5) 0.0400 240.1 265.7
250(6) 0.02778 239.9 263.0
242(5) 0.0400 239.6 260.7
238(5) 0.0400 239.4 258.7
233(5) 0.0400 239.2 256.9
245(5) 0.0400 239.0 255.3
245(5) 0.0400 238.8 253.9
244(5) 0.0400 238.6 252.7
241(5) 0.0400 238.4 251.6
249(5) 0.0400 238.2 250.6
249(5) 0.0400 238.0 249.6
237(5) 0.0400 237.8 248.8
237(5) 0.0400 237.6 248.0
232(5) 0.0400 237.4 247.3
235(5) 0.0400 237.2 246.7
244(5) 0.0400 237.0 246.1
241(5) 0.0400 236.8 245.6
236(5) 0.0400 236.6 245.1
238(5) 0.0400 236.4 244.7
240(5) 0.0400 236.2 244.3
235(5) 0.0400 236.1 244.0
238(5) 0.0400 235.9 243.7
245(5) 0.0400 235.7 243.4
240(5) 0.0400 235.5 243.3
234(5) 0.0400 235.4 243.2
228(5) 0.0400 235.2 243.3
235(5) 0.0400 235.0 243.6
248(5) 0.0400 234.8 244.3
249(5) 0.0400 234.7 245.8
251(5) 0.0400 234.5 248.6
257(5) 0.0400 234.3 253.4
261(6) 0.02778 234.2 260.9
275(5) 0.0400 234.0 271.7
290(6) 0.02778 233.9 285.7
307(6) 0.02778 233.7 302.1
337(6) 0.02778 233.5 318.9
345(6) 0.02778 233.4 333.1
343(6) 0.02778 233.2 339.9
349(6) 0.02778 233.1 335.1
341(6) 0.02778 232.9 319.8
309(6) 0.02778 232.7 299.6
280(5) 0.0400 232.6 280.0
262(5) 0.0400 232.4 264.2
253(5) 0.0400 232.3 253.4
241(5) 0.0400 232.1 246.9
249(5) 0.0400 231.9 243.6
247(5) 0.0400 231.8 242.5
249(5) 0.0400 231.6 243.0
248(6) 0.02778 231.5 244.8
254(5) 0.0400 231.3 247.8
260(5) 0.0400 231.1 251.8
270(5) 0.0400 231.0 256.2
281(6) 0.02778 230.8 260.4
281(5) 0.0400 230.7 263.0
287(6) 0.02778 230.5 262.8
284(6) 0.02778 230.3 259.3
270(5) 0.0400 230.2 253.7
262(5) 0.0400 230.0 247.7
246(5) 0.0400 229.8 242.6
231(5) 0.0400 229.7 238.8
234(5) 0.0400 229.5 236.2
230(5) 0.0400 229.3 234.6
237(5) 0.0400 229.2 233.7
234(5) 0.0400 229.0 233.1
236(5) 0.0400 228.8 232.6
229(5) 0.0400 228.7 232.3
229(5) 0.0400 228.5 232.0
229(5) 0.0400 228.3 231.7
231(5) 0.0400 228.1 231.4
223(5) 0.0400 228.0 231.1
229(5) 0.0400 227.8 230.9
232(5) 0.0400 227.6 230.6
230(5) 0.0400 227.4 230.4
218(5) 0.0400 227.2 230.2
230(5) 0.0400 227.1 230.0
228(5) 0.0400 226.9 229.7
221(5) 0.0400 226.7 229.5
227(5) 0.0400 226.5 229.3
223(5) 0.0400 226.3 229.1
213(5) 0.0400 226.1 228.9
221(5) 0.0400 225.9 228.7
229(5) 0.0400 225.8 228.5
225(5) 0.0400 225.6 228.3
224(5) 0.0400 225.4 228.1
221(5) 0.0400 225.2 227.9
230(5) 0.0400 225.0 227.7
230(5) 0.0400 224.8 227.5
239(5) 0.0400 224.6 227.4
239(5) 0.0400 224.4 227.2
237(5) 0.0400 224.2 227.0
233(5) 0.0400 224.0 226.8
226(5) 0.0400 223.8 226.6
226(5) 0.0400 223.6 226.4
229(5) 0.0400 223.4 226.3
234(5) 0.0400 223.2 226.1
227(5) 0.0400 223.0 225.9
229(5) 0.0400 222.8 225.7
227(5) 0.0400 222.5 225.6
225(5) 0.0400 222.3 225.4
225(5) 0.0400 222.1 225.3
229(5) 0.0400 221.9 225.1
226(5) 0.0400 221.7 225.0
222(5) 0.0400 221.5 224.8
226(5) 0.0400 221.3 224.7
221(5) 0.0400 221.1 224.7
222(5) 0.0400 220.8 224.6
227(5) 0.0400 220.6 224.7
218(5) 0.0400 220.4 225.0
227(5) 0.0400 220.2 225.4
228(5) 0.0400 220.0 226.1
239(5) 0.0400 219.7 227.0
231(5) 0.0400 219.5 228.0
228(5) 0.0400 219.3 228.9
223(5) 0.0400 219.1 229.4
221(5) 0.0400 218.9 229.2
227(5) 0.0400 218.6 228.3
227(5) 0.0400 218.4 227.0
230(5) 0.0400 218.2 225.8
220(5) 0.0400 217.9 224.8
219(5) 0.0400 217.7 224.1
218(5) 0.0400 217.5 223.7
225(5) 0.0400 217.3 223.4
218(5) 0.0400 217.0 223.4
230(5) 0.0400 216.8 223.4
221(5) 0.0400 216.6 223.5
220(5) 0.0400 216.4 223.6
222(5) 0.0400 216.1 223.8
234(5) 0.0400 215.9 224.0
228(5) 0.0400 215.7 224.3
226(5) 0.0400 215.4 224.7
230(5) 0.0400 215.2 225.2
225(5) 0.0400 215.0 225.7
221(5) 0.0400 214.8 226.4
227(5) 0.0400 214.5 227.2
225(5) 0.0400 214.3 228.1
227(5) 0.0400 214.1 229.3
224(5) 0.0400 213.8 230.7
225(5) 0.0400 213.6 232.4
231(5) 0.0400 213.4 234.4
238(5) 0.0400 213.2 237.0
236(5) 0.0400 212.9 240.2
244(5) 0.0400 212.7 244.3
251(5) 0.0400 212.5 249.9
261(6) 0.02778 212.3 258.3
287(6) 0.02778 212.0 271.8
308(6) 0.02778 211.8 295.5
357(7) 0.02041 211.6 337.8
426(7) 0.02041 211.4 411.0
546(8) 0.01563 211.1 529.7
704(10) 0.01000 210.9 705.5
942(11) 0.00826 210.7 936.8
1194(12) 0.00694 210.5 1198.1
1434(13) 0.00592 210.3 1440.0
1589(13) 0.00592 210.0 1597.1
1613(13) 0.00592 209.8 1601.0
1439(12) 0.00694 209.6 1436.7
1199(11) 0.00826 209.4 1170.3
892(9) 0.01235 209.2 889.3
618(7) 0.02041 209.0 652.3
444(6) 0.02778 208.7 481.7
340(6) 0.02778 208.5 373.7
294(6) 0.02778 208.3 312.0
267(5) 0.0400 208.1 278.7
240(5) 0.0400 207.9 260.6
246(5) 0.0400 207.7 249.8
238(5) 0.0400 207.5 242.7
237(5) 0.0400 207.3 237.4
227(5) 0.0400 207.1 233.3
231(5) 0.0400 206.9 229.9
223(5) 0.0400 206.7 227.1
221(5) 0.0400 206.5 224.7
222(5) 0.0400 206.3 222.7
223(5) 0.0400 206.1 221.0
223(5) 0.0400 205.9 219.5
212(5) 0.0400 205.7 218.2
211(5) 0.0400 205.5 217.0
222(5) 0.0400 205.3 216.0
226(5) 0.0400 205.1 215.1
226(5) 0.0400 205.0 214.2
220(5) 0.0400 204.8 213.5
215(5) 0.0400 204.6 212.8
215(5) 0.0400 204.4 212.2
218(5) 0.0400 204.2 211.6
213(5) 0.0400 204.1 211.1
210(5) 0.0400 203.9 210.6
212(5) 0.0400 203.7 210.1
203(5) 0.0400 203.6 209.7
207(5) 0.0400 203.4 209.4
207(5) 0.0400 203.2 209.0
213(5) 0.0400 203.1 208.7
214(5) 0.0400 202.9 208.4
207(5) 0.0400 202.7 208.2
207(5) 0.0400 202.6 207.9
208(5) 0.0400 202.4 207.7
210(5) 0.0400 202.3 207.5
214(5) 0.0400 202.1 207.4
209(5) 0.0400 202.0 207.3
194(5) 0.0400 201.8 207.2
207(5) 0.0400 201.7 207.2
213(5) 0.0400 201.5 207.2
205(5) 0.0400 201.4 207.3
210(5) 0.0400 201.2 207.5
200(5) 0.0400 201.1 207.8
212(5) 0.0400 201.0 208.3
210(5) 0.0400 200.8 209.1
207(5) 0.0400 200.7 210.5
220(5) 0.0400 200.6 213.1
219(5) 0.0400 200.5 218.0
228(5) 0.0400 200.3 226.6
245(5) 0.0400 200.2 240.8
265(6) 0.02778 200.1 261.9
292(6) 0.02778 200.0 289.7
325(6) 0.02778 199.9 320.4
360(6) 0.02778 199.7 347.5
363(6) 0.02778 199.6 362.5
352(6) 0.02778 199.5 358.1
345(6) 0.02778 199.4 335.2
324(6) 0.02778 199.3 303.1
273(5) 0.0400 199.2 271.6
248(5) 0.0400 199.1 246.3
228(5) 0.0400 199.0 228.8
217(5) 0.0400 198.9 218.0
209(5) 0.0400 198.8 211.9
200(5) 0.0400 198.7 208.7
208(5) 0.0400 198.7 206.8
209(5) 0.0400 198.6 205.7
210(5) 0.0400 198.5 204.9
208(5) 0.0400 198.4 204.3
207(5) 0.0400 198.3 203.8
205(5) 0.0400 198.3 203.5
203(5) 0.0400 198.2 203.2
203(5) 0.0400 198.1 203.0
205(5) 0.0400 198.0 202.8
200(5) 0.0400 198.0 202.7
207(5) 0.0400 197.9 202.7
207(5) 0.0400 197.8 202.7
202(5) 0.0400 197.8 202.8
201(5) 0.0400 197.7 203.0
198(5) 0.0400 197.7 203.4
205(5) 0.0400 197.6 204.2
218(5) 0.0400 197.6 205.8
209(5) 0.0400 197.5 208.6
217(5) 0.0400 197.5 213.7
222(5) 0.0400 197.4 221.8
238(5) 0.0400 197.4 233.4
251(5) 0.0400 197.3 247.9
257(5) 0.0400 197.3 262.8
273(6) 0.02778 197.3 274.4
278(5) 0.0400 197.2 278.2
279(6) 0.02778 197.2 272.1
263(5) 0.0400 197.2 258.4
249(6) 0.02778 197.1 242.4
231(5) 0.0400 197.1 228.1
222(5) 0.0400 197.1 217.4
211(5) 0.0400 197.1 210.4
201(5) 0.0400 197.0 206.3
208(5) 0.0400 197.0 204.1
202(5) 0.0400 197.0 202.9
209(5) 0.0400 197.0 202.2
208(5) 0.0400 197.0 201.8
206(5) 0.0400 197.0 201.5
199(5) 0.0400 196.9 201.3
202(5) 0.0400 196.9 201.2
203(5) 0.0400 196.9 201.1
203(5) 0.0400 196.9 201.0
204(5) 0.0400 196.9 201.0
195(5) 0.0400 196.9 201.0
198(5) 0.0400 196.9 201.0
196(5) 0.0400 196.9 201.0
193(5) 0.0400 196.9 201.1
196(5) 0.0400 196.9 201.2
207(5) 0.0400 196.9 201.3
194(5) 0.0400 196.9 201.4
204(5) 0.0400 197.0 201.6
206(5) 0.0400 197.0 201.8
201(5) 0.0400 197.0 202.0
196(5) 0.0400 197.0 202.2
208(5) 0.0400 197.0 202.5
205(5) 0.0400 197.0 202.9
206(5) 0.0400 197.0 203.3
207(5) 0.0400 197.1 203.7
203(5) 0.0400 197.1 204.3
193(5) 0.0400 197.1 204.9
198(5) 0.0400 197.1 205.6
211(5) 0.0400 197.2 206.5
200(5) 0.0400 197.2 207.5
201(5) 0.0400 197.2 208.7
208(5) 0.0400 197.2 210.3
210(5) 0.0400 197.3 212.2
213(5) 0.0400 197.3 214.7
217(5) 0.0400 197.3 218.2
221(5) 0.0400 197.4 223.7
235(5) 0.0400 197.4 233.3
245(5) 0.0400 197.4 250.4
285(6) 0.02778 197.5 280.9
344(6) 0.02778 197.5 331.9
423(8) 0.01563 197.5 408.7
523(8) 0.01563 197.6 510.7
631(9) 0.01235 197.6 624.9
734(9) 0.01235 197.6 725.0
784(9) 0.01235 197.7 777.1
758(10) 0.01000 197.7 755.6
681(8) 0.01563 197.8 668.1
553(7) 0.02041 197.8 551.4
423(7) 0.02041 197.8 440.0
325(6) 0.02778 197.9 352.4
265(5) 0.0400 197.9 292.9
230(5) 0.0400 198.0 257.0
226(5) 0.0400 198.0 237.1
220(5) 0.0400 198.1 226.4
217(5) 0.0400 198.1 220.5
210(5) 0.0400 198.2 216.8
214(5) 0.0400 198.2 214.3
207(5) 0.0400 198.3 212.4
206(5) 0.0400 198.3 210.9
210(5) 0.0400 198.4 209.8
205(5) 0.0400 198.4 208.9
207(5) 0.0400 198.4 208.3
208(5) 0.0400 198.5 207.7
201(5) 0.0400 198.5 207.4
207(5) 0.0400 198.6 207.3
206(5) 0.0400 198.6 207.5
215(5) 0.0400 198.7 208.1
214(5) 0.0400 198.7 209.7
215(5) 0.0400 198.8 212.6
223(5) 0.0400 198.8 217.6
228(5) 0.0400 198.9 224.8
241(5) 0.0400 198.9 234.0
255(5) 0.0400 199.0 243.5
261(5) 0.0400 199.0 250.7
256(5) 0.0400 199.1 252.7
254(6) 0.02778 199.1 248.3
241(5) 0.0400 199.2 239.6
234(5) 0.0400 199.2 229.9
230(5) 0.0400 199.3 221.8
210(5) 0.0400 199.3 216.3
204(5) 0.0400 199.4 213.5
211(5) 0.0400 199.4 212.7
211(5) 0.0400 199.5 212.9
216(5) 0.0400 199.5 213.1
224(5) 0.0400 199.6 212.6
219(5) 0.0400 199.6 211.3
220(5) 0.0400 199.6 209.6
206(4) 0.0625 199.7 207.9
205(5) 0.0400 199.7 206.6
208(5) 0.0400 199.8 205.7
204(5) 0.0400 199.8 205.1
213(5) 0.0400 199.9 204.8
212(5) 0.0400 199.9 204.7
203(5) 0.0400 200.0 204.6
197(5) 0.0400 200.0 204.6
201(5) 0.0400 200.0 204.7
204(5) 0.0400 200.1 204.8
203(4) 0.0625 200.1 204.9
201(5) 0.0400 200.2 205.0
206(5) 0.0400 200.2 205.1
200(5) 0.0400 200.2 205.2
202(5) 0.0400 200.3 205.4
206(5) 0.0400 200.3 205.6
198(5) 0.0400 200.3 205.9
202(5) 0.0400 200.4 206.1
207(5) 0.0400 200.4 206.4
207(5) 0.0400 200.4 206.7
211(5) 0.0400 200.5 207.1
210(5) 0.0400 200.5 207.6
207(5) 0.0400 200.5 208.2
206(5) 0.0400 200.6 208.9
213(5) 0.0400 200.6 209.8
211(5) 0.0400 200.6 211.3
201(5) 0.0400 200.6 213.7
209(5) 0.0400 200.7 217.8
226(5) 0.0400 200.7 224.9
239(6) 0.02778 200.7 236.1
253(5) 0.0400 200.7 252.1
269(6) 0.02778 200.7 271.6
291(6) 0.02778 200.8 291.4
305(6) 0.02778 200.8 305.5
307(6) 0.02778 200.8 308.2
306(5) 0.0400 200.8 298.0
289(6) 0.02778 200.8 279.8
259(5) 0.0400 200.8 260.5
244(5) 0.0400 200.9 244.5
228(5) 0.0400 200.9 233.3
228(5) 0.0400 200.9 226.8
221(5) 0.0400 200.9 223.7
224(5) 0.0400 200.9 222.8
223(5) 0.0400 200.9 223.2
222(5) 0.0400 200.9 224.5
235(5) 0.0400 200.9 226.4
227(5) 0.0400 200.9 229.0
226(5) 0.0400 200.9 232.3
226(5) 0.0400 200.9 236.5
233(5) 0.0400 200.9 242.0
247(6) 0.02778 200.9 249.5
263(5) 0.0400 200.9 260.7
271(6) 0.02778 200.9 279.2
325(6) 0.02778 200.9 312.2
375(7) 0.02041 200.9 372.0
491(8) 0.01563 200.9 475.5
701(10) 0.01000 200.9 639.5
911(10) 0.01000 200.8 870.0
1201(12) 0.00694 200.8 1147.6
1495(13) 0.00592 200.8 1417.0
1644(14) 0.00510 200.8 1592.7
1598(13) 0.00592 200.8 1595.2
1383(12) 0.00694 200.8 1419.1
1093(11) 0.00826 200.7 1147.8
809(9) 0.01235 200.7 876.2
597(8) 0.01563 200.7 660.8
465(7) 0.02041 200.7 518.9
426(7) 0.02041 200.6 441.2
405(7) 0.02041 200.6 404.8
391(7) 0.02041 200.6 384.9
389(7) 0.02041 200.6 364.1
364(6) 0.02778 200.5 336.7
320(6) 0.02778 200.5 306.8
290(6) 0.02778 200.5 279.8
258(5) 0.0400 200.4 258.6
238(5) 0.0400 200.4 243.6
228(5) 0.0400 200.3 233.8
226(5) 0.0400 200.3 227.5
226(6) 0.02778 200.3 223.4
224(5) 0.0400 200.2 220.4
220(5) 0.0400 200.2 218.2
215(5) 0.0400 200.1 216.4
218(5) 0.0400 200.1 214.8
215(5) 0.0400 200.0 213.5
223(5) 0.0400 200.0 212.4
220(5) 0.0400 199.9 211.4
216(5) 0.0400 199.9 210.5
216(5) 0.0400 199.8 209.7
210(5) 0.0400 199.7 209.0
215(5) 0.0400 199.7 208.4
216(5) 0.0400 199.6 207.9
206(5) 0.0400 199.6 207.3
210(5) 0.0400 199.5 206.9
211(5) 0.0400 199.4 206.5
202(4) 0.0625 199.4 206.1
200(5) 0.0400 199.3 205.8
214(5) 0.0400 199.2 205.5
209(5) 0.0400 199.2 205.3
213(5) 0.0400 199.1 205.1
212(5) 0.0400 199.0 205.2
208(5) 0.0400 198.9 205.3
216(5) 0.0400 198.9 205.5
218(5) 0.0400 198.8 205.8
211(5) 0.0400 198.7 205.9
207(5) 0.0400 198.6 205.6
214(5) 0.0400 198.6 205.1
211(5) 0.0400 198.5 204.4
207(5) 0.0400 198.4 203.7
198(5) 0.0400 198.3 203.2
200(5) 0.0400 198.2 202.7
209(5) 0.0400 198.1 202.4
207(5) 0.0400 198.0 202.1
204(5) 0.0400 198.0 201.9
199(5) 0.0400 197.9 201.8
206(5) 0.0400 197.8 201.6
205(5) 0.0400 197.7 201.5
202(5) 0.0400 197.6 201.3
202(5) 0.0400 197.5 201.2
199(4) 0.0625 197.4 201.1
198(5) 0.0400 197.3 201.0
200(5) 0.0400 197.2 200.9
209(5) 0.0400 197.1 200.8
197(5) 0.0400 197.0 200.7
197(5) 0.0400 196.9 200.7
202(5) 0.0400 196.8 200.7
199(4) 0.0625 196.7 200.8
201(5) 0.0400 196.5 201.0
203(5) 0.0400 196.4 201.1
210(5) 0.0400 196.3 201.1
205(5) 0.0400 196.2 201.0
201(4) 0.0625 196.1 200.8
200(5) 0.0400 196.0 200.5
199(5) 0.0400 195.9 200.3
199(5) 0.0400 195.8 200.1
195(5) 0.0400 195.6 200.0
201(5) 0.0400 195.5 200.0
204(5) 0.0400 195.4 199.9
202(5) 0.0400 195.3 199.9
199(5) 0.0400 195.2 200.0
202(5) 0.0400 195.0 200.0
202(5) 0.0400 194.9 200.1
210(5) 0.0400 194.8 200.2
203(5) 0.0400 194.7 200.3
196(5) 0.0400 194.5 200.5
204(4) 0.0625 194.4 200.7
199(5) 0.0400 194.3 201.0
205(5) 0.0400 194.2 201.3
197(5) 0.0400 194.0 201.6
195(5) 0.0400 193.9 202.1
204(5) 0.0400 193.8 202.6
210(5) 0.0400 193.6 203.3
200(5) 0.0400 193.5 204.0
208(5) 0.0400 193.4 205.0
205(5) 0.0400 193.2 206.1
199(5) 0.0400 193.1 207.6
201(5) 0.0400 193.0 209.4
209(5) 0.0400 192.8 211.6
218(5) 0.0400 192.7 214.5
214(5) 0.0400 192.6 218.5
222(5) 0.0400 192.4 224.6
235(5) 0.0400 192.3 234.6
257(5) 0.0400 192.1 252.6
292(6) 0.02778 192.0 285.1
348(6) 0.02778 191.9 340.9
451(7) 0.02041 191.7 428.1
592(8) 0.01563 191.6 548.2
721(9) 0.01235 191.4 689.2
817(10) 0.01000 191.3 819.9
895(9) 0.01235 191.1 893.5
877(9) 0.01235 191.0 873.0
755(9) 0.01235 190.8 767.6
610(8) 0.01563 190.7 625.3
471(7) 0.02041 190.6 489.4
356(6) 0.02778 190.4 382.6
284(5) 0.0400 190.3 309.8
250(5) 0.0400 190.1 265.5
229(5) 0.0400 190.0 240.6
220(5) 0.0400 189.8 226.8
216(5) 0.0400 189.7 218.9
207(5) 0.0400 189.5 213.8
204(5) 0.0400 189.4 210.2
216(5) 0.0400 189.2 207.5
206(5) 0.0400 189.1 205.4
205(5) 0.0400 188.9 203.8
197(5) 0.0400 188.8 202.8
195(5) 0.0400 188.6 202.4
204(5) 0.0400 188.5 203.0
212(5) 0.0400 188.3 204.8
208(5) 0.0400 188.2 207.8
215(5) 0.0400 188.0 211.9
210(5) 0.0400 187.8 216.1
211(5) 0.0400 187.7 218.8
211(5) 0.0400 187.5 218.5
210(5) 0.0400 187.4 214.9
207(5) 0.0400 187.2 209.6
205(5) 0.0400 187.1 204.2
201(5) 0.0400 186.9 199.7
195(5) 0.0400 186.8 196.4
203(5) 0.0400 186.6 194.3
197(5) 0.0400 186.5 192.9
192(5) 0.0400 186.3 192.0
193(5) 0.0400 186.2 191.4
198(5) 0.0400 186.0 190.9
187(5) 0.0400 185.9 190.5
190(5) 0.0400 185.7 190.2
185(5) 0.0400 185.5 189.9
185(4) 0.0625 185.4 189.6
182(5) 0.0400 185.2 189.3
182(4) 0.0625 185.1 189.0
187(5) 0.0400 184.9 188.8
187(5) 0.0400 184.8 188.6
190(5) 0.0400 184.6 188.4
189(5) 0.0400 184.5 188.2
187(5) 0.0400 184.3 188.0
186(5) 0.0400 184.2 187.8
191(5) 0.0400 184.0 187.6
191(5) 0.0400 183.9 187.5
188(5) 0.0400 183.7 187.3
180(4) 0.0625 183.6 187.2
185(5) 0.0400 183.4 187.1
185(5) 0.0400 183.3 187.0
184(5) 0.0400 183.1 186.9
184(4) 0.0625 183.0 186.9
184(5) 0.0400 182.8 186.9
189(5) 0.0400 182.7 187.0
187(4) 0.0625 182.5 187.3
190(5) 0.0400 182.4 187.7
193(5) 0.0400 182.2 188.2
192(5) 0.0400 182.1 188.7
189(4) 0.0625 181.9 189.0
188(4) 0.0625 181.8 188.9
188(4) 0.0625 181.6 188.6
194(4) 0.0625 181.5 188.1
187(4) 0.0625 181.3 187.8
182(4) 0.0625 181.2 187.6
185(4) 0.0625 181.0 187.6
188(4) 0.0625 180.9 187.8
187(4) 0.0625 180.7 188.1
184(4) 0.0625 180.6 188.6
188(4) 0.0625 180.5 189.3
192(4) 0.0625 180.3 190.3
188(4) 0.0625 180.2 191.7
192(4) 0.0625 180.0 193.7
196(4) 0.0625 179.9 197.1
199(5) 0.0400 179.7 203.3
217(4) 0.0625 179.6 214.4
237(5) 0.0400 179.5 233.5
275(5) 0.0400 179.3 263.4
313(6) 0.02778 179.2 304.9
353(6) 0.02778 179.0 354.0
401(6) 0.02778 178.9 400.1
415(6) 0.02778 178.8 426.7
404(6) 0.02778 178.6 420.2
363(6) 0.02778 178.5 383.7
327(6) 0.02778 178.4 334.3
284(5) 0.0400 178.2 287.2
242(5) 0.0400 178.1 250.1
218(5) 0.0400 178.0 224.9
212(5) 0.0400 177.8 209.4
203(4) 0.0625 177.7 200.6
199(4) 0.0625 177.6 195.5
194(4) 0.0625 177.5 192.4
192(5) 0.0400 177.3 190.3
195(4) 0.0625 177.2 188.9
186(4) 0.0625 177.1 187.8
189(4) 0.0625 176.9 187.0
184(4) 0.0625 176.8 186.4
187(4) 0.0625 176.7 186.0
184(4) 0.0625 176.6 185.7
186(5) 0.0400 176.5 185.6
186(4) 0.0625 176.3 185.5
187(4) 0.0625 176.2 185.6
192(4) 0.0625 176.1 185.7
184(4) 0.0625 176.0 186.0
185(4) 0.0625 175.9 186.4
186(4) 0.0625 175.7 187.0
187(4) 0.0625 175.6 187.8
184(4) 0.0625 175.5 189.0
193(5) 0.0400 175.4 190.7
198(4) 0.0625 175.3 193.5
202(4) 0.0625 175.2 198.6
210(5) 0.0400 175.1 207.4
226(5) 0.0400 174.9 222.3
250(5) 0.0400 174.8 245.1
278(5) 0.0400 174.7 276.0
320(6) 0.02778 174.6 311.6
350(6) 0.02778 174.5 343.7
371(6) 0.02778 174.4 360.3
359(6) 0.02778 174.3 352.7
327(6) 0.02778 174.2 325.5
291(5) 0.0400 174.1 291.2
257(5) 0.0400 174.0 259.8
230(5) 0.0400 173.9 236.2
221(5) 0.0400 173.8 221.2
207(5) 0.0400 173.7 213.3
211(5) 0.0400 173.6 210.4
210(5) 0.0400 173.5 210.8
205(5) 0.0400 173.4 213.5
214(5) 0.0400 173.3 218.6
228(5) 0.0400 173.2 227.2
240(5) 0.0400 173.1 242.1
262(5) 0.0400 173.0 269.0
320(6) 0.02778 172.9 317.5
418(7) 0.02041 172.8 400.0
542(8) 0.01563 172.8 527.4
720(9) 0.01235 172.7 701.0
944(10) 0.01000 172.6 902.5
1110(11) 0.00826 172.5 1085.5
1197(12) 0.00694 172.4 1180.4
1141(11) 0.00826 172.3 1136.6
996(10) 0.01000 172.2 977.5
797(9) 0.01235 172.2 774.7
557(8) 0.01563 172.1 586.6
400(6) 0.02778 172.0 441.2
323(6) 0.02778 171.9 343.1
266(5) 0.0400 171.8 283.3
232(5) 0.0400 171.8 249.0
221(5) 0.0400 171.7 229.3
212(5) 0.0400 171.6 217.2
201(5) 0.0400 171.5 209.1
201(5) 0.0400 171.5 203.3
195(5) 0.0400 171.4 198.9
196(5) 0.0400 171.3 195.4
195(5) 0.0400 171.3 192.6
194(5) 0.0400 171.2 190.4
195(5) 0.0400 171.1 188.6
189(5) 0.0400 171.1 187.1
187(5) 0.0400 171.0 185.8
180(4) 0.0625 170.9 184.8
193(5) 0.0400 170.9 184.0
183(5) 0.0400 170.8 183.3
185(5) 0.0400 170.7 182.9
184(5) 0.0400 170.7 182.6
185(5) 0.0400 170.6 182.6
190(5) 0.0400 170.6 183.1
189(5) 0.0400 170.5 184.3
194(5) 0.0400 170.4 187.0
196(5) 0.0400 170.4 191.9
204(5) 0.0400 170.3 200.0
208(5) 0.0400 170.3 211.7
226(5) 0.0400 170.2 226.2
236(5) 0.0400 170.2 240.7
242(5) 0.0400 170.1 250.4
248(5) 0.0400 170.1 250.4
243(5) 0.0400 170.0 240.5
230(5) 0.0400 170.0 225.5
210(5) 0.0400 169.9 210.6
198(5) 0.0400 169.9 198.3
191(5) 0.0400 169.9 189.7
180(4) 0.0625 169.8 184.3
176(4) 0.0625 169.8 181.2
176(4) 0.0625 169.7 179.5
178(4) 0.0625 169.7 178.7
186(5) 0.0400 169.6 178.3
179(4) 0.0625 169.6 178.2
188(5) 0.0400 169.6 178.6
185(5) 0.0400 169.5 179.7
184(4) 0.0625 169.5 181.8
187(5) 0.0400 169.5 185.4
200(5) 0.0400 169.4 190.7
202(5) 0.0400 169.4 197.6
216(5) 0.0400 169.4 205.1
224(5) 0.0400 169.3 211.2
220(5) 0.0400 169.3 213.9
222(5) 0.0400 169.3 212.9
217(5) 0.0400 169.2 210.6
207(5) 0.0400 169.2 209.8
210(5) 0.0400 169.2 211.3
213(5) 0.0400 169.2 214.2
213(5) 0.0400 169.1 215.8
209(5) 0.0400 169.1 213.5
208(5) 0.0400 169.1 207.2
203(5) 0.0400 169.1 199.1
193(5) 0.0400 169.1 191.5
186(5) 0.0400 169.0 185.5
184(5) 0.0400 169.0 181.4
182(4) 0.0625 169.0 178.9
184(5) 0.0400 169.0 177.5
181(4) 0.0625 169.0 176.8
184(4) 0.0625 169.0 176.5
178(4) 0.0625 168.9 176.4
180(4) 0.0625 168.9 176.5
185(5) 0.0400 168.9 176.8
179(4) 0.0625 168.9 177.3
177(4) 0.0625 168.9 177.9
181(4) 0.0625 168.9 178.8
181(5) 0.0400 168.9 180.1
187(5) 0.0400 168.9 182.2
187(5) 0.0400 168.8 185.9
195(5) 0.0400 168.8 192.3
212(5) 0.0400 168.8 203.6
225(5) 0.0400 168.8 221.8
240(5) 0.0400 168.8 248.3
286(6) 0.02778 168.8 282.1
319(6) 0.02778 168.8 318.0
340(6) 0.02778 168.8 345.5
346(6) 0.02778 168.8 352.1
326(6) 0.02778 168.8 334.0
294(6) 0.02778 168.8 300.8
259(5) 0.0400 168.8 265.2
232(5) 0.0400 168.8 234.9
203(5) 0.0400 168.8 212.9
195(5) 0.0400 168.8 198.8
182(4) 0.0625 168.8 190.8
186(5) 0.0400 168.8 186.6
188(5) 0.0400 168.8 184.6
186(5) 0.0400 168.8 184.2
190(5) 0.0400 168.8 185.1
193(5) 0.0400 168.8 187.8
199(5) 0.0400 168.8 193.5
209(5) 0.0400 168.8 203.6
228(5) 0.0400 168.8 219.5
251(5) 0.0400 168.8 241.4
268(5) 0.0400 168.9 267.2
290(6) 0.02778 168.9 291.1
296(6) 0.02778 168.9 304.1
291(6) 0.02778 168.9 299.1
273(5) 0.0400 168.9 278.7
253(5) 0.0400 168.9 252.4
235(5) 0.0400 168.9 227.6
214(5) 0.0400 168.9 208.2
194(5) 0.0400 168.9 194.9
188(5) 0.0400 168.9 186.6
182(4) 0.0625 169.0 181.8
176(4) 0.0625 169.0 179.1
187(5) 0.0400 169.0 177.5
181(4) 0.0625 169.0 176.4
178(4) 0.0625 169.0 175.6
177(4) 0.0625 169.0 175.1
173(4) 0.0625 169.0 174.6
177(4) 0.0625 169.1 174.2
175(4) 0.0625 169.1 173.9
176(4) 0.0625 169.1 173.7
177(4) 0.0625 169.1 173.5
177(4) 0.0625 169.1 173.3
175(4) 0.0625 169.2 173.2
170(4) 0.0625 169.2 173.1
176(4) 0.0625 169.2 173.1
173(4) 0.0625 169.2 173.1
176(4) 0.0625 169.2 173.1
166(4) 0.0625 169.2 173.3
169(4) 0.0625 169.3 173.7
180(5) 0.0400 169.3 174.3
181(4) 0.0625 169.3 175.3
172(4) 0.0625 169.3 176.7
175(4) 0.0625 169.3 178.4
177(4) 0.0625 169.4 179.9
175(4) 0.0625 169.4 180.7
165(4) 0.0625 169.4 180.3
172(4) 0.0625 169.4 179.1
176(4) 0.0625 169.5 177.5
176(4) 0.0625 169.5 176.0
174(4) 0.0625 169.5 174.8
177(4) 0.0625 169.5 174.1
170(4) 0.0625 169.5 173.7
174(4) 0.0625 169.6 173.5
176(4) 0.0625 169.6 173.5
169(4) 0.0625 169.6 173.6
175(4) 0.0625 169.6 173.8
175(4) 0.0625 169.7 174.3
174(4) 0.0625 169.7 175.1
179(4) 0.0625 169.7 176.4
179(4) 0.0625 169.7 178.4
181(4) 0.0625 169.8 181.0
191(5) 0.0400 169.8 184.0
187(5) 0.0400 169.8 186.7
196(5) 0.0400 169.8 188.0
198(5) 0.0400 169.9 187.2
193(5) 0.0400 169.9 184.8
184(5) 0.0400 169.9 181.9
181(4) 0.0625 169.9 179.3
192(5) 0.0400 170.0 177.3
184(4) 0.0625 170.0 176.0
184(5) 0.0400 170.0 175.2
178(4) 0.0625 170.0 174.9
179(4) 0.0625 170.1 174.7
179(4) 0.0625 170.1 174.7
169(4) 0.0625 170.1 174.7
175(4) 0.0625 170.1 174.8
178(4) 0.0625 170.2 174.9
174(4) 0.0625 170.2 175.0
180(4) 0.0625 170.2 175.2
180(4) 0.0625 170.2 175.4
177(4) 0.0625 170.3 175.7
179(4) 0.0625 170.3 176.0
185(5) 0.0400 170.3 176.3
182(4) 0.0625 170.3 176.7
179(4) 0.0625 170.4 177.2
177(4) 0.0625 170.4 177.9
183(5) 0.0400 170.4 178.8
183(5) 0.0400 170.5 180.4
182(5) 0.0400 170.5 182.8
193(5) 0.0400 170.5 186.7
198(5) 0.0400 170.5 192.4
205(5) 0.0400 170.5 200.0
211(5) 0.0400 170.6 208.6
215(5) 0.0400 170.6 216.4
224(5) 0.0400 170.6 220.5
223(5) 0.0400 170.6 219.0
212(5) 0.0400 170.7 213.0
208(5) 0.0400 170.7 205.6
208(5) 0.0400 170.7 198.9
192(5) 0.0400 170.7 194.1
190(5) 0.0400 170.8 191.3
195(5) 0.0400 170.8 190.2
186(5) 0.0400 170.8 190.4
189(5) 0.0400 170.8 191.5
192(5) 0.0400 170.9 193.4
196(5) 0.0400 170.9 196.2
194(5) 0.0400 170.9 199.9
201(5) 0.0400 170.9 204.9
208(5) 0.0400 170.9 212.0
220(5) 0.0400 171.0 222.1
233(5) 0.0400 171.0 236.9
254(5) 0.0400 171.0 259.9
293(6) 0.02778 171.0 296.4
346(6) 0.02778 171.0 354.6
425(7) 0.02041 171.1 443.9
550(8) 0.01563 171.1 569.6
700(9) 0.01235 171.1 725.4
880(10) 0.01000 171.1 884.9
988(11) 0.00826 171.1 997.3
1031(11) 0.00826 171.2 1007.4
939(10) 0.01000 171.2 908.2
795(9) 0.01235 171.2 749.8
608(8) 0.01563 171.2 587.1
450(7) 0.02041 171.2 451.5
352(6) 0.02778 171.2 353.3
282(5) 0.0400 171.3 289.6
251(5) 0.0400 171.3 251.6
223(5) 0.0400 171.3 229.7
217(5) 0.0400 171.3 216.8
211(5) 0.0400 171.3 208.7
196(5) 0.0400 171.3 203.1
196(5) 0.0400 171.4 199.0
195(5) 0.0400 171.4 195.7
200(5) 0.0400 171.4 193.1
191(5) 0.0400 171.4 191.0
184(5) 0.0400 171.4 189.3
189(5) 0.0400 171.4 187.9
180(4) 0.0625 171.4 186.7
181(4) 0.0625 171.4 185.8
184(5) 0.0400 171.5 185.0
178(4) 0.0625 171.5 184.4
173(4) 0.0625 171.5 184.0
176(4) 0.0625 171.5 183.6
178(4) 0.0625 171.5 183.4
178(4) 0.0625 171.5 183.3
179(4) 0.0625 171.5 183.4
185(5) 0.0400 171.5 183.5
180(4) 0.0625 171.5 183.8
182(5) 0.0400 171.5 184.3
178(4) 0.0625 171.5 185.1
182(5) 0.0400 171.5 186.2
187(4) 0.0625 171.6 187.8
192(4) 0.0625 171.6 190.3
189(4) 0.0625 171.6 194.7
196(4) 0.0625 171.6 202.2
213(5) 0.0400 171.6 214.9
236(5) 0.0400 171.6 234.9
274(5) 0.0400 171.6 263.3
305(6) 0.02778 171.6 298.9
334(6) 0.02778 171.6 336.5
367(6) 0.02778 171.6 365.8
385(6) 0.02778 171.6 375.0
372(6) 0.02778 171.6 362.0
349(6) 0.02778 171.6 337.5
322(6) 0.02778 171.6 313.3
282(5) 0.0400 171.6 294.8
272(5) 0.0400 171.6 281.0
263(5) 0.0400 171.6 267.2
250(5) 0.0400 171.6 250.9
236(5) 0.0400 171.6 233.8
214(5) 0.0400 171.6 218.3
208(5) 0.0400 171.6 206.0
202(4) 0.0625 171.6 197.0
185(4) 0.0625 171.6 191.1
185(4) 0.0625 171.6 187.3
185(4) 0.0625 171.6 185.0
183(4) 0.0625 171.6 183.6
184(4) 0.0625 171.5 182.7
175(4) 0.0625 171.5 182.0
177(4) 0.0625 171.5 181.6
177(4) 0.0625 171.5 181.4
177(4) 0.0625 171.5 181.4
176(4) 0.0625 171.5 181.7
181(4) 0.0625 171.5 182.6
179(4) 0.0625 171.5 184.3
189(4) 0.0625 171.5 187.2
189(4) 0.0625 171.5 191.6
197(4) 0.0625 171.5 197.7
207(5) 0.0400 171.4 204.8
212(5) 0.0400 171.4 211.4
214(5) 0.0400 171.4 215.0
225(5) 0.0400 171.4 213.7
214(5) 0.0400 171.4 208.3
205(4) 0.0625 171.4 201.3
198(4) 0.0625 171.4 194.6
191(4) 0.0625 171.3 189.5
184(4) 0.0625 171.3 185.9
180(4) 0.0625 171.3 183.8
181(4) 0.0625 171.3 182.9
183(4) 0.0625 171.3 182.7
179(4) 0.0625 171.3 183.2
179(4) 0.0625 171.2 184.6
180(4) 0.0625 171.2 187.1
186(4) 0.0625 171.2 191.3
192(4) 0.0625 171.2 197.2
199(4) 0.0625 171.2 204.7
205(5) 0.0400 171.1 212.7
212(5) 0.0400 171.1 219.0
224(5) 0.0400 171.1 220.9
216(5) 0.0400 171.1 217.5
206(5) 0.0400 171.0 210.7
209(5) 0.0400 171.0 203.2
201(4) 0.0625 171.0 196.9
190(4) 0.0625 171.0 192.4
191(4) 0.0625 170.9 189.6
179(4) 0.0625 170.9 188.2
186(4) 0.0625 170.9 187.8
182(4) 0.0625 170.9 188.1
193(4) 0.0625 170.8 188.8
185(4) 0.0625 170.8 189.9
184(4) 0.0625 170.8 191.3
195(4) 0.0625 170.7 193.1
195(4) 0.0625 170.7 195.2
183(4) 0.0625 170.7 197.9
186(4) 0.0625 170.7 201.3
203(5) 0.0400 170.6 205.5
204(5) 0.0400 170.6 211.1
213(5) 0.0400 170.6 219.0
223(5) 0.0400 170.5 231.0
233(5) 0.0400 170.5 250.9
272(6) 0.02778 170.5 284.6
326(6) 0.02778 170.4 340.6
411(7) 0.02041 170.4 427.7
523(8) 0.01563 170.4 550.7
671(9) 0.01235 170.3 704.3
845(10) 0.01000 170.3 865.8
987(11) 0.00826 170.2 989.5
1041(11) 0.00826 170.2 1019.7
976(10) 0.01000 170.2 939.4
838(10) 0.01000 170.1 791.2
659(8) 0.01563 170.1 630.5
510(7) 0.02041 170.0 491.5
386(6) 0.02778 170.0 387.6
319(6) 0.02778 170.0 318.6
282(6) 0.02778 169.9 277.2
249(5) 0.0400 169.9 254.9
237(5) 0.0400 169.8 245.2
245(5) 0.0400 169.8 245.0
258(5) 0.0400 169.8 254.0
275(6) 0.02778 169.7 273.6
303(6) 0.02778 169.7 305.1
343(6) 0.02778 169.6 347.5
389(7) 0.02041 169.6 395.5
432(7) 0.02041 169.5 437.7
454(7) 0.02041 169.5 457.9
447(7) 0.02041 169.4 448.1
420(7) 0.02041 169.4 418.3
392(7) 0.02041 169.3 384.6
357(6) 0.02778 169.3 356.3
327(6) 0.02778 169.2 333.8
307(6) 0.02778 169.2 312.2
282(6) 0.02778 169.1 288.2
274(6) 0.02778 169.1 263.9
248(5) 0.0400 169.0 242.2
232(5) 0.0400 169.0 224.9
221(5) 0.0400 168.9 212.3
209(5) 0.0400 168.9 203.7
194(5) 0.0400 168.8 198.3
190(5) 0.0400 168.8 194.9
195(5) 0.0400 168.7 192.9
193(5) 0.0400 168.7 191.6
190(5) 0.0400 168.6 190.9
192(5) 0.0400 168.6 190.7
201(5) 0.0400 168.5 190.8
202(5) 0.0400 168.5 191.5
213(5) 0.0400 168.4 193.0
210(5) 0.0400 168.4 195.6
212(5) 0.0400 168.3 200.0
206(5) 0.0400 168.2 206.4
215(5) 0.0400 168.2 215.2
223(5) 0.0400 168.1 225.7
232(5) 0.0400 168.1 236.1
244(5) 0.0400 168.0 243.4
246(5) 0.0400 168.0 245.0
239(5) 0.0400 167.9 241.0
239(5) 0.0400 167.8 234.8
245(5) 0.0400 167.8 229.3
237(5) 0.0400 167.7 226.4
237(5) 0.0400 167.7 227.0
254(5) 0.0400 167.6 231.8
273(6) 0.02778 167.5 241.8
291(6) 0.02778 167.5 259.9
343(6) 0.02778 167.4 291.4
389(7) 0.02041 167.3 344.9
468(7) 0.02041 167.3 431.0
574(8) 0.01563 167.2 559.1
722(9) 0.01235 167.2 730.4
904(10) 0.01000 167.1 931.2
1065(11) 0.00826 167.0 1123.7
1187(12) 0.00694 167.0 1243.8
1202(12) 0.00694 166.9 1236.1
1124(12) 0.00694 166.8 1112.8
992(11) 0.00826 166.8 939.5
799(10) 0.01000 166.7 772.1
662(9) 0.01235 166.6 635.2
541(8) 0.01563 166.6 528.9
463(8) 0.01563 166.5 444.3
386(7) 0.02041 166.4 376.3
332(6) 0.02778 166.4 323.3
288(6) 0.02778 166.3 283.5
257(6) 0.02778 166.2 254.7
237(5) 0.0400 166.2 234.5
207(5) 0.0400 166.1 220.8
204(5) 0.0400 166.0 211.6
206(5) 0.0400 166.0 205.2
201(5) 0.0400 165.9 200.7
197(5) 0.0400 165.8 197.3
190(5) 0.0400 165.7 194.9
190(5) 0.0400 165.7 193.2
194(5) 0.0400 165.6 192.5
190(5) 0.0400 165.5 193.0
197(5) 0.0400 165.5 195.3
200(5) 0.0400 165.4 200.2
203(5) 0.0400 165.3 208.2
214(5) 0.0400 165.2 219.4
226(5) 0.0400 165.2 232.7
243(6) 0.02778 165.1 245.4
245(6) 0.02778 165.0 252.7
251(6) 0.02778 165.0 250.6
233(5) 0.0400 164.9 239.9
224(5) 0.0400 164.8 225.3
209(5) 0.0400 164.7 210.9
198(5) 0.0400 164.7 199.0
193(5) 0.0400 164.6 190.3
184(5) 0.0400 164.5 184.5
180(5) 0.0400 164.4 181.0
177(5) 0.0400 164.4 179.0
180(5) 0.0400 164.3 178.0
186(5) 0.0400 164.2 178.0
189(5) 0.0400 164.1 178.8
185(5) 0.0400 164.1 180.4
188(5) 0.0400 164.0 182.7
184(5) 0.0400 163.9 185.5
199(5) 0.0400 163.8 187.8
199(5) 0.0400 163.8 188.6
203(5) 0.0400 163.7 187.3
184(5) 0.0400 163.6 184.3
191(5) 0.0400 163.5 180.9
181(5) 0.0400 163.5 177.7
176(5) 0.0400 163.4 175.2
183(5) 0.0400 163.3 173.4
175(5) 0.0400 163.2 172.2
174(5) 0.0400 163.1 171.4
173(5) 0.0400 163.1 171.0
174(5) 0.0400 163.0 170.7
166(5) 0.0400 162.9 170.6
174(5) 0.0400 162.8 170.6
168(5) 0.0400 162.8 170.6
167(5) 0.0400 162.7 170.8
163(5) 0.0400 162.6 171.0
175(5) 0.0400 162.5 171.5
176(5) 0.0400 162.4 172.1
168(5) 0.0400 162.4 173.0
169(5) 0.0400 162.3 174.6
182(5) 0.0400 162.2 177.3
187(5) 0.0400 162.1 181.9
182(5) 0.0400 162.0 189.3
190(5) 0.0400 162.0 200.4
208(5) 0.0400 161.9 215.7
225(6) 0.02778 161.8 234.1
253(6) 0.02778 161.7 252.9
260(6) 0.02778 161.6 266.4
274(6) 0.02778 161.6 268.5
249(6) 0.02778 161.5 258.0
240(6) 0.02778 161.4 240.2
224(6) 0.02778 161.3 221.2
206(5) 0.0400 161.2 204.8
189(5) 0.0400 161.2 192.3
193(5) 0.0400 161.1 183.9
177(5) 0.0400 161.0 178.8
172(5) 0.0400 160.9 176.1
168(5) 0.0400 160.8 175.1
167(5) 0.0400 160.8 175.7
177(5) 0.0400 160.7 177.6
176(5) 0.0400 160.6 181.0
184(5) 0.0400 160.5 185.7
196(5) 0.0400 160.4 191.1
191(5) 0.0400 160.4 195.9
198(5) 0.0400 160.3 198.0
199(5) 0.0400 160.2 196.3
186(5) 0.0400 160.1 191.5
180(5) 0.0400 160.0 185.5
184(5) 0.0400 159.9 179.9
185(5) 0.0400 159.9 175.4
174(5) 0.0400 159.8 172.1
177(5) 0.0400 159.7 169.9
166(5) 0.0400 159.6 168.6
169(5) 0.0400 159.5 167.8
164(5) 0.0400 159.5 167.3
166(5) 0.0400 159.4 167.1
177(5) 0.0400 159.3 166.9
177(5) 0.0400 159.2 166.8
173(5) 0.0400 159.1 166.8
172(5) 0.0400 159.1 166.8
173(5) 0.0400 159.0 167.0
165(5) 0.0400 158.9 167.1
171(5) 0.0400 158.8 167.4
166(5) 0.0400 158.7 167.8
167(5) 0.0400 158.7 168.4
168(5) 0.0400 158.6 169.3
170(5) 0.0400 158.5 170.5
173(5) 0.0400 158.4 172.3
181(5) 0.0400 158.3 174.5
183(5) 0.0400 158.2 177.1
188(5) 0.0400 158.2 179.8
191(5) 0.0400 158.1 181.8
190(5) 0.0400 158.0 182.7
200(5) 0.0400 157.9 182.4
186(5) 0.0400 157.8 181.8
191(5) 0.0400 157.8 181.5
183(5) 0.0400 157.7 182.0
178(5) 0.0400 157.6 183.4
187(5) 0.0400 157.5 186.3
187(5) 0.0400 157.4 191.1
186(5) 0.0400 157.4 199.0
210(6) 0.02778 157.3 211.6
222(5) 0.0400 157.2 231.2
252(6) 0.02778 157.1 260.1
295(7) 0.02041 157.0 299.7
342(8) 0.01563 157.0 349.6
415(8) 0.01563 156.9 406.1
461(8) 0.01563 156.8 460.8
507(9) 0.01235 156.7 504.0
547(9) 0.01235 156.7 534.4
577(9) 0.01235 156.6 561.9
594(9) 0.01235 156.5 592.5
608(9) 0.01235 156.4 618.5
610(9) 0.01235 156.3 619.7
604(9) 0.01235 156.3 580.9
518(9) 0.01235 156.2 510.7
448(8) 0.01563 156.1 430.6
374(7) 0.02041 156.0 357.4
299(6) 0.02778 155.9 298.7
252(6) 0.02778 155.9 256.2
233(6) 0.02778 155.8 227.9
209(5) 0.0400 155.7 210.2
192(5) 0.0400 155.6 199.4
187(5) 0.0400 155.6 193.0
184(5) 0.0400 155.5 189.1
187(5) 0.0400 155.4 187.1
189(5) 0.0400 155.3 186.7
185(5) 0.0400 155.2 188.2
189(5) 0.0400 155.2 192.5
195(5) 0.0400 155.1 200.5
209(5) 0.0400 155.0 213.2
229(6) 0.02778 154.9 230.9
245(6) 0.02778 154.9 252.5
267(6) 0.02778 154.8 274.5
285(6) 0.02778 154.7 290.7
287(6) 0.02778 154.6 293.9
279(6) 0.02778 154.6 282.1
253(6) 0.02778 154.5 261.3
245(6) 0.02778 154.4 238.6
219(6) 0.02778 154.3 218.7
203(5) 0.0400 154.3 203.7
184(5) 0.0400 154.2 194.0
186(5) 0.0400 154.1 189.2
186(5) 0.0400 154.0 188.9
194(5) 0.0400 154.0 193.2
198(5) 0.0400 153.9 202.8
221(6) 0.02778 153.8 218.5
234(6) 0.02778 153.8 240.7
260(6) 0.02778 153.7 268.2
278(6) 0.02778 153.6 297.0
299(7) 0.02041 153.5 319.6
305(7) 0.02041 153.5 326.5
295(6) 0.02778 153.4 314.1
275(6) 0.02778 153.3 288.7
246(6) 0.02778 153.2 259.7
233(5) 0.0400 153.2 233.4
215(5) 0.0400 153.1 212.2
199(5) 0.0400 153.0 196.4
182(5) 0.0400 153.0 185.3
176(5) 0.0400 152.9 177.8
171(5) 0.0400 152.8 172.8
160(4) 0.0625 152.8 169.4
162(4) 0.0625 152.7 167.1
162(4) 0.0625 152.6 165.4
166(5) 0.0400 152.5 164.2
164(5) 0.0400 152.5 163.3
162(5) 0.0400 152.4 162.6
155(4) 0.0625 152.3 162.1
172(5) 0.0400 152.3 161.8
165(5) 0.0400 152.2 161.7
167(5) 0.0400 152.1 161.8
164(5) 0.0400 152.1 162.3
161(4) 0.0625 152.0 163.1
155(4) 0.0625 151.9 164.6
165(5) 0.0400 151.9 166.5
162(5) 0.0400 151.8 168.9
176(5) 0.0400 151.7 171.4
177(5) 0.0400 151.7 173.2
171(5) 0.0400 151.6 173.6
163(5) 0.0400 151.5 172.6
173(5) 0.0400 151.5 170.8
169(5) 0.0400 151.4 169.0
162(4) 0.0625 151.3 167.8
172(5) 0.0400 151.3 167.3
166(5) 0.0400 151.2 168.0
170(5) 0.0400 151.2 170.2
170(5) 0.0400 151.1 174.5
185(5) 0.0400 151.0 181.9
194(5) 0.0400 151.0 193.6
212(5) 0.0400 150.9 210.6
234(5) 0.0400 150.8 233.1
265(6) 0.02778 150.8 259.5
292(6) 0.02778 150.7 285.9
308(6) 0.02778 150.7 304.8
304(6) 0.02778 150.6 308.5
298(6) 0.02778 150.5 295.7
285(6) 0.02778 150.5 273.3
252(6) 0.02778 150.4 249.1
221(5) 0.0400 150.4 227.4
208(5) 0.0400 150.3 209.6
197(5) 0.0400 150.2 195.5
187(5) 0.0400 150.2 184.7
176(5) 0.0400 150.1 176.7
167(5) 0.0400 150.1 170.9
167(5) 0.0400 150.0 166.8
166(5) 0.0400 149.9 164.0
160(4) 0.0625 149.9 162.0
164(5) 0.0400 149.8 160.6
156(4) 0.0625 149.8 159.6
167(5) 0.0400 149.7 158.9
163(5) 0.0400 149.7 158.4
167(5) 0.0400 149.6 158.0
159(4) 0.0625 149.6 157.8
155(4) 0.0625 149.5 157.7
153(4) 0.0625 149.4 157.8
161(4) 0.0625 149.4 158.1
159(4) 0.0625 149.3 158.6
155(5) 0.0400 149.3 159.4
170(5) 0.0400 149.2 160.2
166(5) 0.0400 149.2 161.0
163(5) 0.0400 149.1 161.7
154(4) 0.0625 149.1 162.0
159(4) 0.0625 149.0 162.0
161(4) 0.0625 149.0 162.0
165(5) 0.0400 148.9 162.3
159(4) 0.0625 148.9 163.0
173(5) 0.0400 148.8 164.5
167(4) 0.0625 148.8 167.1
179(4) 0.0625 148.7 171.6
185(5) 0.0400 148.7 179.0
194(5) 0.0400 148.6 190.7
215(5) 0.0400 148.6 207.9
242(5) 0.0400 148.5 231.4
269(5) 0.0400 148.5 260.4
302(6) 0.02778 148.4 291.5
318(6) 0.02778 148.4 318.1
330(6) 0.02778 148.3 330.4
328(6) 0.02778 148.3 322.5
295(6) 0.02778 148.3 298.3
253(5) 0.0400 148.2 267.4
234(5) 0.0400 148.2 237.4
196(4) 0.0625 148.1 212.4
184(5) 0.0400 148.1 193.6
178(4) 0.0625 148.0 180.6
172(4) 0.0625 148.0 172.1
176(4) 0.0625 147.9 166.8
165(4) 0.0625 147.9 163.5
158(4) 0.0625 147.9 161.4
165(4) 0.0625 147.8 160.0
162(4) 0.0625 147.8 158.9
157(4) 0.0625 147.7 158.2
155(4) 0.0625 147.7 157.7
158(4) 0.0625 147.7 157.4
160(4) 0.0625 147.6 157.3
155(4) 0.0625 147.6 157.5
157(4) 0.0625 147.5 158.2
170(4) 0.0625 147.5 159.4
164(4) 0.0625 147.5 161.5
168(4) 0.0625 147.4 164.6
172(4) 0.0625 147.4 168.5
185(5) 0.0400 147.3 173.1
182(4) 0.0625 147.3 177.5
184(5) 0.0400 147.3 180.5
181(4) 0.0625 147.2 180.8
180(4) 0.0625 147.2 178.2
178(4) 0.0625 147.2 174.2
173(4) 0.0625 147.1 169.9
167(4) 0.0625 147.1 166.2
165(4) 0.0625 147.1 163.7
157(4) 0.0625 147.0 162.4
160(4) 0.0625 147.0 162.5
158(4) 0.0625 147.0 164.2
165(4) 0.0625 146.9 167.7
175(4) 0.0625 146.9 173.4
184(5) 0.0400 146.9 181.5
181(4) 0.0625 146.8 191.8
199(5) 0.0400 146.8 203.4
207(5) 0.0400 146.8 214.4
225(5) 0.0400 146.8 221.4
215(5) 0.0400 146.7 221.8
219(5) 0.0400 146.7 216.1
206(5) 0.0400 146.7 207.3
201(4) 0.0625 146.6 198.1
183(4) 0.0625 146.6 189.9
183(4) 0.0625 146.6 182.8
176(4) 0.0625 146.6 176.7
175(4) 0.0625 146.5 171.7
171(4) 0.0625 146.5 167.9
161(4) 0.0625 146.5 165.3
161(4) 0.0625 146.5 163.6
156(4) 0.0625 146.4 162.8
162(4) 0.0625 146.4 162.7
161(4) 0.0625 146.4 163.1
165(4) 0.0625 146.4 164.2
167(4) 0.0625 146.3 166.1
172(4) 0.0625 146.3 169.2
182(4) 0.0625 146.3 174.1
176(4) 0.0625 146.3 181.9
199(5) 0.0400 146.3 194.3
216(5) 0.0400 146.2 212.8
241(5) 0.0400 146.2 238.7
283(5) 0.0400 146.2 271.9
327(6) 0.02778 146.2 310.2
364(6) 0.02778 146.2 347.7
376(6) 0.02778 146.1 374.4
371(6) 0.02778 146.1 379.4
355(6) 0.02778 146.1 360.3
319(6) 0.02778 146.1 325.8
286(5) 0.0400 146.1 287.2
248(5) 0.0400 146.1 251.9
217(5) 0.0400 146.0 223.5
197(4) 0.0625 146.0 202.8
187(4) 0.0625 146.0 189.2
177(4) 0.0625 146.0 181.2
174(4) 0.0625 146.0 177.4
171(4) 0.0625 146.0 177.0
172(4) 0.0625 146.0 179.0
182(4) 0.0625 146.0 183.0
183(4) 0.0625 145.9 188.2
190(4) 0.0625 145.9 193.5
195(4) 0.0625 145.9 197.0
191(4) 0.0625 145.9 197.3
189(4) 0.0625 145.9 194.4
179(4) 0.0625 145.9 189.8
180(4) 0.0625 145.9 184.9
179(4) 0.0625 145.9 180.3
172(4) 0.0625 145.9 176.1
172(4) 0.0625 145.9 172.1
168(4) 0.0625 145.8 168.5
162(4) 0.0625 145.8 165.6
161(4) 0.0625 145.8 163.4
158(4) 0.0625 145.8 161.9
152(4) 0.0625 145.8 160.9
160(4) 0.0625 145.8 160.4
165(4) 0.0625 145.8 160.2
164(4) 0.0625 145.8 160.4
163(4) 0.0625 145.8 160.8
161(4) 0.0625 145.8 161.5
168(4) 0.0625 145.8 162.6
165(4) 0.0625 145.8 164.2
170(4) 0.0625 145.8 166.5
165(4) 0.0625 145.8 169.7
173(4) 0.0625 145.8 173.9
171(4) 0.0625 145.8 179.2
180(4) 0.0625 145.8 185.3
182(4) 0.0625 145.8 191.5
183(4) 0.0625 145.8 196.7
191(4) 0.0625 145.8 199.7
202(4) 0.0625 145.8 200.3
196(4) 0.0625 145.8 199.6
189(5) 0.0400 145.8 199.3
191(4) 0.0625 145.8 200.8
205(5) 0.0400 145.8 205.5
229(5) 0.0400 145.8 214.9
239(5) 0.0400 145.8 231.6
266(5) 0.0400 145.8 259.0
315(6) 0.02778 145.8 301.5
373(6) 0.02778 145.8 363.1
457(7) 0.02041 145.9 446.2
565(8) 0.01563 145.9 549.1
687(8) 0.01563 145.9 663.1
781(9) 0.01235 145.9 769.1
841(9) 0.01235 145.9 837.3
832(9) 0.01235 145.9 842.2
766(9) 0.01235 145.9 785.8
667(8) 0.01563 145.9 695.3
563(7) 0.02041 145.9 597.9
483(7) 0.02041 145.9 508.1
421(6) 0.02778 145.9 430.2
359(6) 0.02778 146.0 364.9
309(6) 0.02778 146.0 312.3
265(5) 0.0400 146.0 271.9
248(5) 0.0400 146.0 242.1
220(5) 0.0400 146.0 220.5
210(5) 0.0400 146.0 205.1
196(4) 0.0625 146.0 194.3
192(4) 0.0625 146.1 186.6
181(4) 0.0625 146.1 181.2
177(4) 0.0625 146.1 177.3
173(4) 0.0625 146.1 174.6
171(4) 0.0625 146.1 172.7
168(4) 0.0625 146.1 171.8
170(4) 0.0625 146.2 171.8
175(4) 0.0625 146.2 172.8
179(4) 0.0625 146.2 175.0
181(4) 0.0625 146.2 178.2
186(4) 0.0625 146.2 182.0
191(4) 0.0625 146.2 185.8
194(4) 0.0625 146.3 188.3
189(4) 0.0625 146.3 188.1
189(4) 0.0625 146.3 185.3
181(4) 0.0625 146.3 180.7
181(4) 0.0625 146.4 175.7
177(4) 0.0625 146.4 171.2
168(4) 0.0625 146.4 167.7
164(4) 0.0625 146.4 165.3
168(4) 0.0625 146.4 164.1
172(4) 0.0625 146.5 164.2
167(4) 0.0625 146.5 165.4
169(4) 0.0625 146.5 168.0
176(4) 0.0625 146.5 171.8
183(4) 0.0625 146.6 176.6
180(4) 0.0625 146.6 181.8
188(4) 0.0625 146.6 186.6
184(4) 0.0625 146.7 189.2
185(4) 0.0625 146.7 188.6
177(4) 0.0625 146.7 185.0
177(4) 0.0625 146.7 179.8
176(4) 0.0625 146.8 174.4
171(4) 0.0625 146.8 169.6
174(4) 0.0625 146.8 165.8
163(4) 0.0625 146.9 163.0
166(4) 0.0625 146.9 161.2
161(4) 0.0625 146.9 160.2
165(4) 0.0625 146.9 159.7
165(4) 0.0625 147.0 159.6
163(4) 0.0625 147.0 159.8
160(4) 0.0625 147.0 160.3
166(4) 0.0625 147.1 161.1
169(4) 0.0625 147.1 162.2
169(4) 0.0625 147.1 163.9
176(4) 0.0625 147.2 166.4
184(4) 0.0625 147.2 170.4
177(4) 0.0625 147.2 176.4
196(4) 0.0625 147.3 185.3
203(5) 0.0400 147.3 197.8
223(5) 0.0400 147.3 214.4
248(5) 0.0400 147.4 234.7
265(5) 0.0400 147.4 257.0
287(5) 0.0400 147.5 277.7
284(5) 0.0400 147.5 291.1
287(5) 0.0400 147.5 292.3
283(5) 0.0400 147.6 280.8
258(5) 0.0400 147.6 261.5
236(5) 0.0400 147.6 240.3
213(5) 0.0400 147.7 220.9
208(5) 0.0400 147.7 205.4
199(4) 0.0625 147.8 194.5
189(4) 0.0625 147.8 188.1
186(4) 0.0625 147.8 185.9
193(4) 0.0625 147.9 187.6
194(4) 0.0625 147.9 193.0
198(4) 0.0625 148.0 201.7
207(5) 0.0400 148.0 213.6
225(5) 0.0400 148.0 227.8
248(5) 0.0400 148.1 242.8
251(5) 0.0400 148.1 256.3
266(5) 0.0400 148.2 266.4
282(5) 0.0400 148.2 273.6
281(5) 0.0400 148.3 279.0
281(5) 0.0400 148.3 282.7
286(5) 0.0400 148.3 282.2
283(5) 0.0400 148.4 274.6
260(5) 0.0400 148.4 260.0
243(5) 0.0400 148.5 241.6
226(5) 0.0400 148.5 223.1
212(5) 0.0400 148.6 206.7
192(4) 0.0625 148.6 193.5
185(4) 0.0625 148.7 183.5
176(4) 0.0625 148.7 176.4
169(4) 0.0625 148.8 171.6
169(4) 0.0625 148.8 168.5
161(4) 0.0625 148.8 166.5
166(4) 0.0625 148.9 165.2
165(4) 0.0625 148.9 164.4
165(4) 0.0625 149.0 164.0
165(4) 0.0625 149.0 163.9
168(4) 0.0625 149.1 164.0
160(4) 0.0625 149.1 164.3
161(4) 0.0625 149.2 164.8
163(4) 0.0625 149.2 165.5
169(4) 0.0625 149.3 166.3
173(4) 0.0625 149.3 167.0
170(4) 0.0625 149.4 167.7
162(4) 0.0625 149.4 168.3
166(4) 0.0625 149.5 168.9
174(4) 0.0625 149.5 169.8
172(4) 0.0625 149.6 170.9
172(4) 0.0625 149.6 172.4
173(4) 0.0625 149.7 174.5
176(4) 0.0625 149.7 177.2
186(4) 0.0625 149.8 180.9
189(4) 0.0625 149.8 186.0
203(5) 0.0400 149.9 193.3
217(5) 0.0400 149.9 204.0
227(5) 0.0400 150.0 219.8
244(5) 0.0400 150.0 242.9
274(5) 0.0400 150.1 275.7
326(6) 0.02778 150.2 320.1
384(6) 0.02778 150.2 376.7
452(7) 0.02041 150.3 443.6
515(7) 0.02041 150.3 515.1
571(8) 0.01563 150.4 579.5
602(8) 0.01563 150.4 619.2
588(8) 0.01563 150.5 618.9
569(8) 0.01563 150.5 578.4
507(7) 0.02041 150.6 513.0
433(7) 0.02041 150.6 440.4
373(6) 0.02778 150.7 372.6
302(5) 0.0400 150.7 315.7
269(5) 0.0400 150.8 271.6
242(5) 0.0400 150.9 239.6
236(5) 0.0400 150.9 217.5
215(5) 0.0400 151.0 202.8
197(4) 0.0625 151.0 193.1
186(4) 0.0625 151.1 186.6
193(4) 0.0625 151.1 182.1
186(4) 0.0625 151.2 178.8
180(4) 0.0625 151.2 176.4
181(4) 0.0625 151.3 174.5
173(4) 0.0625 151.3 173.1
176(4) 0.0625 151.4 172.0
178(4) 0.0625 151.5 171.3
172(4) 0.0625 151.5 170.8
174(4) 0.0625 151.6 170.5
173(4) 0.0625 151.6 170.5
166(4) 0.0625 151.7 170.8
164(4) 0.0625 151.7 171.4
173(4) 0.0625 151.8 172.4
171(4) 0.0625 151.9 174.1
183(4) 0.0625 151.9 176.7
178(4) 0.0625 152.0 180.8
187(4) 0.0625 152.0 187.1
190(4) 0.0625 152.1 196.6
208(5) 0.0400 152.1 210.0
224(5) 0.0400 152.2 228.2
253(5) 0.0400 152.3 251.3
280(5) 0.0400 152.3 278.2
305(6) 0.02778 152.4 306.4
334(6) 0.02778 152.4 331.1
346(6) 0.02778 152.5 345.6
348(6) 0.02778 152.5 344.8
325(6) 0.02778 152.6 329.9
310(6) 0.02778 152.6 306.6
286(5) 0.0400 152.7 281.0
259(5) 0.0400 152.8 256.8
235(5) 0.0400 152.8 235.5
216(5) 0.0400 152.9 217.7
207(5) 0.0400 152.9 203.5
191(4) 0.0625 153.0 192.8
182(4) 0.0625 153.0 184.9
179(4) 0.0625 153.1 179.2
177(4) 0.0625 153.2 175.2
175(4) 0.0625 153.2 172.4
177(4) 0.0625 153.3 170.4
165(4) 0.0625 153.3 169.0
163(4) 0.0625 153.4 168.1
169(4) 0.0625 153.4 167.6
167(4) 0.0625 153.5 167.4
171(4) 0.0625 153.5 167.7
169(4) 0.0625 153.6 168.3
171(4) 0.0625 153.7 169.4
171(4) 0.0625 153.7 170.9
168(4) 0.0625 153.8 172.9
177(4) 0.0625 153.8 175.1
178(4) 0.0625 153.9 177.3
169(4) 0.0625 153.9 178.9
172(4) 0.0625 154.0 179.5
169(4) 0.0625 154.0 179.0
171(4) 0.0625 154.1 177.7
165(4) 0.0625 154.2 176.3
174(4) 0.0625 154.2 175.2
173(4) 0.0625 154.3 175.0
165(4) 0.0625 154.3 175.8
173(4) 0.0625 154.4 178.1
174(4) 0.0625 154.4 182.3
180(4) 0.0625 154.5 188.9
196(4) 0.0625 154.5 198.1
204(5) 0.0400 154.6 209.9
222(5) 0.0400 154.6 223.9
245(5) 0.0400 154.7 238.8
262(5) 0.0400 154.8 252.4
254(5) 0.0400 154.8 261.3
269(5) 0.0400 154.9 262.3
260(5) 0.0400 154.9 255.3
250(5) 0.0400 155.0 242.6
227(5) 0.0400 155.0 227.9
220(5) 0.0400 155.1 213.7
204(5) 0.0400 155.1 201.5
184(4) 0.0625 155.2 191.7
182(4) 0.0625 155.2 184.5
179(4) 0.0625 155.3 179.5
182(4) 0.0625 155.3 176.2
180(4) 0.0625 155.4 174.3
176(4) 0.0625 155.4 173.2
168(4) 0.0625 155.5 172.8
178(4) 0.0625 155.5 172.9
174(4) 0.0625 155.6 173.6
177(4) 0.0625 155.6 174.8
184(4) 0.0625 155.7 176.8
181(4) 0.0625 155.7 180.0
184(4) 0.0625 155.8 184.7
192(4) 0.0625 155.8 191.5
199(4) 0.0625 155.9 200.9
210(5) 0.0400 155.9 213.0
215(5) 0.0400 156.0 227.7
232(5) 0.0400 156.0 244.3
253(5) 0.0400 156.1 260.7
263(5) 0.0400 156.1 274.0
263(5) 0.0400 156.2 280.5
267(5) 0.0400 156.2 278.1
265(5) 0.0400 156.2 268.0
257(5) 0.0400 156.3 254.0
242(5) 0.0400 156.3 239.5
221(5) 0.0400 156.4 226.9
213(5) 0.0400 156.4 217.9
219(5) 0.0400 156.5 213.2
212(5) 0.0400 156.5 213.4
226(5) 0.0400 156.6 218.9
231(5) 0.0400 156.6 229.9
247(5) 0.0400 156.6 246.1
261(5) 0.0400 156.7 266.9
279(5) 0.0400 156.7 290.6
300(5) 0.0400 156.8 314.3
318(6) 0.02778 156.8 333.0
333(6) 0.02778 156.9 341.2
331(6) 0.02778 156.9 335.9
299(5) 0.0400 156.9 319.0
294(5) 0.0400 157.0 295.8
268(5) 0.0400 157.0 271.2
239(5) 0.0400 157.1 248.4
231(5) 0.0400 157.1 229.1
213(5) 0.0400 157.1 213.8
208(5) 0.0400 157.2 202.3
195(4) 0.0625 157.2 194.0
195(4) 0.0625 157.3 188.4
185(4) 0.0625 157.3 184.7
185(4) 0.0625 157.3 182.4
190(4) 0.0625 157.4 181.1
174(4) 0.0625 157.4 180.5
171(4) 0.0625 157.4 180.6
184(4) 0.0625 157.5 181.4
184(4) 0.0625 157.5 183.1
187(4) 0.0625 157.5 185.9
190(4) 0.0625 157.6 190.1
189(4) 0.0625 157.6 196.0
204(5) 0.0400 157.6 204.0
210(5) 0.0400 157.7 214.1
225(5) 0.0400 157.7 226.0
248(5) 0.0400 157.7 238.7
260(5) 0.0400 157.8 250.8
260(5) 0.0400 157.8 259.8
266(5) 0.0400 157.8 263.2
258(5) 0.0400 157.9 260.6
245(5) 0.0400 157.9 253.4
240(5) 0.0400 157.9 244.5
232(5) 0.0400 158.0 236.6
230(5) 0.0400 158.0 231.4
225(5) 0.0400 158.0 230.5
224(5) 0.0400 158.0 235.1
237(5) 0.0400 158.1 246.5
256(5) 0.0400 158.1 265.7
300(5) 0.0400 158.1 293.3
327(6) 0.02778 158.1 329.3
370(6) 0.02778 158.2 372.2
422(6) 0.02778 158.2 418.6
469(7) 0.02041 158.2 462.3
497(7) 0.02041 158.2 494.2
519(7) 0.02041 158.3 504.6
517(7) 0.02041 158.3 489.9
457(7) 0.02041 158.3 455.3
414(6) 0.02778 158.3 410.5
368(6) 0.02778 158.4 364.1
308(6) 0.02778 158.4 321.5
284(5) 0.0400 158.4 285.5
255(5) 0.0400 158.4 256.8
227(5) 0.0400 158.4 235.2
223(5) 0.0400 158.5 219.6
204(5) 0.0400 158.5 208.9
202(4) 0.0625 158.5 201.7
200(4) 0.0625 158.5 197.1
200(4) 0.0625 158.5 194.3
192(4) 0.0625 158.6 192.9
189(4) 0.0625 158.6 192.8
190(4) 0.0625 158.6 194.0
190(4) 0.0625 158.6 196.9
203(4) 0.0625 158.6 201.9
210(5) 0.0400 158.6 209.6
213(5) 0.0400 158.6 220.5
229(5) 0.0400 158.7 235.1
246(5) 0.0400 158.7 253.3
267(5) 0.0400 158.7 274.5
291(5) 0.0400 158.7 297.0
315(6) 0.02778 158.7 317.7
337(6) 0.02778 158.7 332.3
348(6) 0.02778 158.7 336.4
339(6) 0.02778 158.7 328.7
313(6) 0.02778 158.8 311.8
299(5) 0.0400 158.8 290.4
268(5) 0.0400 158.8 268.6
254(5) 0.0400 158.8 249.1
239(5) 0.0400 158.8 233.3
228(5) 0.0400 158.8 222.0
221(5) 0.0400 158.8 215.1
208(5) 0.0400 158.8 212.6
221(5) 0.0400 158.8 214.0
223(5) 0.0400 158.8 218.8
221(5) 0.0400 158.8 226.4
238(5) 0.0400 158.8 235.9
261(5) 0.0400 158.8 245.8
256(5) 0.0400 158.8 254.4
260(5) 0.0400 158.8 259.7
261(5) 0.0400 158.8 260.5
266(5) 0.0400 158.8 257.3
260(5) 0.0400 158.8 251.8
241(5) 0.0400 158.8 245.1
236(5) 0.0400 158.8 237.6
230(5) 0.0400 158.8 229.4
208(5) 0.0400 158.8 220.8
206(5) 0.0400 158.8 212.4
196(4) 0.0625 158.8 204.9
197(4) 0.0625 158.8 198.6
191(4) 0.0625 158.8 193.8
187(4) 0.0625 158.8 190.3
199(4) 0.0625 158.8 188.1
193(4) 0.0625 158.8 187.2
188(4) 0.0625 158.8 187.7
189(4) 0.0625 158.8 189.5
190(4) 0.0625 158.8 193.1
199(4) 0.0625 158.8 199.0
204(5) 0.0400 158.8 207.7
217(5) 0.0400 158.8 219.8
230(5) 0.0400 158.8 235.8
243(5) 0.0400 158.8 255.9
271(5) 0.0400 158.8 279.4
314(6) 0.02778 158.7 305.0
332(6) 0.02778 158.7 329.8
350(6) 0.02778 158.7 349.7
362(6) 0.02778 158.7 359.4
356(6) 0.02778 158.7 356.0
341(6) 0.02778 158.7 340.5
321(6) 0.02778 158.7 317.3
286(5) 0.0400 158.7 291.4
277(6) 0.02778 158.7 266.3
247(5) 0.0400 158.6 244.0
221(5) 0.0400 158.6 225.6
205(5) 0.0400 158.6 211.2
193(4) 0.0625 158.6 200.5
189(4) 0.0625 158.6 192.9
180(4) 0.0625 158.6 187.8
186(4) 0.0625 158.6 184.4
182(4) 0.0625 158.5 182.3
183(4) 0.0625 158.5 181.0
182(4) 0.0625 158.5 180.1
173(4) 0.0625 158.5 179.4
188(4) 0.0625 158.5 178.6
179(4) 0.0625 158.4 177.6
178(4) 0.0625 158.4 176.6
175(4) 0.0625 158.4 175.5
176(4) 0.0625 158.4 174.5
175(4) 0.0625 158.4 173.7
178(4) 0.0625 158.3 173.1
173(4) 0.0625 158.3 172.7
174(4) 0.0625 158.3 172.4
178(4) 0.0625 158.3 172.4
177(4) 0.0625 158.3 172.6
170(4) 0.0625 158.2 173.0
174(4) 0.0625 158.2 173.6
174(4) 0.0625 158.2 174.5
168(4) 0.0625 158.2 175.7
178(4) 0.0625 158.1 177.6
184(5) 0.0400 158.1 180.2
189(5) 0.0400 158.1 183.9
192(5) 0.0400 158.1 189.2
202(5) 0.0400 158.0 196.4
203(5) 0.0400 158.0 206.0
208(5) 0.0400 158.0 218.3
233(5) 0.0400 158.0 233.1
252(5) 0.0400 157.9 250.2
270(5) 0.0400 157.9 268.3
284(6) 0.02778 157.9 285.4
300(6) 0.02778 157.8 298.8
318(6) 0.02778 157.8 305.0
317(6) 0.02778 157.8 302.5
303(6) 0.02778 157.7 292.2
285(6) 0.02778 157.7 277.1
271(6) 0.02778 157.7 260.5
247(5) 0.0400 157.7 244.7
233(5) 0.0400 157.6 231.4
226(5) 0.0400 157.6 221.5
223(5) 0.0400 157.6 215.5
226(5) 0.0400 157.5 213.5
226(5) 0.0400 157.5 215.2
225(5) 0.0400 157.5 220.5
229(5) 0.0400 157.4 228.6
236(5) 0.0400 157.4 238.9
246(5) 0.0400 157.4 249.9
262(5) 0.0400 157.3 259.9
261(5) 0.0400 157.3 266.4
271(5) 0.0400 157.3 267.6
269(5) 0.0400 157.2 262.7
263(5) 0.0400 157.2 253.2
249(5) 0.0400 157.2 241.1
235(5) 0.0400 157.1 228.4
226(5) 0.0400 157.1 216.5
217(5) 0.0400 157.0 206.2
216(5) 0.0400 157.0 197.7
194(5) 0.0400 157.0 191.1
188(5) 0.0400 156.9 186.3
186(5) 0.0400 156.9 183.0
193(5) 0.0400 156.9 180.9
183(5) 0.0400 156.8 179.7
184(5) 0.0400 156.8 179.4
182(5) 0.0400 156.8 179.9
179(4) 0.0625 156.7 181.2
189(5) 0.0400 156.7 183.5
191(5) 0.0400 156.6 187.2
195(5) 0.0400 156.6 192.5
199(5) 0.0400 156.6 200.1
207(5) 0.0400 156.5 210.3
217(5) 0.0400 156.5 223.4
229(5) 0.0400 156.4 239.6
251(5) 0.0400 156.4 258.4
282(6) 0.02778 156.4 278.9
298(6) 0.02778 156.3 299.2
311(6) 0.02778 156.3 316.6
310(6) 0.02778 156.2 327.5
327(6) 0.02778 156.2 328.9
315(6) 0.02778 156.2 320.5
290(6) 0.02778 156.1 304.6
279(6) 0.02778 156.1 284.7
275(6) 0.02778 156.0 264.1
246(5) 0.0400 156.0 244.9
224(5) 0.0400 156.0 228.3
210(5) 0.0400 155.9 214.8
208(5) 0.0400 155.9 204.7
200(5) 0.0400 155.8 197.6
195(5) 0.0400 155.8 193.3
190(5) 0.0400 155.7 191.2
189(5) 0.0400 155.7 190.8
193(5) 0.0400 155.7 191.7
199(5) 0.0400 155.6 193.4
191(5) 0.0400 155.6 195.2
194(5) 0.0400 155.5 196.5
194(5) 0.0400 155.5 196.9
188(5) 0.0400 155.5 196.3
187(5) 0.0400 155.4 194.9
193(5) 0.0400 155.4 193.0
191(5) 0.0400 155.3 190.7
190(5) 0.0400 155.3 188.0
189(5) 0.0400 155.2 185.1
186(5) 0.0400 155.2 181.9
184(5) 0.0400 155.2 178.8
179(4) 0.0625 155.1 175.9
184(5) 0.0400 155.1 173.3
184(5) 0.0400 155.0 171.2
178(4) 0.0625 155.0 169.4
172(4) 0.0625 155.0 168.0
168(4) 0.0625 154.9 167.0
167(4) 0.0625 154.9 166.2
170(4) 0.0625 154.8 165.7
178(4) 0.0625 154.8 165.4
163(4) 0.0625 154.7 165.2
158(4) 0.0625 154.7 165.2
164(4) 0.0625 154.7 165.3
159(4) 0.0625 154.6 165.5
168(4) 0.0625 154.6 165.9
168(4) 0.0625 154.5 166.4
169(4) 0.0625 154.5 166.9
174(4) 0.0625 154.5 167.5
173(4) 0.0625 154.4 168.2
175(4) 0.0625 154.4 168.9
174(4) 0.0625 154.3 169.6
174(4) 0.0625 154.3 170.3
176(4) 0.0625 154.3 171.2
183(5) 0.0400 154.2 172.4
181(5) 0.0400 154.2 174.0
174(4) 0.0625 154.1 176.4
181(4) 0.0625 154.1 179.9
184(5) 0.0400 154.1 184.7
191(5) 0.0400 154.0 191.4
205(5) 0.0400 154.0 200.1
220(5) 0.0400 153.9 211.2
238(5) 0.0400 153.9 224.7
237(5) 0.0400 153.9 240.4
260(5) 0.0400 153.8 257.7
272(5) 0.0400 153.8 275.4
291(6) 0.02778 153.8 291.6
301(6) 0.02778 153.7 303.7
305(6) 0.02778 153.7 309.6
305(6) 0.02778 153.6 308.3
306(6) 0.02778 153.6 300.9
295(6) 0.02778 153.6 289.4
285(6) 0.02778 153.5 275.8
258(5) 0.0400 153.5 261.5
246(5) 0.0400 153.5 247.0
229(5) 0.0400 153.4 233.0
214(5) 0.0400 153.4 220.0
207(5) 0.0400 153.4 208.4
189(5) 0.0400 153.3 198.6
185(5) 0.0400 153.3 190.5
189(5) 0.0400 153.2 183.9
180(4) 0.0625 153.2 178.8
175(4) 0.0625 153.2 174.8
175(4) 0.0625 153.1 171.7
181(4) 0.0625 153.1 169.4
176(4) 0.0625 153.1 167.6
172(4) 0.0625 153.1 166.2
172(4) 0.0625 153.0 165.2
172(4) 0.0625 153.0 164.4
165(4) 0.0625 153.0 163.7
161(4) 0.0625 152.9 163.2
162(4) 0.0625 152.9 162.8
161(4) 0.0625 152.9 162.5
162(4) 0.0625 152.8 162.2
162(4) 0.0625 152.8 162.0
154(4) 0.0625 152.8 161.9
151(4) 0.0625 152.8 161.7
161(4) 0.0625 152.7 161.5
162(4) 0.0625 152.7 161.3
162(4) 0.0625 152.7 161.2
158(4) 0.0625 152.6 161.0
164(4) 0.0625 152.6 160.9
160(4) 0.0625 152.6 160.9
153(4) 0.0625 152.6 160.9
161(4) 0.0625 152.5 161.1
164(4) 0.0625 152.5 161.4
158(4) 0.0625 152.5 161.9
159(4) 0.0625 152.5 162.6
165(4) 0.0625 152.4 163.4
165(4) 0.0625 152.4 164.3
165(4) 0.0625 152.4 165.4
169(4) 0.0625 152.4 166.5
167(4) 0.0625 152.4 167.5
164(4) 0.0625 152.3 168.2
167(4) 0.0625 152.3 168.5
164(4) 0.0625 152.3 168.3
159(4) 0.0625 152.3 167.7
159(4) 0.0625 152.3 166.8
159(4) 0.0625 152.2 165.8
160(4) 0.0625 152.2 164.8
157(4) 0.0625 152.2 163.8
157(4) 0.0625 152.2 163.0
159(4) 0.0625 152.2 162.3
155(4) 0.0625 152.1 161.8
158(4) 0.0625 152.1 161.4
161(4) 0.0625 152.1 161.2
161(4) 0.0625 152.1 161.1
156(4) 0.0625 152.1 161.1
159(4) 0.0625 152.1 161.2
159(4) 0.0625 152.1 161.3
155(4) 0.0625 152.0 161.5
151(4) 0.0625 152.0 161.8
157(4) 0.0625 152.0 162.2
162(4) 0.0625 152.0 162.7
162(4) 0.0625 152.0 163.3
156(4) 0.0625 152.0 164.0
158(4) 0.0625 152.0 164.9
162(4) 0.0625 152.0 165.9
161(4) 0.0625 152.0 167.0
158(4) 0.0625 152.0 168.3
167(4) 0.0625 152.0 169.6
168(5) 0.0400 151.9 171.0
168(5) 0.0400 151.9 172.2
165(5) 0.0400 151.9 173.2
170(5) 0.0400 151.9 174.0
168(5) 0.0400 151.9 174.6
164(5) 0.0400 151.9 175.0
166(5) 0.0400 151.9 175.3
169(5) 0.0400 151.9 175.9
178(4) 0.0625 151.9 176.7
177(5) 0.0400 151.9 178.0
172(4) 0.0625 151.9 179.8
180(5) 0.0400 151.9 182.4
184(5) 0.0400 151.9 186.0
193(5) 0.0400 151.9 191.0
200(5) 0.0400 151.9 197.7
202(5) 0.0400 151.9 206.5
215(5) 0.0400 151.9 218.1
233(5) 0.0400 151.9 232.8
244(6) 0.02778 151.9 251.0
259(6) 0.02778 151.9 273.0
293(6) 0.02778 151.9 298.4
325(7) 0.02041 151.9 326.8
361(6) 0.02778 151.9 357.0
385(7) 0.02041 152.0 387.1
393(7) 0.02041 152.0 413.9
423(7) 0.02041 152.0 433.9
437(7) 0.02041 152.0 443.2
440(7) 0.02041 152.0 439.8
434(7) 0.02041 152.0 424.7
404(7) 0.02041 152.0 400.8
374(7) 0.02041 152.0 372.3
344(7) 0.02041 152.0 342.7
311(6) 0.02778 152.0 314.5
293(6) 0.02778 152.1 289.2
272(6) 0.02778 152.1 267.9
248(6) 0.02778 152.1 250.9
247(6) 0.02778 152.1 238.3
235(5) 0.0400 152.1 229.9
228(5) 0.0400 152.1 225.6
226(5) 0.0400 152.1 225.3
224(5) 0.0400 152.2 228.7
237(5) 0.0400 152.2 235.8
242(5) 0.0400 152.2 246.5
260(6) 0.02778 152.2 260.8
272(6) 0.02778 152.2 278.3
295(6) 0.02778 152.3 298.4
309(6) 0.02778 152.3 320.2
329(6) 0.02778 152.3 342.1
352(7) 0.02041 152.3 361.8
368(7) 0.02041 152.4 376.7
373(6) 0.02778 152.4 383.9
372(6) 0.02778 152.4 382.0
363(6) 0.02778 152.4 371.5
348(6) 0.02778 152.4 354.6
342(6) 0.02778 152.5 334.3
321(6) 0.02778 152.5 313.3
300(6) 0.02778 152.5 293.7
291(6) 0.02778 152.6 276.8
271(5) 0.0400 152.6 263.4
259(6) 0.02778 152.6 254.2
256(5) 0.0400 152.6 249.1
244(6) 0.02778 152.7 248.2
246(5) 0.0400 152.7 251.0
259(5) 0.0400 152.7 257.0
269(6) 0.02778 152.8 265.4
274(5) 0.0400 152.8 275.1
286(6) 0.02778 152.8 284.9
293(6) 0.02778 152.9 293.0
291(6) 0.02778 152.9 297.8
299(6) 0.02778 152.9 298.4
293(5) 0.0400 153.0 294.4
285(6) 0.02778 153.0 286.7
270(5) 0.0400 153.0 276.7
265(6) 0.02778 153.1 265.4
262(5) 0.0400 153.1 253.7
256(5) 0.0400 153.2 242.2
230(5) 0.0400 153.2 231.3
227(5) 0.0400 153.2 221.4
223(5) 0.0400 153.3 212.6
213(5) 0.0400 153.3 205.1
204(5) 0.0400 153.4 199.0
200(5) 0.0400 153.4 194.1
195(5) 0.0400 153.4 190.4
194(5) 0.0400 153.5 187.8
187(5) 0.0400 153.5 186.1
185(5) 0.0400 153.6 185.4
189(5) 0.0400 153.6 185.5
190(5) 0.0400 153.7 186.5
189(5) 0.0400 153.7 188.5
196(5) 0.0400 153.7 191.5
201(5) 0.0400 153.8 195.5
203(5) 0.0400 153.8 200.7
198(5) 0.0400 153.9 207.1
215(5) 0.0400 153.9 214.5
222(5) 0.0400 154.0 222.7
232(5) 0.0400 154.0 231.5
232(5) 0.0400 154.1 240.1
246(5) 0.0400 154.1 248.0
256(5) 0.0400 154.2 254.0
265(5) 0.0400 154.2 257.5
275(6) 0.02778 154.3 257.9
258(5) 0.0400 154.3 255.5
255(5) 0.0400 154.4 251.2
262(5) 0.0400 154.4 246.1
261(5) 0.0400 154.5 241.3
240(5) 0.0400 154.5 237.7
239(5) 0.0400 154.6 236.1
248(5) 0.0400 154.6 237.1
243(5) 0.0400 154.7 241.1
241(5) 0.0400 154.7 248.4
256(5) 0.0400 154.8 259.1
277(6) 0.02778 154.9 273.0
288(6) 0.02778 154.9 289.7
309(6) 0.02778 155.0 308.4
329(6) 0.02778 155.0 328.1
344(6) 0.02778 155.1 347.1
358(6) 0.02778 155.1 363.1
367(6) 0.02778 155.2 373.8
370(6) 0.02778 155.3 377.2
371(6) 0.02778 155.3 372.6
358(6) 0.02778 155.4 360.7
342(6) 0.02778 155.4 343.4
319(6) 0.02778 155.5 323.2
305(6) 0.02778 155.5 302.1
291(6) 0.02778 155.6 281.5
268(6) 0.02778 155.7 262.6
242(5) 0.0400 155.7 245.8
239(5) 0.0400 155.8 231.4
224(5) 0.0400 155.8 219.5
217(5) 0.0400 155.9 210.0
209(5) 0.0400 156.0 202.6
205(5) 0.0400 156.0 197.0
197(5) 0.0400 156.1 192.9
194(5) 0.0400 156.2 190.2
195(5) 0.0400 156.2 188.5
189(5) 0.0400 156.3 187.8
187(5) 0.0400 156.3 188.1
191(5) 0.0400 156.4 189.2
188(5) 0.0400 156.5 191.3
197(5) 0.0400 156.5 194.3
211(5) 0.0400 156.6 198.4
205(5) 0.0400 156.7 203.6
216(5) 0.0400 156.7 209.9
222(5) 0.0400 156.8 217.1
225(5) 0.0400 156.9 225.2
244(5) 0.0400 156.9 233.7
246(5) 0.0400 157.0 242.2
252(5) 0.0400 157.0 250.0
253(5) 0.0400 157.1 256.1
268(5) 0.0400 157.2 259.7
264(5) 0.0400 157.2 260.2
268(5) 0.0400 157.3 257.6
262(5) 0.0400 157.4 252.5
242(5) 0.0400 157.4 245.5
234(5) 0.0400 157.5 237.9
237(5) 0.0400 157.6 230.3
224(5) 0.0400 157.6 223.4
214(5) 0.0400 157.7 217.6
213(5) 0.0400 157.8 213.2
206(5) 0.0400 157.8 210.4
207(5) 0.0400 157.9 209.2
217(5) 0.0400 158.0 209.5
217(5) 0.0400 158.0 211.3
215(5) 0.0400 158.1 214.3
221(5) 0.0400 158.2 218.3
223(5) 0.0400 158.2 222.6
223(5) 0.0400 158.3 226.9
233(5) 0.0400 158.4 230.5
236(5) 0.0400 158.4 232.7
240(5) 0.0400 158.5 232.9
236(5) 0.0400 158.6 231.1
228(5) 0.0400 158.6 227.5
230(5) 0.0400 158.7 222.4
224(5) 0.0400 158.8 216.5
206(5) 0.0400 158.8 210.4
208(5) 0.0400 158.9 204.3
202(5) 0.0400 159.0 198.7
193(5) 0.0400 159.0 193.6
184(5) 0.0400 159.1 189.1
183(5) 0.0400 159.2 185.4
178(5) 0.0400 159.2 182.3
175(5) 0.0400 159.3 179.8
169(5) 0.0400 159.3 177.8
174(5) 0.0400 159.4 176.2
175(4) 0.0625 159.5 175.1
174(5) 0.0400 159.5 174.2
174(5) 0.0400 159.6 173.5
173(5) 0.0400 159.7 173.1
167(4) 0.0625 159.7 172.7
169(5) 0.0400 159.8 172.5
171(5) 0.0400 159.9 172.4
171(4) 0.0625 159.9 172.3
175(5) 0.0400 160.0 172.4
169(5) 0.0400 160.1 172.5
175(5) 0.0400 160.1 172.6
169(5) 0.0400 160.2 172.8
177(4) 0.0625 160.2 173.1
176(5) 0.0400 160.3 173.4
175(4) 0.0625 160.4 173.7
175(5) 0.0400 160.4 174.1
183(5) 0.0400 160.5 174.6
184(5) 0.0400 160.6 175.1
177(5) 0.0400 160.6 175.7
176(5) 0.0400 160.7 176.4
176(5) 0.0400 160.7 177.3
182(5) 0.0400 160.8 178.4
181(5) 0.0400 160.9 179.8
187(5) 0.0400 160.9 181.5
177(5) 0.0400 161.0 183.8
178(5) 0.0400 161.0 186.6
187(5) 0.0400 161.1 190.1
185(5) 0.0400 161.2 194.4
195(5) 0.0400 161.2 199.5
199(5) 0.0400 161.3 205.4
202(5) 0.0400 161.3 212.2
209(5) 0.0400 161.4 219.7
224(6) 0.02778 161.5 227.7
228(6) 0.02778 161.5 236.0
228(6) 0.02778 161.6 244.0
247(6) 0.02778 161.6 251.3
256(6) 0.02778 161.7 257.1
267(6) 0.02778 161.7 260.8
271(6) 0.02778 161.8 262.0
265(6) 0.02778 161.9 260.6
249(6) 0.02778 161.9 257.0
255(6) 0.02778 162.0 251.9
252(6) 0.02778 162.0 245.6
244(6) 0.02778 162.1 238.8
229(6) 0.02778 162.1 231.9
215(6) 0.02778 162.2 225.1
224(6) 0.02778 162.2 218.7
213(6) 0.02778 162.3 212.7
199(5) 0.0400 162.3 207.4
197(5) 0.0400 162.4 202.9
195(5) 0.0400 162.4 199.1
195(5) 0.0400 162.5 196.0
189(5) 0.0400 162.5 193.7
185(5) 0.0400 162.6 192.1
190(5) 0.0400 162.6 191.1
185(5) 0.0400 162.7 190.7
183(5) 0.0400 162.7 191.0
189(5) 0.0400 162.8 191.8
190(5) 0.0400 162.8 193.3
201(5) 0.0400 162.9 195.4
192(5) 0.0400 162.9 198.2
195(5) 0.0400 163.0 201.7
202(5) 0.0400 163.0 205.9
203(5) 0.0400 163.1 210.8
214(6) 0.02778 163.1 216.4
215(6) 0.02778 163.1 222.4
232(5) 0.0400 163.2 228.9
236(5) 0.0400 163.2 235.5
241(5) 0.0400 163.3 241.9
248(6) 0.02778 163.3 247.6
256(6) 0.02778 163.4 252.4
250(6) 0.02778 163.4 255.7
256(6) 0.02778 163.4 257.5
264(6) 0.02778 163.5 257.9
259(6) 0.02778 163.5 257.3
263(6) 0.02778 163.6 256.4
256(6) 0.02778 163.6 255.8
251(6) 0.02778 163.6 256.3
248(6) 0.02778 163.7 258.3
252(6) 0.02778 163.7 262.4
267(6) 0.02778 163.8 269.0
272(6) 0.02778 163.8 278.4
281(6) 0.02778 163.8 290.8
292(6) 0.02778 163.9 306.2
325(6) 0.02778 163.9 324.6
351(7) 0.02041 163.9 345.5
368(7) 0.02041 164.0 368.4
406(7) 0.02041 164.0 392.4
438(7) 0.02041 164.0 416.2
455(8) 0.01563 164.1 438.1
459(7) 0.02041 164.1 456.2
473(8) 0.01563 164.1 468.4
486(8) 0.01563 164.2 473.2
479(8) 0.01563 164.2 469.8
476(8) 0.01563 164.2 458.7
449(8) 0.01563 164.3 441.2
416(7) 0.02041 164.3 419.3
392(7) 0.02041 164.3 394.9
368(7) 0.02041 164.3 369.6
344(7) 0.02041 164.4 344.7
321(6) 0.02778 164.4 321.1
298(6) 0.02778 164.4 299.5
272(6) 0.02778 164.5 280.1
268(6) 0.02778 164.5 263.1
249(6) 0.02778 164.5 248.6
245(6) 0.02778 164.5 236.4
228(5) 0.0400 164.6 226.2
216(5) 0.0400 164.6 218.0
211(5) 0.0400 164.6 211.3
207(5) 0.0400 164.6 206.0
202(5) 0.0400 164.7 201.8
199(5) 0.0400 164.7 198.4
199(5) 0.0400 164.7 195.7
191(5) 0.0400 164.7 193.6
188(5) 0.0400 164.8 191.9
187(5) 0.0400 164.8 190.5
186(5) 0.0400 164.8 189.4
185(5) 0.0400 164.8 188.4
194(5) 0.0400 164.8 187.7
199(5) 0.0400 164.9 187.1
192(5) 0.0400 164.9 186.6
187(5) 0.0400 164.9 186.2
187(5) 0.0400 164.9 186.0
186(5) 0.0400 164.9 185.8
182(5) 0.0400 165.0 185.8
181(5) 0.0400 165.0 185.8
177(5) 0.0400 165.0 186.0
184(5) 0.0400 165.0 186.4
186(5) 0.0400 165.0 186.9
186(5) 0.0400 165.1 187.7
191(5) 0.0400 165.1 188.7
187(5) 0.0400 165.1 190.0
184(5) 0.0400 165.1 191.7
188(5) 0.0400 165.1 193.9
194(5) 0.0400 165.1 196.6
194(5) 0.0400 165.2 200.0
197(5) 0.0400 165.2 204.1
209(5) 0.0400 165.2 209.0
218(6) 0.02778 165.2 214.7
223(6) 0.02778 165.2 221.3
238(6) 0.02778 165.2 228.8
246(6) 0.02778 165.3 237.0
256(6) 0.02778 165.3 245.9
264(6) 0.02778 165.3 255.2
265(6) 0.02778 165.3 264.5
281(6) 0.02778 165.3 273.6
302(7) 0.02041 165.3 281.8
293(6) 0.02778 165.3 288.4
304(7) 0.02041 165.4 292.9
301(7) 0.02041 165.4 294.7
301(7) 0.02041 165.4 293.7
299(7) 0.02041 165.4 290.0
289(6) 0.02778 165.4 284.0
284(6) 0.02778 165.4 276.3
270(6) 0.02778 165.5 267.6
265(6) 0.02778 165.5 258.5
252(6) 0.02778 165.5 249.3
250(6) 0.02778 165.5 240.6
235(6) 0.02778 165.5 232.4
221(6) 0.02778 165.5 224.9
218(6) 0.02778 165.5 218.3
214(6) 0.02778 165.6 212.5
200(5) 0.0400 165.6 207.6
199(5) 0.0400 165.6 203.6
197(5) 0.0400 165.6 200.2
192(5) 0.0400 165.6 197.6
197(5) 0.0400 165.6 195.5
192(5) 0.0400 165.6 194.0
183(5) 0.0400 165.7 192.9
192(5) 0.0400 165.7 192.2
192(5) 0.0400 165.7 191.8
194(5) 0.0400 165.7 191.7
193(5) 0.0400 165.7 191.8
193(5) 0.0400 165.7 192.2
191(5) 0.0400 165.8 192.7
196(5) 0.0400 165.8 193.5
189(5) 0.0400 165.8 194.5
191(5) 0.0400 165.8 195.6
204(5) 0.0400 165.8 196.9
200(5) 0.0400 165.8 198.4
196(5) 0.0400 165.9 200.1
191(5) 0.0400 165.9 201.9
201(5) 0.0400 165.9 203.9
197(5) 0.0400 165.9 205.9
206(5) 0.0400 165.9 208.1
207(5) 0.0400 166.0 210.5
217(6) 0.02778 166.0 213.0
219(6) 0.02778 166.0 215.7
213(5) 0.0400 166.0 218.9
221(6) 0.02778 166.0 222.6
233(6) 0.02778 166.1 227.1
236(6) 0.02778 166.1 232.6
238(6) 0.02778 166.1 239.4
241(6) 0.02778 166.1 247.8
259(6) 0.02778 166.2 258.0
275(6) 0.02778 166.2 270.2
281(6) 0.02778 166.2 284.7
292(6) 0.02778 166.2 301.6
317(7) 0.02041 166.3 320.9
346(7) 0.02041 166.3 342.6
368(7) 0.02041 166.3 366.5
391(7) 0.02041 166.3 392.4
403(7) 0.02041 166.4 419.6
443(8) 0.01563 166.4 447.5
482(8) 0.01563 166.4 475.1
506(9) 0.01235 166.5 501.0
516(9) 0.01235 166.5 523.7
535(9) 0.01235 166.5 541.5
553(9) 0.01235 166.5 553.0
551(9) 0.01235 166.6 557.0
552(9) 0.01235 166.6 553.1
552(9) 0.01235 166.6 541.6
528(9) 0.01235 166.7 523.9
498(9) 0.01235 166.7 501.3
480(8) 0.01563 166.7 475.5
444(8) 0.01563 166.8 448.1
432(8) 0.01563 166.8 420.4
398(8) 0.01563 166.9 393.3
360(7) 0.02041 166.9 367.5
340(7) 0.02041 166.9 343.7
313(7) 0.02041 167.0 322.0
304(7) 0.02041 167.0 302.7
285(6) 0.02778 167.1 285.9
269(6) 0.02778 167.1 271.4
267(6) 0.02778 167.1 259.3
257(6) 0.02778 167.2 249.2
248(6) 0.02778 167.2 241.1
243(6) 0.02778 167.3 234.8
241(6) 0.02778 167.3 230.1
237(6) 0.02778 167.4 226.7
230(6) 0.02778 167.4 224.7
237(6) 0.02778 167.5 223.8
228(6) 0.02778 167.5 223.9
226(6) 0.02778 167.6 225.1
239(6) 0.02778 167.6 227.3
239(6) 0.02778 167.7 230.4
245(6) 0.02778 167.7 234.3
242(6) 0.02778 167.8 239.2
244(6) 0.02778 167.8 244.7
262(6) 0.02778 167.9 251.0
261(6) 0.02778 167.9 257.9
269(6) 0.02778 168.0 265.2
270(6) 0.02778 168.1 272.7
277(6) 0.02778 168.1 280.2
290(6) 0.02778 168.2 287.2
303(6) 0.02778 168.2 293.4
303(6) 0.02778 168.3 298.3
317(6) 0.02778 168.4 301.6
314(6) 0.02778 168.4 302.9
312(6) 0.02778 168.5 302.1
295(6) 0.02778 168.6 299.4
289(6) 0.02778 168.6 294.8
290(6) 0.02778 168.7 288.9
283(6) 0.02778 168.8 282.0
279(6) 0.02778 168.8 274.6
265(6) 0.02778 168.9 267.1
255(6) 0.02778 169.0 259.7
251(6) 0.02778 169.0 252.7
252(6) 0.02778 169.1 246.3
235(5) 0.0400 169.2 240.6
230(5) 0.0400 169.3 235.7
227(5) 0.0400 169.3 231.7
210(5) 0.0400 169.4 228.5
210(5) 0.0400 169.5 226.1
220(5) 0.0400 169.6 224.5
230(5) 0.0400 169.6 223.6
221(5) 0.0400 169.7 223.4
223(5) 0.0400 169.8 223.7
218(5) 0.0400 169.9 224.4
218(5) 0.0400 170.0 225.4
219(5) 0.0400 170.0 226.6
225(5) 0.0400 170.1 227.8
227(5) 0.0400 170.2 229.0
229(5) 0.0400 170.3 229.9
237(5) 0.0400 170.4 230.7
233(5) 0.0400 170.5 231.1
230(5) 0.0400 170.5 231.3
233(5) 0.0400 170.6 231.2
236(5) 0.0400 170.7 230.8
234(5) 0.0400 170.8 230.1
235(5) 0.0400 170.9 229.1
235(5) 0.0400 171.0 227.8
229(5) 0.0400 171.1 226.2
224(5) 0.0400 171.2 224.4
224(5) 0.0400 171.2 222.4
223(5) 0.0400 171.3 220.4
220(5) 0.0400 171.4 218.4
221(5) 0.0400 171.5 216.5
217(5) 0.0400 171.6 214.8
214(5) 0.0400 171.7 213.4
212(5) 0.0400 171.8 212.2
209(6) 0.02778 171.9 211.3
205(5) 0.0400 172.0 210.8
203(5) 0.0400 172.1 210.7
214(5) 0.0400 172.2 211.0
208(5) 0.0400 172.3 211.8
204(5) 0.0400 172.4 213.1
204(5) 0.0400 172.4 214.8
215(5) 0.0400 172.5 217.0
214(6) 0.02778 172.6 219.8
228(6) 0.02778 172.7 223.1
224(6) 0.02778 172.8 227.0
231(6) 0.02778 172.9 231.4
233(6) 0.02778 173.0 236.3
242(6) 0.02778 173.1 241.7
243(6) 0.02778 173.2 247.5
253(6) 0.02778 173.3 253.6
268(6) 0.02778 173.4 260.0
268(6) 0.02778 173.5 266.5
272(6) 0.02778 173.6 273.0
289(6) 0.02778 173.7 279.2
293(6) 0.02778 173.8 285.0
295(6) 0.02778 173.8 290.1
307(7) 0.02041 173.9 294.4
301(7) 0.02041 174.0 297.7
294(6) 0.02778 174.1 300.0
296(7) 0.02041 174.2 301.3
295(7) 0.02041 174.3 302.0
292(7) 0.02041 174.4 302.2
306(7) 0.02041 174.5 302.3
297(7) 0.02041 174.6 302.7
292(7) 0.02041 174.6 303.7
305(7) 0.02041 174.7 305.7
303(7) 0.02041 174.8 308.8
317(7) 0.02041 174.9 313.4
310(7) 0.02041 175.0 319.6
323(7) 0.02041 175.1 327.5
326(7) 0.02041 175.1 337.3
335(7) 0.02041 175.2 348.9
360(8) 0.01563 175.3 362.3
371(8) 0.01563 175.4 377.4
384(8) 0.01563 175.5 394.0
409(8) 0.01563 175.5 411.8
423(8) 0.01563 175.6 430.4
442(9) 0.01235 175.7 449.3
447(9) 0.01235 175.7 468.0
484(9) 0.01235 175.8 485.6
505(9) 0.01235 175.9 501.5
501(9) 0.01235 176.0 514.7
517(9) 0.01235 176.0 524.4
524(9) 0.01235 176.1 530.1
534(10) 0.01000 176.1 531.4
521(10) 0.01000 176.2 528.3
531(10) 0.01000 176.3 521.0
535(10) 0.01000 176.3 510.0
530(10) 0.01000 176.4 496.1
504(10) 0.01000 176.4 479.8
471(10) 0.01000 176.5 462.0
461(10) 0.01000 176.5 443.1
427(9) 0.01235 176.6 423.7
405(9) 0.01235 176.6 404.3
394(9) 0.01235 176.7 385.1
356(9) 0.01235 176.7 366.6
339(8) 0.01563 176.7 348.9
335(8) 0.01563 176.8 332.2
317(8) 0.01563 176.8 316.6
314(8) 0.01563 176.8 302.3
299(8) 0.01563 176.9 289.3
284(8) 0.01563 176.9 277.7
289(8) 0.01563 176.9 267.3
273(8) 0.01563 176.9 258.0
245(7) 0.02041 177.0 250.0
265(7) 0.02041 177.0 242.9
244(7) 0.02041 177.0 236.8
240(7) 0.02041 177.0 231.6
240(7) 0.02041 177.0 227.0
228(7) 0.02041 177.0 223.2
224(7) 0.02041 177.0 219.9
224(7) 0.02041 177.0 217.1
225(7) 0.02041 177.0 214.7
207(7) 0.02041 177.0 212.7
211(6) 0.02778 177.0 211.1
217(7) 0.02041 177.0 209.6
220(7) 0.02041 177.0 208.4
209(6) 0.02778 177.0 207.4
220(7) 0.02041 177.0 206.6
198(6) 0.02778 176.9 205.9
207(6) 0.02778 176.9 205.4
206(6) 0.02778 176.9 204.9
195(6) 0.02778 176.9 204.5
195(6) 0.02778 176.8 204.2
201(6) 0.02778 176.8 203.9
203(6) 0.02778 176.8 203.7
195(6) 0.02778 176.7 203.5
196(6) 0.02778 176.7 203.4
198(6) 0.02778 176.6 203.2
201(6) 0.02778 176.6 203.0
202(6) 0.02778 176.5 202.9
201(6) 0.02778 176.5 202.8
204(6) 0.02778 176.4 202.6
204(6) 0.02778 176.4 202.6
214(7) 0.02041 176.3 202.5
197(7) 0.02041 176.2 202.6
186(7) 0.02041 176.2 202.7
192(7) 0.02041 176.1 202.9
205(7) 0.02041 176.0 203.3
205(7) 0.02041 176.0 203.8
194(7) 0.02041 175.9 204.5
200(7) 0.02041 175.8 205.4
201(7) 0.02041 175.8 206.5
210(7) 0.02041 175.7 207.9
205(7) 0.02041 175.6 209.5
215(7) 0.02041 175.5 211.3
216(7) 0.02041 175.4 213.5
224(8) 0.01563 175.4 216.0
214(7) 0.02041 175.3 218.8
216(7) 0.02041 175.2 221.9
216(7) 0.02041 175.1 225.4
223(7) 0.02041 175.0 229.2
231(8) 0.01563 174.9 233.2
240(8) 0.01563 174.9 237.6
239(8) 0.01563 174.8 242.2
243(8) 0.01563 174.7 247.0
251(8) 0.01563 174.6 251.9
248(8) 0.01563 174.5 256.8
264(8) 0.01563 174.4 261.8
276(10) 0.01000 174.4 266.7
295(10) 0.01000 174.3 271.4
278(10) 0.01000 174.2 275.9
284(10) 0.01000 174.1 279.9
281(10) 0.01000 174.1 283.4
288(10) 0.01000 174.0 286.2
288(10) 0.01000 173.9 288.2
296(10) 0.01000 173.9 289.2
288(10) 0.01000 173.8 289.3
289(10) 0.01000 173.7 288.3
283(10) 0.01000 173.7 286.3
280(10) 0.01000 173.6 283.4
299(10) 0.01000 173.6 279.7
266(9) 0.01235 173.6 275.3
272(9) 0.01235 173.5 270.4
279(10) 0.01000 173.5 265.2
285(10) 0.01000 173.5 259.8
270(10) 0.01000 173.5 254.4
249(9) 0.01235 173.5 249.0
244(9) 0.01235 173.5 243.7
253(9) 0.01235 173.5 238.7
221(9) 0.01235 173.5 233.9
208(8) 0.01563 173.6 229.4
217(8) 0.01563 173.6 225.3
212(8) 0.01563 173.7 221.6
224(11) 0.00826 173.7 218.3
209(10) 0.01000 173.8 215.3
226(10) 0.01000 173.9 212.7
237(11) 0.00826 174.0 210.5
219(11) 0.00826 174.1 208.6
210(10) 0.01000 174.3 207.0
199(10) 0.01000 174.4 205.8
220(10) 0.01000 174.6 204.9
204(10) 0.01000 174.8 204.2
203(10) 0.01000 175.0 203.8
212(10) 0.01000 175.2 203.6
198(10) 0.01000 175.4 203.6
210(10) 0.01000 175.7 203.8
208(10) 0.01000 176.0 204.1
209(10) 0.01000 176.3 204.6
194(10) 0.01000 176.6 205.2
206(10) 0.01000 177.0 205.9
202(10) 0.01000 177.4 206.7
200(10) 0.01000 177.8 207.6
207(10) 0.01000 178.2 208.5
203(10) 0.01000 178.7 209.4
221(10) 0.01000 179.2 210.4
217(11) 0.00826 179.7 211.4
205(10) 0.01000 180.3 212.3
204(10) 0.01000 180.9 213.2
210(14) . . .
227(15) . . .
204(14) . . .
222(15) . . .
220(15) . . .
216(14) . . .
202(14) . . .
210(15) . . .
206(14) . . .
215(15) . . .
191(14) . . .
213(14) . . .
204(14) . . .
222(15) . . .
201(15) . . .
199(14) . . .
227(15) . . .
214(15) . . .
204(15) . . .
211(14) . . .
231(15) . . .
213(15) . . .
248(15) . . .
184(15) . . .
0(15) . . .
